Lawrence C. Bank

JOHN WILEY & SONS, INC.

This book is printed on acid-free paper. 嘷 ⬁ Copyright 䉷 2006 by John Wiley & Sons, Inc. All rights reserved Published by John Wiley & Sons, Inc., Hoboken, New Jersey Published simultaneously in Canada No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, recording, scanning, or otherwise, except as permitted under Section 107 or 108 of the 1976 United States Copyright Act, without either the prior written permission of the Publisher, or authorization through payment of the appropriate per-copy fee to the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, (978) 750-8400, fax (978) 750-4470, or on the web at www.copyright.com. Requests to the Publisher for permission should be addressed to the Permissions Department, John Wiley & Sons, Inc., 111 River Street, Hoboken, NJ 07030, (201) 748-6011, fax (201) 748-6008, e-mail: [email protected] Limit of Liability / Disclaimer of Warranty: While the publisher and author have used their best efforts in preparing this book, they make no representations or warranties with respect to the accuracy or completeness of the contents of this book and speciﬁcally disclaim any implied warranties of merchantability or ﬁtness for a particular purpose. No warranty may be created or extended by sales representatives or written sales materials. The advice and strategies contained herein may not be suitable for your situation. You should consult with a professional where appropriate. Neither the publisher nor author shall be liable for any loss of proﬁt or any other commercial damages, including but not limited to special, incidental, consequential, or other damages. For general information on our other products and services or for technical support, please contact our Customer Care Department within the United States at (800) 762-2974, outside the United States at (317) 572-3993 or fax (317) 572-4002. Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic books. For more information about Wiley products, visit our web site at www.wiley.com. Library of Congress Cataloging-in-Publication Data: Bank, Lawrence Colin, 1956– Composites for construction : structural design with FRP materials / Lawrence C. Bank. p. cm. Includes index. ISBN-13: 978-0471-68126-7 ISBN-10: 0-471-68126-1 (cloth) 1. Fiber reinforced plastics—Textbooks. 2. Polymeric composites— Textbooks. 3. Structural design—Textbooks. I. Title. TA455.P55B36 2006 624.1⬘892—dc22 2005030950 Printed in the United States of America 10 9 8 7 6 5 4 3 2 1

CONTENTS Preface 1

Introduction 1.1 1.2 1.3

1.4 1.5 1.6 1.7 1.8

2

xiii

Overview, 1 Historical Background, 2 FRP Reinforcements for New Concrete Structural Members, 3 1.3.1 FRP Bars or Grids for Reinforced Concrete Members, 4 1.3.2 FRP Tendons for Prestressed Concrete Members, 6 1.3.3 Stay-in-Place FRP Formwork for Reinforced Concrete Members, 8 FRP Strengthening of Existing Structural Members, 10 FRP Proﬁles for New Structures, 18 Other Emerging Applications of Interest to Structural Engineers, 23 Properties of FRP Products for Structural Engineering Design, 25 Published Design Guides, Codes, and Speciﬁcations for FRP Composites in Structural Engineering, 34 1.8.1 FRP Reinforcing Bars and Tendons, 34 1.8.2 FRP Strengthening Systems, 34 1.8.3 FRP Pultruded Proﬁles, 35 1.8.4 Manufacturers’ Design Manuals, 35 1.8.5 Key Conferences Series, 36 1.8.6 Archival Journals, 37

Materials and Manufacturing 2.1 2.2

1

40

Overview, 40 Raw Materials, 41 2.2.1 Reinforcing Fibers, 41 2.2.2 Polymer Resins, 45 v

vi

CONTENTS

2.3

3

75

Properties of FRP Composites 3.1 3.2

3.3

3.4

4

Manufacturing Methods, 51 2.3.1 Pultrusion, 52 2.3.2 Hand Layup, 68 2.3.3 Other Manufacturing Processes,

Overview, 78 Theoretical Determination of Properties, 78 3.2.1 Fiber Level, 78 3.2.2 Lamina Level, 83 3.2.3 Laminate Level, 89 3.2.4 Full-Section Level, 103 Experimental Determination of Properties, 104 3.3.1 Fiber Level, 105 3.3.2 Lamina Level, 106 3.3.3 Laminate Level, 107 3.3.4 Full-Section Level, 110 Relevant Standard Test Methods for FRP Composites for Structural Engineers, 118 3.4.1 American Society of Testing and Materials Test Methods, 118 3.4.2 Full-Section Test Methods for FRP Bars and Laminates, 120

Design Basis for FRP Reinforcements 4.1 4.2 4.3 4.4

78

Overview, 128 Introduction, 129 Properties of FRP Reinforcing Bars, 129 Design Basis for FRP-Reinforced Concrete, 133 4.4.1 Resistance Factors, 134 4.4.2 Minimum Reinforcement Requirements, 135 4.4.3 Determination of Guaranteed Properties of FRP Rebars, 135 4.4.4 Design for Environmental Effects on FRP Rebars, 136 4.4.5 Special Considerations Regarding FRP Rebars, 137 4.4.6 Design for Serviceability, 139 4.4.7 Temperature and Shrinkage Reinforcement in Slabs, 140

128

CONTENTS

5

FRP Flexural Reinforcement 5.1 5.2 5.3

5.4

5.5

5.6 6

6.4 6.5 7

143

Overview, 143 Introduction, 143 Flexural Strength of an FRP-Reinforced Section, 145 5.3.1 Overreinforced Section, 147 5.3.2 Underreinforced Section, 148 5.3.3 Minimum Flexural Reinforcement, 151 Design Procedure for an FRP-Reinforced Flexural Member, 151 5.4.1 Design of FRP-Reinforced Bridge Deck Slabs, 160 Serviceability Design of FRP-Reinforced Beams, 166 5.5.1 Deﬂections Under Service Loads, 166 5.5.2 Flexural Cracking, 169 5.5.3 Creep and Fatigue at Service Loads, 170 Design Procedure for Serviceability, 170

FRP Shear Reinforcement 6.1 6.2 6.3

182

Overview, 182 Introduction, 182 Shear Design of an FRP-Reinforced Concrete Section, 185 6.3.1 Concrete Contribution to Shear Capacity, 185 6.3.2 Shear Capacity of FRP Stirrups, 187 6.3.3 Punching Shear Capacity in Slabs, 189 Limits on Shear Reinforcement and Shear Strengths for Shear Design, 189 Design Procedure for FRP Shear Reinforcement, 190

FRP Reinforcement Detailing 7.1 7.2 7.3 7.4 7.5 7.6 7.7 7.8

vii

Overview, 198 Introduction, 198 Geometric Details, 200 7.3.1 Calculation of Bar Spacing, 202 Bond Strength of FRP Bars, 204 Development of Straight FRP Bars, 205 Development of Hooked FRP Bars, 206 Lap Splices for FRP Bars, 207 Design Procedure to Detail FRP Bars in a Beam,

198

207

viii

8

CONTENTS

Design Basis for FRP Strengthening 8.1 8.2 8.3 8.4

8.5 8.6 9

Overview, 214 Introduction, 215 Properties of FRP Strengthening Systems, 217 Design Basis for FRP Strengthening Systems, 219 8.4.1 Resistance Factors, 219 8.4.2 Guaranteed Properties, 220 8.4.3 Environmental Effects, 220 8.4.4 Limits on Strengthening, 221 8.4.5 Limits on Stresses in FRP Strengthening Systems at Service Loads, 223 8.4.6 Compression Strengthening in Flexural Members, 223 Deﬂections in FRP-Strengthened Structures, 223 FRP Strengthening System Area Calculations, 223

FRP Flexural Strengthening 9.1 9.2 9.3

9.4

9.5 9.6 9.7 9.8

214

Overview, 227 Introduction, 227 Flexural Capacity of an FRP-Strengthened Member, 230 9.3.1 Stress in the FRP Strengthening System, 233 9.3.2 Strain in the Internal Reinforcing Steel, 234 9.3.3 Neutral-Axis Depth, 234 9.3.4 Existing Substrate Strain, 235 Determination of Failure Modes and Flexural Capacity, 236 9.4.1 Mode 1a: Concrete Crushing After Steel Yields, 237 9.4.2 Mode 1b: Concrete Crushing Before Steel Yields, 238 9.4.3 Mode 2a: FRP Failure After Steel Yields, 239 9.4.4 Mode 2b: FRP Failure Before Steel Yields, 241 Balanced Condition, 243 Detailing for Flexural Strengthening, 244 Design Procedure for a Flexurally Strengthened Concrete Member, 245 Serviceability of FRP-Strengthened Flexural Members, 266

227

CONTENTS

ix

9.8.1 9.8.2

9.9

10

FRP Shear Strengthening 10.1 10.2 10.3 10.4 10.5 10.6

11

288

Overview, 288 Introduction, 289 Shear Capacity of an FRP-Strengthened Member, 293 Effective Strain in the FRP for Shear Strengthening, 296 Design Procedure for Shear Strengthening, 298 Shear Strengthening of Fully Wrapped Axially Loaded Columns, 308

FRP Conﬁning 11.1 11.2 11.3

11.4 11.5 11.6

11.7 11.8 11.9 12

Cracked FRP Strengthened Section, 266 Service-Level Stress in the Internal Steel Reinforcing Bars, 268 9.8.3 Service-Level Stress in the FRP Strengthening System, 270 Load–Deﬂection Response of FRP-Strengthened Flexural Members, 271

316

Overview, 316 Introduction, 316 FRP Conﬁning for Axial Strengthening, 324 11.3.1 Serviceability for FRP-Strengthened Axial Members, 326 Design Procedure for FRP Axial Strengthening of RC Circular Columns, 327 FRP-Strengthened Eccentrically Loaded Columns, 333 FRP Conﬁning for Increased Ductility, 346 11.6.1 Lateral Displacement Ductility, 347 11.6.2 Flexural Hinge Conﬁnement, 348 Design Procedure for Flexural Hinge Conﬁnement, 350 Lap Splice Region Conﬁnement, 351 Plastic Shear Overstrength Demand, 352

Design Basis for FRP Proﬁles 12.1 12.2 12.3 12.4

Overview, 359 Introduction, 360 Properties of Pultruded Proﬁles, 363 Design Basis for FRP Pultruded Structures,

359

369

x

CONTENTS

12.5 13

373

Pultruded Flexural Members 13.1 13.2 13.3 13.4 13.5 13.6

13.7

13.8 14

12.4.1 Allowable Stress Design, 370 12.4.2 Load and Resistance Factor Design, Performance-Based Design, 380

Overview, 384 Introduction, 384 Stresses in Flexural Members, 385 Deformations in Flexural Members, 388 Determination of Deﬂections and Stresses for Serviceability and Ultimate Limit States, 392 Serviceability Limits States, 393 13.6.1 Deformation Limit State: Transverse Deﬂection, 393 13.6.2 Long-Term Deﬂection in Pultruded Beams, 397 Ultimate Limit States, 401 13.7.1 Lateral–Torsional Buckling, 401 13.7.2 Local Buckling of Walls Due to In-Plane Compression, 403 13.7.3 Local Buckling of Walls Due to In-Plane Shear, 413 13.7.4 Web Crushing and Web Buckling in the Transverse Direction, 414 13.7.5 Additional Factors Affecting Local Buckling in Pultruded Proﬁles, 415 13.7.6 Flange and Web Longitudinal Material Failure, 417 13.7.7 Flange and Web Material Shear Failure, 418 Design Procedure for Flexural Members, 419

Pultruded Axial Members 14.1 14.2 14.3 14.4 14.5 14.6 14.7

384

Overview, 436 Introduction, 436 Concentrically Loaded Compression Members, 437 Deformations in Concentrically Loaded Compression Members, 439 Determination of Deﬂections and Stresses for Serviceability and Ultimate Limit States, 439 Serviceability Limit States: Axial Shortening, 439 Ultimate Limit States, 440

436

CONTENTS

xi

14.7.1 14.7.2 14.7.3 14.7.4

14.8 14.9

14.10

14.11

14.12 14.13

15

Global Flexural Buckling, 440 Global Torsional Buckling, 442 Local Buckling Due to Axial Loads, 443 Interaction Between Local and Global Buckling Modes in Intermediate-Length Compression Members, 450 14.7.5 Flange and Web Longitudinal Material Failure, 453 Design Procedure for Concentrically Loaded Compression Members, 453 Concentrically Loaded Tension Members, 467 14.9.1 Deformations in Concentrically Loaded Tension Members, 468 Determination of Deﬂections and Stresses for Serviceability and Ultimate Limit States: Axial Elongation, 468 Ultimate Limit States, 469 14.11.1 Longitudinal Material Failure on the Gross Area, 469 14.11.2 Longitudinal Material Failure on the Net Area, 469 Design Procedure for Concentrically Loaded Tension Members, 470 Combined Load Members, 471 14.13.1 Members Subjected to Combined Flexure and Compression (Beam-Columns), 471 14.13.2 Members Subjected to Combined Flexure and Tension, 477

Pultruded Connections 15.1 15.2

15.3 15.4 15.5 15.6

Overview, 484 Introduction, 485 15.2.1 Conventional Pultruded Connections, 485 15.2.2 Custom Pultruded Connections, 488 Mechanical Fasteners and Connection Parts, 490 15.3.1 FRP Nuts and Bolts, 492 Research on Heavy Beam-to-Column Pultruded Connections, 492 Bolted Pultruded Connections, 496 Light-Truss Pultruded Connections, 498 15.6.1 Lap Joint Connections, 499

484

xii

CONTENTS

15.7 15.8 15.9

Heavy-Frame Pultruded Connections, 503 Design of Bolted Pultruded Connections, 504 Determination of Stresses in In-Plane Lap Joints, 505 15.9.1 Bearing Stress in the Base Pultruded Material, 505 15.9.2 Net-Tension Stress in the Base Pultruded Material, 506 15.9.3 Shear-Out Stress in the Base Pultruded Material, 506 15.9.4 Shear Stress on a Bolt, 507 15.10 Stresses in Out-of-Plane Shear Connections, 507 15.10.1 Longitudinal Shear Stress at the Heel of an Angle, 507 15.10.2 Flexural Stress in the Leg of an Angle Bolted to a Column Member, 508 15.10.3 Transverse Tensile Stress in a Web–Flange Junction of a Column, 509 15.10.4 Block Shear in a Beam Web, 509 15.10.5 Flexural and Shear Stresses in Flexible Seated Connections, 510 15.11 Critical Connection Limit States, 510 15.12 Design Procedure for a Pultruded Connection, 512 References

527

Index

545

PREFACE Fiber-reinforced polymer (FRP) composite materials have developed into economically and structurally viable construction materials for buildings and bridges over the last 20 years. FRP composite materials used in structural engineering typically consist of glass, carbon, or aramid ﬁbers encased in a matrix of epoxy, polyester, vinylester, or phenolic thermosetting resins that have ﬁber concentrations greater than 30% by volume. They have been used in structural engineering in a variety of forms: from structural proﬁles to internal reinforcing bars for concrete members to strips and sheets for external strengthening of concrete and other structures. Depending on the form of the FRP product used in structural engineering, the FRP material is supplied either as a ready-to-use structural component such as a wide-ﬂange proﬁle or a reinforcing bar, or it is supplied in its constituent forms as dry ﬁber and liquid polymer resin and formed and cured in situ to create a structural component. These two forms should be familiar to structural engineers, as they have analogs in conventional structural materials such as steel beams or steel reinforcing bars which are supplied in ready-to-use form from a steel mill, or portland cement concrete, which is supplied in the form of cement, aggregate, and water constituents and is formed in situ to create a structural element. The purpose of Composites for Construction is to provide structural engineering students, educators, and professionals with a code-based text that gives detailed design procedures for FRP composites for civil engineering structures. The emphasis of the book is on the design of structural members and structural systems that use FRP composites as one or all of the structural materials in the structure. The emphasis of the book is not on the design of the FRP composite materials themselves, and the book provides only a brief review of topics related to constituent materials, micro- and macromechanics of composite materials, and manufacturing methods of composite materials. It is important to emphasize that this book is self-contained and that no prior knowledge of FRP composite materials is required to use the book and to learn how to design with FRP composites in structural engineering. Fiberreinforced composite materials have been used for many decades in the aerospace, automotive, and the industrial and recreational products industries. Many excellent textbooks and reference books are available that cover the manufacturing, mechanics, and design of ﬁber composite materials. Nor does the book cover topics of structural analysis or structural mechanics, except where needed to explain design procedures or design philosophy. xiii

xiv

PREFACE

Composites for Construction is intended primarily for use as a collegelevel text in civil and structural engineering curricula. It is intended for seniorlevel (fourth-year) undergraduate students in civil engineering programs or ﬁrst-year graduate students in structural engineering programs and for their instructors. Users of the book will ﬁnd that its form is similar to that of traditional structural engineering design textbooks used to teach subjects such as steel design, reinforced concrete design, and wood design. The book is intended to be covered in a one-semester three-credit lecture-style course on FRP composites in structural engineering. Alternatively, the book can be used to supplement course material in courses on reinforced concrete design, steel design, or wood design since many of the topics covered have parallels to analytical and design methods in these subjects and are logical extensions of the methods used in these subjects. When used for a stand-alone course in a civil or structural engineering program, it is expected that students will have had at least one course in structural analysis, one course in reinforced concrete design, and one course in structural steel design (or design of wood structures). If students have the appropriate background, the book can also be used in architectural engineering or in construction engineering curricula. Composites for Construction is divided into four parts. The ﬁrst part provides an introduction to FRP applications, products, and properties and to the methods of obtaining the characteristic properties of FRP materials for use in structural design. The second part covers the design of concrete structural members reinforced with FRP reinforcing bars. The third part covers the design of FRP strengthening systems such as strips, sheets, and fabrics for upgrading the strength and ductility of reinforced concrete structural members. The fourth part covers the design of trusses and frames made entirely of FRP structural proﬁles produced by the pultrusion process. From a mechanics point of view, the type of FRP material examined in the three design parts of the book increases in complexity from a one-dimensional FRP reinforcing bar to a two-dimensional thin FRP strip or plate to a three-dimensional thin-walled FRP proﬁle section. As the geometric complexity of the FRP component increases, so does its anisotropy and hence so does the number of properties that need to be considered in the structural design. The format for each of the three design parts of Composites for Construction is similar. It starts with a discussion of the design basis and material properties used for the speciﬁc application of the FRP material in the design considered in that part. This is followed by sections related to design of speciﬁc types of structural members and structural systems (such as beams and columns or trusses and frames) that are unique to the different types of FRP materials examined in each part. In each chapter, examples of the design of typical members and structures are provided in a step-by-step, annotated format that enables the reader to follow the design processes. Each chapter concludes with a set of recommended homework problems. Each design part of the book also discusses important construction- and constructability-related

PREFACE

xv

aspects of FRP composites in structures. FRP materials are generally new to structural designers, and most designers have not yet inculcated an intuitive understanding of their behavior as they have for traditional materials such as concrete, steel, and wood. It is therefore important to understand how FRP materials are erected or installed or applied in the ﬁeld and how the construction process can inﬂuence the design process. As noted, Composites for Construction is code-based, which means that it provides design procedures in accordance with published structural engineering design codes, guides, and speciﬁcations. The discussion of FRP reinforcing bars and FRP strengthening systems follows a load and resistance factor design basis and presents design procedures for FRP materials used in combination with reinforced concrete according to the most recent editions of the design guides published by the American Concrete Institute: ACI 440.1R-06, Guide for the Design and Construction of Structural Concrete Reinforced with FRP Bars, and ACI 440.2R-02, Guide for Design and Construction of Externally Bonded FRP Systems for Strengthening Concrete Structures. The ﬁnal part of the book provides design guidance for FRP proﬁle sections according to a combination of recommendations of the ASCE Structural Plastics Design Manual, the Eurocomp Design Code and Handbook, the AASHTO Speciﬁcations, and manufacturer-published design guides. Procedures are provided for the structural designer on how to use this combination of codelike documents to design with FRP proﬁles. When Composites for Construction is used as a textbook for a one-semester (15-week) course, the following allocation of time is recommended: Part One, three weeks; Part Two, four weeks; Part Three, four weeks; Part Four, four weeks. Composites for Construction is based on course notes developed by the author while teaching this course over a number of years at the University of Wisconsin–Madison and at Stanford University (while on sabbatical in 2003–2004). Based on the author’s experience in teaching this course in recent years, a number of more advanced topics will need to be omitted, depending on the students’ background, to be able to cover all the material in a one-semester course. This includes an in-depth treatment of micromechanics and lamination theory (in Chapter 3), FRP bars for bridge decks (in Chapter 5), load–deﬂection response in FRP-strengthened structures (in Chapter 9), FRP shear strengthening of columns (in Chapter 10), FRP conﬁnement for ductility enhancement in columns (in Chapter 11), FRP proﬁle beam-columns (Chapter 14), and combined FRP ﬂexural–tension members (in Chapter 14). A midterm examination covering Parts One and Two and a ﬁnal examination covering Parts Three and Four is recommended. In addition, individual or group design projects that run the length of the entire semester are recommended. The imperial inch–pound–second system of units is used throughout the book, as these units are commonly used in U.S. design practice. SI (System International) and metric cm–g–s units are used occasionally where standard

xvi

PREFACE

practice is to report material properties in these units (even in the United States). However, a complete SI version of the design examples and problems is not included at this time, in the interest of brevity. Composites for Construction focuses on the mainstream application areas of FRP composites in structural engineering at the time of writing. Over the years there have been a number of other applications and uses of FRP composites in structural engineering. In many cases, code-based guidance has only recently been developed or is currently being developed for these applications. The applications include FRP tendons for internal or external prestressing of concrete; FRP stay cables for bridges or guy wires for towers; FRP grids, meshes, and gratings for reinforcing concrete; FRP stay-in-place forms for concrete beams, slabs, or columns; FRP strengthening of prestressed concrete structures; FRP strengthening of masonry structures; FRP strengthening of steel, aluminum, or timber structures; mechanically fastened FRP strengthening systems; FRP pretensioned sheets for strengthening; and FRP strengthening for blast loads on structures. ACKNOWLEDGMENTS Composites for Construction is based on notes I developed for a three-credit lecture course taught at the University of Wisconsin–Madison and at Stanford University, and on notes developed for short courses taught through the Department of Engineering Professional Development at the University of Wisconsin and at the University of Arizona. I am indebted to all the students who attended my courses at the University of Wisconsin and at Stanford University who provided both feedback and motivation to improve the early drafts of the book and helped to provide critical insights for improving and reﬁning the examples and homework problems in the text. I am thankful for the advice, encouragement, and support that I have received from many of my colleagues and friends in the FRP composites for construction community. I extend my special thanks to Toby Mottram, Antonio Nanni, Carol Shield, Joseph Hanus, Brahim Benmokrane, Kenneth Neale, Sami Rizkalla, Urs Meier, Charles Bakis, Jin-Guang Teng, Jian-Fei Chen, Jack Lesko, Thomas Keller, and Edward Nawy. The support of my colleagues in industry who were always forthcoming with technical data and information was also critical to the development of the book. I would like to thank Doug Gremel (Hughes Brothers), Glenn Barefoot (Strongwell), Rick Johansen (ET Techtonics), Dustin Troutman (Creative Pultrusions), Jay Thomas (Structural Preservation Systems), Ben Bogner (BP Chemical), Dave White (Sika Corporation), and Pete Milligan (Fyfe Company) for their willingness to provide information. Composites for Construction would not have been possible without the support of my colleagues at the University of Wisconsin–Madison. In particular, I would like to thank Jeffrey Russell for his constant guidance and

ACKNOWLEDGMENTS

xvii

feedback, and Michael Plesha for his insightful reﬂections on book writing. Sincere thanks also go to the Structures and Geomechanics Group of the Civil and Environmental Engineering Department at Stanford University who hosted me as a UPS Visiting Professor at Stanford University while on sabbatical from the University of Wisconsin in 2003–2004. It was during this year that much of the manuscript was completed. In particular, I would like to thank Kincho Law of Stanford University for his support over the past 20 years. My thanks also go out to colleagues who have worked with me over the years, especially Timothy Kao, Russell Gentry, and Terry Gerhardt, and to Jim Harper at John Wiley & Sons for his understanding and guidance. Finally, this book would never have been written without the constant, continuing, and unwavering support of my wife, Rebecca, daughter, Anna, and son, Jacob. It was their persistence, and their faith in me, that made this book a reality. LARRY BANK Madison, Wisconsin January 2006

1 1.1

Introduction OVERVIEW

Over the last decade there has been signiﬁcant growth in the use of ﬁberreinforced polymer (FRP) composite materials as construction materials in structural engineering, which for the purposes of this book is deﬁned as the ﬁeld of engineering that covers the analysis and design of primary, loadbearing structural members and systems in buildings and bridges by civil and structural engineers. Also known as ﬁber-reinforced plastics, or advanced composite materials (ACMs), these materials have proven themselves to be valuable for use in the construction of new buildings and bridges and for the upgrading of existing buildings and bridges. As these materials have transitioned from the research laboratory to implementation in actual structures, so have codes and speciﬁcations developed for them for use in civil engineering structural design in the last decade. Now, at the beginning of the twenty-ﬁrst century, the structural engineering community is about to enter a stage in which structural design with FRP composites is poised to become as routine as structural design with classical structural materials such as masonry, wood, steel, and concrete. In this chapter we review the historical development of FRP composite materials for use in structural engineering. The review and design chapters that follow focus on the use of FRP composite materials in three primary areas: (1) reinforcements for new concrete structural members, (2) strengthening for existing structural members, and (3) proﬁles for new structures. In what follows, code-based design procedures are provided for these three topics. The historical review concentrates on actual engineering structures that have been designed by professional engineers and constructed using construction techniques and technologies used routinely in the architecture, engineering, and construction (AEC) industry. The review is intended to give realworld examples of the use of FRP composite materials to construct structures, or important elements of structures, that have traditionally been constructed from conventional construction materials. In addition to the foregoing three topics, other applications in large-scale civil infrastructure engineering, such as electric power transmission-line towers, luminaries supports, masonry strengthening, and timber strengthening, are described, even though codebased design procedures have not been developed at this time for these applications. This is to provide evidence of the feasibility of constructing safe Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

1

2

INTRODUCTION

and reliable structures that have a direct bearing on the construction of buildings and bridges and as an indication of future applications for which code guidance is currently being developed. The historical development of advanced composite materials and their widespread applications in the aerospace, automotive, industrial, and recreational products, although of great general technological interest, is not of speciﬁc relevance to buildings and bridges and is not included in this review. Following the review of the building and bridge structures that have been constructed using FRP composite materials, a survey of the key mechanical and physical properties of representative FRP composite material products that are currently available is presented. 1.2

HISTORICAL BACKGROUND

FRP composites have been used on a limited basis in structural engineering for almost 50 years for both new construction and for repair and rehabilitation of existing structures. Structural and civil engineers have been afﬁxing their professional stamps to designs for buildings and bridges for many years, even though these materials have not been recognized by ofﬁcial building codes, and no code-approved design procedures have existed until very recently. These forward-thinking engineers have tended to be people who have specialized expertise in the use of FRP composites in structural engineering or who were in-house structural engineers directly afﬁliated with a manufacturer of FRP components. In addition to being registered structural engineers involved in engineering practice, many of these engineers have had fundamental knowledge of the materials, manufacturing methods, and fabrication and installation methods for FRP composite in civil engineering structures. Many have worked on teams to develop new FRP components for civil engineering structures (Bank, 1993b). Since the mid-1990s, however, other structural engineers and architects have begun to design with FRP composites on a fairly routine basis. In general, these engineers and architects have not had specialized training or exposure to FRP composites as construction materials. These designs are completed with the aid of published design procedures or by proof testing, and often, with the aid of an in-house engineer from an FRP product manufacturer, who advises on the details of the design and provides sample speciﬁcations for the FRP material for the contract documents. Many structural engineers of this type have also afﬁxed their professional seals to these designs over the past decade. The historical review provides selected examples of where FRP composites have been used in building and bridges in the past half-century. More attention is paid to the applications from the 1990s, which were designed in a routine fashion by structural engineers, as opposed to those from before the 1990s, which were generally designed by engineers with a specialized knowledge of composites. The review describes applications that used FRP components and

1.3

FRP REINFORCEMENTS FOR NEW CONCRETE STRUCTURAL MEMBERS

3

products available at the time of their manufacture. Many FRP products used in these projects are no longer produced or have been replaced by improved parts and products. The state of the art of the early work, from 1980 to 1990, in the area of FRP composites for reinforcing and retroﬁtting of concrete structures in the United States, Japan, Canada, and Europe is detailed in collections of papers and reports edited by Iyer and Sen (1991) and Nanni (1993b). In 1993, a series of biannual international symposia devoted to FRP reinforcement of concrete structures was initiated.1 At about this time, international research interest in the use of FRP in concrete increased dramatically. Collections of papers on the use of FRP proﬁle sections in structures have been published by the American Society of Civil Engineers (ASCE) since the early 1980s by the now-disbanded Structural Plastics Research Council (SPRC) and in proceedings of the ASCE Materials Congresses.2 In 1997, the American Society of Civil Engineers (ASCE) founded the Journal of Composites for Construction, which today is the main international archive for reporting on research and development in the ﬁeld of FRP materials for the AEC industry.3 In 2003, the International Institute for FRP in Construction (IIFC) was established in Hong Kong. To date, thousands of research studies and structural engineering projects using FRP materials have been reported worldwide. Reviews of developments in the ﬁeld from 1990 to 2000 can be found in ACI (1996), Hollaway and Head (2001), Teng et al. (2001), Bakis et al. (2002), Hollaway (2003), Van Den Einde et al. (2003), and Ta¨jlsten (2004).

1.3 FRP REINFORCEMENTS FOR NEW CONCRETE STRUCTURAL MEMBERS FRP reinforcements for new concrete structural members have been of interest to structural engineers since the earliest days of the FRP composites industry. In 1954, in his seminal paper on the development of pultrusion technology, Brandt Goldsworthy speculated that ‘‘the chemical inertness of this material allows its use in . . . concrete reinforcing and all types of structural members that are subject to corrosive action in chemical plants or other areas where corrosive conditions exist’’ (Goldsworthy, 1954). Since then, engineers have endeavored to ﬁnd ways to realize this dream in a number of ways, and at

1 Known as FRPRCS: ﬁber-reinforced polymers in reinforced concrete structures. They have been held in Vancouver (1993), Ghent (1995), Sapporo (1997), Baltimore (1999), Cambridge (2001), Singapore (2003), Kansas City (2005), and Patras (2007). 2 Sponsored by the ASCE Materials Engineering Division (now incorporated into the ASCE Construction Institute) and held in 1990 (Denver), 1992 (Atlanta), 1994 (San Diego), and 1999 (Cincinnati). 3 Additional international symposia and journal series focused on FRP composites in structural engineering of note are listed at the end of this chapter.

4

INTRODUCTION

present, FRP reinforcements for new concrete structural members can be divided into three primary areas: (1) FRP bars or grids for reinforced concrete (RC) members, (2) FRP tendons for prestressed concrete (PC) members, and (3) stay-in-place FRP formwork for reinforced concrete members. 1.3.1

FRP Bars or Grids for Reinforced Concrete Members

The use of FRP reinforcing bars and grids for concrete is a growing segment of the application of FRP composites in structural engineering for new construction. From 1950s to the 1970s, a small number of feasibility studies were conducted to investigate the use of small-diameter (⬃–14 -in. or 6-mm) glass FRP rods, with and without surface deformations, to reinforce or prestress concrete structural members (Nawy et al., 1971; Nawy and Neuwerth, 1977). In the early 1980s, glass helical–strand deformed reinforcing bars were produced for structural engineering applications by Vega Technologies, Inc. of Marshall, Arkansas (Pleimann, 1991). These bars were used to build magnetic resonance imaging facilities, due to their electromagnetic transparency. At the time, these FRP bars were cost-competitive with stainless steel bars, which were the only other alternative for this application. Many single-story castin-place wall and slab structures, which look identical to conventional reinforced concrete structures, were built. Designs were performed by registered structural engineers using the working stress design basis, and the buildings were constructed using conventional construction technology. In the late 1980s, interest in the use of FRP rebars received a boost as attention focused on ways to mitigate corrosion in steel-reinforced concrete structures exposed to the elements, especially highway bridge decks. In the United States, International Grating, Inc. developed a sand-coated glass ﬁber– reinforced bar that was used experimentally in a number of bridge deck projects. This was followed in the 1990s by the development of deformed FRP bars by Marshall Composites, Inc. A number of companies experimented with FRP bars with helically wound spiral outer surfaces. These included Creative Pultrusions, Glasforms, Vega Technologies, International Grating, Hughes Brothers, and Pultrall.4 In the late 1990s a number of these producers also experimented with carbon ﬁber FRP bars with deformed, helically wound, and sand-coated surfaces. Extensive research was conducted in the 1990s on the behavior of concrete beams and slabs reinforced with various types of FRP bars (Daniali, 1990; Faza and GangaRao, 1990, 1993; Nanni, 1993a; Benmokrane et al., 1996a,b; Michaluk et al., 1998). Studies were also conducted on the use of glass ﬁber pultruded FRP gratings in reinforced concrete slabs (Bank and Xi, 1993). ACI published its ﬁrst design guide, ACI 440.1R01, for FRP-reinforced concrete in 2001 (ACI, 2001). The guide was subse-

4 Many of the companies mentioned no longer exist or have ceased production of these products. The information is provided for historical purposes.

1.3

FRP REINFORCEMENTS FOR NEW CONCRETE STRUCTURAL MEMBERS

5

quently revised in 2003 (ACI 440.1R-03), and the current version, ACI 440.1R-06, was published in 2006 (ACI, 2006).5 Figure 1.1 shows samples of a number of commercially produced glass- and carbon-reinforced FRP bars for concrete reinforcing. At the same time that glass ﬁber FRP bars were being developed for reinforcing concrete in corrosive environments in the United States, a parallel effort was under way in Japan. The Japanese effort focused, to a large extent, on carbon ﬁber reinforcement, due to concern for the degradation of glass ﬁbers in alkaline environments. A two-dimensional grid product called NEFMAC (new ﬁber composite material for reinforced concrete) was developed successfully and commercialized by Shimizu Corporation (Fujisaki et al., 1987; Fukuyama, 1999). Grids with carbon ﬁbers, glass ﬁbers, and carbon– glass hybrid ﬁbers were produced. The majority of applications of NEFMAC appear to have been in tunnels, where the noncorrosive properties and panel sizes of the grids were very effective when used with shotcreteing methods. Design guides for reinforced concrete design with FRP bars were published in Japan in 1995 and 1997 (BRI, 1995; JSCE, 1997). Efforts were also directed to developing polyvinyl alcohol (PVA) FRP bars, but these were never commercialized. Figure 1.2 shows carbon and glass NEFMAC grids developed in Japan in the 1980s. Today, FRP reinforcing bars for concrete with both glass and carbon ﬁbers are produced by a number of companies in North America, Asia, and Europe. The use of FRP bars has become mainstream and is no longer conﬁned to demonstration projects. However, this is still a niche area in structural engineering; competition among manufacturers is fairly ﬁerce and only the strong

Figure 1.1 Glass- and carbon-reinforced FRP bars.

5 This book provides design procedures in accordance with the 2006 version of ACI 440.1R-06 and should not be used with older versions. Substantial changes related to ASCE 7-02 load and resistance factors were introduced in 2006.

6

INTRODUCTION

Figure 1.2 NEFMAC FRP grids.

companies are surviving. Applications have become routine for certain specialized environments. Most current applications appear to be in underground tunnels and in bridge decks. Figure 1.3 shows a large glass ﬁber FRP reinforcing cage being readied for placement in forms for a tunneling application. The FRP bars are used to create a ‘‘soft eye’’ for subsequent drilling through a vertical concrete shaft wall. These FRP bars are lap spliced to the steel bars in a conventional fashion. Figure 1.4 shows a bridge deck slab with a glass FRP top mat being poured. In addition to FRP bars for reinforcing concrete, FRP dowel bars for concrete highway pavements and FRP ground anchors have also been commercialized successfully in recent years. Explicit design procedures according to the ACI are given in this book for the design of concrete structures reinforced with FRP bars. 1.3.2

FRP Tendons for Prestressed Concrete Members

Development of FRP tendons for prestressing concrete took place in Holland, Germany, and Japan in the early 1980s. This was motivated primarily by the desire to reduce corrosion in prestressed concrete elements. A rectangular aramid FRP strip called Arapree was developed in Holland by the Hollandsche Beton Groep (HBG) and Akzo, and a glass ﬁber tendon in an external polymer sheath called Polystal was developed by Strabag Bau AG and Bayer AG in Germany. These products were used in a number of bridge demon-

1.3

FRP REINFORCEMENTS FOR NEW CONCRETE STRUCTURAL MEMBERS

7

Figure 1.3 Reinforcing cage being readied for placement in forms for a tunneling application. (Courtesy of Hughes Brothers.)

Figure 1.4 Bridge deck slab with a glass FRP top mat being poured. (Courtesy of Hughes Brothers.)

8

INTRODUCTION

stration projects in Europe, but their production has been discontinued. Arapree is now produced by Sireg in Italy. In the 1980s in Japan, a national project was undertaken to develop FRP reinforcements for concrete that focused primarily on tendons (Fukuyama, 1999). Many different aramid and carbon ﬁber products were developed and over 50 demonstration projects were completed. The Advanced Composite Cable Club (ACC Club) was founded to coordinate and commercialize FRP prestressing products in Japan. These included twisted-strand carbon tendons called carbon ﬁber composite cable (CFCC), known as Tokyo Rope, by Tokyo Seiko K.K.; aramid ﬁber rods and strips, called Arapree (under license from HBG), by Nippon Aramid Co.; aramid ﬁber rods, called Technora Rods, by Teijin Ltd.; aramid ﬁber tendons, called FiBRA, by Kobe Steel Cable; and carbon ﬁber tendons, called Leadline, by Mitsubishi Chemical Corporation. As conventional steel chucks and anchors could not be used, due to the low transverse strength of FRP tendons, all the manufacturers developed specialized prestressing anchors. This has proved to be the Achilles heel of the FRP prestressing industry. Both technical difﬁculties with the anchors and their high prices made them unattractive to the construction industry. Through the 1990s a number of demonstration projects were conducted in the United States and Canada using Japanese and European FRP prestressing products, but routine use of these FRP tendons has not occurred. These FRP rods have also been used as conventional reinforcing bars in a number of demonstration projects. An FRP tendon and anchorage system has not been commercialized in the United States. The design of FRP pretressed concrete is discussed in the Japanese guide for FRP reinforcements (JSCE, 1997). A guide for the design of concrete structures with FRP prestressing tendons, ACI 440.4R-04, has been published (ACI, 2004b). FRP prestessing products produced in Japan in the 1980s and 1990s are shown in Fig. 1.5. 1.3.3

Stay-in-Place FRP Formwork for Reinforced Concrete Members

The use of FRP composites as stay-in-place (SIP) formwork has been explored for a number of years. FRP SIP formwork systems that act to reinforce the concrete after it has cured and systems used only as SIP forms have been developed. A stay-in-place bridge deck panel produced by Diversiﬁed Composites, Inc. in the United States has been used on two multispan highway bridges in Dayton, Ohio (1999) and Waupun, Wisconsin (2003). The deck form has a corrugated proﬁle and is intended as a noncorroding substitute for stay-in-place metal and prestressed concrete deck forms. When used as a stayin-place deck form, the FRP composite serves as the tensile reinforcement after the concrete has hardened. Figure 1.6 shows an FRP deck form being placed over concrete prestressed girders. FRP tubular stay-in-place forms have also been used to manufacture beam and column members. They are also referred to as concrete-ﬁlled FRP tubes. A carbon shell system consisting of concrete-ﬁlled carbon FRP tubes has been

1.3

FRP REINFORCEMENTS FOR NEW CONCRETE STRUCTURAL MEMBERS

9

Figure 1.5 Japanese FRP prestressing tendons.

Figure 1.6 Placement of FRP stay-in-place forms for a bridge deck. (Courtesy of Adam Berg.)

10

INTRODUCTION

used to produce girders for the superstructure of a highway bridge in California (Van Den Einde et al., 2003). Figure 1.7 shows FRP–concrete tubular piling manufactured by Lancaster Composites in the United States.

1.4 FRP STRENGTHENING OF EXISTING STRUCTURAL MEMBERS FRP materials used to strengthen and repair load-bearing structural members are popular applications of FRP composites in structural engineering. Collectively, these applications are known as retroﬁtting applications, as they are used in existing structures and not in the construction of new structures. Retroﬁtting applications can be classiﬁed broadly into two types. One type is strengthening, where the original structure’s strength or ductility (typically, its displacement capacity) is increased from the loads (or displacements) for which it was originally designed. This increase may be necessitated by the desire to make the structure compatible with existing building codes (particularly in the case of seismic retroﬁtting) or may be desired due to changes in use of the structure. FRP retroﬁtting to improve the performance (load carrying and ductility) of a structure when subjected to blast and impact loading has become of interest of late. The other type of FRP retroﬁtting can be classiﬁed as repair. In this case, the FRP composite is used to retroﬁt an existing and deteriorated structure to bring its load-carrying capacity or duc-

Figure 1.7 FRP piles. (Courtesy of Lancaster Composites.)

1.4

FRP STRENGTHENING OF EXISTING STRUCTURAL MEMBERS

11

tility back to the loads or displacements for which it was designed (and hence is, in fact, a type of strengthening). Repair is necessitated when the original structure has deteriorated due to environmental effects, such as corrosion of steel reinforcing in concrete structures or when the original structure has been damaged in service or was not constructed according to the original design. For example, reinforcing bars may be omitted in a beam at the time of construction due to a design or construction error. Although these two types of applications are similar, there are important differences that are related primarily to evaluation of the existing structural capacity and the nature of the repair to be undertaken before FRP can be used. In many cases, a repair design will include strengthening to add a level of safety to the repaired structure and to account for uncertainty in the retroﬁt design. FRP retroﬁtting has been used successfully on reinforced concrete structures, prestressed concrete structures, timber structures, and masonry and metal structures. At this time, code design guidance is only available for FRP retroﬁtting of reinforced concrete structures, particularly as applied to strengthening. Consequently, this historical review focuses primarily on the use of FRP retroﬁtting technologies for reinforced concrete and prestressed concrete structures. Two primary methods are used to attach FRP composite materials to concrete structures (and to masonry, timber, and even metallic structures) for retroﬁtting purposes. One method employs premanufactured rigid6 FRP strips 1 [approximately 4 in. (100 mm) wide and –– 16 in. (1.6 mm) thick] that are adhesively bonded to the surface of the structural member. The other method, known as hand layup, consists of in situ forming of the FRP composite on the surface of the structural member using ﬂexible dry ﬁber fabrics or sheets of width approximately 6 to 60 in. (150 to 1500 mm) and liquid polymers. In recent years a new variant of the premanufactured strip method called near surface mounting (NSM) has been developed. In this method, a thin, narrow FRP strip [⬃–18 ⫻ –34 in. (3 by 18 mm)] or small-diameter round FRP bar [⬃–14 in. (6 mm)] is inserted and then bonded adhesively into a machined groove at the surface of the concrete member. FRP retroﬁtting has been used with bridge and building structures to strengthen static and quasistatic loads (such as increases in dead or live load in a bridge or building structure), and for dynamic loads (such as strengthening for improved seismic or blast response in a bridge or building structure). FRP composites have been used successfully for ﬂexural strengthening of concrete beams and slabs, shear strengthening of concrete beams, and axial strengthening and ductility enhancement of concrete columns. The use of FRP composites for retroﬁtting concrete structures appears to have evolved at approximately the same time, in the late 1980s, in Europe (particularly in Switzerland) and in Japan. Both of these initiatives were fol6

Rigid is used here in the qualitative sense to describe a solid but nevertheless deformable material.

12

INTRODUCTION

lowed very soon afterward by research and applications in the United States and Canada. Initially, research focused on ﬂexural strengthening of structural members (concrete and timber). This was followed very closely by studies on conﬁnement of concrete columns with FRP composite fabrics and sheets, known as wraps, to address a number of deﬁciencies in concrete columns, particularly in highway bridges, subjected to lateral loads due to earthquakes. Both of these FRP applications grew out of the experience gained with retroﬁtting of reinforced concrete using steel plates or steel jackets. The use of steel plates to strengthen reinforced concrete structural members was an accepted technology by the mid-1980s, particularly for bridge retroﬁtting (Eberline et al., 1988). The use of steel jackets to retroﬁt concrete columns developed into a routine practice in the United Sates following the Loma Prieta earthquake in 1989 (Chai et al., 1991). FRP shear strengthening of concrete beams has been studied since the early 1990s (soon after ﬂexural strengthening) and numerous applications in concrete structures, particularly precast prestressed concrete T-beams, have been undertaken. Strengthening of concrete slabs for punching shear has been studied in recent years but is not yet an accepted technology. Adhesively bonded precured carbon ﬁber-reinforced epoxy FRP strengthening strips for ﬂexural strengthening of concrete beams was ﬁrst studied and used in Switzerland in the late 1980s by Urs Meier and his colleagues at the Swiss Federal Laboratories for Material Testing and Research (EMPA). Activities at EMPA from the mid-1980s to the mid-1990s have been reviewed by Meier (1995). An FRP strengthening strip known as Carbodur was developed at EMPA and commercialized by Sika. The ﬁre safety and fatigue life of the system have been studied at EMPA. These strips have been used in hundreds of building, bridge, and chimney retroﬁt projects in Europe (Taerwe and Matthys, 1999). An L-shaped precured strip has recently been developed by EMPA for shear strengthening of beams. Today, precured strips are produced by a number of manufacturers, including S&P Clever Reinforcement Company in Austria; Hughes Brothers, Strongwell, and FyfeCo in the United States; and Sika in Switzerland. Since the mid-1990s, following commercialization of the precured FRP strip, hundreds of research projects and thousands of FRP retroﬁts for static or nonseismic dynamic loads (e.g., vehicular loads, wind loads) have been carried out throughout the world. Figure 1.8 shows installation of a precured FRP strip. Manufacturers of FRP products themselves have traditionally provided design guidance for the use of precured FRP strengthening strips. The ﬁrst English-language edition of the Sika Carbodur design guide appeared in 19977 (Sika, 1997). Current editions have replaced earlier editions as more information has become available and new FRP strengthening products have been introduced. A design guide is published by the S&P Reinforcement Company

7

Key design guides and speciﬁcations are listed at the end of this chapter and in the references.

1.4

FRP STRENGTHENING OF EXISTING STRUCTURAL MEMBERS

13

Figure 1.8 Installation of a precured FRP strip. (Courtesy of Sika Corporation.)

that covers their products (S&P, 1998). More recently, professional organizations have developed general-purpose design guides for use of precured (and bonded) FRP strengthening products for concrete structures, which in time will probably replace manufacturers’ guides (TR 55, 2004; FIB, 2001; ACI, 2002; CSA, 2002). Code guidance for NSM systems is currently being developed. Figure 1.9 shows the installation of NSM strips in a concrete slab. Hand-layup FRP composite systems for retroﬁtting concrete structures were developed and commercialized in Japan in the late 1980s. This was soon followed by work in the United States. In Japan attention focused on the use of unidirectional carbon ﬁber sheets (known as tow sheets). The Tonen Corporation developed the Forca tow sheet, Mitsubishi Chemical developed the Replark sheet, and Toray developed the Torayca fabric system. As opposed to the European focus, which was on strengthening for static load-carrying capacity, the Japanese effort was driven primarily by the need to retroﬁt building and bridge structures for earthquake-induced seismic loads. Consequently, much of the research was directed toward wrapping of columns to increase their lateral load-carrying capacity (Katsumata et al., 1988). In Japan during this time there was also work in the area of ﬂexural and shear strengthening of concrete beams and slabs (Nanni, 1995). To date, Japanese FRP sheet products have been used in hundreds of bridge and building retroﬁt projects in Japan. A dramatic increase in FRP retroﬁtting projects in Japan was seen after the 1995 Hyogoken–Nanbu earthquake, which devastated the city of Kobe. Karbhari (1998) provided an extensive database of key projects completed in Japan at that time. In addition to manually applied hand-layup systems, the Ohbayashi Corporation pioneered the development of an automated carbon ﬁber winding machine for strengthening tall chimneys. A design

14

INTRODUCTION

Figure 1.9 Installation of near-surface-mounted (NSM) strips. (Courtesy of Structural Group.)

guide was published by the Japan Society of Civil Engineers (JSCE) in 2001. An English edition of the Forca tow sheet technical manual was published in 1996 (Tonen, 1996), and an English edition of the Replark technical manual was published in 1999 (Replark, 1999). Early work in the United States on FRP strengthening of concrete structures was undertaken for the purpose of seismic retroﬁtting of reinforced concrete columns. The Fyfe Company developed a glass fabric and epoxy hand-layup system for column retroﬁtting in the early 1990s that was tested at the University of California San Diego (UCSD) (Priestley et al., 1992). This work was followed by further development and testing of FRP column wrapping systems, with research being conducted primarily at UCSD (Priestley and Seible, 1995). Based on much of this earlier work, Acceptance Criteria 125 was published by the International Conference of Building Ofﬁcials (ICBO) to provide guidance to contractors and designers who wished to use the method in the United States (AC 125, 1997).

1.4

FRP STRENGTHENING OF EXISTING STRUCTURAL MEMBERS

15

Simultaneously, a number of researchers in the United States studied ﬂexural strengthening of beams using hand-layup ﬁber sheets and fabrics of glass or carbon ﬁbers (Saadamanesh, 1994). The Forca tow sheet carbon sheet strengthening system, called the MBrace System (MBrace, 1998), was commercialized in the United States by Master Builders, Inc. of Ohio together with Structural Preservation Systems of Maryland. The Fyfe Company developed and commercialized the Tyfo System (Tyfo, 1998). Installation of a fabric sheet is shown in Figure 1.10. Hexcel supplies fabric strengthening systems for Sika known as SikaHex. Nowadays numerous companies market a variety of fabric and sheet strengthening materials in the United States, including VSL, Edge Structural Composites, and Quakewrap. Figure 1.11 shows installation of an FRP wrap on a rectangular column. Hand-layup fabrics and sheets have been used in thousands of projects in the United States and around the world. Since the 1994 Northridge earthquake in California, hundreds of highway columns have been retroﬁtted in California and neighboring states. Wrapping of circular columns with FRP is most effective; however, rectangular columns have also been retroﬁtted for both strength and ductility successfully using FRP wraps. FRP retroﬁtting of a highway column is shown in Fig. 1.12. FRP strengthening sheets and fabrics have been used to strengthen precast T-beams for shear strength enhancement in numerous parking garage structures. Flexural strengthening projects for bridge beams and slabs with sheets

Figure 1.10 Installation of a carbon ﬁber fabric sheet. (Courtesy of Fyfe Company.)

16

INTRODUCTION

Figure 1.11 Installation of FRP wrap. (Courtesy of Sika Corporation.)

and fabrics have been carried out in almost every state in the United States. In recent years FRP sheets and fabrics have been used to strengthen concrete shear walls for seismic retroﬁt and for blast strengthening (also know as hardening). Figure 1.13 shows carbon fabrics being installed on an interior concrete shear wall of a building for the purpose of seismic retroﬁtting.

Figure 1.12 FRP wrap being installed on a highway column. (Courtesy of Sika Corporation.)

1.4

FRP STRENGTHENING OF EXISTING STRUCTURAL MEMBERS

17

Figure 1.13 FRP fabrics for building shear wall retroﬁt. (Courtesy of Racquel Hagen.)

Other strengthening systems, used in the United States primarily for column retroﬁts, have used prefabricated FRP shells and automated ﬁber winding. A prefabricated FRP composite shell system called the Snaptite system, which consists of ﬂexible thin FRP shells that are bonded in multiple layers, was produced by the C.C. Myers company of California in the late 1990s (Xiao and Ma, 1997). Use of the Snaptite system is shown in Fig. 1.14. Large

Figure 1.14 Use of the Snaptite system. (Courtesy of Yan Xiao.)

18

INTRODUCTION

cylindrical rigid shells, similar to steel jackets, have been produced by Hardcore Composites of Delaware and used in a number of experimental projects. In the late 1990s, XXSys of San Diego, California, developed a ﬁber winding system, similar to the Japanese Ohbayashi system, for bridge retroﬁts. None of these systems was ever used routinely in the United States for FRP retroﬁtting of concrete structures. FRP sheets and fabrics have also been used extensively to retroﬁt concrete masonry wall systems as well as timber beams and steel and aluminum members. These uses are discussed in what follows as ‘‘other’’ applications of FRP composites in structural engineering since code-based design guidance is not yet available for these applications. 1.5

FRP PROFILES FOR NEW STRUCTURES

A cost-effective method of producing high-quality constant-cross-section FRP proﬁle shapes, called pultrusion, was developed in the 1950s in the United States. Initially, small proﬁles were produced primarily for industrial applications, but the method was always envisioned as being used for developing FRP substitutes for conventional beams and columns in buildings and bridges. To quote Brandt Goldsworthy again: ‘‘The chemical inertness of this material allows its use in . . . all types of structural members that are subject to corrosive action in chemical plants or other areas where corrosive conditions exist’’ (Goldsworthy, 1954). By the late 1960s and early 1970s a number of pultrusion companies were producing ‘‘standard’’ I-shaped and tubular proﬁles. The Structural Plastics Research Council (SPRC) was established in 1971 by the American Society of Civil Engineers (ASCE), and a manual was developed for the design of structural plastics (McCormick, 1988). Called the Structural Plastics Design Manual (SPDM), it was originally published in 1979 as an FHWA report and subsequently by the ASCE in 1984 (ASCE, 1984). This guide was not restricted to pultruded proﬁles. In 1996, a European design guide for polymer composite structures was published (Eurocomp, 1996), and in 2002 the European Union published the ﬁrst standard speciﬁcation for pultruded proﬁles (CEN, 2002a). The ﬁrst large structures constructed from FRP proﬁles were single-story gable frames that were used in the emerging computer and electronics industry for Electromagnetic Interference (EMI) test laboratories. The electromagnetic transparency of the FRP proﬁles was a key beneﬁt in these buildings which required no magnetic material above the foundation level. Custom pultruded proﬁles and building systems were developed and commercialized by Composites Technology, Inc. (CTI), founded by Andrew Green in Texas in the 1960s (Smallowitz, 1985). In 1985, CTI designed and constructed an innovative EMI building for Apple Computer. Similar structures were also constructed from FRP pultruded proﬁles produced by Morrison Molded Fiberglass Company (MMFG, now Strongwell) in Virginia for IBM and others

1.5

FRP PROFILES FOR NEW STRUCTURES

19

in the 1980s. Figure 1.15 shows a FRP gable frame building during the installation of the FRP cladding. For much of this time, designing was done by an MMFG subsidiary called Glass-Steel. A design manual for the MMFG proﬁle shape Extren was published in 1973. Creative Pultrusions began producing standard shapes in the late 1970s, called Pultex, and developed a design manual. Current editions of these manuals are published regularly and are available from these two companies. The next major development in building systems for FRP proﬁles, which continues to be the largest market segment for large pultruded building components, was in the cooling tower industry. An FRP building system was developed in the 1980s by Composite Technology, Inc. for Ceramic Cooling Tower (CCT) and commercialized as the Unilite system (Green et al., 1994). The Unilite system consisted of a number of unique beam, column, and panel FRP pultruded components. Today, a number of pultrusion companies supply specialized parts for FRP cooling tower systems to a variety of cooling tower manufacturers as shown in Figure 1.16. In addition to custom cooling tower structures, FRP proﬁles have been used in ‘‘stick-built’’ cooling towers since the late 1980s. These systems are typically constructed using tubular FRP sections 2 ⫻ 2 in. (50 ⫻ 50 mm) and 3 ⫻ 3 in. (75 ⫻ 75 mm) covered with an FRP or nonreinforced polymer cladding system. Designers typically use standard off-the-shelf pultruded proﬁles in these structures and design them according to applicable building codes. A stick-built cooling tower under construction is shown in Fig. 1.17. To date, standard FRP proﬁle shapes have not seen much use in multistory frame building structures for commercial or residential construction. One of the major difﬁculties with multistory frame structures using FRP proﬁles is the development of economical and effective means of connecting the individual members. Research has been conducted on the subject of FRP connections since the early 1990s, but no simple and effective connection system

Figure 1.15 FRP gable frame structure under construction. (Courtesy of Strongwell.)

20

INTRODUCTION

Figure 1.16 FRP cooling tower. (Courtesy of SPX Cooling Technologies, Inc.)

Figure 1.17 Stick-built cooling tower under construction. (Courtesy of Strongwell.)

1.5

FRP PROFILES FOR NEW STRUCTURES

21

has yet been developed or commercialized for FRP pultruded proﬁles. Most current designs use steel-like connection details that are not optimized for FRP proﬁles. A prototype multistory framed building called the Eyecatcher, constructed by Fiberline Composites in Basel, Switzerland in 1999, is shown in Fig. 1.18. The building was constructed for the Swissbau Fair as a demonstration of the potential for FRP proﬁle shapes (Keller, 1999). In the ﬁeld of bridge engineering, FRP proﬁle shapes have seen increased application since the mid-1970s. Both the light weight of the FRP components and their noncorrosive properties serve to make them attractive as bridge decking panels and as superstructure members. Hundreds of 30 to 90 ft (9 to 27 m)-long short span pedestrian footbridges of the truss variety have been designed and constructed worldwide using small FRP proﬁles. Figure 1.19 shows a FRP bridge designed and constructed by ET Techtonics. In 1992, a 131-m-long cable-stayed pedestrian bridge was constructed in Aberfeldy, Scotland, using the Advanced Composite Construction System (ACCS), a FRP plank system designed by Maunsell Structural Plastics (Burgoyne and Head, 1993; Cadei and Stratford, 2002). A ﬁber rope called Paraﬁl was used for the cable stays. In 1997, a 40.3-m cable-stayed pedestrian bridge

Figure 1.18 Eyecatcher building. (Courtesy of Thomas Keller.)

22

INTRODUCTION

Figure 1.19 Light-truss pedestrian bridge pultruded structure. (Photo and design by ET Techtonics.)

was constructed over a railway line using FRP proﬁles in Kolding, Denmark (Braestrup, 1999). Both of these structures are worth noting, due to their extensive use of FRP pultruded proﬁles that facilitated rapid and economical construction. In the 1990s, a signiﬁcant effort was undertaken by a number of FRP manufacturers to develop an FRP bridge deck system that could be used on conventional steel or concrete girders. Besides the potential for long-term durability of an FRP bridge deck, an added beneﬁt exists when FRP decks are used to replace deteriorated reinforced concrete decks. Due to the significant decrease in dead weight of the structure, the live-load capacity for the re-decked structure can be increased, which may be beneﬁcial, especially on bridges with load postings. FRP deck systems have been developed and commercialized by Creative Pultrusions, Martin Marietta Composites, Atlantic Research Corp., Hardcore Composites, and others (Bakis et al., 2002). As with FRP frame systems, the connections between the prefabricated FRP deck panels and those between the FRP deck and the superstructure have been sources of the greatest difﬁculty in realizing this technology. The high cost of glass FRP decks compared with conventional concrete decks does not appear to be able to offset savings in weight and construction productivity. Developing an approved bridge guardrail for FRP deck systems has also proved to be a challenge that has not been resolved satisfactorily at this time. In 2001, a glass–carbon FRP pultruded proﬁle 36 in. high by 18 in. wide known as the double-web beam (DWB) was developed by Strongwell for use as a bridge girder. Figure 1.20 shows FRP girders on the Dickey Creek bridge in Virginia in 2001. FRP rods have also been developed for use as guy wires for towers and for suspension cables for bridges. Pultruded glass FRP rods have been used since the mid-1970s in numerous applications in the United States as guy

1.6

OTHER EMERGING APPLICATIONS OF INTEREST

23

Figure 1.20 FRP DWB girders on Dickey Creek bridge. (Courtesy of Strongwell.)

wires or bracing cables in antenna towers. The use of carbon FRP cables for bridges was ﬁrst suggested in the early 1980s by Urs Meier of the Swiss Federal Laboratories for Materials Testing and Research (EMPA) in Dubendorf, Switzerland, as an alternative to steel cables for very long span suspension bridges, where the weight of the cable itself can be a limiting factor (Meier, 1986). Since then, EMPA and BBR Ltd. in Zurich, Ciba AG in Basle, and Stesalit AG in Zullwil, Switzerland, have worked together on developing carbon FRP cables for bridges. In 1997, two carbon FRP cables consisting of 241 5-mm (0.2-in.)-diameter carbon–epoxy FRP rods were used in the Storchen cable-stayed bridge in Winterthur, Switzerland. Figure 1.21 is a close-up of the multistrand carbon FRP cable used. FRP proﬁles have also been used as stays in the Kolding FRP pedestrian bridge constructed in Denmark in 1997, and carbon ﬁber cables were used in the Laroin footbridge constructed in France in 2002. 1.6 OTHER EMERGING APPLICATIONS OF INTEREST TO STRUCTURAL ENGINEERS Strengthening of masonry structures with FRP strips, sheets, and fabrics is one of the largest emerging application areas of FRP composites in structural engineering. Unfortunately, no code-based design guidance is available for masonry strengthening at this time. Literature on the subject is reviewed in Nanni and Tumialan (2003). Most FRP strengthening of masonry has been on non-load-bearing in-ﬁll walls and in historic masonry structures. Strengthening of both brick and hollow concrete masonry unit (CMU) structures is used to increase both the out-of-plane and in-plane capacity of masonry walls

24

INTRODUCTION

Figure 1.21 Carbon ﬁber cables used in the Storchen bridge in Switzerland. (Courtesy of Urs Meier.)

for both dynamic and static loads. Out-of-plane blast strengthening of masonry walls with FRPs is used to preserve the integrity of a masonry wall during a blast (Tan and Patoary, 2004). Anchorage of FRP composite material to the masonry itself and to the reinforced concrete frame in the case of an in-ﬁll wall remains a challenge. Early experimental work on strengthening of masonry walls was conducted by Schwegler at EMPA (Schwegler, 1994) and by Priestley and Seible at UCSD (Priestley and Seible, 1995). Strengthening of timber structures, primarily glulam (glue-laminated) beams, with FRP strips and manufacturing of glulam beams containing FRP layers to increase strength at the outer ﬁbers has been used since the early 1990s. In the United States, early research and commercialization of the method was performed by Tingley (Tingley et al., 1997). Strengthening systems are designed on a case-by-case basis according to standard mechanics principles and bonded adhesively to the timber member. Mechanical fasteners such as lag bolts are often used also. Due to moisture in the wood, the choice of adhesive is critical, and differential thermal and moisture expansion between the FRP layers and the wood lamina can cause signiﬁcant problems. At this time, code guidance is not available for FRP-strengthened timber structures. Retroﬁtting of metallic structures has recently attracted some interest in the structural engineering community. In most cases the steel or aluminum structure is sufﬁciently stiff and strong. The FRP composite is generally used to increase fatigue resistance and to arrest cracks. In the United States, FRP composite wraps have been used successfully to repair fatigue damage on overhead aluminum sign support bridges (Pantelides et al., 2003). In this

1.7

PROPERTIES OF FRP PRODUCTS

25

particular application, the FRP strengthening system is preferable to in situ welding, which is difﬁcult and time consuming. FRP composite products have been used for many years for luminaire poles and in electric power-line towers and components. Code guidance is provided by AASHTO (2001) for designing luminaire supports and sign bridge structures using FRP structural members. A recent manual published by ASCE addresses the use of FRP products in overhead utility line structures (ASCE, 2003). FRP products have also been used extensively in ladders and cooling towers, and standards and speciﬁcations for these specialized applications can be useful to the structural engineer (ANSI, 2000; CTI, 2003). The use of mechanical fasteners instead of adhesive bonding as a method to attach FRP strips to concrete beams has been studied in recent years (Lamanna et al., 2001, 2004; Rizzo et al., 2005). Mechanical fastening has advantages that include very little surface preparation, rapid installation, lower costs, and immediate use of the strengthened structure. The method requires special FRP strips that have high bearing strength and longitudinal stiffness, and it cannot be used with conventional unidirectional carbon–epoxy FRP strips. 1.7 PROPERTIES OF FRP PRODUCTS FOR STRUCTURAL ENGINEERING DESIGN To design a load-bearing structure, a structural engineer must have both qualitative and quantitative knowledge of the properties of the materials that are used in the design. Qualitative knowledge of the material properties is required to understand which of the physical and mechanical properties of the FRP composite material are important for structural design and why they are important. Quantitative knowledge of the material properties is required so that analysis can be performed to predict the behavior and capacity of structural members and structures that are wholly or partially made of FRP composite materials in order to size them appropriately to meet both strength and serviceability demands. For conventional structural materials such as steel, concrete, and timber, existing design codes and speciﬁcations prescribe both speciﬁc material properties and standardized tests method to be used to obtain the properties for design. For example, in the case of reinforced concrete, standard cylinders are tested in accordance with ASTM C 39, Standard Test Method for Compressive Strength of Cylindrical Concrete Specimens. In addition, standard speciﬁcations published by the ASTM specify the properties of the constituent materials of the concrete (cements, aggregates, and admixtures) and of the steel reinforcing bars (ASTM, 2006). With a quantitative knowledge of the properties of the concrete and the steel reinforcing bars, a structural engineer can design a structural member to carry code-stipulated design loads safely and economically according to ACI 318, Building Code Requirements for

26

INTRODUCTION

Structural Concrete (ACI, 2005). With a qualitative knowledge of the properties of concrete and steel reinforcing bars, a structural engineer can decide on such matters as whether or not to use certain admixtures in the concrete mix and whether or not to specify epoxy-coated reinforcing bars rather than uncoated bars. Guide speciﬁcations and test methods for the use of FRP composites in structural engineering have been developed for the three design topics covered in this book: FRP reinforcing bars, FRP strengthening systems, and FRP proﬁles. These speciﬁcations are not as developed or as mature as those that have been developed for conventional materials over approximately the past 100 years. Nevertheless, suitable material speciﬁcations do exist and can be used for structural engineering design, as is demonstrated in the design chapters that follow. The perceived lack of standard material speciﬁcations and test methods for FRP composite materials in structural engineering, often given as a reason for not using FRP products, is no longer a convincing reason for not specifying FRP composites for use in structural engineering. The primary theoretical and experimental methods used to predict and measure the characteristic values of the properties of FRP composite materials for use in structural engineering are provided in Chapter 3. Many excellent textbooks on the mechanics of laminated composite materials and experimental characterization of composite materials are available that cover this subject in great detail (Tsai and Hahn, 1980; Agarwal and Broutman, 1990; Daniel and Ishai, 1994; Adams et al., 2003). These books are focused primarily on advanced composites for aerospace applications. Typically, the characteristic value of a material property is obtained from tests on a speciﬁed number of samples of the material. In this section we do not discuss how a speciﬁc property to be used in an analytical equation in a code-based design procedure to design a structural member, such as the speciﬁed compressive strength, is derived from the characteristic value of the property. The determination of a property that is used in a design procedure is described in later chapters, where the design of particular FRP structural members is discussed. The determination of the design property depends on the design basis used, such as the load and resistance factor design (LRFD) or the allowable stress design (ASD) basis. To determine the design value of a material property, a structural engineer needs to know how the characteristic value was obtained. The characteristic properties of FRP composite materials for use in structural engineering design are usually obtained by experimental testing of FRP materials and products. Pertinent experimental test methods are reviewed in Chapter 3. The FRP composite properties may be determined experimentally on one of four levels: (1) ﬁber level (e.g., a single ﬁber in a ply of the ﬂange of a wide-ﬂange proﬁle); (2) lamina level [e.g., one ply (or layer) of the ﬂange of a wide-ﬂange proﬁle]; (3) laminate level (e.g., a ﬂange of a wide-ﬂange proﬁle); and (4) full-section level (e.g., a wide-ﬂange proﬁle). The approximate ranges of the cross-sectional dimensions of the four levels, from smallest to largest, are: ﬁber level, less than 0.0004 in. (25 m); lamina level, from

1.7

PROPERTIES OF FRP PRODUCTS

27

0.0004 to 0.04 in. (25 m to 1 mm); laminate level, from 0.04 to 0.5 in. (1 mm to 1.3 cm); full-section level, greater than 0.5 in. (1.3 cm). In some cases, the FRP product in its entirety (e.g., an FRP strengthening strip) is at the lamina or laminate level, and the dimensional ranges given above may not be applicable. In some situations, properties at higher levels can be predicted from the experimentally determined properties at lower levels, using the theoretical models described in Chapter 3. For example, if the properties of a single ply of the FRP composite material are measured in a test (lamina level), theoretical models can be used to predict the properties on the laminate level and then on the full-section level. For structural engineering applications it is generally preferred to determine properties experimentally on the full-section or laminate level of the FRP product and not to rely on theoretical models. However, this is not always possible. A commonly used method in engineering practice to obtain characteristic properties of materials is to use manufacturer-supplied speciﬁcations, often referred to as spec sheets. A structural engineer must know how to interpret the properties reported in manufacturer-published spec sheets for FRP products for use in structural engineering. At this time there is no uniformity in the manner in which manufacturers report their property data, and this can lead to confusion. A manufacturer will often report properties on a number of different levels for a single FRP product, and the structural engineer will need to develop the design properties from a mixed set of properties. In the design-oriented chapters that follow, speciﬁc design examples are provided in which manufacturer-published data are used. Ranges of mechanical and physical properties of representative FRP products for use in structural engineering are provided below for the reader to get a feel for the order of magnitude of the values available. As noted in the historical review, the manufacturers of FRP products for use in structural engineering have tended to change over the years, and the products listed are representative of those in production in 2006. It is important to note that the properties listed below, taken from manufacturer-published speciﬁcation sheets, are not the maximum possible values for these FRP materials, nor do they necessarily correspond to the values from a speciﬁc test of a single FRP composite product. Neither are they design values or characteristic values. In the chapters on design procedures that follow, the calculation of design values from characteristic values obtained from speciﬁed numbers of tests is discussed in greater detail in the context of the design basis for a particular FRP product. In Tables 1.1 to 1.5, typical properties of FRP composites of interest to the structural designer are listed. Since FRP composite products are anisotropic, properties are reported for the longitudinal direction, the transverse direction, and the shear planes separately, where available.8

8 The reader should consult Chapter 3 for details on the mechanics of anisotropic composite materials and the effects of this anisotropy on the engineering properties.

28

Source: 1 Aslan (Hughes Brothers); 2 V-rod (Pultrall); 3 Leadline (Mitsubishi). a Estimated b NR, not reported by manufacturers.

Barcol hardness 24-hr water absorption (% max.) Density [lb / in3 (g / cm3)]

CTE, transverse [10⫺6 ⬚F⫺1 (10⫺6 ⬚C⫺1)]

Compressive modulus, longitudinal [Msi (GPa)] CTE, longitudinal [10⫺6 ⬚F⫺1 (10⫺6 ⬚C⫺1)]

Tensile modulus, longitudinal [Msi (GPa)]

Bond strength [ksi (MPa)]

Compressive strength, longitudinal [ksi (MPa)] Shear strength, out-of-plane [ksi (MPa)]

50–60 Unidirectional 90–100 (620–690) NRb 22–27 (152–186) 1.7 (12) 5.9–6.1 (41–42) NR 3.7–4.9 (6.7–8.8) 12.2–18.7 (22.0–33.7) 60 NR 0.072 (2.1)

Glass-Reinf. Vinylester Bar1,2 [0.5 in. (13 mm) diam.] 50–60 Unidirectional 80 (552) NR 22 (152) 1.7 (12) 5.9 (41) NR 3.7 (6.7) 18.7 (33.7) 60 NR 0.072 (2.1)

Glass-Reinf. Vinylester Bar1 [1 in. (25 mm) diam.]

Properties of Typical Commercially Produced FRP Reinforcing Bars

Fiber volumea Fiber architecture Tensile strength, longitudinal [ksi (MPa)]

TABLE 1.1

1.3 (9) 18 (124) NR ⫺4.0–0 (⫺7.2–0) 41–58 (73.8–104.4) 48–55 NR NR

50–60 Unidirectional 300 (2070) NR NR

Carbon-Reinf. Vinylester1 Bar [0.5 in. (13 mm) diam.]

NR NR 0.058 (1.6)

21 (145) NR 0.38 (0.7) NR

NR

50–60 Unidirectional 327 (2255) NR NR

Carbon-Reinf. Epoxy Bar 3 [0.5 in. (13 mm) diam.]

29

4

NR

NR

65–70 Unidirectional 0.047 (1.2) 2–4 (50–100) 188 (1290) NRc 43.5 (300) NR

High-Modulus Carbon-Reinf. Epoxy Strip1

Source: Carbodur (Sika); Tyfo (Fyfe); Mbrace (Wabo / S&P); Aslan (Hughes Brothers). a All strips must be bonded with manufacturer-supplied compatible adhesives. b Estimated. c NR, not reported by manufacturers.

3

NR

2

Barcol hardness

1

NR

CTE transverse [10⫺6 ⬚F⫺1 (10⫺6 ⬚C⫺1)]

CTE longitudinal [10⫺6 ⬚F⫺1 (10⫺6 ⬚C⫺1)]

Tensile strain (max.), longitudinal (%) Tensile modulus, longitudinal [Msi (GPa)]

Tensile strength, longitudinal [ksi (MPa)]

Width [in. (mm)]

65–70 Unidirectional 0.047–0.075 (1.2–1.9) 2–4 (50–100) 390–406 (2690–2800) 1.8 22.5–23.9 (155–165) NR

Standard Modulus Carbon-Reinf. Epoxy Strip1–3

Properties of Typical Commercially Produced FRP Strengthening Stripsa

Fiber volumeb Fiber architecture Nominal thickness [in. (mm)]

TABLE 1.2

NR

NR

65–70 Unidirectional 0.055–0.075 (1.4–1.9) 2–4 (50–100) 130 (900) 2.2 6.0 (41) NR

Glass-Reinf. Epoxy Strip2

60 Unidirectional 0.079 (2.0) 0.63 (16) 300 (2070) 1.7 19.0 (131) ⫺4.0–0.0 (⫺7.2–0) 41–58 (73.8–104.4) 48–55

Carbon-Reinf. Vinylester Strip4

30

Source: 1 MBrace (Wabo); 2 Tyfo (Fyfe); 3 Replark (Mitsubishi); 4 SikaWrap (Sika). a All dry ﬁber sheet must be used with manufacturer-supplied compatible polymer resins. b NR, not reported by manufacturers.

Fiber tensile strain (max.), longitudinal (%) Fiber tensile modulus, longitudinal [Msi (GPa)]

Typ. width [in. (mm)] Fiber architecture Fiber tensile strength, longitudinal [ksi (MPa)]

0.0065–0.013 (0.165–0.330) 24 (600) Unidirectional 550 (3790) 1.67–1.7 33.0 (230)

Standard Modulus Carbon Fiber Tow Sheet1–3 0.0065 (0.165) 24 (600) Unidirectional 510 (3520) 0.94 54.0 (370)

High-Modulus Carbon Fiber Tow Sheet1,2

0.014 (0.356) 48 (1200) Unidirectional 220–470 (1520–3240) 2.1–4.5 10.5 (72)

Glass Fiber Unidirectional Fabric1,2

Properties of Typical Commercially Produced FRP Sheet and Fabric Strengthening Materialsa

Thickness [in. (mm)]

TABLE 1.3

NR Various 508 (3500) 1.7 33.0 (230)

NRb

Carbon Fiber Multiaxial Fabric2,4

31

Bearing Longitudinal Transverse

Flexural Longitudinal Transverse

Shear In-plane Out-of-plane

Compressive Longitudinal Transverse

Tensile Longitudinal Transverse

30–46 (207–317) 7–12 (48–83) 30–52 (207–359) 16–20 (110–138) 4.5–7 (31–48) 3.9–4.5 (27–31) 30–49 (207–338) 10–19 (69–131) 30–39 (207–269) 26–34 (179–234)

25–40 Roving and mat

Glass-Reinf. Vinylester Shapes (WF)1,2 [0.25–0.5 in. (6–13 mm) thick]

6 (41) 30–35 (207–241) 15–18 (103–124) 32 (221) 32 (221)

20 (138) 10 (69) 24 (165) 16 (110) NR

Strength [ksi (MPa)]

20–35 Roving and mat

Glass-Reinf. Vinylester Flat Sheet1,2 [–38 –1 in. (9–25 mm) thick]

NR NR

NR

NR

NR

NR

NR

NR

NR

406 (2800) NR

65 Tow only

Carbon-Reinf. Epoxy Strips3 [0.047 in. (1.2 mm) thick]

NR

8 (55) 100 (690) NR

NR

65 (448) NR

100 (690) NRb

50–60 Roving only

Glass-Reinf. Vinylester Rods1,2 [0.25–1 in. (6–25 mm) diam.]

Mechanical Properties of Typical Commercially Produced FRP Pultruded Materials

Fiber volumea Fiber architecture

TABLE 1.4

32

(Continued )

2

3

2.6–4.1 (18–28) 0.8–1.4 (6–10) 2.6–3.8 (18–26) 1.0–1.9 (7–13) 0.43–0.50 (3.0–3.4) 1.6–2.0 (11–14) 0.8–1.7 (6–12) 0.33–0.35

Glass-Reinf. Vinylester Shapes (WF)1,2 [0.25–0.5 in. (6–13 mm) thick]

Glass-Reinf. Vinylester Flat Sheet1,2 [–38 –1 in. (9–25 mm) thick]

2.0 (14) 1.1–1.4 (7.6–9.7) 0.32

1.8 (12) 1.4 (10) 1.8 (12) 1.0 (7) NR

Modulus [Msi (GPa)]

Source: Strongwell (2002); Creative Pultrusions (2000); Sika (2000). a Estimated. b NR, not reported by manufacturers.

1

Poisson ratio, longitudinal

Flexural Longitudinal Transverse

Shear, in-plane

Compressive Longitudinal Transverse

Tensile Longitudinal Transverse

TABLE 1.4

NR

6.0 (41) NR

NR

NR

NR

NR

NR

NR NR

NR

23.9 (165) NR

Carbon-Reinf. Epoxy Strips3 [0.047 in. (1.2 mm) thick]

NR

6.0 (41) NR

Glass-Reinf. Vinylester Rods1,2 [0.25–1 in. (6–25 mm) diam.]

33

Source: 1 Strongwell (2002); 2 Creative Pultrusions (2000); 3 Sika (2000). a Estimated. b NR, not reported by manufacturers.

Density [lb / in3 (g / cm3)]

CTE, transverse [10⫺6 ⬚F⫺1 (10⫺6 ⬚C⫺1) Barcol hardness 24-hr water absorption (% max.) Dielectric strength, longitudinal [kV / in. (V / mm)]

25–40 Roving and mat 4.4 (7.9) NR 45 0.6 35–40 (1380–1580) 0.060–0.070 (1.7–1.9)

Glass-Reinf. Vinylester Shapes (WF)1,2 [0.25–0.5 in. (6–13 mm) thick] 20–25 Roving and mat 8.0 (14.4) NR 40 0.6 35–40 (1380–1580) 0.060–0.070 (1.7–1.9)

Glass-Reinf. Vinylester Flat Sheet1,2 [–38 –1 in. (9–25 mm) thick] 50–60 Roving only 3.0 (5.4) NR 50–55 0.25 60 (2360) 0.072–0.076 (2.0–2.1)

Glass-Reinf. Vinylester Rods1,2 [0.25–1 in. (6–25 mm) diam.]

Physical and Electrical Properties of Typical Commercially Produced FRP Pultruded Materials

Fiber volumea Fiber architecture CTE, longitudinal [10⫺6 ⬚F⫺1 (10⫺6 ⬚C⫺1)

TABLE 1.5

NR

NR NR NR NR

65 Tow only NRb

Carbon-Reinf. Epoxy Strips3 [0.047 in. (1.2 mm) thick]

34

INTRODUCTION

1.8 PUBLISHED DESIGN GUIDES, CODES, AND SPECIFICATIONS FOR FRP COMPOSITES IN STRUCTURAL ENGINEERING In recent years a signiﬁcant number of design guides, codes, and speciﬁcations have been published by technical organizations that give extensive guidance to structural engineers for design with FRP materials. Much of the seminal research conducted in the last 10–15 years on the subject of FRP composites for construction was published in a select number of conference proceedings and journals. The key publications are listed below.

1.8.1

FRP Reinforcing Bars and Tendons

ACI (2004), Prestressing Concrete Structures with FRP Tendons, ACI 440.4R-04, American Concrete Institute, Farmington Hills, MI. ACI (2006), Guide for the Design and Construction of Structural Concrete Reinforced with FRP Bars, ACI 440.1R-06, American Concrete Institute, Farmington Hills, MI. BRI (1995), Guidelines for Structural Design of FRP Reinforced Concrete Building Structures, Building Research Institute, Tsukuba, Japan. See also Design guidelines of FRP reinforced concrete building structures, Journal of Composites for Construction, Vol. 1, No. 3, pp. 90–115, 1997. CSA (2000), Canadian Highway Bridge Design Code, CSA-06-00, Canadian Standards Association, Toronto, Ontario, Canada. CSA (2002), Design and Construction of Building Components with Fibre-Reinforced Polymers, CSA-S806-02, Canadian Standards Association International, Toronto, Ontario, Canada. JSCE (1997), Recommendation for Design and Construction of Concrete Structures Using Continuous Fiber Reinforcing Materials, Concrete Engineering Series 23, Japan Society of Civil Engineers, Tokyo.

1.8.2

FRP Strengthening Systems

AC 125 (1997), Acceptance Criteria for Concrete and Reinforced and Unreinforced Masonry Strengthening Using Fiber-Reinforced Polymer (FFP) Composite Systems, ICC Evaluation Service, Whittier, CA. AC 187 (2001), Acceptance Criteria for Inspection and Veriﬁcation of Concrete and Reinforced and Unreinforced Masonry Strengthening Using Fiber-Reinforced Polymer (FFP) Composite Systems, ICC Evaluation Service, Whittier, CA. ACI (2002), Guide for the Design and Construction of Externally Bonded FRP Systems for Strengthening Concrete Structures, ACI 440.2R-02, American Concrete Institute, Farmington Hills, MI. FIB (2001), Externally Bonded FRP Reinforcement for RC Structures, International Federation for Structural Concrete, Lausanne, Switzerland.

1.8

PUBLISHED DESIGN GUIDES, CODES, AND SPECIFICATIONS

35

JSCE (2001), Recommendation for Upgrading of Concrete Structures with Use of Continuous Fiber Sheets, Concrete Engineering Series 41, Japan Society of Civil Engineers, Tokyo. TR 55 (2004), Design Guidance for Strengthening Concrete Structures Using Fibre Composite Materials, The Concrete Society, Camberley, Surrey, England. TR 57 (2003), Strengthening Concrete Structures with Fibre Composite Materials: Acceptance, Inspection and Monitoring, The Concrete Society, Camberley, Surrey, England.

1.8.3

FRP Pultruded Proﬁles

ASCE (1984), Structural Plastics Design Manual, ASCE Manuals and Reports on Engineering Practice 63, American Society of Civil Engineers, Reston, VA. CEN (2002), Reinforced Plastic Composites: Speciﬁcations for Pultruded Proﬁles, Parts 1–3, EN 13706, Comite´ Europe´en de Normalisation, Brussels, Belgium. Eurocomp (1996), Structural Design of Polymer Composites: EUROCOMP Design Code and Handbook, Clark, J. L. (ed.) E&FN Spon, London.

1.8.4

Manufacturers’ Design Manuals

In addition to the association- or standards organization-developed design manuals listed above, manufacturers of FRP products for structural engineering applications also provide design guidance. In some cases, the association design guides have been developed from early versions of manufacturers’ guides. FRP Strengthening Systems MBrace (1998), MBrace Composite Strengthening System: Engineering Design Guidelines, Master Builders, OH. Current edition at www.mbrace.com. Replark (1999), Replark System: Technical Manual, Mitsubishi Chemical Corporation, Sumitomo Corporation of America, New York. Current edition at www. sumitomocorp.com. Sika (1997), Sika Carbodur: Engineering Guidelines for the Use of Sika Carbodur (CFRP) Laminates for Structural Strengthening of Concrete Structures, Sika Corporation, Lyndhurst, NJ. Current edition at www.sikaconstruction.com /. S&P (1998), Clever Reinforcement Company, Schere & Partners, Brunnen, Switzerland. Current edition at www.sp-reinforcement.ch. Tonen (1996), Forca Towsheet Technical Manual, Rev. 5.0, Tonen Corporation, Tokyo. Tyfo (1998), Design Manual for the Tyfo Fibrwrap System, Fyfe Co. LLC, San Diego, CA. Current edition at www.fyfeco.com.

FRP Pultruded Proﬁles Bedford Reinforced Plastics Design Guide (2005), Bedford Plastics, Bedford, PA. Current edition at www.bedfordplastics.com.

36

INTRODUCTION

Extren Design Manual (2002), Strongwell, Bristol, VA. Current edition at www. strongwell.com. The Fiberline Design Manual (2003), Fiberline Composites, Kolding, Denmark. Current edition at www.ﬁberline.com. The Pultex Pultrusion Global Design Manual (2004), Creative Pultrusions, Alum Bank, PA. Current edition at www.pultrude.com.

1.8.5

Key Conferences Series

FRPRCS (Fiber Reinforced Composites in Reinforced Concrete Structures) Series 1993 1995 1997 1999 2001 2003 2005

Vancouver, British Columbia, Canada, ACI Ghent, Belguim, RILEM Sapporo, Japan, JSCE Baltimore, Maryland, ACI Cambridge, UK, E&F Spon Singapore, New World Publishers Kansas City, Missouri, ACI

ACMBS (Advanced Composite Materials in Bridges and Structures) Series

1992 1996 2000 2004

Sherbrooke, Quebec, Canada, CSCE Montreal, Quebec, Canada, CSCE Ottowa, Ontario, Canada, CSCE Calgary, Alberta, Canada, CSCE

ASCE Materials Congress Series 1990 1991 1992 1994 1999

Denver, Colorado, ASCE Las Vegas, Nevada, FRP Specialty Conference, ASCE Atlanta, Georgia, ASCE San Diego, California, ASCE Cincinnati, Ohio, ASCE

ICCI (International Conference for Composites for the Infrastructure) Series 1996 1998 2002

Tucson, Arizona Tucson, Arizona San Francisco, California

PROBLEMS

37

CICE (Composites in Civil Engineering) Series 2001 2004 2006

Hong Kong, China Adelaide, Australia Miami, Florida

ACIC (Advanced Polymer Composites for Structural Applications in Construction) Series 2002 2004 2007 1.8.6

Southhampton, UK Surrey, UK Bath, UK

Archival Journals

The major international English language journals that have published and continue to publish key technical papers on the topic of FRP composites in structural engineering are: Composite Structures, Elsevier Construction and Building Materials, Elsevier Journal of Composites for Construction, ASCE Structural Journal, ACI PROBLEMS 1.1 Find information about the FRP composite structures and FRP-related organizations and publications listed below. For each item, provide a short written description of the product or application, a Web page link, and a picture of relevance. Aberfeldy Bridge, Scotland American Composites Manufacturers Association (ACMA) Committee 440, American Concrete Institute (ACI) Committee AC207, Transportation Research Board (TRB) Composites Bridge Alliance Europe (COBRAE) Composites Technology EMPA, Switzerland European Pultrusion Technology Association (EPTA) Eyecatcher building, Switzerland High Performance Composites

38

INTRODUCTION

International Institute for FRP in Construction (IIFC) ISIS Canada Journal of Composites for Construction, ASCE Kolding Bridge, Denmark NetComposites Education Pultrusion Industry Council (PIC) 1.2 Find information about the selected FRP manufacturers listed below and the products they produce for structural engineering applications. For each item, provide a short written description of the company and its product for use in structural engineering applications. Provide an image of the product and a URL. BBR Carbon Fiber Stay Cables: FRP stay cables Bedford Reinforced Plastics: pultruded products Creative Pultrusions: pultruded products Edge Structural Composites: strengthening systems ET Techtonics: pultruded bridges Exel Composites: pultruded products Fibergrate Composite Structures: pultruded products Fiberline Composites: pultruded products Fyfe Co.: strengthening systems Hughes Brothers: FRP reinforcements Lancaster Composites: pilings Marley Cooling Technologies: FRP cooling towers Martin Marietta Composites: FRP bridge decks Mitsubishi Composites: FRP tendons and strengthening systems Paciﬁc Composites: pultruded products Powertrusion Poles: FRP poles Pultrall: FRP reinforcements Quakewrap: strengthening systems Roechling-Haren: pultruded products S&P–Clever Reinforcement Company: strengthening systems Seasafe: FRP grating Shakespeare: FRP poles Sika: strengthening systems Sireg: FRP tendons Strongwell: pultruded products Techfab: FRP reinforcements Tokyo Rope: FRP tendons Topglass Italy: pultruded products

PROBLEMS

39

VSL: strengthening systems Wabo MBrace: strengthening systems 1.3 Visit your library (physically or virtually) and compile a list of all the journals and magazines that publish papers (exclusively or in part) and articles related to ﬁber-reinforced polymer composite materials. Try to determine what the focus of the publication is: for example, material characterization, theoretical mechanics, structural applications, mechanical engineering, aerospace engineering, polymer science, civil engineering.

2 2.1

Materials and Manufacturing OVERVIEW

In much the same way that a structural engineer has a working knowledge of the composition of structural materials such as steel, concrete, and wood and how they are made into products for use in structures, a similar working knowledge of FRP composite materials is needed by the structural engineer. This includes having a qualitative knowledge of the constituent or raw materials and the processing methods used to produce the parts and how these affect the eventual mechanical and physical properties of the FRP part. The intent of this chapter is to provide the structural engineer with sufﬁcient materials background to have a working knowledge of the FRP material that will be speciﬁed in the construction documents of a project. Since, by and large, the same raw materials are used in a number of different manufacturing processes to manufacture FRP composite materials used in structural engineering, a general description of the characteristics and properties of these raw materials is ﬁrst given in this chapter. Glass and carbon ﬁbers are the principal synthetic ﬁber materials used to manufacture FRP products for use in structural engineering, and these ﬁbers are discussed in detail. The polymer resins used most widely in FRP products for structural engineering applications are thermosetting epoxies, polyesters, and vinylesters, and these resins are discussed in detail. Less commonly used ﬁber and resin systems are discussed brieﬂy, as they are not used widely in FRP products for structural engineering at this time. This is followed by a discussion of the manufacturing methods used to produce FRP products or parts from the raw materials. The principal methods used to manufacture FRP composite products used in structural engineering are pultrusion and hand layup. These two processes are by far the most widely used processes for manufacturing FRP composites for structural engineering. Pultrusion is used to manufacture FRP proﬁles, FRP strengthening strips, and FRP reinforcing bars. Hand layup is used to fabricate formed-in-place FRP strengthening sheets, fabrics, and wraps. In addition, at present, detailed codebased design provisions have been developed only for FRP products for structural engineering made by pultrusion and hand layup. Less commonly used methods for FRP products for structural engineering, such as ﬁlament winding and closed molding, are discussed brieﬂy.

40

Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

2.2

2.2

RAW MATERIALS

41

RAW MATERIALS

To produce an FRP composite material, two primary raw material constituents are required, reinforcing ﬁbers and a polymer resin matrix. In this section we review key properties and characteristics of the raw materials used to produce FRP products for structural engineering. We do not provide information on how the raw materials are produced; the reader is referred to the composite materials literature for coverage of this subject (e.g., Schwartz, 1997a,b). However, it is worth noting that all the raw materials are produced at high temperatures in industrialized processes that require highly specialized equipment and control. Analogous to the state of affairs that exists today, where a structural engineer does not typically have extensive knowledge of how portland cement is produced from limestone, a structural engineer is not expected to have extensive knowledge of how polymer resin is produced from crude oil or how glass ﬁber is produced from silica sand. Except in very rare circumstances, the raw ﬁber and polymer constituents cannot be used in their as-produced forms to manufacture an FRP composite material. After the ﬁber ﬁlaments are produced, they are postprocessed in a number of secondary operations to produce ﬁber products such as strands, sheets, fabrics, and mats that can be used in a manufacturing process. Similarly, the raw polymer, which is generally referred to as the base polymer or neat resin, is often blended with other resins and mixed with a variety of additives and process aids to produce a resin system (or resin mix) for manufacturing. The ﬁber and resin systems are discussed later in the manufacturing sections of this chapter, as they are manufacturing method–dependent. Numerous companies manufacture and distribute both raw and postprocessed raw materials for use in production of FRP composites. The annual Sourcebook (Sourcebook, 2006) provides an extensive list of U.S.-based manufacturers and suppliers. 2.2.1

Reinforcing Fibers

The ﬁber phase of an FRP composite material consists of thousands of individual micrometer-diameter individual ﬁlaments. In the large majority of ﬁber forms used in FRP products for structural engineering, these ﬁbers are indeﬁnitely long and are called continuous. This is to differentiate them from short ﬁbers of length 10 to 50 mm (⬃0.5 to 2 in.) that are used in the spray-up process for boat building and consumer products or in reinforced cementitious materials [known as glass-reinforced cements (GRCs) or ﬁberreinforced cementitous (FRC) composites]. Continuous ﬁbers are used at a relatively high volume percentage (from 20 to 60%) to reinforce the polymer resin: thus the term ﬁber-reinforced polymer (FRP). The mechanical properties of the ﬁbers are typically orders of magnitude greater than those of the polymer resins that they reinforce; however, due to their ﬁlamentary nature

42

MATERIALS AND MANUFACTURING

they cannot be used as stand-alone construction materials and must be used in a synergistic fashion with polymer resins to realize their superior mechanical properties. Glass Fibers Glass ﬁbers are used in a multitude of FRP products for structural engineering, from FRP reinforcing bars for concrete, to FRP strengthening fabrics, to FRP structural proﬁle shapes. Glass is an amorphous inorganic compound of primarily metallic oxides that is produced in ﬁbrous form in a number of standard formulations or types. Silica dioxide (SiO2) is the largest single compound in all glass formulations, constituting from 50 to 70% by weight of the glass. Different grades of glass ﬁber are identiﬁed by letter nomenclature. A borosilicate glass known as E-glass (electrical glass) because of its high electrical resistivity is used to produce the vast majority of glass ﬁber used in FRP products for structural engineering. A-glass (window glass) and C-glass (corrosion resistant, also know as AR-glass or alkaliresistant glass) are used to produce specialized products for use in structural engineering. S-glass (structural or high-strength glass) is used to produce the high-performance ﬁbers used primarily in the aerospace industry. The diameter of an individual glass ﬁber or ﬁlament ranges from approximately 3 to 24 m (0.00118 to 0.00945 in.).1 The 17-m (0.0067-in.)diameter ﬁber is most commonly used for FRP products for structural engineering. A glass ﬁber has a distinctive bright white color to the naked eye. Glass is usually considered to be an isotropic material. Approximate properties of commonly used grades of glass ﬁbers are given in Table 2.1. Values presented in Table 2.1 are intended as a guide and should not be used in design calculations. Glass ﬁbers are produced at melt temperatures of about 1400⬚C (⬃2550⬚F). Individual ﬁlaments are produced with a surface coating called a sizing that serves to protect the ﬁlaments when they are formed into a bundle or a strand.

TABLE 2.1 Grade of Glass Fiber E A C S

Approximate Properties of Common Grades of Glass Fibers Density [g / cm3 (lb / in3)] 2.57 2.46 2.46 2.47

(0.093) (0.089) (0.089) (0.089)

Tensile Modulus [GPa (Msi)]

Tensile Strength [MPa (ksi)]

72.5 73 74 88

3400 2760 2350 4600

(10.5) (10.6) (10.7) (12.8)

(493) (400) (340) (667)

Max. Elongation (%) 2.5 2.5 2.5 3.0

1 The properties of the ﬁber and resin constituent materials are typically given in metric units by manufacturers. However, in the United States, the properties of the ﬁber products (fabrics and rovings) and the FRP parts are typically given in imperial units.

2.2

RAW MATERIALS

43

The sizing also contains coupling agents, usually silanes, that are specially formulated to enhance bonding between the glass ﬁber and the particular polymer resin being used when making a glass-reinforced FRP composite material. Today, most commercially available glass ﬁbers can be obtained with sizings that are compatible with the three major thermosetting resin systems used in structural engineering: epoxy, polyester, and vinylester. The commonly used term ﬁberglass is generally used to refer to the glass ﬁberreinforced polymer composite material itself and not solely to the glass ﬁber constituent material. When referring to the ﬁbrous reinforcement alone, the term glass ﬁber is preferred. Glass ﬁbers are particularly sensitive to moisture, especially in the presence of salts and elevated alkalinity, and need to be well protected by the resin system used in the FRP part. Glass ﬁbers are also susceptible to creep rupture and lose strength under sustained stresses (Bank et al., 1995b). The endurance limit of glass ﬁbers is generally lower than 60% of the ultimate strength. Glass ﬁbers are excellent thermal and electrical insulators (hence, their extensive use in buildings and the electric power industry as insulation materials) and are the most inexpensive of the high-performance ﬁbers. Carbon Fibers Carbon ﬁbers are used in structural engineering applications today in FRP strengthening sheets and fabrics, in FRP strengthening strips, and in FRP prestressing tendons. Carbon ﬁber is a solid semicrystalline organic material consisting on the atomic level of planar two-dimensional arrays of carbon atoms. The two-dimensional sheetlike array is usually known as the graphitic form; hence, the ﬁbers are also known as graphite ﬁbers (the three-dimensional array is well known as the diamond form). Carbon ﬁber is produced in grades known as standard modulus, intermediate modulus, high strength, and ultrahigh modulus (SM, IM, HS, UHM).2 Carbon ﬁbers have diameters from about 5 to 10 m (0.00197 to 0.00394 in.). Carbon ﬁber has a characteristic charcoal-black color. Due to their twodimensional atomic structure, carbon ﬁbers are considered to be transversely isotropic, having different properties in the longitudinal direction of the atomic array than in the transverse direction. The longitudinal axis of the ﬁber is parallel to the graphitic planes and gives the ﬁber its high longitudinal modulus and strength. Approximate properties of common grades of carbon ﬁbers are given in Table 2.2. Carbon ﬁber is produced at high temperatures [1200 to 2400⬚C (⬃2200 to 4300⬚F)] from three possible precursor materials: a natural cellulosic rayon textile ﬁber, a synthetic polyacrilonitrile (PAN) textile ﬁber, or pitch (coal tar). Pitch-based ﬁbers, produced as a by-product of petroleum processing, are generally lower cost than PAN- and rayon-based ﬁbers. As the temperature

2 Carbon ﬁbers are generally identiﬁed by their speciﬁc trade names. The properties of a carbon ﬁber produced by different manufacturers, even similar grades, can vary widely.

44

MATERIALS AND MANUFACTURING

TABLE 2.2

Approximate Properties of Common Grades of Carbon Fibers

Grade of Carbon Fiber Standard High strength High modulus Ultrahigh modulus

Density [g / cm3 (lb / in3)] 1.7 1.8 1.9 2.1

(0.061) (0.065) (0.068) (0.076)

Tensile Modulus [GPa (Msi)]

Tensile Strength [MPa (ksi)]

250 250 500 800

3700 4800 3000 2400

(36.3) (36.3) (72.5) (116.0)

(537) (696) (435) (348)

Max. Elongation (%) 1.2 1.4 0.5 0.2

of the heat treatment increases during production of the carbon ﬁber, the atomic structure develops more of the sheetlike planar graphitic array, giving the ﬁber higher and higher longitudinal modulus. For this reason, early carbon ﬁbers were also known as graphite ﬁbers. The term carbon ﬁber is used to describe all carbon ﬁbers used in structural engineering applications. The term graphite ﬁber is still used in the aerospace industry; however, this term is slowly dying out. Similar to glass ﬁbers, carbon ﬁbers need to be sized to be compatible with a resin system. Historically, carbon ﬁbers have been used primarily with epoxy resins, and suitable sizings for epoxy resin systems are readily available. Nowadays, carbon ﬁbers are being used with vinylester and blended vinylester–polyester resins for FRP proﬁles and FRP strengthening strips. Sizing for carbon ﬁbers for polyester and vinylester resins are not as common. Care must be taken when specifying a carbon ﬁber for use with a nonepoxy resin system to ensure that the ﬁber is properly sized for the resin system used. Carbon ﬁbers are very durable and perform very well in hot and moist environments and when subjected to fatigue loads. They do not absorb moisture. They have a negative or very low coefﬁcient of thermal expansion in their longitudinal direction, giving them excellent dimensional stability. They are, however, thermally and electrically conductive. Care must be taken when they are used in contact with metallic materials, as a galvanic cell can develop due to the electropotential mismatch between the carbon ﬁber and most metallic materials. Some research has suggested that this can lead to degradation of the polymer resin in the FRP composite, especially in the presence of chlorides and to corrosion of the metallic material (Alias and Brown, 1992; Torres-Acosta, 2002). Aramid Fibers Aramid ﬁbers were used to produce ﬁrst-generation FRP prestressing tendons in the 1980s in Europe and Japan; however, few manufacturers still produce aramid ﬁber FRP reinforcing bars or tendons. Aramid fabrics are occasionally used in FRP strengthening applications to wrap columns and as sparse-volume weft (ﬁll) ﬁbers in unidirectional glass or carbon fabrics for FRP strengthening. Aramid ﬁbers consist of aromatic polyamide molecular chains. They were ﬁrst developed, and patented, by DuPont in 1965 under the trade name Kevlar.

2.2

RAW MATERIALS

45

A combination of their relatively high price, difﬁculty in processing, high moisture absorption (up to 6% by weight), low melting temperatures [around 425⬚C (⬃800⬚F)], and relatively poor compressive properties have made them less attractive for FRP parts for structural engineering applications. Their advantages include extremely high tenacity and toughness, and consequently, they are used in many industrial products, either in bare fabric form or as reinforcements for FRP composites where energy absorption is required, such as in bulletproof vests (body armor), helmets, and automotive crash attenuators. They have a distinctive yellow color and are similar in cost to carbon ﬁbers. Like carbon ﬁbers, they have a negative coefﬁcient of thermal expansion in the ﬁber longitudinal direction. They are the lightest of the highperformance ﬁbers, having a density of around 1.4 g/cm3 (0.051 lb/in3). Depending on the type of aramid ﬁber, the ﬁber longitudinal tensile strength ranges from 3400 to 4100 MPa (⬃500 to 600 ksi), and its longitudinal tensile modulus ranges from 70 to 125 GPa (⬃10,000 to 18,000 ksi). Other Fibers Other ﬁbers that are now in the development phase for use in FRP products for structural engineering include thermoplastic ultrahighmolecular-weight (UHMW) polyethylene ﬁbers and polyvinyl alcohol (PVA) ﬁbers. PVA ﬁbers have been used in FRP bars and FRP strengthening sheets in Japan. UHMW short ﬁbers are being used in the development of ductile ﬁber-reinforced cements (FRCs) but have not yet been used in FRP products for structural engineering. Inorganic basalt ﬁbers, produced in Russia and the Ukraine, may see future applications in FRP products in structural engineering, due to their superior corrosion resistance and similar mechanical properties to glass ﬁbers. Thin steel wires have been developed for use in FRP strengthening fabrics with either polymer or cementitious binders. Natural ﬁbers such as hemp, sisal, and ﬂax, as well as bamboo ﬁbers, have been used in experimental applications to produce FRP composites, but no commercial FRP products are available that contain these ﬁbers at this time. It is anticipated that FRP products in structural engineering that will be developed in the ﬁrst half of the twenty-ﬁrst century will probably use more of these natural ﬁbers as sustainability and recyclability become more important drivers in the construction industry. 2.2.2

Polymer Resins

The term polymer is used to describe an array of extremely large molecules, called macromolecules, that consist of repeating units, or chains, in which the atoms are held together by covalent bonds. The term polymer is generally used to describe an organic material of this type; however, it can also be used to describe an inorganic material. The term polymer resin, or simply resin, is used in the composites industry to refer to the primary polymer ingredient in the nonﬁbrous part of the FRP material that binds the ﬁbers together. This nonﬁbrous part is also known as the matrix or binder. When used in commercial and industrial products a polymer-based material is often known as

46

MATERIALS AND MANUFACTURING

a plastic and the acronym FRP is also often used to denote a ﬁber-reinforced plastic. The acronym RP is often used to connote a reinforced plastic, although this is mostly used to describe short-ﬁber-reinforced plastic products of lower strength and stiffness. The differences between organic polymers depend on the functional groups present in the polymer chains and the extent of the interaction between these chains. Chains, which have a molecular backbone, may be linear or branched. (Seymour, 1987). Two primary groups of polymers exist today, thermosetting polymers and thermoplastic polymers. They are distinguished from one another by how the polymer chains are connected when the polymer is in its solid form. Thermosetting polymers are cross-linked, which means that their molecular chains are joined to form a continuous three-dimensional network by strong covalently bonded atoms. Thermoplastic polymers are not crosslinked, and their molecular chains are held together by weak van der Waals forces or by hydrogen bonds (Schwartz, 1997b). This affects their mechanical and physical properties. Due to cross-linking, a thermosetting polymer’s structure is set when it solidiﬁes or cures during the polymerization process, and it cannot be heated and softened and then re-formed into a different shape. On the other hand, a thermoplastic polymer does not set but remains plastic, and the molecular chains can ‘‘ﬂow’’ when the solid polymer is heated such that it softens and can be reset into a different shape upon cooling. Synthetic organic polymers are produced by polymerization techniques, either chain (or additional) polymerization or step (or condensation) polymerization. Most high-performance polymers are produced by condensation of difunctional reactants. The best known chain polymerization reaction is freeradical polymerization, in which an electron-deﬁcient molecule (or free radical) is initially added to a monomer, forming a new, larger free radical. The chain reaction continues until the reactive constituents are expended. The thermal response of polymers plays a large role in their processing, properties, and behavior. Pure crystalline solids such as metals undergo a phase change from solid to liquid at a transition temperature, called the melting point, Tm. This is the only thermal transition possible in a pure crystalline solid. Since polymers are semicrystalline solids that contain noncrystalline amorphous regions, other thermal transitions occur at lower temperatures than Tm. A thermal transition of particular interest to structural engineering, known as the glass transition temperature, Tg, occurs in the amorphous region of the polymer at a temperature below the melting temperature. At the Tg the physical (density, heat capacity) and mechanical (stiffness, damping) properties of the polymer undergo a change. When the temperature approaches Tg from below, the polymer changes from a rigid (known as glassy) to a viscous (known as rubbery) state, and vice versa, when the temperature approaches from above Tg.3 The glass transition temperature may be referred to as the 3

Note that the term glass transition temperature is not related to the glass ﬁber used to reinforce many FRPs. The term comes from the materials terminology that is used to distinguish between glassy or rubbery materials. A carbon ﬁber–reinforced polymer composite has a glass transition temperature.

2.2

RAW MATERIALS

47

heat distortion temperature or heat deﬂection temperature in polymer manufacturers’ literature. Although not precisely the same property, these three transition temperatures are usually close in value (within 10⬚C) and are used interchangeably in the industry to describe roughly the same physical phenomenon. Both thermosetting and thermoplastic polymers have glass transition temperatures. A thermoplastic polymer liqueﬁes at its melting temperature, whereas a thermosetting polymer begins to decompose at its melting temperature. Above the melting temperature a thermoplastic or thermosetting polymer will pyrolize in an oxygen-rich atmosphere. In structural engineering, FRP composites must be used in their rigid states at operating temperatures below their glass transition temperatures. At temperatures higher than the glass transition temperature, the modulus of the resin, and hence the FRP composite, decreases. Since deﬂection criteria are used routinely in structural engineering design, an FRP part can become unserviceable at temperatures close to its glass transition temperature. In addition, the FRP part will be less durable and will have lower strength at temperatures above its glass transition temperature. On the other hand, elastomeric polymers like those used in asphalt binders are used above their glass transition temperatures in their viscous state. When these polymers are used below their glass transition temperatures, they become brittle and crack. Polymer resins are good insulators and do not conduct heat or electricity provided that they have low void ratios. Water in the voids of a polymer composite can allow the composite to conduct electricity. For glass-reinforced polymer electric power parts, stringent limits are placed on the void ratio (usually less than 1%). Polymer resins are usually considered to be isotropic viscoeleastic materials. They creep under sustained stresses or loads and relax under constant strains or displacements. Most polymer resins are susceptible to degradation in ultraviolet light (White and Turnbull, 1994). Thermosetting polymer resins are generally not suitable for use at temperatures greater than 180⬚C (⬃350⬚F) and in ﬁres if not protected in a fashion similar to steel structural members. Polymer materials have been shown to have acceptable ﬁre ratings when used in appropriately designed protection systems and ﬁreretarding additives. Thermoplastic polymers have been developed for high temperatures up to 450⬚C (⬃800⬚F). Most liquid polymer resins have a shelf life between 6 and 12 months and should be stored at cool temperatures between 10 and 15⬚C (50 to 60⬚F). Unsaturated Polyester Resin Polyester resin is widely used to make pultruded FRP proﬁles for use in structural engineering and is also used to make some FRP rebars. When greater corrosion resistance is desired in FRP parts, higher-priced vinylester resins are generally recommended, although the corrosion resistance of some polyester resins may be as good as that of vinylester resins. Polyester resins can also be used for FRP strengthening for structures. However, epoxy resins are preferred at this time for FRP strengthening applications because of their adhesive properties, low shrinkage, and environmental durability.

48

MATERIALS AND MANUFACTURING

Unsaturated polyester resin is the most widely used resin system for producing industrial and commercial FRP composite material parts. It is referred to as an unsaturated polymer because the double-covalent bonds in its polymer chains are not saturated with hydrogen atoms. By dissolving the polymer in a reactive dilutent, typically a styrene monomer, an exothermic free-radical polymerization chain reaction takes place. This polymerization reaction occurs only in the presence of a catalyst, usually a peroxide. The reactive styrene is added at concentrations of 20 to 60 parts per hundred (pph) of the total resin mix by weight. Based on the type of acid monomer used in the production of the resin, three types of polyester resin, having increasingly better physical and mechanical properties, are produced: orthophthalic, isophthalic, and teraphthalic polyesters. The ﬁrst unsaturated polyester resin was produced by Ellis and Rust in 1940 (Seymour, 1987). Polyester resins are particularly versatile and can easily be ﬁlled and pigmented. They can be formulated in hundreds of different ways to tailor their properties to different manufacturing processes and end-use environments. In 2004, unsaturated polyester resins cost between $0.60 and $1.00 per pound ($1.32 to $2.2 per kilogram). They have a density between 1.15 and 1.25 g/ cm3 (0.042 and 0.046 lb/in3). Depending on the polyester formulation and on the catalyst used, polyester resins can be cured at room temperatures or at elevated temperatures and can therefore have glass transition temperatures ranging from about 40 to 110⬚C (⬃105 to 230⬚F). Polyester resins usually are clear to greenish in color. Epoxy Resins Epoxy resins are used in many FRP products for structural engineering applications. Most carbon ﬁber–reinforced precured FRP strips for structural strengthening are made with epoxy resins. In addition, epoxy resin adhesives are used to bond precured FRP strips to concrete (and other materials) in the FRP strengthening process. Epoxy resins are also used extensively in FRP strengthening applications, where the epoxy resin is applied to the dry ﬁber sheet or fabric in the ﬁeld and then cured in situ, acting as both the matrix for the FRP composite and as the adhesive to attach the FRP composite to the substrate. When applied to dry ﬁber sheets or fabrics, the epoxy resins are often referred to saturants. Epoxy resins have also been used to manufacture FRP tendons for prestressing concrete and FRP stay cables for bridges. They are not used extensively to produce larger FRP proﬁles, due to their higher costs and the difﬁculty entailed in processing large pultruded FRP parts. An epoxy resin contains one or more epoxide (or oxirane) groups that react with hydroxyl groups. Most common are the reaction products of bisphenol A and epichlorohydrin, called bis A epoxies, or those made from phenol or alkylated phenol and formaldehyde and called novolacs. The resins are cured (or hardened) with amines, acid anhydrides, (Lewis acids) by condensation polymerization and not, like polyesters, by free-radical chain polymerization. The epoxy resin and the curing agent (or hardener) are supplied in two parts

2.2

RAW MATERIALS

49

and are mixed in speciﬁc proportions (usually about 2 to 3 parts to 1 part by weight) just prior to use to cause the curing reaction. The ﬁrst epoxy resin was produced by Schlack in 1939 (Seymour, 1987). Epoxy resins are particularly versatile and can be formulated in a range of properties to serve as matrix materials for FRP composites or to serve as adhesives. The epoxies used as the resins in FRP parts for structural engineering belong to the same family as the more familiar epoxies currently used in a variety of structural engineering applications, such as for concrete crack injection, as anchors for concrete, and for bonding precast concrete elements. Epoxy resins are known to have excellent corrosion resistance and to undergo signiﬁcantly less shrinkage than polyester or vinylester resins when cured. Consequently, they are less prone to cracking under thermal loads. Epoxy resins have been developed for high-temperature applications of 180⬚C (350⬚F) and higher and have been the thermosetting resins of choice in the aerospace industry for the last 50 years. Epoxies based on bisphenol A resins cost about $1.10 per pound ($2.4 per kilogram); those based on the novolac resins cost about $2.00 per pound ($4.4 per kilogram) (2004 costs). The density of epoxy resin is about 1.05 g/cm3 (0.038 lb/in3). Epoxy resins can be cured at room temperature or at high temperature. In many aerospace applications, epoxy resin composites are postcured at elevated temperatures to raise their glass transition temperatures and to improve their physical and mechanical properties. The glass transition temperature of an epoxy is therefore highly formulation and cure temperature–dependent and can range from 40⬚C up to 300⬚C (⬃100 to 570⬚F). Epoxy resins usually are clear to yellowish or amber in color. Vinylester Resins Developed in the last 20 years, vinylester resins have become attractive polymer resins for FRP products for structural engineering due to their good properties, especially their corrosion resistance and their ease of processing (Blankenship et al. 1989). Today, vinylester resins are used to make the majority of FRP rebars sold in the world and are also used widely in FRP pultruded proﬁles. Most manufacturers of pultruded proﬁles make proﬁles of identical shapes in both a polyester and a vinylester resin series. Vinylester resins have also been used to make FRP strengthening strips and FRP rods for near-surface-mounting applications. They are generally replacing polyester resins in FRP products in structural engineering, due to their superior environmental durability in alkaline environments. A vinylester resin is a hybrid of an epoxy and an unsaturated polyester resin and is sometimes referred to as an epoxy vinylester resin or a modiﬁed epoxy resin. It is an unsaturated polymer that is produced from an epoxy and an acrylic ester monomer. When it is dissolved in styrene, it reacts with the styrene monomer in the same way as an unsaturated polyester does and cures by free-radical chain polymerization with a peroxide catalyst. Consequently, it tends to have many of the desirable physical properties of an epoxy resin and many of the desirable processing properties of a polyester resin. The two

50

MATERIALS AND MANUFACTURING

major groups of epoxies used to produce vinylester resins are bisphenol A and novolac epoxies (Starr, 2000). Vinylester resins can be ﬁlled and pigmented. They have densities from 1.05 to 1.10 g/cm3 (0.038 to 0.042 lb/in3) and glass transition temperatures from 40 to 120⬚C (⬃100 to 250⬚F). They can be cured at room temperatures or at elevated temperatures. The cost of vinylester resins range from $1.20 to $1.60 per pound ($2.60 to $3.50 per kilogram) (2004 costs), making them more expensive than general-purpose unsaturated polyester resin. Vinylester resins have a color similar to that of polyester resins, ranging from clear to greenish. Phenolic Resins Phenolic resins are the oldest and most widely used thermosetting resins; however, they have only recently been used for FRP products for structural engineering, due to the difﬁculty of reinforcing them and curing them by condensation polymerization. They were ﬁrst developed by Leo Baekeland in the early 1900s and called Bakelite when ﬁlled with wood ﬂour (Seymour, 1987). Until the 1980s they had to be cured at high temperatures from 150 to 300⬚C (⬃300 to 570⬚F). They are used extensively in the production of plywood and other engineered wood products. They are being introduced into FRP products for structural engineering because they have superior ﬁre resistance, and they char and release water when burned. They can be ﬁlled and reinforced; however, they are difﬁcult to pigment and have a characteristic brownish color. Their costs are similar to that of lowperformance polyesters, about $0.60 per pound ($1.30 per kilogram) (2004 costs). Their density is around 1.50 to 2.0 g/cm3 (0.054 to 0.072 lb/in3). They have glass transition temperatures from 220 to 250⬚C (⬃430 to 480⬚F). At this time they are used in a limited number of FRP products, particularly in walkway gratings for offshore platforms and in FRP strengthening strips for timber structures. Polyurethane Resins Thermosetting polyurethane resins have recently been introduced into the market as structural resins. They were ﬁrst produced in the 1930s by Otto Bayer and consist of long-chain urethane molecules of isocyanate and hydroxyl-containing molecules (polyols). They have been used extensively in their thermoplastic formulation to produce insulation and structural polymer foam materials for decades. Only recently have they been produced in high-density forms that can be used in resin molding and pultrusion operations (Connolly et al., 2005). Polyurethane resins have high toughness and when used with glass ﬁbers produce composites with high transverse tensile and impact strengths. Their cost is approximately the same as that of high-performance vinylester resins. Polyurethane resins do not require styrene to polymerize as do unsaturated polyester and vinylester resins. Other Polymer Resins Thermoplastic resin systems such as polyethylene teraphthalate (PET, a saturated polyester), polypropylene, and nylon have been used in a very limited fashion to produce FRP parts for structural en-

2.3

51

MANUFACTURING METHODS

gineering. Thermoplastic composites based on polyether ether ketone (PEEK), polyphenylene sulﬁde (PPS), and polyimide (PI) thermoplastic resins, as well as many others, are being used extensively in the high-temperature aerospace composites market. The attractiveness of using thermoplastic resin systems in structural engineering is due to their ability to be heated, softened, and reformed, which may give the parts the potential to be joined by a local heating processes, akin to welding of metals. In addition, they are generally less expensive than thermosetting resins and are recyclable. However, they are difﬁcult to process and generally have lower strength and stiffness than thermosets. They do, however, have higher elongations than thermosets (up to 20%), making them tougher and more ductile. A comparison of the properties of thermosetting resins for FRP products for structural engineering is given in Table 2.3. FRP products produced for use in structural engineering can include signiﬁcantly more ingredients than just the primary constituents: ﬁbers and polymer resins. Fibers are produced with surface coatings called sizings and are supplied in many different strand and broadgood forms. Resins can contain ﬁllers, catalysts, accelerators, hardeners, curing agents, pigments, ultraviolet stabilizers, ﬁre retardants, mold release agents, and other additives. These have different functions, from causing the resin to polymerize to helping the processing to modifying the ﬁnal properties of the FRP part. These many different supplementary constituents are manufacturing method–dependent and are discussed below.

2.3

MANUFACTURING METHODS

Two main manufacturing methods are used to produce FRP composite material products for use in structural engineering. The one method is an automated industrialized process, developed in the early 1950s, called pultrusion, in which the FRP products are produced in a factory and shipped to the construction site for fabrication and installation or erection. The other method is a manual method, known as hand layup or wet layup, in which the FRP product is manufactured in situ at the construction site at the time it is in-

TABLE 2.3

Approximate Properties of Thermosetting Polymer Resins Density [g / cm3 (lb / in3)]

Polyester Epoxy Vinylester Phenolic Polyurethane

1.2 (0.043) 1.2 (0.043) 1.12 (0.041) 1.24 (0.045) varies

Tensile Modulus [GPa (Msi)] 4.0 3.0 3.5 2.5 2.9

(0.58) (0.44) (0.51) (0.36) (0.42)

Tensile Strength [MPa (ksi)] 65 90 82 40 71

(9.4) (13.1) (11.9) (5.8) (10.3)

Max. Elongation (%) 2.5 8.0 6.0 1.8 5.9

52

MATERIALS AND MANUFACTURING

stalled. It is the original method used to produce ﬁber-reinforced polymer composites and dates back to the development of FRP materials in the 1940s. However, as described below, the hand-layup method as it is used in structural engineering is signiﬁcantly different from that used in the rest of the composites industry. The pultrusion process is used to manufacturer FRP reinforcing bars, FRP strengthening strips, and FRP proﬁles and is the most cost-competitive method for producing high-quality FRP parts for use in structural engineering. The hand-layup method is used to manufacture and install dry ﬁber strengthening sheets and fabrics and is also very cost-competitive, as it is particularly easy to use in the ﬁeld. Other methods that have been used to produce specialized FRP products for use in structural engineering, such as ﬁlament winding and resin transfer molding, are discussed very brieﬂy since code-based design guides for use of these products in structural engineering are either not available or are insufﬁciently developed at this time. 2.3.1

Pultrusion

Pultrusion is an automated and continuous process used to produce FRP parts from raw materials. Figure 2.1 shows a photograph of typical FRP pultruded parts used in structural engineering. A pultruded part can have an open cross section, such as a plate or a wide-ﬂange proﬁle; a single closed cross section, such as a hollow tube; or a multicellular cross section, such as panel with

Figure 2.1 Pultruded I-shaped beams. (Courtesy of Racquel Hagan.)

2.3

MANUFACTURING METHODS

53

internal webs. The cross section does not have to have a constant thickness throughout. Although there is great ﬂexibility in the shape, thickness variation, and size of the part cross section, the cross section must remain constant along its length. In addition, the part must be straight and cannot be cured into a curved shape. A pultruded part can be produced to any desired length, and if it is ﬂexible enough, it can be coiled onto a spool for shipping (such as a thin FRP strip for strengthening or a small-diameter FRP rebar). Modiﬁcations to the pultrusion process have been developed for nonconstant cross sections or for producing curved parts; however, these are nonroutine variants of the pultrusion process. In other variants, a core material is used in a cellular part to ﬁll the cavity in the part. A pultrusion line or a pultrusion machine is used to produce the pultruded part. The ﬁrst pultrusion machine, called the Glastruder, was developed by Brandt Goldsworthy in the early 1950s (Goldsworthy, 1954). In 1959, a U.S. patent for a pultrusion machine and the method for producing pultruded parts was awarded to Goldsworthy and Landgraf (1959). Pultrusion machines can now be purchased from a number of companies or can be built from scratch from available off-the-shelf materials and parts. Experienced pultrusion companies tend to develop and build their own pultrusion machines in-house. A schematic of a typical pultrusion line or machine is shown in Fig. 2.2. To produce FRP parts for structural engineering, dry ﬁbers impregnated with a low-viscosity4 liquid thermosetting polymer resin are guided into a

Figure 2.2 Pultrusion line. (Courtesy of Strongwell.)

4 The viscosity of the polymer resin used in pultrusion depends on the part reinforcement and geometry and is a processing variable; it is usually between 500 and 3000 centipoise (cP), similar to that between motor oil and house paint.

54

MATERIALS AND MANUFACTURING

heated chrome-plated steel die, where they are cured to form the desired FRP part. The FRP is cured as the material is pulled through the die by a pulling apparatus: hence, the name pultrusion. A number of variations of this basic process exist and are described by Meyer (1970). After exiting the die and extending past the pullers, the part is cut to length by a diamond blade cutoff saw. The rate of production of a pultruded part depends on the size of the part. Small –14 in. (⬃6-mm)-round pultruded rods can be produced at rate of up to 60 in./min (150 mm/min), although larger complex multicellular parts can be produced at a rate of only a few inches per minute. As the surface area of the cross section increases, a greater amount of force is needed to overcome the frictional forces to pull the part through the die. Typical pultrusion machines have pulling capacities of 10,000, 20,000, and 40,000 lb (approximately 50, 100, and 200 kN). The length of the heated steel die used to produce an FRP part is typically from 20 to 40 in. (500 to 1000 mm). The die, which is heated by electric resistance heaters or oil heat, is often heated in two or three separate regions along its length to different temperatures from 200 to 400⬚F (⬃90 to 180⬚C) in order to develop the best curing conditions for the type of resin system used in the part. The entrance to the die is typically cooled to prevent premature curing of the resin system. When parts are not required to have a smooth exterior surface, such as a deformed FRP reinforcing bar, a long die is not used. Rather, the impregnated ﬁber is pulled though a forming ring and is then cured by radiant heat in 6- to 8-ft (1.8- to 2.4-m)-long cylindrical ovens. The pulling apparatus and the cutoff saw are located downstream of the ovens. When thick parts are pultruded, radio-frequency (RF) heating is frequently used to preheat the resin before the part enters the heated die to assist the curing process. The dry ﬁber is supplied in various forms on spools or rolls and is spliced ‘‘on-the-ﬂy’’ to create a never-ending source of ﬁber. The dry ﬁber is usually impregnated or wet-out in a resin bath, which is continuously reﬁlled and is usually open to the environment, which is ventilated. Most pultrusion manufacturers run their machines on a 24-hour continuous cycle and do not stop the process until the required lot of the FRP part is produced. Typically, only one operator is needed to oversee the line when it is running smoothly. Setup time for a pultrusion line can take from a few hours to a few days, depending on the complexity of the part, and typically involves two to three operators. Cleanup time for the line usually takes a few hours. Acetone is typically used to clean the parts of the pultrusion line that have been exposed to the polymer resin. The raw materials that are used in the pultrusion process can be broadly viewed as breaking down into two main systems: the ﬁber system and the resin system. The ﬁber system contains all the dry reinforcements that are pulled into the resin system for wetting-out prior to entering the die. The resin system refers to the mix of ingredients that is used to saturate the ﬁbers. The

2.3

MANUFACTURING METHODS

55

resin system is typically premixed in large batches [usually, 55-gallon (⬃200L) drums] in a mixing room in a pultrusion plant before it is brought to the pultrusion line and pumped or poured into the resin bath. Fiber System for Pultrusion The ﬁber system used in an FRP pultruded part can consist of different types and architectures of ﬁber materials. The raw ﬁber is processed and supplied either in strand form on a spool and known as roving or tow, or in broadgoods form on a roll and known as mat, fabric, veil, or tissue. The dry ﬁber is fed into the pultrusion die in a speciﬁc arrangement so as to locate the various different ﬁbers and ﬁber forms in speciﬁc parts of the part cross section. High-density polyethylene (HDPE) or Teﬂon-coated plates with holes and slits or vinyl tubes, through which the individual ﬁber types pass guide the ﬁbers through the resin bath and into the die. The guides also help to remove excess resin from the resin-saturated ﬁbers before the ﬁbers enter the die mouth. In FRP proﬁles, individual strands and mats or fabrics are usually laid out in symmetric and balanced alternating layers, giving the pultruded material a laminated or layered internal architecture.5 Figure 2.3 shows a close-up of the corner of a pultruded tube with a –14 -in. (6.3-mm) wall thickness. The layup consists of mat layers on the exterior of the part and rovings in the interior. In FRP reinforcing bars and FRP strengthening strips, only ﬁber strands are used and the FRP part consists only of longitudinally aligned ﬁbers and is referred to as unidirectionally

Figure 2.3 Pultruded tubular proﬁle, showing roving and mat layers. (Courtesy of Saiphon Jacque.)

5 The laminate must be symmetric and balanced, to prevent unwanted axial–shear coupling and bending–extension when it is loaded. See Chapter 3 for more detail on the mechanics of laminates.

56

MATERIALS AND MANUFACTURING

reinforced. FRP reinforcing bars may also have helically wound ﬁber strands at the surface to create bar deformations for load transfer to the concrete. Glass and carbon ﬁber are currently used to reinforce most FRP pultruded parts for structural engineering applications. A very small amount of aramid ﬁber is used in pultrusion. Glass ﬁber is used in pultruded proﬁles due to its low cost. Carbon ﬁber is used in FRP strengthening strips due to its high modulus. A small number of proﬁles and strips have been produced with a mixture of glass and carbon ﬁbers to optimize the mechanical properties and costs of the part. These FRP pultruded parts are called hybrids. In addition to the reinforcing ﬁbers, which give the FRP composite its strength and stiffness, nonreinforcing polyester and glass surfacing mats or veils are used at the surface of the part to aid in processing and to create a smooth surface ﬁnish. Glass Fiber Rovings Individual continuous glass ﬁlaments are bundled, generally without a twist, into multiﬁlament strands known as rovings that are used in the pultrusion process either as is or in fabrics produced from rovings. In the United States, roving quantity is traditionally measured in units of yield (yd/lb). Roving is produced in yields of 56, 62, 113, 225, 250, 450, 495, 650, and 675. Not all producers manufacture all yields. The number of ﬁlaments in an individual roving with a speciﬁc yield depends on the ﬁber diameter of the ﬁlament. The most common roving used in pultruded parts is a 113 yield roving, which has approximately 4000 ﬁlaments, usually having a diameter of 24 m (93 ⫻ 10⫺3 in.) each. Figure 2.4 shows a spool of 113 yield glass ﬁber roving. In the metric system, roving quantity is measured in units of TEX (g/km). A 113 yield roving is equal to a 4390 TEX roving. Its crosssectional ﬁber area is 0.00268 in2 (1.729 mm2). The following relationships (Barbero, 1999) relate these quantities: TEX(g/km) ⫽

Aƒ(in2) ⫽

496,238 yield(yd/lb)

1 ƒ(lb/in3) ⫻ yield(yd/lb) ⫻ 36(in./yd)

(2.1)

(2.2)

Rovings are supplied on spools weighing approximately 50 lb (22 kg) each. Typically, tens to hundreds of separate rovings are pulled into a pultruded FRP part. Many large industrial companies manufacture glass ﬁber roving throughout the world. In 2004, the price of glass ﬁber roving was about $0.70 per pound ($1.5 per kilogram). In the pultrusion process, the rovings are aligned along the direction of the pultruded part, which is known as the machine direction or lengthwise (LW) direction. In composite mechanics, this direction is known as the longitudinal

2.3

MANUFACTURING METHODS

57

Figure 2.4 113 yield glass roving on a spool.

or zero-degree (0⬚) direction of the composite material. In structural design, this direction typically coincides with the longitudinal axis of the FRP bar, FRP strip, FRP beam, or FRP column. Consequently, the rovings provide the pultruded part with the majority of its axial and ﬂexural strength and stiffness. For parts requiring only high longitudinal strength and stiffness, such as FRP reinforcing bars or thin FRP strengthening strips, high percentages of rovings on the order of 50 to 60% of the total volume of the FRP composite are used. However, such parts have low crosswise (CW) or transverse strength and stiffness. To develop transverse strength and stiffness in a pultruded part, ﬁber mats and fabrics are used in addition to the rovings. The polymer resin is typically relied on to provide the out-of-plane and transverse shear properties of the pultruded material. When producing tubular parts, glass ﬁber roving can also be wound in the circumferential direction around the tube to provide an outer layer of hoop reinforcement. Three-dimensional ﬁber reinforcement preforms for pultrusion that can give out-of-plane, or through-the-thickness, strength and stiffness are not used in regular parts, and a typical pultruded part has a platelike layered structure with alternating layers of roving and mats or fabrics through the plate thickness. In the pultrusion operation, the roving spools are stacked on metal racks called creels. Creel racks should be metal and grounded to prevent electrostatic charge buildup during production. The roving is pulled off the individual spools and guided into the resin bath, where it is saturated with liquid resin (also known as wet-out). The roving is usually the ﬁrst ﬁber reinforcement

58

MATERIALS AND MANUFACTURING

material to be wet-out. It is important to ensure that the roving bundles do not bunch together in the resin bath, as this can lead to rovings not being fully wet-out, which will lead to dry-ﬁber areas in the ﬁnished product, which is highly undesirable. Glass Fiber Mats Continuous ﬁlament mat (CFM), also referred to in the United States as continuous strand mat, is the second most widely employed glass ﬁber product used in the pultrusion industry. CFM is used to provide crosswise (CW) or transverse strength and stiffness in platelike parts or portions of parts (e.g., the ﬂange of a wide-ﬂange proﬁle). CFMs consist of random, swirled, indeﬁnitely long continuous glass ﬁber ﬁlaments held together by a resin-soluble polymeric binder. They are different from copped strand mats (CSMs), which consist of short [1 to 2 in. (25 to 50 mm)] ﬁbers held together in mat form by a resin-soluble binder 6 which are used mainly in sheet molding compounds. Because of the pulling forces exerted on the mats in the pultrusion processes, chopped stand mats are generally not suitable for pultrusion except when used together with a preformed combination fabric system (these fabrics are discussed below). Continuous ﬁlament mats also help to keep the individual rovings in position as they move through the die. Due to the random orientation of the ﬁbers in the plane of the continuous mat, the mat, and hence the layer of the cured pultruded material that contains the mat, can be assumed to have equal properties in all directions (i.e., isotropic properties) in its plane. CFMs are now produced by a number of companies, although for many years Owens-Corning Fiberglas (OCF) held a patent on the product and was the sole producer. E- and A-glass mats are used in pultrusion. For strength and stiffness, E-glass mats are used. A-glass mats are used primarily for better surface ﬁnish. A detailed discussion of the properties of various pultruded materials with E- and A-glass mats can be found in Smith et al. (1998) and Smith (2002). E-glass mats are typically available in weights of 1 to 3 oz/ft2 (300 to 900 g/m2) in –14 -oz/ft2 (75-g/m2) increments. A-glass mats are available in –12 - to 1–12 -oz/ft2 (150- to 450-g/m2) weights in –14 -oz/ft2 (75-g/m2) increments. It is very important to note that in the United States, mat weights are given in ounces per square foot, while other broadgood materials, such as fabrics (discussed below) are given in ounces per square yard. Fiber mats are typically supplied on paperboard tubes 3 in. in diameter up to lengths of 84 in. (2.1 m). To use the mat product in pultrusion, the large roll is cut up into rolls of narrow widths, as required for the dimensions of the pultruded part being produced. In the pultrusion operation, the CFM is typically wet-out after the rovings. A hose, funnel, or chute may be used to pour the liquid resin directly onto

6 Be aware that in the industry the acronym CSM is often used for both continuous strand mat and chopped strand mat.

2.3

MANUFACTURING METHODS

59

the mat surface as it is fed through guides. When the mat is light, it is often simply wet-out by the excess resin that is carried by the rovings into the forming guides. When the saturated mat and rovings enter the die, they are squeezed into the die opening. This squeezing produces an internal die pressure of around 80 psi (⬃550 kPa). The pressure tends to compress the mat layers. A rule of thumb used in the industry is that a 1-oz/ft2 (300-g/m2) Eglass CFM will occupy a thickness of 20 mils (0.50 mm) in the ﬁnished pultruded part and that a –12 -oz/ft2 (150-g/m2) A-glass mat will occupy a thickness of 16 mils (0.41 mm). Due to the structure of the swirled ﬁlaments in an E-glass CFM, the volume faction of ﬁbers in a layer of pultruded material containing a E-glass mat is typically only in the range 20 to 25%. In 2004, the price of E-glass ﬁber continuous stand mat was about $1.20 per pound ($2.6 per kilogram). The increase in price over the cost of the roving material is due to the cost of the additional manufacturing process required to produce the mat from the ﬁlaments. Figure 2.5 shows an E-glass CFM. Glass Fiber Fabrics Since unidirectional rovings give the pultruded composite reinforcement in its longitudinal direction, and the continuous stand mats give reinforcement in all in-plane directions equally (i.e., isotropically), the range of mechanical properties of the pultruded composite consisting of only rovings and mats is limited. To obtain a greater range of properties and to ‘‘tailor’’ the layup (or the ﬁber architecture) of the pultruded composite to yield speciﬁc structural properties, fabric reinforcements can be used in which ﬁbers are oriented in speciﬁc directions and at speciﬁc volume percentages

Figure 2.5 1.5-oz / ft2 E-glass continuous ﬁlament mat.

60

MATERIALS AND MANUFACTURING

to the pultrusion axis. This design approach, in which multiaxial plies (or layers) are used, is routine in the hand-layup technique; however, it is only in recent years that multiaxial fabrics have been used successfully in the pultrusion process. This is because pulling an off-axis ply (say, one with a 45⬚ orientation to the pultrusion direction) is a nontrivial matter and special preformed fabrics are needed that can be pulled without causing distortion of the ﬁber orientations. Although now available, multiaxial fabrics are still used only in very special pultruded parts, as their costs can be considerably more than that of mats. They are not as easy to wet-out and pull as rovings and CFMs. It is, however, generally recognized in the composites industry that to optimize the mechanical properties of pultruded proﬁles for structural engineering, the next generation of proﬁles will need to use more multiaxial fabrics, possibly with hybrid ﬁber types, and have more sophisticated crosssectional shapes. The recent double-web beam produced by Strongwell, shown in Fig. 2.6, is an example of such a engineered hybrid proﬁle developed for bridge girders. Glass ﬁber fabric materials for pultrusion are generally of two types. One type is a woven roving fabric; the other type is a stitched roving fabric. Woven roving is used routinely in hand-layup applications such as boat building and is supplied in weights between 6 and 48 oz/yd2 (200 to 1600 g/m2) and has ﬁber orientations of 0⬚ and 90⬚. The percentage of 0⬚ and 90⬚ ﬁbers [known as the warp and the weft (or ﬁll) directions in the textile industry] depends

Figure 2.6 Double-web hybrid ﬁber pultruded beam. (Courtesy of Strongwell.)

2.3

MANUFACTURING METHODS

61

on the weave pattern. Most woven fabrics made for use in pultrusion are of the plain or square pattern, with almost equal percentages of ﬁbers in the two directions. To use a woven roving in a pultrusion process, it needs to be attached to a glass mat (usually, a chopped strand mat) to prevent it from distorting when pulled. Either powder bonding, stitching with a polyester or glass yarn, or needling are used to attach the woven fabric to the mat, which is then known as a combination fabric. Many different combinations of woven roving weights and mat weights are available. Commonly used types are 18oz/yd2 woven roving with a 1-oz/ft2 mat (600-g/m2 woven roving with a 300-g/m2 mat). A close-up of a woven roving combination fabric is shown in Fig. 2.7. The other type of fabric type that is used in pultrusion is a stitched fabric where the unidirectional layers of rovings in different directions are stitched together with or without a chopped mat. Popular types of stitched fabrics are biaxial (having equal percentages of 0⬚ and 90⬚ or ⫹45⬚ and ⫺45⬚ ﬁber orientations) and triaxial (having ﬁbers in the 0⬚, ⫹45⬚, and ⫺45⬚ ﬁber orientations). ⫹45⬚ and ⫺45⬚ ﬁber orientations are used to give a pultruded part high in-plane shear strength and stiffness properties. Unidirectional stitched fabrics in which the ﬁbers in one direction are stitched to a mat can also be obtained. These are particularly useful when 90⬚ ﬁber orientation is needed in a pultruded part to give it high transverse strength and stiffness. For unique applications, unbalanced stitched fabrics can be obtained. As noted previously,

Figure 2.7 Woven glass roving combination fabric.

62

MATERIALS AND MANUFACTURING

it is important to ensure that the resulting layup is both symmetric and balanced when using stitched and combination-stitched fabrics. A close-up of a stitched fabric is shown in Fig. 2.8. The nomenclature used in the specialty fabric industry is often confusing and varies from manufacturer to manufacturer.7 In one commonly used fabric nomenclature, the 18-oz/yd2 woven roving with a 1-oz/ft2 mat described previously is referred to as a 1810 woven-roving-mat fabric or a 600/300 woven-roving-mat fabric (in metric nomenclature). The ﬁrst two digits give the weight of the bare fabric, in oz/yd2, and the second two digits give the weight of the mat that is attached to the bare fabric, in oz/ft2. In the metric system, both bare fabric and mat are given in g/m2, and a slash is used to indicate the weight of the fabric and the mat, respectively. The digits are usually preceded by various letters to indicate the ﬁber type (glass, carbon, aramid), bare fabric type (woven or stitched), ﬁber orientations,8 and whether or not a mat is used (M). In addition to woven and stitched fabrics, braided and knitted fabrics are also produced for use in the pultrusion process. The braiding process is used

Figure 2.8 Stitched glass ﬁber fabric.

7 The nomenclature used for specialized fabrics is highly producer dependent. The structural engineer is cautioned to be very familiar with the nomenclature used by the fabric producer before specifying a product for use in structural engineering. 8 L, longitudinal (0); T, transverse (90); B, biaxial (0 / 90); X, Ⳳ45 ply; TT, triaxial (0 / Ⳳ45) Q, quadriaxial (0 / Ⳳ45 / 90).

2.3

MANUFACTURING METHODS

63

to produce tubular ‘‘sleeves’’ and narrow strips having biaxial and triaxial (inplane) ﬁber orientations. A special mandrel and ﬁber-forming system is required to use a braided sleeve in the pultrusion process to make a tubular product. Figure 2.9 shows a braided sleeve. Carbon Fiber Tows Carbon ﬁber strands called tows can be used in the pultrusion process and have been used since the 1970s to pultrude small specialized items such as archery arrows and solid rods. However, they have not generally been used to produce pultruded proﬁles for structural engineering, due to their high cost relative to glass ﬁber roving. In recent years, carbon ﬁber–reinforced epoxy pultruded FRP strengthening strips have increased the use of carbon ﬁber FRP products in structural engineering signiﬁcantly. TEX is used to refer to the quantity of carbon ﬁber in a tow. Yield is not generally used for carbon ﬁber. A carbon ﬁber tow is identiﬁed by the number of individual carbon ﬁber ﬁlaments in the tow, which usually ranges from 1000 to 48,000 (known as 1K to 48K size tows); however, in recent years, highyield tows up to 300,000 ﬁlaments (300K tow) have been produced. The relationships between tow size, TEX, cross-sectional area, and ﬁber density for a carbon ﬁber tow are (Barbero, 1999) TEX(g/km) ⫽ tow size(K) ⫻ Aƒ(m2) ⫻ ƒ(g/cm3) Aƒ(cm2) ⫽

TEX(g/km) ƒ(g/cm3) ⫻ 105

(2.3) (2.4)

Large standard modulus carbon tow sells for between $7 and $10 per pound ($15 to $22 per kilogram) ((2004), making it considerably more expensive than glass ﬁber roving. It has long been a stated goal of the carbon ﬁber producers to get carbon ﬁber down to $5 per pound ($11 per kilogram); however, this still seems unattainable, and cycles of feast and famine still plague the industry. Carbon ﬁber has signiﬁcantly higher modulus and lower density than glass ﬁber, which can make it particularly advantageous to use in certain products for structural engineering (such as for FRP pultruded strengthening strips). Figure 2.10 shows a 12K carbon ﬁber tow on a spool. When using carbon ﬁber in the pultrusion process the pultrusion line usually needs to be physically isolated from other lines in the plant. Carbon ﬁber is electrically conductive, and carbon ﬁber dust can cause short-circuiting in electrical boxes. In addition, when carbon ﬁbers are being used in a plant where glass ﬁber pultruded parts requiring high electrical resistivity are produced (such as insulators for electric power lines), stray amounts of carbon ﬁber dust can contaminate the glass ﬁber part and cause signiﬁcant quality control problems. Consequently, carbon ﬁber production facilities are often placed in separate sections or buildings in a pultrusion plant.

64

MATERIALS AND MANUFACTURING

Figure 2.9 Glass ﬁber braided sleeve.

Figure 2.10 Carbon ﬁber tow on a spool.

2.3

MANUFACTURING METHODS

65

Carbon Fiber Fabrics Carbon ﬁber fabrics are generally available in the same types of weaves and stitched goods as glass ﬁber fabrics. They range in weights from 6 to 32 oz/yd2 (200 to 1050 g/m2) and are typically produced in biaxial 0/90 and Ⳳ45 bias-ply layups. They are produced by fewer manufacturers than glass fabrics and are typically produced as special orders from the major suppliers of specialty fabrics for unique pultrusion applications. At present, only a small number of pultruded FRP products are produced with carbon ﬁber fabrics for use in structural engineering. Carbon ﬁber fabrics are signiﬁcantly more expensive than glass ﬁber fabrics. Continuous ﬁlament carbon ﬁber mat, like a glass CFM, can also be obtained from specialty manufacturers. Hybrid Fabrics Most specialty fabric producers manufacture custom hybrid fabrics consisting of carbon, glass, and often also aramid ﬁbers in different orientations and weights; however, these are not used in any regular FRP pultruded parts for structural engineering. They tend to be much higher priced and are used in one-off molding operations such as layup and resin transfer molding to produce more exotic composite material industrial products and sporting goods such as surfboards, skis, snowboards, and racquets. Surfacing Veils An important characteristic of an FRP pultruded part is the quality of the surface. A smooth and regular surface without signiﬁcant ﬁber fabric or roving pattern deformations on the surface is usually desired. In some pultruded parts, such as FRP rebars, this is not a concern, as surface deformation is desired. To achieve a good, smooth surface quality, often referred to as a low-proﬁle surface, a very lightweight surfacing fabric, called a veil or tissue, is used as the outer layer of the pultruded part. Veils are typically made of nonwoven polyester ﬁlaments or C- and E-glass monoﬁlament mats. Veils are much lighter than regular continuous ﬁlament mats and have nominal weights of 1 to 2 oz/yd2 (⬃30 to 60 g/m2). The surfacing veil tends to have a higher resin volume fraction than the other reinforcement layers, such as mats and rovings, and gives the part a resin-rich surface layer similar to that of a gel coat in a hand layup. The resin-rich surface also gives the part greater corrosion and ultraviolet resistance. Figure 2.11 shows a polyester veil. Resin System for Pultrusion The three main thermosetting resins used in the pultrusion process are unsaturated polyesters, unsaturated vinylesters, and epoxies. To each of these base resins supplementary constituents are added to cause the polymerization reaction to occur, to modify the processing variables, and to tailor the properties of the ﬁnal FRP pultruded part.9 The ad-

9 There is no single ‘‘resin mix recipe’’ for any of these resin systems; the mix depends on the FRP part to be pultruded and the pultrusion process variables.

66

MATERIALS AND MANUFACTURING

Figure 2.11 Polyester veil.

ditional constituents that are added can be broadly grouped into three main categories: polymerization agents, ﬁllers, and additives. Polymerization agents are known as either catalysts or curing agents (or even hardeners), depending on the resin type being used. Fillers are sometimes called extenders. Additives are also known as modiﬁers or process aids. Examples of some sample pultrusion resin systems, with trade names and precise quantities of the various constituents used, can be found in Meyer (1985) and Starr (2000). Most pultruders regard their mixes as proprietary and therefore usually do not openly publicize the exact details of their resin systems. Resin systems are typically developed by a pultrusion company in collaboration with a resin manufacturer. Polymerization Agents Unsaturated polyester and vinylester resins that react with a styrene monomer are catalyzed with organic peroxides. The peroxide is used to ‘‘kick-off’’ or initiate the curing reaction and is heat-activated by the die so that the resin does not begin to gel and cure in the resin bath.10 Different catalysts are chosen to cause the polymerization processes to occur at a controlled time and lengthwise position in the pultrusion die. They are referred to as kicker peroxides, medium-reactivity peroxides, and ﬁnishing 10 For room-temperature processing, a MEKP (methyl ethyl ketone peroxide) catalyst is generally used. An accelerator or promoter, usually a cobalt napthanate, is also required to initiate the reaction. In addition, a dimethyl analine (DMA) promoter is also required with a roomtemperature-cured vinylester.

2.3

MANUFACTURING METHODS

67

peroxides (Starr, 2000). Peroxides are added in quantities of between 0.25 and 1.5% by weight of the resin and are given as parts per hundred (pph) by weight.11 It is also not uncommon for additional styrene monomer to be added to the base resin (also known as the neat resin) during the resin mixing operation. Ten to 15% by weight can be added to aid in processing (it decreases the resin viscosity) and to decrease costs. However, the quantity of styrene in the resin mix must be carefully controlled, as unreacted styrene in the cured part can lead to a part with poor environmental durability. Blended polyester and vinylester resins are also used in pultrusion to exploit beneﬁcial processing and property characteristics of each resin type. Epoxy resins used in pultrusion are polymerized by the addition of curing agents, typically of the amine type. The curing agent or hardener is usually referred to as part B, and the epoxy resin is referred to as part A. Curing agents are generally added at ratios of 25 to 50% by weight of the epoxy resin. Curing agent accelerators may also be used in small percentages (less than 1% by weight). Epoxy resins are signiﬁcantly more difﬁcult to pultrude than polyester or vinylester resins because of their lower shrinkage, higher viscosity, and longer gel times (Starr, 2000). Because of this, the pultrusion line is usually slower and requires more pulling force when an epoxy resin is used. Specially formulated epoxies that cure only at high temperatures are also required. Limited epoxy formulations are used in pultrusion. Epoxies are used where signiﬁcant mechanical or physical property advantages can be obtained. At this time, no routinely produced standard FRP proﬁle shapes are made with epoxy resin systems; however, most pultruded FRP strengthening strips are produced with epoxy resins. Fillers Inorganic particulate ﬁllers are used to ﬁll or ‘‘extend’’ the base polymer resin used for pultrusion for three primary reasons: to improve processing dynamics, to reduce cost, and to alter cured part properties (Lackey and Vaughan, 2002). Inorganic ﬁllers have particle sizes between 0.5 and 8 m (0.0002 to 0.0032 in.) and can have spherical or platelike geometries. The three primary types of inorganic ﬁllers used in pultrusion are kaolin clay (aluminum silicate), calcium carbonate, and alumina trihydrate (ATH). Typical polyester and vinylester pultruded FRP proﬁles shapes and FRP rebars have between 10 and 30% by weight of ﬁller in the resin mix. Small pultruded parts having primarily unidirectional roving reinforcement usually have low ﬁller percentages, from no ﬁller to 5% by weight. Epoxy resin pultrusions can also be ﬁlled. Small parts such as FRP strengthening strips are generally not ﬁlled. The density of the inorganic ﬁllers is between 2.4 and 2.6 g/cm3 (0.0865 to 0.0937 lb/in3), making it approximately equal to glass ﬁber and

11 The percentage is given as parts per hundred of the base resin (i.e., 100 parts of base polymer resin) or parts per hundred of the total resin mix (i.e., 100 parts of the total resin mix, including all secondary constituents). In this case the base resin could be as low as 50 pph of the total mix.

68

MATERIALS AND MANUFACTURING

about twice the density of the resin. Fillers are substantially less costly than either resins or ﬁbers. In addition to serving as a ﬁller, alumina trihydrate serves a dual role as a ﬁre-retardant additive. Fillers usually decrease the key longitudinal mechanical properties and the corrosion resistance of an FRP pultruded part (Lackey et al., 1999). However, ﬁllers can be used to improve properties, especially in the transverse direction and to modify the physical properties (Meyer, 1985) of an FRP pultruded part. Recently, pultruders have begun to experiment with nanosized particle ﬁllers, and results show FRP parts with greater corrosion resistance. Additives The third group of constituents that are added to the resin mix are those used to assist in the processing or to modify the properties of the cured FRP part (Lackey and Vaughan, 2002). Chemical release agents, typically metallic stearates, fatty acids, or waxes, are used to prevent the FRP part from sticking to the die interior. A foaming agent is often used to remove entrained air from the resin mix. Pigments, or colorants, are mixed in the resin to give the ﬁnished part different colors. Ultraviolet stabilizers are added to protect the resin in the cured part from the effects of sunlight. Additives that retard ﬂame spread in the cured FRP part, such as antimony trioxide, may be added to FRP proﬁles to meet code-stipulated ﬁre and ﬂammability ratings.12 In addition, thickening agents, toughening agents, and viscosity control agents may be used to modify the characteristics of the resin mix. These additives are generally added in quantities less than 1% by weight of the resin. The one additive that is often added in a signiﬁcantly higher percentage is a lowproﬁle or shrink additive. Low-proﬁle additives are usually thermoplastic polymer materials and are added to the mix to prevent shrinkage cracking in the interior of thick parts and at the surface of thin parts. Silane coupling agents may be added to the resin mix to improve the bond between the ﬁbers and the resin; however, these coupling agents are usually in the sizing on the ﬁber itself. It is important to note that all of these additives can inﬂuence both the physical and mechanical properties of the FRP part since they all affect the resin chemistry (Lackey and Vaughan, 2002). Even a seemingly innocuous additive such as a pigment can have a signiﬁcant effect on properties, and changing the color of a FRP pultruded part is not necessarily a trivial matter. 2.3.2

Hand Layup

Hand layup is the term given to the manual method of constructing an FRP composite part by laying up, or rather, putting down, successive layers of ﬁbers and impregnating them with a liquid polymer resin, which then cures to form a solid FRP composite element. The solid part takes the form and

12 The use of heavy metals in plastics is being reevaluated due to possible health hazards. Leadbased pigments are no longer used in the industry.

2.3

MANUFACTURING METHODS

69

shape of the mold or surface to which it is applied. The method is also known as laminating or wet layup or simply layup and is used to make laminates or panels of FRP composites. The hand-layup method is probably the oldest method of producing FRP parts and is used to make a variety of FRP products. The method is deceptively simple, and producing a high-quality FRP part using the method requires a signiﬁcant degree of skill and good quality control. For use in industrial products, laminates constructed using the hand-layup method are usually thin, less than –18 in. (3.2 mm) in thickness. They can be much thicker in the marine industry, where FRP boat hulls can approach thicknesses of 6 in. (150 mm) or more. A foam or balsa core is often used to create a sandwich structure, with the FRP layers serving as the outer skins. Sandwich layups are used extensively in the boat-building and recreational products industries to produce surfboards of all types. The method is used with various degrees of sophistication, which all serve to improve the quality or the part, deﬁned as a part with a high-volume fraction of ﬁbers, precise ﬁber placement, and very few voids, the most signiﬁcant of these being the use of higher temperatures and pressures to cure the layers after they have been impregnated with the resin, and the precise control of the amount of resin that is applied to the ﬁbers. In its most sophisticated form it is widely used in the aircraft industry to manufacture airfoils and fuselage parts for aircraft. In this form the resin system is preimpregnated in precise amounts onto unidirectional ﬁbers that are partially cured into sheetlike products called prepregs. The prepregs are then cut and shaped and placed in different orientations on a mold which is then inserted into a polymeric bag from which the air is extracted by vacuum (known as a vacuum bag) and cured at high temperature and pressure in an autoclave. Numerous manufacturers produce prepregs for the aerospace and recreational products industries. Although the hand-layup method as it is used in structural engineering appears to be similar to that used in other industrial processes, it is different in one very important aspect. When an industrial product such as a sailboat hull or tennis racquet is produced, the product is made in, or on, a mold and it is removed from the mold after curing. In fact, the removal, or the release, from the molding surface is usually achieved by using a chemical or natural release agent to ensure that the FRP part does not stick to the mold or surface on which it was formed. In the structural engineering application, the situation is opposite. The FRP composite that is applied by hand layup onto the surface of an existing structural element needs to be ﬁrmly adhered to, or be ﬁrmly in contact with, the surface in order to perform its strengthening function. Herein lies the difﬁculty in using the hand-layup method in structural engineering. Not only is the method being used to produce the FRP strengthening element, but it is being used to create the interface between the FRP element and the existing structural element. This interface, or interfacial region, is in and of itself a vital part of the FRP strengthening system. (When premanu-

70

MATERIALS AND MANUFACTURING

factured pultruded FRP strips are used for strengthening, it is only the adhesive interfaces that are created in the ﬁeld, and the application of precured strips can be thought of as a form of the hand-layup method, even though the actual FRP composite itself is not produced by the hand-layup method.) Because of this key difference between the industrial hand-layup method and the structural engineering hand-layup method, it is crucial to select the ﬁber and resin systems very carefully, such that both the adhesive function and the wetting-out function of the resin are present. Since the adhesive properties of the resin system will depend on the surface to which it is being bonded and the method of application, proven, well-tested combinations of ﬁbers and resins and application methods should be used only in structural engineering applications. Although ﬁber fabrics and resins can be purchased almost anywhere, not any ﬁber and resin can necessarily be used to strengthen a structural element. At this time only code-based design guidance is available to structural engineers for ﬁber and resin systems that are used to strengthen reinforced concrete structural members. It is these FRP systems for structural strengthening, as they are known, that are discussed in more detail in what follows and for which design procedures are given in later chapters. In addition, speciﬁc guidance is given in published guide construction speciﬁcations for commercially available FRP strengthening systems for concrete as to how the FRP material must be applied in the ﬁeld and what level of training and experience is required of the ﬁeld contactor. Although there are many known applications of FRP strengthening systems to masonry and timber structures, a design guide does not exist at this time for strengthening these structures with FRP composites. When used in structural engineering, the hand-layup method is typically used in its most elementary form, with the resin-impregnated ﬁbers being cured at ambient temperatures without the use of externally applied pressure or high temperature. In this case, the FRP composite laminate is formed directly on the structural element to be strengthened, such as a beam or a column, and cured in place, in much the same way that reinforced concrete is cured in place. In a few rare cases, attempts have been made to use vacuum bags or elevated temperatures in the ﬁeld. When dry ﬁber broadgoods and liquid resins are used to form the composite in the ﬁeld on the substrate to be strengthened or repaired, hand layup is performed in one of two ways, depending on the type of dry ﬁber material that is used. When precured FRP strips are used, the FRP composite is produced by the pultrusion method described previously and afﬁxed to the substrate using a hand-layup method. In the case of a lightweight ﬁber tow sheet, the method is similar to that used to apply wallpaper. Following application of a primer sealant and ﬁlling of holes with putty, the surface is coated with a thin layer of the liquid resin system (also called the saturant) using a fabric roller, similar to the way in which paint is applied (in fact, the viscosity of the resin is typically like that of paint). An appropriate length of the ﬁber tow sheet is then cut and placed on the wet resin layer. Plastic serrated rollers are then used to depress the

2.3

MANUFACTURING METHODS

71

ﬁber sheet into the resin, causing the ﬁbers to get wet-out by the resin and forcing excess resin and air out of the FRP composite. If insufﬁcient resin was applied initially to wet-out the ﬁbers, a second overcoat layer is applied. If additional layers of FRP tow sheet are required, additional resin is applied to the surface of the existing ﬁber layer and the procedure is repeated. Typically, no speciﬁc measures beyond rolling and forcing out the resin and air with hand rollers are used to consolidate the layup, and often no special measures are taken to ensure that a speciﬁc amount of resin is applied. Hence, the eventual volume fraction for the ﬁbers in the cured composite and the thickness of the cured composite are not controlled directly as they would be in a closed molding operation. The installer decides whether or not the ﬁber is sufﬁciently wet-out. In the same way as a wallpaper installer has a ‘‘feel’’ for how much adhesive to apply and how to squeeze out and remove air bubbles, so an FRP strengthening system installer needs to develop a feel for, and experience with, the application process. In the other case, where heavier woven fabrics are used, the method is similar; however, the fabric is usually wet-out prior to being lifted into place and applied to the structure. It is more difﬁcult to wet-out thicker and heavier woven fabrics than to wet-out thin unidirectional tow sheets, and simply placing the fabric up on the previously wet surface will not yield sufﬁcient liquid resin to wet-out the fabric. Many FRP structural strengthening systems suppliers have developed proprietary pieces of ﬁeld equipment (typically called saturators) that consist of rollers and resin baths to wet-out the fabrics just prior to installation. After the fabric is saturated with the resin in the saturator, it is rerolled onto a plastic PVC pipe and then taken to the location where it is to be installed and unrolled again onto the concrete surface. After the saturated fabric is in place, it is rolled with hand rollers to expel surplus resin and air. Somewhat better control of the resin-to-ﬁber ratio can be achieved using a saturator than with a manual method; however, precise control of the amount of resin used is still difﬁcult to achieve.13 The rate of installation in both methods depends very much on the pot life of the resin, which is the time that the mixed resin will stay in liquid form before beginning to gel and then cure. A typical epoxy resin used for structural hand layup will have a pot life of 1 to 4 hours between 60 and 80⬚F (15 and 27⬚C). At higher ambient temperatures pot life decreases, and at low temperatures some resins will not cure. Therefore, a surface area that can reasonably be covered in this amount of time by two installers is usually selected. If multiple layers of the FRP are to be used, all the layers must be cured simultaneously, and therefore all the layers must be applied when the resin is still wet.

13 Some manufacturers recommend that a speciﬁc ﬁber-to-resin volume or weight ratio be used with their systems and provide instructions for weighing wet samples in the ﬁeld to determine the appropriate resin quantity.

72

MATERIALS AND MANUFACTURING

Fiber System for Hand Layup Two primary types of ﬁber systems are used when the hand-layup method is used for FRP strengthening: unidirectional tow sheets and uni- or multidirectional woven or stitched fabrics. Carbon and E-glass are the most commonly used ﬁber types; however, some manufacturers do supply aramid ﬁber fabrics and also hybrid ﬁber fabrics. AR-glass ﬁber fabrics can be obtained for corrosive environments. Carbon Fiber Tow Sheets The term tow sheet is used to describe a wide, dry carbon ﬁber product in which individual carbon tows, usually 12K tows, are aligned parallel to each other and held in place by an open-weave glass ﬁber scrim cloth and epoxy-soluble adhesive. The scrim cloth is oriented at a Ⳳ45⬚ angle to the tow ﬁber as shown in Fig. 2.12. It is called a sheet, to differentiate it from a fabric, because it is very thin and is not woven or stitched. The tow sheet is supplied with a waxed paper backing to keep the thin layers separate and to aid in unrolling during installation. The thickness of a carbon ﬁber tow sheet is on the order of 0.005 to 0.015 in. (0.127 to 0.381 mm), and it weighs from 5 to 9 oz/yd2 (150 to 400 g/m2). The ﬁbers in the tow sheet are straight and are called stretched ﬁbers by some manufacturers. They do not have the undulating form that ﬁbers in a woven fabric have due to the warp and weft weave. Unlike prepreg sheets, the ﬁbers in tow sheets are not preimpregnated with a resin system and tow sheets should not be confused with prepregs, even though they are similar in appearance. Carbon ﬁber tow sheets are supplied in widths from 12 to 40 in. (300 to 1000 mm) and are available in standard and high-modulus carbon ﬁbers. Carbon

Figure 2.12 Carbon ﬁber tow sheet.

2.3

MANUFACTURING METHODS

73

ﬁber tow sheets of this type were ﬁrst produced in Japan in the 1980s by the Tonen Corporation (now the Nippon Steel Composites Company Ltd.) and were known as the Forca tow sheet (FTS). The term tow sheet is the preferred term to use to describe a carbon ﬁber product that has continuous ﬂat ﬁbers held together by a very lightweight scrim cloth. However, this nomenclature is, unfortunately, not universal. Some manufacturers refer to conventional stitched fabrics (where the transverse ﬁber is a structural ﬁber and not a scrim ﬁber used solely to hold the primary longitudinal ﬁbers in place) as tow sheets, and to tow sheets as fabrics. A number of manufacturers also refer to glass ﬁber tow sheets, which are usually woven with a very sparse and lightweight weft roving. For this reason, a structural engineer should always request to see a sample of the actual product being used in a structural design and listed in the project speciﬁcations and should not rely solely on verbal or written descriptions of the product. It is important to note that the thickness measurement given for a carbon ﬁber tow sheet is a nominal measurement and is the average thickness of the ﬁbers only and is not the thickness of the tow sheet after it has been impregnated with resin and cured. In addition, the longitudinal strength and stiffness properties generally reported by manufacturers for a tow sheet are the properties of the ﬁber only and are not the properties of the FRP composite material. Carbon and Glass Fiber Fabrics The other large family of ﬁber products used for FRP strengthening applications are of the woven or stitched fabric type. These fabrics are similar to those used in pultrusion applications; however, they are typically supplied with a predominantly 0⬚ ﬁber system (or a unidirectional ﬁber system), as shown in Fig. 2.13. Notice that the individual tows in the fabric product can be clearly identiﬁed, as opposed to the carbon tow sheet, where individual tows cannot be identiﬁed. The undulating pattern of the weave can also be seen in the fabric. Bidirectional fabrics with ﬁbers that are usually balanced in the 0⬚ and 90⬚ orientations are also available and can be used in cases in which bidirectional strengthening is desired, such as walls or two-way slabs. Both carbon and glass fabrics for structural strengthening are available and range in weights from 9 to 27 oz/yd2 (300 to 900 g/m2). Many of the unidirectional fabrics that are produced have a sparsely spaced (usually, at about 1 in. along the length) transverse weft ﬁber that holds the unidirectional carbon tows or glass rovings together. Fabrics are dry and are not supplied with a backing paper. Some unidirectional fabrics are supplied stitched to surfacing veils or mats similar to those used in pultruded products to hold the longitudinal ﬁbers together. Fabrics are generally available in widths up to 84 in. Resin System for Hand Layup Epoxy resins are used almost exclusively for structural hand layup for FRP strengthening applications. This is due largely to their superior adhesive properties and their low shrinkage when cured relative to polyester and vinylester resins that are used extensively in

74

MATERIALS AND MANUFACTURING

Figure 2.13 Carbon ﬁber fabric with an aramid weft ﬁber.

the industrial hand-layup method. Epoxy resins are reasonably easy to mix in the ﬁeld, typically requiring the mixing of one large amount, the epoxy resin, together with another large amount, the curing agent. This is very different from polyester and vinylester resins, which require very small percentages (often less than 1%) of catalysts and processing aids to be added at the time of mixing to process the resin. In addition, the properties of the epoxy are not as highly dependent on the mix ratios as polyester and vinylester resins, which can be affected signiﬁcantly by small amounts of additive or catalyst. For FRP strengthening applications, the epoxy resin is usually sold in a packaged system together with the ﬁber sheet or fabric and additional surface primers and putties, which are also epoxy based. These packaged epoxies are typically formulated by FRP strengthening system manufacturers to be compatible with their fabrics and sheets and to be of the appropriate viscosity to be used in the ﬁeld (either as a saturating resin or as an adhesive). These epoxies are typically unﬁlled systems that are clear to yellow or amber color. Many manufacturers pigment their brand-name epoxy resin formulations so that they are identiﬁable. Green, blue, and gray systems are common. They have a fairly low viscosity of around 500 to 1000 cP, similar to that of 10weight motor oil. They are easily rolled with paint rollers. But due to their lower viscosity, they tend to run and drip if overapplied, making the installation process somewhat messy, especially in overhead applications. It is important to note that where epoxy resins are used to saturate ﬁber sheets or to bond precured FRP strips to concrete substrates at room temper-

2.3

MANUFACTURING METHODS

75

atures, the glass transition temperature of the cured FRP strengthening system will be in the range 50 to 60⬚C (120 to 140⬚F). This temperature is close to the upper limits of the regular operating temperature of a bridge or building structure on a hot day in some parts of the world. The glass transition temperature can be increased only by postcuring the layup at elevated temperatures, which is difﬁcult to do in the ﬁeld but has been tried by a number of researchers. Nevertheless, consideration should be given to postcuring FRP strengthening systems in the ﬁeld with heaters if at all possible. As noted previously, the condition of the surface to which the FRP strengthening system is applied in the hand-layup method is very important. When the FRP strengthening system is applied to a reinforced concrete member, for example, the surface of the concrete needs to be smoothed to a speciﬁc proﬁle, sandblasted, and cleaned. If the concrete is damaged (e.g., due to corrosion), it must ﬁrst be repaired. Protrusions must be ground down. The surface must be dried and a primer must be applied to seal the concrete. Thereafter, a putty is used to ﬁll holes and cracks. After the FRP layers have been applied, a protective coating is usually applied as the last coat. An architectural ﬁnish can also be applied over the strengthening system if desired. These details must be speciﬁed by the structural engineer in the project speciﬁcations and should not be left to the FRP system installer as a ‘‘performance’’ item. Guide speciﬁcations and construction checklists published by the National Cooperative Highway Research Program in the United States should be consulted and followed (NCHRP, 2004). Epoxy resin systems used as adhesives to bond precured pultruded FRP strips have different formulations from those used in the dry ﬁber and liquid resin hand layup method. These epoxy systems, which are referred to as adhesive pastes, are typically ﬁlled with inorganic ﬁllers (silica sand, silica fume, clays) and have a much higher viscosity, in the range of 100,000 cP, and a consistency similar to that of peanut butter. They are applied with a spatula or trowel much like drywall compound (vinyl spackle). 2.3.3

Other Manufacturing Processes

A number of other processing methods are used in a limited way to produce FRP composite material parts for structural engineering applications. These processes are typically industrialized processes that produce single units (oneoff) rather than being continuous production processes like that of pultrusion (Schwartz, 1997b). Tubular products used as stay-in-place column or beam forms, or as FRP piles, are manufactured using a ﬁlament winding process from either glass or carbon ﬁbers with epoxy, vinylester, and polyester resins. In ﬁlament winding a resin-saturated ﬁber roving or tow is wound continuously around a cylindrical mandrel at a variety of wind angles. The part is cured using heaters and is then removed from the mandrel, which may be collapsible. Filament winding is used to make FRP pressure tanks and FRP poles. A planar variant of ﬁlament winding is used to manufacture FRP grids for concrete reinforcement.

76

MATERIALS AND MANUFACTURING

FRP bridge deck panels, FRP fender piles, and rigid FRP jackets for column strengthening have been produced using different variations of open and closed molding, including resin transfer molding (RTM), resin infusion molding (RIM), or vacuum-assisted resin transfer molding (VARTM). In this process the dry ﬁber forms, usually fabrics, are arranged on molds or on core materials, and the entire ﬁber form is then saturated with resin and cured. If the molded is closed, the resin is transferred under pressure and the resulting parts have two ﬁnished sides. If the mold is single sided, it is usually enclosed in a vacuum bag and the resin is infused using vacuum pressure. The resin is sucked into the vacuum bag, ﬂows through the ﬁber perform, and excess resin then exits the bag through special ports. Large bridge deck panels have been produced using this method (Bakis et al., 2002).

PROBLEMS 2.1 Find information about the FRP composite material constituents and products listed below. For each item, provide a short written description of the product, a Web page link, and a picture of the product. A&P Technology: braided fabrics Akzo: peroxides Aldrich: dimethyl analine AOC: polyester resins Ashland: hetron resins Dow: momentum resins DuPont: aramid ﬁbers Engelhard: kaolin clay ﬁllers Entec Composite Machines: pultrusion equipment Frekote: mold releases Georgia Paciﬁc: phenolic resins Hexcel: carbon epoxy prepregs Hollinee: A-glass continuous strand mats Huber Engineered Materials: ﬁllers Magnolia Plastics, Inc.: epoxy resins Nexus: veils Owens-Corning Fiberglas: E-glass continuous ﬁlament mat PPG: 113 yield glass roving Reichhold: vinylester resins Resolution Specialty Materials: epoxy resins Saint Gobain Fibers: stitched fabrics Sudaglass: basalt ﬁbers Toho: carbon ﬁbers

SUGGESTED ACTIVITIES

77

Toray: carbon ﬁbers Vectorply Corporation: multiaxial fabrics Zoltek: carbon ﬁbers SUGGESTED ACTIVITIES 2.1 Visit a pultrusion company. They usually welcome tours of students. Contact the American Composites Manufacturers Association (ACMA), the PIC (Pultrusion Industry Council), or the EPTA (European Pultrusion Technology Association) for information on nearby pultrusion companies. 2.2 Do a hand layup using standard boat cloth and polyester resin with MEKP catalyst. Obtain materials from a marine supply store (West Marine) or Fiberglast or other local source. 2.3 Obtain a sample of a pultruded proﬁle. Cut, polish, and examine the cross section with an optical microscope to see the layered structure of mats and rovings. Drill and cut the specimen with a diamond blade circular saw. Understand the need for ventilation and vacuum cleaning composite dust. Get a feel for the products and how to work with them. Bond a strain gauge to an FRP part and measure strains. 2.4 Mix up some epoxy resins. Change the part ratios and study the effect. Use a thermometer to measure the exothermic temperature. Mix similar quantities in a tall, narrow cylinder and a low, ﬂat pan and observe the differences. 2.5 Get some carbon sheet and fabric and try to cut it in a straight line! Experiment with various cutting tools. Try to cut an aramid ﬁber fabric with regular scissors. Record your observations. 2.6 Cut up a composite tennis (or squash or racquetball) racquet and look inside. Write a short paper on how composite material racquets are made. What kinds of ﬁbers and resins are used? 2.7 Purchase a quick-setting two-component epoxy from your local hardware store (⬍$5). Mix up in a plastic container (e.g., the bottom section of a disposable 0.5-L water bottle). Hold the container in your hand and feel the temperature rise. If a thermocouple is available, insert it in the epoxy while the epoxy is curing and measure the exothermic reaction temperature. Observe the change of state (liquid to solid) as the temperature changes.

3

Properties of FRP Composites

3.1

OVERVIEW

To design a structure with an FRP composite, a structural engineer must have knowledge of the physical, and especially, the mechanical properties of the FRP material being used in the design. These properties are typically provided by the manufacturer of the FRP material product. However, at this time there is no standard format for providing mechanical and physical property data. Often, incomplete property data are provided, and in many cases it is not clear if the property data reported are actual test data or have been reduced by a safety factor for design purposes. Therefore, it is important for a structural engineer to understand how properties of FRP composites are determined so that independent checks or tests can, if necessary, be conducted to verify the FRP material properties reported. Essentially, there are two ways to determine the properties of an FRP composite for use in design. The ﬁrst is via theoretical calculations, and the second is via experimental measurements. Since an FRP composite is an inhomogeneous material, it can be characterized theoretically and experimentally on a number of different levels (or scales), as discussed in Chapter 1. Structural engineers should understand what these different characterization levels are when specifying material tests or when conducting numerical modeling, such as ﬁnite element analysis. As noted in Chapter 1, an FRP composite material can be characterized on one of four levels: (1) the ﬁber level, (2) the lamina level, (3) the laminate level, and (4) the full-section level. Below, methods are described for determining the properties at each of these levels by both theoretical and experimental methods. 3.2

THEORETICAL DETERMINATION OF PROPERTIES

3.2.1

Fiber Level

Many properties of FRP composite can be predicted from the properties of the ﬁber and polymer resin system (known as the matrix in mechanics terminology1). This ﬁber-level analysis is known as micromechanics. Both phys1 The term matrix is used to designate the entire resin system, including the polymer, the ﬁllers, the additives, and the processing aids.

78

Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

3.2

THEORETICAL DETERMINATION OF PROPERTIES

79

ical and mechanical properties can be predicted using micromechanics models. Different levels of sophistication exist in micromechanics models that have been developed over the years (Bank, 1993a). For FRP composites in structural engineering, micromechanics is used for three primary reasons: (1) to relate mass or weight fractions of the constituents to their volume fractions, (2) to get estimates of the stiffness properties and selected strength properties of unidirectional composites, and (3) to approximate the longitudinal strength and longitudinal modulus of a ﬁber sheet material by ignoring the mechanical contribution of the matrix material in the longitudinal direction. For structural engineering calculations, only simple micromechanics models, based on the rule of mixtures, are commonly used for these purposes. To use micromechanics models to predict the properties of an FRP composite, the physical and mechanical properties of the ﬁber and matrix constituents need to be known. These are usually obtained by experimental methods. In simple models it is assumed that the matrix is a homogeneous material that is isotropic and linear elastic. At the ﬁrst approximation the ﬁbers are also usually assumed to be homogeneous, isotropic, and linear elastic.2 Assuming that there are no voids in the FRP composite, the relationship between the weight (or mass) fractions, w, and the volume fractions, v, of the ﬁber (subscript ƒ) and matrix (subscript m) constituents of an FRP composite (subscript c) are

vƒ ⫽ wƒ

c ƒ

(3.1a)

vm ⫽ wm

c m

(3.1b)

c ⫽ vƒƒ ⫹ vm m ⫽

1 wƒ / ƒ ⫹ wm / m

(3.1c)

vƒ ⫹ vm ⫽ 1

(3.1d)

wƒ ⫹ wm ⫽ 1

(3.1e)

vƒ ⫽

wƒ (vƒƒ ⫹ vm m) ƒ

(3.1ƒ)

2 Glass ﬁbers are, in fact, isotropic; however, carbon ﬁbers are anisotropic. If available, the anisotropic properties of the carbon ﬁber can be used in the micromechanics equations (see Tsai and Hahn, 1980).

80

PROPERTIES OF FRP COMPOSITES

vƒ ⫽

Vƒ Vc

wƒ ⫽

Wƒ Wc

(3.1g)

vm ⫽

Vm Vc

wm ⫽

Wm Wc

(3.1h)

where Vi is the volume of constituent i, Wi the weight (or mass) of constituent i, and i the weight density (or mass density) of constituent i. The mass and volume fraction relationships above are important in the production of FRP composites, since quantities of material are usually measured by weight when mixed or when priced. The four independent engineering properties of an orthotropic (or transversely, isotropic3) unidirectional FRP composite (Ex, Ey, Es, x) with known isotropic ﬁber properties (Eƒ, ƒ, Gƒ), isotropic matrix properties (Em, m, Gm), and ﬁber and matrix volume fractions (vƒ, vm) can be estimated at a ﬁrst approximation by the following rule-of-mixtures equations: Ex ⫽ vƒ Eƒ ⫹ vm Em

(3.2a)

vƒ 1 v ⫽ ⫹ m Ey Eƒ Em

(3.2b)

vƒ 1 v ⫽ ⫹ m Es Gƒ Gm

(3.2c)

x ⫽ vƒƒ ⫹ vmm

(3.2d)

y Ex ⫽ x Ey

(3.2e)

where Ex is the longitudinal modulus in the ﬁber direction, Ey the transverse modulus perpendicular to the ﬁber direction, Es the in-plane shear modulus, x the longitudinal (or major) Poisson ratio, and y the transverse (or minor) Poisson ratio.4 The longitudinal tensile strength of a unidirectional composite, Xt, which is dominated by the properties of the ﬁber, can be estimated at a ﬁrst approximation by

冉 冊

Xt ⫽ vƒ ult ƒ,t ⫹ vm Em

ult ƒ,t Eƒ

(3.3)

3 The transversely isotropic composite is the three-dimensional version of the two-dimensional unidirectional composite. It has ﬁve independent constants, the four noted above plus an out-ofplane Poisson ratio (see Bank, 1993a). 4 The stiffness properties of a unidirectional composite are discussed further below.

3.2

THEORETICAL DETERMINATION OF PROPERTIES

81

where ult ƒ,t is the ultimate tensile strength (UTS) of the ﬁber and it is assumed that in the longitudinal direction the ﬁber fails before the matrix. The second term in the equation is usually small, and therefore the longitudinal tensile strength of a unidirectional composite can be approximated conservatively by Xt ⫽ vƒ ult ƒ,t

(3.4)

When the ﬁbers are continuous, as is typically the case, the ﬁber volume fraction is often replaced by the ﬁber area fraction, aƒ. This leads to the equation often used with FRP strengthening systems for the modulus (EFRP) and the strength (FRP) of the strengthening system when the contribution of the polymer matrix is ignored, as EFRP ⫽ aƒ Eƒ

(3.5)

FRP ⫽ aƒ ƒult

(3.6)

The transverse tensile strength, Yt, the longitudinal compressive strength, Xc, the transverse compressive strength, Yc, and the in-plane shear strength, S, are all matrix-dominated properties and are signiﬁcantly lower than the longitudinal tensile strength. Equations to estimate their values can be found in Agarwal and Broutman (1990); however, these are regarded only as order-ofmagnitude estimates. Reliable theoretical equations for prediction of the properties in the matrix-dominated failure modes as a function of the properties of the ﬁber and the matrix are not available. The expansion and transport properties of an FRP composite can also be predicted at a ﬁrst approximation from the constituent properties of the ﬁber and the matrix material. In a unidirectional FRP composite, these properties are anisotropic, and values need to be determined for both the longitudinal and transverse directions of the composite. The coefﬁcients of thermal expansion, ␣x and ␣y, and the coefﬁcients of moisture expansion, x and y, are used to determine the longitudinal and transverse strains in an FRP composite when subjected to thermal or hygroscopic loads. The transport properties, which also have both longitudinal and transverse values, are diffusivity, Dx and Dy; the thermal conductivity, kx and ky; the electrical conductivity, ex and ey; and the magnetic permeability, mx and my. Both the hygroscopic expansion coefﬁcients and the transport coefﬁcients are usually predicted at a ﬁrst approximation using the rule of mixtures for the longitudinal and transverse directions, respectively, and the ﬁber and matrix constituents are usually assumed to have isotropic hygroscopic and transport properties (Bank, 1993a). Other important physical properties of an FRP composite that have a signiﬁcant inﬂuence on the long-term durability of the composite, such as the glass transition temperature, the fatigue life, creep compliance, ignition and

82

PROPERTIES OF FRP COMPOSITES

combustion temperatures, impact resistance, and damping ratios, are not generally predicted from micromechanics (see Bank, 1993a). The glass transition temperature, Tg, of the unidirectional FRP composite is often assumed to be equal to the glass transition temperature of the matrix material. Analysis Example 3.15 An E-glass/vinylester unidirectional rod is to be used as an FRP reinforcing bar. The rod has an 80% ﬁber weight fraction. Assuming that there are no voids in the composite, determine the ﬁber volume fraction and the stiffness properties of the composite rod. You are given the following properties for the ﬁber and the matrix: E-glass fiber:

ƒ ⫽ 9.4 ⫻ 10⫺2 lb/in3, Eƒ ⫽ 10.5 ⫻ 106 psi, ƒ ⫽ 0.20

Vinylester matrix: m ⫽ 4.57 ⫻ 10⫺2 lb/in3, Em ⫽ 500,000 psi, m ⫽ 0.38 SOLUTION Gƒ ⫽

Gm ⫽

Eƒ 2(1 ⫹ ƒ) Em 2(1 ⫹ m)

⫽ 4.375 ⫻ 106 psi

⫽ 181,159 psi

c ⫽ vƒƒ ⫹ vm m ⫽

1 wƒ / ƒ ⫹ wm / m

⫽

1 0.8/0.094 ⫹ 0.2/0.0457

⫽ 0.0776 lb/in3 vƒ ⫽ wƒ

冉 冊

c 0.0776 ⫽ 0.8 ⫽ 0.66 ƒ 0.094

Ex ⫽ vƒ Eƒ ⫹ vm Em ⫽ 0.66(10.5 ⫻ 106) ⫹ 0.34(0.5 ⫻ 106) ⫽ 7.1 ⫻ 106 psi vƒ 1 v 0.66 0.34 ⫽ ⫹ m ⫽ ⫹ Ey Eƒ Em 10.5 ⫻ 106 0.5 ⫻ 106 ⫽ 7.42 ⫻ 10⫺7 ⇒ Ey ⫽ 1.35 ⫻ 106 psi

5 In analysis examples in this book, results are often provided to three or even four signiﬁcant ﬁgures to enable the reader to follow the calculations. However, such precision is not advised for practical engineering calculations since the properties of the constituents are known only to one or two signiﬁcant ﬁgures.

3.2

THEORETICAL DETERMINATION OF PROPERTIES

83

vƒ 1 v 0.66 0.34 ⫽ ⫹ m ⫽ ⫹ 6 Es Gƒ Gm 4.375 ⫻ 10 0.181 ⫻ 106 ⫽ 2.029 ⫻ 10⫺6 ⇒ Es ⫽ 492,778 psi

x ⫽ vƒƒ ⫹ vmm ⫽ 0.66(0.20) ⫹ 0.34(0.38) ⫽ 0.26 y ⫽

3.2.2

Ey 1.35 ⫽ (0.26) ⫽ 0.049 Ex x 7.1

Lamina Level

A single ply (or lamina) of a planar FRP composite material that contains all of its ﬁbers aligned in one direction is called a unidirectional ply. The unidirectional ply plays a key role in characterizing the behavior of FRP composites in structural engineering for the following reasons: (1) Many FRP products used in structural engineering, such as FRP rebars, FRP sheets, and FRP fabrics, are used in the unidirectional form as the FRP end product; (2) the properties of FRP composites are often obtained experimentally by testing unidirectional FRP materials; and (3) the unidirectional ply is the basic building block for calculating the properties of a multidirectional FRP laminate, often used to represent the walls of a pultruded proﬁle or the structure of a hand-laid-up composite. It is assumed that the unidirectional ply is a two-dimensional plate and that its thickness is very small compared to its in-plane dimensions. The constitutive relations (or the stress–strain relations) for a unidirectional ply deﬁne the relationships between the in-plane stresses (x, y, s) and the inplane strains (x, y, s) in a local or ply x,y,s coordinate system.6 The global or structural in-plane coordinate system is deﬁned as a 1,2,6 coordinate system, and the stresses and strains in the global system are 1, 2, 6 and 1, 2, 6, respectively.7 The ply is assumed to be linear elastic and orthotropic with the local x-axis aligned parallel to the ﬁber direction and the local yaxis perpendicular to the ﬁber direction. Tensile and compressive moduli are assumed to be equal. As shown in Fig. 3.1, the angle, , measured counterclockwise from the global 1-direction to the local x-direction, deﬁnes the inplane relationship between the orthogonal coordinate systems.

6 This chapter follows the notation, terminology, and sign convention of Tsai and Hahn (1980). In many other texts, the local coordinate system is identiﬁed as the (L,T,LT) system (longitudinal, transverse, and shear orientations). The global coordinate system is often identiﬁed as the (1,2,12) or (11,22,12) system. 7 This form is known as the contracted notation. The shear direction is the s or the 6 direction. The shear strain in this notation is the engineering shear strain and is equal to twice the tensorial shear strain (i.e., s ⫽ ␥xy ⫽ xy ⫹yx and 6 ⫽ ␥12 ⫽ 12 ⫹ 21).

84

PROPERTIES OF FRP COMPOSITES

2

y

x θ 1

Figure 3.1 In-plane coordinate systems for a unidirectional FRP lamina.

The unidirectional ply is orthotropic in the x,y,s coordinate system but anisotropic in the 1,2,6 coordinate system.8 The stress–strain relations in the x,y,s coordinate system, also called the on-axis orientation, in terms of the ﬁve engineering constants (Ex, Ey, x, y, and Es) of the unidirectional ply are expressed most conveniently in compliance form as

冦冧 s y s

⫺y 1 Ex Ey ⫺x 1 ⫽ Ex Ey

冤 冥 0

0

0 0

1 Es

冦冧 x y s

(3.7)

or in indicial form as i ⫽ Sijj

(i,j ⫽ x,y,s)

(3.8)

where the longitudinal modulus, Ex, the transverse modulus, Ey, the major Poisson ratio, x, the minor Poisson ratio, y, and the in-plane shear modulus, Es,9 are deﬁned as

8

The unidirectional ply is often referred to in the literature as specially orthotropic, since it is orthotropic in the global system only when is zero. 9 The shear modulus is often denoted by the letter G and deﬁned as G ⫽ / ␥.

3.2

Ex ⫽

THEORETICAL DETERMINATION OF PROPERTIES

x 1 ⫽ x Sxx

(x ⫽ 0, y, s ⫽ 0)

y Syx x ⫽ ⫺ ⫽ ⫺ x Sxx

Ey ⫽

y 1 ⫽ y Syy

Es ⫽

(3.9a)

(x ⫽ 0, y, s ⫽ 0)

(y ⫽ 0, x, s ⫽ 0)

Sxy y ⫽ ⫺ x ⫽ y Syy s 1 ⫽ s Sss

85

(3.9b) (3.9c)

(y ⫽ 0, x, s, ⫽ 0) (s ⫽ 0, x, y ⫽ 0)

(3.9d) (3.9e)

Since the compliance matrix, Sij, is symmetric, only four of the engineering constants are independent. The minor Poisson ratio is found using the symmetry relations y ⫽

Ey Ex x

(3.10)

It is important to note that the shear modulus is an independent quantity for an orthotropic ply and cannot be determined from the isotropic relation: G⫽

E

(3.11)

2(1 ⫹ )

For an isotropic material plate (or ply), Ex ⫽ Ey ⫽ E, x ⫽ y ⫽ , and Es ⫽ G, of which only two of the three constants are independent. In addition, these elastic constants are independent of orientation. For laminate calculations the stiffness form of the stress strain relations is preferred and is given as

冦冧 x y s

冤

y Ex Ex 1 ⫺ xy 1 ⫺ xy x Ey Ey ⫽ 1 ⫺ xy 1 ⫺ xy

or in indicial notation as

0

0

0 0

冥

Es

冦冧 x y s

(3.12)

86

PROPERTIES OF FRP COMPOSITES

i ⫽ Qijj

(i,j ⫽ x,y,s)

(3.13)

where the Qij are the ply on-axis stiffness coefﬁcients. When the unidirectional ply is rotated through a counterclockwise angle, , into an off-axis orientation as shown in Fig. 3.1, the stresses and strains in the local x,y,s ply coordinate system can be obtained from the stresses and strains in the global 1,2,6 coordinate system using the following transformation equations:

冦冧 冤 冦冧 冤 x y s

⫽

cos2 sin2 ⫺cos sin

x y s

cos2 ⫽ sin2 ⫺2 cos sin

sin2 cos2 cos sin

冥冦 冧 冥冦 冧

2 cos sin ⫺2 cos sin cos2 sin2

1 2 6

sin2 cos sin cos2 ⫺cos sin 2 cos sin cos2 sin2

1 2 6

(3.14a)

(3.14b)

In addition, the anisotropic off-axis stiffness coefﬁcients of the unidirectional ply can be obtained in terms on the orthotropic on-axis stiffness coefﬁcients from

冦冧冤

Q11 cos4 Q22 sin4 Q12 cos2 sin2 ⫽ Q66 cos2 sin2 Q16 cos3 sin Q26 cos sin3

sin4 cos4 cos2 sin2 cos2 sin2 ⫺cos sin3 ⫺cos3 sin

冥冦 冧

2 cos2 sin2 4 cos2 sin2 2 2 2 cos sin 4 cos2 sin2 4 4 cos ⫹ sin ⫺4 cos2 sin2 2 2 ⫺2 cos sin (cos2 ⫺ sin2)2 3 3 cos sin ⫺ cos sin 2(cos sin3 ⫺ cos3 sin ) cos3 sin ⫺ cos sin3 2(cos3 sin ⫺ cos sin3)

Qxx Qyy Qxy Qss

(3.15)

The six independent off-axis compliance coefﬁcients can be obtained directly from the on-axis compliance coefﬁcients or by inversion of the 3 ⫻ 3 stiffness matrix as follows: Sij ⫽ Qij⫺1

(i,j ⫽ 1,2,6)

(3.16)

The compliance matrix for the off-axis ply can be written in terms of nine off-axis ‘‘effective’’ engineering constants (of which six are independent) as follows:

3.2

THEORETICAL DETERMINATION OF PROPERTIES

冦冧 1 2 6

冤 冥

1 16 ⫺ 12 E1 E2 E6 21 1 26 ⫽ E1 E2 E6 61 62 1 E1 E2 E6

冦冧 1 2 6

87

(3.17)

or i ⫽ Sijj

(i,j ⫽ 1,2,6)

(3.18)

The off-axis engineering constants are deﬁned as E1 ⫽

1 1 ⫽ 1 S11

(1 ⫽ 0, 2, 6 ⫽ 0) longitudinal modulus

21 ⫽ ⫺

2 S ⫽ ⫺ 21 1 S11

(1 ⫽ 0, 2, 6 ⫽ 0) major Poisson ratio

61 ⫽

6 S ⫽ 61 1 S11

2 1 ⫽ 2 S22

1 S ⫽ ⫺ 12 2 S22

6 S ⫽ 62 2 S22

6 1 ⫽ 6 S66

(3.19e)

(2 ⫽ 0, 1, 6 ⫽ 0) shear–transverse coupling ratio

E6 ⫽

(3.19d)

(2 ⫽ 0, 1, 6 ⫽ 0) minor Poisson ratio

62 ⫽

(3.19c)

(2 ⫽ 0, 1, 6 ⫽ 0) transverse modulus

12 ⫽ ⫺

(3.19b)

(1 ⫽ 0, 2, 6 ⫽ 0) shear–longitudinal coupling ratio

E2 ⫽

(3.19a)

(3.19ƒ)

(6 ⫽ 0, 1, 2 ⫽ 0) in-plane shear modulus

(3.19g)

88

PROPERTIES OF FRP COMPOSITES

16 ⫽

1 S ⫽ 16 6 S66

(6 ⫽ 0, 1, 2 ⫽ 0) longitudinal–shear coupling ratio

26 ⫽

2 S ⫽ 26 6 S66

(3.19h)

(6 ⫽ 0, 1, 2 ⫽ 0) transverse–shear coupling ratio

(3.19i)

Due to symmetry of the compliance matrix, only six of these constants are independent. Usually, E1, E2, E6, 21, 61, and 62 are determined experimentally from uniaxial and pure shear tests, and 12, 16, 26 are calculated using the symmetry relations. Note that Sij ⫽ Sji but that ij ⫽ ji. The strength of a unidirectional ply is typically described by ﬁve independent ultimate stresses (called strengths) and ﬁve independent ultimate strains (called rupture strains). The ﬁve strengths of the unidirectional ply are the longitudinal tensile strength, Xt; the longitudinal compressive strength, Xc; the transverse tensile strength, Yt; the transverse compressive strength, Yc; and the in-plane shear strength, S. The failure strains are the longitudinal tensile rupture strain, xt ; the longitudinal compressive rupture stain, xc; the transverse tensile rupture strain, yt ; the transverse compressive rupture strain, yc; and the in-plane shear rupture strain, s. The strengths are typically obtained from uniaxial and pure shear tests. Both strengths and rupture strains are used to deﬁne the ultimate capacity of a unidirectional ply even though it is assumed for the purpose of stress analysis that the unidirectional ply is linear elastic (which would mean that the rupture strain could be calculated directly from the strengths and the moduli). However, in reality, the unidirectional ply is not linear elastic, especially in the transverse and shear directions at moderate to high stress levels (see Adams et al., 2003). Therefore, whereas the linear elastic assumption is reasonable for prediction of the behavior of the unidirectional ply at service load stresses, it is not appropriate when the unidirectional ply is subjected to loads that approach its ultimate stresses and strains. When the unidirectional ply is subjected to a uniaxial state of stress or strain, failure is determined by comparing the applied stress or strain to the corresponding strength or rupture strain. In the case of FRP composites for structural engineering, this is often the case for unidirectional products such as FRP rebars and strips and sheets. However, if a multiaxial state of stress and strain exists in the unidirectional ply due to a complex set of applied loads, or if the ply is loaded in its off-axis orientation, a multiaxial failure criterion needs to be employed to predict the combination of loads under which the unidirectional ply will fail. The most popular failure criteria used today are the maximum stress failure criterion, the maximum strain failure criterion, the Tsai–Wu quadratic failure criterion, and the Tsai–Hill (or maximum work) failure criterion (Tsai and Hahn, 1980; Agarwal and Broutman,

3.2

THEORETICAL DETERMINATION OF PROPERTIES

89

1990; Daniel and Ishai, 1994; Adams et al., 2003). Of these criteria, the ﬁrst two do not account for the interactive effect of multiaxial stresses and strains, whereas the latter two do account for these effects. 3.2.3

Laminate Level

A multidirectional laminate is constructed from a number of unidirectional plies that are stacked at various on- and off-axis angles relative to the global 1,2,6 axes. A stacking sequence is used to deﬁne the layup. The stacking sequence shows the individual plies of the laminate, from the bottom ply to the top ply, in an ordered sequence of angles of the plies, such as [0/90/ ⫹45/ ⫺45]. It is generally assumed that all plies have equal thickness. If they do not, or they are made of different materials, the stacking sequence notation is modiﬁed to indicate this. Depending on the stacking sequence, a multidirectional laminate may be orthotropic or anisotropic in its plane or out of its plane and may have coupling between in-plane and out-of plane responses. In-plane response is known as extensional response and out-of-plane response is known as ﬂexural response. Classical lamination theory (CLT) is generally used as a ﬁrst approximation to describe the constitutive relations of a thin laminate. According to CLT, the in-plane response is described by three extensional stress resultants, N1, N2, N6, and the out-of-plane response is described by three ﬂexural stress resultants, M1, M2, M6.10 Corresponding to these stress resultants are six generalized strain resultants: the midplane strains, 01, 02, 06 and the plate curvatures, 1, 2, 6. The general constitutive relation for a multidirectional laminate is given as

冦冧冤

N1 A11 N2 A21 N6 A61 ⫽ M1 B11 M2 B21 M6 B61

A12 A22 A62 B12 B22 B62

A16 A26 A66 B16 B26 B66

冥冦 冧

B11 B12 B16 B21 B22 B26 B61 B62 B66 D11 D12 D16 D21 D22 D26 D61 D62 D66

01 02 06 1 2 6

(3.20)

The stiffness matrix above is often referred to as the [A–B–D] matrix. The Aij terms deﬁne the extensional response, the Dij terms the ﬂexural response, and the Bij terms the extension-bending coupled response.11 Note that the entire [A–B–D] matrix is symmetric and that the [A], [B], and [D] submatrices themselves are symmetric so that the [A–B–D] matrix has at most 18 inde-

10 Note that the in-plane resultants N have units of force / length, whereas the moments M have units of force since the resultants are deﬁned per unit width of the laminate. 11 The A terms have units of force / length, the B terms units of force, and the D terms units of force ⫻ length.

90

PROPERTIES OF FRP COMPOSITES

pendent terms. The [A–B–D] matrix can be obtained by summation of the stiffness coefﬁcients of the individual on- and off-axis plies as follows:

冘 Q (z ⫺ z n

Aij ⫽

k ij

k

k⫽1

Bij ⫽ Dij ⫽

冘Qh n

k⫺1) ⫽

k ij k

1 2

冘 Q (z ⫺ z

)⫽

k⫽1

1 3

冘 Q (z ⫺ z

)⫽

n

k ij

2 k

3 k

k⫽1

冘 Q (⫺z h ) n

2 k⫺1

k ij

(3.22)

k k

k⫽1

n

k ij

(3.21)

k⫽1

冘 Q 冉h z ⫹ 12h 冊 n

3 k⫺1

k ij

2 k k

3 k

(3.23)

k⫽1

where zk is the distance from the midplane to the top of ply k, zk the distance to the middle of ply k, hk the thickness of ply k, and n the total number of plies in the laminate, as shown in Fig. 3.2. Note that the coordinate z is positive for a ply above the midplane and negative for a ply below the midplane. A very common class of laminates is the class in which the layup is symmetric about the midplane. This implies that for every material type, orientation, and thickness of ply below the midplane there exists an identical (a mirror image) ply above the midplane at the identical distance from the midplane. In this case, the B submatrix is identically zero. Only in very special circumstances are unsymmetric laminates used. Their use in structural engineering should be avoided unless their unique properties are beneﬁcial. Unsymmetric laminates have extensional-bending coupling that can affect the response of thin laminates, especially those used for strengthening applications.12

k=n

k=i

midplane, z = 0

z k = z1

zk = z1 k=2

hk = h2

k=1

Figure 3.2 Laminate notation.

12

Extensional-bending coupling can cause undesirable debonding of FRP strengthening strips.

3.2

THEORETICAL DETERMINATION OF PROPERTIES

91

In a symmetric laminate the extensional and bending responses are uncoupled (although they can have bending–twisting coupling) and the individual [A] and [D] submatrices can be inverted separately13 to give extensional and bending compliance matrices, known as the [a] and the [d] matrices, as follows: aij ⫽ A⫺1 ij

(i,j ⫽ 1,2,6)

(3.24)

dij ⫽ Dij⫺1

(i,j ⫽ 1,2,6)

(3.25)

Effective in-plane engineering constants can then be deﬁned for the symmetric laminate of thickness, h, by deﬁning an average in-plane stress in the laminate, , as follows: i ⫽

Ni (i ⫽ 1,2,6) h

(3.26)

The compliance relationship then becomes 0i ⫽ haijj

(i,j ⫽ 1,2,6)

(3.27)

or

01 02 06

冦冧

冤

1 E 01 0 ⫽ ⫺ 210 E1 0 61 E 01

⫺

012 E 02

016 E 06

0 1 26 0 E 2 E 60 0 62 1 0 E 2 E 06

冥

1 2 6

冦冧

(3.28)

The nine effective in-plane (also known as extensional) engineering constants are deﬁned analogously to the engineering constants for the off-axis unidirectional ply [see equations (3.19a) to (3.19i)]; for example, E 01 ⫽

1 1 ⫽ 01 a11h

(1 ⫽ 0, 2 ⫽ 6 ⫽ 0) longitudinal in-plane modulus

(3.29a)

13 Note that in the general case, when Bij ⫽ 0 the full 6 ⫻ 6 stiffness matrix must be inverted to obtain the compliance matrix.

92

PROPERTIES OF FRP COMPOSITES

E 06 ⫽

6 1 ⫽ 06 a66h

(6 ⫽ 0, 1 ⫽ 2 ⫽ 0) shear in-plane modulus

0 21 ⫽⫺

02 a ⫽ ⫺ 21 0 1 a11

(3.29b)

(1 ⫽ 0, 2 ⫽ 6 ⫽ 0) Major in-plane Poisson ratio

(3.29c)

0 0 0 0 0 and analogously for E 02, 12 , 16 , 61 , 26 , 62 . In a similar fashion, effective engineering ﬂexural properties can be deﬁned in terms of the effective stress at the outer surface, deﬁned as14

ƒi ⫽

6Mi h2

(i ⫽ 1,2,6)

(3.30)

and the actual strain at the outer surface, deﬁned as ƒi ⫽

i h 2

(i ⫽ 1,2,6)

(3.31)

The effective ﬂexural stress–strain relation is then deﬁned as ƒi ⫽

h3 d ƒ 12 ij j

(i,j ⫽ 1,2,6)

(3.32)

which in terms of the effective ﬂexural engineering constants is written as

ƒ1 ƒ2 6ƒ

冦冧

冤

1 Eƒ1 ƒ ⫽ ⫺ 21 Eƒ1 ƒ 61 Eƒ1

ƒ ⫺ 12 ƒ

冥

ƒ16 Eƒ6

E2 ƒ 1 26 Eƒ2 Eƒ6 ƒ 62 1 Eƒ2 Eƒ6

ƒ1 ƒ2 6ƒ

冦冧

(3.33)

where, for example,

14 This terminology follows Tsai (1988). In plate theory, a positive bending moment is generally deﬁned as ‘‘tension on the top,’’ which is opposite to that used in conventional beam theory.

3.2

Eƒ1 ⫽

ƒ1 12 ⫽ 1ƒ d11h3

THEORETICAL DETERMINATION OF PROPERTIES

( ƒ1 ⫽ 0, ƒ2, ƒ6 ⫽ 0) longitudinal ﬂexural modulus

Eƒ6 ⫽

ƒ6 12 ⫽ 6ƒ d66h3

(3.34a)

( ƒ6 ⫽ 0, ƒ1, ƒ2 ⫽ 0) twisting (shear–ﬂexural) modulus

ƒ21 ⫽ ⫺

93

ƒ2 d ⫽ ⫺ 21 1ƒ d11

(3.34b)

( ƒ1 ⫽ 0, ƒ2, ƒ6 ⫽ 0) longitudinal ﬂexural Poisson ratio (3.34c)

and analogously for the remaining six effective ﬂexural engineering constants, Eƒ2, ƒ12, ƒ16, ƒ61, ƒ26, ƒ62, following the same logic as equations (3.19a) to (3.19i) for the off-axis engineering constants deﬁned previously. In structural engineering, every effort is made to use laminates that in addition to being symmetric, have in-plane orthotropic properties so that no coupling exists between in-plane extension and in-plane shear (i.e., A16 ⫽ A26 ⫽ A61 ⫽ A62 ⫽ 0). Only speciﬁc types of symmetric laminates have no extension–shear coupling. These are: (1) cross-ply laminates, in which the laminate consists of only 0⬚ and 90⬚ plies (e.g., a 0/0/90/90/0/0 laminate); (2) balanced laminates, in which for every ply at a positive off-axis orientation there exists a ply at a negative off-axis orientation (e.g., a ⫺30/ ⫹30/ ⫹30/ ⫺30 laminate); and (3) quasi-isotropic laminates, in which the ply angles are separated by an angle of 360⬚ divided by the total number of plies in the laminate, n, where n is an even number equal to or greater than 6 (e.g., a ⫺60/60/0/0/60/ ⫺60 laminate). Note that for a quasi-isotropic laminate the in-plane properties are not direction dependent and that the isotropic relationship between the engineering constants holds (hence the name quasiisotropic15), E 01 ⫽

E 06 2(1 ⫹ ) 0 21

⫽

E 06 2(1 ⫹ 012)

(3.35)

Of the three type of laminates described above, only the symmetric cross-ply laminate is also orthotropic in its ﬂexural properties (i.e., D16 ⫽ D26 ⫽ D61 ⫽ D62 ⫽ 0). A number of unique types of laminates exist that have ﬂexural orthotropy but not in-plane orthotropy (an example of this is the unsymmetric

15 The laminate is known as quasi-isotropic since it is not isotropic in the thickness direction nor isotropic with respect to its ﬂexural properties.

94

PROPERTIES OF FRP COMPOSITES

angle-ply laminate, ⫹ / ⫺ / ⫹ / ⫺, commonly produced by the ﬁlament winding process). In structural engineering applications, laminates are typically thin relative to their two in-plane dimensions, and loaded in-plane, and therefore most attention is paid to their in-plane properties. In rare situations such as in thinshell structures, where laminates are loaded out-of-plane, their ﬂexural properties may be used. Consequently, in design procedures for FRP composites for structural engineering the in-plane effective engineering properties of the laminate are used in calculations involving sheets, strips, and thin-walled sections. The strengths (and ultimate strains) of an FRP composite laminate are difﬁcult to predict, and a variety of mechanics models are used to estimate when a laminate will fail due to the loads applied. The general procedure is to determine the stresses and strains in each ply of the laminate as the laminate is loaded in an incremental fashion. At each load increment the stress state in the ply is checked with regard to one of the failure criteria for the unidirectional ply described previously. When the ﬁrst ply fails (i.e., satisﬁes its failure criterion), the condition is known as ﬁrst ply failure (FPF). However, a multidirectional laminate can often continue to carry additional loads beyond its FPF load. A nonlinear analysis must then be performed using reduced stiffnesses for the laminate’s surviving plies (see Agarwal and Broutman, 1990). Often, the ﬁrst ply failure condition is used as a conservative criterion to deﬁne laminate failure for design purposes. Computer programs are available to perform simple nonlinear calculations16 to determine the FPF and ultimate failure loads of two-dimensional laminates according to commonly used failure criteria. They are useful for obtaining an order-of-magnitude estimate of the ultimate strengths of a laminate when loaded by a speciﬁc set of applied loads. For structural engineering design the strength and rupture strain properties of the laminate are usually obtained by experimental testing in a fashion similar to that used to determine the strength properties for an on-axis unidirectional ply. Since, as noted previously, most laminates used in structural engineering are orthotropic, in-plane testing along the orthotropy axes is an effective means of obtaining both the strength and stiffness properties of laminates for design purposes. Analysis Example 3.2 Given is a three-layer E-glass/polyester pultruded composite material with a thickness of 0.125 in. The composite consists of two outer layers of continuous ﬁlament mat17 (CFM) with a thickness of 0.020 in. each and an internal layer of unidirectional rovings with a thickness of 0.085 in. The continuous ﬁlament mat has a 23% glass ﬁber volume fraction and the following quasi-isotropic mechanical properties:

16 17

CompositePro, Peak Innovations, Littleton, Colorado, for example. Also known as continuous strand mat (see Chapter 2).

3.2

THEORETICAL DETERMINATION OF PROPERTIES

95

Ex ⫽ 0.91 ⫻ 106 psi Ey ⫽ 0.91 ⫻ 106 psi Es ⫽ 0.34 ⫻ 106 psi x ⫽ 0.35

The unidirectional roving layer has a 51% ﬁber volume fraction and the following orthotropic mechanical properties: Ex ⫽ 5.66 ⫻ 106 psi Ey ⫽ 1.50 ⫻ 106 psi Es ⫽ 0.48 ⫻ 106 psi x ⫽ 0.28

It is assumed that the tensile and compressive moduli are equal for both layers. For the FRP composite material given, determine (a) the in-plane stiffness coefﬁcients, Qij, for the continuous ﬁlament mat layer; (b) the in-plane stiffness coefﬁcients, Qij, for the unidirectional roving layer; (c) the [A] and [D] matrices (indicate the units for the terms in the matrices); and (d) the effective in-plane and ﬂexural engineering properties for the layup. SOLUTION (a) Determine Qij for the CFM layers: y ⫽ x

Ey ⫽ 0.35 Ex

m ⫽ (1 ⫺ xy)⫺1 ⫽ 1.140 Qxx ⫽ mEx ⫽ 1.140(0.91 ⫻ 106) ⫽ 1.037 ⫻ 106 psi Qyy ⫽ Qxx ⫽ 1.037 ⫻ 106 psi Qxy ⫽ Qyx ⫽ mx Ey ⫽ 3.630 ⫻ 105 psi Qss ⫽ Es ⫽ 0.34 ⫻ 106 psi

96

PROPERTIES OF FRP COMPOSITES

(b) Determine Qij for the unidirectional (UD) layer: y ⫽ x

Ey ⫽ 0.074 Ex

m ⫽ (1 ⫺ xy)⫺1 ⫽ 1.021 Qxx ⫽ mEx ⫽ 1.021(5.66 ⫻ 106) ⫽ 5.780 ⫻ 106 psi Qyy ⫽ mEy ⫽ 1.532 ⫻ 106 psi Qxy ⫽ Qyx ⫽ mx Ey ⫽ 4.2789 ⫻ 105 psi Qss ⫽ Es ⫽ 0.48 ⫻ 106 psi (c) To determine the [A–B–D] matrix, determine z values assuming that the middle UD layer is divided into two equal-thickness layers about the midplane: z0 ⫽ ⫺0.0625 in.

z3 ⫽ 0.0425 in.

z1 ⫽ ⫺0.0425 in.

z4 ⫽ 0.0625 in.

z2 ⫽ 0.0

冘 Q (z ⫺ z n

Aij ⫽

k ij

k

)

k⫺1

k⫽1

A11 ⫽ 2{(1.037 ⫻ 106)[⫺0.0425 ⫺ (⫺0.0625)] ⫹ (5.780 ⫻ 106)[0.0 ⫺ (⫺0.0425)]} ⫽ 2[(20,740) ⫹ (245,650)] ⫽ 532,780 lb/in.

A22 ⫽ 171,000 lb/in.

A66 ⫽ 54,400 lb/in.

A12 ⫽ 50,985 lb/in.

A16 ⫽ A26 ⫽ 0

[a] ⫽ [A]⫺1 (can invert upper 2 ⫻ 2 matrix and A66 separately, due to orthotropy) 兩A兩 ⫽ A11A22 ⫺ A12A21 ⫽ 8.888 ⫻ 1010 (lb/in.)2

3.2

THEORETICAL DETERMINATION OF PROPERTIES

a11 ⫽

A22 1.717 ⫻ 105 ⫽ ⫽ 1.932 ⫻ 10⫺6 in./lb 兩A兩 8.888 ⫻ 1010

a22 ⫽

A11 5.328 ⫻ 105 ⫽ ⫽ 5.995 ⫻ 10⫺6 in./lb 兩A兩 8.888 ⫻ 1010

a21 ⫽

⫺A21 ⫺0.510 ⫻ 105 ⫽ ⫽ ⫺5.738 ⫻ 10⫺7 in./lb 兩A兩 8.888 ⫻ 1010

a66 ⫽

1 1 ⫽ ⫽ 1.838 ⫻ 10⫺5 in./lb A66 0.544 ⫻ 105

a16 ⫽ a26 ⫽ 0 Bij ⫽ 0 since the laminate is symmetric.

冘 Q (z ⫺ z n

Dij ⫽ –31

k ij

3 k

3 k⫺1

)

k⫽1

D11 ⫽ –23 {(1.037 ⫻ 106)[⫺0.04253 ⫺ (⫺0.06253)] ⫹ (5.780 ⫻ 106)[0.0 ⫺ (⫺ 0.04253)]} ⫽ 2[(173.594 ⫹ (443.731)] ⫽ 411.550 lb-in.

D22 ⫽ 194.137 lb-in.

D66 ⫽ 62.510 lb-in.

D21 ⫽ 62.467 lb-in.

D16 ⫽ D26 ⫽ 0

[d] ⫽ [D]⫺1 兩D兩 ⫽ D11D22 ⫺ D12D21 ⫽ 75,985.3 (lb-in.)2

d11 ⫽

D22 194.1 ⫽ ⫽ 2.554 ⫻ 10⫺3 1/lb-in. 兩D兩 75,985

d22 ⫽

D11 ⫽ 5.417 ⫻ 10⫺3 1/lb-in. 兩D兩

d21 ⫽

⫺D21 ⫺62.5 ⫽ ⫽ ⫺8.225 ⫻ 10⫺4 1/lb-in. 兩D兩 75,985

97

98

PROPERTIES OF FRP COMPOSITES

d66 ⫽

1 1 ⫽ ⫽ 1.60 ⫻ 10⫺2 1/lb-in. D66 62.5

a16 ⫽ a26 ⫽ 0 (d) Effective in-plane engineering properties: E 01 ⫽

E 02 ⫽

E 06 ⫽

021 ⫽

012 ⫽

1 a11h 1 a22h 1 a66h ⫺a21

a11 ⫺a21

a22

Symmetry check:

⫽

1 ⫽ 4.141 ⫻ 106 psi (1.932 ⫻ 10⫺6)(0.125)

⫽

1 ⫽ 1.334 ⫻ 106 psi (5.995 ⫻ 10⫺6)(0.125)

⫽

1 ⫽ 0.435 ⫻ 106 psi (1.838 ⫻ 10⫺5)(0.125)

⫽

⫺(⫺5.738 ⫻ 10⫺7) ⫽ 0.297 1.932 ⫻ 10⫺6

⫽

⫺(⫺5.738 ⫻ 10⫺7) ⫽ 0.096 5.995 ⫻ 10⫺6

E 01 012 ⫽ E 02 021 ⫽ 3.97 ⫻ 105 psi

Effective ﬂexural engineering properties: Eƒ1 ⫽

12 12 ⫽ ⫽ 2.406 ⫻ 106 psi 3 d11h (2.554 ⫻ 10⫺3)(0.125)3

Eƒ2 ⫽

12 12 ⫽ ⫽ 1.134 ⫻ 106 psi 3 d22h (5.417 ⫻ 10⫺3)(0.125)3

Eƒ6 ⫽

12 12 ⫽ ⫽ 0.384 ⫻ 106 psi d66h3 (1.838 ⫻ 10⫺5)(0.125)3

ƒ21 ⫽

ƒ12 ⫽

⫺d21

d11 ⫺d21

d22

⫽

⫺(⫺8.225 ⫻ 10⫺4) ⫽ 0.032 2.554 ⫻ 10⫺3

⫽

⫺(⫺8.225 ⫻ 10⫺4) ⫽ 0.015 5.417 ⫻ 10⫺3

3.2

Symmetry check:

THEORETICAL DETERMINATION OF PROPERTIES

99

Eƒ1 ƒ12 ⫽ Eƒ2 ƒ21 ⫽ 3.6 ⫻ 104 psi

Analysis Example 3.3 Given is a three-layer carbon–epoxy composite material with a total thickness of 0.05 in. The composite consists of two outer layers (top and bottom) of ⫹10⬚ off-axis unidirectional composite with a thickness of 0.010 in. each and an internal layer of 0⬚ unidirectional composite with a thickness of 0.030 in. Each unidirectional carbon–epoxy layer has a 60% ﬁber volume fraction and the following orthotropic elastic constants: Ex ⫽ 20.05 ⫻ 106 psi

Es ⫽ 0.74 ⫻ 106 psi

Ey ⫽ 1.46 ⫻ 106 psi

x ⫽ 0.26

It is assumed that the tensile and compressive moduli are equal for both layers. For the given FRP composite material, determine (a) the in-plane stiffness coefﬁcients, Qij, for the on-axis layer; (b) the in-plane stiffness coefﬁcients, Qij, for the off-axis layer; (c) the [A] and [D] matrices (indicate the units for the terms in the matrices); and (d) the effective engineering properties for the layup. SOLUTION (a) Determine Qij for the 0⬚ (on–axis) layer:

y ⫽ x

Ey ⫽ 0.0189 Ex

m ⫽ (1 ⫺ xy)⫺1 ⫽ 1.0049 Qxx ⫽ mEx ⫽ 1.0049(20.05 ⫻ 106) ⫽ 20.15 ⫻ 106 psi Qyy ⫽ mEy ⫽ 1.467 ⫻ 106 psi Qxy ⫽ Qyx ⫽ myEx ⫽ 3.815 ⫻ 105 psi Qss ⫽ Es ⫽ 0.74 ⫻ 106 psi (b) Determine Qij for the ⫹10⬚ (off-axis) layer:

100

PROPERTIES OF FRP COMPOSITES

冦冧冤

Q11 cos4 Q22 sin4 Q12 cos2 sin2 ⫽ Q66 cos2 sin2 Q16 cos3 sin Q26 cos sin3

sin4 cos4 cos2 sin2 cos2 sin2 ⫺cos sin3 ⫺cos3 sin

2 cos2 sin2 2 cos2 sin2 cos4 ⫹ sin4 ⫺2 cos2 sin2 cos sin3 ⫺ cos3 sin cos3 sin ⫺ cos sin3

冥冦 冧

4 cos2 sin2 4 cos2 sin2 ⫺4 cos2 sin2 (cos2 ⫺ sin2)2 2(cos sin3 ⫺ cos3 sin 2(cos3 sin ⫺ cos sin3)

Q11 ⫽ 1.906 ⫻ 107 psi

Q66 ⫽ 1.263 ⫻ 106 psi

Q22 ⫽ 1.507 ⫻ 106 psi

Q16 ⫽ 3.035 ⫻ 106 psi

Q12 ⫽ 9.048 ⫻ 105 psi

Q26 ⫽ 1.597 ⫻ 105 psi

Qxx Qyy Qxy Qss

(c) Determine the [A–B–D] matrix by determining the z values: z0 ⫽ ⫺0.025 in.

z3 ⫽ 0.015 in.

z1 ⫽ ⫺0.015 in.

z4 ⫽ 0.025 in.

z2 ⫽ 0.0

冘Qh n

Aij ⫽

k ij k

k⫽1

A11 ⫽ 2(1.906 ⫻ 107)(0.01) ⫹ (2.015 ⫻ 107) (0.03) ⫽ 9.875 ⫻ 105 lb/in. A22 ⫽ 7.415 ⫻ 104 lb/in. A12 ⫽ 2.954 ⫻ 104 lb/in. A66 ⫽ 4.747 ⫻ 104 lb/in. A16 ⫽ 6.070 ⫻ 104 lb/in. A26 ⫽ 3.194 ⫻ 103 lb/in. Invert [A] to obtain [a] (full 3 ⫻ 3 matrix inversion required):

3.2

THEORETICAL DETERMINATION OF PROPERTIES

冢

9.857 ⫻ 105 2.954 ⫻ 104 A ⫽ 2.954 ⫻ 104 7.415 ⫻ 104 6.07 ⫻ 104 3.194 ⫻ 103

冣

6.07 ⫻ 104 3.194 ⫻ 103 4.746 ⫻ 104

101

lb/in.

a ⫽ A⫺1

冢

1.112 ⫻ 10⫺6 a ⫽ ⫺3.828 ⫻ 10⫺7 ⫺1.396 ⫻ 10⫺6

⫺3.828 ⫻ 10⫺7 1.366 ⫻ 10⫺5 ⫺4.295 ⫻ 10⫺7

⫺1.396 ⫻ 10⫺6 ⫺4.295 ⫻ 10⫺7 2.289 ⫻ 10⫺5

冣

in./lb

Bij ⫽ 0 since the laminate is symmetric.

冘Q n

Dij ⫽

k ij

k⫽1

冉

hkt k2 ⫹

hk3 12

冊

冋

D11 ⫽ 2(1.906 ⫻ 107) 0.01(0.02)2 ⫹

册

冉 冊

(0.01)3 0.033 ⫹ (2.015 ⫻ 107) 12 12

⫽ 200.994 lb-in.

D22 ⫽ 15.608 lb-in. D12 ⫽ 8.248 lb-in. D66 ⫽ 11.98 lb-in. D16 ⫽ 24.786 lb-in. D26 ⫽ 1.304 lb-in. Invert to obtain [d]:

D⫽

冢

200.994 8.248 24.786

冣

8.248 24.786 15.608 1.304 1.304 11.98

in.-lb

d ⫽ D⫺1

冢

6.77 ⫻ 10⫺3 d ⫽ ⫺2.429 ⫻ 10⫺3 ⫺0.014

⫺2.429 ⫻ 10⫺3

0.066 ⫺2.107 ⫻ 10⫺3

冣

⫺0.014 ⫺2.107 ⫻ 10⫺3

(d) Effective in-plane engineering properties:

0.112

(in.-lb)⫺1

102

PROPERTIES OF FRP COMPOSITES

E 01 ⫽

1 1 ⫽ ⫽ 17.99 ⫻ 106 psi a11h (1.112 ⫻ 10⫺6)(0.05)

E 02 ⫽

1 1 ⫽ ⫽ 1.464 ⫻ 106 psi a22h (1.366 ⫻ 10⫺5)(0.05)

E 06 ⫽

1 1 ⫽ ⫽ 0.874 ⫻ 106 psi a66h (2.289 ⫻ 10⫺5)(0.05)

0 21 ⫽

0 12 ⫽

⫺a21

a11 ⫺a21

a22

⫽

⫺(⫺3.828 ⫻ 10⫺7) ⫽ 0.344 1.112 ⫻ 10⫺6

⫽

⫺(⫺3.828 ⫻ 10⫺7) ⫽ 0.028 1.366 ⫻ 10⫺5

0 16 ⫽

a16 ⫺1.396 ⫻ 10⫺6 ⫽ ⫽ ⫺0.061 a66 2.289 ⫻ 10⫺5

0 26 ⫽

a26 ⫺4.295 ⫻ 10⫺7 ⫽ ⫽ ⫺0.019 a66 2.289 ⫻ 10⫺5

0 61 ⫽

a61 ⫺1.396 ⫻ 10⫺6 ⫽ ⫽ ⫺1.255 a11 1.112 ⫻ 10⫺6

0 62 ⫽

a62 ⫺4.295 ⫻ 10⫺7 ⫽ ⫽ ⫺0.031 a22 1.366 ⫻ 10⫺5

Symmetry checks:

0 0 E 10 12 ⫽ E 20 21 ⫽ 5.042 ⫻ 105 psi

E 01 016 ⫽ E 06 061⫽ ⫺1.097 ⫻ 106 psi E 02 026 ⫽ E 06 062 ⫽ ⫺2.748 ⫻ 104 psi Effective ﬂexural engineering properties: Eƒ1 ⫽

12 12 ⫽ ⫽ 14.2 ⫻ 106 psi d11h3 (6.77 ⫻ 10⫺3)(0.05)3

Eƒ2 ⫽

12 12 ⫽ ⫽ 1.454 ⫻ 106 psi d22h3 (6.60 ⫻ 10⫺2)(0.05)3

Eƒ6 ⫽

12 12 ⫽ ⫽ 8.57 ⫻ 105 psi d66h3 (11.2 ⫻ 10⫺2)(0.05)3

3.2

ƒ 21 ⫽

ƒ 12 ⫽

THEORETICAL DETERMINATION OF PROPERTIES

⫺d21

d11 ⫺d21

d22

⫽

⫺(⫺2.429 ⫻ 10⫺3) ⫽ 0.359 6.77 ⫻ 10⫺3

⫽

⫺(⫺2.429 ⫻ 10⫺3) ⫽ 0.037 6.60 ⫻ 10⫺2

ƒ16 ⫽

d16 ⫺1.4 ⫻ 10⫺2 ⫽ ⫽ ⫺0.125 d66 11.2 ⫻ 10⫺2

ƒ26 ⫽

d26 ⫺2.107 ⫻ 10⫺3 ⫽ ⫽ ⫺0.188 d66 11.2 ⫻ 10⫺2

ƒ61 ⫽

d61 ⫺1.4 ⫻ 10⫺2 ⫽ ⫽ ⫺2.068 d11 6.77 ⫻ 10⫺3

ƒ62 ⫽

d62 ⫺2.107 ⫻ 10⫺3 ⫽ ⫽ ⫺0.322 d22 6.60 ⫻ 10⫺2

Symmetry checks:

103

ƒ ƒ E1ƒ 12 ⫽ E2ƒ 21 ⫽ 5.3 ⫻ 105 psi

Eƒ1 ƒ16 ⫽ Eƒ6 ƒ61 ⫽ ⫺1.78 ⫻ 106 psi Eƒ2 ƒ26 ⫽ Eƒ6 ƒ62 ⫽ ⫺2.73 ⫻ 105 psi 3.2.4

Full-Section Level

When the FRP composite is used in the ﬁeld it is usually referred to as a component or a part, such as an FRP strengthening wrap or an FRP pultruded beam. In this case, theoretical methods can be used to determine the material and section properties of the entire FRP part. In most structural engineering design, one-dimensional theories such as bar and beam theories are used, which require determination of the effective composite18 section properties of the FRP part.19 In the case of an FRP reinforcing bar or an FRP strengthening strip or wrap, the cross-sectional area, A, and the longitudinal mechanical properties, EL and L, are the key properties used in design. The full-section properties in the longitudinal direction are then typically obtained by the rule of mixtures to yield a composite axial stiffness, ELA, and a composite axial capacity, LA.

18 Where full-section mechanics are concerned, the term composite is used to describe a part made of multiple materials in the mechanics of materials sense (e.g., composite construction of steel and concrete). This can be a source of confusion in the FRP composite terminology. 19 More details on this concept are provided in the design chapters.

104

PROPERTIES OF FRP COMPOSITES

In these applications, the bending and shear stiffness of the FRP part are not usually considered in the design. In the case of a symmetric FRP proﬁle used as a beam or used as a column, the geometric properties of primary interest are the cross-sectional area, A; the second moment of area, I; and the shear area, As. When the proﬁle consists of FRP laminates (or panels) having different in-plane properties, the effective properties are obtained by conventional one-dimensional section analysis20 to give a composite ﬂexural stiffness, ELI; axial stiffness, ELA; and shear stiffness, GLT As (Bank, 1987). The bending moment capacity, axial capacity, and transverse shear capacity are then determined for the full section based on stress analysis according to a ﬁrst ply failure or ultimate failure criterion. If twisting is included, a composite torsional stiffness, GLT J, is deﬁned. If warping of the cross section is included, a warping stiffness, ELCw, is deﬁned. If the panels of the proﬁle are anisotropic in-plane, a one-dimensional theory may not be appropriate (Coﬁe and Bank, 1995). A simpliﬁed one-dimensional theory for bending and twisting coupling in FRP beams is presented in Bank (1990). 3.3

EXPERIMENTAL DETERMINATION OF PROPERTIES

Many standards organizations around the world publish standard test methods for FRP composite materials; among these are the American Society for Testing and Materials (ASTM) and the International Organization for Standardization (ISO) (ASTM, 2006; ISO, 2006). Literally thousands of standardized test methods are available for testing ﬁber, resin, and additives and for testing FRP composites on the ﬁber, lamina, and laminate levels. However, not many standards are available for testing FRP composites on the full-section level in a form that is required for structural engineering applications. In recent years a number of organizations have developed test method standards directly related to the use of FRP composites in structural engineering. These include the American Concrete Institute (ACI), the European Committee for Standardization (CEN), the Japan Society for Civil Engineers (JSCE), and the Canadian Standards Association (CSA). In this chapter we review the tests available for FRP composites for the ﬁber, lamina, laminate, and full-section levels. More discussion and detail is provided for full-section test methods that have been developed speciﬁcally for the use for FRP composites in structural engineering. At this time there is no general agreement between materials suppliers, part manufacturers, structural engineers, and other stakeholders on precisely which test methods should be used. However, there is general agreement as to which physical and mechanical properties are important in design. The

20

Such as the transformed section method for ﬂexural stiffness, EI.

3.3

EXPERIMENTAL DETERMINATION OF PROPERTIES

105

choice of the speciﬁc test method is often left to the constituent material supplier, the FRP composite material producer, or the FRP part manufacturer. Test results are reported according to the requirements of the test method chosen and can therefore be subject to interpretation as to their relevance for structural engineering design. In an engineering project, a structural engineer is usually required to develop a material speciﬁcation for the FRP composites used in the project for inclusion in contract documents. In this speciﬁcation, the structural engineer is required to specify the test methods to be used and the way in which the FRP material properties are to be reported. In addition, the designer may specify speciﬁc values of certain properties that must be achieved by the FRP material in a particular test. Limits for FRP materials can be found in model speciﬁcations (e.g., Bank et al., 2003), in speciﬁcations for pultruded proﬁles published by the European Committee on Standardization (CEN, 2002a), and in the speciﬁcations for reinforced plastic ladders21 published by the American National Standards Institute (ANSI, 2000). Determination of design values for speciﬁc design bases for FRP reinforcing bars, FRP strengthening systems, and FRP proﬁles is discussed in the design chapters that follow. It is important to note that although full-section test methods have been developed for testing FRP composite products for use in structural engineering on a full scale, this does not mean to imply that tests on the ﬁber, lamina, and laminate levels are not needed or required. Full-section test methods have been developed to characterize FRP products for use in structural engineering where appropriate coupon-type tests are not felt to be applicable, due to a specimen’s size or the data reduction methods used. An FRP material speciﬁcation for FRP composite products for use in structural engineering can include tests of the FRP material on the lamina and laminate levels as appropriate, and a speciﬁcation for the material constituents on the ﬁber level. 3.3.1

Fiber Level

For structural engineering applications of FRP composite materials, very little testing is performed or speciﬁed by the end user (i.e., the FRP part manufacturer or structural engineer) on the ﬁber level. Most speciﬁcations for FRP composites for use in structural engineering concentrate on specifying properties of the FRP composite after it has been manufactured or fabricated (i.e., on the lamina, laminate, or full-section level). Manufacturers of raw ﬁber, polymer resins, and additives typically conduct standard tests on the constituents and report them in product speciﬁcation sheets. 21 Although dealing with ladders, this speciﬁcation is concerned primarily with pultruded proﬁles and full-scale performance testing of FRP products and is therefore pertinent to specifying pultruded proﬁles in structural engineering. The commercial success of FRP ladders over the last 20 years can be attributed largely to the development of this rigorous material and performance speciﬁcation for pultruded products.

106

PROPERTIES OF FRP COMPOSITES

Many standard test methods for obtaining mechanical, physical, and chemical properties of polymer resins (also known as plastics for this purpose) in their liquid and hardened states are available from ASTM and other standards organizations.22 These have been developed primarily by the plastics industry over the past 50 years. It should be noted that the properties of the polymer are typically obtained from tests on cast resin samples that have been postcured at elevated temperatures.23 Tests for the secondary constituents of the polymer matrix (see Chapter 2) are reported in a similar fashion according to ASTM or other industry-speciﬁc test methods. To obtain the properties of reinforcing ﬁbers used in FRP composites, testing can be conducted on single ﬁbers taken from rovings or tows using a single-ﬁber test method such as ASTM C 1557 or D 3379.24 However, singleﬁber testing is difﬁcult, and the data obtained from tests on single ﬁbers are not necessarily representative of their properties when in the FRP composite itself. Consequently, ﬁber manufacturers usually report the mechanical properties of their ﬁbers when impregnated with a commonly used resin and tested as an FRP composite. The impregnated ﬁber test used by glass ﬁber manufacturers is ASTM D 2343, and the test used by carbon ﬁber manufacturers is ASTM D 4018. Fiber properties are then calculated from the FRP composite test data using the rule-of-mixtures approximations given previously. 3.3.2

Lamina Level

By far the majority of tests conducted on FRP composites for structural engineering applications are conducted on coupons cut from as-fabricated FRP composite parts. When these tests are conducted on coupons cut from an FRP composite containing only unidirectional ﬁbers (such as FRP strengthening strips and sheets or FRP reinforcing bars), the testing conducted is of a unidirectional ply (i.e., on the lamina level). When the coupon is cut from an FRP composite that contains multidirectional plies or mats (such as an FRP strengthening fabric or an FRP proﬁle), testing is on a multidirectional plate (i.e., on the laminate level.) For FRP composites for structural engineering applications, every effort should be made to test coupons cut from an asfabricated in situ part, and to test it at the as-fabricated full thickness of the part. When multiple plies of the same unidirectional composite are used to create full-part thickness in the ﬁeld (as in the case of a multilayer FRP strengthening system), it is permissible to test one unidirectional ply and to calculate the properties of the composite based on the ply values.25 When

22 Many standard ASTM test methods for the properties of plastics are also used to obtain the properties of reinforced plastics (i.e., FRP composites), and these methods are discussed in Sections 3.3.2 and 3.3.3. 23 This is also typically done when the polymer is used in the hand-layup method for FRP strengthening, even when the resin is cured at ambient temperature in the ﬁeld. 24 A list of the titles of all the ASTM test methods cited in this chapter is given in Section 3.4. 25 ACI 440.2R-02 allows this approach.

3.3

EXPERIMENTAL DETERMINATION OF PROPERTIES

107

multidirectional plies are used in FRP strengthening fabric, the as-fabricated full-thickness part should be tested to obtain the design properties. When determining properties of FRP composites on either the lamina or laminate level, the same ASTM tests are used since the test is conducted on the macroscopic level and assumes, for the purposes of conducting the test, that the coupon is made of a homogenous material. Tests commonly used for an FRP lamina or laminate are given in Table 3.1. The physical tests noted should be conducted on samples taken from the FRP composite and not on samples taken from the polymer matrix alone. This is because the ﬁber can have an inﬂuence on many of the physical properties that are often assumed to be a function of the resin alone, such as the hardness, glass transition temperature, and ﬂash ignition temperature. Another useful guide to testing of composite materials that can be consulted in addition to Table 3.1 is ASTM D 4762. This guide also provides test methods for additional properties of interest to structural engineers, such as creep, fatigue, and fracture properties of FRP composites. Additional guidance on conducting tests on composite material unidirectional and multidirectional laminates may be found in Adams et al. (2003). The distinction between testing of the unimpregnated single-ﬁber level and the impregnated roving or tow on the lamina level is of particular importance for the structural engineer in the design of FRP strengthening systems. ACI 440.2R-02 (2002) allows two different methods for designing FRP strengthening systems. One method uses the properties of the FRP composite, which are calculated using the measured gross area of the FRP composite; the other method uses the properties of the ﬁbers, which are calculated using the manufacturer-supplied area of the ﬁbers in a dry sheet or fabric. However, according to ACI 440.3R-04 (2004) Test Method L.2,26 when the area of the ﬁber method is used, the ﬁber properties are not obtained from single-ﬁber tests. For either design method both the longitudinal strength and stiffness of either the FRP composite or the ﬁbers are obtained from a test on the FRP composite at the ply level. Consequently, the methods lead to identical designs. 3.3.3

Laminate Level

As noted above, the test methods used for a multidirectional laminate are technically the same as those used for a unidirectional ply, as shown in Table 3.1. However, when used for multidirectional composites, two key differences should be noted. First, as can be seen in Table 3.1, only longitudinal mechanical tests are conducted on the unidirectional ply, whereas both longitudinal and transverse tests are required for the multidirectional laminate. Second, the exact requirements of the ASTM tests cannot always be satisﬁed, due to the thickness of the FRP parts used in structural engineering and to

26

Titles of ACI 440.3R-04 test methods are listed in Section 3.4.

108

Mechanical properties Strength properties Longitutinal tensile strength Longitudinal compressive strength Longitudinal bearing strength Longitudinal short beam shear strength In-plane shear strength Impact resistance Transverse tensile strength Transverse compressive strength Transverse short beam shear strength Transverse bearing strength Stiffness properties Longitudinal tensile modulus Longitudinal compressive modulus Major (longitudinal) Poisson ratio In-plane shear modulus Transverse tensile modulus Transverse compressive modulus D D D D D D

D D D D D D D D D D 3039, 3410, 3039, 5379 3039, 3410,

冧 D 5083, D 638 D 695

冧

D 5083, D 638, D 3916 D 695 D 5083, D 638

冧

冧

3039, D 5083, D 638, D 3916 3410, D 695 953, D 5961 2344, D 4475 5379, D3846 256 3039, D 5083, D 638 3410, D 695 2344 953, D 5961

ASTM Test Method(s)

Recommended Test Methods for FRP Composites at the Lamina and Laminate Levels

Ply or Laminate Property

TABLE 3.1

Multidirectional laminate only

Unidirectional ply and multidirectional laminate

Multidirectional laminate only

Unidirectional ply and multidirectional laminate

Test Required

109

Source: Adapted from Bank et al. (2003).

Physical properties Fiber volume fraction Density Barcol hardness Glass transition temperature Water absorbed when substantially saturated Longitudinal coefﬁcient of thermal expansion Transverse coefﬁcient of thermal expansion Dielectric strength Flash ignition temperature Flammability and smoke generation D 3171, D 2584 D 792 D 2583 E 1356, E 1640, D 648, E 2092 D 570 E 831, D 696 E 831, D 696 D 149 D 1929 E 84, D 635, E 662

Unidirectional ply and multidirectional laminate

110

PROPERTIES OF FRP COMPOSITES

the fact that they may have fabric and mat layers. ASTM D 6856 provides recommendations on the modiﬁcations that need to be made to the standard test methods when fabric composites (which also tend to be thicker than traditional unidirectional ply layup composites) are used. 3.3.4

Full-Section Level

FRP composites are used in structural engineering applications in the form of FRP parts or components, such as FRP reinforcing bars, FRP strips or wraps, and FRP proﬁle sections. When designing, a structural engineer performs iterative analytical calculations in terms of member stress resultants, such as the bending moment (M), twisting moment (T), shear force (V), and axial force (F), which are obtained from the applied loads to determine the member deformations and capacities (also known as strengths) using the geometric and material properties of the members. The member deformations are obtained using the member’s rigidities, the bending rigidity (EI), the torsional rigidity (GJ), the axial rigidity (EA), and the transverse shear rigidity (GAs27), which are obtained from the geometric dimensions of the member cross section and the material properties. The member load-carrying capacities are obtained from the material strengths and geometric properties of the section (e.g., M ⫽ bS, P ⫽ a A). In homogeneous isotropic materials such as steel, the material strengths and stiffnesses are not location dependent in the section, and the load-carrying capacity is determined relatively easily. However, in FRP members, the stiffness and strength properties are location dependent within the cross section on the ﬁber, lamina, and laminate levels due to the inhomogeneity and anisotropy of the material. This tends to complicate the design process, as the calculation of full-section rigidities and load-carrying capacities are more difﬁcult to write in the form of simple stress-resultant equations. However, as described in the design sections of this book, numerous simplifying assumptions can be made in the analysis of FRP parts for structural engineering and the design process is consequently also simpliﬁed signiﬁcantly. One common assumption made is that the properties of the FRP part can be considered to be homogeneous on a full-section level for certain types of calculations. In this case, the full-section member properties needed for structural engineering design for an as-delivered or as-produced part are then obtained from tests on the entire cross section (and often the entire length) of the part. These tests, known as full-section tests, attempt to determine effective properties for design calculations based on the as-intended performance of the entire FRP part when it is in service. FRP parts used in structural engineering are typically large [rebar and proﬁle lengths greater than 10 ft (3 m)], with surface areas of strips and wraps

27

Where As is the effective or shear area for transverse shear deformation, often given as kA, where k is known as the Timoshenko shear coefﬁcient.

3.3

EXPERIMENTAL DETERMINATION OF PROPERTIES

111

greater than 50 ft2 (5 m2), and may be relatively thick [⬎0.25 in. (6 mm)]. Therefore, testing them at their full section (or full size) often requires specialized ﬁxtures and procedures that are different from those used to test FRP materials in small coupon form at the lamina and laminate levels. For the three different categories of FRP parts used in structural engineering, different full-section tests have been developed by a number of organizations. Full-Section Tests for FRP Reinforcing Bars Full-section tests for FRP reinforcing bars that have been developed by the ACI, CSA, and JSCE are listed at the end of the chapter. These methods are used to test FRP reinforcing bars to develop design properties for quality control and assurance purposes as well as for research purposes. Since FRP reinforcing bars have a variety of cross-sectional shapes and surface irregularities that are required to enhance bond properties, a test method has been developed to determine the nominal cross-sectional area and nominal diameter of an irregularly shaped bar (ACI B.1; CSA Annex A and JSCE E-131). Since FRP bars have signiﬁcantly lower compressive strength in the transverse direction than tensile strength in the longitudinal direction, they have a tendency to crush in the grips when tested in tension. Due to their irregular surface proﬁle, standard grips used for smooth FRP rods recommended by ASTM D 3916 cannot be used to test FRP reinforcing bars. Therefore, special methods are used to anchor FRP bars in a tensile testing machine when conducting tension tests (ACI Appendix A and CSA Annex B). The provisions detail a number of methods to embed the FRP bars ends in a steel sleeve to enable testing to failure at full-section loads (which can approach 200 kips for larger-diameter FRP bars). Figure 3.3 shows FRP rebars with steel end sleeves attached. Since FRP reinforcing bars have different moduli and surface textures from those of conventional steel reinforcing bars, provisions are given for determining either the development length (CSA Annex D) or the pull-out bond strength (ACI B.3; CSA Annex H, and JSCE E-539) for FRP bars. These test methods can be used to investigate the bond behavior of FRP bars in concrete and to compare their bond behavior to that of conventional bars under different loading and environmental conditions. Since the strength of the bent

Figure 3.3 FRP reinforcing bar with steel sleeves for tensile testing.

112

PROPERTIES OF FRP COMPOSITES

portion of the FRP reinforcing bar can be signiﬁcantly less than that of the same straight bar due to the particular FRP manufacturing process used, tests for bent FRP bars for use as stirrups in beams are provided (ACI B.5 and B.12 and CSA Annex E). The values obtained in the bond strength and bentbar strength tests provide important data for design of concrete structures with FRP reinforcing bars. In some cases, these test data have been incorporated in design equations listed in the ACI 440.1R-06 design provisions. They are also used by manufacturers to provide properties for their bars that can be used in design directly by the structural engineer. Since an FRP reinforcing bar is anisotropic, its shear strength cannot be calculated from its tensile strength. The transverse shear strength of an FRP reinforcing bar is needed to determine the dowel strength of FRP reinforcing bars. Test methods for determining the shear strength in direct shear (as opposed to in bending) are provided in ACI B.4, CSA Annex, and JSCE E-540. Since FRP reinforcing bars are nonmetallic, they do not corrode in aqueous environments, due to electrochemical effects. However, they are susceptible to chemical and physical degradation of their polymer resins, additives, and ﬁbers. Glass ﬁber–reinforced composites are particularly susceptible to degradation in alkaline environments. Test methods for durability (ACI B.6, CSA Annex O, and JSCE E-538) are used to determine the residual tensile strength of a bar (with appropriate testing anchorages) following accelerated conditioning in prescribed alkaline solutions that are intended to simulate the concrete pore-water alkalinity. To date, these methods have not been used to develop design procedures but are used only as a guide to the long-term durability of FRP bars in concrete. In a similar fashion, test methods are provided for creep rupture (ACI B.8, CSA Annex J, and JSCE E-533) and fatigue (ACI B.7, CSA Annex L, and JSCE E-534). All of the tests noted above are conducted on lengths of FRP reinforcing bars using the full cross-sectional area of the bar with all of its surface irregularities. It is important to note that the properties of FRP reinforcing bars are bar size (usually given in terms of the nominal diameter)–dependent and that tests must be conducted for each discrete bar size. This is due to the anisotropic nature of the FRP materials used and the fact that resins and additives used for thicker bars (0.5 in. and larger in diameter) are usually different from those used for smaller bars. Thicker bars tend to develop thermal shrinkage cracks during curing, and low-proﬁle shrink additives (see Chapter 2) are added to prevent this cracking. These additives may have an effect on the mechanical properties of the bars. Since different manufacturers use different constituent materials, processes, and surface deformations, each manufacturer generally conducts the tests on the bars they produce and reports the data for use by structural engineers. JSCE-E-131 can be used to identify the constituent materials and geometric features of an FRP reinforcing bar in a standardized fashion. JSCE-E-131 also provides guaranteed mechanical properties for speciﬁc bars referenced in JSCE (2001). An alternative speciﬁcation for identifying constituent materials of FRP reinforcing bars is discussed in Bank et al. (2003).

3.3

EXPERIMENTAL DETERMINATION OF PROPERTIES

113

Since FRP reinforcing bars are anisotropic and are manufactured from a variety of ﬁbers and resin systems, they have different coefﬁcients of thermal expansion (CTEs) in their longitudinal and transverse directions. The coefﬁcients of thermal expansion of an FRP reinforcing bar can be obtained by use of conventional thermal mechanical analysis (TMA) according to CSA Annex M and JSCE E-536. It should be noted that due to the nature of the TMA test device used, small coupons are used and that this is not a full-section test method. In addition, only the longitudinal CTE is measured in the methods noted above. This method is equivalent to ASTM E 831. No unique full-section test methods have been developed for testing FRP grids and gratings used as reinforcements for concrete. The test methods used for FRP bars are intended for use with FRP grids and gratings. According to the test methods, individual bars in the grid or grating should be cut from the grid and tested. This is not entirely appropriate, as grid intersections create regions of stress concentrations and have very different properties from those of nonintersection regions. In addition, grid bars are generally smooth and not speciﬁcally deformed for bond to the concrete. Grids and gratings acquire their bonding properties from the anchorage provided by the perpendicular grid members in the concrete. Although a standard test method has not been developed to determine the development length of a grid or grating bar, it is generally accepted that at least two perpendicular bars are required to fully develop a single grid bar (Bakht et al., 2000, p. 10). In addition, while splicing of individual FRP reinforcing bars by overlapping is reasonable, splicing of FRP grids and gratings by overlapping splices cannot generally be carried out (unless the grids are very thin and ﬂexible) and specialized splicing methods are required for grids and gratings. In-house test methods developed for the NEFMAC FRP grid material are reviewed in Sugita (1993). No test methods have been developed for FRP stay-in-place (SIP) formwork systems that are required to serve the dual purpose of forms for the uncured (i.e., wet) concrete and of reinforcements for the cured (i.e., hardened) concrete. Often, these FRP systems have quite complex cross-sectional shapes, and coupon-level testing is difﬁcult. In addition, since they serve as tensile reinforcement for FRP reinforced concrete in much the same way as do FRP reinforcing bars, the extent of the bond and the development length of the FRP SIP form and the concrete needs to be determined. Since FRP SIP forms are bonded to the concrete on only one side, the determination of the bond and development length properties often require specialized in-house test methods to be developed that depend on the geometry of the FRP SIP form. Full-Section Tests for FRP Precured Strips and Hand-Laid-Up Sheets and Fabrics A number of test methods have been developed to test FRP precured strips and FRP hand-laid-up sheets or fabrics (known as wraps when they partially or fully encircle a member) that are adhesively bonded to the surface of concrete or masonry structures. The full-section tests developed include those for testing the direct tensile pull-off bond strength of the cured FRP

114

PROPERTIES OF FRP COMPOSITES

when bonded adhesively to the concrete, the longitudinal shear bond strength, and the development length of the cured FRP when bonded adhesively to the concrete, and tensile and tensile splice tests of the FRP itself (i.e., not bonded to the concrete). The test methods developed for the tensile testing (ACI L.2, CSA Annex G, and JSCE E-541) are essentially modiﬁcations of the standard coupon tests used to test FRP unidirectional materials on the laminate level, such as ASTM D 3039. The key differences between the standard tensile test methods and those developed for FRP strips and fabrics lie in the methods of specimen preparation and in the techniques of data reduction. Since FRP laid-up sheets and fabrics are fabricated in situ, a procedure (ACI L.2) is described to fabricate test panels (also known as witness panels) in the ﬁeld at the time of actual fabrication of the FRP composite on the concrete surface. The procedure allows the fabricator to use a roller to ‘‘work out trapped air in the laminate’’ and the use of a ﬂat cover plate when curing the test panel to create a smooth top surface (but not to apply signiﬁcant pressure to the laminate). Coupons cut from the cured test panel are then tested to determine the in situ properties of the FRP hand laid-up materials. It is very important to note that this procedure requires the fabricator to cure the test panel at the same conditions as those of the FRP material. If postcuring is not used on the in-ﬁeld applied FRP material, postcuring must not be used on the test panel. A procedure is also described for producing a laboratory test panel for a laid-up FRP material system. The laboratory procedure is similar to the ﬁeld procedure, however, it allows the fabricator to forcibly push out excess resin using a ﬂat-edged paddle, and furthermore, it allows the laminate to be cured under pressure and/or elevated temperature provided that ‘‘the engineer and material supplier . . . agree on a representative specimen fabrication process’’28 (ACI L.2). When precured FRP strips are tested, the strip must be tested at its full thickness. It is important to note that in all the methods described above, the laminate tested must be the full thickness of the actual laminate used in the ﬁeld. Testing of individual unidirectional plies and calculation of effective properties are not permitted. This is in contradiction to the design procedures in ACI 440.2R-02. It is also important to note that the ACI L.2 test method is applicable only to unidirectional or bidirectional (cross-ply) FRP materials. The second key difference between the full-section test method and the standard tensile test method lies in the methods allowed for data reduction to determine the effective tensile strength and stiffness of an FRP laminate. In 28 When using test data from manufacturer speciﬁcation sheets it is very important to know whether the test panel has been produced similar to the in situ material or has been in produced in laboratory-controlled conditions. Removing excess resin to increase ﬁber volume fraction and elevated temperature postcuring of an FRP laminate can have a signiﬁcant inﬂuence on both the mechanical (e.g., strengths, stiffnesses) and physical (e.g., glass transition temperature, hardness) properties of the laminate.

3.3

EXPERIMENTAL DETERMINATION OF PROPERTIES

115

addition to allowing the fabricator to obtain the properties based on the gross cross-sectional area of the coupon (which is standard for composite material test methods), an alternative data reduction method based on the net crosssectional area of the ﬁbers (only) in the coupon can be used.29 The distinction between the way in which these data are reported and how they are used in design is of utmost importance, and a structural engineer must know if the tensile properties reported are for the FRP laminate or for the ﬁbers only. The test methods for overlap splices for FRP strips and hand-laid-up sheets and fabrics (ACI L.3, CSA Annex Q, and JSCE-E 542) are similar to those used to test laminates in single- or double-lap conﬁgurations. However, the key differences detailed above for specimen fabrication and data reduction are also applied to lap splice specimens. Two types of test methods are provided to test the properties of the bond between the FRP laminate (precured or hand laid-up) and the concrete substrate. One is a direct tension test that can be used to measure tensile bond strength normal to the FRP laminate; the other is a shear and peeling test that can be used to measure shear bond strength and interfacial fracture energy parallel to the FRP laminate. The direct tension pull-off test (ACI L.1, CSA Annex E, and JSCE-E 545) uses a standard pull-off test ﬁxture to measure the bond strength between the FRP and the concrete. Modiﬁcations have been made to the standard pull-off test that deﬁne allowable types of failure modes when the tester is used to test laminates bonded to concrete. Allowable failure modes are cohesive failure with the laminate, cohesive failure in the concrete substrate, or interfacial failure at the interface of the adhesive and the concrete or the FRP. It is important to note that the ACI version of this method does not permit failure in the interfacial region. The results of this test are not actually used for design of FRP strengthening systems but rather, to perform tests on the concrete substrate to determine its suitability for strengthening. The design guides for FRP strengthening generally require that the concrete pull-off tensile strength in the surface layer to which the FRP is bonded exceeds 200 psi (1.4 MPa) (ACI 440.2R-02, 2002). The other bond test is a single-lap shear test (CSA Annex P and JSCE E543) in which the FRP is bonded to the concrete and then placed in longitudinal tension so as to shear it off the concrete to simulate the stress state in the FRP strengthening system when it is used as a tensile strengthening element. The test method depends on the determination of an effective bond length.30 The results of the test can be used to determine bond stress, effective length, and interfacial fracture energy. However, they cannot generally be used 29

In this method the area of the ﬁbers is obtained from manufacturers’ speciﬁcation sheets. It has been shown that shear force transfer in a bonded laminate occurs only over a limited length, called the effective length, and that the bond stress can therefore not increase in an unlimited manner. The effective length is a function of properties of the concrete substrate, the FRP material, and the adhesive, and is usually determined by experiment. 30

116

PROPERTIES OF FRP COMPOSITES

at this time to predict either laminate-end debonding or midspan debonding of FRP laminates, due to the lengthwise-varying stress resultants, peeling stresses at the plate ends, and crack patterns that develop in beams when loaded in ﬂexure. Test methods have also been developed for evaluating the long-term fatigue and durability of FRP strengthening systems when used to strengthen concrete (JSCE-E 546, JSCE-E 547, JSCE-E 548, and JSCE-E 549). These test methods use essentially the same specimen types as the tensile tests (or bond tests in the case of JSCE-E 549) but expose the specimens to different accelerated conditioning environments to determine residual properties. Full-Section Tests for FRP Proﬁles FRP pultruded proﬁle sections commonly used in structural engineering include I-shaped beams, channels, angles, and square and rectangular tubes. Channels and angles are generally used in back-to-back conﬁgurations to create double-channel and doubleangle sections that have coincident centroids and shear centers. The mechanical and physical properties of FRP materials used in these pultruded proﬁles are obtained from tests on coupons cut from the sections (i.e., on the laminate level) or from tests on test panels that are produced by pultrusion having nominally identical properties (Wang and Zurelck, 1994). Most pultrusion manufacturers report the properties of their pultruded materials for an entire class of structural shapes (e.g., I-beams, plates) and resin systems even though layup of the roving and mat layers may differ within a class. The properties of the thinner pultruded material shapes [⬍–14 in. (6 mm)] are generally penalized at the expense of the thicker parts [⬎–14 in. (6 mm)] in order to publish lower bound values for use in design. A designer may want to use test data to determine design values of the pultruded material for a speciﬁc part used in a design in lieu of the manufacturer-reported values. In general, pultruded proﬁles for braced frame and truss structures are designed using the properties obtained from the coupon test and appropriate theoretical methods as explained in the design chapters of this book. However, in certain situations it is often preferred to use full-section tests on individual proﬁles or on subassemblies of proﬁles to develop full-section properties or capacities for use in design. This is because there are situations in which a full-section property is easier to use in a design or when coupon property data cannot be used with conﬁdence to predict the performance of complicated details. Since designs of pultruded proﬁles are often controlled by serviceability and buckling criteria,31 the bending, transverse shear, and torsional rigidities of the full section (EI, GAs, and GJ) are needed in design (Roberts and AlUbaidi, 2002). Although theoretical methods are available to predict these properties from coupon data, this requires the designer to make a number of simplifying assumptions related to the proﬁle’s geometry, homogeneity, and 31

This includes ﬂexural (Euler) buckling, torsional buckling, lateral buckling, and local buckling.

3.3

EXPERIMENTAL DETERMINATION OF PROPERTIES

117

anisotropy (Bank et al., 1995a). Full-section testing is a way to obtain an effective property for a proﬁle that can be used in a stress-resultant theory. The most widely used full-section test is the test for the full-section modulus, or E-modulus as it referred to by most manufacturers. In this test, the FRP proﬁle is tested in three- or four-point bending, and an effective longitudinal modulus is determined from load and midspan deﬂection data (CEN Part 2 Annex D). However, due to the presence of shear deformation effects in pultruded proﬁles because of moderately high longitudinal-to-shear modulus ratios (4 to 6 for glass-reinforced proﬁles) and because pultruded proﬁles are generally used on shorter spans than steel beams, the results of the fullsection bending test need to be interpreted with caution (Bank, 1989a,b). As noted in the CEN test method, the effective ﬂexural modulus is a spandependent property, due to the effect of shear deformations. To minimize the effects of the shear deformation, the CEN test method requires the proﬁle to be tested over a span-to-depth ratio of at least 20. In addition, the measured value of the full-section modulus that is obtained from the test is multiplied by a factor of 1.05 to compensate approximately for the effects of shear deformation. However, this test does not yield the full-section transverse shear rigidity (GAs) that is often needed in a design where a shear deformation beam theory is used to predict deﬂections. CEN Part 2 Annex G provides a method to measure the bending rigidity (EI) and the shear rigidity (GAs) of a proﬁle section simultaneously by testing it on different span lengths and performing a data analysis. This method has been used by a number of researchers and manufacturers to obtain results that can be used in design, and had become a de facto standard prior to publication by CEN (Bank, 1989a,b; Roberts and Al-Ubaidi, 2002; Giroux and Shao, 2003). CEN Part 2 Annex G also provides a method to determine the full-section torsional stiffness of an FRP proﬁle using a ﬁxture that applies a uniform torsional moment to the proﬁle and measures the rotation. It is important to note that the torsional stiffness thus obtained is the unrestrained or nonwarping restrained torsional stiffness (also known as the Saint-Venant torsional stiffness). In most structural engineering applications the ends of the structural members are restrained against warping and the warping torsional constant (ECw) is needed for design. This can be measured in an indirect method using a nonuniform torsion test (Roberts and Al-Ubaidi, 2002). It should also be pointed out that singly symmetric open-cross-section FRP proﬁles have very low torsional rigidity and should not be used in situations where signiﬁcant torsional moment carrying resistance is needed. When used as beams and columns, FRP proﬁles must be laterally braced to prevent lateral or torsional instability under bending or axial loads. Full-section tests to determine the strengths and stiffness of connections in pultruded structures are not standardized at this time. Most manufacturers of pultruded proﬁles provide load tables for simple framing connections. These tables are based on full-section testing of subassemblies of proﬁles conducted using undisclosed in-house methods. Data are generally not provided on fail-

118

PROPERTIES OF FRP COMPOSITES

ure modes or deformations, nor are they correlated with coupon property data obtained from bearing tests. Neither is there a standard procedure for fullsection testing of semirigid connections for pultruded frame structures that is needed to obtain strength and moment–rotation characteristics for these connections for use in the analysis of frames with semirigid connections. Singleand double-beam methods proposed by Bank et al. (1990) and Mottram and Zheng (1999a,b) have been used in a number of investigations.

3.4 RELEVANT STANDARD TEST METHODS FOR FRP COMPOSITES FOR STRUCTURAL ENGINEERS 3.4.1

American Society of Testing and Materials Test Methods

ASTM Standard Test Methods C 1557 D 149 D 256 D 570 D 635 D 638 D 648 D 695 D 696 D 790 D 792 D 953 D 1929 D 2343 D 2344

Standard Test Method for Tensile Strength and Young’s Modulus of Fibers Standard Test Method for Dielectric Breakdown Voltage and Dielectric Strength of Solid Electrical Insulating Materials at Commercial Power Frequencies Standard Test Methods for Determining the Izod Pendulum Impact Resistance of Plastics Standard Test Method for Water Absorption of Plastics Standard Test Method for Rate of Burning and/or Extent and Time of Burning of Plastics in a Horizontal Position Standard Test Method for Tensile Properties of Plastics Standard Test Method for Deﬂection Temperature of Plastics Under Flexural Load in the Edgewise Position Standard Test Method for Compressive Properties of Rigid Plastics Standard Test Method for Coefﬁcient of Linear Thermal Expansion of Plastics Between ⫺30⬚C and 30⬚C with a Vitreous Silica Dilatometer Standard Test Methods for Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials Standard Test Methods for Density and Speciﬁc Gravity (Relative Density) of Plastics by Displacement Standard Test Methods for Bearing Strength of Plastics Standard Test Method for Determining Ignition Temperature of Plastics Standard Test Method for Tensile Properties for Glass Fiber Strands, Yarns, and Rovings Used in Reinforced Plastics Standard Test Method for Short-Beam Strength of Polymer Matrix Composite Materials and Their Laminates

3.4

D 2583 D 2584 D 3039 D 3171 D 3379 D 3410 D 3846 D 3916 D 4018 D 4475 D 4476 D 4762 D 5083 D 5379 D 5961 D 6856 E 84 E 662 E 831 E 1356 E 1640 E 2092

RELEVANT STANDARD TEST METHODS

119

Standard Test Method for Indentation Hardness of Rigid Plastics by Means of a Barcol Impressor Standard Test Method for Ignition Loss of Cured Reinforced Resins Standard Test Method for Tensile Properties of Polymer Matrix Composite Materials Standard Test Method for Constituent Content of Composite Materials Standard Test Method for Tensile Strength and Young’s Modulus of High-Modulus Single-Filament Materials Standard Test Method for Compressive Properties of Polymer Matrix Composite Materials with Unsupported Gage Section by Shear Loading Standard Test Method for In-Plane Shear Strength of Reinforced Plastics Standard Test Method for Tensile Properties of Pultruded GlassFiber-Reinforced Plastic Rod Standard Test Methods for Properties of Continuous Filament Carbon and Graphite Fiber Tows Standard Test Method for Apparent Horizontal Shear Strength of Pultruded Reinforced Plastic Rods by the Short-Beam Method Standard Test Method for Flexural Properties of Fiber-Reinforced Pultruded Plastic Rods Standard Guide for Testing Polymer Matrix Composite Materials Standard Test Method for Tensile Properties of Reinforced Thermosetting Plastics Using Straight-Sided Specimens Standard Test Method for Shear Properties of Composite Materials by the V-Notched Beam Method Standard Test Method for Bearing Response of Polymer Matrix Composite Laminates Standard Guide for Testing Fabric-Reinforced ‘‘Textile’’ Composite Materials Standard Test Method for Surface Burning Characteristics of Building Materials Standard Test Method for Speciﬁc Optical Density of Smoke Generated by Solid Materials Standard Test Method for Linear Thermal Expansion of Solid Materials by Thermomechanical Analysis Standard Test Method for Assignment of the Glass Transition Temperatures by Differential Scanning Calorimetry or Differential Thermal Analysis Standard Test Method for Assignment of the Glass Transition Temperature by Dynamic Mechanical Analysis Standard Test Method for Distortion Temperature in Three-Point Bending by Thermal Mechanical Analysis

120

PROPERTIES OF FRP COMPOSITES

ASTM Standard Terminologies C 162 C 904 D D D D D

123 883 907 3878 3918

E6 E 631

Standard Terminology Standard Terminology lic Materials Standard Terminology Standard Terminology Standard Terminology Standard Terminology Standard Terminology Products Standard Terminology Standard Terminology

of Glass and Glass Products Relating to Chemical-Resistant NonmetalRelating to Textiles Relating to Plastics of Adhesives of Composite Materials Relating to Reinforced Plastic Pultruded Relating to Methods of Mechanical Testing of Building Constructions

ASTM Standard Speciﬁcations D 3917

Standard Speciﬁcation for Dimensional Tolerance of Thermosetting Glass-Reinforced Plastic Pultruded Shapes

ASTM Standard Practices C 581 D 618 E 122 E 632

3.4.2

Standard Practice for Determining Chemical Resistance of Thermosetting Resins Used in Glass-Fiber-Reinforced Structures Intended for Liquid Service Standard Practice for Conditioning Plastics for Testing Standard Practice for Calculating Sample Size to Estimate, with a Speciﬁed Tolerable Error, the Average for a Characteristic of a Lot or Process Standard Practice for Developing Accelerated Tests to Aid Prediction of the Service Life of Building Components and Materials Full-Section Test Methods for FRP Bars and Laminates

ACI Test Methods for FRP Bars for Concrete Structures B.1 B.2 B.3 B.4 B.5 B.6 B.7 B.8

Test Method for Cross-Sectional Properties of FRP Bars Test Method for Longitudinal Tensile Properties of FRP Bars Test Method for Bond Strength of FRP Bars by Pullout Testing Test Method for Transverse Shear Strength of FRP Bars Test Method for Strength of FRP Bent Bars and Stirrups at Bend Locations Accelerated Test Method for Alkali Resistance of FRP Bars Test Method for Tensile Fatigue of FRP Bars Test Method for Creep Rupture of FRP Bars

3.4

RELEVANT STANDARD TEST METHODS

121

B.9 B.10 B.11 B.12

Test Method for Long-Term Relaxation of FRP Bars Test Method for Performance of Anchorages of FRP Bars Test Method for Tensile Properties of Deﬂected FRP Bars Test Method for Determining the Effect of Corner Radius on Tensile Strength of FRP Bars Appendix A: Anchor for Testing FRP Bars Under Monotonic, Sustained and Cyclic Tension ACI Test Methods for FRP Laminates for Concrete and Masonry L.1 Test Method for Direct Tension Pull-off Test L.2 Test Method for Tension Test of Flat Specimen L.3 Test Method for Overlap Splice Tension Test Appendix B: Methods for Calculating Properties of Flat Specimen CEN 13706 Test Methods for FRP Pultruded Proﬁles CEN Normative Test Methods Part Part Part Part Part

2 2 2 2 2

Annex Annex Annex Annex Annex

A B C D E

Visual Defects: Descriptions and Acceptance Levels Dimensional Tolerance for Pultruded Proﬁles Workmanship Determination of Effective Flexural Modulus Determination of the Pin Bearing Strength

CEN Informative Test Methods Part 2 Annex F Part 2 Annex G

Recommended Test Methods for Particular Requirements Determination of Flexural Shear and Torsional Stiffness Properties

CSA S806 Standard Test Methods for FRP Bars and Laminates CSA Normative Test Methods Annex A Annex B Annex Annex Annex Annex Annex

C D E F G

Determination of Cross-Sectional Area of FRP Reinforcement Anchor for Testing FRP Specimens Under Monotonic, Sustained and Cyclic Tension Test Method for Tensile Properties of FRP Reinforcements Test Method for Development Length of FRP Reinforcement Test Method for FRP Bent Bars and Stirrups Test Method for Direct Tension Pull-off Test Test Method for Tension Test of Flat Specimens

122

PROPERTIES OF FRP COMPOSITES

CSA Informative Test Methods Annex Annex Annex Annex Annex

H J K L M

Annex N Annex O Annex P Annex Q

Test Method for Bond Strength of FRP Rods by Pullout Testing Test Method for Creep of FRP Rods Test Method for Long-Term Relaxation of FRP Rods Test Method for Tensile Fatigue of FRP Rods Test Method for Coefﬁcient of Thermal Expansion of FRP Rods Test Method for Shear Properties of FRP Rods Test Methods for Alkali Resistance of FRP Rods Test Methods for Bond Strength of FRP Sheet Bonded to Concrete Test Method for Overlap Splice in Tension

Japan Society of Civil Engineers Standard Test Methods for Continuous Fiber Reinforcing Materials JSCE-E-131 JSCE-E 531 JSCE-E 532 JSCE-E 533 JSCE-E 534 JSCE-E 535 JSCE-E 536 JSCE-E 537 JSCE-E 538 JSCE-E 539 JSCE-E 540

Quality Speciﬁcation for Continuous Fiber Reinforcing Materials Test Method for Tensile Properties of Continuous Fiber Reinforcing Materials Test Method for Flexural Tensile Properties of Continuous Fiber Reinforcing Materials Test Method for Creep of Continuous Fiber Reinforcing Materials Test Method for Long-Term Relaxation of Continuous Fiber Reinforcing Materials Test Method for Tensile Fatigue of Continuous Fiber Reinforcing Materials Test Method for Coefﬁcient of Thermal Expansion of Continuous Fiber Reinforcing Materials by Thermo Mechanical Analysis Test Method for Performance of Anchors and Couplers in Prestressed Concrete Using Continuous Fiber Reinforcing Materials Test Method for Alkali Resistance of Continuous Fiber Reinforcing Materials Test Method for Bond Strength of Continuous Fiber Reinforcing Materials by Pull-out Testing Test Method for Shear Properties of Continuous Fiber Reinforcing Materials by Double Plane Shear

Japan Society of Civil Engineers Standard Test Methods for Continuous Fiber Sheets JSCE-E 541

Test Method for Tensile Properties of Continuous Fiber Sheets

PROBLEMS

JSCE-E 542 JSCE-E 543 JSCE-E 544 JSCE-E 545 JSCE-E 546 JSCE-E 547 JSCE-E 548 JSCE-E 549

123

Test Method for Overlap Splice Strength of Continuous Fiber Sheets Test Method for Bond Properties of Continuous Fiber Sheets to Concrete Test Method for Bond Strength of Continuous Fiber Sheets to Steel Plate Test Method for Direct Pull-off Strength of Continuous Fiber Sheets with Concrete Test Method for Tensile Fatigue of Continuous Fiber Sheets Test Method for Accelerated Artiﬁcial Exposure of Continuous Fiber Sheets Test Method for Freeze-Thaw Resistance of Continuous Fiber Sheets Test Method for Water, Acid and Alkali Resistance of Continuous Fiber Sheets

PROBLEMS 3.1 Write a computer program to calculate the stiffness properties (Ex, Ey, Gxy ⫽ Es, and x) of a two-dimensional FRP composite given the properties of the ﬁber and matrix. Assume that both the matrix and the ﬁber are isotropic and use the material properties given below. Use the rule-of-mixtures micromechanics equations. (a) Use your program to verify the results of Analysis Example 3.1. (b) Plot the stiffness properties (Ex, Ey, Gxy ⫽ Es, and x) for an Eglass/vinylester composite and for a carbon–epoxy composite as a function of ﬁber volume fraction from 20 to 60%. (c) Plot the longitudinal strength of the two FRP composites above as a function of ﬁber volume from 20 to 60%. (d) Plot the ﬁber weight (or mass) fraction as a function of ﬁber volume fraction from 20 to 60%. The following properties are given for the ﬁbers and matrices. For the E-glass ﬁber: E (psi) ult ƒ (psi) (lb/in3) For the carbon ﬁber:

10,500,000 0.20 270,000 9.400 ⫻ 10⫺2

124

PROPERTIES OF FRP COMPOSITES

E (psi) ult (psi) (lb/in3)

33,000,000 0.20 570,000 6.500 ⫻ 10⫺2

For the vinylester matrix: E (psi) ult (psi) (lb/in3)

500,000 0.38 11,000 4.570 ⫻ 10⫺2

E (psi) ult (psi) (lb/in3)

620,000 0.34 11,300 4.570 ⫻ 10⫺2

For the epoxy:

3.2 Write a computer program to calculate the off-axis stiffness coefﬁcients [Qij (i,j ⫽ 1,2,6)] for a composite lamina with on-axis stiffness coefﬁcients [Qij (i,j ⫽ x,y,s)] rotated at an angle from the structural axes (1,2,6) when given the engineering constants (Ex, Ey, Es, x) of the lamina. You can use any programming language. A high-level language/program such as MathCad, MatLab, or Excel is recommended. (a) Use your program to verify the off-axis stiffness coefﬁcients of the ⫹10⬚ carbon–epoxy lamina in Analysis Example 3.3. (b) For the 51% volume fraction E-glass/polyester lamina in Example 3.2, provide a plot of the engineering constants (E1, E2, E6, 21) as a function of the angle from 0 to 360⬚. Discuss how the properties vary relative to one another as the lamina (ply) is rotated through 360⬚. (c) For the 23% continuous ﬁlament mat lamina in Analysis Example 3.2, provide a plot of the engineering constants (E1, E2, E6, 21) as a function of the angle from 0 to 360⬚. Discuss how the properties vary relative to one another as the lamina (ply) is rotated through 360⬚. 3.3 Write a computer program to (1) calculate the [A–B–D] matrix for a three-ply laminate with arbitrary ply thicknesses and properties, and (2) calculate the effective in-plane and ﬂexural engineering properties of the laminate. You can use any programming language. A high-level language/program such as MathCad, MatLab, or Excel is recommended.

PROBLEMS

125

(a) Use the program to verify the results of Analysis Example 3.2. (b) Use the program to verify the results of Analysis Example 3.3. 3.4 Given a quasi-isotropic eight-layer [0/90/ ⫹45/ ⫺45]s laminate of Eglass/polyester with a 51% ﬁber volume fraction per layer. Use material properties from Analysis Example 3.2. Show that the laminate is isotropic for its in-plane stiffness but not isotropic for its ﬂexural stiffness; that is, show that E 01 ⫽ E 02

Eƒ1 ⫽ Eƒ2

and E 06 ⫽

E 01 2(1 ⫺ 01)

Eƒ6 ⫽

Eƒ1 2(1 ⫹ ƒ1)

3.5 An FRP laminate is to be used to strengthen a concrete structure. The laminate is constructed of three plies of SikaWrap Hex 103C unidirectional carbon ﬁber fabric and SikaDur Hex 306 epoxy resin. The layup for the laminate is given as [0/90/0]. The longitudinal axis (the 1-direction) of the laminate is at 0⬚. Manufacturer speciﬁcation sheets for the fabric–resin system are available at www.sikaconstruction.com. You are required to consult the speciﬁcation sheets to obtain the data you need for the calculations to follow. Use the average values measured at room temperature for the lamina properties. In addition to the data provided in the speciﬁcation sheets, you are given that the major Poisson ratio for a single composite ply of the SikaWrap Hex 103C unidirectional carbon ﬁber fabric with SikaDur Hex 306 epoxy resin is x ⫽ 0.32 (since this property is not reported by the manufacturer). For the FRP laminate described, ﬁnd the following: (a) The on-axis stiffness matrix [Q] for a single ply of the SikaWrap Hex 103C unidirectional carbon ﬁber fabric and SikaDur Hex 306 epoxy resin. (b) The [A] matrix for the three-ply laminate. (c) The effective longitudinal in-plane (extensional) modulus of the laminate (in the 0⬚ direction). (d) The ﬁber volume fraction (assuming no voids in the composite). 3.6 Given a –14 -in.-thick pultruded material that will be used in a 6 ⫻ 6 in. wide ﬂange pultruded proﬁle (i.e., the ﬂange width is 6 in. and the web depth is 6 in.). The FRP material consists of E-glass/polyester and consists of four 1.0-oz/ft2 E-glass continuous ﬁlament mats and two layers of unidirectional 113 yield glass roving, as shown in Fig.

126

PROPERTIES OF FRP COMPOSITES

1-oz CFM, t = 0.02 in. 100-113 yield E-glass rovings, t = 0.085 in. two 1-oz CFM, t = 0.04 in. 100-113 yield E-glass rovings, t = 0.085 in. 1-oz CFM, t = 0.02 in.

Figure P3.6 Pultruded material layup.

P3.6 (in a 6-in. width). The area of one 113 yield roving is given as 2.615 ⫻ 10⫺3 in2. The isotropic properties of the E-glass/polyester resin matrix are as follows: Eglass ⫽ 10.5 ⫻ 106 psi

Epolyester ⫽ 4.7 ⫻ 105 psi

glass ⫽ 0.20

polyester ⫽ 0.38

ult ⫽ 270 ksi

ult ⫽ 10.4 ksi

The in-plane engineering properties of the CFM layer are E ⫽ 1.26 ⫻ 106 psi

⫽ 0.35

Xt ⫽ 12.45 ksi

Determine the following: (a) The ﬁber volume fraction in the roving layer. (b) The engineering stiffness properties (Ex, Ey, Es, x, y) of the roving layer using the rule-of-mixtures equations. (c) The engineering stiffness properties (Ex, Ey, Es, x, y) of the CFM layer. (d) The [A] matrix of the layup. (e) The [D] matrix of the layup. (f) The effective engineering in-plane extensional properties of the material: E 0x , E y0, E s0, x0, y0. Compare these properties with those given by Strongwell and Creative Pultrusions for their E-glass/polyester pultruded proﬁles (see online speciﬁcation sheets). Discuss the differences and similarities between the calculated and manufacturerreported data. (g) Provide an estimate of the longitudinal tensile strength of the material. Justify your answer with an explanation and show how you have calculated the strength.

PROBLEMS

127

3.7 Review ASTM test methods D 3039, D 638, and D 5083 for tensile testing of composites and plastics and list their similarities and differences in tabulated form. 3.8 Review ASTM test methods D 3171 and D 2548 for volume fraction testing and discuss the various methods. Explain why different methods are used for different types of composite materials. 3.9 Review ASTM test methods D 1356, D 1640, and D 648 for glass transition temperature and heat deﬂection temperature. Do these test methods measure the same physical or mechanical property for the ﬁber-reinforced polymer? Why are these properties important to know when using FRP composites in structural engineering? 3.10 To determine the four independent in-plane engineering stiffness constants (Ex, Ey, Es, x) of an orthotropic lamina of FRP composite material, longitudinal (for Ex, x), transverse (for Ey), and in-plane shear (for Es) tests are required. It is often difﬁcult or impossible to perform transverse and in-plane shear testing due to the coupon size required for the testing relative to the size of the part from which it is cut or 1 the complexity of the test itself. For example, a 4-in. wide by –– 16 -in. FRP strengthening strip is too narrow to comply with the requirements of ASTM D 3039 for tensile testing or too thin to be used in the special testing ﬁxture for shear testing in accordance with ASTM D 5379. In addition, the special ﬁxture needed for shear testing (called the Iosipescu ﬁxture) requires time-consuming specimen preparation and strain gauging. It is, however, possible to obtain the four independent properties of an orthotropic lamina by using only the tensile test. To do this, one tests a coupon cut parallel to the major axis of orthotropy (the ﬁber direction) and another coupon cut at an angle (typically, 10 to 15⬚) from the major axis of orthotropy. In both tests the longitudinal and the transverse strains (parallel and perpendicular to the coupon edges) are measured as a function of applied load (or stress). Show analytically how the experimental data obtained from these two tests can be used to calculate all four of the in-plane stiffness properties of the orthotropic lamina. (Hint: Use the expressions for engineering properties and the on- and off-axis compliance relationships.)

4 4.1

Design Basis for FRP Reinforcements OVERVIEW

In this chapter we introduce the subject of FRP reinforcing bars (FRP rebars) for reinforced concrete structures such as beams and slabs. The properties of FRP reinforcing bars are reviewed and their behavior under different loads is discussed. The primary focus of this book is on glass ﬁber reinforced bars. Although the design procedures presented are applicable to FRP rebars made of other reinforcing ﬁbers, such as carbon or aramid ﬁbers, at present economical rebars of these types are not generally available for concrete reinforcing applications. We then proceed to describe the basis for the design of concrete members reinforced with FRP bars. This basis is in accordance with American Concrete Institute publication ACI 440.1R-06, Guide to the Design and Construction of Structural Concrete Reinforced with FRP Bars (ACI, 2006). This document is compatible with ACI publication ACI 318-05, Building Code Requirements for Structural Concrete and Commentary (ACI, 2006). Throughout this chapter and subsequent chapters that describe in detail the procedures for the design of concrete structures with FRP rebars, it is assumed that the reader has reasonable familiarity with ACI 318-05 and that the reader is familiar with the design of concrete beams and slabs reinforced with conventional steel reinforcing bars. The equations and examples presented in what follows use U.S. standard units throughout since these are the familiar units for design in the United States, where the ACI codes are mainly used. With regard to FRP reinforcing bars, one of the purposes of the book is to point out the key differences between design with steel bars and design with FRP bars. Extensive examples are not presented; rather, a limited number of detailed illustrative examples are presented. These examples generally follow those in ACI 440.1R-06 and are intended to allow the reader to analyze these examples critically and compare them to steel-reinforced design. After studying the book readers are challenged to open their favorite text on reinforced concrete design and attempt to compete the example problems in that text using FRP rebars rather than steel rebars. Only by understanding the differences between steel and FRP reinforced concrete design can readers truly get a feel for design with FRP bars.

128

Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

4.3

4.2

PROPERTIES OF FRP REINFORCING BARS

129

INTRODUCTION

Fiber-reinforced plastic (FRP) reinforcing bars and grids have been produced for reinforcing concrete structures for over 30 years (Nanni, 1993b; ACI, 1996). FRP reinforcing bars have been developed for prestressed and nonprestressed (conventional) concrete reinforcement. In this section we consider only nonprestressed reinforcement for concrete structures. A review of design recommendations for FRP reinforcement for prestressed concrete structures can be found in Gilstrap et al. (1997). ACI guide 440.4R-04 (ACI, 2004b) provides design guidelines for prestressing concrete with FRP tendons. Current FRP reinforcing bars (referred to as FRP rebars in what follows) and grids are produced commercially using thermosetting polymer resins (commonly vinylester and epoxy) and glass, carbon, or aramid reinforcing ﬁbers. The bars are primarily longitudinally reinforced with volume fractions of ﬁbers in the range 50 to 65%. FRP reinforcing bars are usually produced by a process similar to pultrusion and have a surface deformation or texture to develop bond to concrete. Photographs of typical FRP rebars are shown in Fig. 1.1. A number of design guides and national standards are currently published to provide recommendations for the analysis, design, and construction of concrete structures reinforced with FRP rebars (JSCE, 1997; Sonobe et al., 1997; Bakht et al., 2000; CSA, 2002; ACI, 2006). This book follows the ACI 440.1R-06 guidelines. A number of industry groups, including the Market Development Alliance of the American Composite Manufacturers Association (ACMA), coordinate activities of FRP rebar producers in the United States. Activities of these organizations are closely coordinated with American Concrete Institute (ACI) Technical Committee 440-FRP Reinforcements. Research in the use of FRP reinforcements in concrete structures has been the focus of intense international research activity since the late 1980s. A biannual series of symposia entitled ‘‘Fiber Reinforced Plastics in Reinforced Concrete Structures’’ (FRPRCS) has been the leading venue for reporting and disseminating research results. Symposia in the series date back to 1993. FRPRCS-7 was held in Kansas City, Missouri, in November 2005.

4.3

PROPERTIES OF FRP REINFORCING BARS

Glass ﬁber reinforced vinylester bars, the most common commercially produced FRP rebars, are available from a number of manufacturers. Bars are typically produced in sizes ranging from –38 in. (9 mm) in diameter to 1 in. (25 mm) in diameter (i.e., No. 3 to No. 8 bars). Bars have either a sandcoated external layer, a molded deformation layer, or a helically wound spiral

130

DESIGN BASIS FOR FRP REINFORCEMENTS

ﬁber layer, to create a nonsmooth surface. The longitudinal strength of FRP rebars is bar size dependent, due to materials used in different-sized bars and due to shear lag effects. The strength of a glass FRP bar decreases as the diameter increases. Figure 4.1 shows an FRP rebar cage produced for a concrete beam 8 ⫻ 12 in. ⫻ 9 ft long. The main bars are No. 7 glass FRP bars and the stirrups and top bars are No. 3 bars. FRP rebars cannot be bent and must be premanufactured with bends. Therefore, hooks at the ends of the beam for anchorage are produced as separate pieces and lap spliced to the main tension bars, as shown in Fig. 4.1. FRP rebars are typically elastic and brittle such that the stress–strain relation in axial tension is linear elastic to failure. Figures 4.2 and 4.3 show the failure mode and the stress–strain curve for a coupon from a glass FRP rebar tested in tension. The failure mode for a full-section test of an FRP rebar potted in end anchors is shown in Fig. 4.4. As noted, the ultimate tensile strength of FRP rebars decreases with bar diameter. Typical properties are given in Table 1.1 for glass ﬁber FRP rebars and carbon ﬁber FRP bars. It should be noted that the carbon ﬁber bars are typically used as prestressing tendons or near-surface-mounted (NSM) strengthening and not as conventional reinforcing bars due to cost considerations. In accordance with ACI 440.1R-06 recommendations for guaranteed tensile strength and longitudinal modulus,1 guaranteed properties of glass– vinylester FRP reinforcing bars commercially manufactured in North America are listed in Table 4.1. As noted, the strength of the reinforcing bar decreases with the diameter of the bar, however, the longitudinal modulus does not change appreciably. FRP rebars are considered to be transversely isotropic from a continuum mechanics perspective (Bank, 1993a). Theoretical equations used to predict the mechanical and physical properties of FRP rebars from the properties of ﬁber and resin constituents are provided in Chapter 3. Theoretical methods are not currently available to predict the bond properties and long-term du-

Figure 4.1 Reinforcing cage for a concrete beam made with FRP rebars. (Courtesy of Dushyant Arora.)

1

To be discussed further in what follows.

4.3

PROPERTIES OF FRP REINFORCING BARS

131

Figure 4.2 Failure of a tensile coupon cut from a No. 7 GRFP rebar. (Courtesy of Joshua Dietsche.)

120

100

Stress (ksi)

80

60

40

20

0 0

0.005

0.01

0.015

0.02

0.025

0.03

0.035

Strain (in./in.) extensometer

stroke

Figure 4.3 Tensile stress–strain curve for a glass FRP rebar coupon.

132

DESIGN BASIS FOR FRP REINFORCEMENTS

Figure 4.4 Pre- and posttested glass FRP rebars tested in end anchorages at full section.

rability characteristics of FRP rebars. Test methods for determining the properties of FRP rebars can be found in ACI 440.3R-04 (ACI, 2004a) and are described in Chapter 3. FRP rebars should only be used at service temperatures below the glass transition temperature of the polymer resin system used in the bar. For typical vinylester polymers this is around 200⬚F (⬃95⬚C). The bond properties have been shown to be highly dependent on the glass transition temperature of the polymer (Katz et al., 1999). TABLE 4.1 Guaranteed Properties of Glass FRP Rebars Produced in North America, 2005a Nominal Bar Size No.

Nominal Diameter (in.)

Nominal Area (in.2)

Reported Measured Area (in.2)

Guaranteed Longitudinal Strength (ksi)

Guaranteed Longitudinal Modulus (Msi)

2 3 4 5 6 7 8 9 10

0.25 0.375 0.50 0.625 0.75 0.875 1.0 1.125 1.25

0.05 0.11 0.20 0.31 0.44 0.60 0.79 1.00 1.27

0.05 0.13 0.23 0.34 0.46 0.59 0.83 1.00 1.25

120–127 110–111 100–103 95–99 90–95 85 80–87 75 70

5.9–6.7 5.9–6.3 5.9–6.4 5.9–6.8 5.9–6.9 5.9 5.9–6.0 5.9 5.9

a Not all manufacturers supply all bar sizes. Manufacturers’ current speciﬁcations must always be consulted for design calculations.

4.4

DESIGN BASIS FOR FRP-REINFORCED CONCRETE

133

The coefﬁcient of thermal expansion of an FRP rebar is not the same in the transverse (radial) direction as in the longitudinal direction (Gentry and Husain, 1999). The coefﬁcient of thermal expansion may be close to an order of magnitude higher in the transverse direction of the bar due to its anisotropic properties (see typical properties in Table 1.1). This may cause longitudinal splitting in the concrete at elevated temperatures if insufﬁcient cover is not provided. FRP rebars, especially those containing glass ﬁbers, can fail catastrophically under sustained load at stresses signiﬁcantly lower than their short-term static tensile strengths, a phenomenon known as creep rupture or static fatigue. The amount of sustained load on FRP rebars is therefore limited by design guides. FRP reinforcing bars made of thermosetting polymers (e.g., vinylester, epoxy) cannot be bent in the ﬁeld and must be produced by the FRP rebar manufacturer with ‘‘bends’’ for anchorages or for stirrups. The strength of the FRP rebar at the bend is substantially reduced and must be considered in the design. FRP rebars with thermoplastic polymer resins, which may allow them to be bent in the ﬁeld, are in the developmental stages. The compressive behavior of FRP rebars has not been studied adequately. It appears that the compressive properties of FRP bars may be lower than their tensile properties (Dietz et al., 2003). In addition, due to their low modulus, FRP rebars have a greater tendency to buckle than do steel rebars.

4.4

DESIGN BASIS FOR FRP-REINFORCED CONCRETE

In what follows the design basis of the American Concrete Institute presented in ACI 318-05 and ACI 440.1R-06 are followed with respect to design philosophy and load and resistance factors for design.2 Similar design bases, conforming to the limit states design procedure, are recommended by many standards organizations and professional organizations for FRP reinforced concrete (JSCE, 1997; Sonobe et al., 1997; Bakht et al., 2000; CSA, 2002). ACI 440.1R-06 recommends the use of traditional methods of strain compatibility and equilibrium to determine internal forces in an FRP reinforced concrete section. This includes the assumption that there is no slip (i.e., local relative longitudinal displacement) between the rebars and the concrete in an FRP-reinforced section. The resistance factors for ﬂexural strength design of glass FRP reinforced members have been developed using the LRFD probability-based approach. A reliability factor, , of at least 3.5 is obtained using the design methods presented in what follows. The calibration for the reliability factor was based on ASCE 7 load combination 2 (1.2D ⫹ 1.6L) and a ratio of dead load to

2 The ultimate strength design procedure, a load and resistance factor design (LRFD) procedure followed by ACI 440.1R-06, is compatible with ACI 318-05, which uses the load factors of ASCE 7.

134

DESIGN BASIS FOR FRP REINFORCEMENTS

live load of 1⬊3. It is important to note that the ﬂexural resistance factors presented in previous editions of ACI 440.1R (ACI, 2001, 2003) were not probabilistically calibrated, although they still provided safe designs. The resistance factor for shear strength design has not yet been probabilistically calibrated in ACI 440.1R-06. 4.4.1

Resistance Factors

The resistance factors for determination of the ultimate ﬂexural capacity and ultimate shear capacity of transversely loaded members (i.e., beams, slabs, and beam-columns) reinforced with FRP rebars as listed in ACI 440.1R-06 are given below.3 Flexural capacity:

冦

0.55 for an underreinforced beam section (ƒ ⬍ ƒb) 0.65 for a substantially overreinforced beam section (ƒ ⬎ 1.4ƒb) ⫽ 0.3 ⫹ 0.25ƒ / ƒb for a lightly overreinforced beam section (ƒb ⬍ ⬍ 1.4ƒb) (ACI 440.1R-06:8-7) Shear capacity: ⫽ 0.75

(ACI 318-05 Sec. 9.3.2.3)

In the equations above, ƒ is the FRP reinforcement ratio and ƒb is the balanced FRP reinforcement ratio for a rectangular cross section: ƒ ⫽

Aƒ bd

(ACI 440.1R-06: 8-2)

The balanced FRP reinforcement ratio is given as ƒb ⫽ 0.851

Eƒ cu ƒ⬘c ƒƒu Eƒ cu ⫹ ƒƒu

(ACI 440.1R-06: 8-3)

In these equations, Aƒ is the area of FRP reinforcement, b the width of the section, d the depth of the FRP reinforcement, 1 a factor that depends on concrete strength and is given in ACI 318-05 (e.g., 0.85 for 4000-psi concrete), ƒ⬘c the cylinder compressive strength of the concrete, Eƒ the guaranteed

3 Throughout this book, where equations are taken directly from ACI guides and codes, they are cited with the equation numbers or section numbers given in the source ACI documents.

4.4

DESIGN BASIS FOR FRP-REINFORCED CONCRETE

135

longitudinal modulus of the FRP rebar, cu the ultimate nominal compressive strain in the concrete (usually taken as 0.003), and ƒƒu the design longitudinal strength of the FRP rebar. Only tensile FRP reinforcement is considered in the design of FRPreinforced sections. If FRP reinforcement exists in the compression zone, it should not be considered in a determination of the strength of the section. Neither is it assumed to reduce the strength of the section. The resistance factors provided above for ﬂexural design do not consider any beneﬁcial or deleterious effect of FRP compression reinforcement on the capacity of the section. Rationale for Flexural Resistance Factors The rationale for the use of the ﬂexural resistance factors given above is based on the nature of the failure modes in over- and underreinforced RC sections with FRP rebars. When the section is underreinforced, the failure is due to rupture of the FRP bars in tension, which is sudden and catastrophic since FRP rebars currently available are brittle and linear elastic to failure. For this case, a resistance factor of ⫽ 0.55 has been obtained. Note that this is less than the factor of ⫽ 0.65 that is used for steel-reinforced concrete when brittle failure occurs per ACI 318-05. When the section is overreinforced, the failure is due to concrete crushing. This failure mode, although brittle, is somewhat less brittle than the mode due to FRP rupture and is assigned a higher resistance factor of ⫽ 0.65 when the overreinforced failure mode can be assured (i.e., the reinforcement ratio is signiﬁcantly above the balanced ratio). This resistance factor is equal to the resistance factor for brittle failure due to concrete crushing for steelreinforced concrete. When the section is slightly overreinforced, the resistance factor is assumed to vary from 0.65 down to 0.55 (equal to the underreinforced resistance factor), due to uncertainty in the actual failure mode that will occur. Note that the well-known ﬂexural resistance factor of ⫽ 0.90 that is used when ductile failure of a steel-reinforced concrete section is assured, when s ⬎ 0.005, can never be used for FRP-reinforced concrete. 4.4.2

Minimum Reinforcement Requirements

A minimum amount of FRP ﬂexural reinforcement is required to prevent sudden brittle failure in FRP underreinforced ﬂexural members. A minimum amount of FRP shear reinforcement is required to prevent sudden brittle shear failure in FRP ﬂexural members. In addition, to prevent cracking, a minimum amount of temperature and shrinkage reinforcement is required for FRPreinforced slabs. Details are provided in later chapters. 4.4.3

Determination of Guaranteed Properties of FRP Rebars

The FRP bar strength (called the guaranteed strength) and strain to failure of FRP rebars (called the guaranteed rupture strain) are deﬁned as the mean

136

DESIGN BASIS FOR FRP REINFORCEMENTS

minus three standard deviations of a minimum of 25 test samples. The guar* , are expected to be anteed design strength, ƒ* ƒu, and design failure strain, ƒu supplied by the manufacturer. FRP rebars must be tested according to the procedures detailed in ACI 440.3R-04 (see Chapter 3 for details). The strength of an FRP rebar at a bend is highly dependent on the manufacturing processes. As noted previously, FRP rebars produced with thermosetting polymer resins such as polyester, vinylester, and epoxy must be bent during production prior to the resin curing. ACI 440.3R-04 provides two test methods for determining the effect of bends on the tensile strength of FRP bars. However, manufacturers at this time, are not required to report a guaranteed strength of FRP bars with bends, nor are there standard dimensions for bend radii at this time. An analytical equation for determining the strength of a bar with a bend is provided in ACI 440.1R-06.

冉

ƒƒb ⫽ 0.05

冊

rb ⫹ 0.3 ƒƒu db

(ACI 440.1R-06:7-3)

where ƒƒb is the tensile strength of the FRP rebar with a bend, rb the inside radius of the bend, and db the diameter of the FRP rebar. A minimum inside radius-to-diameter ratio of 3 is required. Standard bend radii are reported by manufacturers and range from 2 to 3 in. for typical FRP rebars.

4.4.4

Design for Environmental Effects on FRP Rebars

The design strength, ƒƒu ,and design failure strain, ƒu , are obtained from the guaranteed strength and guaranteed failure strain by multiplying them by an environmental reduction factor, CE, which depends on the ﬁber type in the bar and the type of service intended, as shown in Table 4.2.

TABLE 4.2 440.1R-06

Environmental Reduction Factors for FRP Rebars from ACI

Exposure Condition Concrete not exposed to ground and weather

Concrete exposed to ground and weather

Fiber Type

Environmental Reduction Factor, CE

Carbon Glass Aramid Carbon Glass Aramid

1.0 0.8 0.9 0.9 0.7 0.8

4.4

DESIGN BASIS FOR FRP-REINFORCED CONCRETE

ƒƒu ⫽ CE ƒ* ƒu

137

(ACI 440.1R-06:7-2)

The environmental reduction factor accounts for the fact that even though FRP rebars are not susceptible to conventional electropotential corrosion that affects metallic materials, they can nevertheless deteriorate in a variety of chemical environments, both alkaline and acidic. This deterioration is accelerated at elevated temperatures. Glass ﬁbers are especially susceptible to corrosion in alkaline and neutral solutions, due to leaching of the ﬁber (Bank et al., 1995b). Aramid ﬁbers do not leach like glass ﬁbers but are known to absorb moisture and swell, leading to loss of mechanical and physical properties. Carbon ﬁbers are the most chemically inert and are generally recommended when extreme exposure to chemical aqueous environments is anticipated. In addition, the polymer matrix is susceptible to deterioration in various chemical environments. Polymer resin producers and manufacturers of FRP products typically supply a corrosion-resistance guide that lists the various chemical exposures that are known to affect their materials. The outer surface of the FRP rebars is the part of the bar that is typically most vulnerable to chemical attack. Once the outer layer has been breached, diffusion of chemical solutions to the interior of the bar can occur more readily. In some cases the exterior helical wrap or deformation layer on the bar can aid in protecting the outer surface, in other cases it has been shown that the outer layer can detach from the core and lead to separation of the exterior layer from the interior core of the bar (Bank et al., 1998). Scanning electron micrographs (SEMs) of deterioration at the surface of a smooth bar and deterioration at the exterior wrap and core interfaces is show in Figs. 4.5 and 4.6. The FRP bar modulus (also called the speciﬁed tensile modulus), Eƒ, measured in the axial direction of the bar, is deﬁned as the average modulus of bars tested in accordance with ACI 440.3R-04. No reduction of the measured modulus is required for either statistical or environmental reasons. 4.4.5

Special Considerations Regarding FRP Rebars

As with steel bars, the design of FRP-reinforced concrete is conducted using only the longitudinal properties (ƒƒu, ƒu, Eƒ) of the bars. This assumes that the transverse properties of the FRP bars and the shear properties of the FRP bars, which are known to be signiﬁcantly lower than the longitudinal properties of the bars due to the anisotropic nature of FRP materials, do not signiﬁcantly inﬂuence the ﬂexural behavior of an FRP-reinforced RC section. This has been veriﬁed in numerous research studies (Faza and Gangarao, 1993; Nanni, 1993b; Benmokrane et al., 1996a). Since FRP reinforcing bars are linear elastic to failure, redistribution of moments and development of plastic hinges in statically indeterminate FRP reinforced concrete structures cannot be assumed to occur as in steel-

138

DESIGN BASIS FOR FRP REINFORCEMENTS

Figure 4.5 Deterioration at the bar surface following accelerated conditioning of a smooth FRP bar.

Figure 4.6 Deterioration at the exterior polymer surface following accelerated conditioning of an FRP bar.

4.4

DESIGN BASIS FOR FRP-REINFORCED CONCRETE

139

reinforced concrete structures. Where FRP bars are used in layers the stress in each of the layers must be calculated separately to determine the moment capacity of the section. The outermost layer of bars must be used to determine the ﬂexural capacity of the member when a beam fails due to FRP rupture. (In steel-reinforced concrete beams it is permissible to assume that the resultant tensile force in the bars acts through the centroid of the bar layers since all bars will be at their yield stress at ultimate failure.) At this time, FRP reinforcing bars should not be use as compression reinforcement, as insufﬁcient test data on the compression properties of FRP bars have been obtained. If FRP bars are placed in the compression zones of members, they should not be assumed to carry any compression load, and they should be conﬁned adequately to prevent local bucking, which could lead to premature concrete compression failure. The use of shear-friction and strut-and-tie design methods (Nilsen et al., 2004) to determine the ultimate capacity of concrete structures reinforced with FRP bars has not been studied in sufﬁcient detail at this time and is not discussed by ACI 440.1R-06. 4.4.6

Design for Serviceability

The design of FRP rebars for the serviceability limit state considers two primary serviceability conditions; deﬂection and cracking. Since FRP rebars typically have a lower modulus than that of steel rebars, the serviceability limit states (deﬂections and crack widths) can often control the design of FRP-reinforced concrete sections. Permissible service load deﬂections for FRP-reinforced concrete structures are generally taken as the same as those for all structures, and pertinent building code guidelines should be followed. Permissible crack widths for FRP-reinforced concrete are not the same as for conventional reinforced concrete structures, due to the superior corrosion resistance of FRP bars. Limits on Crack Widths Limits on maximum crack width under service loads for FRP-reinforced concrete are recommended. The limits on crack widths are intended to limit the ingress of ﬂuids that could degrade the FRP bars, and also to ensure an acceptable aesthetic appearance of an FRPreinforced ﬂexural member. Although perhaps not technically unsafe, large ﬂexural cracks may cause public discomfort, due to a perceived risk of structural collapse. The maximum crack widths recommended by ACI 440.1R-06 are listed in Table 4.3 together with the historically recognized permissible crack widths for steel-reinforced concrete from ACI 318-95 (ACI, 1995). It is important to note that since ACI 318-99 (ACI, 1999) the explicit calculation of crack widths and limits on crack widths in reinforced concrete structures has not been required for design of steel-reinforced concrete. An indirect method based on the spacing of the reinforcing bars as a function of the bar stress at service loads and the concrete cover is now used for steel-reinforced concrete. However, due to the possibility of low ﬂexural rigidity and the high

140

DESIGN BASIS FOR FRP REINFORCEMENTS

TABLE 4.3

Permissible Crack Widths for FRP and Steel RC Structures

Exposure

FRP-Reinforced Concrete [in. (mm)]

Steel-Reinforced Concrete [in. (mm)]

Exterior Interior

0.020 (0.5) 0.028 (0.7)

0.013 (0.3) 0.016 (0.4)

strength of FRP-reinforced concrete members, ACI 440.1R-06 still recommends the explicit calculation of crack widths in concrete structures reinforced with FRP bars. Limits on Service Load Stresses To prevent failure of FRP-reinforced beams at service loads due to creep rupture, fatigue, or other long-term environmental effects, the stress in FRP rebars under sustained service loads or fatigue loads is limited by ACI 440.1R-06 to a fraction of its design strength. These limits depend on the type of ﬁber in the FRP rebar. For glass FRP rebars, the limiting stress is 20% of the ultimate strength (i.e., 0.2ƒƒu.) For aramid- and carbon-reinforced FRP bars, the limits are 0.3ƒƒu and 0.55ƒƒu, respectively. 4.4.7

Temperature and Shrinkage Reinforcement in Slabs

In one-way slabs, a minimum amount of reinforcement is required perpendicular to the main bars to limit cracking parallel to the main bars that may develop due to thermal and shrinkage effects in the concrete. A modiﬁed version of the ACI 318-05 equations for steel rebars is provided by ACI 440.1R-06. The minimum amount of temperature and shrinkage reinforcement required is ƒ,ts ⫽ 0.0018

冉 冊

60,000 Es ƒƒu Eƒ

(ACI 440.1R-06:10-1)

but not less than 0.0014. The reinforcement ratio, ƒ,ts, is computed over the gross concrete area, and Es is the modulus of grade 60 steel rebar. The spacing of the FRP temperature and shrinkage reinforcement should not exceed three times the slab thickness, or 12 in. PROBLEMS 4.1 Visit the following FRP rebar manufacturers’4 Web sites and request or download copies of their FRP rebar property speciﬁcation sheets. These will be needed for solving design problems in the chapters that follow. 4 No endorsement of the manufacturers listed is implied. The reader is free to choose any manufacturer’s products to use in the examples that follow, and is encouraged to collect similar data for locally available FRP rebars.

PROBLEMS

141

Hughes Brothers (Aslan 100, Aslan 200): www.hughesbros.com Pultrall (V-Rod): www.pultrall.adsinc.ca or www.ﬁberglassrebar.com Scho¨ck (comBAR): www.schoeck.com Pullwell (R-bar): www.pullwellpultrusions.com 4.2 For the following FRP rebars, determine5 the ACI 440.1R-06 design strength, ƒƒu, the design failure strain, ƒu, and the design longitudinal modulus, Eƒ, when the rebar is used in a concrete structure exposed to the ground. Also, indicate the weight per unit length and the current sales price of the rebar per foot of length.6 Attach copies of the manufacturer’s speciﬁcation sheets to your homework. (a) No. 3 Aslan 100 GFRP bar (b) No. 3 V-Rod GFRP bar (c) No. 8 Aslan 100 GFRP bar (d) No. 8 V-Rod GFRP bar (e) No. 3 Aslan 200 CFRP bar (f) No. 3 V-rod CFRP bar (g) 8 comBAR GFRP bar (h) 32 comBAR GFRP bar (i) 9 R-bar GFRP bar (j) 32 R-bar GFRP bar 4.3 Derive the expression for the balanced reinforcement ratio for an FRPreinforced beam given in ACI 440.1R-06 as ƒb ⫽ 0.851

ƒ⬘c Eƒcu ƒƒu Eƒcu ⫹ ƒƒu

4.4 Determine the balanced reinforcement ratio for the beams listed in Table P4.4 when they are used in interior construction. Provide a bar graph comparing the balanced reinforcement ratios for the beams and discuss why there are such signiﬁcant differences in the balanced ratios for various types of reinforcement. 4.5 For the bars listed in the Problem 4.2, determine the strength of the bar at a bend. Assume a minimum bar radius at the bend equal to 3. Also, determine the percent decrease in bar strength at the bend for these bars. 4.6 Obtain strength, failure strain, stiffness, weight per foot, and cost per foot data for currently produced No. 3, No. 8, 8, and 32 steel and epoxy-coated steel reinforcing bars. Compare these data to those for the

5 This requires the manufacturer guaranteed strength as deﬁned by ACI 440.1R-06. If this is not provided, use the reported strength but be aware of the difference. 6 You will need to contact a distributor or the manufacturer to obtain pricing.

142

DESIGN BASIS FOR FRP REINFORCEMENTS

TABLE P4.4

Properties of Beams

Beam

ƒ⬘c (psi)

1 2 3 4 5 6 7 8 9 10

4000 4000 4000 4000 4000 8000 8000 8000 8000 8000

Rebar Type No. No. No. No. No. No. No. No. No. No.

4 6 8 3 6 4 6 8 3 6

Aslan 100 Aslan 100 Aslan 100 Aslan 200 grade 60 steel Aslan 100 Aslan 100 Aslan 100 Aslan 200 grade 60 steel

FRP bars obtained in Problem 4.2. Explain how the nominal strength, failure strain, and stiffness of a steel reinforcing bar are determined. List the numbers of the applicable ASTM test methods used to determine properties of steel and epoxy-coated steel reinforcing bars. How is the effect of the environment accounted for in the design of concrete structures reinforced with steel and epoxy-coated steel bars? SUGGESTED ACTIVITIES 4.1 Obtain samples of 3- to 4-ft No. 3 or No. 4 GFRP rebars. Also, obtain equivalent-diameter steel rebars. Try to bend the bars to create a permanent 90⬚ bend in the middle of the bar. Clamp one end in a vice and bend the other end by sliding a steel pipe over the free end to obtain some leverage. Push the FRP bar in only one direction and be careful, as the bar may break suddenly. Heat the FRP bar locally to see if this will help you to bend the FRP bar into the shape required. Now bend the FRP bar back and forth about 20 times, each time pushing a little farther. Record your observations with a digital camera. Write a 1000word report on your qualitative study of the properties of FRP rebars and steel bars under ﬂexural loads. (Make sure to take appropriate safety precautions when doing this activity. Coordinate this project with your laboratory manager and your safety engineer. Wear gloves, boots, long pants, and safety glasses. If heating, make sure that the room is ventilated and do not allow the bar to ignite.) 4.2 Obtain samples of small- and large-diameter (e.g., No. 3 and 7) glass FRP rebars. Cut short (1- to 2-in.) lengths of the bars using a circular saw with a masonry or diamond blade. Polish a cut end (to 200-grit paper) and observe it under an optical microscope. Observe ﬁber bundles, resin-rich areas, and surface deformations. Cut lengthwise sections of the bars and perform similar studies. Write a 1000-word report on your observations (including photomicrographs).

5 5.1

FRP Flexural Reinforcement OVERVIEW

In this chapter the design of ﬂexural members, such as beams and slabs, reinforced with FRP rebars is discussed. This includes procedures to determine the strength of either an over- or an underreinforced FRP concrete section according to ACI 440.1R-06 using the LRFD basis. We also provide procedures to design a ﬂexural member for serviceability limit states, which include deﬂection, ﬂexural crack width limitations, and maximum sustained stress on FRP bars under service loads. The design of ﬂexural members to resist transverse shear forces is discussed in Chapter 6. The geometric details, bond, and development length of FRP reinforcing bars are discussed in Chapter 7. The design procedures presented in this chapter follow ACI 440.1R-06, which is compatible with ACI 318-05. The reader is assumed to have familiarity with the design of ﬂexural members with conventional steel reinforcing bars. This includes having an understanding of the design of the section for serviceability and includes an understanding of the issues of bond and development length. In this chapter the ﬂexural design of a rectangular reinforced concrete section is discussed. The section may be a beam, which needs additional shear reinforcement to carry transverse loads, or it may be a slab, which may not need, and for constructability reasons should not have, shear reinforcement. In recent years, reinforcement of slabs has emerged as a large application area for FRP bars, particularly in highway bridge decks (Benmokrane et al., 2004). In the ﬂexural design of a slab without additional shear reinforcement, special attention must be paid to the shear capacity discussed in Chapter 6. The amount of tensile reinforcement in a slab can depend on the shear capacity of the slab, something that does not occur in a steelreinforced slab. 5.2

INTRODUCTION

Most structural engineers are relatively unfamiliar with the design of overreinforced beam sections, since traditional steel-reinforced concrete design philosophy strongly encourages the use of underreinforced sections. This is to ensure a ductile failure mode in steel-reinforced concrete beams. The desired failure mode in a steel-reinforced beam is yielding of the tension steel, Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

143

144

FRP FLEXURAL REINFORCEMENT

followed by eventual crushing of the concrete in the compression zone of the member. It is important for the reader to review the fundamentals of steelreinforced concrete design and to understand that even though the Whitney stress block is used to determine the strength of an underreinforced section, the failure is nevertheless due to the steel yielding and depends upon the plastic strain capacity of steel reinforcing bars. To an experienced structural engineer this may be obvious, but engineering students need to come to appreciate this fundamental fact. Since FRP reinforcing bars are linear elastic to failure when loaded in tension and fail in a brittle manner, a ductile steel-like failure does not occur in FRP-reinforced concrete. This is fundamentally different from steelreinforced concrete and makes the choice between an over- and underreinforced section much less clear. In fact, as will be seen in what follows, failure by concrete crushing, which is generally avoided in steel-reinforced concrete design, is slightly preferred in FRP-reinforced concrete design. This is because conﬁned concrete has some measure of postpeak large strain capacity, albeit at reduced stress levels. However, this large stain capacity is nothing like the large strain capacity of steel reinforcing bars. It will be seen in what follows that the commonly used Whitney rectangular compression stress block, which is so familiar to structural engineers who design underreinforced steel sections, will be used in the design of overreinforced FRP reinforced sections. This requires some new thinking and a different perspective on reinforced concrete design. Therefore, the reader is encouraged to review the fundamental derivation of the equations for steel-reinforced concrete design and to derive equations for the overreinforced concrete steel section using strain compatibility and equilibrium of the resultant forces in the section. This is discussed in most reinforced concrete textbooks, but usually not in great detail (Nilson et al., 2004). Figure 5.1 shows the difference in the behavior of steel- and FRPreinforced concrete beams based on the results of tests on six 98-in.-long (90in. simple span) reinforced concrete beams, all with the same 8 ⫻ 12 in. cross section (Ozel et al., 2003). The FRP beams were reinforced with three No. 7 glass FRP bars (FRP 1 and 2), and the steel beams were reinforced with three No. 6 grade 60 bars (steel 1 and 2) and three No. 5 grade 60 bars (steel 3 and 4), respectively. The relative reinforcement ratios, ƒ / bƒ and / b, for the FRP- and steel-reinforced beams were 3.14, 0.50, and 0.35, respectively. The concrete strength was close to 5000 psi in all beams. The steel-reinforced beams failed due to yielding of the steel rebars followed by crushing of the compression zone in the concrete. The FRP-reinforced beams failed due to crushing of the concrete in the compression zone (FRP 2) or debonding of the stirrups in the tension zone (FRP 1) (Ozel et al., 2003). The FRP reinforcement cage details for the FRP-reinforced beams were shown in Fig. 4.1. The failure modes of the FRP-reinforced beams are shown in Figs. 5.4 and 6.1. Notice the lower stiffness of the FRP-reinforced beams in the elastic range, even though their reinforcement ratios are much larger than those of the steel

5.3

FLEXURAL STRENGTH OF AN FRP-REINFORCED SECTION

80

145

STEEL 1 STEEL 2

Load (kips)

60

STEEL 4

STEEL 3

40 FRP 2

20

FRP 1

0 0.0

0.5

1.0

1.5

2.0

2.5

3.0

3.5

Crosshead Displacement (in.) Figure 5.1 Comparison of behavior of FRP- and steel-reinforced beams.

beams. Also notice the elastic–plastic behavior of the steel-reinforced beams and their eventual failure at large deﬂections. Note also, however, that due to their lower ﬂexural stiffness, the FRP-reinforced beams undergo large deﬂections that serve as a warning to the user. Recognize that the service loads that would typically be placed on this beam would be in the 30-kip range, and compare the deﬂection of the two beams in this range. Then compare the ultimate deﬂections of beams to the service load deﬂections of beams. One can see that the ratios of the ultimate deﬂections and service deﬂections are about two to three times greater in the steel-reinforced beams, even though the postpeak failure of the FRP-reinforced beam appears to have some measure of ductility. Note, however, that this data set shows the results of tests conducted in displacement control (as is usually the case in a laboratory), not in load control (as is usually the case in a real structure). 5.3

FLEXURAL STRENGTH OF AN FRP-REINFORCED SECTION

The proportioning of a member with FRP rebars1 for ﬂexural strength (or capacity) follows the ACI strength design method, a load and resistance factor

1 Only singly reinforced rectangular sections are considered in this book. Since FRP bars are not used in compression, doubly reinforced sections are not designed. Procedures for T-beams can be developed following the procedures described in what follows.

146

FRP FLEXURAL REINFORCEMENT

design (LRFD) method. In this approach the factored nominal moment resistance, Mn, of the member must be greater than the factored (ultimate) moment demand, Mu: Mn ⬎ Mu

(5.1)

According to ACI 440.1R-06, the nominal moment capacity of FRPreinforced concrete members is determined in a fashion similar to that of a steel-reinforced section. However, since FRP rebars do not yield (i.e., are linear elastic to failure), the ultimate strength of the bar replaces the yield strength of the steel rebar, ƒy, in the traditional reinforced concrete analysis procedure, which assumes equilibrium of forces and that plane sections remain plane. The design of either under- or overreinforced sections is permitted, but due to serviceability limits (deﬂections and crack widths), most glass FRP-reinforced ﬂexural members will be overreinforced. The strains, stresses, and resulting section forces in the balanced condition are shown in Fig. 5.2. The depth of the compression zone, which is equal to the distance from the extreme outer concrete surface to the neutral axis of the section, cb, is given as cb ⫽

cu d cu ⫹ ƒu

(ACI 440.1R-06: 8-6c)

and the balanced FRP reinforcement ratio (also given in Chapter 4) is ƒb ⫽ 0.851

Eƒcu ƒc⬘ ƒƒu Eƒcu ⫹ ƒƒu

(ACI 440.1R-06: 8-3)

To determine the compressive force resultant in an FRP-reinforced section, it is assumed that the Whitney rectangular stress block (Whitney, 1937) can

εcu −

cb

0.85fc⬘

fc fc⬘

β1cb

C = 0.85fc⬘β1cbb

d

Af

+

εfu

ffu

T = Af ffu

b

Figure 5.2 Strains, stresses, and section forces in the balanced condition of an FRPreinforced beam.

5.3

FLEXURAL STRENGTH OF AN FRP-REINFORCED SECTION

147

be used to represent the nonlinear stress in the concrete at the balanced condition shown in Fig. 5.2. However, it is important to recognize that the stability of the section at the balanced state in the FRP-reinforced beam is not analogous to that of a steel-reinforced beam in the balanced state. In a steelreinforced beam the balanced state is deﬁned as when the reinforcing bar yields, not when it fails, which means that the section can continue to carry loads beyond this point since the steel will not rupture, there will be some stress redistribution in the concrete, and a gradual pseudoductile failure or an excessive deﬂection will occur. In the case of an FRP-reinforced beam, when the FRP bar fails there can be no redistribution of stresses in the section and a catastrophic collapse will occur. In addition, in typical FRP-reinforced beams the neutral axis will be much higher up in the section than in a steel-reinforced beam at the balanced condition because of the large strain to failure in the FRP rebar relative to the yield strain in a steel bar. This means that the depth of the compression zone (or the distance from the extreme outer concrete surface to the neutral axis of the section), cb, can be very small in an FRP-reinforced beam. Often, the compression zone will be contained entirely above the top bars of the section and will be unconﬁned by the shear stirrups, making it more susceptible to failure as soon as the concrete compressive strain is reached at the top of the section. Note that this also implies that the top bars in the section can provide some, albeit very limited, additional tensile reinforcement to the section. 5.3.1

Overreinforced Section

When ƒ ⬎ ƒb (and c ⬎ cb), a section2 will fail due to concrete crushing, and the nominal moment capacity is given in a fashion similar to that for a section reinforced with steel rebar (where the rebar has not yet reached its yield stress). The strains, stresses, and force resultants for the overreinforced condition are shown in Fig. 5.3. The nominal moment capacity of the overreinforced section is given as

冉 冊

Mn ⫽ Aƒƒƒ d ⫺

a 2

(ACI 440.1R-06: 8-4a)

where a⫽

Aƒƒƒ 0.85ƒc⬘b

(ACI 440.1R-06: 8-4b)

and

2

The term section is used, as the procedure can be used for any rectangular beam section and is applicable to a beam and a slab.

148

FRP FLEXURAL REINFORCEMENT

εcu −

fc

0.85fc fc⬘

c >cb

β1 c

C = 0.85fc⬘β1cb

d

Af

+

εf

ff

T = Af ff

b

Figure 5.3 Strains, stresses, and force resultants in an overreinforced FRP beam section.

ƒƒ ⫽

冪

(Eƒcu)2 0.851ƒc⬘ ⫹ Eƒcu ⫺ 0.5Eƒcu 4 ƒ

(ACI 440.1R-06: 8-4d)

Here ƒƒ is the stress in the FRP rebar at concrete compressive failure, and a is the depth of the Whitney stress block in the concrete. Figure 5.4 shows an overreinforced FRP reinforced beam that has failed due to concrete crushing. 5.3.2

Underreinforced Section

When ƒ ⬍ ƒb (and c ⬍ cb), a section will fail due to rupture of the FRP rebars in tension before the concrete has reached its ultimate strain. Since the FRP reinforcement will not yield prior to rupturing, failure cannot be assumed to occur due to concrete compression failure following the rebar yielding (as in the case of a steel rebar). Consequently, the Whitney stress block cannot be assumed to exist in the concrete, and the compression force resultant and its location need to be calculated using the nonlinear stress distribution in the

Figure 5.4 FRP-reinforced beam failure due to concrete crushing (FRP 1). (Courtesy of Dushyant Arora.)

5.3

FLEXURAL STRENGTH OF AN FRP-REINFORCED SECTION

149

concrete. In addition, the depth of the neutral axis is not known in this case. The strains, stresses, and force resultants in an underreinforced section are shown in Fig. 5.5. Calculation of the nominal moment capacity of an underreinforced section therefore requires use of the nonlinear stress–strain curve of the concrete, and this necessitates a numerical solution procedure, which is not suited to design calculations. To overcome this situation, the ACI 440.1R-06 guide recommends computing the approximate (and conservative) nominal ﬂexural capacity in an underreinforced section using the approximate equation

冉

Mn ⫽ Aƒƒƒu d ⫺

1cb 2

冊

(ACI 440.1R-06: 8-6b)

where cb is the depth of the neutral axis at the balanced reinforcement ratio, given previously. Since c ⬍ cb, it follows that 1c ⬍ 1cb and that the moment arm calculated using 1cb will be less than the moment arm calculated using 1c, and therefore the term in parentheses will be greater than that for the actual condition. Numerical solution using the nonlinear stress–strain characteristics of the concrete requires the use of a nonlinear stress–strain model for the concrete.3 Two commonly used models are the Todeshini model (Todeshini et al., 1964) and the FIB model (FIB, 2001). To use these models, the nonlinear concrete stress–strain relation is converted to an equivalent rectangular stress block using two strain- and stress-dependent parameters, 1 and ␥ (see ACI 440.2R02). In the case of a balanced or overreinforced section, where the Whitney stress block applies, ␥ is 0.85 and 1 depends on concrete strength according

εc

γ fc⬘

fc

β1

c

C = γ fc⬘β1cb

d

Af

+

εfu

ffu

T = Af ffu

b

Figure 5.5 Strains, stresses, and force resultants in an underreinforced section.

3 Note that the nonlinear calculation procedure is permitted by ACI 440.1R-06; however, the equations presented in this section are not provided in ACI 440 design guides.

150

FRP FLEXURAL REINFORCEMENT

to ACI 318-05 (e.g., 0.85 for 4000-psi concrete). The height and the depth of the equivalent rectangular stress block for the nonlinear models are, 1c and ␥ƒc⬘, respectively. The stress–strain curve of Todeshini et al. (1964) is given by a single function as ƒc ⫽

2ƒ⬘c(c / ⬘c) 1 ⫹ (c / ⬘c)2

(5.2)

where ⬘c is the concrete strain at ƒc⬘. The equivalent stress block parameters for the Todeshini model are given as (MBrace, 1998) 1 ⫽ 2 ⫺

4[(c / ⬘c) ⫺ tan⫺1(c / ⬘c)] (c / ⬘c)ln[1 ⫹ (c / ⬘c)2]

(5.3)

␥⫽

0.90 ln[1 ⫹ [c / ⬘c)2] 1(c / ⬘c)

(5.4)

⬘c ⫽

1.71ƒ⬘c Ec

(5.5)

The iterative solution consists of the following steps: 1. Assume a depth of the neutral axis of c ⬍ cb (i.e., ƒ ⬍ ƒb). 2. Calculate the strain in the concrete, c (ƒ ⫽ ƒu since failure is due to FRP rupture). 3. Calculate the parameters of the equivalent stress block, 1 and ␥. 4. Calculate the actual depth of the neutral axis, c, from the equilibrium equation c⫽

Aƒƒƒu ␥ƒc⬘1b

(5.6)

5. Compare the calculated c with the assumed c and iterate until they are equal. 6. Calculate the nominal moment with the ﬁnal values of 1 and c using

冉

Mn ⫽ Aƒƒƒu d ⫺

冊

1c 2

(ACI 440.1R-06:8-6a)

This numerical solution is accomplished readily using a simple spreadsheet computer program.

5.4

5.3.3

DESIGN PROCEDURE FOR AN FRP-REINFORCED FLEXURAL MEMBER

151

Minimum Flexural Reinforcement

A minimum amount of ﬂexural reinforcement should be provided when the FRP-reinforced beam is designed to fail by FRP bar rupture to prevent failure at concrete cracking (i.e., Mn ⱖ Mcr). The amount is given as Aƒ,min ⫽

4.9兹ƒc⬘ 330 bw d ⱖ b d ƒƒu ƒƒu w

(ACI 440.1R-06:8-8)

5.4 DESIGN PROCEDURE FOR AN FRP-REINFORCED FLEXURAL MEMBER The design procedure presented in what follows is applicable to FRPreinforced beams having rectangular sections. It is applicable to any type of brittle linear-elastic FRP bar. For the sake of completeness, the procedure includes the steps for shear and serviceability design that are covered later in the book. However, the focus of this section and the design example that follows is on ﬂexural strength design. Step 1. Determine the design loads and the moment capacity required. Calculate the nominal and factored loads using ACI 318-05 load factors for the design. For a slab, calculate all loads per unit width (typically, 1 ft). Use 1.2 for dead loads and 1.6 for live loads (ASCE 7-02). For the selfweight, estimate the depth using the maximum deﬂection limits recommended by ACI 440.1R-06, shown in Table 5.1. For a beam, estimate the width as two-thirds of the beam height. Using the depths in Table 5.1 will lead to overreinforced section designs. Step 2. Assume a bar size and obtain ƒ*ƒu from the manufacturer’s speciﬁcations. Assume a stirrup diameter (if stirrups are required) and a concrete cover depth (2db is recommended) and calculate d. The bar size needs to be chosen a priori since the bar strength is a function of the bar size. The

TABLE 5.1 Minimum Thickness of FRP-Reinforced Flexural Members from ACI 440.1R-06a Support Conditions Element Type Solid one-way slabs Beams a

Simply Supported

One End Continuous

Both Ends Continuous

Cantilever

l / 13 l / 10

l / 17 l / 12

l / 22 l / 16

l / 5.5 l/4

Based on a target maximum deﬂection of l / 240.

152

FRP FLEXURAL REINFORCEMENT

procedure used to design steel-reinforced beams whereby the area of reinforcement is determined ﬁrst based on the demand cannot be used easily. Step 3. Calculate the balanced reinforcement ratio. Calculate the design strength of the FRP bar, ƒƒu, which depends on the service environment and is given by CE. Then calculate the balanced reinforcement ratio, ƒb. Step 4. Choose the numbers of bars. For an overreinforced design, select the number of bars such that ƒ ⬎ 1.0ƒb. For an underreinforced design, select ƒ ⬍ 1.0ƒb. For an overreinforced design, ƒ ⬃ 1.4 ƒb is recommended, as these beams are more likely to be yield designs that also satisfy deﬂection and crack width serviceability criteria. Check the beam width to ensure that the number of bars selected can actually ﬁt in the beam. Note that bend radii of FRP stirrups (see Chapter 7) are generally larger than those of steel stirrups. Calculate the actual reinforcement ratio ƒ ⫽ Aƒ /bd. Step 5. Calculate the nominal moment capacity of the section. For an overreinforced section, ﬁrst calculate the stress in the FRP bars at concrete failure, ƒƒ. Conﬁrm that this stress is less than the design strength of the bar. Calculate the depth of the Whitney stress block, a, and then the nominal moment capacity, Mn. For an underreinforced beam, ﬁrst calculate the depth of the neutral axis at the balanced condition, then calculate the depth of the Whitney stress block, a, and then the nominal moment capacity, Mn. For an underreinforced beam, check the minimum ﬂexural reinforcement requirements. Step 6. Calculate the ﬂexural resistance factor. Determine the ﬂexural resistance factor based on the actual FRP reinforcement ratio. Step 7. Calculate the factored moment capacity. Calculate Mn and compare with Mu. If Mn ⬍ Mu, go to step 1 and repeat the design with different section dimensions and/or bar sizes and numbers (remember to use a new value of ƒƒu if you change the bar size). If Mn ⬎ Mu, the beam design for strength capacity is completed. However, it may be unable to meet serviceability design criteria. If Mn ⬎⬎ Mu, the beam is overdesigned for ﬂexural capacity and may be able to be optimized. However, it is always advisable to check the serviceability design criteria before doing too much optimization. To meet the serviceability criteria, FRP beams are often well overdesigned (by as much as 100%) for ﬂexural capacity. Step 8. Design the beam for the serviceability limit state. Serviceability design is discussed in detail later in this chapter.4 Step 9. Check the section shear capacity and design the shear reinforcement. See Chapter 6 for shear design procedures. Step 10. Detail the cross section. Draw a sketch of the cross section to scale, showing the bars and stirrups. Plot the strain and stress proﬁles at the 4 Note that steps 8 and 9 are required in a general ﬂexural design procedure; however, they are discussed separately later in the book.

5.4

DESIGN PROCEDURE FOR AN FRP-REINFORCED FLEXURAL MEMBER

153

ultimate condition to get a physical feel for the location of the neutral axis and the compression zone depth. Design Example 5.1: Strength Design of an FRP-Reinforced Beam5 Design a simply supported interior beam for a l ⫽ 11-ft span. Design the beam for the strength limit state.6 Use ƒ⬘c ⫽ 4000-psi concrete and the fol* ⫽ lowing FRP manufacturer-guaranteed rebar properties: ƒ* ƒu ⫽ 90 ksi, ƒu 0.014, Eƒ ⫽ 6500 ksi. (Assume to begin with that the bar strength is not a function of the bar diameter.) Design the beam for the following loads: live load: 400 lb/ft. Superimposed dead load: 208 lb/ft (does not include the beam self-weight, which must be added to this to obtain the total dead load on the beam). SOLUTION Step 1. Determine the design loads and the moment capacity required. The beam depth is estimated to be 12 in. (132/10 ⯝ 13). Ideally, a beam depth larger than that suggested in Table 5.1 is actually recommended, since deﬂection limits may be greater than l/240 and the reinforcement ratio may be lower than assumed in developing the recommendations. The width is estimated to be 7 in., as this is the minimum width recommended for two No. 5 or two No. 6 main bars, assuming No. 3 stirrups and 1–12 in. of clear cover on all sides and that bend radii are used for steel bars (Wang and Salmon, 2002, p. 68). (See Chapter 7 for further discussion as to the applicability of this assumption.) This assumes that No. 3 FRP stirrups can be obtained with the same bend radii as steel bars (i.e., 2db in this case). This may not actually be the case in practice, and the designer should always check with FRP rebar suppliers as to their production capability. The unfactored (service) loads on the beam are wLL ⫽ 400 lb/ft wDL ⫽ 208 lb/ft ⫹ 150 (lb/ft3)(7/12)(12/12) ⫽ 295.5 lb/ft The factored loads according to ACI 318-05 are Wu ⫽ 1.2(87.5 ⫹ 208) ⫹ 1.6(400) ⫽ 994.67 lb/ft Mu ⫽ 5

Wul2 994.6(11)2 ⫽ ⫽ 15,043 lb-ft ⫽ 15.04 kip-ft ⫽ 180.5 kip-in. 8 8

Design of the serviceability limit states for this beam is discussed later in the chapter. This example follows the Beam Design Example given in Part 5 of ACI 440.1R-06. 7 In the example problems in this book ‘‘extra’’ signiﬁcant ﬁgures will often be used that are not typically ‘‘carried’’ in engineering calculations. This is to enable the reader to follow subsequent calculations. In actual engineering design, such numbers should be rounded. 6

154

FRP FLEXURAL REINFORCEMENT

Step 2. Assume a bar size and obtain ƒ* ƒu from the manufacturer’s speciﬁcations. Reinforcement bar sizes are also needed at this stage to estimate the effective depth, d. Assume reinforcement of two No. 6 main bars (since this is the largest bar permitted for a 7-in. beam width) and No. 3 stirrups: db ⫽ 0.75 in. and Abar ⫽ 0.44 in2. Note that the area of the bar given above is obtained from the nominal diameter of the bar and is a nominal area. The actual cross-sectional area of an FRP bar as determined by ACI 440.4R-03 test method B.1 by water displacement may be different (usually, larger) than that determined from the nominal diameter (see Table 4.1 for reported actual bar areas). Use of the nominal area is recommended for design calculations. Assume a clear cover of 1.5 in. The effective depth of the section is therefore d ⫽ h ⫺ cover ⫺ stirrup diameter ⫺ 0.5(bar diameter) ⫽ 12 ⫺ 1.5 ⫺ 0.375 ⫺ 0.5(0.75) ⫽ 9.75 in.

The guaranteed properties of the No. 6 glass FRP bar provided are given as ƒ*ƒu ⫽ 90 ksi8, ƒu * ⫽ 0.014, and Eƒ ⫽ 6500 ksi. Step 3. Calculate the balanced reinforcement ratio. The design strength of the bar is determined using the environmental conditions speciﬁed and the type of ﬁber in the FRP bar. For a glass-reinforced FRP bar designed for interior exposure, CE ⫽ 0.8 and ƒƒu ⫽ CEƒ*ƒu ⫽ 0.8(90 ksi) ⫽ 72 ksi ƒu ⫽ CE* ƒu ⫽ 0.8(0.014) ⫽ 0.011

Eƒ ⫽ 6500 ksi (no reduction in the modulus is taken from the manufacturer-guaranteed value) The ultimate compressive strain in the concrete is taken as cu ⫽ 0.003 per ACI 318-05. ƒb ⫽ 0.851

Eƒcu ƒ⬘c ƒƒu Eƒcu ⫹ ƒƒu

冉 冊冋

⫽ 0.85(0.85)

4 72

册

6500(0.003) ⫽ 0.0086 6500(0.003) ⫹ (72)

8 Note that this is a hypothetical example. In reality, the strength of the bar is a function of the bar diameter and cannot be assumed a priori. This tends to complicate the design of FRPreinforced beams.

5.4

DESIGN PROCEDURE FOR AN FRP-REINFORCED FLEXURAL MEMBER

155

Step 4. Choose the numbers of bars. To achieve a compression-controlled failure that will give a beam that will probably satisfy the deﬂection limits given in Table 5.1 and used to size the beam in this example, choose a reinforcement ratio greater than 1.0ƒb for an overreinforced beam. If 1.4ƒb is chosen, the use of the higher resistance factor ( ⫽ 0.65) is allowed. Therefore, it is advisable to choose 1.4 ƒb as a starting point for the design. reqd ⫽ 1.4ƒb ⫽ 1.4(0.0086) ⫽ 0.0120 ƒ

Areqd ⫽ ƒreqdbd ⫽ 0.0120(7)(9.75) ⫽ 0.82 in2 ƒ Aƒb ⫽ ƒbbd ⫽ 0.0086(7)(9.75) ⫽ 0.59 in2 Note that for two No. 5 bars, Aƒ ⫽ 0.62 in2 would be sufﬁcient for an overreinforced design; however, this is very close to the balanced condition and may lead to the beam not meeting serviceability criteria and perhaps not failing in the desired mode.9 Therefore, two No. 6 bars are chosen as the main tensile reinforcement: Aƒ ⫽ 0.88 in2 ƒ ⫽

0.88 ⫽ 0.0129 ⫽ 1.5ƒb 7(9.75)

Step 5. Calculate the nominal moment capacity of the section. Since the beam is overreinforced, the FRP bar will be at a stress less than its design strength, and the stress in the FRP bar at concrete compression failure is calculated as ƒƒ ⫽

冪

⫽

冪

(Eƒcu)2 0.851ƒc⬘ ⫹ Eƒcu ⫺ 0.5Eƒcu 4 ƒ (6500)2(0.003)2 0.85(0.85)(4)(6500)(0.003) ⫹ 4 0.0129

⫺ 0.5(6500)(0.003) ⫽ 57.06 ksi

The depth of the Whitney rectangular compression block is a⫽

Aƒƒƒ 0.88(57.06) ⫽ ⫽ 2.110 in. 0.85ƒc⬘b 0.85(4)(7)

The nominal moment capacity is

9

The detailed calculation for this case is given in ACI 440.1R-06, Part 5.

156

FRP FLEXURAL REINFORCEMENT

冉 冊

Mn ⫽ Aƒƒƒ d ⫺

冉

冊

a 2.110 ⫽ 0.88(57.06) 9.75 ⫺ 2 2

⫽ 436.6 kip-in. ⫽ 36.4 kip-ft

Step 6. Calculate the ﬂexural resistance factor. Since ƒ ⬎ 1.4 ƒb, ⫽ 0.65. Step 7. Calculate the factored moment capacity. Mn ⫽ 0.65(436.6) ⫽ 283.8 kip-in. ⬎ 180.5 kip-in. (Mu)

This is a safe design, but the beam appears to be overdesigned by quite a large amount (i.e., 57%). However, serviceability criteria need to be checked to see if the beam is, in fact, overdesigned. This is done in the serviceability example that follows. Discussion of Alternative Designs Results for alternative designs for this beam are now presented to compare a number of different designs for the beam. In design there is no right answer. Many good designs are possible, and the choice will often be made on the basis of nonstructural issues such as geometrical constraints, costs, and availability of FRP bars and stirrups. All other items being equal, the choice will probably be made on a cost basis. Option a: Alternative overreinforced beam design If two No. 5 bars had been chosen initially, the design procedure outlined above is used. It is assumed that the guaranteed strength does not increase for the smaller bar. The effective depth is calculated as d ⫽ 9.81 in. The nominal moment is calculated to be Mn ⫽ 385.0 kip-in. ⫽ 32.08 kip-ft. Since ƒ ⫽ 0.0090 and 1.0ƒb ⬍ ƒ ⬍ 1.4ƒb, the resistance factor is calculated as

⫽ 0.3 ⫹

ƒ 0.0090 ⫽ 0.3 ⫹ ⫽ 0.56 4ƒb 4(0.0086)

and the factored moment is Mn ⫽ 0.56(385.0) ⫽ 215.6 kip-in. ⬎ 180.5 kip-in. (Mu)

5.4

DESIGN PROCEDURE FOR AN FRP-REINFORCED FLEXURAL MEMBER

157

This is also a safe design and the beam appears to be well designed for strength (only 19% overdesigned for strength). However, this beam does not satisfy serviceability criteria (as noted in ACI440.1R-06, Part 5.) Option b: Underreinforced beam design with the same beam height Consider an underreinforced design as an alternative. Assume that the beam is designed using ﬁve No. 3 main bars (Aƒ ⫽ 0.55 in2) that are bundled in twos at the corners, stacked vertically. The two –38 -in. bundled bars are then equivalent in dimensions to one No. 6 bar, and the effective depth is d ⫽ 9.75 in., as before. The use of bundled FRP bars is not prohibited. (See provisions of ACI 318-05: Section 7.6.6.) Note that this assumes that the bar strength does not change and that the design strength for the No. 3 bars is ƒƒu ⫽ 72 ksi (ƒ* ƒu ⫽ 90 ksi)). (What happens when the guaranteed bar strength is changed to ƒ* ƒu ⫽ 110 ksi is discussed in what follows.) The actual reinforcement ratio for this conﬁguration is ƒ ⫽

0.55 ⫽ 0.0081 ⬍ 0.0086 7(9.75)

(ƒb based on ƒ* ƒu ⫽ 90 ksi)

To design the underreinforced beam, the approximate method is used. The depth of the neutral axis at the balanced condition is calculated: cb ⫽

cu 0.003 d⫽ (9.75) ⫽ 2.089 in. cu ⫹ ƒu 0.003 ⫹ 0.011

and the nominal moment is

冉

Mn ⫽ Aƒƒƒu d ⫺

冊

冋

册

1cb 0.85(2.089) ⫽ 0.55(72) 9.75 ⫺ 2 2

⫽ 350.9 kip-in. ⫽ 29.2 kip-ft

Since the beam is underreinforced, the resistance factor, ⫽ 0.55, and the factored capacity is Mn ⫽ 0.55(350.9) ⫽ 190.0 kip-in. ⬎ 180.5 kip-in. (Mu)

The underreinforced beam is also safely designed from a strength design perspective, but may not meet serviceability criteria. Option c: Underreinforced design using a deeper cross section. Consider an underreinforced beam using two No. 6 bars, but designed intentionally to be underreinforced. In this case, choose reqd ⫽ ƒb ⫽ 0.0086. Assume that d ⫽ h ⫺ 2.25 in. and that b is 7 in., as before. dreqd ⫽ Aƒ / reqd b ⫽ 0.88/ 0.0086(7) ⫽ 14.6 in. → use 14.75 in. Therefore, h ⫽ 14.75 ⫹ 2.25 ⫽ 17.0 in.

158

FRP FLEXURAL REINFORCEMENT

Recalculate the design loads: wLL ⫽ 400 lb/ft wDL ⫽ 208 lb/ft ⫹ 150 (lb/ft3)(7/12)(17/12) ⫽ 332 lb/ft Factor the load according to ACI 318-05: Wu ⫽ 1.2(332) ⫹ 1.6(400) ⫽ 1038.4 lb/ft Mu ⫽

Wu l2 1038.4(11)2 ⫽ ⫽ 15,706 lb-ft ⫽ 15.71 kip-ft ⫽ 188.5 kip-in. 8 8

Determine the depth of the neutral axis in the balanced condition: cb ⫽

cu 0.003 d⫽ (14.75) ⫽ 3.161 in. cu ⫹ ƒu 0.003 ⫹ 0.011

The nominal moment capacity is

冉

Mn ⫽ Aƒƒƒu d ⫺

冊

冋

册

1cb 0.85(3.161) ⫽ 0.88(72) 14.75 ⫺ 2 2

⫽ 849.4 kip-in. ⫽ 70.8 kip-ft

The factored capacity is Mn ⫽ 0.55(849.4) ⫽ 467.2 kip-in. ⬎ 188.5 kip-in. (Mu)

Therefore, the design is safe, but the beam appears to be signiﬁcantly overdesigned. As noted in the overreinforced case, the beam must still be checked for serviceability criteria. However, in this case the underreinforced beam will usually not have difﬁculty meeting the serviceability criteria, due to its large cross section. Therefore, the beam design may be optimized by choosing less reinforcement (e.g., two No. 5 bars) and decreasing the beam height. For this underreinforced beam, check the minimum ﬂexural reinforcement: Aƒ ⫽ 0.88 in2 Aƒ,min ⫽ but not less than

4.9兹ƒc⬘ 4.9兹4000 bwd ⫽ (7)(14.75) ⫽ 0.44 in2 ƒƒu 72,000

5.4

DESIGN PROCEDURE FOR AN FRP-REINFORCED FLEXURAL MEMBER

159

330 330 b d⫽ (7)(14.75) ⫽ 0.47 in2 ƒƒu w 72,000 Therefore, the second condition controls, and Aƒ must be greater than 0.47 in2. Since Aƒ ⫽ 0.88 in2, the minimum ﬂexural reinforcement has been provided for the underreinforced beam, and catastrophic, brittle failure at the cracking moment cannot occur. Option d: Effect of higher bar strength for smaller bars Reconsider the beam designed in option b, with ﬁve No. 3 bars in a 7 ⫻ 12 in. cross section. Now assume that the guaranteed strength of the No. 3 bar is ƒ*ƒu ⫽ 110 ksi, and determine the capacity of the beam. The design strength of the bar is ƒƒu ⫽ 0.8(110) ⫽ 88 ksi, and the balanced reinforcement ratio must be recalculated: ƒb ⫽ 0.851

Eƒcu ƒ⬘c ƒƒu Eƒcu ⫹ ƒƒu

冉 冊冋

⫽ 0.85(0.85)

4 88

册

6500(0.003) ⫽ 0.0060 6500(0.003) ⫹ (88)

Notice that this is signiﬁcantly less than the ratio of 0.0086 obtained previously with ƒƒu ⫽ 72 ksi. Now the beam with ﬁve No. 3 bars (ƒ ⫽ 0.0081) is actually overreinforced, and an overreinforced calculation needs to be made. Following the procedure above yields ƒƒ ⫽

冪

⫽

冪

(Eƒcu)2 0.851ƒc⬘ ⫹ Eƒcu ⫺ 0.5Eƒcu 4 ƒ (6500)2(0.003)2 0.85(0.85)(4)(6500)(0.003) ⫹ 4 0.0081

⫺ 0.5(6500)(0.003) ⫽ 74.23 ksi

a⫽

Aƒƒƒ 0.55(74.23) ⫽ ⫽ 1.715 in. 0.85ƒc⬘b 0.85(4)(7)

冉 冊

Mn ⫽ Aƒƒƒ d ⫺

冉

冊

a 1.715 ⫽ 0.55(74.23) 9.75 ⫺ ⫽ 363.0 kip-in. 2 2

⫽ 30.25 kip-ft

⫽ 0.3 ⫹

ƒ 0.0081 ⫽ 0.3 ⫹ ⫽ 0.64 4ƒb 4(0.0086)

Mn ⫽ 0.64(363.0) ⫽ 231.4 kip-in. ⬎ 180.5 kip-in. (Mu)

160

FRP FLEXURAL REINFORCEMENT

A summary of the design alternatives is presented in Table 5.2 for comparison purposes. It can be seen that all of the beams have sufﬁcient strength to carry the design loads. The choice of which beam to use is made based on serviceability criteria described in what follows. 5.4.1

Design of FRP-Reinforced Bridge Deck Slabs

The use of FRP rebars in highway bridge decks is viewed as a promising method to increase the durability of highway bridges. A number of projects have been completed in North America in recent years in which FRP rebars have been used in place of epoxy-coated steel bars to reinforce bridge decks (Benmokrane et al., 2004). Other bridges have used combinations of bottom mat steel and top mat FRP bars (Bradberry and Wallace, 2003) or FRP grids (Steffen et al., 2003; Bank et al., 2006). Combinations of FRP bars, FRP grids, and FRP stay-in-place forms have also been used in full-scale highway bridge projects in recent years (Berg et al., 2006). Bridge Deck Design Procedure In what follows a design procedure for FRP-reinforced bridge decks spanning transverse to the trafﬁc direction that is compatible with ACI 440-1R.06 and the AASHTO Standard Speciﬁcation for Highway Bridges10 (AASHTO, 2002) is discussed. The loads, load factors, and other reinforcement requirements follow the AASHTO load factor design (LFD) method, and the resistance factors are taken from ACI 440.1R-06 in this design procedure. In the AASHTO LFD procedure the bridge is designed for a dead load factor of DL ⫽ 1.3 and a live load factor of LL ⫽ 1.3(1.67) ⫽ 2.17. In addition, the nominal live load is subject to an impact factor that is given as

TABLE 5.2

Summary of FRP-Reinforced Beam Design Alternatives a

Beam

Bars

Original Option a Option b Option c Option d

Two Two Five Two Five

No. No. No. No. No.

ƒ* ƒu (ksi) 6 5 3 6 3

90 90 90 90 110

Dimensions, b ⫻ h (in.)

Over- or Underreinforced

Mn (kip-in.)

Mn (kip-in.)

⫻ ⫻ ⫻ ⫻ ⫻

Over Over Under Under Over

436.6 385.0 350.9 834.5 363.0

283.8 215.6 193.0 458.9 231.4

7 7 7 7 7

12 12 12 17 12

The moment demand for these designs: Mu ⫽ 180.5 kip-in (except Option C: Mu ⫽ 188.5 kipin).

a

10

Alternatively, the loads could be taken from the AASHTO LRFD Bridge Design Speciﬁcations (2005).

5.4

DESIGN PROCEDURE FOR AN FRP-REINFORCED FLEXURAL MEMBER

I⫽

50 L ⫹ 125

161

(5.7)

where L is the span length in feet and I is the impact factor, which has a maximum of 30%. For bridge decks that span transversely between longitudinal girders, this implies that the nominal live load is multiplied by 1.3 prior to application of the load factors. The live load moment in units of ft-lb per foot width of the slab (ft-lb/ft) is given by AASHTO for HS20 loading as S⫹2 P20 32

(5.8)

where S is the clear span length in feet perpendicular to the trafﬁc (i.e., between the girders). If the slab is continuous over three or more supports (i.e., girders), the live load moment can be taken as 80% of the above (called a continuity factor). The concentrated wheel load for HS20 loading, P20 ⫽ 16,000 lb. The main slab top and bottom reinforcement transverse to the trafﬁc direction is designed using the dead load of the slab, any additional dead load due to a possible future wearing surface (usually taken as 20 lb/ft2), and the live load given above. Reinforcement in the longitudinal trafﬁc direction in the slab, called distribution reinforcement, is given as a percentage of the required main reinforcement: percentage ⫽

220 兹S

maximum 67%

(5.9)

This amount of distribution reinforcement must be placed in the middle half of the slab (i.e., in the positive moment region for the transverse reinforcement). Not less than 50% of this amount can be used in outer quarters of the slab (i.e., nearer the girders in the negative moment region for the main transverse reinforcement). The distribution reinforcement is usually distributed equally across the width of the slab and tied below the top main bars and above the bottom main bars. When designing a steel rebar deck, the designer is not required to check for shear or bond, as these are assumed to be adequate for steel reinforcing bars designed for the dead and live loads stipulated. Neither is there a requirement to check for deﬂections or crack widths. In the case of FRP bars, these assumptions are not appropriate. Even if AASHTO loads and load factor procedures are used, the FRP deck must be checked for shear and deﬂections (and even bond). ACI 440.1R-06 provisions should be followed to determine

162

FRP FLEXURAL REINFORCEMENT

shear strength (transverse shear and punching shear) and serviceability criteria (deﬂection, crack width, and creep rupture stress). For the punching shear design, the tire footprint (AASHTO, 2002) is taken as a rectangle with an area 0.01P in2. The ratio of the width to the length of the rectangle is taken as 2.5 (i.e., the footprint is wider in the direction perpendicular to the girders than in the direction parallel to the girders). Bridge Parapet Design The bridge parapet, or more precisely the bridge guardrail, is an integral part of a reinforced concrete bridge deck slab. At this time a FRP-rebar-reinforced standard parapet design has not been crash tested and approved by the U.S. Federal Highway Administration according to NCHRP 350 crash test procedures. However, a reinforced concrete parapet with FRP reinforcing bars has been tested in recent years using pendulum impact and static test methods (El-Salakawy et al., 2003; Dietz et al., 2004). A FRP-reinforced guardrail has been used on an FRP-reinforced deck constructed in Canada. In many projects where FRP deck reinforcing has been used, conventional epoxy-coated steel reinforcing has been used for the parapet. Design Example 5.2: FRP-Reinforced Bridge Deck Slab Design a bridge deck reinforced with GFRP rebars for a simply supported two-lane highway bridge 100 ft long by 42 ft wide. The bridge is to be designed for AASHTO HS20-44 loading according to the AASHTO Standard Speciﬁcation for Highway Bridges (AASHTO, 2002). The bridge superstructure consists of prestressed concrete I-girders with rigid ﬂanges that act compositely with the deck slab and are spaced at 7 ft on-center. The width of the top ﬂange of the prestressed girder is 18 in. Assume that there is no overhang and that conventional steel-reinforced parapets will be used. The bridge deck is designed of concrete with ƒ⬘c ⫽ 4000 psi and has a minimum depth of 8 in. An instantaneous deﬂection limit of L/1200 ⫽ 0.08 inches is prescribed and maximum crack widths per ACI 440.1R-06 for exterior harsh exposure. A clear cover of 0.75 in. is used per ACI 318-05 recommendations for slabs. SOLUTION Step 1. Determine the design loads and the moment capacity required. For dead load calculations use 150 lb/ft3 for concrete and a future wearing surface of 20 lb/ft2. For live loads use the AASHTO formula plus 30% impact. The deck span is calculated from the face of the girder when rigid girders are used. The dead and live load moments are calculated per foot width of the deck. S ⫽ 7(12) ⫺ 2(9) ⫽ 66 in. ⫽ 5.5 ft

5.4

DESIGN PROCEDURE FOR AN FRP-REINFORCED FLEXURAL MEMBER

163

wDL ⫽ (150 lb/ft3)(8/12) ⫹ 20 lb/ft2 ⫽ 120 lb/ft mDL ⫽

wDLS2 120(5.5)2 ⫽ ⫽ 454 lb-ft/ft ⫽ 0.45 kip-ft/ft 8 8

mLL⫹I ⫽

5.5 ⫹ 2 S⫹2 P20(1.3) ⫽ 16(1.3) ⫽ 4.88 kip-ft/ft 32 32

Factored moments for simple spans: Mu ⫽ 1.3(0.45) ⫹ 2.17(4.88) ⫽ 11.22 kip-ft/ft Multiplying by 0.8 for continuity gives the design demand: Mu ⫽ 0.8(11.22) ⫽ 8.98 kip-ft/ft Step 2. Assume a bar size and obtain ƒ* ƒu from the manufacturer’s speciﬁcations. A glass FRP No. 5 bar with ƒ*ƒu ⫽ 95 ksi and Eƒ ⫽ 5920 ksi is selected for a trial design. A bottom clear cover of 0.75 in. is used. For top bars (for a negative moment capacity over the girders) the top cover is usually taken as 2.5 in. for steel bars. For FRP bars this may be excessive. 2db is suggested for constructability reasons. Calculate the effective depth for the bottom bars for positive moment capacity. d ⫽ h ⫺ cover ⫺ 0.5(bar diameter) ⫽ 8 ⫺ 0.75 ⫺ 0.5(0.625) ⫽ 6.94 in.

Step 3. Calculate the balanced reinforcement ratio. For a glass FRP bar designed for exterior exposure, CE ⫽ 0.7 and ƒƒu ⫽ CEƒ* ƒu ⫽ 0.7(95 ksi) ⫽ 66.5 ksi ƒb ⫽ 0.851

Eƒcu ƒ⬘c ƒƒu Eƒcu ⫹ ƒƒu

冉 冊冋

⫽ 0.85(0.85)

4 66.5

册

5920(0.003) ⫽ 0.0092 5920(0.003) ⫹ (66.5)

Step 4. Choose the numbers of bars. 1.4 ƒb ⫽ 1.4(0.0092) ⫽ 0.0129

164

FRP FLEXURAL REINFORCEMENT

Choose three No. 5 bars with Aƒ ⫽ 0.93 in2 and ƒ ⫽ 0.0112 (slightly less than 1.4 ƒb). Step 5. Calculate the nominal moment capacity of the section. The stress in the FRP bars at ﬂexural failure is ƒƒ ⫽

冪

⫽

冪

(Eƒcu)2 0.851ƒc⬘ ⫹ Eƒcu ⫺ 0.5Eƒcu 4 ƒ (5920)2(0.003)2 0.85(0.85)(4)(5920)(0.003) ⫹ 4 0.0122

⫺ 0.5(5920)(0.003) ⫽ 59.4 ksi

The depth of the Whitney rectangular compression block is a⫽

Aƒƒƒ 0.93(59.4) ⫽ ⫽ 1.35 in. 0.85ƒc⬘b 0.85(4)(12)

The nominal moment capacity is

冉 冊

Mn ⫽ Aƒƒƒ d ⫺

冉

冊

a 1.35 ⫽ 0.93(59.4) 6.94 ⫺ ⫽ 346.09 kip-in./ft 2 2

⫽ 28.8 kip-ft/ft

Step 6. Calculate the ﬂexural resistance factor. ⫽ 0.3 ⫹

ƒ 0.00112 ⫽ 0.3 ⫹ ⫽ 0.60 4ƒb 4(0.0092)

Step 7. Calculate the factored moment capacity. Mn ⫽ 0.60(28.2) ⫽ 17.3 kip-ft/ft ⬎ 8.98 kip-ft/ft

With the chosen reinforcement, the slab can easily meet the positive moment ﬂexural demand. However, the slab needs to be checked for shear before ﬁnalizing the design. The required distribution reinforcement is 67% of the main reinforcement. Choose two No. 5 bars. Since the slab is overdesigned in ﬂexure, it could be argued that too much distribution reinforcement is being provided in the FRP slab. However, it is common practice to have reasonably balanced bidirectional reinforcement in bridge deck slabs, where punching shear under the wheel loads is typically the failure mode observed.

5.4

DESIGN PROCEDURE FOR AN FRP-REINFORCED FLEXURAL MEMBER

165

The slab reinforcement proposed at this stage of the design for ﬂexural capacity is three No. 5 (No. 5 at 4 in.) GFRP bars in the transverse direction at the top and bottom of the slab and a distribution reinforcement of two No. 5 (No. 5 at 6 in.) GFRP bars in the longitudinal direction. Note that the effective depth for the top bars may be less than the design depth assumed for the bottom bars, depending on the clear cover used for the top bars. A thicker clear cover is generally used for top bars in bridge decks reinforced with steel bars; however, it is not known if such a conservative approach is needed for FRP-reinforced decks. A clear top cover of 1.0 in. has been used on two FRP-reinforced decks built in Wisconsin (Berg et al., 2006; Bank et al., 2006). This design can be compared with the published data for the FRPreinforced bridge deck on the Morristown Bridge in Morristown, Vermont, constructed in 2002 (Benmokrane et al., 2004). A 9-in.-thick deck with top and bottom clear covers of 2.5 and 1.5 in., respectively (typical steel clear covers) were used. Girder spacing was 7 ft on center. The design was based on a maximum ﬂexural crack width of 0.020 in. and called for No. 5 at 4 in. bottom main bars, No. 6 at 4 in. top main bars, and No. 5 at 6 in. distribution bars (top and bottom). For constructability reasons, the actual reinforcement used in the bridge was No. 6 at 4 in. main bars (top and bottom) and No. 6 at 6 in. distribution bars. A photograph of the FRP bars in place prior to concrete placement is shown in Fig. 5.6.

Figure 5.6 Glass FRP bars on the Morristown, Vermont, bridge in 2002. (Courtesy of Brahim Benmokrane.)

166

FRP FLEXURAL REINFORCEMENT

The punching shear design for the slab is considered in Chapter 6. The transverse shear capacity is often assumed to be satisfactory if the punching shear capacity is satisfactory. Deﬂection, crack width, and creep rupture checks must still be performed. However, since the slab is overreinforced and the AASHTO load factors are signiﬁcantly larger than the ASCE 7 (i.e., ACI 318-05) load factors, the serviceability design should be sufﬁcient. However, this must be veriﬁed with calculations in an engineering design, since the deﬂection limits imposed for bridges are more severe than in building-related applications. 5.5

SERVICEABILITY DESIGN OF FRP-REINFORCED BEAMS

For the serviceability limit state, both deﬂections and crack widths must be checked according to procedures detailed in ACI 440.1R-06. The designer is also required to check stresses under sustained service loads against creep rupture stress limits and fatigue stress limits. The strain and stress distributions and resultant forces in the cracked section at service loads are shown in Fig. 5.7. 5.5.1

Deﬂections Under Service Loads

Due to the lower modulus of glass FRP rebars relative to steel rebars, deﬂections in FRP-reinforced beams for equivalent reinforcement ratios to steelreinforced beams will be much larger. Deﬂections should be determined under service loads for both immediate (i.e., short-term) and long-term sustained loads and compared with building code–permitted deﬂections. Similar to the case of steel-reinforced concrete members, an ‘‘effective’’ second moment of area based on the gross, Ig, and cracked, Icr, cross section second moments is used to calculate deﬂections of an FRP-reinforced beam. A modiﬁed form of the Branson equation is used for FRP-reinforced beams to determine the efεc

fc

− c = kd

2c/ 3

C = 0.5fccb

d

Af

+

εf

ff

T = Af ffu

b

Figure 5.7 Strains, stress, and force resultants at service loads.

5.5

SERVICEABILITY DESIGN OF FRP-REINFORCED BEAMS

167

fective second moment of the section as a function of maximum applied service load moment, Ma, as follows: Ie ⫽

冉 冊 Mcr Ma

冋 冉 冊册

3

3

Mcr Ma

dIg ⫹ 1 ⫺

Icr ⱕ Ig

(ACI 440.1R-06:8-13a)

where Mcr is the moment at cracking and d is a reduction coefﬁcient for FRP-reinforced beams and is given as d ⫽

冉 冊

1 ƒ ⱕ 1.0 5 ƒb

(ACI 440.1R-06:8-13b)

As in conventional steel-reinforced concrete, the cracked (transformed) second moment of area is given as Icr ⫽

bd3 3 k ⫹ ƒ Aƒ d 2(1 ⫺ k)2 3

(ACI 440.1R-06:8-11)

where k ⫽ c/d is the ratio of the depth of the neutral axis to the effective depth of the section under service loads and ƒ is the modular ratio for the FRP reinforcement, k ⫽ 兹(ƒƒ)2 ⫹ 2ƒƒ ⫺ ƒƒ ƒ ⫽

Eƒ Ec

(ACI 440.1R-06:8-12) (5.10)

The gross second moment of area is taken as Ig ⫽

bh3 12

(5.11)

Alternatively, the properties of the cracked section under service loads can be calculated directly using the bimodular (composite beam) material formula (Gere and Timoshenko, 1997). The location of the neutral axis shown in Fig. 5.8, is given, by deﬁnition, by the equation E1

冕 y dA ⫹ E 冕 y dA ⫽ 0 1

1

2

2

2

(5.12)

Substituting E1 ⫽ Ec, E2 ⫽ Eƒ, and y ⫽ c ⫽ the distance from the neutral axis to the top of the section, integrating, and rearranging gives the quadratic equation for c as

168

FRP FLEXURAL REINFORCEMENT

E1

y

c Neutral axis

d

E2

Figure 5.8 Cracked section dimensions and notation.

Ecb

c2 ⫹ Eƒ Aƒ(c ⫺ d) ⫽ 0 2

(5.13)

The ﬂexural stiffness (EI) of the composite section is given as

冘 EI ⫽ E I ⫹ E I 1 1

(5.14)

2 2

and the cracked (transformed) second moment of area as

Icr ⫽

冘 EI Ec

(5.15)

The long-term deﬂection in an FRP-reinforced beam that includes the effects of creep and shrinkage of the concrete under sustained long-term service loads (i.e., the dead load and sustained live load) is calculated in a fashion similar to that of a steel rebar–reinforced beam and is given as ⌬cp⫹sh ⫽ 0.6(⌬i)sus

(ACI 440.1R-06:8-14)

For FRP reinforcements where no compression reinforcement is used, ⫽ . is the conventional ACI multiplier for additional deﬂection due to longterm effects in reinforced concrete members, and is the time-dependent factor for sustained loads. ⫽ 2.0 for sustained loads with a duration of ﬁve years as per ACI 318-05. The 0.6 coefﬁcient is added for an FRP-reinforced

5.5

SERVICEABILITY DESIGN OF FRP-REINFORCED BEAMS

169

beam to account for larger initial deﬂection in an FRP-reinforced beam and for the compressive creep of the concrete. 5.5.2

Flexural Cracking

The width of ﬂexural cracks in beams reinforced with FRP rebars is limited by ACI 440.1R-06. The crack width for FRP-reinforced members may be calculated from w⫽2

冪

冉冊

ƒƒ s kb d c2 ⫹ Eƒ 2

2

(ACI 440.1R-06:8-9)

where w is the maximum crack width in inches, ƒƒ the service load stress in the FRP reinforcement in ksi, Eƒ the modulus of the FRP rebars in ksi,  the ratio of the distance between the neutral axis and the bottom of the section (i.e., the tension surface) and the distance between the neutral axis and the centroid of reinforcement (as shown in Fig. 5.9), dc the thickness of the concrete cover from the tension face to the center of the closest bar, s the centerto-center bar spacing of the main FRP bars, and kb a bond-related coefﬁcient (Frosch, 1999).  is calculated from ⫽

h2 h ⫺ kd ⫽ h1 d(1 ⫺ k)

(5.16)

where the distances h1 and h2 are as shown in Fig. 5.9, The stress in the FRP at service loads can be calculated from ƒƒ,s ⫽

mDL⫹LL ƒ d(1 ⫺ k) Icr

(5.17)

or

c d h2

h1 dc

Figure 5.9 Cross-sectional dimensions used to calculate .

170

FRP FLEXURAL REINFORCEMENT

ƒƒ,s ⫽

mDL⫹LL Eƒ(d ⫺ c) EI

冘

(5.18)

ACI 440.1R-06 recommends that the bond-related coefﬁcient is taken as kb ⫽ 1.4 for commercially produced FRP rebars. Lower values of kb can be used if experimental data are available to support such a value. For steel bars, kb ⫽ 1.0, which implies that FRP bars have a different bond behavior than that of steel bars. 5.5.3

Creep and Fatigue at Service Loads

FRP-reinforced concrete beams must be checked for possible failure due to creep rupture or fatigue under service loads. Creep rupture is checked with respect to all sustained service loads, and fatigue is checked with respect to all sustained loads plus the maximum loading induced in a fatigue loading cycle. ƒƒ,creep rupture ⫽

msusƒ d(1 ⫺ k) Icr

(5.19)

ƒƒ,creep rupture ⫽

msus Aƒ d(1 ⫺ k/3)

(5.20)

or

The stress limits for creep rupture and fatigue given by ACI 440.1R-06 are 0.2ƒƒu, 0.3ƒƒu, and 0.55ƒƒu for glass, aramid, and carbon FRP bars, respectively.

5.6

DESIGN PROCEDURE FOR SERVICEABILITY

The design for serviceability is usually performed after the strength design for reinforced concrete members. The design typically involves checking to see that the section and reinforcement selected can meet the code-mandated serviceability requirements. Serviceability design in the LRFD approach is performed by setting all the load factors to 1.0 and all the resistance factors to 1.0. Therefore, the loads are the nominal service loads, and the calculated effects (deﬂections and stresses) are the actual effects (i.e., they are not modiﬁed by any factors). The approach is therefore the same approach as that used to calculate deﬂections and service-level stresses in the old working stress design (WSD) method (the equivalent of the allowable stress design method). A similar approach is used for FRP-reinforced sections. The procedure for the serviceability check is as follows:

5.6

DESIGN PROCEDURE FOR SERVICEABILITY

171

Step 1. Determine the service loads and moments. The service moments due to dead loads, live load, and the sustained dead and live loads are calculated. Step 2. Calculate the properties of the uncracked and cracked transformed section. The cracked section properties can be calculated by the transformed section method or the composite mechanics method. Note, however, that the properties of the cracked section with the reinforcement transformed to the equivalent properties of the concrete are used in calculating the FRP-reinforced beam deﬂection using the modiﬁed Branson equation. Step 3. Calculate the immediate (short-term) and long-term deﬂection of the section. Using the modiﬁed Branson equation, calculate the immediate deﬂection due to the full dead and live loads. Then calculate the long-term deﬂection due to creep and shrinkage under the sustained loads only. Compare the calculated deﬂections with the code-permitted short- and longterm deﬂections. Step 4. Calculate the width of the cracks due to the ﬂexural load. The ﬂexural crack width is determined and the value is compared with the ACI 440.1R06 code-permitted maximum crack widths for either interior or exterior exposures given in Table 4.3. Step 5. Calculate the axial stress in the FRP bars under long-term sustained service and fatigue loads. The stresses in the FRP bars under sustained loads are compared with the ACI 440.1R-06-permitted maxima to prevent failure due to creep rupture or fatigue. Step 6. Modify the design if the serviceability limits are exceeded. If any of the three serviceability limits are exceeded, the section must be redesigned. Since the redesign may require changing the size of the FRP rebars, the strength design needs to be rechecked with the new section and bar properties. Design Example 5.3: Serviceability Design for an FRP-Reinforced Beam Check the serviceability of the 12 ⫻ 7 in. overreinforced beam in Design Example 5.2. The geometric and material properties of the section are: simply supported beam, 11-ft span; 4000-psi concrete; FRP bar design strength, ƒƒu ⫽ 72 ksi; two No. 6 main bars; Aƒ ⫽ 0.88 in2; d ⫽ 9.75 in.; wLL ⫽ 400 lb/ ft; wDL ⫽ 295.5 lb/ft (includes beam self-weight). Additionally, it is given that 20% of the live load is sustained and that the maximum permitted deﬂection under long-term sustained loads is L/240. The maximum crack width permitted for interior exposure is 0.028 in. (often referred to as 28 mils11). The maximum allowable stress in the glass FRP bars under sustained load is 0.2ƒƒu ⫽ 0.2(72) ⫽ 14.4 ksi.

11

1 mil ⫽ 1 / 1000 in.

172

FRP FLEXURAL REINFORCEMENT

SOLUTION Step 1. Determine the service loads and moments. mDL ⫽

wDLl 2 (87.5 ⫹ 208) (11)2 ⫽ ⫽ 4469.4 lb-ft ⫽ 53.6 kip-in. 8 8

mLL ⫽

wLLl 2 400(11)2 ⫽ ⫽ 6050 lb-ft ⫽ 72.6 kip-in. 8 8

mDL⫹LL ⫽ mS ⫽ 126.2 kip-in. Step 2. Determine the modular ratio and section (cracked and gross) properties. Modular ratio: ƒ ⫽

Eƒ 6,500,000 ⫽ ⫽ 1.8 Ec 57,000兹4000

Neutral-axis depth ratio, k ⫽ c/d: k ⫽ 兹(ƒƒ)2 ⫹ 2ƒƒ ⫺ ƒƒ ⫽ 兹[0.0129(1.8)]2 ⫹ 2(0.0129)(1.8) ⫺ 0.0129(1.8) ⫽ 0.194

Cracked transformed second moment of area: Icr ⫽ ⫽

bd 3 3 k ⫹ ƒ Aƒ d 2(1 ⫺ k)2 3 7(9.75)3 (0.194)3 ⫹ 1.8(0.88)(9.75)2(1 ⫺ 0.194)2 ⫽ 114 in4. 3

Gross second moment of area: Ig ⫽

bh3 7(12)3 ⫽ ⫽ 1008 in4 12 12

Alternatively, calculate directly using the bimodular (composite beam) material formula (see Fig. 5.8). Use the equation

5.6

E1

DESIGN PROCEDURE FOR SERVICEABILITY

173

冕 y dA ⫹ E 冕 y dA ⫽ 0 1

1

2

2

2

with E1 ⫽ Ec ⫽ 57,000兹4000 ⫽ 3605 ksi E2 ⫽ Eƒ ⫽ 6500 ksi y ⫽ c (distance from the neutral axis to the top of the section) 3605(7)c

c ⫹ 6500[⫺(9.75 ⫺ c)](0.88) ⫽ 0 2

12,617.5c 2 ⫹ 5720c ⫺ 55,770 ⫽ 0 Solving the quadratic equation and taking the positive root yields c ⫽ 1.888 in.

or k ⫽

c 1.888 ⫽ ⫽ 0.194 in. d 9.75

The ﬂexural stiffness (EI) of the composite section is given as

冘 EI ⫽ E I ⫹ E I 1 1

冋

3,605,000

2 2

册

7(1.888)3 ⫹ 6,500,000(0.88)(9.75 ⫺ 1.888)2 3

⫽ 4.102 ⫻ 108 lb-in2

and Icr ⫽

冘 EI ⫽ 4.102 ⫻ 10 ⫽ 113.8 in ⬇ 114 in 8

4

Ec

4

3,605,000

Note that this is the same answer as obtained before using the transformed section method and ACI equations. The tensile strength of the concrete ƒr ⫽ 7.5兹ƒc⬘ ⫽ 7.5兹4000 ⫽ 474.3 psi Calculate the cracking moment:

174

FRP FLEXURAL REINFORCEMENT

Mcr ⫽

2ƒr Ig 2(474.3)(1008) ⫽ ⫽ 79,689 lb-in. h 12

⫽ 79.7 kip-in. ⬍ 126.2 kip-in. (mS)

The check that the cracking moment is smaller than the total service load moment is an important check for FRP-reinforced beams. This means that the beam is cracked under service loads. If this is not the case, the beam is uncracked under service loads, and the full gross second moment, Ig, is used in all the serviceability calculations (i.e., deﬂection, crack widths, and sustained stresses). Step 3. Calculate the immediate (short-term) and long-term deﬂection of the section. Calculate the effective second moment of area (modiﬁed Branson formula). First, calculate the FRP reduction coefﬁcient. d ⫽

Ie ⫽

冉 冊 冉 冊 冉 冊 冋 冉 冊册 冉 冊 冋 冉 冊册 1 ƒ 1 0.0129 ⫽ ⫽ 0.30 ⱕ 1.0 5 ƒb 5 0.0086 Mcr MDL⫹LL

79.7 Ie ⫽ 126.2

3

3

dIg ⫹ 1 ⫺

Mcr MDL⫹LL

3

Icr ⱕ Ig

79.7 (0.30)(1008) ⫹ 1 ⫺ 126.2

3

(114) ⫽ 160.8 in4

The immediate deﬂection under the total (uniformly distributed) service load is ⌬i ⫽

冉 冊

5(wDL ⫹ wLL)l4 5(295.5 ⫹ 400)(11)4 (12)3 ⫽ ⫽ 0.395 in. 384EcIe 384(3605)(160.8) (1000)

The long-term sustained load (i.e., the cause of the creep deﬂection) is wsus ⫽ wLL(sus) ⫹ wDL ⫽ 0.2(400) ⫹ (208 ⫹ 87.5) ⫽ 375.5 lb/ft (⌬i)sus ⫽ ⌬i

冉 冊

wsus 375.5 ⫽ 0.395 ⫽ 0.213 in. wDL ⫹ wLL 695.5

The deﬂection due to the long-term sustained loads is ⌬(cp⫹sh) ⫽ 0.6(⌬i)sus ⫽ 0.6(2)(0.213) ⫽ 0.256 in.

5.6

DESIGN PROCEDURE FOR SERVICEABILITY

175

The total deﬂection at a time in the future (greater than ﬁve years) is the sum of the instantaneous deﬂection due to the live load only plus the long-term deﬂection due to the sustained loads: ⌬i(LL) ⫽ ⌬i ⌬long

term

冉 冊

wLL 400 ⫽ 0.395 ⫽ 0.227 in. wDL ⫹ wLL 695.5

⫽ ⌬i(LL) ⫹ ⌬cp⫹sh ⫽ 0.227 ⫹ 0.256 ⫽ 0.483 in. ⬍ 0.55 in. (⌬allowable ⫽ L/240)

The beam therefore meets the long-term deﬂection limit. However, it is somewhat overdesigned for deﬂection limits (as it was for strength). Step 4. Calculate the width of the cracks due to the ﬂexural load. To calculate the width of the ﬂexural cracks, the center-to-center spacing of the main bars is needed. For two No. 6 bars, this is s ⫽ 2.5 in. (see Chapter 7 for details). The bond-related coefﬁcient, kb ⫽ 1.4, as recommended by ACI 440.1R-06 since no additional data are provided to reduce this number. The stress in the bars at service and the  ratio are, as follows: Using the transformed crack second moment yields ƒƒ ⫽

mDL⫹LL ƒ d(1 ⫺ k) 126.1(1.8)(9.75)(1 ⫺ 0.194) ⫽ ⫽ 15.7 ksi Icr 114

or using the composite ﬂexural stiffness gives us ƒƒ ⫽

mDL⫹LLEƒ (d ⫺ c) 126.1(6500)(9.75 ⫺ 1.89) ⫽ ⫽ 15.7 ksi 4.102 ⫻ 105 EI

⫽

h2 h ⫺ kd 12 ⫺ 0.194(9.75) ⫽ ⫽ ⫽ 1.286 h1 d(1 ⫺ k) 9.75(1 ⫺ 0.194)

冘

Substituting in the expression for the ﬂexural crack width gives

冪

冉冊

ƒƒ s w⫽2 k d 2 ⫹ Eƒ b c 2

冉 冊

⫽2

2

冪

冉 冊

15.7 2.5 (1.286)(1.4) (2.25)2 ⫹ 6500 2

⫽ 0.024 in. ⬍ 0.028 in. (wallowable)

Therefore, the beam meets crack width requirements.

2

176

FRP FLEXURAL REINFORCEMENT

TABLE 5.3 No. 6 Bars

Summary of Flexural Design for a 7 ⴛ 12 Section with Two

Criterion Flexural strength Maximum long-term deﬂection Crack width Creep rupture stress

Designed

Required (or Permitted)

Overdesign Factor

283.8 kip-in. 0.483 in. 0.024 in. 8.46 ksi

180.5 kip-in. 0.550 in. 0.028 in. 14.4 ksi

1.57 1.14 1.17 1.70

Step 5. Calculate the axial stress in the FRP bars under long-term sustained service and fatigue loads. msus ⫽ ƒƒ ⫽

375.5(11)2 ⫽ 5679 lb-ft ⫽ 5.68 kip-ft ⫽ 68.16 kip-in. 8 msus ƒ d(1 ⫺ k) 68.16(1.8)(9.75)(1 ⫺ 0.194) ⫽ Icr 114

⫽ 8.46 ksi ⬍ 14.4 ksi (0.2 ƒƒu)

Therefore, long-term creep rupture of the FRP bars is not a concern. The ﬂexural design of a 7 ⫻ 12 in. beam with two No. 6 main bars is summarized in Table 5.3. It can be seen that the beam is optimized from a serviceability perspective but is quite overdesigned with regard to ﬂexural strength and creep rupture stress. This will generally be the case with glass FRP bars that have a relatively low longitudinal modulus but high strength. It should be also recalled that this beam is overreinforced. It is important to note that the deﬂection or the crack width limits often control design. Therefore, it is advisable to check the serviceability limits before optimizing the design for strength or starting the design from the serviceability calculation.

PROBLEMS Note to the reader: The analysis and design homework problems provided here address the capacity and serviceability of reinforced concrete beams and slabs subjected to ﬂexural loads. Additional design problems for beams and slabs that include ﬂexure (capacity and serviceability), shear, and detailing in an integrated fashion are given in Chapter 7. 5.1

The expression for the nominal moment capacity for an overreinforced FRP-reinforced section with two layers of tension reinforcement is

PROBLEMS

冉

Mn ⫽ Aƒ1ƒƒ1 d1 ⫺

冊

冉

177

冊

1c c ⫹ Aƒ2ƒƒ2 d2 ⫺ 1 2 2

where Aƒ1 and Aƒ2 are the areas of the FRP reinforcements in the ﬁrst (lowest) and second rows of the reinforcement. ƒƒ1 and ƒƒ2 the stresses at concrete compression failure in the reinforcements, and d1 and d2 the effective depths for the two layers. The layers have moduli Eƒ1 and Eƒ2, respectively. Derive the expression for the depth of the neutral axis, c, for use in the expression above and provide expressions for calculating ƒƒ1 and ƒƒ2. 5.2

An approximate expression for the nominal moment capacity for an underreinforced FRP-reinforced section with two layers of tension reinforcement (assuming that the lowest layer ruptures ﬁrst) is

冉

Mn ⫽ Aƒ1ƒƒu1 d1 ⫺

冊

冉

冊

1cb c ⫹ Aƒ2ƒƒ2 d2 ⫺ 1 b 2 2

where Aƒ1 and Aƒ2 are the areas of the FRP reinforcements in the ﬁrst (lowest) and second rows of the reinforcement, ƒƒu1 the design strength of the FRP reinforcement in the lowest layer, ƒƒ2 is the stress in the second layer at failure of the section, and d1 and d2 are the effective depths for the two layers. The layers have moduli Eƒ1 and Eƒ2, respectively. Provide an equation for the neutral axis at the balanced condition, cb, and an equation for ƒƒ2 for use in the expression above. 5.3

Prove that the following two equations, which are used to calculate the stress in the FRP reinforcement under sustained service loads, are equivalent: ƒƒ,sus ⫽

5.4

msus Aƒ d(1 ⫺ k/3)

ƒƒ,sus ⫽

msusnƒ d(1 ⫺ k) Icr

Consider the FRP-reinforced concrete beams listed in Table P5.4.12 The beams are to be used in interior construction, and a clear cover of 1.5 in. is to be used for all bars. Assume that No. 3 GFRP stirrups are provided and that shear is not critical. Use one layer of main bars. Determine the nominal moment capacity, Mn, and the factored moment capacity, Mn, for the beams. Comment on the effect of high-strength concrete on the beam capacities for both over- and underreinforced beams. Provide a bar graph comparing the moment capacities (nominal and factored) of the eight beams.

12 Instructors may assign only selected beams. A choice of both under- and overreinforced beams is recommended.

178

FRP FLEXURAL REINFORCEMENT

TABLE P5.4

Properties of FRP-Reinforced Beams for Analysis

Beam

ƒ⬘c (psi)

1 2 3 4 5 6 7 8

4000 4000 4000 4000 8000 8000 8000 8000

Bars 4 4 4 4 4 4 4 4

No. No. No. No. No. No. No. No.

4 6 8 4 4 6 8 4

Aslan Aslan Aslan Aslan Aslan Aslan Aslan Aslan

100 100 100 200 100 100 100 200

b (in.)

h (in.)

12 12 12 12 12 12 12 12

18 18 18 18 18 18 18 18

5.5

For the beams listed in Table P5.4, determine the load-carrying capacity (wDL, wLL, and wDL ⫹ wLL) per unit length (lb/ft) based on the factored moment capacity of the beam (determined in Problem 5.4). Assume that the beams are simply supported, uniformly loaded beams with an 18-ft span and that the ratio of dead load to live load is 1⬊3. Compare the load-carrying capacities of the eight beams in a bar graph. Also, compare the load-carrying capacity to the beam self-weight (per linear foot) and to the load that causes cracking in the beam. Discuss your observations.

5.6

For the load-carrying capacities determined for the FRP beams in Table P5.4, design grade 60 epoxy-coated steel-reinforced beams at 0.4b (and width-to-height ratios of approximately 1 to 1.5) according to ACI 318-05. Consider only moment capacity in your design of the steel beams. Compare the costs of the FRP beams to the steel-reinforced beams. Consider main bars only (assume straight bars with no bends) in your cost calculations. Assume epoxy-coated steel bars at $0.45 per pound. For concrete, use $75 per cubic yard for 4000 psi and $100 per cubic yard for 8000 psi. Assume the following costs for straight FRP bars: GRPF No. 4, $0.65 per foot; GRFP No. 6, $1.25 per foot; GRFP No. 8, $1.80 per foot, CFRP No. 4, $5.50 per foot. Provide a comparison table showing FRP versus steel beam size, main bars, and costs.

5.7

Consider the beam in Design Example 5.1. Design the beam using carbon FRP bars instead of glass FRP bars. Use the same 7 ⫻ 12 in. cross section as in the design example. Consider an overreinforced design and an underreinforced design. Bundle bars if larger CFRP bar diameters are not available. The guaranteed properties for Nos. 3 and 4 CFRP rebars are ƒ*ƒu ⫽ 300 ksi and E*ƒ ⫽ 18,000 ksi. Consider only the ﬂexural strength in this problem. Compare your results to those of the design example.

5.8

Consider the beam in Design Example 5.1. Design the beam using 8000-psi concrete instead of 4000-psi concrete. Consider an overrein-

PROBLEMS

179

forced design and an underreinforced design. Compare your results to those of the design example. 5.9

Consider the underreinforced beams in Design Example 5.1 (options b and c). Redesign the beams using the nonlinear concrete stress–strain relations instead of the approximate method given in ACI 440.1R-06 (and in the design example). Use equations (5.3) to (5.5) to determine the rectangular stress block parameters and use the iterative procedure described in Section 5.3.2. Compare your results to those of the design example. Comment on the applicability of the ACI 440.1R-06 approximate procedure. Is it conservative?

5.10 Determine the nominal and the factored moment capacities (per foot of width) of the one-way FRP-reinforced concrete slabs listed in Table P5.10. Use a 0.75-in. clear cover for slabs and do not use shear reinforcement. 5.11 Consider the beams in Table P5.4 (except for beams 1 and 513). The beams are used in interior construction and loaded with a uniformly distributed superimposed dead load of 100 lb/ft and a uniformly distributed live load of 900 lb/ft over a simply supported span of 18 ft. Assume that 20% of the live load is sustained on the beam. Determine (a) the maximum midspan instantaneous deﬂection under short-term loading, (b) the maximum midspan deﬂection under long-term loading, (c) the maximum crack width, and (d) the sustained stress in the FRP bars. To calculate the bar spacing, s, in the crack width equation, assume a clear cover of 1.5 in. to the side of the beam and that the strirrup has a bend radius of 3db. Compare the maximum deﬂections to L/360, and the crack widths and maximum sustained stresses in the bars to maximums permitted by ACI 440.1R-06. Indicate which of the beams satisfy the serviceability requirements. 5.12 Consider Design Example 5.1. Perform the serviceability checks (instantaneous and long-term deﬂection, crack width, and FRP stress un-

TABLE P5.10

Properties of FRP-Reinforced Slabs for Analysis

Slab

ƒc (psi)

1 2 3 4 5

4000 4000 4000 5000 5000

Bars No. No. No. No. No.

5 6 4 5 6

Aslan 100 at 4 in. on center Pultrall GFRP at 6 in. on center Aslan 200 CFRP at 4 in. on center Aslan 100 at 4 in. on center Pultrall GFRP at 6 in. on center

h (in.) 7 7 7 9 9

13 Beams 1 and 5 do not have the moment capacity to carry the loads stipulated. Verify as an exercise.

180

FRP FLEXURAL REINFORCEMENT

der sustained loads) for design options a, b, c, and d. (Be aware that the section may not necessarily be cracked under the service loads.) Provide a summary of your results by expanding Table 5.2 and adding to the table the deﬂection, crack width, and FRP stresses under sustained loads. Indicate which beam designs satisfy both strength and serviceability requirements and which do not. 5.13 Consider the CFRP-reinforced beams designed in Problem 5.7. Perform the serviceability checks (instantaneous and long-term deﬂection, crack width, and FRP stress under sustained loads) for these beams. Compare the behavior of the CFRP over- and underreinforced beams with the GFRP over- and underreinforced beams (Design Example 5.1 and option a). 5.14 Consider the FRP-reinforced one-way slabs listed in Table P5.10. The slabs are to be used as simply supported one-way ﬂoor slabs spanning 12 ft between beams. They are loaded with a superimposed dead load of 30 lb/ft2 (which acts in addition to the self-weight of the slab) and a live load of 100 lb/ft2. Determine the maximum midspan deﬂection after 20 years of service, the maximum crack width, and the stress in the FRP due to sustained loads on the slabs. 5.15 Design a GFRP-reinforced beam to carry a dead load of 500 lb/ft (not including the beam self-weight) and a live load of 1500 lb/ft for a built-in (ﬁxed ends) beam in interior construction on a 20-ft span. Use 5000-psi concrete. Design the beam for positive and negative moment capacity, a long-term deﬂection of less than L/360, a maximum crack width of less than 28 mils, and a sustained stress of less than 0.2ƒƒu. Assume that the top bars can be sufﬁciently developed and anchored at the ﬁxed supports. 5.16 Design a GFRP-reinforced normal-weight concrete slab for an interior ﬂoor system in a commercial building. Design for a superimposed dead load of 20 lb/ft2 and a live load of 125 lb/ft2 (10% sustained). Use 5000-psi concrete. The slab spans continuously over beams (nonintegral supports) spaced at 10 ft on center. Assume one-way slab action and use ACI coefﬁcients for slab negative and positive moments (ACI 318-05 8.3.3). Recall that FRP bars are not effective as ﬂexural reinforcements in compression. Design the slab for both ﬂexural strength and serviceability. Limit long-term deﬂections to L/360. Provide temperature and shrinkage FRP reinforcement in the transverse direction. Calculate the FRP reinforcement cost per square foot. Consider only ﬂexural design. 5.17 Design a bridge deck slab using GFRP rebars for a steel girder highway bridge with a girder spacing of 8 ft on center. The girder top ﬂange is 8 in. wide. Use 4000-psi concrete and use a 1-in. clear cover for the

PROBLEMS

181

bottom bars and a 1.5-in. cover for the top bars. Use the AASHTO standard speciﬁcations for the slab moments. Perform serviceability checks of the slab assuming an effective width strip E ⫽ 8S/(S ⫹ 2) for a single concentrated wheel load (S is the effective span perpendicular to the girders, and one-way action of the slab is assumed). Design the distribution reinforcement. Provide a reinforcement diagram for the slab. Determine the cost of the FRP reinforcement per square foot. Compare this to the cost of a traditional 8-in.-deep epoxy-coated steel bridge deck with main (transverse to trafﬁc) bars of No. 5 at 7.5 in. and distribution (parallel to trafﬁc) bars of No. 4 at 7.5 in. 5.18 Design a simply supported GFRP-reinforced beam to carry a dead load of 800 lb/ft (not including the beam self-weight) and a live load of 2500 lb/ft in interior construction on a 20-ft span. Use 5000-psi concrete. For architectural reasons, the beam height is limited to 24 in. Use a double layer of FRP tension reinforcement and use maximum No. 10 bars (see Problem 5.1). Design the beam for moment capacity, a long-term deﬂection of less than L/300, a maximum crack width of less than 28 mils, and a sustained stress of less than 0.2ƒƒu.

6 6.1

FRP Shear Reinforcement OVERVIEW

In this chapter we discuss the design of concrete ﬂexural members subjected to transverse shear forces and that have FRP main tension reinforcing bars. This includes the determination of the shear capacity of the concrete itself when the section is reinforced with FRP main bars, and the design of additional shear reinforcement in the form of stirrups if this additional reinforcement is needed. The ﬂexural members that fall into the scope of this chapter are slabs, which will have no additional shear reinforcement, and beams, which will usually have additional shear reinforcement. As discussed in detail, the shear capacity of the concrete itself when FRP main bars are used is signiﬁcantly less than when conventional steel bars are used. This is a signiﬁcant fact that has a major impact on the design of both beams and slabs reinforced with FRP bars (even though additional shear reinforcement is not used in slabs.) We do not address the design of torsion of reinforced concrete members. The design procedures presented in this chapter follow ACI 440.1R-06, which is compatible with ACI 318-05. As noted in Chapter 4, the design follows the LRFD basis for strength with a resistance factor of ⫽ 0.75. This is the same factor that is used for steel-reinforced concrete according to ACI 318-05. The reader is assumed to have familiarity with the procedures used for shear design of concrete ﬂexural member using steel reinforcing bars. 6.2

INTRODUCTION

The shear strength of a reinforced concrete section is traditionally assumed to come from a number of different material and geometric properties of the section. It is also assumed that a critical diagonal shear crack develops in the section. In a simply-supported beam the critical shear crack typically initiates from a ﬂexural crack at the bottom of the beam and propagates toward the top surface, but does not reach the top surface except at the ultimate state. The shear resistance at this time is provided by (1) the shear strength of the portion of the concrete section at the top of the beam that is not cracked by the diagonal crack; (2) the resistance provided by the friction between the two sides of the beam on either side of the critical crack, known as aggregate interlock; (3) the vertical component of shear force that is carried in the main 182

Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

6.2

INTRODUCTION

183

tensile reinforcement, which tends to prevent the shear crack from displacing vertically at the bottom of the beam, known as dowel action; (4) the vertical component of the force provided by any additional reinforcing bars, if they exist, that are placed along the length of the beam in the cross-sectional plane, known as shear reinforcement; and (5) in deep beams, the additional thrust provided by the compression arch that develops in the section roughly parallel to the shear cracks, known as arching action. No analytical methods are currently available, even for steel-reinforced concrete, to quantitatively determine the magnitude of any of these individual contributions, and the shear design of reinforced concrete members is still largely an empirical endeavor. Current reinforced concrete design practice is to lump all the contributions to shear capacity, except for the contribution from the added shear reinforcement, in what is known as the concrete contribution to shear capacity and given the symbol Vc. The contribution due to the additional shear reinforcement is given the symbol Vs. The value of Vc has traditionally been determined based on empirical data obtained from tests of beams without shear reinforcement but with steel main reinforcement. The value of Vs has been obtained by assuming that the steel stirrups yield locally where they cross the critical diagonal shear crack. The force Vs is then obtained simply as the vertical component of this tensile force in the bar, which is given by the bar area multiplied by the yield strength of the bar.1 The model for shear capacity of a reinforced concrete member described above is problematic if it is applied to the shear capacity of FRP-reinforced sections and the empirical approach above is not necessarily applicable to FRP-reinforced sections. Considering the ﬁve contributors to the shear capacity of a steel-reinforced section described above, the following can be noted (in order): (1) The depth of the neutral axis in the FRP-reinforced section is typically much less than in a steel-reinforced beam, so the contribution from the concrete itself to shear resistance is lower in the FRPreinforced beam; (2) the width of the critical diagonal crack in an FRP-reinforced beam is likely to be wider than in a steel-reinforced beam since the ﬂexural stiffness of the FRP-reinforced beam will be lower than its steel counterpart (for the same load-carrying capacity); (3) the transverse shear force resisted by the FRP main bars will be less than that resisted by steel bars since FRP bars are anisotropic and even for the same area will have lower shear rigidity than that of steel bars; (4) FRP stirrups do not yield, so the stress in the FRP stirrup cannot be calculated in the simple manner in which the force in the steel stirrup is calculated (the force that will develop in the FRP bar will depend on the displacement of the bar, which in turn will depend on how much the shear crack opens at the location where the FRP bar crosses it; this is not a trivial calculation); and (5) arching action should

This is known as the truss model for shear. A 45⬚ inclination of the critical shear crack is traditionally assumed.

1

184

FRP SHEAR REINFORCEMENT

not be affected by the FRP bar provided that the compression zone in the top of the beam stays intact (larger shear cracks and vertical displacements should not affect arching action but may well affect user perception, but arching action is applicable only to a section with special aspect ratios and cannot be relied on in long beams (a/d ⬎ 6). In addition to the above, the development of ﬂexural cracking in a beam will depend on the bond coefﬁcient of the main bars to the concrete, which as noted in Chapter 5, is larger than in steel-reinforced concrete (at least at service loads). Few ﬂexural cracks usually lead to fewer shear cracks. Fewer cracks mean that each crack is wider and that the critical shear crack in an FRP-reinforced beam will be wider than in a steel-reinforced beam, leading to less shear resistance in the section (for many of the reasons above). The comparisons above serve to support the opinion that the shear resistance of an FRP-reinforced section designed for the same nominal momentcarrying capacity as a steel-reinforced section will have a much reduced concrete shear capacity than that of an equivalent steel-reinforced beam. These observations have been supported by tests on FRP-reinforced beams and slabs that have failed in shear (Michaluk et al., 1998; Yost et al., 2001; Tureyen and Frosch, 2002; El-Sayed et al., 2005). The research identiﬁes the lower longitudinal modulus of glass FRP bars as being the primary factor leading to the lower shear capacity of concrete reinforced with FRP bars. Figure 6.1 shows an FRP-reinforced beam that failed initially in shear due to debonding of the FRP shear stirrups. The two U-shaped FRP stirrups used in the FRP-reinforced beams are shown in Fig. 6.2 alongside a steel stirrup used for the steel beams. The FRP stirrups were anchored in the tension zone, which is not permitted. However, these were the only size of stirrups that the manufacturer could provide at the time. Notice the large diagonal shear crack on the left side of the beam where failure occurred. Compare this with Fig. 5.4, where the beam failed due to compression failure at a higher load than the beam shown in Fig. 6.1.

Figure 6.1 Shear failure of an FRP-reinforced beam. (Courtesy of Dushyant Arora.)

6.3

SHEAR DESIGN OF AN FRP-REINFORCED CONCRETE SECTION

185

Figure 6.2 Steel and FRP stirrups in test beams.

6.3 SHEAR DESIGN OF AN FRP-REINFORCED CONCRETE SECTION The LRFD design for shear strength for a reinforced concrete member subjected to ﬂexural loading requires that the factored nominal shear resistance, Vn, of the member be greater than the factored (ultimate) shear demand, Vu: Vn ⬎ Vu

(6.1)

The nominal shear capacity, Vn, of an FRP-reinforced beam according to ACI 440.1R-06 is given as Vn ⫽ Vc ⫹ Vƒ

(6.2)

where Vc is the concrete contribution to the shear capacity as deﬁned in ACI 440.1R-06 (to be deﬁned in what follows), and Vƒ the contribution to the shear capacity from the FRP stirrups (hence the subscript ƒ). It is important to note that the deﬁnition of Vc in ACI 440.1R-06 is different from the traditional deﬁnition of Vc in ACI 318-05. 6.3.1

Concrete Contribution to Shear Capacity

The equation to determine the concrete contribution to the shear capacity when FRP bars are used as main bars has evolved with the three editions of

186

FRP SHEAR REINFORCEMENT

ACI440.1R. In the ﬁrst two editions, the concrete contribution to the shear capacity of the FRP-reinforced section was given as Vc,ƒ ⫽

AƒEƒ V AsEs c

(6.3)

where Vc,ƒ was used to denote the shear capacity in the concrete beam reinforced with FRP bars and Vc was deﬁned in the traditional manner as the ‘‘conventional’’ shear capacity of the concrete, usually taken as Vc ⫽ 2兹ƒc⬘ bwd

(6.4)

The ratio of the axial stiffness of the FRP bars, AƒEƒ, to the axial stiffness of an equivalent area of steel bars, AsEs, was used to ‘‘decrease’’ the traditional concrete contribution. In ACI 440.1R-06, the symbol Vc,ƒ is no longer used as an equation that accounts directly for the axial stiffness of the main reinforcing bars is used to ﬁnd the shear contribution of the concrete. This new equation can be used for both FRP bars and steel bars and hence the subscript ƒ is dropped. The equation given in ACI 440.1R-06 is Vc ⫽ 5兹ƒ⬘c bwc

(ACI 440.1R-06:9-1)

or Vc ⫽

5k (2兹ƒc⬘ bwd) 2

(ACI 440.1R-06:9-1a)

where bw is the width of the beam web and c is the depth of the neutral axis in the cracked elastic section as deﬁned for the serviceability limit state ﬂexural behavior in Chapter 5 and given there as c ⫽ kd k ⫽ 兹(ƒƒ)2 ⫹ 2ƒƒ ⫺ ƒƒ ƒ ⫽

Eƒ Ec

As can be seen in the second form of the equation for Vc, it is the traditional equation multiplied by 2.5k. Since the FRP bars have less axial stiffness than that of steel bars, the value of k will be less than that of steel bars and the contribution to the shear capacity will be less than in the case of steel bars.

6.3

SHEAR DESIGN OF AN FRP-REINFORCED CONCRETE SECTION

187

The equation is empirical and was developed by ﬁtting to test data (Tureyen and Frosch, 2003). 6.3.2

Shear Capacity of FRP Stirrups

The shear capacity of the FRP stirrups, Vƒ, is given by equations similar to those given for steel stirrups. The equation, which assumes a 45⬚ inclination of the critical shear crack to the longitudinal axis of the beam, is for vertical stirrups, Aƒvƒƒvd s

(ACI 440.1R-06:9-2)

Aƒvƒƒvd (sin ␣ ⫹ cos ␣) s

(ACI 440.1R-06:9-5)

Aƒvƒƒv d sin ␣ s

(ACI 440.1R-06:9-6)

Vƒ ⫽ for inclined stirrups, Vƒ ⫽ and for continuous spirals, Vƒ ⫽

where Aƒv is the total area of the stirrups across the shear crack, ƒƒv the stress in the FRP stirrups, s the stirrup spacing measured along the beam axis (also called the pitch), and ␣ the angle between the beam axis and the inclined stirrup. The use of bent-up main bars as shear reinforcement is not recommended, due to the strength reduction at the bend in the bar. In addition, bentup bars are not generally available, and their use in reinforced concrete has not been tested. Inclined stirrups, if used, should be closed or U-shaped stirrups, similar to vertical stirrups. As indicated previously, FRP stirrups will not yield like steel stirrups. Neither do they rupture when the beam fails in shear, and therefore the design strength of an FRP stirrup cannot be used in place of the yield stress in the case of the steel stirrup. The stress in the FRP stirrup is limited by its tensile strain. The tensile strain in the stirrup is limited to prevent the diagonal shear crack from opening too much, thereby reducing the effectiveness of the concrete contribution to the shear strength. In addition, a large shear crack can lead to overall instability of the section, due to rigid-body rotations (as can be seen in Fig. 6.1). The strength of the FRP stirrup, ƒƒv, is limited by the smaller of

188

FRP SHEAR REINFORCEMENT

ƒƒv ⫽ 0.004Eƒ ⱕ ƒƒb

(ACI 440.1R-06:9-3)

where ƒƒb is the tensile strength of the FRP rebar with a bend (given in Chapter 4),

冉

ƒƒb ⫽ 0.05

冊

rb ⫹ 0.3 ƒƒu db

(ACI 440.1R-06:7-3)

where rb is the inside radius of the bend and db is the diameter of the FRP rebar. A minimum inside radius-to-diameter ratio of 3 is required for FRP bars according to ACI 440.1R-06. Figure 6.3 is a close-up of bends in Nos. 7 and 3 FRP bars from different manufacturers. Due to the manufacturing method used to produce FRP bars with bends, the corner of the bar at the bend is ‘‘ﬂattened’’ and the thickness of the bar is smaller in the bend region. Internal ﬁbers on the exterior of the bend are longer than those on the interior of the bend. As the bar is stretched, the corner of the bar experiences through-the-thickness radial stresses, which cause premature failure of the linear–elastic material in the FRP bar. This is quite unlike a steel stirrup with a bend, where the permanent set due to plastic deformation in the corner region causes the bend. For elastic–plastic materials such as steel, the yield stress in the corner region is not reduced and no reduction is taken for bends in steel bars.

Figure 6.3 Close-up of bends in Nos. 7 and 3 FRP bars and No. 3 steel bar shown for comparison.

6.4

6.3.3

LIMITS ON SHEAR REINFORCEMENT AND SHEAR STRENGTHS

189

Punching Shear Capacity in Slabs

The punching shear capacity of concrete slabs reinforced with FRP bars in two orthogonal directions can be calculated from Vc ⫽ 10 兹ƒc⬘ b0c

(ACI 440.1R-06:9-8)

where b0 is the perimeter of critical section evaluated at d/2 away from the point load (or support). To calculate the reinforcement ratio, the average area and average depth of the reinforcement in both directions in the tensile reinforcement layer only (if there are two layers) are used (Ospina, 2005).

6.4 LIMITS ON SHEAR REINFORCEMENT AND SHEAR STRENGTHS FOR SHEAR DESIGN Similar to steel-reinforced beams, the maximum spacing permitted for FRP stirrups is given as smax ⫽

d 2

or

24 in.

(6.5)

This condition often determines the minimum amount of shear reinforcement that needs to be provided in FRP-reinforced beams that are appropriately designed for ﬂexural capacity. This condition ensures that the assumed shear crack at 45⬚ will be intercepted by at least one stirrup. The tail length of 90⬚ hooks in the stirrups should be at least 12db. Hooks must be anchored in the compression zone of the member. This is particularly important to recall for continuous members. In addition, a minimum amount of shear reinforcement is required to prevent brittle shear failure of the beam when Vu ⬎ Vc /2. The amount (which is given by the same formula as that for steel-reinforced beams) is given as Aƒv,min ⫽

50bw s ƒƒv

(ACI 440.1R-06:9-7)

To prevent shear crushing failure, the shear capacity of the concrete is limited to Vc ⱕ 8兹ƒc⬘ bwd

(6.6)

190

6.5

FRP SHEAR REINFORCEMENT

DESIGN PROCEDURE FOR FRP SHEAR REINFORCEMENT

Step 1. Determine the shear demand. The shear demand is calculated in the same way as in ACI 318-05 and is calculated using the same loading as that used for ﬂexural design of the member. Step 2. Determine the concrete shear capacity with FRP rebars. The concrete shear capacity is calculated using the ACI 440.1R-06 formula. This calculation has the most signiﬁcant effect on the design of FRP members for transverse loads (both shear and ﬂexure) and is the most signiﬁcant difference between the steel and FRP design procedures for concrete members for shear. Step 3. Check if additional shear reinforcement is required. According to ACI 318-05, the following are checked: If Vu ⱖ 0.5Vc, minimum shear reinforcement is required to be provided; if Vu ⱖ Vc, additional shear reinforcement is required to be designed. Step 4. Design the shear reinforcement. FRP shear reinforcement is designed using strain limits to determine the maximum permissible stress in the FRP stirrups. The designer should conﬁrm that FRP stirrups of the sizes anticipated in the design can actually be obtained from a manufacturer. Consider varying the stirrup spacing along the beam length to economize the stirrup costs, if possible. Step 5. Determine the factored shear strength of the beam and compare it with the demand. A resistance factor of ⫽ 0.75 is used per ACI 318-05 to determine the factored shear strength of the member. If the demand is not met, redesign the beam or slab for shear capacity. For slabs in which no additional shear reinforcement is provided, this may require a complete ﬂexural redesign of the slab, which could lead to a thicker slab or more ﬂexural reinforcement and even a change in the failure mode designed. This is signiﬁcantly different from the design of slabs with steel bars, where shear does not usually control the ﬂexural design (or thickness) of commonly designed slabs. Step 6. Check the limits on reinforcement and concrete strength. Check the minimum amount of (or maximum spacing for) the stirrups. If maximum spacing controls, the stirrups can be redesigned using a smaller-diameter bar for the stirrups if available. Step 7. Detail the stirrups. Use closed loops with 90⬚ hooks with a minimum tail length of 12db. Place the hooks in the compression zone of the beam (i.e., the top for a simply supported beam). (For further discussion on detailing of FRP rebars, see Chapter 7.) Draw a sketch of the ﬁnal design to scale (including the bend radii) to make sure that the beam size is sufﬁcient to ﬁt the FRP stirrups and that the main bar spacing is as needed for bond development length calculations (see Chapter 7).

6.5

DESIGN PROCEDURE FOR FRP SHEAR REINFORCEMENT

191

Design Example 6.1: Beam Design for Shear Strength Design shear reinforcement for the overreinforced beam discussed in Design Example 5.1. The geometric and material properties are: simply supported beam, 11-ft span; 4000-psi concrete; FRP bar design strength, ƒƒu ⫽ 72 ksi; two No. 6 main bars; Aƒ ⫽ 0.88 in2; d ⫽ 9.75 in. (No. 3 FRP strirrups were assumed in the ﬂexural design); wLL ⫽ 400 lb/ft (20% sustained); wSDL ⫽ 208 lb/ft (superimposed dead load); wDL ⫽ (150 lb/ft3)(7/12)(12/12) ⫽ 87.5 lb/ft (selfweight); Wu ⫽ 1.2(87.5 ⫹ 208) ⫹ 1.6(400) ⫽ 1094 lb/ft. SOLUTION Step 1. Determine the shear demand. For a simply supported beam, calculate Vu at a distance d from the support: Vu ⫽ Wu

冉 冊

冉

冊

l 11 9.75 ⫺ d ⫽ 994.6 ⫺ ⫽ 4662 lb ⫽ 4.66 kips 2 2 12

Step 2. Determine the concrete shear capacity with FRP rebars. The properties of the elastic section were determined previously as follows: k ⫽ 兹(ƒƒ)2 ⫹ 2ƒƒ ⫺ ƒƒ ⫽ 兹[0.0129(1.8)]2 ⫹ 2(0.0129)(1.8) ⫺ 0.0129(1.8) ⫽ 0.194

Therefore, c ⫽ kd ⫽ 0.194(9.75) ⫽ 1.89 in. and Vc ⫽ 5兹ƒc⬘bwc ⫽ 5兹4000(7)(1.89) ⫽ 4184 lb ⫽ 4.18 kips Notice that the concrete contribution to shear resistance of concrete beam with FRP bars is signiﬁcantly less than for conventional steel bars. For steel bars the contribution would have been calculated using the ACI 318-05 equation as Vc ⫽ 2兹ƒc⬘ bwd ⫽ 2兹4000(7)(9.75) ⫽ 8633 lb ⫽ 8.6 kips Step 3. Check if additional shear reinforcement is required. If Vu ⱖ 0.5Vc, 4.66 kips ⱖ 0.5(0.75)(4.18) ⫽ 1.57 kips ⬖minimum shear reinforcement required

192

FRP SHEAR REINFORCEMENT

If Vu ⱖ Vc, 4.66 kips ⱖ 0.75(4.18) ⫽ 3.140 kips ⬖additional shear reinforcement required

Step 4. Design the shear reinforcement. Assume No. 3 FRP stirrups. Aƒv ⫽ 2(0.11) ⫽ 0.22 in2. The design strength of the FRP stirrups is the lesser of 0.004Eƒ ⫽ 0.004(6500) ⫽ 26 ksi or

冉

ƒƒb ⫽ 0.05

冊

rb ⫹ 0.3 ƒƒu ⫽ [0.05(3.0) ⫹ 0.3](72) ⫽ 32.4 ksi db

Therefore, ƒƒv ⫽ 26.0 ksi. Note that in the calculation of the strength of a bar with the bend, rb /db ⫽ 3 has been assumed and the strength of the No. 3 bar is not increased (i.e., taken as 72 ksi). If the bar strength were increased to ƒƒu ⫽ 88 ksi (for ƒ*ƒu ⫽ 110 ksi), the strength of the bar with the bend would increase. It most cases this will not control since the bar strength as required for the strain limit on the FRP bar will control. Similarly, if a larger rb /db were used, as is most likely to be the actual case for FRP bars with bends, the strength of the bar with the bend will increase. The stirrup spacing required is given by the lesser of s⫽

Aƒvƒƒvd 0.75(0.22)(26)(9.75) ⫽ ⫽ 27.4 in. Vu ⫺ Vc 4.66 ⫺ 0.75(4.18)

or s⫽

d 9.75 ⫽ ⫽ 4.9 in. 2 2

Therefore, use s ⫽ 4.5 in. Step 5. Determine the factored shear strength of the beam and compare it with the demand. The shear capacity provided by the FRP stirrups is Vƒ ⫽

Aƒvƒƒvd 0.22(26)(9.75) ⫽ ⫽ 12.39 kips s 4.5

The shear capacity of the concrete is

6.5

DESIGN PROCEDURE FOR FRP SHEAR REINFORCEMENT

193

Vc ⫽ 4.18 kips and Vn ⫽ Vc ⫹ Vƒ ⫽ 4.18 ⫹ 12.39 ⫽ 16.57 kips Vn ⫽ 0.75(16.57) ⫽ 12.43 kips ⬎ 4.66 kips (Vu)

The beam is well overdesigned for shear since the maximum spacing controls. Step 6. Check the minimum limits on reinforcement and concrete strength. Amin ƒv ⫽

50bs 50(7)(4.5) ⫽ ⫽ 0.06 in2 ⬍ 0.22 in2 → OK ƒƒv 26,000

Vc ⱕ 8兹ƒc⬘ bd ⫽ 8兹4000(7)(9.75) ⫽ 34,532 lb ⫽ 34.5 kips (⬎Vc ⫽ 4.18) → OK

Step 7. Detail the stirrups. Use closed loops with 90⬚ hooks with a minimum tail length of 12db ⫽ 12(0.375) ⫽ 4.5 in. Place the hooks in the compression zone of the beam (i.e., the top for the simply supported beam given). Design Example 6.2: Punching Shear Design for a Bridge Deck Slab The bridge deck in Design Example 5.2 is revisited to determine if the punching shear capacity of the slab with three No. 5 GFRP main bars and two No. 5 GFRP distribution bars is sufﬁcient. SOLUTION Step 1. Determine the punching shear demand. The punching shear load is the factored P20 wheel load plus the impact multiplied by the appropriate AASHTO live load factors and calculated as Vu ⫽ 2.17(16.0)(1.3) ⫽ 45.14 kips Step 2. Determine the concrete shear capacity with FRP rebars. For punching shear under the wheel load, only the bottom reinforcement mat is regarded as active. The average depth and the average reinforcement ratios of the transverse and longitudinal bars need to be calculated. For the main reinforcement (No. 5 at 4 in.) in the transverse direction (superscript T in what follows), we have previously calculated, d T ⫽ 6.94 in. and Tƒ ⫽ 0.0112. For the distribution reinforcement (No. 5 at 6 in.) in the longitudinal direction (superscript L in

194

FRP SHEAR REINFORCEMENT

what follows), we obtain the following: dL ⫽ 6.31 in. and Lƒ ⫽ 0.0082. The average values are d ⫽ 6.63 in. and ƒ ⫽ 0.0097. The distance to the neutral axis of the cracked section of the slab is found using the average effective depth and the average reinforcement ratio as follows: The modular ratio is ƒ ⫽

Eƒ 5,920,000 ⫽ ⫽ 1.64 Ec 57,000兹4000

The neutral-axis depth ratio, k ⫽ c/d, k ⫽ 兹(ƒƒ)2 ⫹ 2ƒƒ ⫺ ƒƒ ⫽ 兹[0.0097(1.64)]2 ⫹ 2(0.0097)(1.64) ⫺ 0.0097(1.64) ⫽ 0.163

c ⫽ kd ⫽ 0.163(6.63) ⫽ 1.08 in. The punching shear perimeter is measured at a distance of d/2 from the tire footprint. The tire area is 0.01P20 ⫽ 0.01(16,000) ⫽ 160 in2 The width of the load patch is therefore 20 in. and the length is 8 in. The punching shear perimeter is found as b0 ⫽ 2[(20 ⫹ 6.63) ⫹ (8 ⫹ 6.63)] ⫽ 82.5 in. and the nominal punching shear capacity of the slab is Vn ⫽ Vc ⫽ 10兹ƒ⬘cb0c ⫽ 10兹4000(82.5)(1.08) ⫽ 56,370 lb ⫽ 56.4 kips The factored punching shear capacity is Vn ⫽ 0.75(56.4) ⫽ 42.3 kips ⬍ 45.1 kips (Vu)

The factored nominal capacity of the slabs is less than the punching shear demand and the slab does not satisfy the loading requirements. The slab bottom reinforcement should be increased slightly for punching shear capacity. The top reinforcement does not need to be redesigned. Increasing the bottom bars to three No. 5 per foot of width (No. 5 at 4 in.), bars in the longitudinal direction will meet the requirements. Note, however, that the AASHTO LFD factors were originally developed to be compatible with the ‘‘old’’ ACI 318-99 resistance factor for shear of ⫽ 0.85. In that case, the design above is satisfactory.

PROBLEMS

195

The slab should also be checked for transverse shear capacity at the edge of the girders. To do this calculation, the shear force per unit width of the slab under the HS 20 wheel load is required. The AASHTO approximate method for determining the moment per foot width of the slab does not provide a value for the shear force per foot width (or does not provide the effective width for the wheel load). The AASHTO LRFD bridge design speciﬁcation provides an equation to calculate the distribution width for deck slabs which can be used to determine the shear force per unit width for this calculation. PROBLEMS Note to the reader: The analysis and design homework problems provided here address the capacity of reinforced concrete beams and slabs subjected to transverse and punching shear loads. Additional design problems for beams and slabs that include ﬂexure (capacity and serviceability), shear, and detailing in an integrated fashion are given in Chapter 7. 6.1 For the beams listed in Table P5.4,2 determine, Vc, the concrete contribution to the shear capacity, and Vƒ, the FRP stirrup contribution to the shear capacity, if No. 3 Aslan 100 GFRP vertical stirrups are provided at the maximum spacing of d/2. Determine the nominal shear capacity, Vn, and the factored shear capacity, Vn, of the beams. Determine the shear capacities of the beams if they are reinforced with grade 60 No. 6 steel main bars (determine an appropriate d for interior construction with steel bars) and grade 60 No. 3 steel stirrups at d/2. Compare the shear capacities of the FRP- and steel-reinforced beams. 6.2 For the values of the factored shear capacities calculated in Problem 6.1, determine the load-carrying capacity (wDL, wLL, and wDL ⫹ wLL) per unit length (lb/ft) for the FRP-reinforced beams. Assume that the beams are simply supported uniformly loaded beams with an 18-ft span and that the ratio of dead load to live load is 1⬊3. Calculate the shear demand at a distance d from the face of the support (assumed to be at the nominal span length). Compare the load-carrying capacities of the eight beams in a bar graph. Also, compare the load-carrying capacities to the load-carrying capacities for the beams based on their ﬂexural capacities (Problem 5.5). Discuss your observations. 6.3 Consider the FRP-reinforced one-way slabs listed in Table P5.6. Determine the nominal shear capacity, Vn, and the factored shear capacity, Vn, of each slab. Check if this shear capacity is sufﬁcient if the slabs 2

Instructors may assign only selected beams from the table.

196

FRP SHEAR REINFORCEMENT

are used as simply supported one-way ﬂoor slabs spanning 12 ft between beams and loaded with a superimposed dead load of 30 lb/ft2 (which acts in addition to the self-weight of the slab) and a live load of 100 lb/ft2. 6.4 Consider the beams in Design Example 5.1, options a to d. Design the shear reinforcement for the beams assuming No. 3 GRFP stirrups with the nominal properties used in Design Example 6.1. Determine the actual shear capacity of the beams if minimum shear reinforcement requirements control. Calculate the cost of the FRP shear reinforcement for each beam. Use $0.40 per foot for No. 3 GFRP bar in addition to $1.00 per bend (i.e., ﬁve bends per closed stirrup with 90⬚ hooks). 6.5 Consider the beams in Table P5.4. The beams are used for interior construction and are loaded with a uniformly distributed superimposed dead load of 100 lb/ft and a uniformly distributed live load of 900 lb/ ft over a simply supported span of 18 ft. Design the shear reinforcement to carry the loads indicated. Assume that the ﬂexural capacity of these beams is sufﬁcient for both strength and serviceability. Calculate the cost of the FRP shear reinforcement for the beams. Use $0.40 per foot for No. 3 GFRP bar and add the cost of bends at $1.00 per bend. 6.6 Consider the beams in Table P5.4. The beams are used for exterior construction and are loaded with a uniformly distributed superimposed dead load of 400 lb/ft and a uniformly distributed live load of 1500 lb/ft over a simply supported span of 18 ft. Design the shear reinforcement to carry the loads indicated. Assume that the ﬂexural capacity of these beams is sufﬁcient for both strength and serviceability. Consider No. 4 GFRP bars for the vertical stirrups. Use minimum shear reinforcement where appropriate in the interior of the span to minimize the cost of the stirrups. Sketch the stirrup layout along the beam length. 6.7 Consider beams 3 and 4 in Table P5.4. The beams are used for exterior construction and are loaded with a uniformly distributed superimposed dead load of 400 lb/ft and a uniformly distributed live load of 1200 lb/ft over a simply supported span of 18 ft. Design the shear reinforcement to carry the loads indicated. Assume that the ﬂexural capacity of these beams is sufﬁcient for both strength and serviceability. Use No. 2 GFRP rectangular spiral reinforcement for the beams. Determine the required pitch of the spiral reinforcement. 6.8 Consider the slabs in Table P5.10 with reinforcement as indicated used in both directions (i.e., two-way slab action). Determine the punching shear capacity of the slab when used in a reinforced concrete building frame with typical square 20 ⫻ 20 in. reinforced concrete columns. 6.9 Consider the FRP-reinforced highway bridge deck discussed in Design Examples 5.2 and 6.2. Determine the transverse shear capacity (as

PROBLEMS

197

opposed to the punching shear capacity) of the deck parallel to the edges of the longitudinal prestressed girders. Assume an effective width strip E ⫽ 8S/(S ⫹ 2) for a single concentrated wheel load (S is the effective span perpendicular to the girders, and one-way action of the slab is assumed). 6.10 Consider a beam with a double layer of main FRP tensile reinforcement such as that discussed in Problems 5.1, 5.2, and 5.17. Discuss how the use of a double layer of main bars will affect the shear capacity of the FRP-reinforced beam.

7 7.1

FRP Reinforcement Detailing OVERVIEW

In this chapter we discuss the subject of the detailing of FRP rebars for use in concrete structures. This includes a discussion of the geometric issues that need to be considered when using FRP bars and the quantitative issues that need to be addressed to ensure that FRP bars are sufﬁciently anchored in the concrete to transfer the required forces from the bars into the concrete. The chapter follows the procedures of ACI 440.1R-06 and the code equations for calculating the development length for FRP bars at different locations along the length of the reinforced concrete member. Since FRP bars are only used in tension, no information is provided on development and anchorage for compression reinforcement. The design procedures presented in this chapter follow ACI 440.1R-06, which is compatible with ACI 318-05. It is assumed that readers are familiar with the subject of bond and development in steel reinforcing bars and with the procedures provided in ACI 318-05 for the calculation of development length for steel reinforcing bars.

7.2

INTRODUCTION

Detailing of reinforcing bars refers to the determination of the dimensions (but not sizes), shapes, and positions of the bars in cross section. The strength and serviceability calculations described previously are used to determine the cross-sectional areas (and bar sizes) of the tension (main) and shear reinforcing bars in a beam or slab; however, these calculations do not give the designer the lengths of the bars, the spacing of the bars, or the location of the bars in the section. (However, recommended geometric spacing limits are used to decide on the number of bars possible in a section.) Neither do these equations check whether the bars are sufﬁciently anchored or embedded in the concrete at all sections along the length to ensure that the strengths calculated can be achieved. This falls to detailing, which should more rightly be called rebar length, shape, and position design. It is important to note that this is a very important part of the design of a reinforced concrete structure and is not simply a construction-related item as the term detailing could imply. 198

Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

7.2

INTRODUCTION

199

In addition to the geometric calculations performed to detail the locations of the FRP bars in the section and along the length of the member, the primary calculations that are performed are those related to what is traditionally known as development and splices of reinforcement, covered in Section 12 of ACI 318-05. From the early days of research into the use of FRP bars as reinforcements for concrete, it was recognized that anchorage of the reinforcement in the concrete and the transfer of stresses between the FRP bar and the concrete were likely to be deﬁning characteristics of FRP bars and their design. Since FRP bars require a high percentage of longitudinal ﬁber to develop their tensile strength and tensile modulus, the key question was how to create a suitable surface in the resin layer on the outside of the bar that would be able to transfer the forces from the concrete and mobilize the longitudinal ﬁbers in the interior of the bar. First-generation FRP bars used a surface layer that contained relatively coarse sand particles and helically wrapped ﬁbers. These were followed by bars that had more controlled helical wraps and a much ﬁner silica sand coating or with bars having a sand coating only. Some manufacturers produced bars with helical wraps and no coatings. Bars were also produced that had a molded surface with protruding deformations that were reinforced with ﬁne silica particles. Many of these products are no longer available on the market. Figure 7.1 shows images of FRP rebars tested by Katz (2000) that are representative of the bars produced in the 1990s. Research was conducted on the durability of the surface deformation layer to determine if the failure of the bond layer due to environmental degradation, high temperature, or cyclic loading would lead to failure of the bar itself or lead to the bar not being able to mobilize its core of unidirectional ﬁber reinforcements (e.g., Nanni et al., 1995; Bank et al., 1998; Katz et al., 1999; Katz, 2000). The other major topic of research related to the bonding of FRP bars focused on characterizing the effect of bar mechanical properties on the

Figure 7.1 Surface textures of various FRP bars of the 1990s. (Courtesy of Amnon Katz.)

200

FRP REINFORCEMENT DETAILING

local constitutive behavior of FRP bars when pulled from concrete (Chaallal and Benmokrane, 1993; Cosenza et al., 1997; Focacci et al., 2000). The objective of this work was to try to determine analytically the embedment length that was required to develop the bar tensile stress. Since the 1990s, the research and development for new types of glass FRP bars has slowed, and two types of bars are available in North America: bars with helically wound surface ﬁbers that create a small undulating bar surface together with a light silica sand coating (Fig. 7.2) and bars with a sand-coated layer only (Fig. 7.3). Both of these bars have been shown to develop a satisfactory bond to concrete.

7.3

GEOMETRIC DETAILS

Although nominally the same as steel bars in terms of bar number sizes, FRP rebars have different geometric features that should be accounted for by the designer. This applies particularly to the available bend radii for bent bars used as strirrups and as hooks. Bent bars are produced in a separate manufacturing process and are not made from straight bars as are steel bent bars. They are therefore really ‘‘bars with bends’’ rather than ‘‘bent bars.’’ Samples of FRP bars with bends are shown in Fig. 7.4. As noted previously, FRP bars are made from thermosetting resins that cannot be bent after they have cured, nor can they be heated and bent. A thermosetting resin will not soften when heated and then re-formed into a different shape upon cooldown [as can be done with a thermoplastic resin (see Chapter 2 for more on materials)]. Therefore, all bent FRP bars must be specially manufactured for the job at the manufacturer’s plant. A selection of bent bars ready for shipment from a manufacturer’s plant is shown in Fig. 7.5. Close coordination with the bar manufacturer is required during the design phase of the job. This is unlike the design of a steel-reinforced member, where it can be assumed that any size bar of bent bar can be obtained. In addition, at this time, due to the way in which bent bars are manufactured, it is not possible to obtain bars with bends of other than 90⬚. Therefore, if FRP bars

Figure 7.2 Close-up of glass FRP bar with helical wrap and ﬁne sand coating.

7.3

GEOMETRIC DETAILS

201

Figure 7.3 Close-up of glass FRP bar with sand coating only.

with other bends are required, the FRP bar manufacturer should be consulted well in advance of the design of the concrete member. It is also not possible to obtain closed-loop stirrups of all sizes. All stirrups must be preordered and manufactured to speciﬁc dimensions. Typical inside bend radii reported by an FRP bar manufacturer and the ratio rb /db needed to calculate the strength of the bar with the bend are given in Table 7.1. The smaller the ratio, the larger the reduction in bar strength; the larger the ratio, the more difﬁcult it is to position bars at the horizontal tangential corner of the stirrup as required for a single layer of bottom bars in a beam, for example. Since Nos. 3 and 4 bars are typically used as stirrups in FRP-reinforced beams, the large inside radii of these bars mean that the ﬁrst ‘‘corner’’ bar is positioned farther from the edge of the beam than in a steel bar-reinforced beam, and standard tables for the number of bars permitted in a given width should be used with care.

Figure 7.4 Samples of FRP bars with bends.

202

FRP REINFORCEMENT DETAILING

Figure 7.5 FRP rebars with bends at manufacturer’s plant ready for shipping. (Courtesy of Hughes Brothers.)

7.3.1

Calculation of Bar Spacing

The side distance for an FRP corner bar is calculated in the same way as for a steel bar. However, the condition that the inside radius be 3db or greater needs to be enforced. Figure 7.6 shows the geometry of the corner bar and the parameters A, B, and C (clear cover, stirrup diameter, and inside stirrup radius) that are used to calculate this distance. For example, a beam with a No. 3 stirrup with an inside bend radius of 2.125 in. and a side clear cover of 1.5 in. gives a distance to the center of the corner bar (edge distance) of A ⫹ B ⫹ C ⫽ 1.5 ⫹ 0.375 ⫹ 2.125 ⫽ 4.0 in. TABLE 7.1 FRP Bars

Typically Available Bend Radii for

Bar Number

Inside Radius (in.)

rb / db

2 3 4 5 6 7 8

1.5 2.125 2.125 2.25 2.25 3.0 3.0

6.0 5.67 4.25 3.6 3.0 3.43 3.0

7.3

GEOMETRIC DETAILS

203

B A

C

D

Diameter of corner bar is assumed to be located to intersect the horizontal tangent to stirrup bend

Figure 7.6 Corner bar side distance calculation parameters. (From Wang and Salmon, 2002, with permission from John Wiley & Sons.)

For a minimum clear (D in Fig. 7.6) spacing of db or 1.0 in. for the main bars, the minimum width of a beam with two No. 6 bars and No. 3 stirrups is therefore minimum width ⫽ edge distance ⫹ –12 db ⫹ db or 1.0-in. space ⫹ –12 db ⫹ edge distance ⫽ 4 ⫹ 0.375 ⫹ 1.0 ⫹ 0.375 ⫹ 4 ⫽ 9.75 in.

For a steel bar this minimum is 7.0 in., since for a No. 3 steel stirrup the inside radius is only twice the stirrup diameter (i.e., 0.75 in.) and A ⫹ B ⫹ C ⫽ 2.625 in. Notice that the 7-in. beam width used in the illustrative examples presented in Chapters 5 and 6 is possible only if it is assumed that a No. 3 stirrup with an inside radius of 3db is available and that the outside clear cover is reduced to 1.125 in., and a minimum clear spacing between the main bars is used. In this case, A ⫹ B ⫹ C ⫽ 1.125 ⫹ 0.375 ⫹ 3(0.375) ⫽ 2.625 and the beam width is edge distance ⫹ –12 db ⫹ db or 1.0-in. space ⫹ –21 db ⫹ edge distance ⫽ 2.625 ⫹ 0.375 ⫹ 1.0 ⫹ 0.375 ⫹ 2.625 ⫽ 7.0 in.

204

7.4

FRP REINFORCEMENT DETAILING

BOND STRENGTH OF FRP BARS

The transfer of forces between the FRP reinforcing bar and the concrete depends on the development of sufﬁcient bond strength between the FRP bar and the surrounding concrete. Fundamentally, the bond stress can be determined using the equilibrium equation ledbu ⫽ Aƒ,barƒƒ

(ACI 440.1R-06:11-1)

which states that the average bond stress (or longitudinal shear stress), u, on the outer surface of the bar over an embedment length, le, must be equal to the tensile stress in the bar, ƒƒ, that acts on the cross-sectional area of that bar, Aƒ,bar. However, the equilibrium equation above is not used in the simple form given since the bond stress over the length le varies, and more important, it may not be able to be mobilized over the full length le due to premature failure of the concrete surrounding the bar or due to the bar pulling out of the concrete. Therefore, an alternative form is provided in ACI 318-05 for steel bars and in ACI 440.1R-06 for FRP bars. One of the fundamental assumptions of reinforced concrete behavior is that strain compatibility exists between the reinforcing bar and the concrete. This means that it is assumed that ‘‘perfect’’ bond exists and that no slip between the reinforcing bar and the concrete occurs when the tensile forces are transferred from the bar to the concrete by shear stresses (or bond stresses) on the surface of the bar. For this to occur, there must be a sufﬁcient amount of the bar embedded in the concrete, le, so that all the tensile stress in the bar can be transferred into the concrete. If insufﬁcient length is available, the amount of tensile force required is not transferred into the concrete and the element can fail, since the internal equilibrium of tensile and compressive forces required for ﬂexure cannot be maintained. However, it is not always possible to transfer all of the tensile force in the bar into the concrete for a given embedment length, since it may not be possible to develop sufﬁcient bond strength, due either to splitting of the concrete surrounding the bar or because the bar pulls out of the concrete (as noted previously). Based on an analysis of beam test data by Wambeke and Shield (2006) in which both splitting and pull-out failures occurred, ACI 440.1R-06 recommends the maximum (effective) stress achievable in an FRP bar based on bond failure be taken as ƒƒe ⫽

兹ƒ⬘c

␣

冉

13.6

冊

le C le ⫹ ⫹ 340 ⱕ ƒƒu db db db

(ACI 440.1R-06:11-3)

where C is the lesser of (1) the distance from the center of the bar to the nearest outer concrete surface in the tension zone or (2) half the on-center spacing of the bars (side by side), and ␣ is the bar location factor. It is taken as 1.0 for bars that are in the bottom 12 in. of the formwork when the concrete

7.5

DEVELOPMENT OF STRAIGHT FRP BARS

205

is cast and as 1.5 when the bars are more than 12 in. above the bottom of the formwork when the beam is cast (known as top bars). ACI 440.1R-06 further recommends that the term C/db not be taken larger than 3.5 and that the minimum embedment length, le, be at least 20 bar diameters, or 20db. It is seen from the equation above that the effective design strength of the FRP rebar can be less than the maximum design strength of the bar based on tensile failure. This is unique to FRP bars and can complicate the design of ﬂexural members since the bar strength is needed in the design process, and usually the details of the reinforcement are not precisely known at the time of the initial ﬂexural design. This does not happen in the design of steelreinforced concrete, in which the bar will always be able to achieve its yield stress and will not fail prematurely due to bond failure provided that it is appropriately detailed (i.e., it has sufﬁcient embedment length or anchorage). Therefore, in steel design, detailing is in fact ‘‘only’’ detailing, and it occurs after the ﬂexural design is completed. This is due primarily to the fact that FRP bars have a very high strength relative to their modulus compared with steel bars. In the ﬂexural design, sections that are controlled by the bar not being able to achieve its design strength due to bond failure are referred to in 440.1R06 as bond-critical sections. In this case the nominal moment capacity should be reevaluated using the lower bar-effective design strength. If the bond strength controls, the design of the beam and its capacity are obtained using the equations for an underreinforced beam, and a resistance factor of ⫽ 0.55 is recommended (even if the section was originally designed as an overreinforced section) since bond failure by splitting is regarded as a brittle failure mode. Alternatively, the beam can be redesigned as an overreinforced beam using the lower bond-critical bar strength, and the resistance factor for an overreinforced beam can be used, 0.55 ⱕ ⱕ 0.65. 7.5

DEVELOPMENT OF STRAIGHT FRP BARS

The development length of a reinforcing bar is the length that is required to anchor the bar in the concrete in order to develop the tensile stress in the bar that is required for internal moment equilibrium at any section. In steelreinforced concrete, in which underreinforced beams are most common, the bar stress that needs to be developed at the maximum moment location is the yield stress of the bar. In FRP design, however, where overreinforced beams will most commonly be designed (primarily for serviceability, as discussed in Chapter 5), the bar is not stressed to its maximum design strength at the maximum moment. Therefore, in FRP-reinforced beams the development length of the bar is determined from the actual stress, ƒƒr, that the bar will experience at the failure of the beam at the location of the maximum moment. This stress is either (1) the design strength of the bar for underreinforced beams, ƒƒu, or (2) the actual

206

FRP REINFORCEMENT DETAILING

stress in the bar for overreinforced sections, ƒƒ, or (3) the effective bond critical design stress in the bar for both over- and underreinforced sections, ƒƒe. The development length, ld, required is then given as ld ⫽

␣(ƒƒr / 兹ƒc⬘) ⫺ 340

13.6 ⫹ C/db

db

(ACI 440.1R-06:11-6)

All other ACI 318-05 provisions related to the development of bars at inﬂection points or at bar cutoffs, for steel bars are all also required for FRP bars. FRP bars should extend a distance d or 12db, whichever is greater, beyond points of inﬂection or where terminated when not required for moment capacity. The provision for the development of FRP bars at simple supports is ld ⱕ

Mn ⫹ la Vu

(ACI 440.1R-06:11-7)

Note that the resistance factor is added to the nominal moment in the numerator of the ﬁrst term. When tension bars are conﬁned by the compressive reaction at the simple support, they have less tendency to cause splitting and the development length can be increased to ld ⱕ 1.3

Mn ⫹ la Vu

(7.1)

For simply supported beams, at least one-third of the main tension bars must extend over the support. 7.6

DEVELOPMENT OF HOOKED FRP BARS

For hooked bars the basic development length is given as a function of the FRP rebar ultimate strength and the concrete strength. For FRP rebars with ultimate strengths in the range 75 to 150 ksi (the typical range for glass FRP rebars), the development length of a hooked bar, lbhƒ, is given as lbhƒ ⫽

ƒƒu db 37.5 兹ƒc⬘

(ACI 440.1R-06:11-5)

and not less than 12db or 9 in. In addition, the tail length of the hooked bar, lthƒ, should be greater than 12db or 9 in., and the radius of the bend should not be less than 3db. Values of lbhƒ for FRP bars with strengths less than 75 ksi or greater than 150,000 ksi are given in ACI 440.1R-06. A photograph of hooks on the ends of No. 7 FRP bars is shown in Fig. 7.7.

7.8

DESIGN PROCEDURE TO DETAIL FRP BARS IN A BEAM

207

Figure 7.7 FRP short bars (J-hooks) with hooked ends.

As can be seen, the ‘‘long’’ leg of the bar is quite short. This is not because it has been cut to length. At the present time it is not actually possible to obtain long glass FRP bars with end hooks; they cannot be produced by the existing manufacturing technology. Only long straight bars or short pieces of bars with bends can be produced. These are commonly referred to as J-hooks. They are spliced to longitudinal bars at their ends, where a hooked anchorage is required, as shown in Fig. 4.1. This can signiﬁcantly crowd the end of the beam region and may lead to splitting. It is therefore recommended that the structural geometry be designed to enable straight FRP bars to be used wherever possible.

7.7

LAP SPLICES FOR FRP BARS

Tension lap splices for FRP rebars are based on recommendations for steel rebars and limited test data. ACI 440.1R-06 recommends that all FRP bar splices be designed as class B lap splices and have a length of 1.3ld.

7.8

DESIGN PROCEDURE TO DETAIL FRP BARS IN A BEAM

Step 1. Determine the bond-critical effective strength of the FRP main bar. The bond-critical effective strength of the FRP bar, ƒƒe, is a function of the embedment length available. This will depend on where along the length of the beam the nominal design moment is calculated. For a simply supported beam with the maximum moment at midspan (such as a uniformly loaded beam), the available embedment length will be half the beam span. Check to see that the bond-critical effective strength is more than that used

208

FRP REINFORCEMENT DETAILING

to determine the ﬂexural capacity for the beam (over- or underreinforced design). If it is not, the main reinforcement must be redesigned. Step 2. Determine the development length of the FRP main bars. Calculate the development length for the main bars. This depends on the bar bottom or side cover and bar spacing across the width of the member. The section details need to be fully designed to determine these numbers. This should have been done during the ﬂexural and shear design stages. The bend radii of the FRP stirrups (if needed) may have a big effect on this step. Step 3. Detail the bars and provide a list of FRP materials. Provide a longitudinal sketch of the concrete member showing the main bar lengths and stirrup details (if stirrups are required). Develop a list of FRP materials for the member designed. Identify each bar by length, size, and geometry. Provide the quantity of each bar type in a list of materials. Design Example 7.1: Detailing of FRP Bars in a Beam Assume that the two No. 6 main bars in the 7 ⫻ 12 in. beam in Design Example 5.1 are extended to the end of the span over the supports, which are 8-in.-wide CMU walls. Assume that a cover of 2db is required at the end of the beam. Detail the main bars. SOLUTION Step 1. Determine the bond-critical effective strength of the FRP main bar. To determine the bond-critical design strength of the FRP bar, ﬁrst ﬁnd the distance, C. The spacing calculation is based on a No. 3 stirrup with an inside radius of 3db, an outside clear cover of 1.125 in., and a bar clear spacing of 1.0 in. (discussed previously) In this case the distance to the closest bar is either (1) the distance to the side of the beam, A ⫹ B ⫹ C ⫽ 1.125 ⫹ 0.375 ⫹ 3(0.375) ⫽ 2.625, or (2) the distance to the bottom on the beam, 1.5 ⫹ 0.375 ⫹ 0.75/2 ⫽ 2.2, or (3) half the center-to-center spacing of the bars, (1.0 ⫹ 0.75)/2 ⫽ 0.875 (controls). The available length for embedment from the point of the maximum moment is half the beam length,

le ⫽

l 11(12) ⫽ ⫽ 66 in. 2 2

The bar location factor, ␣ ⫽ 1.0, since the bars are bottom bars.

PROBLEMS

209

C 0.875 ⫽ ⫽ 1.167 ⬍ 3.5 → OK db 0.75 ƒƒe ⫽ ⫽

兹ƒc⬘

␣

冉

13.6

兹4000

1.0

冉

冊

le C le ⫹ ⫹ 340 db d b d b

13.6

冊

66 0.875 66 ⫹ ⫹ 340 ⫽ 103,689 psi 0.75 0.75 0.75

⫽ 103.7 ksi ⬎ 72 ksi (ƒƒu)

Therefore, the bar is not bond critical, and the ﬂexural capacity determined previously for the beam can be achieved. If ƒƒe had been less than ƒƒu, the beam would have needed to be redesigned for ﬂexural capacity using the lower bar design strength. Step 2. Determine the development length of the FRP main bars. The beam is overreinforced and the stress in the bar at failure is ƒƒ ⫽ 57.06 ksi. The bar stress in the development length equation is the lesser of (1) the bond-critical strength, 103.6 ksi, (2) the bar design strength, 72 ksi, and (3) the bar stress at failure, 57.06 ksi. Therefore, use ƒƒr ⫽ 57.06 ksi. ld ⫽

␣(ƒƒr / 兹ƒc⬘) ⫺ 340

13.6 ⫹ C/db

db ⫽

(1.0)[57,060/ 兹4000] ⫺ 340 (0.75) ⫽ 28.6 in. 13.6 ⫹ 0.875/0.75

Check that the development length is less than that allowed for a simple support. Assume that la ⫽ 0. Since the bars extend over the support and they are in the bottom of the section, they are conﬁned and the length available for development is 1.3

Mn 0.65(436.6) ⫹ la ⫽ (1.3) ⫹ 0 ⫽ 79.2 in. ⬎ 28.6 in. → OK Vu 4.66

PROBLEMS 7.1 Determine the bond-critical effective FRP bar strength, ƒƒe, for the FRP bars listed in Table P7.1 for the embedment lengths speciﬁed. Assume that the bars are spaced at the minimum on-center bar spacing permitted (i.e., minimum of 1-in. clear spacing, or db) and that this controls the bar-edge spacing parameter, C.

210

FRP REINFORCEMENT DETAILING

TABLE P7.1 No. 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18

Bar Bond Stress and Development Length Analysis Bar Type No. No. No. No. No. No. No. No. No. No. No. No. No. No. No. No. No. No.

4 GFRP 6 GFRP 8 GFRP 10 GFRP 4 GFRP 6 GFRP 8 GFRP 10 GFRP 4 GFRP 6 GFRP 8 GFRP 10 GFRP 4 GFRP 6 GFRP 8 GFRP 10 GFRP 4 GFRP 4 GFRP

ƒ⬘c (psi)

Location

le

4000 4000 4000 4000 4000 4000 4000 4000 8000 8000 8000 8000 4000 4000 4000 4000 4000 4000

Bottom Bottom Bottom Bottom Bottom Bottom Bottom Bottom Bottom Bottom Bottom Bottom Top Top Top Top Bottom Bottom

20db 20db 20db 20db 40db 40db 40db 40db 20db 20db 20db 20db 20db 20db 20db 20db 20db 40db

7.2 Determine the required development length, ld, for the bars listed in Table P7.1 assuming they are used in underreinforced FRP reinforced beams and that they have sufﬁcient embedment length so as not to be bond critical. 7.3 Consider the GFRP-reinforced test beams (FRP1 and FRP2) shown in Fig. 4.1, whose load deﬂection results are shown in Fig. 5.1. The beams were reinforced with three No. 7 GFRP Aslan 100 main bars and No. 3 Aslan GFRP stirrups at 5 in. on center. The stirrups were two-part horizontal U shapes with inside corner radii of 3.25 in. (shown on the left side of Fig. 7.4). The beam had an 8 ⫻ 12 in. cross section and was fabricated with 5000-psi design strength concrete (5880-psi actual 28-day strength). The bottom and side clear covers were 1 in. The beam was 98 in. long and was loaded in four-point bending over a 90-in. span at its third points (i.e., the moment and shear spans all equal 30 in.). The failure mode of beam FRP 1 is shown in Fig. 6.1, and the failure mode of FRP 2 is shown in Fig. 5.4. As noted in the text, FRP 1 failed in shear, whereas FRP 2 failed in ﬂexure, due to concrete crushing. You are required to use the theory presented in the text to critically evaluate the results of the experiments on FRP 1 and FRP 2. (a) Determine the nominal moment and nominal shear capacities of the beams predicted and compare with the experimental results (note that Fig. 5.1 shows the total load on beam and that the deﬂection due to the beam self-weight is not included).

PROBLEMS

211

(b) Construct the load–deﬂection curves for the beams from zero to the maximum predicted load at 5-kip intervals. Plot the prediced load– deﬂection curves for the beams and compare these to the experimentally measured curves (plot the experimental curves approximately by taking measurements from Fig. 5.1). (c) Critically evaluate the results and comment on the ability of the theory to predict the beam behavior in the service load range and in the ultimate state (including the failure modes). Were the J-hooks required for the main bars? (d) Perform the same exercise for the steel-reinforced beams and comment on the accuracy of the predictions for the steel-reinforced beams. (The steel beams had closed loop No. 3 steel stirrups at 5 in. on center.) 7.4 Calculate the costs of the GFRP- and steel-reinforced beams in Problem 7.3. Assume uncoated steel (black steel) bars at a cost of $0.35 per pound. For concrete use $75 per cubic yard for 5000-psi design strength. For FRP bar costs, use data provided in the problem sections of Chapters 5 and 6 and interpolate if necessary (or obtain pricing from the bar manufacturer). Determine the strength/cost, stiffness/cost, and energy absorbed1 /cost ratios for the GFRP and steel beams. Compare the results. 7.5 Design a 28-ft-long two-span continuous FRP-reinforced beam having a rectangular cross section. Use 5000-psi concrete and Aslan 100 GFRP rebars (main bars, stirrups, and hooks if necessary). The beam depth is limited to 20 in. You are given the following design loads and serviceability limits: dead load 400 lb/ft, live load 900 lb/ft (20% sustained), maximum long-term deﬂection L/360. (a) Design the beam for ultimate (ﬂexure, shear) and service limit states (deﬂection control, crack width control, creep rupture control). Identify the failure modes of the beam. Explain your design choices where necessary. (b) Provide a bar layout diagram showing bar cutoffs and stirrup layout. Show cross sections in the positive moment spans and over the middle support. Provide a list of FRP rebar materials, giving the number, size, and length of each bar type and a small sketch of each bar. 7.6 Design a 75-ft-long continuous GFRP-reinforced beam having a rectangular cross section to support an overhead 10-ton gantry crane in a highly corrosive chemical plant. The continuous beam is supported on 10-in.-wide column brackets at 15 ft on center. The overhead crane

1 Assume that the energy absorbed by the beams is equal to the area under the load–deﬂection curves.

212

FRP REINFORCEMENT DETAILING

gantry weights 1000 lb and is 30 ft wide. The crane has a lift capacity of 10 tons (20 kips). The gantry travels along the FRP-reinforced concrete beams (typically called crane rails). The beams have an additional superimposed dead load of 50 lb/ft of mechanical equipment. Due to space limitations, the width of the beam is limited to 12 in. maximum. A durable 6000-psi concrete is speciﬁed. The maximum long-term deﬂection of the beam is limited to 0.20 in. according to the crane mechanical speciﬁcations. Design the crane rail. Determine the section size, the main and shear reinforcement, and detail the FRP reinforcing bars for the negative and positive moments. Check the FRP bars for longterm sustained stress and for fatigue stresses. Show a diagram of the beam over the six supports (brackets). Indicate where bars are terminated along the length, if required. Provide a bill of materials for the beam, listing the quantity, size, and type of all FRP rebars to be used to reinforce the beam. Explain all your design assumptions and justify your design decisions as necessary. SUGGESTED FRP-REINFORCED CONCRETE STRUCTURAL DESIGN PROJECTS The following design projects are suggested for students in a composites for construction design class. The types of projects selected are those in which the noncorrosive properties of FRP reinforcements are known to be beneﬁcial and could result in service life savings over traditional steel-reinforced concrete. The design project should preferably be done in groups of two or three students. Students should be given 4 to 6 weeks to compete the design project (which therefore needs to be assigned early in the semester). The ﬁnal deliverable should be a design proposal2 that includes the problem statement, scope, codes and speciﬁcations, loads, materials, design calculations, design drawings, and a cost analysis. A presentation of the design proposal should be given in class. It is recommended that the current conditions of the existing structure and any corrosion-related problems be discussed and that owners and designers be invited to form part of the project jury to obtain feedback from industry on the designs presented. 7.1 FRP-reinforced concrete pedestrian bridge. Design an FRP-reinforced concrete bridge to replace an existing pedestrian bridge/elevated walkway (originally concrete, steel, or timber). Students should scout the local area (campus, downtown, etc.) to ﬁnd a pedestrian bridge with 20to 40-ft spans and use this bridge as the basis for the design. If possible, the original plans of the structure should be obtained from the university

2

Items listed are at the discretion of the instructor.

SUGGESTED FRP-REINFORCED CONCRETE STRUCTURAL DESIGN PROJECTS

213

physical facilities department (or equivalent). Design the concrete slab and support beams (girders, stringers) as required, depending on the type of structural system used. Use the AASHTO Guide Speciﬁcation for Design of Pedestrian Bridges (1997) for loads and dynamic requirements or other applicable codes. 7.2 FRP-reinforced concrete retaining wall. Design an FRP-reinforced concrete retaining wall (or foundation wall) to replace an existing retaining wall. Students should scout the local area (campus, downtown, etc.) to ﬁnd a small retaining wall structure 8 to 12 ft high and use this wall as the basis for the design. If possible, obtain the original plans of the structure from the university physical facilities department (or equivalent). Design the wall and the foundation as required using FRP reinforcements. 7.3 FRP-reinforced concrete beams in a wastewater treatment plant. Visit your local wastewater treatment plant3 and identify any cast-in-place reinforced concrete structures (preferably beam and slab structures, which are usually near the settling tanks). Consult with the operator of the facility and discuss any corrosion-related problems at the facility. Redesign a concrete beam or ﬂat slab member using FRP reinforcements. 7.4 FRP-reinforced precast double T-beams. Prestressed and precast doubleT ﬂoor beams are frequently used in the construction of precast parking garages. Scout your local area and identify a parking structure of this type. Obtain typical plans and speciﬁcations for the double-T beams (available in textbooks and other resources). Redesign the nonprestressed reinforcement in the ﬂanges and the shear reinforcement in the webs of such a member using FRP-reinforced concrete. Be sure to address the issue of the steel ﬂange inserts (shear connectors) that are used to attach the ﬂanges together to create the ﬂoor diaphragm (typically, by on-site welding). Consider how to use FRP materials for this purpose.

3 The environmental engineering faculty may be able to be of assistance in recommending a local facility and contacts.

8 8.1

Design Basis for FRP Strengthening OVERVIEW

This chapter provides an introduction to the subject of FRP strengthening materials, systems, and methods for strengthening and retroﬁtting reinforced concrete structures such as beams, slabs, and columns. The properties of FRP strengthening systems are reviewed and their behavior under various loads is discussed. Since FRP strengthening systems are used both to increase the strength of reinforced concrete members and to increase their ductility, the subject of strengthening is more complex than that of reinforcing with FRP rebars. To apply a strengthening system to a concrete member, the surface must be suitably prepared. This important aspect of strengthening of concrete structures is not covered in this book, as it is not directly related to the design of the strengthening system but rather, to the constructability. It is assumed that the reader is familiar with these procedures.1 Part of a strengthening design often includes evaluation of the current strength of an existing structure. Often, the original plans are no longer available, and the structure may have deteriorated since its original construction. This can present one of the most challenging engineering aspects of designing a strengthening system. Determination of the existing capacity of a deteriorated concrete structure is not covered in this book. In this chapter we describe the basis for the design of concrete members strengthened with FRP materials. This basis is in accordance with the American Concrete Institute publication ACI 440.2R-02, Guide for the Design and Construction of Externally Bonded FRP Strengthening Systems for Strengthening Concrete Structures (ACI, 2002). This document is compatible with ACI publication ACI 318-99, Building Code Requirements for Structural Concrete and Commentary (ACI, 1999). It is very important to note that the current ACI FRP strengthening design guide is not compatible with ACI 31805 (or ACI 318-02) provisions and is not compatible with ASCE 7-02 (ASCE, 2002) load factors. In particular, the load factors used with ACI 440.2R-02 are the ‘‘old’’ ACI load factors, the most common of these being 1.4 for the

1

See Chapter 2 for discussion and guidance on this topic.

214

Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

8.2

INTRODUCTION

215

dead load and 1.7 for the live load. The resistance factors presented in what follows for the design of FRP strengthening systems must therefore be used only with the 1.4 and 1.7 load factors.2 Throughout this chapter and the chapters that follow that describe in detail the procedures for the design of concrete structures with FRP strengthening systems, it is assumed that the reader has reasonable familiarity with ACI 318-99 and is familiar with the design of concrete beams and slabs reinforced with conventional steel reinforcing bars. The equations and examples that follow use U.S. standard units since these are the familiar units for design in the United States, where the ACI codes are mainly used.

8.2

INTRODUCTION

Fiber-reinforced-plastic (FRP) reinforcing systems for strengthening structurally deﬁcient concrete structural members and for repairing damaged or deteriorated concrete structures have been used since the mid-1980s. The ﬁrst applications involved beams strengthened to increase their ﬂexural capacity using high-strength lightweight ﬁber-reinforced epoxy laminates bonded to the sofﬁts of the beams (e.g., Meier and Kaiser, 1991; Saadatmanesh and Ehsani, 1991; An et al., 1999; Triantaﬁllou et al., 1992; Meier, 1995). The method is a modiﬁcation of the method using epoxy-bonded steel plates to strengthen concrete beams which has been in use since the mid-1960s. The FRP systems were shown to provide signiﬁcant beneﬁts over the steel plates in constructibility and durability. Work was conducted on strengthening of concrete columns to enhance their axial capacity, shear capacity, and ductility, primarily for seismic loadings (e.g., Fardis and Khalili, 1981; Katsumata et al., 1988; Priestley et al., 1992; Seible et al., 1997). This method is a modiﬁcation of one using steel jackets to strengthen concrete columns. This was followed closely by work on shear strengthening of beams (e.g., Chajes et al., 1995; Khalifa et al., 1998; Triantaﬁllou, 1998). A review of the state of the art on the subject can be found in Bakis et al. (2002) and Teng et al. (2001). The method has also been used to strengthen masonry and timber structures; however, applications of this type are not covered in this book. In recent years a variant of the FRP strengthening method called the nearsurface-mounted (NSM) method has been developed. In this method the FRP strip is adhesively bonded into a slot (or groove) that is saw-cut to a shallow depth [0.5 to 1.0 in. (13 to 25 mm)] in the concrete. Current FRP strengthening systems for concrete fall into two popular types. One type consists of factory-manufactured (typically, unidirectional pul-

2 ACI Committee 440 is currently in the process of revising ACI 440.2R to be compatible with ACI 318-05. The reader should keep this in mind when using future editions of the ACI guide in conjunction with this book.

216

DESIGN BASIS FOR FRP STRENGTHENING

truded) laminates (also known as strips or plates) of carbon- or glassreinforced thermosetting polymers (epoxy or vinylester) bonded to the surface of the concrete using an epoxy adhesive. The manufactured laminates typically have a volume fraction of ﬁbers in the range 55 to 65% and are cured at high temperatures (typically, ⬎300⬚F) but bonded in the ﬁeld at ambient temperatures. The other type consists of layers (or plies) of unidirectional sheets or woven or stitched fabrics of dry ﬁbers (glass, carbon, or aramid) that are saturated in the ﬁeld with a thermosetting polymer (epoxy or vinylester) which simultaneously bonds the FRP laminate (thus formed) to the concrete. These formed-in-place or laid-up FRP systems typically have a ﬁber volume fraction between 20 and 50% and are cured at ambient temperatures in the ﬁeld. Figure 8.1 shows a concrete beam with a bonded precured strip, and Fig. 8.2 shows a concrete beam with a laid-up sheet. As reviewed in Chapter 1, a number of design guides and national standards are currently published that provide recommendations for the analysis, design, and construction of concrete structures strengthened with FRP materials (AC 125, 1997; FIB, 2001; JSCE, 2001; ACI, 2002; TR 55, 2004). Manufacturers of FRP strengthening systems for concrete typically provide their own design and installation guides for their proprietary systems. Since the performance of the FRP strengthening system is highly dependent on the adhesive or saturating polymer used, the preparation of the concrete surface prior to application of the FRP strengthening system, and the ﬁeld installation and construction procedures, manufacturers typically certify ‘‘approved contractors’’ to ensure that their systems are designed and installed correctly. In addition, code guidance is provided to ensure that FRP strengthening systems are installed appropriately (AC 187, 2001; ACI, 2002; TR 57, 2003; NCHRP, 2004). Research into the use of FRP strengthening systems for concrete structures has been the focus of intense international research activity since the early

Figure 8.1 Beam with a bonded precured FRP strip.

8.3

PROPERTIES OF FRP STRENGTHENING SYSTEMS

217

Figure 8.2 Beam with a laid-up FRP sheet.

1990s. A biannual series of symposia entitled ‘‘Fiber Reinforced Plastics in Reinforced Concrete Structures’’ (FRPRCS) has been the leading venue for reporting and disseminating research results. Recent symposia in the series, dating back to 1993, were held in Singapore in July 2003 (Tan, 2003) and in Kansas City in November 2005 (Shield et al., 2005).

8.3

PROPERTIES OF FRP STRENGTHENING SYSTEMS

Carbon ﬁber–reinforced epoxy laminates (or strips) are most commonly used in the adhesively bonded products. Depending on the type of carbon ﬁber used in the strip, different longitudinal strengths and stiffness are produced. Strips are typically thin [less than 0.100 in. (2.5 mm)] and are available in a variety of widths [typically, 2 to 4 in. (50 to 100 mm)]. Since the strips are reinforced with unidirectional ﬁbers, they are highly orthotropic and have very low properties in the transverse and through-the-thickness directions. Narrow strips and small-diameter FRP rebars are also used in the NSM strengthening method. Manufacturers typically only report properties in longitudinal directions and report very few data on physical properties. The strips are bonded to the concrete with a compatible adhesive that is supplied by the strip manufacturer. Typical properties of strips are given in Table 1.2. It is important to note that the properties shown for the strips are the properties of the FRP composite, not the properties of the ﬁbers alone. In the types of products for FRP strengthening that consist of dry ﬁbers in sheet or fabric form with compatible polymer-saturating resins, there is a greater array of products available that depend on ﬁber type and sheet or fabric architecture. In this group of products, a unidirectional highly ortho-

218

DESIGN BASIS FOR FRP STRENGTHENING

tropic carbon ﬁber tow sheet is produced by a number of manufacturers and is often used in strengthening applications. The individual carbon tows in the sheet are held together by a very light polymeric binder (or a light stitching), are supplied on a wax paper backing, and have a typical weight of –21 oz/ft2 (⬃150 g/m2). Sheets are typically 10 to 40 in. (250 to 1000 mm) wide and may be applied in multiple layers with different orientations. Common fabric materials in this group are woven or stitched glass or carbon ﬁber materials, typically consisting of 12 to 24 oz/yd2 (360 to 720 g/m2) materials with a variety of weaves, which can give the fabric properties from highly orthotropic to square symmetric. Carbon ﬁber tow fabrics and hybrid fabrics (with more than one ﬁber type) are also available. Fabrics are typically much thicker than tow sheets and can also be used in multiple layers. Because of the wide variety of products available and their different thicknesses, it is not easy to compare their properties directly. In addition, the ﬁbers must be used with a compatible resin system applied with a controlled volume fraction in order to achieve an FRP composite with measurable properties. In the case of sheet and fabric materials, manufacturers typically report the mechanical properties of the dry ﬁbers and the thickness (or area) of the ﬁbers. It is important to note that when reported in this fashion, the properties are not the properties of the FRP composite. Also, if the fabric has bidirectional or multidirectional ﬁbers, only those ﬁbers in the direction that is to be strengthened must be used to determine the ﬁber area for strengthening. Properties of some commonly available unidirectional ﬁber sheet and ﬁber fabric materials are listed in Table 1.3. The performance of the FRP strengthening system is highly inﬂuenced by the properties of the adhesive layer in the case of the bonded strip and by the properties of the saturating polymeric resin in the case of the sheets and fabrics. The interface between the FRP composite and the concrete substrate transfers the loads from the concrete to the FRP composite. In the case of ﬂexural, shear, or axial tensile strengthening, this load transfer is primarily in shear, and the properties and quality of the interface bond between the FRP composite and the concrete effect load transfer into the FRP strengthening system. Such applications are termed bond-critical applications. In the case of axial compressive strengthening, where the role of the strengthening system is to conﬁne the lateral expansion of the cracked concrete, the interface bond is not as critical as long as the FRP strengthening system is in intimate contact with the concrete and is wrapped around the concrete continuously so as to provide a required conﬁning pressure. Such applications are termed contact critical. It is important to note, however, that in either type of system the polymer resin still plays a critical role in the FRP composite in transferring load to the ﬁbers and protecting the ﬁbers. A poorly applied sheet or fabric having a low ﬁber volume fraction (⬍20%) and a relatively thick uneven thickness polymer layer with a large void content (⬎3%) will not provide a durable FRP strengthening system, even though the amount of ﬁber placed in the wrap may be according to design requirements.

8.4

DESIGN BASIS FOR FRP STRENGTHENING SYSTEMS

219

Since most FRP strengthening systems depend on curing of polymer adhesives or resins at ambient temperature, the cured glass transition temperatures of these components may be quite low [120 to 180⬚F (⬃50 to 80⬚C)]. Since the effectiveness of the strengthening system depends to a great degree on the stiffness of the adhesive or resin used to bond the FRP composite to the concrete, an FRP strengthening system can become unserviceable at even moderately high temperatures (⬃100⬚F). In certain cases where the ﬁbers are sufﬁciently anchored away from the region subjected to the high temperature, the FRP strengthening system may still be effective. Designers should always be aware of the glass transition temperature of the FRP composite or adhesive they are using in a design. In the event of a ﬁre, the integrity of an FRP strengthening system may be severely compromised in a very short time unless it is protected by insulation. This is currently the subject of ongoing research studies (Bisby et al., 2005).

8.4

DESIGN BASIS FOR FRP STRENGTHENING SYSTEMS

In what follows the design basis of the American Concrete Institute presented in ACI 318-99 and ACI 440.2R-02 are followed with respect to design philosophy and load and resistance factors for design.3 Similar design bases, conforming to the limit states design procedure, are recommended by many standards organizations and professional organizations for FRP-reinforced concrete (JSCE, 2001; FIB, 2001; CSA, 2002; TR 55, 2004). 8.4.1

Resistance Factors

For the design of concrete members with FRP strengthening systems, the ACI 440.2R.-02 recommends use of the traditional resistance factor, , which is a function of the intended use (or the dominant stress) of the structural member. The resistance factor is applied to the nominal capacity of the member to obtain the factored capacity for use in the strength design method. For FRP strengthening systems, ACI 440.2R-02 also recommends the use of a strength reduction factor (similar to a material partial safety factor), ƒ, which is applied to the FRP system only. The strength reduction factor is applied to the stress in the FRP material to obtain the nominal capacity of the structural member. Consequently, the factored (ultimate) capacity of a concrete member depends on the member resistance factor and on the FRP strength reduction factor. The following factors are provided by ACI 440.2R-02 for design of FRP-strengthened concrete structures.

3 The ultimate strength design procedure, a load and resistance factor design (LRFD) procedure, is followed by ACI 440.2R-02; however, at this time, resistance factors are not probabilistically based. Load factors are those recommended by ACI 318-99 for all concrete structures.

220

DESIGN BASIS FOR FRP STRENGTHENING

Flexural capacity (for tensile strengthening) (ACI 440.2R-02:9-5):

冦

for a ductile failure when the member fails after steel yielding and s ⬎ 0.005 for a brittle failure when the member fails prior to steel yielding and s ⬍ sy for a semiductile failure when the member fails after steel yielding and s ⬎ sy but s ⬍ 0.005

0.9

⫽

0.7 0.7 ⫹

0.2(s ⫺ sy) 0.005 ⫺ sy

ƒ ⫽ 0.85 for FRP bond-critical designs

Shear capacity (for shear strengthening) (ACI 318-99): ⫽ 0.85 ƒ ⫽

再

0.85 0.95

for FRP bond-critical designs for FRP contact-critical designs

Axial compressive capacity (for conﬁnement) (ACI 318-99): ⫽

再

0.75 0.70

for steel spiral reinforcement for steel tied reinforcement

ƒ ⫽ 0.95 for FRP contact-critical designs

8.4.2

Guaranteed Properties

The tensile strength of an FRP strengthening system (called the ultimate tensile strength) and tensile strain to failure of FRP strengthening systems (called the ultimate rupture strain) are deﬁned by ACI 440.2R-02 as the mean minus three standard deviations of a minimum of 20 test samples. The ultimate strength, ƒ* * , are expected to be supplied by ƒu, and ultimate rupture strain, ƒu the manufacturer. FRP strengthening systems must be tested according to the procedures detailed in in ACI 440.3R-04 (see Chapter 3 for details). 8.4.3

Environmental Effects

The design strength, ƒƒu, and design failure strain, ƒu, are obtained from the ultimate strength and ultimate rupture failure strain by multiplying them by an environmental reduction factor, CE, which depends on the type of FRP system used and the type of intended service of the structure, as shown Table 8.1. The FRP system tensile modulus (also called the speciﬁed tensile modulus), Eƒ, measured in the axial direction of the ﬁber is deﬁned as the average

8.4

DESIGN BASIS FOR FRP STRENGTHENING SYSTEMS

221

TABLE 8.1 Environmental Reduction Factors for FRP Strengthening Systems per ACI 440.2R-02

Exposure Condition Interior (FRP system in an indoor environment) Exterior (FRP system exposed to the elements) Especially aggressive environments (chemical exposure, wastewater)

FRP System Type

Environmental Reduction Factor, CE

Carbon–epoxy Glass–epoxy Aramid–epoxy Carbon–epoxy Glass–epoxy Aramid–epoxy Carbon–epoxy Glass–epoxy Aramid–epoxy

0.95 0.75 0.85 0.85 0.65 0.75 0.85 0.50 0.70

modulus of the test data in accordance with ACI 440.3R-04. No reduction to the measured modulus is taken, for either statistical or environmental reasons. The environmental reduction factor accounts for the fact that even though FRP systems are not susceptible to conventional electropotential corrosion that affects metallic materials, they can nevertheless deteriorate in various chemical environments, both alkaline and acidic. This deterioration is accelerated at elevated temperatures. Glass ﬁbers are especially susceptible to corrosion in alkaline and neutral solutions, due to leaching of the ﬁber (Bank et al., 1995b). Aramid ﬁbers do not leach like glass ﬁbers but are known to absorb moisture and swell, leading to loss of mechanical and physical properties. Carbon ﬁbers are the most chemically inert and are generally recommended when extreme exposure to chemical aqueous environments is anticipated. In addition, the polymer matrix is also susceptible to deterioration in different chemical environments. However, carbon ﬁbers are not electrochemically inert and can cause a phenomenon known as galvanic corrosion to occur when they are in contact with metals, as discussed in Chapter 1. This is not likely to be a problem in FRP-strengthened concrete since the FRP does not come into contact with the steel reinforcing bars. However, if metallic anchor bolts or plates are used to anchor a carbon FRP system, this can be a consideration. 8.4.4

Limits of Strengthening

Although ﬂexural strengthening over 100% of original design strength is possible to achieve, ACI 440.2R-02 limits the amount of strengthening to prevent catastrophic failure of the concrete member in the event of loss of, or damage to, the strengthening system (due to vandalism or environmental degradation). The ACI recommends that the strengthened member still have sufﬁcient orig-

222

DESIGN BASIS FOR FRP STRENGTHENING

inal factored capacity (i.e., discounting the strengthening system) to resist a substantial portion of the future load on the strengthened member, given as 1.2D ⫹ 0.85L

(8.1)

where D is the dead load effect4 and L is the live load effect on the strengthened structure. To account for ﬁre, additional restrictions are placed on the factored capacity of the FRP-strengthened structured. In this case the portion of the new load on the strengthened member is given as 1.0D ⫹ 1.0L

(8.2)

The maximum permissible strengthening of a section is a function of the ratio of future live load to future dead load on the strengthened beam. If the original factored moment capacity of a beam, (Mn)orig, is known the maximum service moment due to the future dead load, mDL(max), and the maximum service load moment due to the future live load, mLL(max), can be obtained from 1.2mDL(max) ⫹ 0.85mLL(max) ⫽ (Mn)orig

(8.3)

Given the load ratio on the strengthened beam, R⫽

mLL(max) mDL(max)

(8.4)

gives5 (Mn)max ⫽ (Mn)orig

1.4 ⫹ 1.7R 1.2 ⫹ 0.85R

(8.5)

and the maximum permissible percentage increase in factored moment capacity is %max ⫽

0.2 ⫹ 0.85R ⫻ 100 1.2 ⫹ 0.85R

(8.6)

When a concrete member is strengthened to increase its capacity in a selected mode (e.g., ﬂexure) the member must be checked to ensure that the capacities in other failure modes (e.g., shear) are not exceeded. If this is the case, the 4

Such as bending moment, shear force, and axial force. This does not necessarily mean that the resistance factor, , will be the same for the original and the strengthened sections.

5

8.6

FRP STRENGTHENING SYSTEM AREA CALCULATIONS

223

strengthening should be decreased or the secondary capacity needs to be enhanced with its own strengthening system. 8.4.5 Limits on Stresses in FRP Strengthening Systems at Service Loads The stress level in the FRP at service loads is limited by the creep rupture properties of different FRP materials and by their fatigue resistance. ACI 440.2R-02 limits the service-level stresses in an FRP strengthening system in strengthened reinforced concrete members according to the ﬁber type used in the strengthening system (Table 8.2). 8.4.6

Compression Strengthening in Flexural Members

At this time, FRP systems should not be used as compression strengthening of ﬂexural members. If FRP strengthening systems are placed in the compression zones of ﬂexural members, they should not be assumed to carry any compression load, and they should be adequately attached, to prevent local bucking, which could lead to premature failure. 8.5

DEFLECTIONS IN FRP-STRENGTHENED STRUCTURES

For deﬂections in ﬂexural members where stresses are in the service range, the contribution of the FRP strengthening system is typically small. Flexural deﬂections in the service range can be estimated by use of an effective composite-section second moment-of-area (Ie) analysis where the tensile contribution of the FRP is added to the contribution of the steel reinforcing. In the inelastic range after the primary reinforcing steel has yielded, the contribution of the FRP strengthening to the postyield stiffness can be considerable and should be accounted for in inelastic analysis. 8.6

FRP STRENGTHENING SYSTEM AREA CALCULATIONS

It is extremely important to note that the method of determining the tensile force resultant in an FRP strengthening system depends on the type of system TABLE 8.2 Maximum Permissible Service Load Stress in an FRP Strengthening System Stress Type Sustained stress plus maximum stress under cyclic load

Glass FRP

Aramid FRP

Carbon FRP

0.20ƒƒu

0.30ƒƒu

0.55ƒƒu

224

DESIGN BASIS FOR FRP STRENGTHENING

used. In bonded strip systems, the ultimate force is obtained from the strength of the FRP composite and the gross cross-sectional area of the strip. In dry ﬁber systems, the ultimate force is obtained from the strength of the ﬁbers and the thickness of the net area of the ﬁbers. The designer must know if the strength (and stiffness) reported for an FRP strengthening system is for the FRP composite (gross cross section) or for the ﬁbers alone (net ﬁber cross section). Both methods of calculation are permitted at this time by the ACI 440.2R-02 guide.

PROBLEMS 8.1 Visit the following FRP strengthening system manufacturers’1 Web sites and request or download copies of their FRP precured strip, sheet, or fabric property speciﬁcation sheets. These will be needed for solving the problems that follow. Sika (SikaWrap Hex fabrics and Carbordur strips): www. sikaconstruction.com Fyfe Company (Tyfo fabrics and strips): www.fyfeco.com Degussa (WaboMBrace sheets and strips): www.wbacorp.com VSL (V-Wrap): www.vsl.net Hughes Brothers (Aslan 400 strips): www.hughesbros.com S&P Clever Reinforcement Company (S&P sheets and laminates): www.sp-reinforcement.ch 8.2 For the following FRP fabric strengthening systems, determine the ACI 440.2R-2 nominal design strength, ƒƒu, the nominal design failure strain, ƒu, and the longitudinal modulus, Eƒ, when the strengthening system is used in an exterior nonaggressive environment. Also indicate the thickness of a single ply of this system, the weight of the fabric in oz/yd2, and whether the design is based on the laminate properties or on the ﬁber properties. Attach copies of the speciﬁcation sheets to your homework. (a) SikaWrap Hex 100G with Sikadur Hex 100 epoxy. (b) Tyfo SEH 51 with Tyfo S epoxy. (c) WaboMbrace CF530 with WaboMbrace epoxy encapsulation resin. (d) VSL V-Wrap C200 with epoxy material type 1. (e) S&P C-sheet 640 with S&P resin epoxy 55/50.

1 No endorsement of the manufacturers listed is implied. The reader is free to choose any manufacturer’s products to use in the examples that follow, and is encouraged to collect similar data for locally available strengthening products.

SUGGESTED ACTIVITIES

225

8.3 For the following FRP precured strip strengthening systems, determine the ACI 440.2R-02 nominal design strength, ƒƒu, the nominal design failure strain, ƒu, and the longitudinal modulus, Eƒ, when the strengthening strip is used in an interior environment. Also, indicate the available thicknesses and widths of a single strip of this system and the adhesives that are speciﬁed by the manufacturer for use with this strip. Attach copies of the speciﬁcation sheets to your homework. (a) Sika Carbodur laminates (b) Tyfo UG composite laminate strip system (c) Aslan 400 laminates (d) S&P laminates CFK 150/2000 8.4 Consider equation (8.6), which gives the maximum permissible ﬂexural strengthening of a member based on its original capacity and the future live load/dead load ratio. Use this equation and show graphically the maximum permissible strengthening as a function of the future live load/ dead load ratio. Plot a graph of the maximum percentage increase in strengthening permitted in an FRP-strengthened section as a function of the live load/dead load ratio from 0.5 to 5. Discuss what can be learned from this graph about the types of structures that are most beneﬁcial to strengthen with FRP materials. 8.5 Develop an equation in a form similar to equation (8.6) that can be used to determine the maximum strengthening permissible when an FRPstrengthened structure needs to be designed for possible ﬁre loads [per equation (8.2)]. Plot a graph of the maximum percentage increase of strengthening permitted in this type of FRP-strengthened section as a function of the live load to dead load ratio from 0.5 to 5, and comment on the results. SUGGESTED ACTIVITIES 8.1 Obtain small (4 ⫻ 4 in. to 6 ⫻ 6 in.) swatches of FRP strengthening sheets and fabrics. Request samples from the vendors of the FRP strengthening systems in Problem 8.1 or obtain samples from regular suppliers of ﬁber fabrics (glass and carbon, primarily) in other parts of the composites industry (see Problem 2.1). If necessary, small sample swatches can be purchased. Ideally, obtain tow sheets or fabrics ranging from about 5 to 24 oz/yd2 (150 to 720 g/m2). Try to obtain thin tow sheets, woven fabrics, and stitched fabrics. (a) Determine the areal weight of the fabrics received and examine the structure of the weave or stitching. (b) Practice handling the fabric materials: folding, cutting, and rolling. Write a two-page report describing the properties and the fabrics

226

DESIGN BASIS FOR FRP STRENGTHENING

you have investigated and describing the difference between tow sheets, woven fabrics, and stitched fabircs. 8.2 Obtain small (4- to 6-in.) lengths of precured unidirectional carbon ﬁber–reinforced FRP strengthening strips (or laminates). Request samples from the vendors of the FRP strengthening systems listed in Problem 8.1. (a) Examine the strip for ﬂatness and note any lengthwise or widthwise curvatures. (b) Experiment with various hand and power saws to cut the strip in the longitudinal and transverse directions. Consult manufacturers’ recommendations on how to cut strips in the ﬁeld. (c) Manually bend (in an attempt to break) a short longitudinal strip (about 6 in. long) and a short transverse strip (about 2 in. long). Notice the difference in ﬂexural behavior in the two directions. Write a brief report on your oversvations. 8.3 Download a copy of the 2004 National Cooperative Highway Research Program (NCHRP) report (number 514), entitled Bonded Repair and Retroﬁt of Concrete Structures Using FRP Composites from http:// trb.org/. Write a six-page double-spaced essay that describes what you learned from the report about repair and strengthening of concrete with FRP composites.

9 9.1

FRP Flexural Strengthening OVERVIEW

This chapter deals with the design and strengthening of reinforced concrete ﬂexural members, such as beams, slabs, walls, and columns with precured FRP strips and plates, and laid-up FRP sheet and fabric systems. Only nonprestressed concrete ﬂexural members that are reinforced with conventional steel reinforcing bars are considered. The design procedures presented in this chapter follow ACI 440.2R-02, which is compatible with ACI 318-99. For the purposes of this chapter, it is assumed that the reader is familiar with both the fundamentals and details of the design of concrete ﬂexural members reinforced with conventional steel reinforcing bars. The examples presented in this chapter and those to follow are based on the examples in ACI 440.2R-02 and are intended to allow the reader to analyze these examples critically and to consider design alternatives not presented in the ACI guide. The material in the chapter covers strength design and serviceability design. For pedagogical and practical reasons, these are separated into two parts. In reality, strength and serviceability design are not separate and must be considered as equally important limit states. When dealing with FRP materials, this is always important to keep in mind.

9.2

INTRODUCTION

Flexural strengthening of reinforced concrete beams, slabs, walls, and columns is achieved by attaching an FRP strengthening system (bonded strip or saturated dry fabric) to the tension face (or a portion thereof) of a ﬂexural member to increase the effective tensile force resultant in the member and thereby increase the moment capacity of the member.1 Typical applications are shown in Figs. 9.1 and 9.2. Flexural strengthening with FRPs is analogous to adding steel strengthening strips (or plates) to the tension face member. However, two fundamental differences exist. First, the FRP strengthening system behaves in a linear elastic fashion and does not yield, and second, the FRP strengthening system

1 In what follows, only singly reinforced rectangular sections are discussed. For doubly reinforced and nonrectangular sections, similar derivations are possible.

Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

227

228

FRP FLEXURAL STRENGTHENING

Figure 9.1 Flexural (and shear) strengthening of a reinforced concrete beam. (Courtesy of Fyfe Company.)

Figure 9.2 Flexural strengthening of a reinforced concrete slab. (Courtesy of Sika Corporation.)

9.2

INTRODUCTION

229

is more susceptible than steel plate systems to detachment (debonding or delamination) failures. Since the steel plates themselves will yield at a similar strain to the internal steel reinforcing, the stress level in the steel strengthening system is limited and epoxy-bonded steel plates are typically anchored with steel bolts at their ends (and also often along their length). In FRP strengthening with FRP systems having ultimate tensile strengths exceeding 300 ksi and stiffness exceeding 40 Msi (see Tables 1.2 and 1.3), the stress level in the FRP can be signiﬁcantly higher than that in steel strengthening systems. Consequently, the strength enhancement provided by the FRP can be much greater than that of steel systems. If the internal steel reinforcing in the strengthened RC beam yields before the FRP strengthening system fails, which is desirable, the FRP system will ‘‘pick up’’ the load beyond the yield load of the internal steel. The large tensile forces in the FRP strengthening systems and the large post-steel-yielding deﬂections in the member can lead to the FRP strengthening system delaminating (or debonding) from the concrete. Therefore, the maximum stress and strain in the FRP usually cannot be attained, and they are limited in the design procedure to prevent this type of failure from occurring. A typical load–midspan deﬂection plot of an FRP strengthened concrete beam is shown in Fig. 9.3 (Alkhrdaji et al., 2000). Initially, the beam behaves like a conventional reinforced concrete beam with internal steel reinforcing bars carrying the majority of tensile force in the section. At some point (generally seen as a change in slope of the load–deﬂection curve) the internal steel yields and cannot carry additional tensile force. This additional tensile force is carried by the FRP system and an increase in the load capacity of

60,000

Load (lb)

40,000

20,000

Experimental (after strengthening) Experimental (before strengthening) 0 0

2

4

6

8

Deflection (in.)

Figure 9.3 Load–deﬂection response of an FRP-strengthened concrete beam. (Courtesy of A. Nanni and R. Mayo.)

230

FRP FLEXURAL STRENGTHENING

the member is obtained. Eventually, the FRP-strengthened beam fails. The various failure modes are discussed below. Notwithstanding the problem of debonding noted previously, the analysis and design of FRP ﬂexural strengthening systems according to the ACI 440.2R-02 guide is based on the traditional assumptions of reinforced concrete design. These assumptions are compatibility of strain through the depth of the section, and equilibrium of the tension and compression force resultants at any point along the length of the member. This implies that there is no relative axial displacement (or slip) between the FRP system and the concrete (i.e., axial strain compatibility exists at the interface) and that the adhesive layer does not deform in shear when it transfers the forces from the concrete to the FRP strengthening system. These assumptions are assumed to hold even after the internal steel has yielded and the concrete cover layer between the tensile steel and the FRP system is signiﬁcantly cracked. Strengthening of members in ﬂexure is achieved only if there is sufﬁcient additional compressive capacity in the concrete to allow for the increase in internal moment in the section. Therefore, ﬂexural strengthening is most suitable for concrete members that are lightly to moderately reinforced, having steel reinforcement in the range 20 to 40% of the balanced steel (unstrengthened) reinforcement ratio. This reinforcement ratio is not uncommon in reinforced concrete members, especially in older structures. In addition, strengthening can be achieved with bonded FRP strengthening systems only if the concrete in the bottom cover layer to which the FRP system is bonded is in suitable condition to permit transfer of the forces into the section above the internal reinforcing. In many older reinforced concrete members in which the internal steel reinforcing has corroded and the cover concrete has spalled, the cover concrete is generally not in good enough condition to perform this function and the concrete needs to be repaired before the FRP strengthening system can be applied.

9.3 FLEXURAL CAPACITY OF AN FRP-STRENGTHENED MEMBER To begin with, it is important to understand that the key to determining the moment capacity of an FRP ﬂexural strengthened member is to understand the ﬂexural failure modes of the system and to account for them in the design process.2 These include rupture of the FRP strengthening system, detachment of the FRP strengthening system (due to a variety of delamination or de-

2 As noted previously, ﬂexural strengthening can cause the strengthened member to be vulnerable to shear failure. Shear strengthening and shear failure modes of transversely loaded ﬂexural members are discussed in Chapter 10.

9.3.

FLEXURAL CAPACITY OF AN FRP-STRENGTHENED MEMBER

231

bonding modes), or compressive failure of the concrete (Arduini and Nanni, 1997; Spadea et al., 1998). All of these modes can occur either before or after the internal steel has yielded. The most desirable mode of failure is concrete compressive failure after the internal steel has yielded with the FRP strengthening system still attached. This is often difﬁcult to achieve, and the mode of FRP detachment (or less frequently, rupture) at large deﬂections after the internal steel has yielded but prior to the concrete crushing often occurs. The strengthening system can detach in a number of ways. The system can delaminate from the concrete substrate (due to failure in the concrete, the adhesive layer, or in the FRP laminate itself) either at the ends (due to high peeling and shear stresses) or in the interior of the beam due to ﬂexural and shear cracks in the beam at large deﬂections (Buyukozturk et al., 2004). The various failure modes are shown schematically in Fig. 9.4. Analytical methods to predict the various detachment (also known as delamination or debonding) failure modes are still not fully developed,3 and the ACI guide does not provide an explicit procedure to determine whether or not a detachment failure will occur. Instead, the ACI guide limits the strain permitted in the FRP strengthening system to ensure that none of the detachment failure modes [modes (d) to (g) in Fig. 9.4] is likely to occur. The maximum effective tensile strain in the FRP strengthening system, ƒe, is obtained by multiplying the design ultimate rupture strain, ƒu, by an empirically obtained bond-dependent coefﬁcient, m, which is a function of the stiffness and thickness of the FRP system and deﬁned as

冦

冉 冉

冊

nEƒtƒ 1 1⫺ ⱕ 0.90 60ƒu 2,000,000 m ⫽ 1 500,000 ⱕ 0.90 60ƒu nEƒtƒ

冊

for

nEƒtƒ ⱕ 1,000,0000 lb/in.

for

nEƒtƒ ⬎ 1,000,000 lb/in. (ACI 440.2R-02:9-2)

where n is the number of layers (or plies) of FRP strips or sheets or fabrics, Eƒ the longitudinal tensile modulus of the FRP composite in the case of strips or the longitudinal modulus of the ﬁbers in the strengthening direction in the case of sheets or fabrics, and tƒ the thickness of an individual strip in the case of FRP strips or the net thickness of the ﬁbers in a single sheet or fabric in the case of sheets or fabrics. Since m must be less than 0.9, the strain in the FRP is never allowed to reach the ultimate rupture strain in the ACI design procedure. Therefore, theoretically, the failure mode of FRP rupture [mode (a) in Fig. 9.4] can never 3 See Teng at al. (2001) for a detailed discussion of existing analytical models to predict the loads at which detachment will occur.

232

FRP FLEXURAL STRENGTHENING

(a)

(b)

FRP rupture

Concrete crushing

(c) Shear crack

(d)

High-stress zone

Crack propagation

(e)

High-stress zone

Crack propagation Load

(f) Crack High-stress zone Crack propagation

Load

(g) High-stress zone

Crack

Crack propagation

Figure 9.4 Failure modes of ﬂexurally strengthened beams. (From Teng et al., 2001, with permission from John Wiley & Sons.)

occur, according to the ACI. According to the ACI 440.2R-02 guide, only two failure modes are assumed to occur for the purposes of design calculations: compressive failure of the concrete (called mode 1 in what follows) and failure of the FRP strengthening system (called mode 2 in what follows). For each of these design failure modes, the stress in the FRP, the internal steel, and the concrete are required to determine the ultimate bending capacity of the section.

9.3.

9.3.1

FLEXURAL CAPACITY OF AN FRP-STRENGTHENED MEMBER

233

Stress in the FRP Strengthening System

Concrete compression failure can occur either after (called mode 1a) or before (called mode 1b) the internal steel has yielded with the FRP system intact and still attached. This is the failure mode of an overreinforced strengthened concrete beam. In this case, the effective strain in the FRP at failure is obtained from the assumed linear variation of the strain through the depth of the section shown in Fig. 9.5. The effective strain in the FRP is given as h⫺c ⫺ bi c

ƒe ⫽ cu

(ACI 440.2R-02:9-3)

where ƒe is the effective strain in the FRP at ultimate failure of the member, cu the ultimate compressive strain in the concrete, c the depth of the neutral axis, h the depth of the section (or more accurately, the distance to the centroid of the FRP material), and bi the existing tensile strain in the concrete substrate at the location of the FRP strengthening system. FRP failure can occur either after (called mode 2a) or before (called mode 2b) the internal steel has yielded, with the concrete in the compression zone below its compression strength and ultimate failure strain (cu ⫽ 0.003). Here failure means any of the possible detachment modes or even FRP rupture if supplemental anchorages are used to prevent detachment failures. This is the failure mode of an underreinforced strengthened concrete beam. In this case, the effective strain in the FRP at failure is obtained from ƒe ⫽ mƒu

(ACI 440.2R-02:9-3)

where ƒu is the design strength of the FRP strengthening system. The effective stress, ƒƒe, in the FRP is the stress in the FRP at failure (either in mode 1 or in mode 2) and is linearly related to the effective strain as εc −

β1 c

c h

γ fc⬘

fc

C = γ fc⬘β1 cb

d

As

+ εs

fs

Ts = As fs

Af

εbi εfe

ffe

Tf = Af ffe

b

Figure 9.5 Strain, stresses, and force resultants in strengthened section at the ultimate state.

234

FRP FLEXURAL STRENGTHENING

ƒƒe ⫽ Eƒƒe 9.3.2

(ACI 440.2R-02:9-4)

Strain in the Internal Reinforcing Steel

For both modes, the strain in the internal reinforcing steel is related linearly to the strain in the FRP at failure as s ⫽ (ƒe ⫹ bi)

d⫺ c h⫺c

(ACI 440.2R-02:9-8)

and the stress in the internal steel, which must be less than or equal to the yield stress of the steel, is given as ƒs ⫽ Ess ⱕ ƒy 9.3.3

(ACI 440.2R-02:9-9)

Neutral-Axis Depth

The depth of the neutral axis for a singly reinforced section,4 c, is obtained from force equilibrium in the x-direction as shown in Fig. 9.5.

冘F ⫽0→T ⫹T ⫺C⫽0 x

s

ƒ

(9.1)

where Ts ⫽ Asƒs

(9.2)

Tƒ ⫽ Aƒƒƒe

(9.3)

C ⫽ ␥ƒ⬘c1cb

(9.4)

Substituting in the equilibrium equation yields c⫽

Asƒs ⫹ Aƒƒƒe ␥ƒc⬘1b

(ACI 440.2R-02:9-10)

where As is the area of the tensile steel, ƒs the stress in the steel at failure, d the depth of the steel reinforcing, 1 the depth ratio of an equivalent rectangular stress block, Aƒ the area of the FRP strip or the ﬁbers in a dry ﬁber system, ␥ the intensity of an equivalent rectangular stress block (also know as the concrete stress resultant factor), and b the width of the section. The nominal moment capacity of the section is then found from

4 For doubly reinforced sections the compression steel can be added following the same procedure. If the compression steel yields, additional failure modes are possible.

9.3.

FLEXURAL CAPACITY OF AN FRP-STRENGTHENED MEMBER

冉

Mn ⫽ Asƒs d ⫺ 9.3.4

冊

冉

冊

1c c ⫹ ƒ Aƒƒƒe h ⫺ 1 2 2

235

(ACI 440.2R-02:9-11)

Existing Substrate Strain

Since the FRP strengthening system is attached to the existing deﬂected structure, strains will already exist in the steel and concrete prior to the FRP being attached. These existing strains must be accounted for in the design process if the member is not shored up during the strengthening operation. Neglecting the existing strain in the concrete will lead to unconservative designs. To illustrate the strain conditions in the strengthened beam, the strains in the section can be depicted as a superposition of strains from before and after the FRP is attached, as shown in Fig. 9.6. The three strain states depicted are (1) the initial state: before the FRP is attached, considering only the exiting load at the time the FRP is attached; (2) the strengthened state: after the FRP has been attached, considering only the supplemental loads that are applied after the FRP has been attached (a hypothetical situation); and (3) the ﬁnal state: after the FRP has been attached with the existing and supplemental loads. Notice how the strain in the initial state is added to the strain that develops in the FRP strengthening system to give the ﬁnal strain state at the underside of the beam. This ﬁnal strain at the underside of the beam must be compatible with the strain in the concrete in the ﬁnal state. Notice, too, how the neutral axis shifts position in the three states. In ACI 440.2R-02 the existing strain at the substrate, b(1), is identiﬁed as bi and can be found from the properties of the transformed cracked section5 as

Initial State

Strengthened State

εc(1) −

εc(final) = εc(1)+εc(2)

εc(2) −

c(1)

c(final)

c(2)

+ + εs(1) εb(1) εf (1) = 0

Final State

−

= εs(2)

εb(2)

+

εf (2) = εb(2)

+

εs(final) = εs(1)+εs(2) εb(final) = εb(1)+ε b(2)

εf (final) = εf (2)

Figure 9.6 Superposition of strains.

5 Throughout the chapters that discuss FRP strengthening the elastic (cracked) properties of the original (i.e., unstrengthened) section are identiﬁed with a subscript 1 and the properties of the strengthened section are identiﬁed with a subscript 2.

236

FRP FLEXURAL STRENGTHENING

bi ⫽

m1(h ⫺ k1d) (Icr)1Ec

(9.5)

where m1 is the service load moment in the beam at the time the FRP system is attached (typically, only the dead load on the beam). The remaining terms are the usual properties of the transformed cracked section of the unstrengthened beam.

9.4 DETERMINATION OF FAILURE MODES AND FLEXURAL CAPACITY The solution to the preceding equations yields the depth of the neutral axis, the stresses and strains in all the materials (concrete, steel, and FRP), and the nominal moment capacity of the strengthened section. The correct solution to the equations depends on correctly identifying the failure mode of the section. As indicated previously, there are two primary failure modes, each with two variations, as follows: Mode Mode Mode Mode

1a: 1b: 2a: 2b:

Concrete crushing after steel yields Concrete crushing before steel yields FRP failure after steel yields FRP failure before steel yields

To arrive at a solution, one of the four failure modes above must ﬁrst be assumed. Thereafter, the location of the neutral axis, c, for this assumed failure mode is determined either by a trial-and-error method or by solving a quadratic equation. The correct value of c is the unique solution that gives the stresses and strains in the materials that are compatible with the assumed failure mode. Each of the four modes is discussed in detail below. It is important to point out that in most practical strengthening designs it is generally accepted that the failures should be in mode 1a or mode 2a; that is, failure occurs in the concrete or the FRP after the internal tension steel has yielded. This is because most FRP strengthening systems have lower moduli and higher strains to failure than the internal reinforcing steel bars, and they are located a similar distance from the neutral axis of the section (i.e., d or h). To utilize the large strain capacity of FRP strengthening systems effectively, the strain in the steel at failure of the strengthened system needs to be much larger than the yield strain of steel, which is 0.00207 for grade 60 rebar. However, for very high modulus strengthening systems, that have lower strains to failure, such as ultrahigh-modulus carbon systems, substantial strengthening can be achieved without the steel yielding before failure (modes 1b and 2b). In addition, for speciﬁc geometries and FRP strengthening con-

9.4

237

DETERMINATION OF FAILURE MODES AND FLEXURAL CAPACITY

ﬁgurations it may not be possible to achieve steel yielding before failure (because of FRP detachment, or an existing high reinforcement ratio, or a very low strength concrete). Also, in some designs the driving design requirement, generally when excessive live loads are a concern, is to reduce the strain in the internal steel at service loads. In these cases, failure after steel yielding is not a desirable failure mode. For all the reasons mentioned above, failure modes 1b and 2b are also covered in full detail in what follows, even though most FRP strengthened members will tend not to fail in these modes. 9.4.1

Mode 1a: Concrete Crushing After Steel Yields

In this mode the steel yields, and this is followed by concrete crushing with the strain in the FRP below its effective rupture strain. Therefore, the steel stress is set to its yield stress and the Whitney stress block parameters are applicable for the concrete. The depth of the neutral axis is found by substituting the following terms in the equilibrium equation: Ts ⫽ Asƒy

冉

(9.6)

冊

h⫺c Tƒ ⫽ Aƒƒƒe ⫽ AƒEƒ cu ⫺ bi c

(9.7)

C ⫽ 0.85 ƒc⬘1cb

(9.8)

Ts ⫹ Tƒ ⫺ C ⫽ 0 and rearranging gives the quadratic equation for c as (0.85ƒ⬘c1b)c2 ⫺ Asƒyc ⫺ AƒEƒ[cu(h ⫺ c) ⫺ bic] ⫽ 0

(9.9)

which can be written in the form Ac2 ⫹ Bc ⫹ C ⫽ 0

(9.10)

with A ⫽ 0.85ƒc⬘1b

(9.11)

B ⫽ ⫺Asƒy ⫹ AƒEƒ(cu ⫹ bi)

(9.12)

C ⫽ ⫺(AƒEƒcuh)

(9.13)

With the value of c obtained, the strains in the steel and FRP are calculated and checked to ensure that the steel strain exceeds the steel yield strain, sy, and that the FRP strain is less than mƒu.

238

FRP FLEXURAL STRENGTHENING

s ⫽ cu ƒe ⫽ cu

d⫺c ⱖ sy c

(9.14)

h⫺c ⫺ bi ⱕ mƒu c

(ACI 440.2R-02:9-3)

If the two conditions above are satisﬁed, the steel stress is taken as ƒy and the FRP stress is taken as ƒƒe ⫽ Eƒƒe

(ACI 440.2R-02:9-4)

The nominal moment capacity is obtained from

冉

Mn ⫽ Asƒy d ⫺

冊

冉

冊

1c c ⫹ ƒ Aƒƒƒe h ⫺ 1 2 2

(ACI 440.2R-02:9-11)

and the factored moment capacity is given as Mn

(9.15)

where ⫽ 0.7 ⫹ 0.2(s ⫺ sy)/(0.005 ⫺ sy) and depends on the value of the strain in the steel at the time of concrete crushing failure. 9.4.2

Mode 1b: Concrete Crushing Before Steel Yields

In this mode, the concrete is crushed before the steel yields with the strain in the FRP below its effective rupture strain. Therefore, the Whitney stress block parameters are applicable for the concrete. The depth of the neutral axis is found by substituting the following terms in the equilibrium equation: d⫺c c

(9.16)

h⫺c Tƒ ⫽ Aƒƒƒe ⫽ AƒEƒ cu ⫺ bi c

(9.17)

C ⫽ 0.85ƒc⬘1cb

(9.18)

Ts ⫽ Asƒs ⫽ As Ess ⫽ As Escu

冉

冊

Ts ⫹ Tƒ ⫺ C ⫽ 0 and rearranging gives the quadratic equation for c as (0.85ƒ⬘c1b)c2 ⫺ As Escu(d ⫺ c) ⫺ AƒEƒ[cu(h ⫺ c) ⫺ bic] ⫽ 0 which can be written in the form

(9.19)

9.4

DETERMINATION OF FAILURE MODES AND FLEXURAL CAPACITY

Ac2 ⫹ Bc ⫹ C ⫽ 0

239

(9.20)

with A ⫽ 0.85ƒ⬘c1b

(9.21)

B ⫽ As Escu ⫹ AƒEƒ(cu ⫹ bi)

(9.22)

C ⫽ ⫺(As Escud ⫹ AƒEƒcuh)

(9.23)

With the value of c obtained, the strains in the steel and FRP are calculated and checked to ensure that the steel strain is less than the steel yield strain, sy, and that the FRP strain is less than mƒu. s ⫽ cu ƒe ⫽ cu

d⫺c ⱕ sy c

(9.24)

h⫺c ⫺ bi ⱕ mƒu c

(ACI 440.2R-02:9-3)

If the two conditions above are satisﬁed, the steel stress is taken as ƒs ⫽ Ess

(ACI 440.2R-02:9-9)

ƒƒe ⫽ Eƒƒe

(ACI 440.2R-02:9-4)

the FRP stress is taken as

the nominal moment capacity is obtained from

冉

Mn ⫽ Asƒs d ⫺

冊

冉

冊

1c c ⫹ ƒ Aƒƒƒe h ⫺ 1 2 2

(ACI 440.2R-02:9-11)

and the factored moment capacity is given as Mn

(9.25)

where ⫽ 0.7 since the steel has not yielded at the time of concrete crushing failure. 9.4.3

Mode 2a: FRP Failure After Steel Yields

In this mode the steel yields, and following this the FRP fails with the strain in the concrete below its ultimate strain. Therefore, the steel stress is set to

240

FRP FLEXURAL STRENGTHENING

its yield stress and the FRP stress is set to its effective FRP failure strength, ƒƒe ⫽ mƒƒu . Since the concrete has not reached its ultimate compressive strain, the Whitney stress block parameters should technically not be used and the stress block parameters, 1 and ␥, should be obtained using a nonlinear analysis. This is the same as the case of the underreinforced section with FRP bars described in Chapter 5. The nonlinear stress–strain law described in Chapter 5 can be used. However, ACI 440.2R-02 permits the use of the Whitney stress block parameters in lieu of conducting a nonlinear iterative analysis since experimental results indicate that the strain in the concrete is typically close to the ultimate strain, when the FRP fails in a well-designed strengthening system. (In a well-designed strengthening system the section is close to the inelastic balanced strengthening ratio, described in detail below). Nevertheless, the strain in the concrete at failure should be checked and compared with the concrete ultimate strain, cu (i.e., 0.003), to verify that the concrete is close to compression failure. If this is not the case, the nonlinear analysis should be considered. The depth of the neutral axis is found by substituting the following terms in the equilibrium equation: Ts ⫽ Asƒy

(9.26)

Tƒ ⫽ Aƒmƒƒu

(9.27)

C ⫽ 0.85ƒc⬘1cb

(9.28)

Ts ⫹ Tƒ ⫺ C ⫽ 0 and rearranging gives the linear equation for c as (0.85ƒ⬘c1b)c ⫺ Asƒy ⫺ Aƒmƒƒu ⫽ 0

(9.29)

which gives c⫽

Asƒy ⫹ Aƒmƒƒu 0.85ƒc⬘1b

(9.30)

With the value of c obtained, the strains in the concrete must be calculated and checked to ensure that the concrete strain is less than the concrete ultimate strain, cu, and the strain in the steel must be calculated to ensure that it has indeed yielded. c ⫽ (ƒe⫹ bi)

c

ⱕ cu

(9.31)

d⫺c ⱖ sy h⫺c

(9.32)

h⫺c

s ⫽ (ƒe ⫹ bi)

If the conditions above are satisﬁed, the steel stress is taken as ƒy and the FRP stress is taken as

9.4

241

DETERMINATION OF FAILURE MODES AND FLEXURAL CAPACITY

ƒƒe ⫽ Eƒƒe ⫽ mƒƒu

(9.33)

The nominal moment capacity is obtained as

冉

Mn ⫽ Asƒy d ⫺

冊

冉

冊

1c c ⫹ ƒ Aƒƒƒe h ⫺ 1 2 2

(ACI 440.2R-02:9-11)

and the factored moment capacity is given as Mn

(9.34)

where ⫽ 0.7 ⫹ 0.2(s ⫺ sy)/(0.005 ⫺ sy) and depends on the value of the strain in the steel at the time of FRP failure. 9.4.4

Mode 2b: FRP Failure Before Steel Yields

In this mode, the FRP fails before the steel yields with the strain in the concrete below its ultimate strain. Therefore, the FRP stress is set to the effective FRP failure strength, ƒƒe ⫽ m ƒƒu. Since the concrete has not reached its ultimate compressive strain, the Whitney stress block parameters should technically not be used and the stress block parameters, 1 and ␥, should be obtained using a nonlinear analysis. As discussed for mode 2a, ACI 440.2R02 permits the use of the Whitney stress block parameters in lieu of conducting a nonlinear iterative analysis since experimental results indicate that the strain in the concrete is typically close to the ultimate strain when the FRP fails in a well-designed strengthening system. Nevertheless, the strain in the concrete at failure should be checked and compared with the concrete ultimate strain, cu (i.e., 0.003), to verify that the concrete is close to compression failure.6 If this is not the case, the nonlinear analysis should be considered. The depth of the neutral axis is found by substituting the following terms in the equilibrium equation. Ts ⫽ Asƒs ⫽ As Ess ⫽ As Es(ƒe ⫹ bi)

d⫺c h⫺c

(9.35)

Tƒ ⫽ Aƒƒƒe ⫽ Aƒmƒƒu ⫽ AƒEƒƒe

(9.36)

C ⫽ 0.85ƒc⬘1cb

(9.37)

Ts ⫹ Tƒ ⫺ C ⫽ 0 and rearranging gives the quadratic equation for c as

6 This can be assumed to be 0.002 or greater if the ultimate strain is taken to be 0.003 according to ACI 318.

242

FRP FLEXURAL STRENGTHENING

(0.85ƒc⬘1b)c(h ⫺ c) ⫺ As Es(ƒe ⫹ bi)(d ⫺ c) ⫺ AƒEƒƒe(h ⫺ c) ⫽ 0

(9.38)

which can be written in the form Ac2 ⫹ Bc ⫹ C ⫽ 0

(9.39)

with, A ⫽ 0.85ƒc⬘1b

(9.40)

B ⫽ ⫺[0.851ƒ⬘cbh ⫹ As Es(ƒe ⫹ bi) ⫹ AƒEƒƒe]

(9.41)

C ⫽ As Es(ƒe ⫹ bi)d ⫹ AƒEƒƒeh

(9.42)

With the value of c obtained, the strains in the concrete must be calculated and checked to ensure that the concrete strain is less than the concrete ultimate strain, cu, and the strain in the steel must be calculated to ensure that it is less than the steel yield strain, sy. c ⫽ (ƒe ⫹ bl) s ⫽ (ƒe ⫹ bi)

c

ⱕ cu

(9.43)

d⫺c ⱕ sy h⫺c

(9.44)

h⫺c

If the two conditions above are satisﬁed, the steel stress is taken as ƒs ⫽ Ess

(ACI 440.2R-02:9-9)

the FRP stress is taken as ƒƒe ⫽ Eƒƒe ⫽ mƒƒu

(9.45)

the nominal moment capacity is obtained from

冉

Mn ⫽ Asƒs d ⫺

冊

冉

冊

1c c ⫹ ƒ Aƒƒƒe h ⫺ 1 2 2

(ACI 440.2R-02:9-11)

and the factored moment capacity is given as Mn

(9.46)

where ⫽ 0.7 since the steel has not yielded at the time of FRP failure.

9.5

9.5

BALANCED CONDITION

243

BALANCED CONDITION

A balanced condition can be deﬁned for the FRP strengthened section in a fashion similar to the balanced condition for a typical reinforced concrete section. The balanced condition for the strengthened section is deﬁned as the condition at which concrete compression failure and FRP failure occur simultaneously. Depending on the strain in the steel at which this simultaneous failure occurs, two balanced conditions are possible: deﬁned herein as the elastic balanced condition, in which the tension steel has not yielded when the balanced strain condition is reached, and the inelastic balanced condition, in which the steel has yield prior to the balanced strain condition being reached. As discussed previously, for practical strengthening designs, the inelastic balanced condition is the balanced condition of principal interest. It is the only one that is presented in what follows; however, the elastic balanced condition can be derived following a similar procedure. The inelastic balanced strain condition is obtained by setting the concrete failure strain to cu ⫽ 0.003 and the FRP failure strain to ƒe ⫽ mƒu and checking that the steel strain s ⱖ sy. Using this condition the inelastic balanced reinforcement ratio can be deﬁned as ƒb ⫽

Aƒb bd

(9.47)

Since the FRP failure strain is a function of the bond coefﬁcient, m, a speciﬁc number of layers, n, of the strengthening system must be assumed to determine the balanced reinforcement ratio. That is, different balanced ratios may exist for the same beam, depending on the number of layers of FRP strengthening system used. This is not a signiﬁcant obstacle in design given that most practical ﬂexural strengthening systems typically use between one and three layers. The depth of the neutral axis at the balanced condition is found from strain compatibility as cb ⫽

cuh cu ⫹ mƒu ⫹ bi

(9.48)

The resulting section forces (see Fig. 9.5) at the inelastic balanced condition are given as C ⫽ 0.85ƒ⬘c1cbb

(9.49)

Ts ⫽ Asƒy

(9.50)

Tƒ ⫽ Aƒbmƒƒu

(9.51)

Substitution into the equilibrium equation yields

244

FRP FLEXURAL STRENGTHENING

冘F ⫽0→T ⫹T ⫺C⫽0 x

s

ƒ

(9.52)

and solving for Aƒb gives Aƒb ⫽

Asƒy 0.85ƒ⬘c1bhcu ⫺ mƒƒu(cu ⫹ mƒu ⫹ bi) mƒƒu

(9.53)

and ƒb ⫽ 0.85

ƒys ƒc⬘1 cu h ⫺ mƒƒu cu ⫹ mƒu ⫹ bi d mƒƒu

(9.54)

Provided that the steel has yielded, s ⫽ (ƒe ⫹ bi)

d ⫺ cb ⱖ sy h ⫺ cb

(9.55)

It is very important to note that unlike in steel reinforced sections, it is not always possible to achieve a balanced condition, due to the wide range of properties of different FRP strengthening systems and the existing dimensions of the concrete section. In particular, it is important to reemphasize that to obtain strengthening the compression force resultant in the section must increase from the unstrengthened (existing) case. For this to happen, the neutral axis of the strengthened section must move downward from its original position (i.e, cb(new) ⬎ cunstrengthened). If the strain to failure in the FRP is high and the modulus is relatively low (such as for a glass FRP system), the opposite may occur (i.e., the neutral axis may move upward), which is not possible and means that the balanced condition cannot be achieved for the number of plies of the FRP system chosen. If the calculation for the balanced reinforcement ratio gives a rational result (i.e., cb(new) ⬎ cunstrengthened), the balanced reinforcement ratio can be useful in determining the optimal area of FRP reinforcement required for a given strengthening demand. In addition, if the balanced ratio can be found for a particular FRP system, it is a useful to tool for designing the FRP system to achieve a desired failure mode (i.e., concrete crushing or FRP failure) since: If Aƒ ⬍ Aƒb, the FRP failure mode (mode 2a) will control and c ⬍ cb. If Aƒ ⬎ Aƒb, the concrete failure mode (mode 1a) will control and c ⬎ cb. 9.6

DETAILING FOR FLEXURAL STRENGTHENING

At the strip ends two empirical checks are required by ACI 440.2R-02 to detail the FRP strip to ensure that premature failure does not occur in the beam prior to it achieving its design ﬂexural strength. These are:

9.7

DESIGN PROCEDURE FOR A CONCRETE MEMBER

245

1. A strength check at the strip end or inﬂection point to prevent delamination due to anchorage failure. According to ACI 440.2R-02, the FRP ﬂexural strengthening system must extend a distance d beyond the point corresponding to the cracking moment under factored loads for a simply supported beam. 2. A strength check at the strip end to prevent shear failure of the beam at the point of FRP strip termination. ACI 440.2R-02 requires that the factored shear force at the FRP strip termination point be less than twothirds of the concrete shear capacity at this point.

9.7 DESIGN PROCEDURE FOR A FLEXURALLY STRENGTHENED CONCRETE MEMBER To design an FRP ﬂexural strengthening system for a reinforced concrete member to achieve a required moment capacity (demand), Mu, for future loads, the following steps should be followed: Step 1. Determine the ﬂexural and shear capacity of the original beam. The original capacity must be known prior to performing a strengthening design. The geometric and material properties of the existing beam are needed for this step. If existing plans and speciﬁcations are available, they can be consulted, but the designer needs to check that these accurately reﬂect the properties of the as-built member that will be strengthened. In many strengthening cases original plans or speciﬁcations no longer exist or can no longer be found, and the designer needs to obtain the data from the existing structure using ﬁeld measurements, material tests, and engineering judgment. Step 2. Determine the section properties of the original beam and the existing strain on the sofﬁt. These properties are needed in subsequent calculations. It is usual to assume that the beam or slab sofﬁt has been cracked by prior loads and that only the dead load will be acting when the strengthening system is applied. If other loads besides dead loads are on the member when it is to be strengthened or a shoring system is used, the designer needs to determine the strain on the sofﬁt for these conditions. Step 3. Determine current and future design loads and capacities and check the ultimate strengthening limits. Based on the given strengthening requirement the future required ﬂexural and shear capacities (demands) need to be determined to determine if in fact strengthening is needed. In some cases strengthening may not actually be needed. This is because the member may have been overdesigned for the original loads due either to minimum reinforcement requirements (especially for shear reinforcement) or due to sizes of available bars and detailing requirements (especially for ﬂexural reinforcement). In this step the maximum code-permitted strength-

246

FRP FLEXURAL STRENGTHENING

ening limits for ﬂexural strengthening should be checked to give the designer a feel for how much strengthening can be obtained and how this compares with the demand strengthening. Step 4. Select an FRP strengthening system and determine its design properties. Numerous different FRP strengthening systems are available. The designer should be aware of which systems can readily be obtained and if a certiﬁed installer is available at the project location. Designs with different FRP systems should be considered. It is advisable to do a design with precured strips and laid-up sheets and to consider both carbon and glass systems. The unit costs of the various systems (both material and installation costs) should be obtained in this step of the design process. Step 5. Estimate the amount of strengthening required and conﬁgure the FRP system. To begin the design, an estimate of the amount of strengthening can be obtained. An estimate of the required FRP area can be found as follows: (i) Determine the additional factored moment that needs to be carried by the FRP, ⌬Mn. Assume ⫽ 0.9 and determine ⌬Mn ⫽ (⌬Mn)/ . (ii) Approximate the stress in the FRP at failure as 80% of the effective strength (i.e., mƒƒu) with m ⫽ 0.8. Since the maximum allowable stress in the FRP is 90% of the design strength, this assumes that failure due to concrete crushing may occur. Also, it assumes that a designer would like to try to stress the FRP system as much as possible to obtain an economically efﬁcient design. (iii) Approximate the depth of the compression block in the concrete as equal to c in the unstrengthened section, recognizing that it must be greater than a since the neutral axis will move downward after the strengthening has been applied. (iv) The additional nominal moment carried by the FRP is given as

冉 冊

⌬Mn ⫽ ƒAƒƒƒe h ⫺

c 2

(9.56)

which gives the estimated required area of FRP strengthening as Aƒreqd ⫽

⌬Mn (h ⫺ c/2) ƒƒƒe

(9.57)

Or, using Aƒ ⫽ ntƒwƒ, the approximate number of layers of the chosen FRP system is found as n⫽

⌬Mn ƒtƒwƒƒƒe(h ⫺ c/2)

(9.58)

9.7

DESIGN PROCEDURE FOR A CONCRETE MEMBER

247

Step 6. Determine the inelastic balanced reinforcement ratio. Determine the inelastic balanced ratio for various numbers of layers of the system chosen, always ensuring that steel yielding has occurred. If a speciﬁc failure mode is desired, choose the number of layers and area of FRP to achieve this failure. To ensure the desired failure mode, it is recommended either 10% more (concrete failure) or less (FRP failure) FRP than the balanced FRP ratio be used. Step 7. Select a trail design. Based on the data collected in steps 5 and 6, select a trail design. Step 8. Determine the capacity and suitability of the section with the trial FRP design. At a very minimum, the ﬂexural capacity for the strengthened member must exceed the ﬂexural demand. However, the suitability of the design should be evaluated. If the FRP system is overdesigned, another iteration should be performed to reduce the amount of FRP used (provided that this does not have a negative impact on constructability). A design whereby failure is by the opposite failure mode from the one chosen in the trail design should be attempted and a cost comparison made between the two designs. A different FRP system may need to be considered in this case since different FRP systems may be not be susceptible to the same failure modes. Step 9. Detail the FRP ﬂexural strengthening system. (a) Check the strength at the strip end or inﬂection point to prevent delamination due to anchorage failure. (b) Check the strength at the strip end to prevent shear failure of the beam at the point of FRP strip termination. Design Example 9.1: FRP Flexural Strengthening of a Beam An existing simply supported reinforced concrete beam in the interior of a building spans 24 ft and is constructed of 5000-psi concrete with three No. 9 grade 60 main bars.7 Shear reinforcement is provided by No. 3 grade 60 stirrups at 10.5 in. on center. The beam was originally designed for the following loads: wDL ⫽ 1.0 kip/ft wLL ⫽ 1.2 kip/ft Wu ⫽ 1.4(1.0) ⫹ 1.7(1.2) ⫽ 3.44 kip/ft

7 This example has the same dimensions and properties as the design example given in Section 14.3 of ACI 440.2R-02 but uses a different solution procedure and discusses design-related issues in more detail.

248

FRP FLEXURAL STRENGTHENING

Due to a change in the use of the structure, the live load carrying–capacity of the beam needs to be increased by 50%. You are required to design an FRP strengthening system for the beam. The dimensions of the existing beam section are given in Fig. 9.7. SOLUTION Step 1. Determine the ﬂexural and shear capacity of the original beam. The ﬂexural capacity of the existing beam: b ⫽ 0.85 ⫽ 0.85

s ⫽

冉

冊

ƒ⬘c 87,000 1 ƒy 87,000 ⫹ ƒy

冉 冊 冉

冊

5000 87,000 (0.80) ⫽ 0.0335 60,000 87,000 ⫹ 60,000

As 3(1.0) ⫽ ⫽ 0.0116 bd 12(21.5) s 0.0116 ⫽ ⫽ 0.34 → i.e., 34% of balanced b 0.0335

Note that the existing beam is underreinforced and is a good candidate for strengthening (less than 40% of the balanced steel).

d = 21.5 in.

h = 24 in.

b = 12 in.

Figure 9.7 Beam cross-sectional dimensions for Example 9.1.

9.7

DESIGN PROCEDURE FOR A CONCRETE MEMBER

a⫽

Asƒy 3.0(60,000) ⫽ ⫽ 3.53 in. 0.85ƒc⬘b 0.85(5000)(12)

c⫽

a 3.53 ⫽ ⫽ 4.41 in. 1 0.80

冉 冊

Mn ⫽ Asƒy d ⫺

冉

249

冊

a 3.53 ⫽ 3.0(60,000) 21.5 ⫺ 2 2

⫽ 3552 lb-in. ⫽ 296 kip-ft

and since the beam is underreinforced, ⫽ 0.908 and Mn ⫽ 0.9(296) ⫽ 266 kip-ft. Based on the existing loads, the original ﬂexural design demand was Mu ⫽

3.44(24)2 ⫽ 247.7 kip-ft ⬍ 266 kip-ft 8

and the original beam design was satisfactory for the existing loads. Note that this is only a check. The shear capacity of the existing beam, Vn ⫽ Vc ⫹ Vs ⫽ 2兹ƒc⬘bd ⫹ ⫽ 2兹5000(12)(21.5) ⫹

Asvƒyd s

2(0.11)(60,000)(21.5) 10.5

⫽ 36,487 ⫹ 27,029 ⫽ 63,516 lb ⫽ 63.5 kips

and the factored shear capacity is Vn ⫽ 0.85(63.5) ⫽ 54.0 kips

Based on the existing loads, the original shear design demand was Vu ⫽ Wu

冉 冊 ᐉ

2

⫺d

冉

⫽ 3.44

冊

24 21.5 ⫺ ⫽ 35.12 kips ⬍ 54.0 kips 2 12

and the beam design is satisfactory for the existing loads. Note that this is only a check.

8

Recall that ACI 440.2R-02 is based on ACI 318-99 load factors and resistance factors.

250

FRP FLEXURAL STRENGTHENING

Step 2. Determine the section properties of the original beam and the existing strain on the sofﬁt. Determine the existing strain on the underside (sofﬁt) of the concrete beam prior to the attachment of the FRP strengthening. Calculate the strain based on the cracked section with only the dead load acting on the beam. To do this, the section properties of the beam are needed. It can generally be assumed that the existing beam has cracked under its prior service loading; however, this should be veriﬁed for the sake of completeness. However, even if it is found by calculation that the beam was not cracked under the service loads, it is advisable and conservative to assume that the beam was previously cracked in service in order to determine the existing strain on the substrate. Calculate the cracking moment: ƒr ⫽ 7.5兹ƒc⬘ ⫽ 7.5兹5000 ⫽ 530.3 psi Ig ⫽ Mcr ⫽ mDL⫹LL ⫽

b h3 12(24)3 ⫽ ⫽ 13,824 in4 12 12 2ƒr Ig 2(530.3)(13,824) ⫽ ⫽ 610,906 lb-in. ⫽ 50.9 kip-ft h 24 wDL⫹LLL2 (1.0 ⫹ 1.2)(24)2 ⫽ ⫽ 158.4 kip-ft ⬎ 50.9 kip-ft 8 8

Therefore, the section is cracked. Calculate the cracked section properties. Method 1: Using the transformed section9 Ec ⫽ 57,000兹ƒc⬘ ⫽ 57,000兹5000 ⫽ 4,030,508 psi ⫽ 4030 ksi s ⫽

Es 29,000,000 ⫽ ⫽ 7.2 Ec 4,030,000

k1 ⫽ 兹(ss)2 ⫹ 2ss ⫺ ss ⫽ 兹[0.0116(7.2)]2 ⫹ 2(0.0116)(7.2) ⫺ 0.0116(7.2) ⫽ 0.334

(Icr)1 ⫽ ⫽

bd3 3 k ⫹ sAsd 2(1 ⫺ k1)2 3 1 12(21.5)3 (0.334)3 ⫹ 7.2(3.0)(21.5)2(1 ⫺ 0.334)2 ⫽ 5909 in4 3

9 Throughout the chapters that discuss FRP strengthening the elastic (cracked) properties of the original (i.e., unstrengthened) section are identiﬁed with a subscript 1 and the properties of the strengthened section are identiﬁed with a subscript 2.

9.7

mDL ⫽ bi ⫽

DESIGN PROCEDURE FOR A CONCRETE MEMBER

251

wDLL2 1.0(24)2 ⫽ ⫽ 72 kip-ft ⫽ 864 kip-in. 8 8 mDL(h ⫺ k1d) 864[24 ⫺ 0.334(21.5)] ⫽ ⫽ 0.000611 (Icr)1Ec 5909(4030)

Method 2: Using composite mechanics Following the procedure described in Chapter 5, the distance from the top of the section to the neutral axis is found from Ecb

c21 ⫹ EsAs[c1 ⫺ d] ⫽ 0 2

(c1)2 ⫹ 29(c1 ⫺ 21.5)(3.0) ⫽ 0 2

4.030(12)

24.18(c1)2 ⫹ 87c1 ⫺ 1870.5 ⫽ 0 Solving the quadratic equation and taking the positive root gives c1 ⫽ 7.18 in. and k1 ⫽

c1 7.18 ⫽ ⫽ 0.334 in. d 21.5

The ﬂexural stiffness (EI)1 of the original section is given as (EI)1 ⫽

冘 EI ⫽ E I ⫹ E I ⫽ E b(c3 ) ⫹ E A (d⫺ c ) 3

1

1 1

2 2

冋

⫽ ⫹ 4,030,000

c

2

s

s

1

册

12(7.18)3 ⫹ 29,000,000(3.0)(21.5 ⫺ 7.18)2 3

⫽ 2.38 ⫻ 1010 lb-in2

and bi ⫽

mDL(h ⫺ k1 d) 864[24 ⫺ 0.334(21.5)] ⫽ ⫽ 0.000611 (EI)1 2.38 ⫻ 1010

which is the same result as obtained above using the transformed section method. In what follows it will be seen that the composite section method is easily adapted to the strengthened section and is recommended for use with the strengthened section.

252

FRP FLEXURAL STRENGTHENING

Note that the transformed cracked second moment can be found from the above from Icr ⫽

(EI)1 2.38 ⫻ 1010 ⫽ ⫽ 5906 in4 ⬇ 5909 in4 Ec 4,030,000

Step 3. Determine the current and future design loads and capacities and check the ultimate strengthening limit. The beam needs to be strengthened to carry the following future loads: wDL ⫽ 1.0 kip/ft wLL ⫽ 1.2 (1.5) ⫽ 1.8 kip/ft Wu ⫽ 1.4(1.0) ⫹ 1.7(1.8) ⫽ 4.46 kip/ft The future design demand Mu ⫽ 4.46(24)2 /8 ⫽ 321.1 kip-ft ⬎ 266 kip-ft, and therefore ﬂexural strengthening is required for the future loads. This is equal to a percentage increase of 20.7% in the moment-carrying capacity. The future shear demand Vu ⫽ 4.46(24/2 ⫺ 21.5/12) ⫽ 45.5 kips ⬍ 54.0 kips, and therefore the existing shear capacity of the beam is sufﬁcient to carry the future loads. Check the strengthening limit for future limit-factored loads and compare with the existing unstrengthened capacity: Wlimit ⫽ 1.2(1.0) ⫹ 0.85(1.8) ⫽ 2.73 kip/ft Mlimit ⫽

2.73(24)2 ⫽ 196.6 kip-ft ⬍ 266 kip-ft 8

Therefore, the beam can be strengthened to carry the future loads without exceeding the ACI mandated limit on the maximum strengthening enhancement allowed.10 The maximum permissible strengthened moment capacity allowed for this beam can also be calculated if desired as follows: (Mn)max ⫽ (Mn)org

1.4 ⫹ 1.7R 1.2 ⫹ 0.85R

Assuming that the live load-to-dead load ratio will remain the same for the maximum strengthening (i.e., R ⫽ 1.8/1.0 ⫽ 1.8), we obtain 10 In the general case, the designer must ensure that the limiting condition is met for the shear capacity as well as the ﬂexural capacity.

9.7

(Mn)max ⫽ 266

DESIGN PROCEDURE FOR A CONCRETE MEMBER

冋

253

册

1.4 ⫹ 1.7(1.8) ⫽ 434.6 kip-ft ⬎ 321.1 kip-ft 1.2 ⫹ 0.85(1.8)

and the maximum permissible % increase over the original capacity (which is not necessarily the original loads) is

%max ⫽

0.2 ⫹ 0.85R ⫻ 100 1.2 ⫹ 0.85R

%max ⫽

0.2 ⫹ 0.85(1.8) ⫻ 100 ⫽ 63.4% ⬎ 20.7% 1.2 ⫹ 0.85(1.8)

Step 4. Select an FRP strengthening system and determine its design properties. Consider a strengthening system with the following ply properties: tƒ ⫽ 0.04 in. wƒ ⫽ 12 in.

ƒ* ƒu ⫽ 90 ksi

Eƒ ⫽ 5360 ksi

* ƒu ⫽ 0.017 ⫽ 1.7%

Note that this is a hypothetical FRP system and does not represent properties of any known actual FRP strengthening system. The properties provided are similar to those of a glass FRP strengthening system, although the ACI 440.2R-02 identiﬁes this as a carbon FRP system. Typically, only the longitudinal properties of an FRP strengthening system are given. However, when using a multiple ﬁber orientation strengthening layup, these properties cannot be used because a multidirectional laminate will have signiﬁcantly different longitudinal properties than the unidirectional properties, as explained in Chapter 3. In this case, the effective longitudinal properties of the multidirectional layup in the direction of the required strengthening must ﬁrst be determined using the methods for multidirectional laminates described in Chapter 3. Recall that all four in-plane stiffnesses and all ﬁve in-plane strengths of the individual orthotropic plies are needed to obtain the in-plane properties of a multidirectional laminate. Determine the design strength and design rupture strain of the FRP system selected: CE ⫽ 0.95

for carbon–epoxy in interior use

ƒƒu ⫽ CEƒ* ƒu ⫽ 0.95(90) ⫽ 85.5 ksi ƒu ⫽ CEƒu * ⫽ 0.95(0.017) ⫽ 0.0162

254

FRP FLEXURAL STRENGTHENING

Step 5. Estimate the amount of strengthening required and conﬁgure the FRP system. The additional moment that needs to be carried by the FRP is ⌬Mn ⫽ 321 ⫺ 266 kip-ft ⫽ 55 kip-ft ⌬Mn ⫽

55 ⫽ 61.1 kip-ft ⫽ 733.20 kip-in. 0.9

Approximate the stress in the FRP at failure as 80% of the effective strength (i.e., mƒƒu) with m ⫽ 0.8. Since the maximum allowable stress in the FRP is 90% of the design strength, this assumes that failure due to concrete crushing may occur. Also, it assumes that a design would like to try to stress the FRP system as much as possible to obtain an economically efﬁcient design, ƒƒe ⫽ 0.8mƒƒu ⫽ 0.8(0.8)(85.5) ⫽ 54.72 ksi Approximate the depth of the compression block in the concrete as equal to c in the unstrengthened section because it will be greater than a with the neutral axis moving downward after the strengthening has been applied, c ⫽ 4.41 in. The additional nominal moment carried by the FRP is given as

冉 冊

⌬Mn ⫽ ƒAƒƒƒe h ⫺

c 2

which gives the estimated required area of FRP strengthening as Aƒreqd ⫽

⌬Mn 773.2 ⫽ ⫽ 0.763 in2 ƒƒƒe(h ⫺ c/2) 0.85(54.72)(24 ⫺ 4.41/2)

Or, using Aƒ ⫽ ntƒwƒ, we ﬁnd the approximate number of layers of the chosen FRP system with a 12-in. width11 (i.e., the maximum width possible since the beam is 12 in. wide) as

11 The designer should also consider the case of the FRP strengthening system not being the full width of the beam. A fully optimized solution will consider both different widths and different number of layers.

9.7

n⫽

DESIGN PROCEDURE FOR A CONCRETE MEMBER

255

⌬Mn 773.20 ⫽ ƒtƒwƒƒƒe(h ⫺ c/2) 0.85(0.04)(12)(54.72)(24 ⫺ 4.41/2) ⫽ 1.6

⬖ try 2 plies

Step 6. Determine the inelastic balanced reinforcement ratio. First, determine the unit stiffness of the FRP strengthening system and the bond-dependent coefﬁcient, m. The procedure is demonstrated for two layers of the FRP system chosen, nEƒtƒ ⫽ 2(5,360,000)(0.04) ⫽ 428,800 ⱕ 1,000,000 lb/in. and therefore, m ⫽

冉

冊

冉

冊

nEƒtƒ 1 1 428,800 1⫺ ⫽ 1⫺ 60ƒu 2,000,000 60(0.0162) 2,000,000

⫽ 0.818 ⱕ 0.90

and cb ⫽

cuh 0.003(24) ⫽ ⫽ 4.27 in. cu ⫹ mƒu ⫹ bi 0.003 ⫹ 0.818(0.0162) ⫹ 0.00061

Observe that 4.27 in. ⬍ 4.41 in., which is the depth of the neutral axis in the original unstrengthened state. Therefore, an area of FRP using two layers of the system chosen will not produce the balanced condition. In addition, it will not be possible to achieve FRP failure for two layers of this system, regardless of the area chosen. The section will fail due to concrete compression. To demonstrate this point, the balanced reinforcement area is calculated for this case. First, conﬁrm that the steel has yielded for this situation: sy ⫽

ƒy 60,000 ⫽ ⫽ 0.00207 Es 29 ⫻ 106

s ⫽ (ƒe ⫹ bi)

d⫺c h⫺c 21.5 ⫺ 4.27 ⫽ 0.0121 ⬎ 0.00207 24 ⫺ 4.27

⫽ [0.818(0.0162) ⫹ 0.00061]

Therefore, the steel has yielded and the inelastic balanced area can be found from

256

FRP FLEXURAL STRENGTHENING

Aƒb ⫽ ⫽

Asƒy 0.85ƒc⬘1bhcu ⫺ mƒƒu(cu ⫹ mƒu ⫹ bi) mƒƒu 0.85(5000)(0.80)(12)(24)(0.0003) 0.818(85,500)[0.003 ⫹ 0.818(0.0162) ⫹ 0.00061] ⫺

3.0(60,000) 0.818(85,500)

⫽ ⫺0.083 in2 ⬍ 0 → not possible!

Clearly, a negative area of FRP is not possible and the solution is invalid. The balanced condition cannot be achieved with two layers of the system chosen. Stated another way, if the neutral axis must move upward (i.e., the compression force resultant in the concrete is reduced from its original value), an additional compression force resultant is required in the section, which can only be supplied by the FRP—which is not possible! At this stage in the design process, it is useful to determine the balanced FRP area for likely numbers of layers of the chosen reinforcement system. As discussed previously, this is useful in understanding how the failure modes relate to the FRP system area and the number of layers. As a result, speciﬁc failure modes can be selected based on the foregoing study. Table 9.1 shows the results of the calculations for one to ﬁve layers of the system chosen. ⫽ Step 7. Select a trail design. Based on the approximate calculation of Areqd ƒ 0.76 in2 of step 5 and the balanced calculations of step 6, two possible trail designs could be considered: Option a: two layers of the FRP system with an estimated width of 9.5 in. (concrete failure mode), and Option b: four layers of the FRP system with an estimated width of 4.75 in. (FRP failure mode). Option a is considered ﬁrst.

TABLE 9.1

Balanced FRP Areas and Width for Various Numbers of Layers

Layers, n

Unit Stiffness, nEƒ tƒ (lb / in.)

Bond Coefﬁcient, m

Depth of NA, cb (in.)

1 2 3 4 5

214,400 428,800 643,200 857,600 1,072,000

0.900 0.818 0.698 0.588 0.480

3.95 4.27 4.83 5.48 6.32

a b

s

Balanced FRP Area, Aƒb (in2)a

Balanced FRP Width, wƒb (in.)

0.0133 0.0121 0.0104 0.0087 0.0072

—b —b 0.28 0.87 1.90

— — 2.36 5.44 9.50

Steel Strain,

If Aƒ ⬍ Aƒb, the failure mode is FRP failure; if Aƒ ⬎ Aƒb, the failure mode is concrete failure. Since cb ⬍ cunstrengthened, a balanced condition is not possible.

9.7

DESIGN PROCEDURE FOR A CONCRETE MEMBER

257

Option a: Two layers of the FRP system chosen with an estimated width of 9.5 in. (concrete failure mode). Since it is known that for any amount of FRP area used, the failure mode will be concrete failure for two layers, a trial design with the maximum possible FRP for two layers (i.e., two layers each 12 in. wide12) is selected. This gives an area of FRP reinforcement Aƒ ⫽ ntƒwƒ ⫽ 2(0.04)(12) ⫽ 0.96 in2, which is greater than the estimate of 0.76 in2 and should therefore be a feasible design. Step 8. Determine the capacity and suitability of the section with the trial FRP design. The failure mode (mode 1a or 1b) must be determined to determine the moment capacity of the strengthened section. This requires determining the depth of the neutral axis and checking that the strains in the concrete, steel, and the FRP are compatible with the assumed failure mode. This can be determined directly from the equilibrium equations of the section as described in Section 9.4.1. Start by assuming failure mode 1b,13 concrete compression failure before the steel has yielded. The characteristic equation to be solved for this assumed failure mode is (0.85ƒ⬘c1b)c2 ⫺ As Escu(d ⫺ c) ⫺ AƒEƒ[cu(h ⫺ c) ⫺ bic] ⫽ 0 which can be written in the form Ac2 ⫹ Bc ⫹ C ⫽ 0 with, A ⫽ 0.85ƒ⬘c1b ⫽ 0.85(5)(0.80)(12) ⫽ 40.80 kip/in. B ⫽ As Escu ⫹ AƒEƒ(cu ⫹ bi) ⫽ 3.0(29,000)(0.003) ⫹ 0.96(5360)(0.003 ⫹ 0.00061)⫽ 279.58 kips

C ⫽ ⫺(As Escud ⫹ AƒEƒcuh) ⫽ ⫺[3.0(29,000)(0.003)(21.5) ⫹ 0.96(5360)(0.003)(24)] ⫽ ⫺5981.98 kip-in.

Solving the quadratic equation and taking the positive root gives

12 Note that this decision was made in hindsight after determining that two layers 9.5 in. wide would not provide the required moment capacity. 13 Mode 1b is checked ﬁrst in this example to demonstrate the solution procedure. Typically, mode 1a would be checked before mode 1b in an actual design and analysis procedure.

258

FRP FLEXURAL STRENGTHENING

c ⫽ 9.15 in. Now, check if, in fact, the steel has not yielded (i.e., s ⬍ sy ⫽ 0.00207 for ƒy ⫽ 60 ksi). If it has yielded, the solution above is not valid: s ⫽ cu

冉

冊

21.5 ⫺ 9.15 d⫺c ⫽ 0.003 ⫽ 0.0405 ⬎ 0.00207 c 9.15

Therefore, the steel has in fact yielded and the solution for c is not valid. Now assume failure mode 1a, concrete crushing after the steel has yielded. The characteristic equation for this case is (0.85ƒc⬘1b)c2 ⫺ Asƒyc ⫺ AƒEƒ[cu(h ⫺ c) ⫺ bic] ⫽ 0 which can be written in the form Ac2 ⫹ Bc ⫹ C ⫽ 0 with A ⫽ 0.85ƒ⬘c1b ⫽ 0.85(5)(0.80)(12) ⫽ 40.80 kip/in. B ⫽ Asƒy ⫹ AƒEƒ(cu ⫹ bi) ⫽ ⫺3.0(60) ⫹ 0.96(5360)(0.003 ⫹ 0.00061) ⫽ ⫺161.42 kips

C ⫽ ⫺(AƒEƒcuh) ⫽ ⫺0.96(5360)(0.003)(24) ⫽ ⫺370.48 kip-in. Solving the quadratic equation and taking the positive root gives c ⫽ 5.58 in. Note that this value is greater than 4.27 in, which is the depth of the neutral axis that would be required to develop a balanced section if it were possible. This conﬁrms, once again, that the failure mode will be concrete compression since c ⬎ cb. Now check the strains in the steel and the FRP, s ⫽ cu

冉

冊

21.5 ⫺ 5.58 d⫺c ⫽ 0.003 ⫽ 0.008 ⬎ 0.00207 → OK c 5.58

Steel has yielded as assumed and

9.7

ƒe ⫽ cu

DESIGN PROCEDURE FOR A CONCRETE MEMBER

冉

259

冊

h⫺c 24 ⫺ 5.58 ⫺ bi ⫽ 0.003 ⫺ 0.00061 c 5.58

⫽ 0.00929 ⬍ mƒu ⫽ 0.818(0.0162) ⫽ 0.0133

Since ƒe ⬍ mƒu, the concrete failure mode is once again conﬁrmed; the FRP will not reach its effective design strain at failure. The stress in the FRP is found as ƒƒe ⫽ Eƒƒe ⫽ 5360(0.00929) ⫽ 49.79 ksi ⬍ ƒƒu ⫽ 85.50 ksi Now determine the nominal moment capacity, a ⫽ 1c ⫽ 0.80(5.58) ⫽ 4.46 in.

冉

Mn ⫽ Asƒy d ⫺

冉

冊

冉

冊

1c c ⫹ ƒ Aƒƒƒe h ⫺ 1 2 2

⫽ 3.0(60) 21.5 ⫺

冊

冉

冊

4.46 4.46 ⫹ 0.85(0.96)(49.79) 24 ⫺ 2 2

⫽ 3468.6 ⫹ 884.7 ⫽ 4352 kip-in. ⫽ 362 kip-ft

Note that the fraction of the nominal moment carried by the FRP is 884.7/ 3453 ⫽ 0.256, or 25.6%. The moment carried by the steel is 3468.6 kip-in. ⫽ 289.1 kip-ft. This is less than the moment of 296 kip-ft carried by the steel in the unstrengthened case since the neutral axis has been moved downward in the strengthened beam (i.e., c ⫽ 5.58 in. versus c ⫽ 4.41 in.). Determine the factored moment capacity. Since the strain in the steel at failure is greater than 0.005, ⫽ 0.90 and Mn ⫽ 0.90(362.0) ⫽ 326.5 kip-ft ⬎ 321 kip-ft

Therefore, the assumed FRP strengthening system meets the desired future moment demand. The width of the FRP could be reduced slightly since the strengthening system is slightly overdesigned in this case (by 5.5 kip-ft or 1.7%). It can be shown that two layers of FRP 10.6 in. wide (Aƒ ⫽ 0.85 in2) will exactly meet the demand on 321 kip-ft. However, a 12-in.-wide FRP system, which is the same width as the beam itself, is much easier to apply in the ﬁeld than a system that is slightly narrower than the beam. Therefore, a 12-in.-wide FRP system should be chosen for constructability reasons. It is also important to note that the approximate design of step 5 (with a 9.5-in. width) would not have produced adequate moment capacity. The approximate calculation should be used as a guide, and detailed calculations must always be performed. A comparison of the approximate design of step

260

FRP FLEXURAL STRENGTHENING

5 with the ﬁnal design of step 7 is shown in Table 9.2. In addition, both serviceability and detailing checks are required for the system before it can be recommended for use. Note on the effect of existing strain on the substrate: Neglecting the effect of the existing strain, bi, in the concrete is not conservative. In the example given, if the existing strain were neglected in the design, the following results would be obtained: A ⫽ 40,800 lb/in. B ⫽ ⫺166,170 lb

(Note: Only the B term changes)

C ⫽ ⫺370,480 lb-in. which gives c ⫽ 5.67 in. ⬎ 5.58 in., ƒe ⫽ 0.00970 ⬎ 0.00929, ƒƒe ⫽ 52.0 ksi ⬎ 49.8 ksi, and Mn ⫽ 4383 kip-in. ⫽ 365 kip-ft ⬎ 362 kip-ft, in comparison to the values obtained when the existing strain was considered. That is, the calculation predicts a larger nominal moment capacity without the existing strain. Therefore, it is not conservative to neglect the existing strain on the substrate. However, it is also seen that the difference is very small in this particular example. Step 9. Detail the FRP ﬂexural strengthening system. Details of the FRP strengthening system must shown on the plans and in the speciﬁcations for an FRP strengthening systems. At the strip ends two empirical checks are required by ACI 440.2R-02 to assist with this detailing:

TABLE 9.2

Comparison of Estimated and Detailed Design Calculations

Design Method Approximate (Aƒ obtained from estimated c and fƒu) Detailed (based on Aƒ estimated from approximate method) Detailed (based on ﬁnal area selected) Detailed (based on area to exactly achieve the moment demand)

Effective Factored Moment Capacity, FRP Area, Depth of NA, Design Stress, fƒe (ksi) Aƒ (in2) c (in.) Mn (kip-ft) 0.76

4.41

54.72

⬇321

0.76

5.37

52.30

316.5 ⬍ 321 NG

0.96

5.58

49.79

326.5 ⬎ 321 OK

0.85

5.48

51.07

321

9.7

DESIGN PROCEDURE FOR A CONCRETE MEMBER

261

1. According to ACI 440.2R-02, the FRP ﬂexural strengthening system must extend a distance d beyond the point corresponding to the cracking moment under factored loads for a simply supported beam. Mcr ⫽

2ƒr Ig 2(530.3)(13,824) ⫽ ⫽ 610,906 lb-in. ⫽ 50.9 kip-ft h 24

wDL ⫽ 1.0 kip/ft wLL ⫽ 1.2(1.5) ⫽ 1.8 kip/ft Wu ⫽ 1.4(1.0) ⫹ 1.7(1.8) ⫽ 4.46 kip/ft Mu ⫽

4.46(24)2 ⫽ 321.1 kip-ft 8

(for comparison)

Determine the distance, x, along the beam from the support at which the moment is equal to the cracking moment, as shown in the free-body diagram in Fig. 9.8. Mx ⫽ Mcr ⫽ Rx ⫺ W →

4.46x2 4.46(24)x ⫺ ⫹ 50.9 ⫽ 0 2 2

x ⫽ 0.992 ft ⫽ 11.9. in ⬍ d (21.5 in.) Since insufﬁcient length is available to anchor the FRP strip, a supplementary anchorage system is required. 2. A capacity check is required at the strip end to prevent shear failure of the beam at the point of FRP strip termination. Check that the factored shear force at the FRP strip termination point is less than two-thirds of the concrete shear capacity at this point. Assuming, conservatively, that the FRP strip terminates at the support,

W = Wux 2/ 2

Mx x

R = WuL/ 2

Figure 9.8 Free-body diagram of beam at distance x from support.

262

FRP FLEXURAL STRENGTHENING

Vu ⫽ R ⫽ 4.46(12) ⫽ 53.5 kips Determine the concrete shear capacity: Vc ⫽ 2兹ƒc⬘ bd ⫽ 2兹5000 (12)(21.5) ⫽ 36,486 lb ⫽ 36.5 kips –23 Vc ⫽ 24.3 kips ⬍ 53.5 kips

This check also requires that the FRP be anchored at the support. A FRP U-wrap at the beam ends is generally used for this purpose (Spadea et al. 1998). Alternatively, proprietary ﬁber-anchors can be used to anchor the FRP strip Teng et al. (2001). In both cases, the strip should be extended as close as possible to the support. The length of the U-wrap should be at least equal to the depth of the beam. The U-wrap is detailed as follows: Provide a U-wrap of width equal to the depth of the beam (24 in. in this case) and use a minimum of two layers. If possible, use the same FRP material system as used for the FRP ﬂexural reinforcement. Apply the U-wrap FRP reinforcement at the same time as the FRP ﬂexural reinforcement (i.e., before the adhesive for the ﬂexural reinforcement has cured). Extend the U-wrap into the compression zone of the concrete. The corners of the beam should be rounded at the edges where the U-wrap is used (–12 in. minimum radius). Figure 9.9 shows the detailing design. If precured FRP laminates are used for the ﬂexural strengthening, a preformed FRP L shape (see Chapter 10) or a wet-layup system can be used to anchor the strip and prevent shear failure of the beam. Steel anchors, steel cover plates, or steel angles can also be used (Hollaway and Garden, 1998). It is advisable to attach the steel plates or angles with drilled expansion bolts

U-wrap (both ends)

h = 24 in.

FRP flexural strengthening layers (under the U-wrap)

b = 12 in.

(Gap shown for illustration purposes)

Figure 9.9 Details of FRP U-wrap at the end of the beam to anchor the FRP ﬂexural strengthening system.

9.7

DESIGN PROCEDURE FOR A CONCRETE MEMBER

263

and to use a ﬁller material (cementitious or resin based) to ensure good contact between the FRP and the cover plate. Holes for the expansion blots should be drilled through the FRP after it has cured. Option b: Four layers of the FRP system chosen with an estimated width of 4.75 in. (FRP failure mode). It has been determined (see Table 9.1) that the balanced condition will occur with four layers of the FRP system selected for a width of the FRP system equal to wƒ ⫽ 5.44 in. and a total FRP area of Aƒ ⫽ 0.87 in2. A trial design is performed with this amount of FRP reinforcement, which is greater than the original estimate of 0.76 in2 (4.75 in. width) based on the approximate calculation. However, recall that this estimate was shown in Table 9.2 to be rather inaccurate. For this design the theory predicts that the FRP will fail at exactly the same instant as the concrete will fail. If the FRP failure mode is to be guaranteed, an area of FRP smaller than 0.87 in2, consisting of four layers, should be selected. The unit stiffness of the FRP strengthening system and the bond-dependent coefﬁcient, m, for the four layers are determined as follows (data were shown in Table 9.1): nEƒtƒ ⫽ 4(5,360,000)(0.04) ⫽ 857,600 ⱕ 1,000,000 lb/in. and therefore m ⫽

冉

冊

冉

冊

nEƒtƒ 1 1 857,600 1⫺ ⫽ 1⫺ 60ƒu 2,000,000 60(0.0162) 2,000,000 ⫽ 0.588 ⱕ 0.90

and ƒe ⫽ mƒu ⫽ 0.588(0.0162) ⫽ 0.0095

ƒƒe ⫽ mƒƒu ⫽ 0.588(85.5) ⫽ 50.27 ksi The failure mode (mode 2a or 2b) must be determined to determine the moment capacity of the strengthened section. This requires ﬁnding the depth of the neutral axis and checking that the strains in the concrete, steel, and the FRP are compatible with the assumed failure mode. This can be determined directly from the equilibrium equations of the section. Start by assuming failure mode 2b,14 FRP failure before the steel has yielded. The characteristic equation to be solved for this assumed failure mode is

14 Mode 2b is checked ﬁrst in this example to demonstrate the solution procedure. Typically, mode 2a would be checked before mode 2b in an actual design and analysis procedure.

264

FRP FLEXURAL STRENGTHENING

(0.85ƒc⬘1b)c(h ⫺ c) ⫺ As Es(ƒe ⫹ bi)(d ⫺ c) ⫺ AƒEƒƒe(h ⫺ c) ⫽ 0 which can be written in the form Ac2 ⫹ Bc ⫹ C ⫽ 0 with A ⫽ 0.85ƒc⬘1b ⫽ 0.85(5)(0.80)(12) ⫽ 40.80 kips/in. B ⫽ ⫺[0.85ƒc⬘1bh ⫹ As Es(ƒe ⫹ bi) ⫹ AƒEƒƒe] ⫽ ⫺[0.85(5)(0.80)(12)(24) ⫹ 3.0(29,000)(0.0095 ⫹ 0.00061) ⫹ 0.87(5,360)(0.0095)] ⫽ ⫺1930.10 kips

C ⫽ As Es(ƒe ⫹ bi)d ⫹ AƒEƒƒeh ⫽ 3.0(29,000)(0.0095 ⫹ 0.00061)(21.5) ⫹ 0.87(5,360)(0.0095)(24) ⫽ 18,901.76 kip-in.

solving the quadratic equation and taking the positive root gives, c ⫽ 13.86 in. Now check if, in fact, the steel has not yielded (i.e., s ⬍ sy ⫽ 0.00207 for ƒy ⫽ 60 ksi). If it has yielded, the solution above is not valid! s ⫽ (ƒe ⫹ bi)

冉

冊

21.5 ⫺ 13.86 d⫺c ⫽ (0.0095 ⫹ 0.00061) h⫺c 24 ⫺ 13.86

⫽ 0.00762 ⬎ 0.00207

Therefore, the steel has in fact yielded and the solution for c is not valid! Now assume failure mode 2a, FRP failure after the steel has yielded. The characteristic equation for this case is linear, not quadratic, and is (0.85ƒ⬘c1b)c ⫺ Asƒy ⫺ Aƒmƒƒu ⫽ 0 which gives c⫽

Asƒy ⫹ Aƒmƒƒu 3.0(60) ⫹ 0.87(0.588)(85.5) ⫽ ⫽ 5.484 in. 0.85ƒc⬘1b 0.85(5)(0.80)(12)

which is equal to the value of cb found previously since the area of the FRP chosen is exactly equal to that which gives the balanced condition.

9.7

DESIGN PROCEDURE FOR A CONCRETE MEMBER

265

Now check that the steel has yielded: s ⫽ (ƒe ⫹ bi)

冉

冊

d⫺c 21.5 ⫺ 5.484 ⫽ (0.0095 ⫹ 0.00061) h⫺c 24 ⫺ 5.484

⫽ 0.0087 ⱖ sy ⫽ 0.00207

Therefore, the steel has yielded and the assumed failure mode is applicable. The strain in the concrete is c ⫽ (ƒe ⫹ bi)

c h⫺c

冉

⫽ (0.0095 ⫹ 0.00061)

冊

5.484 21.5 ⫺ 5.484

⫽ 0.003 ⫽ cu

This conﬁrms that a balanced failure occurs for the chosen value of Aƒ. The nominal moment capacity is obtained as

冉

Mn ⫽ Asƒy d ⫺

冉

冊

冉 冊 冊

1c c ⫹ ƒ Aƒƒƒe h ⫺ 1 2 2

⫽ 3.0(60) 21.5 ⫺

0.8(5.484) 2

冋

⫹ 0.85(0.87)(50.27) 24 ⫺

册

0.8(5.484) 2

⫽ 4285 kip-in. ⫽ 357 kip-ft

and the factored moment capacity is given as Mn ⫽ (0.9)(357) ⫽ 321.3 kip-ft ⬎ 321 kip-ft

which meets the strengthening demand. Discussion A comparison of the results for options a and b is presented in Table 9.3. However, if option a with a width of 10.6 ln is chosen (see pg. 259) the identical capacity can be achieved with the same area of FRP for either two or four layers of the material (small differences are due to numerical roundoff). However, the failure is controlled by different mechanisms. If slightly less than the balanced area was chosen for the four-layer system, FRP failure would control. However, the balanced condition was chosen to demonstrate this special case. This is not surprising if one observes that the overreinforced

266

FRP FLEXURAL STRENGTHENING

TABLE 9.3

Comparison of the results of Example 9.1 Options a and b Factored Moment Capacity, Mn (kip-ft)

FRP FRP Depth Width, Area, Stress at of NA, wƒ Aƒ Failure, c (in.) Option Layers (in.) (in2) fƒe (ksi) a 9.1

2 2

12.0 10.6

0.96 0.85

49.79 51.07

5.58 5.477

9.2

4

5.4

0.87

50.27

5.484

Failure Mode

326.5 Concrete 320.9 (⬃ 321) Concrete (and FRP) 321.3 (⬃ 321) FRP (and concrete)

case with concrete failure or the underreinforced case with FRP failure use the identical equation for determining the nominal moment shown previously:

冉

Mn ⫽ Asƒy d ⫺

冊

冉

冊

1c c ⫹ ƒ Aƒƒƒe h ⫺ 1 2 2

(ACI 440.2R-02:9-11)

9.8 SERVICEABILITY OF FRP-STRENGTHENED FLEXURAL MEMBERS Under service loads the ACI 440.2R-02 guide requires the designer to check that the stresses in the existing steel and the FRP do not exceed speciﬁc limits to prevent failure of the strengthened beam due to creep and fatigue effects. In the service load range, a cracked elastic section analysis is used to determine the service load stresses. This is similar to conventional service load analysis of reinforced concrete members with an additional requirement. In the strengthened state the contribution of the FRP strengthening system is included in the cracked elastic section properties. No speciﬁc requirements are given for deﬂections or crack control under service loads. The appropriate cracked section properties are used to determine service load deﬂections in FRP-strengthened beams. In general, the contribution of the FRP strengthening to the stiffness of the section in the service load range is rather small. 9.8.1

Cracked FRP Strengthened Section

To analyze the stresses and strains in the section that has been strengthened, the properties of the cracked section with the FRP strengthening system attached are required. The strain distribution, stress distribution, and force resultants in the service load range are shown in Fig. 9.10. To calculate the properties of the cracked FRP-strengthened section, the transformed section method may be used or the composite section method may be used.

9.8

267

SERVICEABILITY OF FRP-STRENGTHENED FLEXURAL MEMBERS

εc

fc

− c2 = k2d h

C = 0.5 fc c2b

2c2 / 3

d

As

+ εs

fs

Ts = As fs

Af

εbi εfe

ffe

Tf = Af ffe

b

Figure 9.10 Strains, stresses, and force resultants in the service load range.

Method 1: Using the Transformed Section Since three different materials are present in the section, both the steel and the FRP must be transformed to the modulus of the concrete and two modular ratios are deﬁned, s ⫽ Es /Ec and ƒ ⫽ Eƒ /Ec, the steel-to-concrete modular ratio and the FRP-to-concrete modular ratio, respectively. The neutral-axis depth ratio, k2 ⫽ c2 /d, is then given as k2 ⫽

冪( ⫹ ) ⫹ 2冉 ⫹ hd冊 ⫺ ( ⫹ ) 2

s

s

ƒ

ƒ

s

s

ƒ

ƒ

s

s

ƒ

ƒ

(9.59)

and

冉 冊

bd 3 3 h (Icr)2 ⫽ k ⫹ sAsd 2(1 ⫺ k2)2 ⫹ ƒ Aƒ d 2 ⫺ k2 3 2 d

2

(9.60)

Method 2: Using Composite Section Mechanics Following the procedure described in Chapter 5, the distance from the top of the section to the neutral axis, shown in Fig. 9.11, is found from Ecb

(c2)2 ⫹ Es As(c2 ⫺ d) ⫹ Eƒ Aƒ(c2 ⫺ h) ⫽ 0 2

(9.61)

Solving the quadratic equation and taking the positive root gives the value of c2. The ﬂexural stiffness (EI) of the strengthened section is given as (EI)2 ⫽

冘EI ⫽ E I ⫹ E I ⫹ E I ⫽ E b(c3 ) ⫹ E A (d ⫺ c ) 3

2

c c

⫹ Eƒ Aƒ(h ⫺ c2)2

and

s s

ƒ ƒ

c

2

s

s

2

(9.62)

268

FRP FLEXURAL STRENGTHENING

Ec

y

c2 Neutral axis

h

d Es

Ef

Figure 9.11 Properties of a strengthened section for determination of the neutral axis.

(Icr)2 ⫽

9.8.2

(EI)2 Ec

(9.63)

Service-Level Stress in the Internal Steel Reinforcing Bars

ACI 440.2R-02 limits the service-level stresses in the internal steel reinforcing bars in the strengthened reinforced concrete member as follows: ƒs,s ⱕ 0.80ƒy

(9.64)

This is to prevent yielding of the internal steel and to decrease the likelihood of fatigue failure of the internal steel rebars under service loads in the strengthened section. When the internal steel yields, the ﬂexural stiffness of the beam decreases signiﬁcantly and large, undesirable deﬂections will occur in the structure at service loads. Since the steel internal reinforcing bars are subjected to stress and strain both before and after the FRP strengthening system is applied, the stress and strain is composed of two distinct stages, as shown in Fig. 9.6. The strains in these two stages of the loading are denoted as follows: s1: the strain in the steel due to the existing loads (usually, the dead loads

only) at the time that the FRP is applied s2: the strain in the steel due to the supplemental applied loads after the FRP has been attached In the unstrengthened beam (stage 1 of the loading),

9.8

SERVICEABILITY OF FRP-STRENGTHENED FLEXURAL MEMBERS

s1 ⫽ b1 b1 ⫽

d ⫺ c1 h ⫺ c1

m1(h ⫺ c1) m1(h ⫺ c1) ⫽ (Icr)1Ec (EI)1

269

(9.65) (9.66)

and the corresponding stress is ƒs1 ⫽ Ess1

(9.67)

or given directly as ƒs1 ⫽

Esm1(d ⫺ c1) (EI)1

(9.68)

where m1 is the moment due to the existing loads at the time the FRP is attached and c1 is the depth of the neutral axis in the unstrengthened beam. Also, recall that b1 is equal to bi, which has previously been described as the strain in the substrate when the FRP is attached. In the strengthened beam (stage 2 of the loading), s2 ⫽ b2 b2 ⫽

d ⫺ c2 h ⫺ c2

m2(h ⫺ c2) m2(h ⫺ c2) ⫽ (Icr)2Ec (EI)2

(9.69) (9.70)

and the corresponding stress is ƒs2 ⫽ Ess2

(9.71)

or given directly as ƒs2 ⫽

Esm2(d ⫺ c2) (EI)2

(9.72)

where m2 is the moment due to the supplemental loads after the FRP has been attached and c2 is the depth of the neutral axis in the strengthened beam. Therefore, the total stress in the internal steel at the service loads (i.e., the loads that existed on the structure at the time that the FRP was attached plus

270

FRP FLEXURAL STRENGTHENING

the loads that are applied to the structure after the FRP was attached15) is given by ƒs,s ⫽ ƒs1 ⫹ ƒs2

(9.73)

or it can be determined directly from ƒs,s ⫽

[(m1 ⫺ m2) ⫹ bi AƒEƒ(h ⫺ k2d/3)](d ⫺ k2d)Es As Es(d ⫺ k2d/3](d ⫺ k2d) ⫹ AƒEƒ[h ⫺ k2d/3)(h ⫺ k2d) (ACI 440.2R-02:9-12)

where k2 ⫽ c2 /d is the ratio of the depth of the neutral axis to the effective depth of the strengthened section (denoted as c2 above). 9.8.3

Service-Level Stresses in the FRP Strengthening System

The loading combination for this FRP stress check is that due to all sustained loads on the structure and the maximum load effect of the cyclic loads on the structure that could lead to fatigue failure. The stress limits for the FRP strengthening system are given in Table 8.2. Since the FRP system is subjected to loading only in stage 2, after the FRP has been applied, the moment used in computing the strains and stresses is equal to the sustained load on the beam after the load has been applied, in addition to the load causing the fatigue moment on the beam, designated previously as m2.16 The strains in the FRP are therefore given as ƒ2 ⫽ b2 b2 ⫽

(9.74)

m2(h ⫺ c2) m2(h ⫺ c2) ⫽ (Icr)2 Ec (EI)2

(9.75)

and the corresponding stress is ƒƒ2 ⫽ Eƒƒ2

(9.76)

or given directly as

15 Note that this assumes that the load that existed on the beam when the FRP was attached remains on the beam after the FRP has been attached. 16 It is possible that the moment m2 that is used to determine the stress in the steel in stage 2 will not be the same as the sustained load plus maximum moment due to the cyclic load, but usually these are assumed to be the same.

9.9

ƒƒ2 ⫽

LOAD–DEFLECTION RESPONSE

Eƒm2(d ⫺ c2) (EI)2

271

(9.77)

Therefore, the stress, ƒƒ,s, in the FRP at service is given as ƒƒ,s ⫽ ƒƒ2

(9.78)

This stress can be calculated directly as ƒƒ,s ⫽

Eƒ m2(h ⫺ c2) (EI)2

(9.79)

Alternatively, the stress in the FRP can be determined directly from the stress in the steel, Eƒ h ⫺ k2d ƒƒ,s ⫽ ƒs,s ⫺ biEƒ Es d ⫺ k2d

(ACI 440.2R-02:9-13)

where k2 ⫽ c2 /d is the ratio of the depth of the neutral axis to the effective depth of the strengthened section (denoted as c2 above), and the steel stress, ƒs,s, is computed for the full service load moment m1 ⫹ m2.

9.9 LOAD–DEFLECTION RESPONSE OF FRP-STRENGTHENED FLEXURAL MEMBERS The load–deﬂection response of an FRP-strengthened ﬂexural member needs to be determined to ensure that serviceability deﬂection criteria are not violated by the strengthened beam under the increased loads. The load–deﬂection response of an FRP-strengthened member can be divided into a number of stages (regimes). Only the increasing (positive stiffness) load–deﬂection response to failure of the strengthened beam is considered in this section. The post-peak load–deﬂection response is not discussed and is beyond the scope of this book. At a ﬁrst approximation, the increasing load–deﬂection response can be divided into three signiﬁcant stages: (1) the linear elastic deﬂection at the time the FRP is applied, (2) the linear elastic deﬂection after the FRP has been applied up to the time the internal steel yields (assuming that the internal steel yields before the member fails in ﬂexure), and (3) the nonlinear inelastic deﬂection from the time the steel yields until the FRP-strengthened beam fails due to concrete crushing or FRP failure. The ﬂexural stiffness, (EI)i, in each of these stages is used to determine the load–deﬂection response in an incremental fashion.

272

FRP FLEXURAL STRENGTHENING

The ﬂexural stiffnesses, (EI)1 and (EI)2 and the cracked transformed second moments (Icr)1 and (Icr)2 for stages (1) and (2) were derived previously. It is assumed that the beam is cracked prior to loading in the ﬁrst stage and therefore that there is no precracking stage in the load–deﬂection response of an FRP-strengthened beam (Arduini and Nanni, 1997; Buyukotzurk and Hearing, 1998). The effective second moment of a concrete beam for deﬂection is generally taken to be that given by the classical Branson equation,

冉 冊 冋 冉 冊册

Mcr Ie ⫽ Ma

3

Ig ⫹ 1 ⫺

Mcr Ma

Icr ⱕ Ig

(9.80)

The Branson equation can be assumed to be a reasonable approximation for the ﬁrst and second stages of the load–deﬂection response since the beam stiffness in these stages is not affected signiﬁcantly by the FRP (El-Mihilmy and Tedesco, 2000). It is also assumed that the response of the cracked section either before or after the FRP has been applied is linear elastic. This implies that the concrete modulus remains constant and equal to its initial value up to yielding of the internal steel. For low steel reinforcement ratios for which ﬂexural strengthening is usually most effective, this assumption is reasonable. The ﬂexural stiffness in the third nonlinear inelastic stage after the internal steel has yielded can be approximated as a linear elastic stage for the purposes of obtaining an estimate of the deﬂection at ultimate load. Since in this stage the concrete stress–strain response is nonlinear and the steel is possibly hardening, it is most appropriate to approach this with a full incremental nonlinear analysis. However, some simplifying assumptions can be made: (1) After the steel has yielded, the steel modulus is set to zero (i.e., perfectly elastoplastic response); (2) after the steel has yielded, the concrete modulus is taken as 50% of its initial modulus (this is reasonable for the range of concrete strain from 0.001 to 0.002, which is the concrete strain for most of this stage),17 and (3) after the steel yields strain, the compatibility between the FRP and the concrete substrate remains in effect even though the cover concrete may be cracked signiﬁcantly. The ﬂexural stiffness (EI)3 and the cracked transformed second moment (Icr)3 for the third stage can be found using the composite mechanics method following the procedure described for the second stage. The distance from the top of the section to the neutral axis, c3, is found from Ec (c3)2 b ⫹ Eƒ Aƒ(c3 ⫺ h) ⫽ 0 2 2

(9.81)

Solving the quadratic equation and taking the positive root gives the value of c3. The ﬂexural stiffness (EI)3 of the strengthened section is given as 17 In reality, this will not make much of a difference in the nonlinear range since the concrete contribution to the stiffness is quite small.

9.9

(EI)3 ⫽

LOAD–DEFLECTION RESPONSE

273

冘 EI ⫽ E I ⫹ E I ⫽ E2 b(c3 ) ⫹ E A (h ⫺ c )

(9.82)

(EI)3 (Ec /2)

(9.83)

3

c

c c

ƒ ƒ

3

2

ƒ

ƒ

3

and (Icr)3 ⫽

Design Example 9.2: Serviceability of an FRP-Strengthened Beam Consider the same geometry and loading as the beam discussed earlier in this chapter in option a of the strength design. Determine (a) The stresses in the steel and the FRP under service loads, and (b) the midspan deﬂection of the strengthened beam under full dead and live loads. The pertinent properties of the beam and FRP system are: ƒƒu ⫽ CEƒ* ƒu ⫽ 0.95(90) ⫽ 85.5 ksi

wƒ ⫽ 12 in.

ƒu ⫽ CEƒu * ⫽ 0.95(0.017) ⫽ 0.0162

bi ⫽ 0.00061

Eƒ ⫽ 5360 ksi

Ec ⫽ 4030 ksi

tƒ ⫽ 0.04 in.

Es ⫽ 29,000 ksi

SOLUTION (a) Stresses in the steel and the FRP under service loads Determine the unfactored service loads. The dead load that acts on the beam at the time the FRP is attached, wDL ⫽ 1.0 kip/ft The dead load plus the new live load that act on the FRP strengthened beam, wDL ⫽ 1.0 kip/ft

wLL⫽ 1.8 kip/ft

Determine the service loads and moments for the original and strengthened sections. Original section: m1 ⫽ mDL ⫽ Strengthened section:

wDLL2 1.0(24)2 ⫽ ⫽ 72 kip-ft ⫽ 864,000 lb-in. 8 8

274

FRP FLEXURAL STRENGTHENING

m2 ⫽ mLL ⫽

wLLL2 1.8(24)2 ⫽ ⫽ 129.6 kip-ft ⫽ 1,555,200 lb-in. 8 8

m1 ⫹ m2 ⫽ 2,419,200 lb-in. Determine the properties of the unstrengthened and strengthened sections. The properties of the original unstrengthened section were determined as follows: c1 ⫽ 7.18 in. k1 ⫽ 0.334

Ec ⫽ 4030 ksi (EI)1 ⫽ 2.38 ⫻ 1010 lb-in2

(Icr)1 ⫽ 5909 in4 The properties of the strengthened section are calculated using method 2, composite mechanics. The distance from the top of the section to the neutral axis is Ecb

(c2)2 ⫹ Es As(c2 ⫺ d) ⫹ Eƒ Aƒ(c2 ⫺ h) ⫽ 0 2

4.030(12)

(c2)2 ⫹ 29(3.0)(c2 ⫺ 21.5) ⫹ 5.36(0.96)(c2 ⫺ 24) ⫽ 0 2

24.18(c2)2 ⫹ 92.15c2 ⫺ 1993.49 ⫽ 0 Solving the quadratic equation and taking the positive root gives c2 ⫽ 7.37 in.

and k2 ⫽

c2 ⫽ 0.343 in. d

(Compare with original section of values of c1 ⫽ 7.18 in. and k1 ⫽ 0.334.) The ﬂexural stiffness (EI)2 of the section is obtained from (EI)2 ⫽

冘 EI ⫽ E I ⫹ E I ⫹ E I ⫽ E b(c3 )

3

2

c c

s s

ƒ ƒ

c

⫹ EsAs(d ⫺ c2)2 ⫹ Eƒ Aƒ(h ⫺ c2)2

冉

⫽ (4.030 ⫻ 106)

冊

12(7.37)3 ⫹ (29 ⫻ 106)(3.0)(21.5 ⫺ 7.37)2 3

⫹ (5.360 ⫻ 106)(24 ⫺ 7.37)2 ⫽ 2.52 ⫻ 1010 lb-in2 ⬎ 2.38 ⫻ 1010 lb-in2

which gives

9.9

LOAD–DEFLECTION RESPONSE

275

(EI)2 2.52 ⫻ 1010 ⫽ ⫽ 6253 in4 ⬎ 5909 in4 Ec 4,030,000

(Icr)2 ⫽

It is interesting to note that the ﬂexural stiffness has only increased by 5.9% in the elastic range due to the addition of the FRP. This implies that the FRP has a small effect on the deﬂections of the beam under the service load in this example. Determine the stresses in the steel under service loads. Determine the strains and stress in the steel when the FRP is attached (stage 1) and after the FRP has been attached (stage 2). Stage 1:

冉

冊

21.5 ⫺ 7.18 d ⫺ c1 ⫽ 0.00061 ⫽ 0.00052 h ⫺ c1 24 ⫺ 7.18

s1 ⫽ bi

and the corresponding stress is ƒs1 ⫽ Ess1 ⫽ (29,000,000)(0.00052) ⫽ 15,080 psi This can also be calculated directly from ƒs1 ⫽ ⫽

Esm1(d ⫺ c1) (EI)1 29,000,000(864,000)(21.5 ⫺ 7.18) ⫽ 15,076 ⬇ 15,080 psi 2.38 ⫻ 1010

Stage 2: ƒs2 ⫽ ⫽

Esm2(d ⫺ c2) (EI)2 29,000,000(1,555,200)(21.5 ⫺ 7.37) ⫽ 25,367 psi 2.52 ⫻ 1010

Therefore, the stress in the steel at service loads is ƒs,s ⫽ ƒs1 ⫹ ƒs2 ⫽ 15,076 ⫹ 25,367 ⫽ 40,443 psi ⫽ 40.4 ksi or calculate directly from

276

FRP FLEXURAL STRENGTHENING

ƒs,s ⫽

[(m1 ⫹ m2) ⫹ bi AƒEƒ(h ⫺ k2d/3)](d ⫺ k2d)Es As Es(d ⫺ k2d/3)(d ⫺ k2d) ⫹ AƒEƒ(h ⫺ k2d/3)(h ⫺ k2d)

k2d ⫽ c2 ⫽ 7.37 in. mDL ⫹ mLL ⫽ 864 ⫹ 1555.218 ⫽ 2419.2 kip-in. [2419.2 ⫹ 0.00061(0.96)(5360)(24 ⫺ 7.37/3)](21.5 ⫺ 7.37)29,000 ƒs,s ⫽ 3(29,000)(21.5 ⫺ 7.37/3)(21.5 ⫺ 7.37) ⫹ 0.96(5360)(24 ⫺ 7.37/3)(24 ⫺ 7.37/3) ⫽ 40.4 ksi

Check the stress limits for the steel. ƒs,s ⱕ 0.80ƒy Substituting values gives ƒs,s ⫽ 40.4 ksi ⬍ 0.8ƒy ⫽ 0.8(60) ⫽ 48 ksi Therefore, the stress in the steel as service loads is OK. Determine the stresses in the FRP under service loads. ƒƒ,s ⫽

Eƒm2(h ⫺ c2) 5360(1,555,200)(24 ⫺ 7.37) ⫽ ⫽ 5.50 ksi (EI)2 2.52 ⫻ 1010

or calculate directly from Eƒ h ⫺ k2d ƒƒ,s ⫽ ƒs,s ⫺ biEƒ Es d ⫺ k2d

冉 冊冉

⫽ 40.4

5360 29,000

冊

24 ⫺ 7.37 ⫺ 0.00061(5360) 21.5 ⫺ 7.37

⫽ 5.51 ksi

Check the stress limits for the FRP. For the carbon–epoxy FRP strengthening system chosen, the limiting stress is

In the example in ACI440.2R-02, this has been rounded to 130 kip-ft ⫽ 1560 kip-in., and hence the total moment is given as 2424 kip-in. This explains the slight difference in the ﬁnal values.

18

9.9

LOAD–DEFLECTION RESPONSE

277

ƒƒ,s ⬍ 0.55ƒƒu Substituting gives 5.51 ksi ⬍ 50 ksi ⫽ 0.55(85.0) Therefore, the stress in the FRP at service loads is OK. (b) Midspan deﬂection of the strengthened beam under full dead and live loads Determine the ﬂexural stiffnesses and cracked transformed second moments for the three stages of load–deﬂection response. For stages 1 and 2 these have been determined previously as (EI)1 ⫽ 2.38 ⫻ 1010 lb-in2

(Icr)1 ⫽ 5909 in4

Ec ⫽ 4030 ksi

(EI)2 ⫽ 2.52 ⫻ 1010 lb-in2

(Icr)2 ⫽ 6253 in4

Mcr ⫽ 610,906 lb-in.

The ﬂexural stiffness (EI)3 of the section is obtained from Ec (c3)2 b ⫹ Eƒ Aƒ(c3 ⫺ h) 2 2 ⫽

4.030 (c )2 (12) 3 ⫹ 5.360(0.96)(c3 ⫺ 24) 2 2

⫽ 12.09(c3)2 ⫹ 5.15c3 ⫺ 123.49 ⫽ 0

Solving the quadratic equation and taking the positive root gives c3 ⫽ 2.990 in. Note how shallow the compression block is in the third stage! The ﬂexural stiffness (EI)3 of the strengthened section is given as (EI)3 ⫽ 兺 EI ⫽

Ec I ⫹ EƒIƒ 2 c

⫽

Ec b(c3)3 ⫹ Eƒ Aƒ(h ⫺ c3)2 2 3

⫽

(4.030 ⫻ 106)(12)(2.990)3 2(3) ⫹ (5.36 ⫻ 106)(0.96)(24 ⫺ 2.990)2

⫽ 2.49 ⫻ 109 lb-in2

and

278

FRP FLEXURAL STRENGTHENING

(Icr)3 ⫽

(EI)3 (2.49 ⫻ 109) ⫽ ⫽ 1236 in4 Ec /2 4.030 ⫻ 106 /2

The load–deﬂection curve can now be constructed using either the values of the ﬂexural stiffness, (EI)i, calculated above or using the Branson formula with the values of (Icr)3. Both methods are used in the example. Method 1: Using the theoretical ﬂexural stiffness To construct the piecewise linear load–deﬂection curve, the applied moments and the maximum deﬂection are required at the beginning and end of each stage. For stage 1, prior to the FRP being applied, the applied load is 1 kip/ft ⫽ 83.3 lb/in., and the maximum moment is m1 ⫽

w1ᐉ2 83.3(24 ⫻ 12)2 ⫽ ⫽ 864,000 lb-in. 8 8

The deﬂection corresponding to this moment is ␦1 ⫽

冉

冊

5 w1ᐉ4 5 83.3(228)4 ⫽ ⫽ 0.314 in. 384 (EI)1 384 2.38 ⫻ 1010

For stage 2 the moment (and distributed load) in the strengthened beam when the steel yields is ﬁrst calculated using ƒs2 ⫽

Esmy(d⫺ c2) (EI)2

rearranged as my ⫽ ⫽

(ƒy ⫺ ƒs1)(EI)2 Es(d ⫺ c2) (60,000 ⫺ 15,076)(2.52 ⫻ 1010) ⫽ 2,762,732 lb-in. (29,000,000)(21.5 ⫺ 7.37)

and wy ⫽ ␦y ⫽

8my ᐉ

2

⫽

8(2,762,732) ⫽ 266.5 lb/in. (288)2

5 wyᐉ4 5 266.5(228)4 ⫽ ⫽ 0.9473 in. 384 (EI)2 384 2.52 ⫻ 1010

At yielding of the internal steel, the total moment applied, total load applied, and total midspan deﬂection of the beam are 3,626,732 lb-in., 349.8 lb/in. (4.12 kip/ft), and 1.261 in., respectively.

9.9

LOAD–DEFLECTION RESPONSE

279

The deﬂection at the design service loads occurs in stage 2 and is computed using the equations above but substituting the service load, which is 1.8 kips/ft (150 lb/in.), and corresponds to a moment of 1,555,200 lb-in. This deﬂection is equal to ␦2 ⫽

冉

冊

5 w2ᐉ4 5 150(228)4 ⫽ ⫽ 0.533 in. 384 (EI)2 384 2.52 ⫻ 1010

and the total service load deﬂection is equal to 0.847 in. This corresponds to a deﬂection ratio of L 288 ⫽ ⫽ 340 ⬍ 360 ␦ 0.847 which implies that the deﬂection of the strengthened beam would exceed a typical allowable deﬂection ratio of 360 (using the constant cracked section properties). For stage 3, the nominal moment at ultimate failure (without the FRP reduction factor, ƒ) and the ultimate deﬂection are calculated using the approximated properties of the third stage as follows:

冉

mmax ⫽ 3.0(60,000) 21.5 ⫺

冊

冉

冊

4.46 4.46 ⫹ 0.96(49,790) 24 ⫺ 2 2

⫽ 3468.6 ⫹ 1040.6 ⫽ 4,509,200 lb-in.

This can be compared with Mn ⫽ 4,352,000 lb-in determined previously in the strength analysis of this beam. The moment increment in the third stage is therefore equal to ⌬m3 ⫽ 4,509,200 ⫺ 3,626,731 ⫽ 883,171 lb-in.

which corresponds to a load increment of ⌬w3 ⫽

8⌬m3 ᐉ

2

⫽

8(883,171) ⫽ 85.2 lb/in. (288)2

and a deﬂection increment of ⌬␦3 ⫽

冉

冊

5 ⌬w3ᐉ4 5 85.2(228)4 ⫽ ⫽ 3.065 in. 384 (EI)3 384 2.49 ⫻ 109

At ultimate load the total moment applied, total load applied, and total midspan deﬂection of the beam are 4,509,200 lb-in., 435 lb/in. (5.22 kips/ ft), and 4.326 in., respectively. The cumulative predicted load–deﬂection be-

280

FRP FLEXURAL STRENGTHENING

havior of the beam, using the assumption of a constant cracked section stiffness in each stage, is shown in Fig. 9.12. Method 2: Using the Branson-modiﬁed ﬂexural stiffness When the Branson formula approach is used, the steps in the procedure are very similar except that the ﬂexural stiffness (EI)i in each stage is replaced by (EcIe)i. Since Ie is a function of the moment applied at any given instant, the lines in the load– deﬂection plots will no longer be straight lines in any of the stages but rather, will be curves. These curves can be constructed using a speadsheet program and incrementing the moment in each stage. In the interests of brevity, only the key points in the load–deﬂection curve (i.e., FRP attachment, service load, steel yielding, and ultimate load) will be computed in this example. Stage (1): (Icr)1 ⫽ 5909 in4 At FRP attachment:

冉 冊 冋 冉 冊册 冉 冊 冋 冉 冋 3

(Ie)1 ⫽

Mcr Mcr I ⫹ 1⫺ Ma g Ma

3

(Icr)1

冊册 册

3

⫽

␦1 ⫽

610,906 610,906 (13,824) ⫹ 1 ⫺ 864,000 864,000

3

(5909) ⫽ 8717 in4

5 w1ᐉ4 5 83.3(288)4 ⫽ ⫽ 0.212 in. 384 Ec(Ie)1 384 (4.03 ⫻ 106)(8717)

5000 3626 kip-in. 1.261 in. Steel yields

Maximum Moment (kip-in.)

4500 4000

4509 kip-in. 4.326 in. Ultimate load

3500 3000 2419 kip-in. 0.847 in. Service load

2500 2000 1500

864 kip-in. 0.314 in. FRP attached

1000 500 0 0

1

2

3

4

5

Midspan Deflection (in.)

Figure 9.12 Load–deﬂection curve using the theoretical ﬂexural stiffness.

9.9

LOAD–DEFLECTION RESPONSE

281

Stage (2) (Icr)2 ⫽ 6253 in4 At service load:

冉 冊 冋 冉 冊册 冉 冊 冋 冉 冋 3

Mcr Mcr ⫽ I ⫹ 1⫺ Ma g Ma

(Ie)2(service)

3

(Icr)2

3

⫽

␦2 ⫽

冊册 3

610,906 610,906 (13,824) ⫹ 1 ⫺ 2,419,200 2,419,200

册

(6253) ⫽ 6375 in4

5 w2ᐉ4 5 150(288)4 ⫽ ⫽ 0.5230 in. 384 Ec(Ie)2 384 (4.03 ⫻ 106)(6375)

Therefore, ␦service ⫽ 0.212 ⫹ 0.5230 ⫽ 0.7350 in., and L 288 ⫽ ⫽ 392 ⬎ 360 ␦ 0.7350

OK!

At steel yielding:

冉 冊 冋 冉 冊册 冉 冊 冋 冉 冊册 冋 册 3

(Ie)2(final) ⫽

Mcr Mcr Ig ⫹ 1 ⫺ Ma Ma

3

Icr

3

⫽

␦2(final) ⫽

3

610,906 610,906 (13,824) ⫹ 1 ⫺ 3,626,732 3,626,732

(6253) ⫽ 6319 in4

5 w2ᐉ4 5 116.5(288)4 ⫽ ⫽ 0.410 in. 384 Ec(Ie)2 384 (4.03 ⫻ 106)(6,319)

Therefore, ␦yielding ⫽ 0.212 ⫹ 0.5230 ⫹0.410 ⫽ 1.145 in. Stage (3) (Icr)3 ⫽ 1236 in4 Ie3(final) ⫽

冉 冊 冋 冉 冊册 冉 冊 冋 冉 冊册 冋 册 Mcr Ma

3

Ig ⫹ 1 ⫺ 3

⫽

␦3(final) ⫽

Mcr Ma

3

(Icr)3

610,906 610,906 (13,824) ⫹ 1 ⫺ 4,509,200 4,509,200

3

(1236) ⫽ 1267 in4

5 w3ᐉ4 5 85.2(288)4 ⫽ ⫽ 2.990 in. 384 Ec(Ie)3 384 (2.02 ⫻ 106)(1267)

Therefore, ␦ultimate ⫽ 0.212 ⫹ 0.5230 ⫹ 0.410 ⫹ 2.990 ⫽ 4.135 in.

282

FRP FLEXURAL STRENGTHENING

Maximum Moment (kip-in.)

5000 4500 4000 3500 3000 2500 2000 1500

EI

1000

Branson

500 0 0

1

2

3

4

5

Midspan Deflection (in.)

Figure 9.13 Comparison between theoretical and modiﬁed Branson load–deﬂection curves.

The load–deﬂection response using the Branson EI method is shown together with the theoretical EI method in Fig. 9.13. It can be seen that there is a small difference between the predictions using the Branson equations and the cracked section EI. However, this small difference in the service load can be signiﬁcant in meeting serviceability design objectives (e.g., a L/360 deﬂection criterion), as shown in this example. PROBLEMS 9.1

For the FRP strengthening systems19 in Table P9.1,20 calculate the bond-dependent coefﬁcient, m, for one, two, three, and four layers (plies) of the system.

9.2

The FRP strengthening systems in Table P9.1 are considered for strengthening an interior reinforced concrete beam with the following properties and loads: L ⫽ 16 ft, b ⫽ 10 in., h ⫽ 16 in., d ⫽ 13.5 in., ƒ⬘c ⫽ 3500 psi, ƒy ⫽ 40,000 psi, two No. 8 bars, dead load⫽ 400 lb/ ft, and live load ⫽ 800 lb/ft. Consider one, two, three, and four layers

19

Instructors may assign selected systems for homework problems. Properties reported in this table are design properties provided by manufacturers in their current (2006) online speciﬁcation sheets and do not necessarily conform to the deﬁnition of the guaranteed property values in ACI 440.2R-02. They are assumed to be guaranteed properties for the purposes of these problems. For actual design, the user should obtain current guaranteed properties from manufacturers. These data can be compared with those obtained by the reader for Problems 8.2 and 8.3. 20

PROBLEMS

TABLE P9.1

283

FRP Strengthening Systems

No.

Fiber

FRP Strengthening System

1 2 3 4

Glass Glass Carbon Carbon

5

Glass

SikaWrap Hex 100G (laminate property) Tyfo SEH 51 (laminate property) WaboMbrace CF130 (ﬁber property) Sika Carbodur laminate (laminate property) Tyfo UG composite laminate (laminate property)

ƒ* ƒu (ksi)

E* ƒ (Msi)

tƒ (in.)

81.0 66.7 550.0 406.0

3.55 3.03 33.0 23.9

0.040 0.050 0.0065 0.047

130.0

6.0

0.055

of the given system. Assume that only the dead load (and self-weight) act on the beam when the FRP strengthening system is applied. Determine if the inelastic balanced reinforcement ratio can be achieved, and if so, its value. Why is the situation of not being able to achieve the balanced ratio not an issue with regard to traditional steel reinforcing? 9.3

Derive an expression [analogous to equation (9.54)] for the ‘‘elastic’’ balanced reinforcement ratio for an FRP-strengthened beam when the tension steel has not yielded in the section when a balanced condition is achieved.

9.4

Given an interior simply supported reinforced concrete beam with the following properties and loads: L ⫽ 16 ft, b ⫽ 10 in., h ⫽ 16 in., d ⫽ 13 in., ƒ⬘c ⫽ 3500 psi, ƒy ⫽ 40,000 psi, two No. 8 bars, dead load ⫽ 300 lb/ft, and live load ⫽ 500 lb/ft. The beam is to be strengthened to increase its live-load carrying capacity. Consider the following strengthening alternatives: two layers each 10 in. wide, of the FRP sheet or fabric systems listed in Table P9.1 (systems 1 to 3) or two strips each 4 in. wide placed side by side of the FRP laminate systems in Table P9.1 (systems 4 and 5). Assume that only the dead load (and self-weight) act on the beam when the FRP strengthening system is applied. Determine (a) the nominal and factored moment capacity of the strengthened beam, and (b) the live-load capacity of the beam when it is strengthened. Compare the strengthening capabilities of the various systems.

9.5

Determine the factored moment capacity of the beam in Design Example 9.1 if ﬁve layers each 9.5 in. wide, of the FRP system are used. Find the required area and width of FRP needed to exactly achieve the moment demand with ﬁve layers of the FRP system. Compare this with the data presented in Table 9.3, which gives the results for two or four layers of the FRP system chosen. Can the moment demand be met with three layers of FRP system? What should the width of the

284

FRP FLEXURAL STRENGTHENING

FRP be in this case, and what will the failure mode be? Compare the results for two, three, four, and ﬁve layers, and discuss the implications for the designer using FRP strengthening systems. What system would you ultimately choose as the best system to meet the strength demand? Do not consider serviceability and detailing or the inﬂuence of the effect of layers on possible shear failure of the strengthened beam. Justify your choice. 9.6

A simply supported reinforced concrete beam in the interior of a residential building spans 20 ft. It has a 12 ⫻ 18 in. cross section and is reinforced with three No. 7 grade 60 steel bars and No. 3 steel stirrups at 7.5 in. on center. It was designed with a clear cover of 1.5 in. The beam is supported on 12-in.-wide supports. ƒ⬘c ⫽ 3500 psi. The beam was originally designed to carry a live load of 400 lb/ft and a dead load of 600 lb/ft (not including its self-weight). The building has been sold and the new owner wants to convert the residential space to ofﬁce space, which requires that the live load on the beam be increased. You are required to investigate a ﬂexural strengthening system using Sika CarboDur Type S 1012 pultruded strips bonded to the beam with Sikadur 30 epoxy paste. For the ﬁve strengthening designs shown in Table P9.6, determine (a) the strengthened ultimate moment capacity (and % increase), (b) the failure mode, and (c) the new allowable live load that can be applied to the beam (and % increase). Follow ACI 440.2R-02 guidelines. What can you conclude about the various strengthening designs? Are more strips necessarily better? Which design would you recommend to the owner to achieve the maximum live load increase and, why? (You do not need to consider serviceability limits for this exercise.)

9.7

Reconsider the beam described in Problem 9.6. Consider the same strengthening problem, but investigate the ﬁve cases using a Tyfo UG (unidirectional glass) laminate strip and Tyfo TC epoxy. Compare the

TABLE P9.6

Strengthening System Layouts

Design Case

Number of Strips

Strip Layout

1 2 3 4 5

1 2 2 3 4

Along centerline Side by side parallel to centerline Double layer along centerlinea Three strips alongside each other (in one layer) Two double-layer strips side by side

a

Precured strips are not usually used in multiple layers, due to their thickness. This example is for illustration purposes.

PROBLEMS

285

results using the glass laminate to those using carbon laminate. Discuss the differences and your observations. 9.8

A 5-in.-thick reinforced concrete slab in a building frame spans continuously over reinforced concrete beams 10 in. wide and 12 ft apart. ƒ⬘c ⫽ 4000 psi. The slab is reinforced with No. 4 grade 60 bars at 12 in. on center for positive and negative moments. It was designed for residential purposes to carry a superimposed dead load of 20 lb/ft2 and a live load of 60 lb/ft2. The building owner would like to increase the live-load capacity to 150 lb/ft2 to use the space as ofﬁce space. Design an FRP strengthening system using one of the FRP systems given in Table P9.1. (Note that the FRP does not have to cover the entire surface and can be provided in strips.) Perform only the design for strength. (Assume that serviceability is not a problem and that the beams have adequate capacity to support the new loads.) Provide strengthening for both the positive and negative moment regions. Detail the strengthening system and show termination points for a typical interior two-bay width (i.e., 24 ft). Discuss how you would detail the FRP strengthening system on the top surface of the ﬂoor.

9.9

A simply supported reinforced concrete beam in the interior of a residential building spans 18 ft. It has a 16 in. wide ⫻ 24 in. high cross section and is reinforced with three No. 9 grade 60 steel bars and No. 3 steel stirrups at 8 in. on center. Assume that the beam was designed with an effective depth of 21.5 in. ƒ⬘c ⫽ 4000 psi. The original dead load/live load ratio (including the beam self-weight) was 1⬊2, and this load ratio is maintained for the future loads. A consultant has designed a strengthening system for this beam to increase its load-carrying capacity. The consultant has recommended strengthening the beam by bonding two layers of 10-in.-wide sheets of WaboMBrace CF130 carbon ﬁber sheets and WaboMBrace epoxy saturant. The sheets are bonded to the underside of the beam and extended to the edges of the supports. You have been called in as an expert in FRP strengthening of concrete structures to peer-review the design. You are not told what the desired strengthening objective was; this is something the owner wants to verify with your check. The owner also wants to verify that the design is in compliance with the ACI 440.2R-02 design guide with regard to the ultimate capacity calculations, failure modes, and strengthening limits (including stresses in the steel and FRP and maximum deﬂection of the strengthened beam under future service loads). You are required to: (a) Determine the failure mode of the strengthened beam. (b) Determine the ultimate moment capacity of the strengthened beam. (c) Determine the percent increase in the ultimate capacity. (d) Determine the future (strengthened) dead- and live-load carrying capacity of the beam.

286

FRP FLEXURAL STRENGTHENING

(e) Determine whether the strengthening is within ACI capacity (strength enhancement) strengthening limits. (f) Determine whether or not shear strengthening is required for future loads. (g) Determine the value of the maximum possible strengthened ultimate moment capacity the owner could obtain according to the ACI ultimate strengthening limits. (h) Determine whether the strengthening is within ACI serviceability strengthening limits and explain why these limits are placed on strengthening. (i) Provide a cost estimate to the owner for the strengthening system.21 9.10 Derive the folllowing equation (given in ACI 440.2R-02 without the subscript 2 on k) for the stress in the steel in the FRP-strengthened member at service loads: ƒs,s ⫽

[(m1 ⫹ m2) ⫹ bi AƒEƒ(h ⫺ k2d/3)](d ⫺ k2d)Es As Es(d ⫺ k2d/3)(d ⫺ k2d) ⫹ AƒEƒ(h ⫺ k2d/3)(h ⫺ k2d)

9.11 For the ﬁve strengthening systems evaluated in Problem 9.4, perform the required serviceability checks and detail the FRP systems. (a) Check the service-level stresses in the steel and compare with the ACI 440.2R-02 permitted value, (b) Check the service-level stresses in the FRP strengthening system and compare with the ACI 440.2R-02 permitted value, (c) Check the maximum midspan deﬂection under service loads using the Branson formula and compare with L/360. (d) Detail the strengthening systems. 9.12 For the ﬁve strengthening system conﬁgurations in Problems 9.6 and 9.7, perform the required serviceability checks. (a) Check the service-level stresses in the steel and compare with the ACI 440 2R-02 permitted value. (b) Check the service-level stresses in the FRP strengthening system and compare with the ACI 440 2R-02 permitted value. (c) Check the maximum midspan deﬂection under service loads using the Branson formula and compare with L/360. (d) Detail the strengthening systems. 9.13 A simply supported ﬂat-slab bridge built in 1930 needs to be strengthened to increase its live-load capacity for current highway loads. The

21 Contact the FRP system supplier for current pricing. Consider both material and installation costs.

PROBLEMS

287

bridge has a span of S ⫽ 23 ft, a width of 26 ft, a 20-in.-thick concrete slab, and a 6-in. asphalt overlay (assume that the asphalt overlay is 130 lb/ft3). The bridge is reinforced with 1920s-era 1.0-in. square ribbed reinforcing bars at 6 in. on center with a yield strength of 33 ksi. The bottom clear cover is 1 in. and the 1920s concrete strength is ƒ⬘c ⫽ 2500 psi. The bridge has been rated by the local department of transportation and given an HS17 inventory load rating. Since it is rated below HS20, it is regarded as structurally deﬁcient. The local authority would like to increase the load rating to HS25 (i.e., a 45-ton tractortrailer, single wheel load, P25 ⫽ 20 kips, not including the impact factor of 30%) for future highway loads. To accomplish this, the nominal moment capacity of the bridge must be increased by 30%. You are required to design a strengthening system for the bridge using WaboMBrace CF130 carbon ﬁber sheets and WaboMBrace epoxy saturant according to ACI 440.2R-02 and the AASHTO Standard Speciﬁcation (AASHTO, 2002)22. You need to perform the following as part of your design: (a) Determine the current nominal moment capacity and current ultimate capacity (kip-ft/ft) and also the future (after the strengthening) nominal and ultimate capacities (kip-ft/ft) of the bridge. (b) Determine the current and future allowable wheel load (live load) for the bridge. Assume that the wheel load is a single concentrated load applied at midspan over an effective width E ⫽ 4 ⫹ 0.06S (where S is the span in feet) of the slab. (Do not forget to include the dead-load moment in this calculation.) (c) Compare this to the wheel load for an HS25 truck (i.e., 20 kips). Note that an additional impact factor of 30% is applied to the live load to account for dynamic effects [i.e., the HS25 required wheel load capacity is 20(1.3) ⫽ 26 kips]. Does the increase in moment capacity you obtained meet the strengthening objectives (i.e., can the bridge carry a HS25 truck load)? (d) Show a sketch of the strengthening system conﬁguration. Note: You do not have to cover the entire surface; you can apply the sheet material in strips of width, wƒ. Clear spacing of the strips should be less than two times the strip width and less than h.

22

See Chapter 5 for AASHTO dead and live load factors, and consult the speciﬁcations.

10 10.1

FRP Shear Strengthening

OVERVIEW

This chapter deals with the design of shear strengthening systems for reinforced concrete ﬂexural members loaded by transverse loads, such as beams, slabs, walls, and columns with precured FRP strips and plates and laid-up FRP sheet and fabric systems. The strengthening of reinforced concrete members subjected to torsion is not discussed. Only nonprestressed concrete members that are reinforced with conventional steel reinforcing bars are considered. For the purposes of this chapter, it is assumed that the reader is familiar with both the fundamentals and details of the shear design of concrete members reinforced with conventional steel reinforcing bars. Although shear strengthening has been carried out in practice for about as long as ﬂexural strengthening, the understanding of the behavior of members strengthened in shear is less developed than that for ﬂexural strengthening. This parallels our understanding of the subject of shear behavior of reinforced concrete members in general, as noted in the discussion related to the shear design of concrete members with FRP rebars. The subject of shear strengthening is additionally complicated by the fact that design of the shear strengthening depends on how the FRP strengthening system encompasses, or wraps around, the concrete member. Therefore, when performing a shear strengthening design it is imperative that a structural engineer has a good knowledge of the particular FRP strengthening system that will be used by the contractor (or that will be speciﬁed in the speciﬁcations). Not all systems can be wrapped around a concrete member, and not all concrete members have their four sides accessible for the FRP to be applied. The design procedures presented in this chapter follow ACI 440.2R-02, which is compatible with ACI 318-99. The examples presented in this chapter are based on the examples in ACI 440.2R-02 and are intended to allow the reader to analyze these examples critically and consider design alternatives not presented in the ACI guide. In recent years there have been signiﬁcant applications of FRP shear strengthening systems to shear-strengthen deﬁcient highway bridge columns in seismically active zones. ACI 440.2R-02 does not speciﬁcally address the issues of strengthening of columns. It has been shown that the axial force on a column can inﬂuence the shear capacity and the lateral displacement capacity. A method due to Priestley and colleagues, for the design of shear strengthening systems for columns that accounts for the effect of axial loads is presented at the end of this chapter. 288

Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

10.2

10.2

INTRODUCTION

289

INTRODUCTION

FRP strengthening systems can be used to increase the shear capacity of concrete beams, columns, and walls. FRP strengthening systems are applied to the webs of beams (or vertical sides of columns and walls) and function in a fashion similar to that of internal steel shear reinforcements such as stirrups, hoops, or ties. The FRP strengthening system is attached to the exterior surface of the concrete member in the transverse plane of the member and resists the transverse shear force resultant (or lateral force in a column or wall), as shown in Figs. 10.1 and 10.2. The FRP strengthening system adds to the shear resistance of the member, which traditionally is derived from the concrete itself and from the internal shear reinforcement. In a general sense, an FRP shear strengthening system is similar in appearance on the exterior of the concrete member to an FRP ﬂexural strengthening system (except for the orientation of the ﬁbers, as explained in what follows). However, from a structural mechanics and constructability point of view, FRP shear strengthening is signiﬁcantly more complex than FRP ﬂexural strengthening. The reasons for this are based on the mechanics of shear strengthening itself and on the shapes and geometries of concrete members relative to the geometries and properties of FRP strengthening materials. In the case of FRP ﬂexural strengthening of a beam, column, or even a wall (typically, for out-of-plane strengthening) the FRP strengthening system is geometrically compatible with the member since the primary orientation of

Figure 10.1 FRP Shear strengthening of a beam. (Courtesy of Structural Group.)

290

FRP SHEAR STRENGTHENING

Figure 10.2 FRP shear strengthening of a wall with openings. (Courtesy of Racquel Hagan.)

the FRP strengthening system is in the lengthwise direction of the member. Therefore, a long precured strip or a unidirectional fabric tow sheet can readily be extended along the length of the member to provide ﬂexural reinforcement. In addition, the bending moment along a ﬂexural member varies along the length of the member, having points of maximum moment, minimum moment, and zero moment (at inﬂection points) along the length. Therefore, the FRP strengthening system is exposed to a varying axial force along its length, and any unit length portion of the adhesive system is only responsible for carrying the moment increment over that unit length. Wherever possible, the FRP strengthening is terminated and anchored at or near these regions of zero moment in the member, which reduces the potential for peeling anchorage failures at the ends of the strip. Added to this, a ﬂexural strengthening system is typically attached at the most advantageous position on the cross section of the member, that is, as far from the neutral axis as possible. Finally, the structural behavior of reinforced concrete ﬂexural members is well understood, and analytical models for ﬂexural behavior have been veriﬁed over

10.2

INTRODUCTION

291

many years. It has been shown (as detailed in earlier chapters) that these models can be extended to FRP strengthening in a relatively straightforward manner provided that the force can be transferred between the FRP strengthening system and the concrete in a controlled fashion.1 Consider now the case of shear strengthening of a reinforced concrete member. In the case of a beam or a column, the structural depth of the member is much smaller than the length. Since the transverse shear force acts parallel to the structural depth of the member, the primary direction of the FRP reinforcement needs to be placed in this direction (the precise angle with respect to the beam axis is explained in what follows). Therefore, the FRP reinforcement can act only over relatively short lengths (and ﬁnite widths) on the sides of the member, which, as noted, is not very deep2 and does not provide much room for anchorage of the FRP system. In addition, unlike the case of FRP ﬂexural strengthening, where the force varies along its length, the force (or stress) in the FRP shear strengthening is constant through the depth of the section at any location along the length.3 To prevent debonding of the FRP shear strengthening system at the top and bottom of the sides of the member, it is possible to wrap the FRP strengthening system around the section, either partially (often called a three-sided U-wrap) or completely around the beam (often called a four-sided wrap), as shown schematically in Fig. 10.3. When the FRP system cannot be wrapped around either the top or the bottom of the section, the system is called a two-

df = h

df

(a)

df

(b)

(c)

Figure 10.3 FRP shear strengthening schemes and effective depths: (a) four-sided; (b) three-sided; (c) two-sided.

1 In fact, it should be noted that strain compatibility at the interface between the concrete and the FRP is not necessarily a requirement for ﬂexural strengthening. 2 For deep beams and walls, where the structural depth is larger, the situation is not as bad. 3 Even though the shear force varies along the length of the member, at any section, the shear force is single-valued according to one-dimensional beam theory.

292

FRP SHEAR STRENGTHENING

sided system. Non-fully wrapped FRP systems are susceptible to detachment failures at their ends and their strains are limited by a shear bond-reduction coefﬁcient. In many cases, shear strengthening is performed on T-shaped sections, either produced as prefabricated T-beams or behaving as T-sections when cast monolithically with a ﬂoor slab or wall section. In this situation a four-sided shear strengthening system can still be achieved if the FRP strengthening system is applied in discrete narrow strips and slits are machined into the concrete slab or wall (which can be a time-consuming and expensive process). Slits can also be used to anchor three-sided systems more effectively in an adjoining the slab or wall. It is important to emphasize that in the case of T-sections the FRP strengthening system should never be extended around the reentrant corner unless an additional anchorage system is provided to prevent radial peeling at the corner. Constructability issues also arise with wrapped or partially wrapped systems. The corners of the beam need to be rounded (chamfered) to prevent the sharp corner edges from causing stress concentrations and premature failure of the FRP wrap. In the case of precured systems, special discrete Lshaped elements (also called straps) must be manufactured, and the radius of the bend needs to be compatible with the chamfer on the beam edge (as shown in Fig. 10.4). For laid-up FRP systems the sheets or fabrics can be applied in ﬁnite-width segments, or they can be applied continuously along the side of the member. In either case, the sheet needs to be cut to a rather short length, and due to its ﬁnite width will need to be placed in multiple sections along the beam length (as seen in Fig. 10.1). The sheet can be applied at inclined angles, ␣, to the beam axis, as shown in Fig 10.5. The sheet width, wƒ, is measured perpendicular to the ﬁber principal direction, while the sheet spacing, sƒ, is measured along the beam axis. The angle of inclination of the postulated

Figure 10.4 L-shaped precured FRP shear reinforcement straps. (Courtesy of Christoph Czaderski.)

10.3

SHEAR CAPACITY OF AN FRP-STRENGTHENED MEMBER

293

FRP strengthening system

Postulated shear cracks

wf wf

β

h

α sf

Figure 10.5 Geometric variables for FRP shear strengthening.

shear crack, typically taken as 45⬚, is denoted as . If this system is wrapped, it creates a spiral along the length of the member, which can have deﬁnite advantages in terms of structural performance and may have some constructability advantages.4 In this case, precured strips cannot be used unless they are manufactured with the appropriate angled bevel at the bottom edge.

10.3

SHEAR CAPACITY OF AN FRP-STRENGTHENED MEMBER

The nominal shear capacity of an FRP-strengthened concrete member with existing steel shear reinforcing is determined by adding the contribution of the FRP strengthening system to the existing shear capacity and is given as Vn ⫽ Vc ⫹ Vs ⫹ ƒVƒ

(10.1)

Vc is the existing shear capacity of the concrete,5 Vs the shear capacity of the existing steel shear reinforcement, and Vƒ the shear capacity of the FRP strengthening system. It is assumed that the contribution of the three different contributors listed above is linearly additive and that no beneﬁcial or harmful synergistic6 effects occur as a result of attaching the FRP to the sides of the concrete member. Recall that the additional capacity reduction factor, ƒ, is used on the FRP contribution. The FRP capacity reduction factor, ƒ, is taken as 0.95 for completely wrapped sections (called contact critical) and as 0.85 for two- or three-sided wrapped sections (called bond critical). The FRP contribution is determined using the same truss analogy as that used to develop the shear resistance provided by steel stirrups. The angle of

4

A continuous spiral can be done only for a four-sided wrap. Due to aggregate interlock, dowel action of the main bars, and resistance of the uncracked compression zone above the shear crack. 6 Such as an increase or decrease in Vc or Vs when the FRP is attached. 5

294

FRP SHEAR STRENGTHENING

the critical shear crack with respect to the longitudinal axis of the member is taken as 45⬚, in accordance with the ACI 318-99 philosophy. Two forms of the equation for the shear contribution for FRP shear strengthening are provided herein, one for intermittent strips having width (measured perpendicular to the major ﬁber orientation of the strengthening system) wƒ and spaced at a spacing sƒ (measured parallel to the member axis) and one for continuous FRP shear strengthening (i.e., full side coverage with no overlapping). Intermittent wrapping is generally preferred (although it is harder to place in the ﬁeld) since it allows moisture to migrate from the concrete to the air. A continuous wrap will fully cover the concrete surface and could trap moisture under the wrap and cause degradation of the interface, substrate, or the FRP composite. In addition, a continuous wrap causes difﬁculties with inspection since the surface of the concrete is not visible. For intermittent strengthening, Vƒ ⫽

Aƒvƒƒe(sin ␣ ⫹ cos ␣)dƒ sƒ

(ACI 440.2R-02:10-3)

Substituting Aƒv ⫽ 2ntƒwƒ

(ACI 440.2R-02:10-4)

gives Vƒ ⫽

2ntƒwƒƒƒedƒ(sin ␣ ⫹ cos ␣) sƒ

(10.2)

with the geometric condition that sƒ ⬎

wƒ sin ␣

(10.3)

ƒƒe ⫽ Eƒƒe is the effective tensile stress in the FRP, ␣ the inclination of the ﬁber in the FRP strengthening system to the longitudinal axis of the member, n the number of layers of shear reinforcement and dƒ the effective depth of the FRP strengthening system (shown in Fig. 10.3). If sƒ ⫽ wƒ /sin ␣, continuous strengthening (full surface coverage) occurs and Vƒ ⫽ 2ntƒƒƒedƒ(sin2␣ ⫹ sin ␣ cos ␣)

(10.4)

For a continuous inclined strip at an angle ␣ to the beam axis that is formed out of discrete strips of width, wƒ, placed side by side along the beam length, the strips must be spaced at

10.3

SHEAR CAPACITY OF AN FRP-STRENGTHENED MEMBER

sƒ ⫽

wƒ sin ␣

295

(10.5)

For the special case where ␣ ⫽ 90⬚, the shear contribution of the FRP strengthening systems is given as follows: For intermittent strengthening, Aƒvƒƒedƒ sƒ

(10.6)

Vƒ ⫽ 2ntƒƒƒedƒ

(10.7)

Vƒ ⫽ For continuous strengthening,

For the special case where ␣ ⫽ 45⬚, the shear contribution of the FRP strengthening systems is given as follows: For intermittent strengthening, Vƒ ⫽

兹2Aƒvƒƒedƒ

sƒ

(10.8)

with the geometric condition that sƒ ⬎ 兹2wƒ

(10.9)

Vƒ ⫽ 2ntƒƒƒedƒ

(10.10)

For continuous strengthening,

which is the same result as for ␣ ⫽ 90⬚ for continuous strengthening. It is interesting to note that in the case of FRP strengthening with sheets there is no apparent beneﬁt to using inclined sheets at 45⬚ as there is with conventional reinforcing bars, as would be implied by use of ACI 440.2R02:10-3. This is because sheets have ﬁnite and usually quite considerable width (10 to 20 in.). In the derivation of ACI 440.2R-02:10-37 (which is similar to that done for steel bars) it is assumed that the shear reinforcing bars occupy a theoretically vanishing area such that they can be brought closer and closer together when inclined but not come into contact, maintaining some separation. Therefore, inclined bars are actually closer to each other than vertical bars for the same horizontal spacing, s, and intersect more inclined shear cracks, leading to the result that they are more effective as shear reinforcement. When the shear reinforcement is in the form of relatively wide sheets, such an assumption cannot be made and the sheets soon begin, the-

7

See Wang and Salmon (2002, p. 154).

296

FRP SHEAR STRENGTHENING

oretically, to come into contact and overlap. The apparent advantage of inclined sheets can be seen when sheets begin to resemble bars in their aspect ratios wƒ /sƒ (0.2 or less). In such a case, sheets become in reality more geometrically similar to near-surface-mounted (or surface-mounted) bars. If the shear crack is not assumed to be at 45⬚, the equations above can be written in terms of the angle of inclination of the shear crack with respect to the longitudinal axis, , shown in Fig. 10.5, as: For intermittent strengthening, Vƒ ⫽

Aƒvƒƒe(cot  sin ␣ ⫹ cos ␣)dƒ sƒ

(10.11)

for continuous strengthening, Vƒ ⫽ 2ntƒƒƒedƒ(cot  sin2␣ ⫹ sin ␣ cos ␣)

(10.12)

and sƒ ⫽

wƒ sin ␣

(10.13)

10.4 EFFECTIVE STRAIN IN THE FRP FOR SHEAR STRENGTHENING The effective strain in the FRP shear strengthening system is limited in ACI 440.2R-02 to prevent detachment failures and also to maintain the integrity of the concrete aggregate interlock in the concrete member. A bond-related coefﬁcient for shear strengthening is introduced to account for the FRP shear strengthening system debonding. This is similar to the empirical approach taken for debonding of FRP systems in ﬂexural strengthening, in which the phenomenon of debonding is accounted for by a bond-related coefﬁcient but the capacity for each speciﬁc failure mode is not determined. Depending on the type of shear strengthening conﬁguration used, the FRP material may fail due either to debonding or to FRP rupture. Explicit procedures to determine the failure in these two modes are discussed in Chen and Teng (2003a,b). For completely wrapped (four-sided) FRP shear strengthening systems, the maximum effective strain in the FRP strengthening system at failure is limited to ƒe ⫽ 0.004 ⱕ 0.75ƒu

(ACI 440.2R-02:10-6a)

For three- or two-sided shear strengthening, the effective shear strain in the FRP strengthening system at failure is limited to

10.4

EFFECTIVE STRAIN IN THE FRP FOR SHEAR STRENGTHENING

ƒe ⫽ vƒu ⱕ 0.004

297

(ACI 440.2R-02:10-6b)

The shear bond-reduction coefﬁcient, v, is a function of the concrete strength, the wrapping type used, and the stiffness of the FRP strengthening system and is given by ACI 440.2R-02 as v ⫽

k1k2Le ⱕ 0.75 468ƒu

(ACI 440.2R-02:10-7)

The equation is a function of the active bond length, Le, over which the shear stress is transferred between the FRP and the concrete. It has been shown that it is this ﬁnite length that limits the maximum force that can be transferred between the two materials, regardless of the bonded length of the FRP strip (Maeda et al., 1997; Ta¨ljsten, 1997; Khalifa et al., 1998; Bizindavyi and Neale, 1999). In ACI 440.2R-02 the active bond length is given by an empirical equation as 2500 (ntƒEƒ)0.58

Le ⫽

(ACI 440.2R-02:10-8)

and the coefﬁcients k1 and k2 are given as

冉 冊

ƒ⬘c k1 ⫽ 4000

2/3

(ACI 440.2R-02:10-9)

For three-sided shear strengthening systems, k2 ⫽

dƒ ⫺ Le dƒ

(ACI 440.2R-02:10-10)

For two-sided shear strengthening systems, k2 ⫽

dƒ ⫺ 2Le dƒ

(ACI 440.2R-02:10-10)

Mechanical anchorages can be used to anchor two- or three-sided wraps, in the compression zone of the web; however, design guidance is not provided by the ACI 440.2R-02 for this at the present time. Steel angles at reentrant corners, steel plates, and ﬁber anchors have all been proposed for this purpose. In addition, slot or slits can be drilled in T-section ﬂanges for anchoring the FRP. The amount of shear reinforcement in a reinforced concrete member is limited by ACI 318-99. When FRP shear strengthening is used in addition to

298

FRP SHEAR STRENGTHENING

conventional steel shear reinforcement, the reinforcement limit must hold for both types of reinforcement: Vs ⫹ Vƒ ⱕ 8兹ƒ⬘cbwd

(ACI 440.2R-02:10-11)

When intermittent strips are used, maximum spacing between the strips is mandated so that every shear crack will be covered by sufﬁcient strip width. The following maximum spacing of intermittent strips is required: smax ⫽ ƒ

10.5

dƒ ⫹ wƒ 4

(10.14)

DESIGN PROCEDURE FOR SHEAR STRENGTHENING

Step 1. Determine the current and future strength requirements and check the strengthening limits. The existing shear capacity of the beam must be determined prior to design of the strengthening system. Step 2. Choose an FRP system strengthening system and conﬁguration. The designer needs to make some a priori choices regarding the type of strengthening system (precured or wet layup) to use and obtain manufacturer-guaranteed properties for approved systems from existing speciﬁcation sheets. Step 3. Determine the number of layers and geometry of the FRP wrap. Unlike in the ﬂexural design, an estimating step is not required. For shear strengthening the amount of FRP material can be determined in closed form once the conﬁguration is chosen. At ﬁrst the amount of material needed for continuous coverage is determined and then the spacing of the intermittent wrap can be found to maximize the FRP used. The shear bond reduction coefﬁcient, v, is determined in this step of the design. Step 4. Calculate the actual shear capacity of the FRP wrap. The actual FRP system used will probably be slightly different from that determined in step 3. This is because commercial sheets and precured strips are supplied in limited widths and for economic reasons the ﬁnal design should attempt to be compatible with premanufactured widths. Step 5. Calculate the factored shear capacity of the future strengthened beam. Calculate the factored shear capacity and compare with the demand. Step 6. Check the maximum FRP reinforcement and spacing limits. Step 7. Detail the FRP strengthening system. Design Example 10.1: FRP Shear Strengthening of a Beam8 A reinforced concrete T-beam with dimensions shown in Fig. 10.6 is subjected to an in8

This example follows Example 14.4 in ACI 440.2R-02.

10.5

DESIGN PROCEDURE FOR SHEAR STRENGTHENING

299

d = 22 in. df = 16 in.

3 in. Three-sided FRP U-wrap bw = 15 in.

Figure 10.6 Geometry of a beam showing pertinent dimensions and an FRP wrap.

creased live load. The beam is an interior beam in a building, constructed originally using ƒ⬘c ⫽ 3000-psi concrete. Prior evaluation of the existing beam has determined that Vc ⫽ 36.4 kips and Vs ⫽ 19.6 kips. A carbon–epoxy FRP strengthening system is requested by the owner. The future total shear demand (at a distance d from the support) due to the increase in live load on the beam is Vu ⫽ 60 kips. SOLUTION Step 1. Determine the current and future strength requirements and check the strengthening limits. The current nominal shear capacity of the beam is given as Vn ⫽ Vc ⫹ Vs ⫽ 36.4 kips ⫹ 19.6 kips ⫽ 56.0 kips and the current factored shear capacity is Vn ⫽ 0.85(56.0) ⫽ 47.6 kips

Since Vu ⬎ Vn, shear strengthening is required in the portion of the beam that has a current capacity less than that required for the future demand. It is important to recognize that the FRP does not need to cover the entire length of the beam web. For a simply supported beam this will be a region from the support a distance x along the beam. This depends on the shear force distribution (i.e., the loading) on the beam. The beam in question is loaded by a uniformly distributed load and a concentrated load. The shear force diagram for a portion of the beam near the support is shown in Fig. 10.7.

300

FRP SHEAR STRENGTHENING

d = 22 in.

Region of the beam that has an existing shear capacity that will not meet the future demand

60.0 kips 47.6 kips

15.0 kips 70 in.

Figure 10.7 Shear force in a beam near the support.

In this example, it is assumed that the ﬂexural capacity of the beam is adequate for the increased loads. In general, this would need to be checked. The shear strengthening limits also need to be checked. For this, the live and dead loads are needed. If these were given, the following check would be made: Wlimit ⫽ 1.2wDL ⫹ 0.85wLL Vlimit ⫽ ƒ(Wlimit) ⱕ 47.6 kips Step 2. Choose an FRP system strengthening system and conﬁguration. A dry ﬁber sheet system with the following guaranteed ﬁber9 properties is chosen. tƒ ⫽ 0.0065 in. ƒ* ƒu ⫽ 550 ksi

ƒu * ⫽ 0.017 (1.7%)

Eƒ ⫽ 33,000,000 psi

Determine the design properties of the FRP system according to the environment. For this case we have interior construction with a carbon FRP and CE ⫽ 0.95. ƒƒu ⫽ 0.95(550) ⫽ 522.5 ksi ƒu ⫽ 0.95(0.017) ⫽ 0.016 (1.6%)

Eƒ ⫽ 33,000,000 psi (unchanged)

9

Note that the ﬁber thickness and modulus properties are used in this example (not the FRP composite properties).

10.5

DESIGN PROCEDURE FOR SHEAR STRENGTHENING

301

Decide on a conﬁguration of the FRP system. Since this is a T-beam, a four-sided all-around complete wrap cannot be used (unless slits are cut through the slab). A three-sided U-wrap or a two-sided wrap can be used. It is advisable wherever possible to use the most effective level of wrapping style. In this case, a three-sided U-wrap is considered ﬁrst. Step 3. Determine the number of layers and the geometry of the FRP wrap. The shear contribution required of the FRP strengthening system can be found from V reqd ⫽ ƒ

冉

冊

冉

冊

1 Vd 1 60 ⫺ Vc ⫺ Vs ⫽ ⫺ 36.4 ⫺ 19.6 ⫽ 17.2 kips ƒ 0.85 0.85

To determine the number of layers and the sizes of the FRP strengthening sheets to be used in the three-sided wrap selected several preliminary design decisions need to be made: (1) continuous or intermittent sheet; (2) inclined or 90⬚ ﬁber orientation. To start it is advisable to assume a continuous 90⬚ system to obtain an initial estimate of the number of layers. Thereafter, the intermittent system can be considered. For further optimization, an inclined FRP system can be used. However, use of an inclined system in a three- or four-sided wrap will cause constructability problems, with ‘‘spiraling’’ of the sheet on the opposite side of the beam. The maximum permissible strain (effective strain) in the FRP is calculated ﬁrst. This is a function of the shear bond coefﬁcient, v, found from v ⫽

k1k2Le ⱕ 0.75 468ƒu

Assuming one layer of the FRP will be used, Le ⫽

2500 2500 ⫽ ⫽ 2.022 in. 0.58 (ntƒEƒ) [1(0.0065)(33,000,000)]0.58

k1 ⫽

冉 冊 冉 冊

k2 ⫽

dƒ ⫺ Le 16 ⫺ 2.022 ⫽ ⫽ 0.874 dƒ 16

ƒ⬘c 4000

which gives

2/3

⫽

3000 4000

2/3

⫽ 0.826

for three-sided U-wraps

302

FRP SHEAR STRENGTHENING

v ⫽

0.826(0.874)(2.022) ⫽ 0.195 ⱕ 0.75 468(0.016)

Since ƒe ⫽ vƒu ⱕ 0.004, ƒe ⫽ 0.195(0.016) ⫽ 0.0031 ⬍ 0.004

For a continuous 90⬚ three-sided wrap, the number of layers required is n⫽ ⫽

V reqd V ƒreqd ƒ ⫽ 2tƒƒƒedƒ 2tƒƒeEƒdƒ 17.2 ⫽ 0.81 → use one layer 2(0.0065)(0.0031)(33,000)(16)

Since the number of layers is less than 1, one continuous layer would provide too much FRP for the required design. An intermittent sheet may therefore be preferable to a continuous sheet in this case. One can obtain the sheet width-to-sheet spacing ratio, Rw / s ⫽ wƒ /ws for an intermittent 90⬚ wrap using Rw / s ⫽

wƒ V ƒreqd 17.2 ⫽ ⫽ ⫽ 0.81 sƒ 2ntƒƒƒedƒ 2(1)(0.0065)(102.3)(16)

(Note that the similarity between the two equations above occurs because for a continuous wrap, wƒ ⫽ sƒ.) It is preferable to choose a sheet width that is a fraction of that of a commercially available sheet width to aid in constructability and to reduce waste. Assuming that the carbon–epoxy sheet chosen is available in 20-in. widths, a sheet width of 10 in. is chosen. For a 10-in. width, the space is calculated as sƒ ⫽

wƒ 10 ⫽ ⫽ 12.35 → use 12-in. spacing Rw / s 0.81

Step 4. Calculate the actual shear capacity of the FRP wrap. Determine the area of the FRP in the ﬁber direction: Aƒv ⫽ 2ntƒwƒ ⫽ 2(1)(0.0065)(10) ⫽ 0.13 in2 Determine the maximum design (effective) stress in the FRP: ƒƒe ⫽ Eƒƒe ⫽ 33,000(0.0031) ⫽ 102.3 ksi Determine the shear contribution for the 90⬚-oriented sheets:

10.5

Vƒ ⫽

DESIGN PROCEDURE FOR SHEAR STRENGTHENING

303

Aƒƒƒedƒ 0.13(102.3)(16) ⫽ ⫽ 17.7 kips ⬎ 17.2 kips → OK sƒ 12

The layout schematic of the FRP strengthening system over the 70-in. critical length for this case is shown in Fig. 10.8. Step 5. Calculate the factored shear capacity of the future strengthened beam. Vn ⫽ (Vc ⫹ Vs ⫹ ƒVƒ) ⫽ 0.85[36.4 ⫹ 19.6 ⫹ (0.85)(17.73)] ⫽ 60.4 kips ⬎ 60 kips

Therefore, Vn ⬎ Vd

and the system chosen is adequate. The percentage increase in the factored shear capacity is 60.4 ⫺ 47.6 (100) ⫽ 26.9% 47.6 Step 6. Check the maximum FRP reinforcement and spacing limits. Vs ⫹ Vƒ ⫽ 19,600 ⫹ 17,700 ⫽ 37,300 lb ⱕ 8兹ƒc⬘ bwd ⫽ 8兹3000(15)(16) ⫽ 105,162 lb → OK

smax ⫽ ƒ

dƒ 16 ⫹ wƒ ⫽ ⫹ 10 ⫽ 14 in. ⬎ 12 in. → OK 4 4

Step 7. Detail the FRP strengthening system. Extend the wrap as close as possible to the ﬂange of the T-beam. Anchors are not required but may be

19 in.

wf = 10 in.

sf = 12 in. 70 in.

Figure 10.8 Layout of FRP shear strengthening strips.

304

FRP SHEAR STRENGTHENING

advisable. Chamfer (round) the bottom corners of the beam to a 0.5-in. radius in the regions in which the FRP strengthening is to be applied (for a threesided U-wrap). Discussion of Alternative FRP Designs A number of different FRP conﬁgurations are given next for comparison purposes. Option a: Single layer continuous 90⬚ three-sided FRP wrap Vƒ ⫽ 2ntƒƒƒedƒ ⫽ 2(0.0065)(102.3)(16) ⫽ 21.3 kips ⬎ 17.7 kips Option b: Single layer continuous 90⬚ two-sided FRP wrap v, ƒe, and ƒƒe: k2 ⫽

dƒ ⫺ 2Le 16 ⫺ 2(2.022) ⫽ ⫽ 0.747 dƒ 16

v ⫽

0.826(0.747)(2.022) ⫽ 0.167 ⱕ 0.75 468(0.016)

Recalculate

ƒe ⫽ 0.167(0.016) ⫽ 0.0027 ⬍ 0.004

ƒƒe ⫽ Eƒƒe ⫽ 33,000(0.0027) ⫽ 88.0 ksi Therefore, Vƒ ⫽ 2ntƒƒƒedƒ ⫽ 2(0.0065)(88.0)(16) ⫽ 18.3 kips ⬎ 17.2 kips → OK and Vn ⫽ (Vc ⫹ Vs ⫹ ƒVƒ) ⫽ 0.85[36.4 ⫹ 19.6 ⫹ (0.85)(18.3)] ⫽ 60.8 kips ⬎ 60 kips → OK

This design would also work and will probably use less FRP material (this depends on the width of the particular beam since the three-sided wrap must provide material under the beam as well). In addition, it will probably be more economical to apply in the ﬁeld since it will not require rounding of the corners of the beam. In this case, extend the FRP sheet to the bottom of the web of the beam (not just to the effective depth, dƒ).

10.5

DESIGN PROCEDURE FOR SHEAR STRENGTHENING

305

Option c: Single layer continuous 45⬚ two-sided FRP wrap Vƒ ⫽ 2ntƒƒƒedƒ(sin2␣ ⫹ sin ␣ cos ␣) ⫽ 2(1)(0.0065)(88.0)(16)(sin245 ⫹ sin 45 cos 45) ⫽ 2(1)(0.0065)(88.0)(16)(0.5 ⫹ 0.5) ⫽ 18.3 kips ⬎ 17.2 kips

The sheets must be spaced at sƒ ⫽

wƒ 10 ⫽ ⫽ 14.14 in. sin ␣ sin 45

Option d: Single layer continuous 60⬚ two-sided FRP wrap Vƒ ⫽ 2ntƒƒƒedƒ(sin2␣ ⫹ sin ␣ cos ␣) ⫽ 2(1)(0.0065)(88.0)(16)(sin260 ⫹ sin 60 cos 60) ⫽ 2(1)(0.0065)(88.0)(16)(0.75 ⫹ 0.433) ⫽ 21.7 kips ⬎ 18.3 kips ⬎ 17.2 kips

sƒ ⫽

wƒ 10 ⫽ ⫽ 11.55 in. sin ␣ sin 60

Note that the 60⬚ continuous wrap is preferable to the 45⬚ and the 90⬚ wraps. Option e: Intermittent 60⬚ two-sided FRP wrap For wƒ ⫽ 10 in., sƒ must be greater than 11.55 in. Take sƒ ⫽ 14 in. Vƒ ⫽ ⫽

2ntƒwƒƒƒedƒ(sin ␣ ⫹ cos ␣) sƒ 2(1)(0.0065)(10)(88.0)(16)(0.866 ⫹ 0.500) 14

⫽ 17.9 kips ⬎ 17.2 kips → OK

Check the maximum spacing for this inclined intermittent wrap as follows: smax ⫽ ƒ

dƒ wƒ 16 10 10 ⫹ ⫽ ⫹ ⫽4⫹ ⫽ 15.55 ⬎ 14 in. → OK 4 sin ␣ 4 sin 60 0.866

Design Example 10.2: Shear Strengthening of a Rectangular Column10 Given a square reinforced concrete column with a 24 ⫻ 24 in. cross section. An increase in shear strength of 60 kips is required. The column is exposed 10

This design example follows Example 14.5 in ACI 440.2R-02.

306

FRP SHEAR STRENGTHENING

to an exterior environment. Design an E-glass/epoxy FRP system to increase the shear capacity of the column. Consider two options: (a) a continuous wrap, and (b) an intermittent wrap. SOLUTION Step 1. Determine the current and future strength requirements and check the strengthening limits. Since the current details and current loads are not given, the current strength and the strengthening limits cannot be checked. All we ⫽ V ucurrent ⫹ 60 kips. are given for design purposes is that V future u Step 2. Choose an FRP system strengthening system and conﬁguration. Choose an E-glass/epoxy system with the following FRP composite11 properties with the following guaranteed properties: tƒ ⫽ 0.051 in. ƒ*ƒu ⫽ 80 ksi

ƒu * ⫽ 0.020 (2.0%)

Eƒ ⫽ 4,000,000 psi

Determine the design properties of the FRP system according to the environment. For this case we have exterior construction with a glass FRP and CE ⫽ 0.65. ƒƒu ⫽ 0.65(80) ⫽ 52 ksi ƒu ⫽ 0.65(0.020) ⫽ 0.013 (1.3%)

Eƒ ⫽ 4,000,000 psi (unchanged) Use a full four-sided wrap with ﬁbers oriented perpendicular to the column axis (i.e., in the hoop direction). Place the FRP strengthening (either continuous or intermittent) over the entire height of the column from the top of the bottom story slab to the bottom of the top story beam or slab since the shear force is constant throughout the height. Step 3. Determine the number of layers and geometry of the FRP wrap. The maximum permissible strain in the FRP for a four-sided wrap is

11 It is important to note that in this example the thickness and modulus properties are given for the FRP composite (as a whole) and not for the ﬁber alone.

10.5

DESIGN PROCEDURE FOR SHEAR STRENGTHENING

307

ƒe ⫽ 0.004 ⱕ 0.75ƒu

0.75ƒu ⫽ 0.75(0.013) ⫽ 0.0098 ⬎ 0.004 Therefore, ƒe ⫽ 0.004. Assume that all the additional shear carrying capacity is obtained from the FRP wrap (i.e., no increase in the concrete shear capacity is obtained from the conﬁnement effect12 or from the axial load on the column). V ƒreqd ⫽

V additional 60 u ⫽ ⫽ 74.3 kips ƒ 0.85(0.95)

Determine the area of the FRP wrap required as a function of the spacing. Areqd ⫽ ƒ

V reqd 74.3sƒ ƒ sƒ ⫽ ⫽ 0.1935sƒ in2 ƒeEƒ dƒ 0.004(4000)(24)

Determine the number of layers as a function of the spacing and width: n⫽

Areqd 0.1935sƒ sƒ ƒ ⫽ ⫽ 1.897 2tƒwƒ 2(0.051)wƒ wƒ

Option a: For a continuous wrap, sƒ ⫽ wƒ and n ⫽ 1.892. Therefore, use two layers (n ⫽ 2). Option b: For an intermittent wrap, assume three 5-in.-wide strips and ﬁnd the required spacing. Rearranging gives us n ⫽ 1.897

sƒ wƒ

as sƒ ⫽

nwƒ 3(5) ⫽ ⫽ 7.9 in. → use 7.5-in. spacing 1.897 1.897

Steps 4 and 5. Calculate the shear capacity of the future strengthened beam. Option a: For a two-layer four-sided continuous wrap,

12

See Chapter 11 for more discussion of conﬁnement.

308

FRP SHEAR STRENGTHENING

Vƒ ⫽ ƒ2ntƒƒƒedƒ ⫽ 0.95(2)(2)(0.051)(0.004)(4000)(24) ⫽ 74.42 kips Vƒ ⫽ 0.85(74.42) ⫽ 63.26 kips ⬎ 60 kips → OK

Option b: For a three-layer four-sided intermittent wrap, Vƒ ⫽

ƒ2ntƒwƒƒƒedƒ 0.95(2)(3)(0.051)(5)(0.004)(4000)(24) ⫽ sƒ 7.5

⫽ 74.42 kips

Vƒ ⫽ 0.85(74.42) ⫽ 63.26 kips ⬎ 60 kips → OK

Step 6. Check the maximum FRP spacing limits. Option a: Spacing limits do not apply since the wrap is continuous. Option b: For a three-layer four-sided intermittent wrap, sƒmax ⫽

dƒ 24 ⫹ wƒ ⫽ ⫹ 5 ⫽ 11 in. ⬎ 8 in. → OK 4 4

Step 7. Detail the FRP strengthening system. Cover the full height of the column with the hoop FRP wraps. If an intermittent wrap is used, ensure that the top and bottom of the column are wrapped. Apply layers continuously if possible [i.e., do not apply layers in discrete sheets (or fabrics) with overlaps; try to use a single sheet (or fabric)]. Use a minimum 6-in. overlap at the end. Chamfer (round) the bottom corners of the column to a 0.5-in. radius. In the case of continuous coverage, overlapping parallel to the ﬁber direction (i.e., the hoop direction) is not required. Butt the edges of the wrap and seal with epoxy.

10.6 SHEAR STRENGTHENING OF FULLY WRAPPED AXIALLY LOADED COLUMNS Shear strengthening of axially loaded members, in particular columns, is the subject of some debate since a question arises as to whether or not to include the effects of the axial load on the column. ACI 440.2R-02 does not address the issue explicitly but does so implicitly in ACI 440.2R-02 Example 14.5, in which no account of the axial load is taken and the shear crack angle is taken as 45⬚. An alternative approach suggested by Priestley et al. (1996) and Seible et al. (1997) accounts for the axial effect and for the shallower angle of the shear crack that is found in axially loaded columns failing in shear that

10.6

SHEAR STRENGTHENING OF FULLY WRAPPED

309

are fully wrapped (i.e., conﬁned) by FRP systems.13 In addition, many columns have circular cross sections, which requires an alternative formulation for the effective depth of the section for design. In this approach the nominal shear resistance14 of an axially loaded column15 is given as Van ⫽ Vac ⫹ Vas ⫹ Vap ⫹ Vaƒ

(10.15)

where Vac , Vas , Vap, and Vaƒ are the concrete, steel reinforcing, axial load effect, and FRP strengthening contributions, respectively, to the shear capacity of the axially loaded column, according to Priestley et al. (1996). The Vac term includes the effect of the axial force on the shear strength and is given as Vac ⫽ k兹ƒc⬘ Ae

(10.16)

where k is a coefﬁcient that depends on the desired column ductility (for example, k ⫽ 1 psi for a displacement ductility ratio of between 3 and 4) [see Chapter 11 and Priestley et al. (1996)]. and,

Ae ⫽ 0.8Agross

(10.17)

The Vas term is taken as a function of the shear crack angle,  [35⬚ is recommended by Priestley et al. (1996) instead of 45⬚] and a different effective depth of the section than that prescribed for circular columns by ACI 318-99 (i.e., 0.8D) is used. For circular columns the Vas term is given as Vsa ⫽

AhƒyhD⬘ cot  2 s

(10.18)

and for rectangular columns it is given as Vsa ⫽

AhƒyhD⬘ cot  s

(10.19)

where Ah and ƒyh are the area and yield strength of the hoop reinforcement, D⬘ the core dimension from center to center of the peripheral hoop (or tie), and  the angle of the shear crack. 13

See Chapter 11 for a detailed discussion of FRP conﬁning of concrete members. The a superscript denotes ‘‘axial’’ and indicates that these values are not the same as those without the a. 15 See Priestley et al. (1996) for application to axially loaded beams. 14

310

FRP SHEAR STRENGTHENING

The Vap term is a function of the angle of the vertical compression strut in the column and is given as Vap ⫽ P tan ␣

(10.20)

where ␣ is the angle16 formed between the column axis and the compression strut, as shown in Fig. 10.9. The Vaƒ term is not premultiplied by a ƒ factor (as in ACI 440.2R-02) and it, too, uses a shallower angle of the shear crack (35⬚ is recommended). For circular columns, Vaƒ ⫽

nt ƒ D cot  2 ƒ ƒe

(10.21)

where ƒƒe ⫽ 0.004Eƒ is the recommended effective strength of the FRP wrap of n layers with a layer thickness of tƒ. For rectangular columns with continuous wraps, the shear strength provided by the FRP wrap is given as

Axial load P

Axial load P Vp

Vp

␣ P cos ␣

␣

P cos ␣

L

␣

␣ c2

c 2

Vp

Vp P

P D

(a) Reversed Bending

D (b) Single Bending

Figure 10.9 Determination of a vertical compression strut. (From Priestley et al., 1996 with permission of John Wiley & Sons.)

Not to be confused with ␣, the angle of inclination of the shear strengthening in ACI 440.2R02 equations.

16

PROBLEMS

Vaƒ ⫽ 2ntƒƒƒeh cot 

311

(10.22)

where h is the overall column dimension parallel to the shear force. Priestley’s method leads to smaller quantities of FRP materials required for shear strengthening of axially loaded columns, which is important from an economical standpoint, especially where massive columns used in highways bridges and elevated roadways are strengthened. This was the case in California in the late 1990s. The reader is referred to Priestley et al. (1996) for further details. In addition to shear strengthening, the conﬁning effect provided by a four-sided FRP wrap can also serve to increase the column axial capacity and to increase its ductility (energy absorption as evidenced by lateral deﬂection) to improve its overall seismic resistance. This topic is discussed further in Chapter 11.

PROBLEMS 10.1 For the FRP strengthening systems listed in Table P10.1, determine the effective active bond length, Le, for one, two, three, and four layers of the system. Compare the effective bond lengths for the various FRP strengthening systems in a bar graph. Is a shorter or a longer effective bond length desirable for shear strengthening? Justify your answers. 10.2 For the FRP strengthening systems in Table P10.1, determine the shear bond-reduction coefﬁcient, v, for one, two, three, and four layers of the strengthening system when used in a three-sided sys-

TABLE P10.1 No. 1 2 3 4

Fiber

FRP Strengthening Systemsa FRP Strengthening System

Carbon SikaWrap Hex 103C (laminate property) Carbon Tyfo SCH 41 (laminate property) Glass WaboMbrace EG900 (ﬁber property) Carbon Sika CarboShear L plates (laminate property)

ƒ*ƒu (ksi) 104.0

E* ƒ (Msi)

tƒ (in.)

9.45 0.040

wƒ (in.) Varies

121.0 11.09 0.040 Varies 220.0 10.5 0.0139 Varies 326.0 17.4 0.055 2

a Properties reported in this table are design properties provided by manufacturers in their current (2006) online speciﬁcation sheets and do not necessarily conform to the deﬁnition of the guaranteed property values in ACI 440.2R-02. They are assumed to be guaranteed properties for the purposes of these problems. For actual design, the user should obtain current guaranteed properties from manufacturers. These data can be compared with those obtained by the reader in Problems 8.2 and 8.3.

312

FRP SHEAR STRENGTHENING

tem.17 The FRP system is to be used to strengthen a 3500-psi rectangular concrete beam with a height of 24 in. and an effective depth of 21 in. The beam is in an exposed highway bridge and is subjected to water, salt, and freeze–thaw conditions (i.e., an aggressive environment). Provide a bar graph comparing the values of the bondreduction coefﬁcient for the various FRP systems and numbers of layers. Discuss your results and compare the effectiveness of the various materials and numbers of layers. 10.3 For the laid-up FRP strengthening systems in Table P10.1 (systems 1, 2, and 3), determine the factored FRP contribution to the shear capacity for one, two, three, and four layers when used in a foursided (complete wrap) system. The FRP system is to be used to strengthen a 3000-psi rectangular concrete beam with a height of 18 in. and an effective depth of 15.5 in. The beam is in interior construction. Provide a bar graph comparing the values of the FRP factored shear contribution for the various FRP systems and numbers of layers. What conclusions can you draw from these data regarding the most effective FRP strengthening system for this beam? 10.4 Derive equation 440.2R-02:10.3, shown below, for the FRP contribution to the nominal shear capacity of a concrete member when intermittent FRP sheets or fabrics are used having width wƒ and spacing sƒ. What are the differences between this equation and the analogous equation for the shear contribution from steel reinforcing bars? Vƒ ⫽

Aƒvƒƒe (sin ␣ ⫹ cos ␣)dƒ sƒ

10.5 Consider Design Example 10.1 and redesign the strengthening system using Sika CarboShear L plates following ACI 440.2R-02 procedures. Assume that the legs of the L plates are terminated at the top of the web. How does your design change if the L plates are anchored into slits in the ﬂange of the T-beam? 10.6 Consider Design Example 10.1 and redesign the FRP strengthening system using the same material as in the Design Example, but use a three-sided two-layer (ply) 90⬚ conﬁguration. Determine the width and the spacing for the two-layer system. Compare the quantity of FRP material used per unit length with that used for the one-layer system in the design example. 10.7 Consider Design Example 10.1 and redesign the FRP strengthening system using the same material as in the design example, but use a

17

Note that CarboShear L plates cannot actually be used in multiply layers; this is just an exercise.

PROBLEMS

313

two-sided two-layer (ply) conﬁguration. Consider three options: (a) One ⫹45⬚ and one ⫺45⬚ layer, (b) one layer at 90⬚ (vertical) and one layer at 0⬚ (horizontal), and (c) two ⫹45⬚ layers. (Note that a 0/90 bidirectional woven fabric with equal ﬁber density in the 0⬚ and 90⬚ directions is a very commonly produced fabric style. If this is rotated through 45⬚, one obtains a ⫹45⬚ / ⫺45⬚ fabric.) Determine the width and spacing of each layer. Compare the quantity of FRP material used in the two options. How do you apply the bond-reduction factor when the two layers are not at the same orientation? Can you think of other advantages to using a ⫹45⬚ and a ⫺45⬚ conﬁguration? 10.8 Determine the angle of inclination of a given intermittent FRP shear strengthening system that provides the most effective shear strength enhancement. Assume that the angle of the critical diagonal crack in the concrete is at 45⬚. Plot the variation of the shear strength contribution from the FRP as a function of the angle from 0⬚ to 90⬚. Is this the same angle as that for a continuous FRP shear strengthening system? 10.9 Reconsider Problem 10.8 but assume that the angle of inclination of the critical diagonal shear crack is 35⬚ rather than 45⬚. 10.10 An existing simply supported reinforced concrete beam in the interior of a building spans 24 ft and is constructed of 5000-psi concrete. The shear reinforcement consists of No. 3 grade 60 stirrups at 10 in. on center. The beam has a 12 ⫻ 24 in. (b ⫻ h) cross section and has a 21.5-in. effective depth, d. The beam was originally designed for a dead load of 1 kip/ft (not including the self-weight) and a live load of 2 kip/ft. Due to change in use of the structure, the dead load is to be increased to 2 kips/ft (not including the self-weight) and the live load increased to 3 kips/ft. Assume that the ﬂexural capacity of the beam is sufﬁcient for future loads (or that it is strengthened appropriately for future loads). Consider two different FRP shear strengthening systems to carry the future loads: (a) A fully wrapped (four-sided) Tyfo SEH-51 glass–epoxy fabric system oriented vertically (at 90⬚ to the beam axis), and (b) a two-sided VSL V-Wrap C200 carbon ﬁber system oriented at 60⬚ to the beam axis. Consult manufacturers’ speciﬁcations online for the guaranteed properties for design. Provide the number of layers, the width, and the spacing of the FRP strengthening system, or the number of layers if the wrap is continuous. Check the strengthening limits. For intermittent designs, use minimum widths of 12 in. Show a side view of the beam, and sketch the location and orientation of the strengthening system for each case. Determine the total area of FRP material used for each case. 10.11 Consider the shear strengthening of the reinforced concrete column described in Design Example 10.2. Redesign the strengthening system

314

FRP SHEAR STRENGTHENING

(consider both a continuous and an intermittent design) if access is available to only three sides of the column, due to an inﬁll wall on the fourth side. Assume that the design shear force is acting parallel to the wall. 10.12 Design a carbon FRP shear strengthening system of your choice to increase the shear capacity by 100 kips in a D ⫽ 30-in.-diameter circular reinforced concrete column in an exterior environment. Assume that the column can be fully wrapped. Use only hoop direction ﬁber orientation in the FRP wrap. Detail the strengthening system and show the amount of overlap required. (Consider the fact that ACI 318 allows one to take the effective depth of a circular column as 0.8D and the width as D for the purposes of determining the concrete contribution and the steel stirrup contribution to shear capacity.) 10.13 A reinforced concrete shear wall in a building forms part of the lateral force resisting system. The wall is 24 ft long, 12 ft high, and 14 in. thick and is on the exterior perimeter of the building. The wall is reinforced with steel reinforcing bars in both directions on both faces. The horizontal wall was originally designed based on shear demand. Due to changes in building code seismic design provisions, the use of shear critical members in buildings of this type is no longer permitted. Rather, the more ductile ﬂexural failure of the wall is desired. To increase the shear capacity of the wall, and hence make the ﬂexural mode critical, the wall needs to be strengthened to carry an additional 300 kips of in-plane shear force. Assume that both faces of the wall can be used but that the ends are not accessible. Also assume that the ﬂexural capacity of the wall is sufﬁcient to carry the lateral loads. Design an FRP strengthening system to increase the shear capacity of the shear wall. Use a laid-up glass FRP strengthening system of your choice. Assume that the wall can be subjected to reverse cyclic loading, which can cause the FRP strengthening system to buckle and detach from the wall. Therefore, mechanical anchors such as ﬁber anchors should be considered. Sketch the layout of the strengthening system. 10.14 Reconsider the shear wall in Problem 13. Due to architectural considerations, only the exterior face of the wall is available for application of the FRP system. Can the wall still be strengthening using an FRP system? Justify your answer by citing the technical literature. Design a one-side shear wall strengthening system if you feel that it is justiﬁed. Review AC 125 (1997). 10.15 Reconsider the design of the circular reinforced concrete column described in Problem 10.12. Design the FRP shear strengthening system using the equations developed by Priestley described in Section 10.6

PROBLEMS

315

(Eq. 10.21). [Do not explicitly consider the shear strength enhancement due to axial loads, and do not adjust the concrete or steel shear strength contributions due to the Priestley equations.18]

18 In an actual design problem where the details of the structure and materials (concrete and steel) and the design target ductility are known, these additional contributions can be incorporated.

11 11.1

FRP Conﬁning

OVERVIEW

This chapter deals with the design of FRP systems to conﬁne reinforced concrete members with compression regions, such as those found in columns, walls, and joint regions, with precured FRP strips and plates and laid-up FRP sheet and fabric systems. At this time, FRP conﬁning is used primarily on columns, and in this chapter we focus on this application. FRP conﬁning can be undertaken for two purposes: (1) to increase the axial load capacity of a column, and (2) to increase the lateral displacement capacity of a column. Only nonprestressed concrete members that are reinforced with conventional steel reinforcing bars are considered. For the purposes of this chapter, it is assumed that the reader is familiar with both the fundamentals and the details of the design of nonslender reinforced concrete columns with conventional steel reinforcing bars. The includes familiarity with construction of load– moment (P–M) interaction diagrams for nonslender columns. Some familiarity with seismic design of reinforced concrete structures is also assumed. The design procedures presented in this chapter for axial capacity enhancement of reinforced concrete columns follow ACI 440.2R-02, which is compatible with ACI 318-99. In recent years there have been signiﬁcant applications of FRP conﬁning to increase both the load-carrying and the displacement ductility of deﬁcient highway bridge columns in seismically active zones. ACI 440-2R.02 does not speciﬁcally address the design issues related to strengthening of columns for increased ductility. A method due to Priestley and colleagues for the design of FRP conﬁning to increase the ductility of reinforced concrete columns, accounting for the axial loads, is presented in this chapter. 11.2

INTRODUCTION

FRP conﬁning can be used to increase the strength and the lateral displacement capacity of reinforced concrete structural members (such as columns, walls, and beams) and reinforced concrete joints and joint regions in reinforced concrete rigid frames. The lateral displacement capacity of a column (also know as the drift) or the transverse displacement capacity of a beam (also known as the deﬂection) when the material response is inelastic and when energy is dissipated has been referred to historically as the plastic ro316

Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

11.2

INTRODUCTION

317

tation capacity or ductility. In recent years there have been attempts to extend the deﬁnition of ductility to include deformation capacity when the material behavior is elastic to failure (Bakht et al., 2000). However, in this chapter, the term ductility is used only to describe a state in which inelastic material response occurs and energy is dissipated, regardless of the extent of the elastic deformation that occurs or the amount of elastic (recoverable) energy that is developed in the member or the structure. The vast majority of the work to date related to retroﬁtting concrete members with FRP wraps has been motivated by increasing the resistance of columns, particularly large circular or ﬂared highway columns, to seismic forces. As discussed in Chapter 1, the ﬁrst use of carbon ﬁber wraps to increase the ductility of reinforced concrete (RC) columns was conducted in Japan in the 1980s (Katsumata et al., 1998) and later in the United States by Fyfe and colleagues (Priestley et al., 1992). The work on FRP conﬁning of RC columns was closely related to work on the conﬁning of RC columns with steel jackets to increase their seismic resistance (Park et al., 1983; Chai et al., 1991). This work was in turn related to work on the effects of conﬁnement on the concrete in a column provided by internal steel spirals (Priestley and Park, 1987). An in-depth review of the historical work and current design recommendations for seismic retroﬁtting of highway bridge columns is provided by Priestley et al. (1996). Only recently have studies been conducted on increasing seismic resistance of RC frames, walls, and joint regions in buildings using FRP composites (Antonopolous and Triantiﬁllou, 2003; Paterson and Mitchell, 2003; Balsamo et al., 2005), and design recommendations for such uses of FRP materials have not been codiﬁed at this time. The use of FRP conﬁning to increase the seismic resistance of reinforced concrete columns is more complex than either FRP ﬂexural strengthening or FRP shear strengthening. This is because the objective of a seismic retroﬁt of an RC column (or frame or wall) is usually not driven by the explicit desire to increase the strength of the member, but rather, is driven by the desire to increase the inelastic lateral displacement capacity (i.e., the ductility). Even though there may not be an explicit desire to increase strength, very often a particular strength increase is needed to increase the lateral displacement capacity. For example, it is well known that larger inelastic displacements (or deﬂections) in RC members (beams, columns, walls) can be obtained when a member is permitted to fail in ﬂexure rather than in shear. This is because internal plastic hinges develop at locations of high bending moments, due to yielding of the internal reinforcing steel. In order, therefore, to permit these large displacements to occur, as a result of the formation of the plastic hinges, the member must often be prevented from failing in other modes before the plastic hinges can develop. These failures can occur in a number of ways. In highway columns the most common among these are shear failure (typically near midheight) and localized failures in the ﬂexural hinge regions due to internal bar rupture or buckling or the failure of lap splices (Seible et al., 1997). In building systems, shear walls can be strengthened (and modiﬁed)

318

FRP CONFINING

to prevent brittle shear failure and cause a preferred ductile ﬂexural failure (Paterson and Mitchell, 2003). The visual appearance of the FRP conﬁning system when applied to an RC member is similar in appearance to that for shear strengthening when a four-sided wrap is used. Figures 11.1 and 11.2 show circular and rectangular RC columns with an FRP conﬁning system being applied to their exterior surfaces. FRP conﬁning systems are usually of the hand-laid-up type and employ ﬁber sheets or fabrics. However, they can also be in the form of precured shells that are bonded in staggered layers to the exterior of the column (see Fig. 1.14) or precured strips that are bonded to a column in spirals (shown in Fig. 11.3), or they can be applied by an automated ﬁber winding machine, as discussed in Chapter 1.

Figure 11.1 FRP system applied to a circular RC column. (Courtesy of Fyfe Company.)

11.2

INTRODUCTION

319

Figure 11.2 FRP wrapping of a rectangular column. (Courtesy of Structural Group.)

Figure 11.3 FRP conﬁnement with a precured spiral-wound FRP strip. (Courtesy of Urs Meier.)

320

FRP CONFINING

As FRP shear strengthening is fundamentally different from FRP ﬂexural strengthening from a mechanics and a constructability perspective, so, too, is FRP conﬁning for strengthening or increasing ductility fundamentally different from both FRP ﬂexural strengthening and FRP shear strengthening. In ﬂexural and shear strengthening, the FRP provides an additional tensile force component to carry either the bending moment or the transverse shear force. Consequently, the FRP must be securely anchored to the RC member. In ACI 440.2R-02 a bond reduction coefﬁcient is used to account for the susceptibility of the FRP ﬂexural or shear strengthening system to detachment from the RC member. In addition, a partial safety factor, ƒ, for the FRP system is used in addition to the standard member resistance factor, , which depends on the conﬁguration of the FRP system (e.g., ƒ is 0.85 for two- and threesided shear systems and 0.95 for four-sided shear systems). In the case of FRP conﬁning, the FRP system when wrapped around the column in the hoop direction appears to perform the role of the internal steel ties or internal steel spiral reinforcement. This, however, is not really the case. Although possibly contributing to the conﬁnement of the concrete core, steel ties and spirals are not designed for such as purpose. Their main purpose is to stabilize and restrain the longitudinal steel reinforcing bars in the compression member (and to provide shear reinforcement in beam-columns). The axial capacity of either a tied or a spirally reinforced RC column is a function of the compressive strength of the concrete, ƒc⬘, and the yield strength, ƒ y, of the steel reinforcing bars. When the steel reinforcing bars yield, the RC column fails in either a more or a less ductile manner, depending on whether spirals or ties are used. Increasing the quantity of ties or spirals can lead to greater axial load-carrying capacity and ductility in an RC column (Mander et al., 1988). However, the increase in axial load capacity is not accounted for in design procedures in an explicit fashion according to ACI 318-99.1 (It is accounted for in the different resistance factors for spiral and tied columns but is not accounted for explicitly as a function of the volume of the spiral reinforcement.) When the FRP hoop reinforcement is added to the exterior of the column, the apparent compressive strength of the concrete is increased. This apparent increase in the concrete strength is due to the conﬁning effect of the FRP, which encircles and wraps the column completely (and thus is often referred to as a jacket). This increased concrete strength, known as the conﬁned com⬘ , occurs only after the concrete in the pressive strength and denoted as ƒcc column has begun to crack and hence dilate. This typically occurs after the internal transverse reinforcing steel has yielded. By preventing the cracked concrete from displacing laterally (or radially), the FRP serves to conﬁne the concrete and allow it to carry additional compressive stress (and hence compressive load). This well-known phenomenon also occurs when a column is

1

ACI 318-99 Section 10.3.6.

11.2

INTRODUCTION

321

constrained by a steel jacket (Chai et al., 1991). After the steel yields and the concrete reaches its unconﬁned compressive strength, ƒc⬘, the concrete continues to increase its load-carrying capacity and displacement until it fails at its ⬘. conﬁned compressive strength, ƒcc The macroscopic stress–strain curve of an FRP conﬁned axially loaded concrete column is shown in Fig. 11.4 together with curves for steel-conﬁned concrete and unconﬁned concrete. The bilinear nature of the effective axial stress–strain curve of the FRP-conﬁned concrete has been veriﬁed in numerous experimental investigations.2 It is important to note that this behavior is different from that of steel jacket–conﬁned concrete, in which the strength decreases after the steel conﬁning jacket yields. Since the FRP jacket is linear to failure, the strength of the conﬁned RC column continues to increase until the FRP wrap fails, due either to tensile stresses or to debonding at the overlap between layers. It has been shown that the ‘‘knee’’ in the bilinear stress–strain curve for the FRP-conﬁned concrete typically occurs at an axial strain close to 0.003 and at the unconﬁned compression strength of the concrete, ƒ⬘c (Nanni and Bradford, 1995; Samaan et al., 1998). Herein lies the fundamental difference between FRP ﬂexural or shear strengthening and FRP conﬁning. In ﬂexural or shear strengthening the FRP serves to add an additional tensile component to that provided by the existing 3.5

Normalized Axial Stress

3.0 2.5 2.0 1.5 Concrete confined with steel hoops

1.0

Concrete confined with FRP wrap Unconfined concrete

0.5 0.0 0

0.005

0.01

0.015

0.02

0.025

0.03

0.035

0.04

0.045

Axial Strain

Figure 11.4 Stress–strain curves for conﬁned and unconﬁned concrete. (Courtesy of A. Mirmiran.) 2 However, many of these investigations have been conducted on small unreinforced compression test cylinders. Scale effects, and the effect of the core and cover (shell) concrete, have yet to be completely resolved for full-sized columns (The´riault et al., 2004).

322

FRP CONFINING

steel internal reinforcing system. The properties of the existing steel and concrete are not changed by the FRP system in these cases. In the case of FRP conﬁning, the FRP system serves to alter the effective compressive properties of the existing concrete. In this manner, FRP conﬁning increases the contribution of the concrete in the internal force equilibrium rather than increasing the contribution of steel reinforcing, as in the case of FRP ﬂexural or shear strengthening. The conﬁning pressure provided by the FRP jacket is uniform around the circumference of the column when the column is circular. A free-body diagram of a half of the cross section of a thin-walled pressure vessel3 is shown in Fig. 11.5. The relationship between the geometric parameters of the column and the thin-walled cylinder (diameter, D, and thickness, t), the circumferential (hoop) stress, ƒ, and the radial stress due to the internal pressure, ƒr, is found from equilibrium as ƒr

2ƒ t D

(11.1)

Substituting ƒ Eƒƒ

(11.2)

and deﬁning the cross-sectional reinforcement ratio as

t

fr fθ

fθ D

Figure 11.5 Free-body diagram of a thin-walled pressure vessel in the cross-sectional plane.

3

Gere and Timoshenko (1997, p. 557).

11.2

ƒ

INTRODUCTION

Aƒ Dntƒ 4ntƒ 2 Ac D /4 D

323

(11.3)

gives the conﬁning pressure in an FRP-wrapped circular column as ƒr

ƒEƒƒ 2

(11.4)

where Eƒ is the FRP modulus in the circumferential direction, ƒ is the FRP strain in the circumferential direction, and n is the number of layers in the FRP wrap. When wrapped around the circumference of the column, an FRP conﬁning system and the concrete in its interior behave like a thin-walled pressure vessel, with the cracked concrete in the interior being the pressurized ‘‘liquid’’ in the cylinder. The amount of conﬁning pressure is linearly related to the circumferential stress, which in the case of an FRP conﬁning wrap is linearly related to the circumferential strain in the FRP wrap. If the FRP material has linear elastic properties in the hoop direction (typically, obtained with a hooponly wrap), the conﬁning stress will increase in a linear fashion until the FRP fails: hence, the bilinear stress–strain curve of FRP-conﬁned concrete. Another very signiﬁcant difference between FRP ﬂexural and shear strengthening and FRP conﬁning is related to the load at which an FRP system begins to take effect. As noted previously, the conﬁning effect takes effect only after the concrete has cracked and begins to dilate. This means that before the concrete cracks, the FRP jacket serves no structural purpose. Because it plays no part in the elastic response of the axially loaded column, it is called a passive strengthening system. Therefore, it is not necessary to consider the existing substrate strain in a concrete column at the time that the FRP conﬁning wrap is attached. This is entirely different from ﬂexural strengthening, where the FRP is active from the moment it is attached, and the prestrain on the substrate needs to be accounted for in the strengthening design. In this regard, FRP conﬁning is somewhat similar to shear strengthening in that it begins to be effective only after shear cracking develops. For noncircular columns, the conﬁning pressure is not uniform around the perimeter of the column and the efﬁciency of the FRP conﬁning decreases significantly. Nevertheless, partial conﬁnement may be possible to obtain with FRP wraps on noncircular columns, as discussed below. The discussion above related to the mechanics of FRP conﬁning has a direct bearing on the constructability of FRP jacketing systems. Since the conﬁning pressure needs to be distributed around the entire circumference (even in the case of a noncircular cross section), the FRP wrap must fully encircle the cross section. Therefore, only complete four-sided FRP wraps can be used for FRP conﬁning. To ensure that a four-sided wrap can maintain the conﬁning pressure required, the FRP wrap must have sufﬁcient strength

324

FRP CONFINING

so as not to fail in tension and must not unravel at its overlapping seams. It is not necessary that the FRP wrap actually be bonded to the surface of the concrete. In fact, it has been shown that unbonded circumferential wraps work as well as bonded ones as long as the end of the wrap does not debond from the layer directly beneath (Katsumata et al., 1988; Nanni and Bradford, 1995; Lees et al., 2002). To prevent the end from unraveling, the wrap must be detailed such that sufﬁcient overlap length exists to prevent a debonding failure. In what follows, FRP conﬁning for the purpose of axial strengthening and FRP conﬁning for the purpose of increasing ductility are discussed separately. 11.3

FRP CONFINING FOR AXIAL STRENGTHENING

Reinforced concrete structural members such as columns and beams can be conﬁned with FRP systems to increase their axial load-carrying capacity. Axial strengthening is most suitable for circular nonslender (i.e., short) reinforced concrete columns. Combined axial and ﬂexural strengthening of short eccentrically loaded reinforced concrete columns will increase their axial and ﬂexural capacity. An axial load-bending moment (P–M) strength interaction diagram can be constructed for an FRP-strengthened reinforced concrete column in a fashion similar to that of a nonstrengthened column. Axial strengthening is obtained by applying the FRP system oriented such that its principal ﬁber direction is in the circumferential (or hoop) direction of the member, perpendicular to its longitudinal axis. In addition to providing axial strengthening, hoop FRP reinforcement provides shear strengthening to the member, since it is oriented perpendicular to the member axis. As noted previously, when strengthening for only a single mode is intended, it is incumbent on the designer to determine the effects of the strengthening on the other modes and to ensure that the member has sufﬁcient capacity in the other modes to resist the higher applied loads. FRP axial strengthening of circular columns can be achieved using either continuous or intermittent coverage. Since the axial load is constant along the full height of the column, the FRP wrap must cover the full height of the column; however, it can be spaced intermittently, in either intermittent or spiral hoop form. It has been shown that the conﬁning effect is reduced when intermittent hoops are used and that the conﬁning effect depends on the spacing of the hoops (or spirals) ( Saadatmanesh et al., 1994; Nanni and Bradford, 1995). Equations to estimate the conﬁnement effectiveness of intermittent hoop strips (or straps) can be found in Saadatmanesh et al. (1994) and Mander et al. (1988). It is important to note that the ACI 440.2R-02 equations presented below apply only to continuous FRP wraps. The theoretical concentric (nominal) axial load capacity of an FRPstrengthened nonslender nonprestressed normal-weight concrete column internally reinforced steel reinforcement is given as

11.3

FRP CONFINING FOR AXIAL STRENGTHENING

P0 0.85ƒƒcc ⬘ (Ag Ast) ƒy Ast

325

(11.5)

where Ag is the gross area of the concrete, Ast the area of the internal longitudinal steel, and ƒy the yield stress of the internal longitudinal steel. Except for the addition of the FRP partial strength reduction factor, ƒ, and use of the conﬁned concrete compressive strength, ƒ⬘cc, instead of the conventional concrete compressive strength, ƒ⬘c, this equation is the same as that used for conventional concrete columns. To account for unintended eccentricities, ACI 318-99 limits the concentric nominal capacity of columns, depending on whether spirals or ties are used for the hoop internal reinforcement. This is called the maximum nominal axial load capacity. For an FRP-strengthened nonslender nonprestressed normalweight concrete column reinforced internally with spiral steel, this is given as Pn(max) 0.85[0.85ƒƒ⬘cc(Ag Ast) ƒy Ast]

(11.6)

The maximum nominal axial capacity of an FRP-strengthened nonslender nonprestressed normal-weight concrete column reinforced internally with tied steel reinforcement is given as Pn(max) 0.80[0.85ƒƒ⬘cc(Ag Ast) ƒy Ast]

(11.7)

where Ag is the gross area of the concrete, Ast the area of the internal longitudinal steel, and ƒy the yield stress of the internal longitudinal steel. According to ACI 440.2R-02, the conﬁned compressive strength, ƒ⬘cc is to be taken as

冉

冪

ƒ⬘cc ƒ⬘c 2.25 1 7.9

冊

ƒl ƒ 2 l 1.25 ƒ⬘c ƒc⬘

(ACI 440.2R-02:11-2)

which is the equation developed for conﬁned concrete strength by Mander et al. (1988). It has been used extensively to predict the strength in columns conﬁned by steel jackets (Chai et al., 1991). It has been shown by Spoelstra and Monti (1999) to be applicable to FRP-strengthened columns, even though the complete stress–strain curve presented by Mander et al. (1988) does not give the appropriate bilinear stress–strain curve that is generally seen in experiments with FRP-conﬁned concrete (Mirmiran and Shahawy, 1997; Nanni and Bradford, 1995; Samaan et al., 1998). Many other equations proposed in the literature exclusively for the conﬁned concrete strength of columns with FRP wraps (Teng et al., 2001) can be used if a full nonlinear moment curvature analysis needs to be performed. However, typically in design equations, only the maximum conﬁned strength and strain are needed.

326

FRP CONFINING

According to ACI 440.2R-02, the conﬁned compressive strength, ƒcc ⬘ , is a function of the unconﬁned concrete strength, ƒc⬘, and the conﬁning pressure provided by the FRP wrap, denoted by ACI 440.2R-02 as ƒl and given as ƒl

aƒEƒƒe 2

(ACI 440.2R-02:11-3)

which is similar to the theoretical equation (Eq. 11.4). The differences are in the notation used for the conﬁning pressure (the l subscript has traditionally been used to denote lateral stress) and in the inclusion of a, which is an efﬁciency factor that depends on the shape of the column. ƒ is the FRP reinforcement ratio deﬁned for circular columns in Eq. (11.3). For fully wrapped systems, ACI 440.2R-02 limits the effective strain in the FRP wrap to ƒe 0.004 0.75ƒƒu

(ACI 440.2R-02:11-4)

At this time, ACI 440.2R-02 recommends using FRP for axial strengthening only for circular columns. In this case the efﬁciency factor a is taken as unity (a 1.0). Although test data do show axial strength increases for rectangular columns (Teng et al., 2001), with FRP hoop wraps such strengthening is not recommended at this time by ACI 440.2R-02, and a value of the efﬁciency factor for axial strengthening of rectangular columns in not provided. Procedures for estimating the effect of the rectangular shape on the conﬁning pressure and the effective area of the concrete core being conﬁned are suggested in TR 55 (2004). Even though ACI 440.2R-02 does not permit the use of FRP wraps to increase the strength of axially loaded rectangular columns, FRP wraps can be used to increase the ductility of rectangular columns according to ACI 440.2R-02, as discussed in what follows. It is important to note that for axial strengthening the ﬁber layers must all be oriented in the hoop direction around the column. If layers are also oriented in the longitudinal direction, these layers should not be considered to contribute to axial (compression) strengthening. If the FRP system is in the form of strips wrapped spirally, only the ﬁber stiffness in the hoop direction should be considered as contributing to the conﬁnement. In this case, Eƒ is found using the transformation equations provided in Chapter 3. The effective failure strain in the hoop direction should still be taken as 0.004 in this case, since this limit is not associated with the strain capacity of the FRP itself but rather, with the shear capacity of the concrete (Priestley et al., 1996, p. 612). 11.3.1

Serviceability for FRP-Strengthened Axial Members

In the service range the concrete in the column cover (or shell) should not approach its transverse cracking strain, and the longitudinal steel should be kept below its yield strain. For this reason, ACI 440.2R-02 limits the service

11.4

DESIGN PROCEDURE FOR FRP AXIAL STRENGTHENING

327

load stress in the concrete to 0.65ƒ⬘c and the service load stress in the longitudinal steel to 0.60ƒy. The stresses in the concrete and the steel at service loads are found from ƒc,s ps

Ec

(11.8)

Ac Ec AstEs

and ƒs,s ps

Es Ac Ec AstEs

(11.9)

where ps is the total axial service load.

11.4 DESIGN PROCEDURE FOR FRP AXIAL STRENGTHENING OF RC CIRCULAR COLUMNS Step 1. Determine the nominal and factored capacities of the existing column. Determine the original design dead and live loads. Determine the strengthening limit. Step 2. Determine the amount of strengthening required. Indicate if this is to be an increase in dead load, live load, or both. Step 3. Choose an FRP strengthening system and determine the effective design strength and strain for the hoop wraps. Step 4. Determine the required number of layers of the strengthening system chosen. To do this, a rearranged form of the analytical equations is used. (i) Determine the required conﬁned concrete compressive strength ƒ⬘cc from ƒ⬘cc

P reqd /0.85 ƒy Ast n h ƒ(Ag Ast)

(11.10)

(h 0.85 for spiral hoops, 0.80 for tied hoops. h is the reduction factor for the maximum nominal axial capacity and must not be confused with , the strength resistance factor.) (ii) Determine the required conﬁning pressure, ƒl, from the quadratic equation

冉

冊

4 4(ƒcc ⬘ /ƒ⬘c 1.25) 40 ƒ⬘cc ƒ ƒl 1.25 (ƒ⬘c)2 ƒ⬘c ƒ⬘c 2 l

2

2.252 0

(11.11)

328

FRP CONFINING

(iii) Determine the number of layers of the FRP material chosen. n

ƒD l 2tƒEƒƒe

(11.12)

Step 5. Recalculate the capacity for the number of layers chosen. Step 6. Check the service-level stresses in the concrete and the steel. Design Example 11.1: FRP Conﬁning for Axial Strengthening of a Concentrically Loaded Circular Column A circular spirally reinforced concentrically loaded nonslender RC column was originally designed to carry a dead load of 320 kips and a live load of 360 kips. It was designed for a concrete strength of 4000 psi and with grade 60 reinforcing steel. The column is exposed to an exterior environment.4 Due to a change in use of the structure, the existing column is subjected to a 60% increase in live-load demand and requires axial strengthening. Two types of FRP strengthening systems are considered: Option (a): a carbon ﬁber sheet with compatible epoxy Option (b): a glass ﬁber fabric with compatible epoxy Following are the details of the existing column obtained from existing plans. Column diameter: h 20 in. Ag 314 in2 Longitudinal steel: 7 No. 11 bars, Ast 10.92 in2 g 0.0347

Spiral reinforcement: No. 3 bars at 2-in. spiral spacing s 0.0115

(Note that some design guides do not recommend FRP axial strengthening if g 3.0%, due to the conﬁning effect of the longitudinal bars, which will prevent dilation of the concrete and activation of the FRP conﬁnement. ACI 440.2R-02 does not impose this restriction.)

4

The original design of this column is given by Wang and Salmon (2002, p. 484).

11.4

DESIGN PROCEDURE FOR FRP AXIAL STRENGTHENING

329

SOLUTION Step 1. Determine the nominal and factored capacities of the existing column. Determine the original design dead and live loads and the strengthening limit. The maximum permitted nominal capacity, Pn(max), of the existing (current) column is found as Pn(max) 0.85[0.85(ƒ⬘c)(Ag Ast) ƒy Ast] 0.85[0.85(4)(314 10.92) (60)(10.92)] 1433 kips

The factored capacity (with 0.75 for spiral hoops per ACI 318-99) is Pn(max) 0.75(1433) 1075 kips 1060 kips

where 1060 kips is the original factored design demand Pu 1.4(320) 1.7(360) 1060 kips. Note that the column is a little overdesigned, due to dimensions and available bar sizes, as is usually the case with a design. Determine the strengthening limit. Since the dead load does not change, this means that the future live-load capacity is limited to 1.2(320) 0.85Lfuture 1.2(320) 0.85Lfuture 1075 kips Lfuture 813 kips Step 2. Determine the amount of strengthening required. Indicate if this is to be an increase in dead load, live load, or both. A 60% increase in the live load is desired [i.e., the new live load is required to be 1.6(360) 576 kips 813 kips]. The new live load of 576 kips is less than the live-load limit of 813 kips determined in step 1. Therefore, the strengthening is permitted by ACI 440.2R-02 for normal use. The future axial demand is Pu 1.4(320) 1.7(576) 1427 kips The minimum factored moment capacity, Pn(max) must be equal to or greater than Pu. Therefore, Pn(max) 1427 kips and the nominal capacity of the strengthened column needs to be Pn(max)

1427 1903 kips 0.75

330

FRP CONFINING

Step 3. Choose an FRP strengthening system and determine the effective design strength and strain for the hoop wraps. For the carbon ﬁber sheet with a compatible epoxy, the following guaranteed properties are obtained from manufacturer speciﬁcations: tƒ 0.0065 in.

ƒu * 0.0167 (1.67%)

ƒ*ƒu 550 ksi

Eƒ 33,000,000 psi

For an exterior exposure the environmental factor for a carbon–epoxy system is 0.85, and the design properties are ƒƒu 0.85(550) 467.5 ksi

0.75ƒu 0.75(0.0142) 0.0106

ƒu 0.85(0.0167) 0.0142 (1.42%)

ƒe 0.004 ⱕ 0.75ƒu

Eƒ 33,000,000 psi (unchanged) For the glass ﬁber fabric with compatible epoxy, the following guaranteed properties are obtained from manufacturer speciﬁcations: tƒ 0.05 in.

ƒu * 0.022 (2.2%)

ƒ*ƒu 83.4 ksi

Eƒ 3,790,000 psi

For an exterior exposure the environmental factor for a glass–epoxy system is 0.65, and the design properties are ƒƒu 0.65(83.4) 54.2 ksi ƒu 0.65(0.022) 0.0143 (1.43%)

0.75ƒu 0.75(0.0143) 0.0107 ƒe 0.004 ⱕ 0.75ƒu

Eƒ 3,790,000 psi (unchanged) Step 4. Determine the required number of layers of the strengthening system chosen. To do this, a rearranged form of the analytical equations is used. For the carbon ﬁber sheet with a compatible epoxy: ⬘, (i) Determine the required conﬁned concrete compressive strength, ƒcc from ƒ⬘cc

(P reqd /0.85) ƒy Ast 1903/0.85 (60)(10.92) n 6.471 ksi h ƒ(Ag Ast) 0.85(0.95)(314 10.92)

11.4

DESIGN PROCEDURE FOR FRP AXIAL STRENGTHENING

331

(ii) Determine the required conﬁning pressure, ƒl, from the quadratic equation: ƒl2

ƒ2l

冉

冊

4 4(ƒ⬘cc /ƒ⬘c 1.25) 40 ƒ⬘cc ƒl 1.25 2 (ƒc⬘) ƒc⬘ ƒ⬘c

2

冉

2.252 0

冊

4 4(6.471/4.0 1.25) 40 6.471 ƒl 1.25 2 (4.0) 4.0 4.0

2

2.252 0

Solving and taking the appropriate root gives ƒl 0.451 ksi 451 psi. (iii) Determine the number of layers of the FRP material chosen. n

ƒD 451(20) l 5.3 2tƒEƒƒe 2(0.0065)(33 106)(0.004)

⬖use six layers

For the glass ﬁber fabric with compatible epoxy: (i) Determine the required conﬁned concrete compressive strength, ƒ⬘cc, from ƒcc ⬘

(P reqd /0.85) ƒy Ast 1903/0.85 (60)(10.92) n 6.471 ksi hƒ(Ag Ast) 0.85(0.95)(314 10.92)

(ii) Determine the required conﬁning pressure, ƒl, from the quadratic equation: ƒl2 ƒ2l

冉

冊

4 4(ƒ⬘cc /ƒ⬘c 1.25) 40 ƒ⬘cc ƒl 1.25 2 (ƒ⬘c) ƒc⬘ ƒ⬘c

冉

2

2.252 0

冊

4 4(6.471/4.0 1.25) 40 6.471 ƒl 1.25 2 (4.0) 4.0 4.0

2

2.252 0

Solving and taking the appropriate root gives ƒl 0.451 ksi 451 psi. Note that steps 4(i) and 4(ii) do not depend on the FRP system. (iii) Determine the number of layers of the FRP material chosen: n

ƒD 451(20) l 5.94 2tƒEƒƒe 2(0.05)(3.79 106)(0.004)

⬖use six layers

Notice that the carbon and glass systems require the same number of FRP layers. The high strength of the carbon cannot be realized since the strain limit of 0.004 controls the design.

332

FRP CONFINING

Step 5. Recalculate the capacity for the number of layers chosen. For the carbon ﬁber sheet with a compatible epoxy,5 calculate the reinforcement ratio: ƒ

Dntƒ 4ntƒ 4(6)(0.0065) Aƒ 0.0078 Ac D2 /4 D 20

Calculate the conﬁning pressure: ƒl

aƒEƒƒe 1.0(0.0078)(33 106)(0.004) 514.8 psi 2 2

Calculate the concrete conﬁned compressive strength:

冉

冪

ƒ⬘cc ƒ⬘c 2.25 1 7.9

冋

冪

冊 冉 冊 冉 冊

ƒl ƒ 2 l 1.25 ƒc⬘ ƒ⬘c

4,000 2.25 1 7.9

册

514.8 514.8 2 1.25 6751 psi 4000 4000

Calculate the maximum nominal capacity: Pn(max) 0.85[0.85ƒƒcc ⬘ (Ag Ast) ƒy Ast] 0.85[0.85(0.95)(6.751)(314 10.92)] 60(10.92) 2127 kips

Calculate the factored capacity and compare with the demand: Pn(max) 0.75(2127) 1595 kips 1427 kips

OK

Step 6. Check the service-level stresses in concrete and steel. The total service load is ps 320 576 896 kips. Ec 57,000兹ƒc⬘ 57,000兹4000 3,604,000 psi 3604 ksi Stresses in the concrete and the steel at service loads are given by

5 Steps 5 and 6 are shown only for the carbon–epoxy system. The glass–epoxy system follows in a similar fashion.

11.5

ƒc,s ps

333

FRP-STRENGTHENED ECCENTRICALLY LOADED COLUMNS

冉

冊

Ec 3604 896 Ac Ec AstEs (314 10.92)(3604) (10.92)(29,000)

2.292 ksi 2292 psi 0.65ƒc⬘ 0.65(4000) 2600 psi → OK

and ƒs,s ps

Es Ac Ec AstEs

冉

896

冊

29,000 (314 10.92)(3604) (10.92)(29,000)

18.44 ksi 18,440 psi 0.60ƒy 0.60(60,000) 36,000 psi → OK

11.5 FRP-STRENGTHENED ECCENTRICALLY LOADED COLUMNS Many reinforced concrete columns are designed to carry both axial load and bending moment since they are eccentrically loaded or they are loaded simultaneously by an axial force and a bending moment. In such a case, a designer will typically construct an axial load–bending moment (P–M) strength interaction diagram to visualize the different combinations of axial load and bending moment that a given column will be able to carry. To construct a P–M diagram for an unstrengthened column, one needs the geometric properties of the cross-section (h, d, d⬘, b, or D, D⬘), the internal reinforcement properties, quantity and placement in the section (ƒy, Es, As, As⬘), and the concrete strength (ƒ⬘c). The maximum strain in the concrete, cu, is taken as 0.003 according to ACI 318-99, and the Whitney stress block is used to represent the nonlinear stress–strain relationship of the concrete at failure in the compression zone. The P–M curve is typically constructed ﬁrst by determining the balanced strain condition and obtaining the values of Pb and eb that correspond to this balanced condition. (Recall that the balanced condition is obtained by setting the strain in the concrete to 0.003 and the strain in the tension steel to sy ƒy /Es.) Thereafter, by choosing different values of the eccentricity, e, either greater than or less than eb points on the interaction diagram in either the tension- or compression-controlled zone are found, and the diagram is constructed. This is described in all textbooks on reinforced concrete design. These days this is accomplished readily with a simple computer program. A typical P–M interaction curve for the nominal capacity of an RC column is shown in Fig. 11.6. Determination of a P–M interaction diagram for an FRP-strengthened column is a nontrivial matter, and limited experimental studies have been re-

334

FRP CONFINING

Pn-axis

Axis of bending

P0

e=

Mn Pn t < y

0.003

e=0

Pb

Section compression controlled

Balanced strain condition

e=

0.003 fy t = y = Transition zone Es Balanced condition Section tension-controlled 0.003

eb

e= M0

Mb Mn-axis

t = 0.005

Mn, bending mooment

Figure 11.6 Schematic load–moment (P–M) interaction diagram for an RC column. (From Wang and Salmon, 2002 with permission from John Wiley & Sons.)

ported on tests to obtain P–M diagrams for FRP-conﬁned columns (Nanni and Norris, 1995). Detailed experimental interaction curves for FRP-conﬁned columns have not been obtained, mainly because these are difﬁcult tests to do, and the demand for such applications is not high. The ACI 440.2R-02 does not directly address the issue of eccentrically loaded FRP conﬁned columns. However, if a number of simplifying assumptions are made, theoretical P–M interaction diagrams for FRP-conﬁned columns can be developed using the equations presented in ACI 440.2R-02. Assumption 1. The FRP conﬁning effect applies to the compressive strength of the concrete regardless of the extent of the compression zone. Then a P–M diagram can be constructed for an FRP-conﬁned column in the same manner as for an unstrengthened column simply by replacing ƒ⬘c with ƒ⬘cc given by the Mander equation. This assumption implies that the compression zone is fully conﬁned by the FRP wrap, even though it does not encircle the compression zone entirely. In addition, ƒ is assumed to be 1.0 for the determination of the nominal axial capacity and nominal moment capacity for points on the P–M diagram (except for Pn(max). If desired a conservative value of ƒ 0.85 can be assumed. Assumption 2. The maximum usable concrete compressive strain for an FRP-wrapped circular column given by ACI 440.2R-02 can be used to determine the neutral-axis depth in the FRP-conﬁned concrete section. The ACI 440.2R-02 equation for the FRP-conﬁned concrete is given as

11.5

FRP-STRENGTHENED ECCENTRICALLY LOADED COLUMNS

⬘cc

1.71(5 ƒcc ⬘ 4ƒc⬘) Ec

335

(ACI 440.2R-02:11-6)

where Ec is the elastic modulus of the original uncracked concrete. Based on these two assumptions and using the maximum conﬁned concrete ⬘ , deﬁned previously, strain, ⬘cc, and the maximum conﬁned concrete stress, ƒcc the P–M interaction curve for an FRP-conﬁned concrete column can be obtained in the same fashion as for an unconﬁned column. For noncircular columns it was noted previously that ACI 440.2R-02 does not permit an increase in strength due to the FRP wrap; however, ACI 440.2R02 does permit an increase in maximum concrete strain. The maximum concrete strain in an FRP-conﬁned rectangular FRP-conﬁned column is given by ACI 440.2R-02:11-6, where the efﬁciency factor, a, for rectangular columns is given as a 1

(b 2r)2 (h 2r)2 3b h(1 g)

(ACI 440.2R-02:11-8)

where h and b are the depth and breadth of the column, r is the corner radius, and g (As As⬘) /Ag is the gross reinforcement ratio. This equation is applicable only when h/b ⱕ 1.5 and when both b and h are less than 36 in., since it has been shown that the conﬁning effect is negligible in rectangular columns with larger aspect ratios and longer sides. The reinforcement ratio for a rectangular FRP-conﬁned column is given as ƒ

2ntƒ(b h) bh

(ACI 440.2R-02:11-7)

It is important to recognize that even though a conﬁned compressive strength for a rectangular column is calculated as an intermediate step in calculating the conﬁned compressive strain, this conﬁned strength should not be used to determine any strength increase in the column. It is used only for determining the maximum conﬁned concrete strain. Therefore, according to ACI 440.2R-02, an FRP-conﬁned P–M interaction curve can be determined for a rectangular column according to the procedures outlined above by utilizing Assumption 2 only. The procedure described above is an approximate procedure that is analogous to the approximate method used for conventional steel-reinforced columns in which the P–M interaction diagram is constructed using the Whitney stress block assumptions. This assumption is made whether the section is conﬁned or unconﬁned (as described above). A more precise method is to construct the P–M diagram using the full stress–strain curve of the FRP-

336

FRP CONFINING

conﬁned concrete (and the unconﬁned concrete, if necessary). In this procedure, the compressive force resultant is found by numerical integration of the nonlinear stress–strain curve for the conﬁned concrete [using stress–strain curves for FRP-conﬁned concrete provided in the literature (see Teng et al., 2001) and not the equation provided by Mander et al. (1988)]. If the FRP strengthening system also provides stiffness in the longitudinal direction of the member in addition to the hoop (circumferential) direction (e.g., when non-90⬚ spiral wraps or when bidirectional fabrics are used), the P–M interaction curve must also account for the strengthening effect of the FRP in the ﬂexural mode. Analysis Example 11.2: Load–Moment Interaction Diagram for an FRPConﬁned Column Consider a column with a rectangular section having a width w 12 in., a depth h 14 in., and a concrete strength ƒ⬘c 6000 psi. It is reinforced with four No. 11 bars (two at each end) with a yield strength of ƒy 60,000 psi and has tied hoops for transverse reinforcement. The effective depth of the section is d 11 in. and the depth to the compression bars is d⬘ 3. The moment is applied about the strong axis of the column. The column is in an interior unexposed environment. The column is wrapped its full height with three layers of carbon–epoxy FRP having the following properties: tƒ 0.0065 in., Eƒ 33 106 psi, ƒ* * 0.017. For the indoor environment, CE 0.95 and ƒu 550,000 psi, ƒu ƒƒe 522,500 psi, and ƒe 0.01615. Prior to application of the FRP material, the corners of the concrete column are rounded with a radius of r 1.0 in. The nominal and ultimate load–moment (P–M) interaction diagrams are constructed for three cases: 1. The unstrengthened column6: ƒ⬘c 6000 psi and cu 0.003. 2. The FRP-wrapped column assuming only an increase in the conﬁned concrete strain: ƒ⬘c ƒ⬘cc 6000 psi and cu ⬘cc. 3. The FRP-wrapped column assuming an increase in the conﬁned con⬘ and cu ⬘cc. crete strain and the conﬁned concrete strength: ƒc⬘ ƒcc (Note that this case is not permitted by ACI 440.2R-02, since an increase in axial load-carrying capacity is not permitted at this time for a rectangular section. It is provided for illustrative purposes.) SOLUTION Step 1. Determine the conﬁned compressive strength and strain in the FRPwrapped column.

6

The unstrengthened case is presented in Nawy (2003, p. 339).

11.5

FRP-STRENGTHENED ECCENTRICALLY LOADED COLUMNS

ƒ

2ntƒ(b h) 2(3)(0.0065)(12 14) 0.00604 bh 12(14)

g

As As⬘ 3.12 3.12 0.0371 Ag 12(14)

a 1

337

(b 2r)2 (h 2r)2 [12 2(1)]2 [14 2(1)]2 1 3bh(1 g) 3(12)(14)(1 0.0371)

0.4972

ƒl

aƒEƒƒe 0.4972(0.00604)(33 106)(0.01615) 799.7 psi 2 2

冉

冪

ƒcc ⬘ ƒ⬘c 2.25 1 7.9

冋

冪

冊

ƒl ƒ 2 l 1.25 ƒ⬘c ƒc⬘

冉 冊 冉 冊

6000 2.25 1 7.9

册

700.7 799.7 2 1.25 6000 6,000

10,243.5 psi ⬇ 10,244 psi ⬘cc

⬘ 4ƒ⬘c) 1.71[5(10,244) 4(6000)] 1.71(5ƒcc 0.0105 1.05% Ec 57,000兹6000

Step 2. Determine Pn and Mn for select points on the interaction diagram for the three cases considered. (a) P–M points A and B, axial load only The nominal and the ACI maximum capacity for the column are calculated using the ACI formula. The nominal moment corresponding to the ACI maximum axial capacity is found by assuming a minimum eccentricity of emin 0.1h 1.4 in. Case 1: P0 0.85 ƒc⬘(Ag Ast) ƒy Ast 0.85(6000)(168 6.24) 60,000(6.24) 1,199,376 lb 1199 kips

Pn(max) 0.80P0 0.8(1199) 959 kips Mn Pn(max)emin 959(1.4) 1343 in.-kips

338

FRP CONFINING

Case 2: P0 0.85ƒƒcc ⬘ (Ag Ast) ƒy Ast 0.85(1.0)(6000)(168 6.24) 60,000(6.24) 1,199,376 lb 1199 kips

Pn(max) 0.80P0 0.8(1199) 9.59 kips Mn Pn(max)emin 959(1.4) 1343 in.-kips Note: Since it is assumed that the FRP wrap does not increase concrete compressive strength, the strength reduction factor is set to unity (i.e., ƒ 1.0). Case 3: P0 0.85ƒƒcc ⬘ (Ag Ast) ƒy Ast) 0.85(0.95)(10,244)(168 6.24) 60,000(6.24) 1,712,814 lb 1713 kips

Pn(max) 0.80P0 0.8(1713) 1370 kips Mn Pn(max)emin 1370(1.4) 1918 in.-kips Note: ƒ 0.95 for determination of Pn(max) only. For all the cases above, the resistance factor for the axially loaded tied column is taken as 0.7 according to ACI 318-99. (b) P–M point C, balanced strain The balanced strain condition deﬁnes the limit of the compression-controlled region of the P–M diagram. At this point, the steel yields at the same instant as the concrete fails in compression (theoretically). The Whitney stress block is used to determine the compressive force resultant in the concrete. Case 1: c

cud 0.003(11) 6.509 in. cu sy 0.0003 0.00207

a 1c 0.75(6.509) 4.882 in. ⬘s cu

冉

c d⬘ 6.509 3 0.003 c 6.509

0.00162 0.00207

冊

⬖ compression steel has not yielded

ƒ⬘s (29 106)(0.00162) 46,980 psi

11.5

339

FRP-STRENGTHENED ECCENTRICALLY LOADED COLUMNS

Cc 0.85ƒ⬘cba 0.85(6000)(12)(4.882) 298,778 lb Cs ƒs⬘As⬘ 46,980(3.12) 146,578 lb Ts ƒy As 60,000(3.12) 187,200 lb Pn Cc Cs Ts 298,778 146,578 187,200 258,156 lb 258 kips

冉 冊 冉 冊 冉 冊 冉 冊 冉 冊

Mn Cc

h a h h Cs d⬘ Ts d 2 2 2 2

298,778

冉

2,697,241 in.-lb 2697 in.-kips

e

Mn 2697 10.45 in. Pn 258

Case 2: c

⬘ccd 0.0105(11) 9.189 in. ⬘cc sy 0.0105 0.00207

a 1c 0.75(9.189) 6.861 in. ⬘s ⬘cc

冊

14 4.882 14 14 146,578 3 187,200 11 2 2 2 2

冉

c d⬘ 9.189 3 0.0105 c 9.189

0.00707 0.00207

冊

⬖ compression steel has yielded

ƒ⬘s ƒy 60,000 psi Cc 0.85ƒ⬘cba 0.85(6000)(12)(6.861) 419,893 lb Cs ƒs⬘As⬘ 60,000(3.12) 187,200 lb Ts ƒy As 60,000(3.12) 187,200 lb Pn Cc Cs Ts 419,893 187,200 187,200 419,893 lb 420 kips

340

FRP CONFINING

冉 冊 冉 冊 冉 冊 冉 冊 冉 冊

Mn Cc

h a h h Cs d⬘ Ts d 2 2 2 2

419,893

冉

冊

14 6.861 14 14 187,200 3 187,200 11 2 2 2 2

2,996,408 in.-lb 2996 in.-kips

e

Mn 2996 7.13 in. Pn 420

Case 3: c

⬘ccd 0.0105(11) 9.189 in. ⬘cc sy 0.0105 0.00207

a 1c 0.65(9.189) 5.973 in. (1 0.65 since ƒ⬘cc 8,000 psi) ⬘s ⬘cc

冉

c d⬘ 9.189 3 0.0105 c 9.198

0.00707 0.00207

冊

⬖ compression steel has yielded

ƒ⬘s ƒy 60,000 psi Cc 0.85ƒ⬘ccba 0.85(10,244)(12)(5.973) 624,112 lb Cs ƒs⬘ A⬘s 60,000(3.12) 187,200 lb Ts ƒy As 60,000(3.12) 187,200 lb Pn Cc Cs Ts 624,112 187,200 187,200 624,112 lb 624 kips

冉 冊 冉 冊 冉 冊 冉 冊 冉 冊

Mn Cc

h a h h Cs d⬘ Ts d 2 2 2 2

624,112

4,002,474 in.-lb 4002 in.-kips

e

冉

冊

14 5.973 14 14 187,200 3 187,200 11 2 2 2 2

Mn 4,002 6.41 in. Pn 624

11.5

341

FRP-STRENGTHENED ECCENTRICALLY LOADED COLUMNS

Note that for all other points on the interaction curve: If e eb, the section is tension controlled. If e eb, the section is compression controlled. The resistance factor is equal to 0.70 for all cases for both Mn and Pn since the section is still regarded as being compression controlled. (c) P–M point D, tension-controlled transition point The tensile strain in the steel at the tension-controlled transition point is set to 0.005 to ensure a ductile ﬂexural failure of the section according to the ACI code. Case 1: cud 0.003(11) 4.125 in. cu s 0.003 0.005

c

a 1c 0.75(4.125) 3.094 in. ⬘s cu

冉

c d⬘ 4.125 3 0.003 c 4.125

0.00082 0.00207

冊

⬖ compression steel has not yielded

ƒs⬘ (29 106)(0.00082) 23,727 psi Cc 0.85ƒ⬘cba 0.85(6000)(12)(3.094) 189,353 lb Cs ƒs⬘As⬘ 23,727(3.12) 74,028 lb Ts ƒy As 60,000(3.12) 187,200 lb Pn Cc Cs Ts 189,353 74,028 187,200 76,181 lb 76 kips

冉 冊 冉 冊 冉 冊 冉 冊 冉 冊

Mn Cc

h a h h Cs d⬘ Ts d 2 2 2 2

187,353

2,066,548 in.-lb 2,067 in.-kips

e

冉

冊

14 3.094 14 14 74,028 3 187,200 11 2 2 2 2

Mn 2067 27.20 in. Pn 76

342

FRP CONFINING

Case 2: c

⬘ccd 0.0105(11) 7.452 in. ⬘cc s 0.0105 0.005

a 1c 0.75(7.452) 5.589 in.

冉

c d⬘ 7.452 3 0.0105 c 7.452

⬘s ⬘cc

0.00627 0.00207

冊

⬖ compression steel has yielded

ƒ⬘s ƒy 60,000 psi Cc 0.85ƒ⬘cba 0.85(6000)(12)(5.589) 342,046 lb Cs ƒs⬘As⬘ 60,000(3.12) 187,200 lb Ts ƒy As 60,000(3.12) 187,200 lb Pn Cc Cs Ts 342,046 187,200 187,200 342,046 lb 342 kips

冉 冊 冉 冊 冉 冊 冉 冊 冉 冊

Mn Cc

h a h h Cs d⬘ Ts d 2 2 2 2

342,046

2,936,074 in.-lb 2936 in.-kips

e

冉

冊

14 5.589 14 14 187,200 3 187,200 11 2 2 2 2

Mn 2936 8.58 in. Pn 342

Case 3: c

⬘ccd 0.0105(11) 7.452 in. ⬘cc s (0.0105 0.005)

a 1c 0.65(7.452) 4.844 in.

11.5

⬘s ⬘cc

343

FRP-STRENGTHENED ECCENTRICALLY LOADED COLUMNS

冉

c d⬘ 7.452 3 0.0105 c 7.452

0.00627 0.00207

冊

⬖ compression steel has yielded

ƒs⬘ ƒy 60,000 psi Cc 0.85ƒ⬘cc ba 0.85(10,244)(12)(4.844) 506,144 lb Cs ƒs⬘As⬘ 60,000(3.12) 187,200 lb Ts ƒy As 60,000(3.12) 187,200 lb Pn Cc Cs Ts 506,144 187,200 187,200 506,144 lb 506 kips

冉 冊 冉 冊 冉 冊 冉 冊 冉 冊

Mn Cc

h a h h Cs d⬘ Ts d 2 2 2 2

506,144

冉

冊

14 4.844 14 14 187,200 3 187,200 11 2 2 2 2

3,814,727 in.-lb 3815 in.-kips

e

Mn 3815 7.54 in. Pn 506

The resistance factor is equal to 0.90 for all cases for both Mn and Pn since the section is tension controlled. The region where 0.00207 s 0.005 is known as the transition region and the resistance factor varies between 0.70 and 0.90 (according to ACI 318-99), depending on the tensile strain in the internal steel reinforcing bars. (d) P–M point E, pure bending The ﬂexural capacity of the section is calculated assuming that A⬘s 0. At this point the column is, in fact, a beam, and a traditional ﬂexural analysis is performed. Case 1: a

Asƒy 3.12(60,000) 3.059 in. 0.85ƒ⬘cb 0.85(6,000)(12)

c

a 3.059 4.078 in. 1 0.75

344

FRP CONFINING

s

dc 11 4.078 cu (0.003 0.0051 0.005 c 4.078

冉 冊

Mn Asƒy d

冉

⬖ 0.90

冊

a 3.059 3.12(60,000) 11 2 2

1,772,878 in.-lb 1773 in.-kips

Case 2: a

Asƒy 3.12(60,000) 3.059 in. 0.85ƒ⬘cb 0.85(6,000)(12)

c

a 3.059 4.078 in. 1 0.75

s

dc 11 4.078 ⬘cc (0.0105) 0.0178 0.005 c 4.078

冉 冊

Mn Asƒy d

冉

⬖ 0.90

冊

a 3.059 3.12(60,000) 11 2 2

1.772,878 in.-lb 1773 in.-kips

Case 3: a

Asƒy 3.12(60,000) 1.792 in. 0.85ƒcc ⬘b 0.85(10,244)(12)

c

a 1.792 2.756 in. 1 0.65

s

dc 11 2.756 ⬘cc (0.0105) 0.0314 0.005 c 2.756

冉 冊

Mn Asƒy d

冉

⬖ 0.90

冊

a 1.792 3.12(60,000) 11 2 2

1.891,469 in.-lb 1892 in.-kips

Table 11.1 shows the results obtained above for the three cases considered. The table also includes data for a number of additional points on the P–M

11.5

FRP-STRENGTHENED ECCENTRICALLY LOADED COLUMNS

345

TABLE 11.1 P–M Data for Three Cases Case 1

2

3

Point A B

C D E A B

C D E A B

C D E

s sy sy

0 0.0003 0.0011 0.00207 0.0050 0.0051 sy sy

0 0.0011 0.00207 0.0050 0.0107 sy sy

0 0.0011 0.00207 0.0050 0.0314

c (in.)

Pn (kips)

Mn (in.-kips)

e (in.)

1199 960 692 619 435 261 76 0 1199 960 692 551 421 342 0 1712 1506 934 771 624 506 0

0 1344 2200 2349 2555 2699 2067 1773 0 1344 2200 2260 2997 2963 1773 0 2108 3307 3675 4002 3814 1891

0 1.4 3.17 3.79 5.87 10.36 27.2

— 11.0 10.0 8.0 6.60 4.13 4.08

— 11.0 10.0 9.19 7.45 4.08

— 11.0 10.0 9.19 7.45 2.76

0 1.4 3.17 4.75 7.11 8.58

0 1.4 3.54 4.68 6.41 7.54

0.70 0.70 0.70 0.70 0.70 0.70 0.90 0.90 0.70 0.70 0.70 0.70 0.70 0.90 0.90 0.70 0.70 0.70 0.70 0.70 0.90 0.90

curves whose calculation is not shown above but follows in an identical manner. The schematic nominal load–moment interaction diagram is shown in Fig. 11.7. It can be seen that the effect of the FRP conﬁnement for the rectangular column is small when only the conﬁning effect on the compressive strain in the concrete is considered (case 2). If the conﬁning effect on the concrete compressive strength is considered (which is not permitted by ACI 440.2R02 at this time), the P–M diagram is expanded signiﬁcantly. In both cases 2 and 3, the transition region (C to D) from the steel strain of 0.005 to the yield strain (0.00207) is much smaller than for the unconﬁned concrete (case 1). It is also important to recall that this is a schematic of the load–moment interaction diagram, where the discrete points (obtained by using the Whitney approximation) that were evaluated have been joined by straight lines. The true load–moment interaction diagram obtained by using the nonlinear stress strain relations for the concrete will have curved lines (as seen in Fig. 11.6). In addition, the horizontal portion of the interaction diagram, which represents the ACI maximum axial load cutoff, intersects the current diagram at a point deﬁned by the minimum eccentricity. Using a nonlinear stress–strain relation for the concrete would enable one to ﬁnd this point precisely.

346

FRP CONFINING

1800

A

1600

Case 1 Case 2 Case 3

B

1400

Pn (kips)

1200

A B

1000 800

C

600 C

400 C

200 E

0 0

D

D

E 2000

1000

D

3000

4000

5000

M n (in.-kips)

Figure 11.7 Nominal load–moment interaction diagram.

The ultimate load–moment interaction diagram is shown in Fig. 11.8 (without the ACI maximum axial load cutoff, for the sake of clarity). It is plotted on the same axes as Fig. 11.6 so that the reduction in the extent of the diagram can be seen. In addition to the reduced size, it is interesting to note the shape of the diagram in the tension transition region up to the balanced strain point of the FRP conﬁned column (cases 2 and 3). This dramatic discontinuity is not seen in the unconﬁned column (case 1). This is due to the increased

1800 1600

Case 1 Case 2 Case 3

Pu (kips)

1400 1200 1000

A B A

800

B

600 400

C

200 E

0 0

1000

C D

D

C D E 2000

3000

4000

5000

Mu (in.-kips)

Figure 11.8 Ultimate load–moment interaction diagram.

11.6

FRP CONFINING FOR INCREASED DUCTILITY

347

compressive strain in the conﬁned concrete. The design of FRP-conﬁned columns in the transition region should be avoided. In addition, the FRP reduction factor, ƒ, has not been included in the ultimate (and nominal) diagrams. This will tend to decrease the size of these diagrams for the FRP strengthened columns. 11.6

FRP CONFINING FOR INCREASED DUCTILITY

The equations presented above for the maximum conﬁned concrete strain for both circular and rectangular columns can be used to design a column to increase its lateral displacement capacity, which is of utmost importance in the seismic design of reinforced concrete structures (Paulay and Priestley, 1992). At this time, ACI 440.2R-02 does not provide detailed instructions on how to use the conﬁned concrete strength to design an FRP retroﬁt system for increasing the ductility of a column. Since this topic is of increasing importance to structural engineers wishing to use FRP materials to retroﬁt concrete structures for increased seismic resistance it is reviewed brieﬂy in this section. At this time the only existing codiﬁed equations for the design of FRP systems to increase the lateral displacement capacity of RC columns have been published in Japanese guidelines (JSCE, 2001). The Japanese code equations are not presented in this book as they refer back to symbols and derivations in the Japanese code that cannot be fully explained here; however, the reader is encouraged to consult this source for further code-based procedures on using FRP to increase lateral ductility in columns. Design equations have also been developed by Priestley et al. (1996) and Seible et al. (1997) for conﬁning RC columns (primarily, highway bridge columns) using FRP jackets, based on pioneering work by these authors and colleagues on retroﬁtting of RC columns with steel and FRP jackets. In what follows, the Priestley approach is outlined. 11.6.1

Lateral Displacement Ductility

Lateral displacement ductility of a structural system depends on the lateral displacement ductility of individual components of a structure, one of these being the member’s lateral displacement ductility (Priestley et al., 1996). In what follows, only the member’s (in particular, a column’s) lateral displacement ductility is addressed. For the relationship between the member’s ductility and the structural ductility, the reader is referred to Paulay and Priestley (1992) and Priestley et al. (1996). The lateral displacement, or drift, of a column when subjected to horizontal forces is due primarily to ﬂexure of the column and is deﬁned as the relative horizontal displacement between the bottom and the top of the column. The total or ultimate lateral displacement of a reinforced concrete column at fail-

348

FRP CONFINING

ure is denoted as ⌬u. This ultimate lateral displacement is made up of an elastic part and an inelastic (or plastic) part. The lateral displacement at the end of the elastic response is known as the yield displacement, ⌬y. The difference between the ultimate displacement and the yield displacement is known as the plastic displacement, ⌬p ⌬u ⌬y. The member lateral ductility displacement factor is deﬁned as the ratio of the yield displacement to the ultimate displacement: ⌬

⌬p ⌬u 1 ⌬y ⌬y

(11.13)

Displacement ductility factors of 6 to 8 are generally recommended for current seismic design (Priestley et al., 1996). Many older reinforced concrete columns have displacement ductility factors of 2 to 3, making them extremely susceptible to failure under seismically induced lateral loads. To increase the displacement ductility factor of a column, the plastic displacement ductility must be increased. This is achieved by conﬁning the concrete in the column to increase its plastic ﬂexural hinge capacity while simultaneously preventing the column from failing prematurely in shear or debonding of the internal reinforcing bars, due to less than required splice overlap lengths. These debonding failures may be either at the column ends, where bars are lap-spliced to foundation ‘‘starter’’ bars, or at the interior of the column, at bar ﬂexural cutoff points. It is very important to note that the contribution of the conﬁning FRP wrap to the shear capacity, the ﬂexural hinge capacity, and the bar lap splice capacity are interrelated. The design of an FRP wrap for increasing the lateral displacement ductility of a column implies that all three of these modes are addressed. The Japanese code (JSCE, 1997) equation for lateral ductility enhancement includes the shear capacity explicitly. Others (Seible et al., 1997) provide separate equations for shear (discussed in Chapter 10), ﬂexural hinge, and lap splice FRP conﬁnement design. 11.6.2

Flexural Hinge Conﬁnement

The conﬁning of the ﬂexural hinge region serves to increase the failure strain of the concrete. The plastic ﬂexural hinge capacity can also be increased by providing additional longitudinal FRP strengthening in the plastic hinge region; however, this requires very careful detailing to ensure that the tensile loads in the FRP can be transferred to the foundation at the column ends at the location of the largest moments. Corresponding to the yield and ultimate displacements mentioned previously, yield moments and curvatures, My and y, and the ultimate moments and curvatures, Mu and u, are deﬁned.7 According to Paulay and Priestley 7 Determination of the yield and ultimate moments and curvatures requires a full non-linear moment-curvature analysis of the section which is beyond the scope of this book. Therefore, no example problems are presented in this section and the reader is referred to Priestley et al. (1996) and Seible et al. (1997) for example calculations.

11.6

FRP CONFINING FOR INCREASED DUCTILITY

349

(1992), the yield moment may be taken as the moment at the ‘‘knee’’ in an approximated bilinear moment–curvature curve for the column. This occurs when all the tensile steel is not at the same depth from the neutral axis and does not yield at the same time (e.g., in a circular column with axial reinforcement distributed equally around the circumference). In this case the yield moment is typically greater than the moment at ﬁrst yielding of the tensile steel in the column and can be approximated as (Paulay and Priestley, 1992, p. 136) My 1.33Myi

(11.16)

where Myi is the moment corresponding to the ﬁrst (or initial) yield in the section. The yield curvature, y, is taken from a linearization of the moment– curvature graph for the section. According to Paulay and Priestley (1992, p. 138), y can be approximated as (except when very high axial reinforcement ratios or high axial forces are present) y 1.33yi

(11.17)

where yi is the curvature at initial yielding of the section, given as yi

sy d cyi

(11.18)

where sy is the yield strain in the tension steel and cyi is the depth of the neutral axis at the time of ﬁrst steel yielding in the section, which is obtained from a moment-curvature analysis of the section. When high axial forces (or high axial reinforcement ratios) exist the concrete will ‘‘yield’’ before the steel and yi is taken as yi

c

cy

(11.19)

with c taken as 0.0015. The ultimate moment, Mu, is deﬁned as the bending moment at ultimate capacity and includes effects of ‘‘overstrength’’ as well as the effects of conﬁnement on the concrete maximum compressive strain and strength (if applicable) (see Paulay and Priestley, 1992). The ultimate curvature can be determined from the concrete strains in the ultimate state as u

cu

cu

(11.20)

350

FRP CONFINING

where cu is the maximum compression strain at the extreme ﬁber in the concrete and cu is the depth of the section neutral axis at the ultimate moment, which is obtained from a full moment-curvature analysis of the section. It is important to remember that in all of the columns considered in this section, the column is subjected to both axial and ﬂexural loads and that the depth of the neutral axis depends on both the value of the axial force and the value of the bending moment. In general, the presence of the axial load will increase y and decrease u (Paulay and Priestley (1992) p. 138). When the yield moment is reached at either the bottom or the top of the column (or both), local yielding will occur in this ﬁnite-length region, which is known as the ﬂexural plastic hinge region. According to Priestley et al. (1996), the length of the plastic hinge region in a column conﬁned by internal spirals or ties is Lp 0.08L 0.15ƒy db ⱖ 0.3ƒy db

(11.21)

where L is the distance from the point of maximum moment (in the plastic hinge region) to the point of zero moment in the column, ƒy is the yield strength (in ksi) of the longitudinal reinforcement in the plastic hinge region, and db is the diameter of a longitudinal reinforcing bar. When the column is conﬁned by an external FRP jacket, the length of the plastic hinge region can be taken as the lower bound of equation (11.21): Lp 0.3ƒy db g

(11.22)

where g is the radial gap between the jacket and the concrete column. For FRP wraps, g can usually be taken as zero since the FRP wrap is applied directly to the surface of the column. The curvature ductility is then given as

u y

(11.23)

and the member displacement ductility factor is given as (Priestley et al., 1996, p. 310) ⌬

冉

冊

Lp Lp Mu 3( 1) 1 0.5 My L L

(11.24)

If it is assumed that the conﬁnement effect on the bending moment capacity of the column is small (as demonstrated in Example 11.2), and the additional ﬂexural overstrength is ignored, Mu My and equation (11.24) becomes (see Paulay and Priestley, 1992)

11.7

351

DESIGN PROCEDURE FOR FLEXURAL HINGE CONFINEMENT

⌬ 1 3

冉

冊 冉

冊

Lp Lp u 1 1 0.5 y L L

(11.25)

For the FRP conﬁned section, it is further assumed that the ultimate curvature can be determined from the conﬁned concrete strain u

⬘cc

cu

(11.26)

11.7 DESIGN PROCEDURE FOR FLEXURAL HINGE CONFINEMENT For a required ductility, the conﬁned concrete compressive strain and the depth of the neutral axis at yield and at ultimate need to be determined for a given axial load. For a trial number of FRP layers of a selected FRP material system, the conﬁned compressive stress can be found, and thereafter the conﬁned compressive strain can be found (both using the ACI 440.2R-02 formula). With the known value of the conﬁned compressive strain, the depth of the neutral axis at ultimate can be found and the ductility factor can be determined. This requires a trial-and-error procedure using a full momentcurvature analysis. An alternative empirical procedure is presented by Seible et al. (1997) to obtain the conﬁned compressive strain in the FRP-wrapped concrete (denoted as ⬘cu to differentiate it from both ⬘cc and cu). In their approach, the conﬁned compressive strength, ƒcc ⬘ , is taken as 1.5 times the unconﬁned compressive strength, and the conﬁned compressive strain in a circular column is given as ⬘cu 0.004

2.8ƒ ƒƒeƒe 2.8ƒƒƒeƒe 0.004 ƒcc ⬘ 1.5 ƒc⬘

(11.27)

where ƒƒe and ƒe are the effective FRP strength and maximum strain in the hoop direction, respectively. For rectangular columns, Seible et al. (1997) recommend modifying equation (11.27) by assuming that the FRP wrap is half as effective, to give ⬘cu 0.004

1.4ƒ ƒƒeƒe 1.4ƒƒƒeƒe 0.004 ƒcc ⬘ 1.5ƒc⬘

(11.28)

In the Seible et al. (1997) approach, the curvature ductility is taken as

352

FRP CONFINING

⬘cu

cu y

(11.29)

where cu and y are obtained from a full moment–curvature analysis of the section. Following ACI 440.2R-02 procedures, a ﬂexural strength resistance factor of 0.9 and an FRP strength reduction factor of ƒ 0.95 should be used in determine the required number of layers of FRP for conﬁnement of the ﬂexural hinge region. For circular columns with aspect ratios deﬁned by M/ VD 4, additional checks should be performed to ensure that bar buckling does not occur in the ﬂexural hinge region (Priestley et al., 1996, p. 314). 11.8

LAP SPLICE REGION CONFINEMENT

FRP wraps in the location of the lap splice in the internal reinforcing bars can be used to ensure that column failure will not occur prematurely due to bond failure of internal reinforcing bars. In experimental studies it has been found that lap splice failures in concrete columns occur when the circumferential strains in the concrete are between 0.001 and 0.002. The lower limit of 0.001 is recommended for FRP wraps (Seible et al., 1997). In Seible et al. (1997) the required conﬁning pressure in the lap splice region (also known as the clamping pressure) is given as ƒl

Abƒy [(p/2nb) 2(db cc)]Ls

(11.30)

where Ab, and db are the area and diameter of a single steel internal bar, nb is the number of spliced bars along the perimeter, p, and cc is the clear concrete cover to the main bars (requiring clamping). Ls is the length of the lap splice for the internal bars and ƒy is the yield strength of the internal bars. Ignoring the conﬁning pressure provided by existing spirals or ties, the lateral pressure can then be written in terms of the FRP reinforcement ratio using the limiting design strain in the FRP of ƒe 0.001, to give ƒl

aƒEƒƒe 0.0005aƒEƒ 2

(11.31)

Rearranging gives the required FRP reinforcement ratio as ƒ

2000ƒl aEƒ

(11.32)

For a circular column with diameter D and a 1.0, the number of layers of the FRP wrap chosen is therefore

11.9

PLASTIC SHEAR OVERSTRENGTH DEMAND

n

500Dƒl Eƒtƒ

353

(11.33)

The FRP wrap should extend over the length of the bar lap splice, Ls. If lap splice lengths are too short, conﬁnement of the lap splice region may not be possible (Priestley et al., 1996).

11.9

PLASTIC SHEAR OVERSTRENGTH DEMAND

Equations for designing a four-sided FRP wrap for shear strengthening of a column according to ACI 440.2R-02 were presented in Chapter 10. Alternative procedures following Priestley et al. (1996) that include the effects of axial load on shear strength were also presented in Chapter 10. As noted previously, to increase the lateral displacement ductility of a column, its shear strength must be adequate to resist the shear forces in both the ﬂexural hinge region, where large plastic rotations occur, and in the interior of the column. To ensure sufﬁcient shear strength to enable the full inelastic ﬂexural capacity of the section to be developed, the shear demand is increased for columns that are conﬁned to increase their lateral ductility. This is known as the maximum plastic shear demand or shear overstrength demand (Paulay and Priestley, 1992) and is denoted as V0 0

My L

(11.34)

where My is the yield moment capacity of the column and L is the height of the column for a column in single curvature (cantilever) and half the height for a column in double curvature (ﬁxed–ﬁxed). For FRP conﬁnement the shear overstrength parameter, 0, is recommended to be 1.5 (Seible et al., 1997). Since different amounts of FRP may be needed for lap-splice conﬁnement, ﬂexural hinge conﬁnement, and shear strength enhancement of a single column, three different wrap reinforcement ratios (and types of reinforcement) could be used simultaneously. The lengths, number of layers, and types of FRP used in the various regions must be clearly marked out on construction plans. It is also important to recognize that if the column requires only ﬂexural hinge conﬁnement to increase its displacement ductility (assuming that the shear strength of the original column is sufﬁcient and that lap splice conﬁnement is not needed), only a portion of the column (near the joint) may need to be wrapped. This is the reason that many photographs of highway bridge retroﬁts (see Fig. 1.12, for example) show FRP wraps only near the bottom of columns, not over their entire height.

354

FRP CONFINING

PROBLEMS 11.1

For the FRP strengthening systems listed in Table P11.1, determine the conﬁning pressure, ƒl, provided by one, two, three, and four layers of the system when used on interior circular reinforced concrete columns with diameters, D, of 16, 24, and 36 in. Provide bar graphs comparing the conﬁning pressures for the various numbers of layers and various column diameters for each FRP system.

11.2

For the FRP strengthening systems listed in Table P11.1, determine the conﬁned concrete compressive strength, ƒ⬘cc, when three layers of the system are used to conﬁne an exterior circular reinforced concrete column with a diameter, D, of 30 in. Consider unconﬁned concrete compressive strengths, ƒ⬘c, of 3000, 5000, and 8000 psi. Provide bar graphs comparing the conﬁned concrete compressive strength for the various unconﬁned concrete strengths for each FRP system.

11.3

For the FRP strengthening systems listed in Table P11.1, determine the maximum conﬁned concrete compressive strain, ⬘cc, when three layers of the system are used to conﬁne an exterior circular reinforced concrete column with a diameter, D, of 30 in. Consider unconﬁned concrete compressive strengths, ƒc⬘, of 3000, 5000, and 8000 psi. Provide bar graphs comparing the maximum conﬁned concrete compressive strain for the various unconﬁned concrete strengths for each FRP system.

11.4

For the FRP strengthening systems listed in Table P11.1, determine the maximum conﬁned concrete compressive strain, ⬘cc, when three layers of the system are used to conﬁne an interior rectangular reinforced concrete column with a depth, h, of 30 in. and a breadth, b, of 20 in. Assume a longitudinal steel reinforcement ratio, g, of 3%

TABLE P11.1

FRP Strengthening Systemsa

No.

Fiber

FRP Strengthening System

ƒ* ƒu (ksi)

E*ƒ (Msi)

tƒ (in.)

1 2 3 4

Glass Aramid Carbon Carbon

SikaWrap Hex 107G (laminate property) Tyfo SAH 41 (laminate property) VSL V-Wrap C-100 (laminate property) WaboMBrace C530 (ﬁber properties)

86.0 88.0 105.0 510.0

3.57 4.64 8.20 54.0

0.040 0.050 0.020 0.0065

a Properties reported in this table are design properties provided by manufacturers in their current (2006) online speciﬁcation sheets and do not necessarily conform to the deﬁnition of the guaranteed property values in ACI 440.2R-02. They are assumed to be guaranteed properties for the purposes of these problems. For actual design, the user should obtain current guaranteed properties from manufacturers. These data can be compared with those obtained by the reader in Problems 8.2 and 8.3.

PROBLEMS

355

and that the corners of the column are rounded to a radius, r, of 0.75 in. Consider unconﬁned concrete compressive strengths, ƒc⬘, of 3000, 5000, and 8000 psi. Provide bar graphs comparing the maximum conﬁned concrete compressive strain for the different unconﬁned concrete strengths for each FRP system. 11.5

A 18-in.-diameter short exterior concrete column needs to be strengthened to resist an additional 100 kips of concentric axial load (50% dead load and 50% live load). The column has 5% longitudinal grade 60 steel, has tied hoops and has ƒ⬘c 4000-psi-design strength concrete. Design and detail a SikaWrap Hex 107G strengthening system to increase the axial load-carrying capacity of the column. Check the strengthening limits (assuming a dead load/live load ratio of 1⬊1 in the original column) and the limiting strains in the FRP and steel in the strengthened column.

11.6

A 16-in.-diameter short exterior concrete column needs to be strengthened to resist an additional 50 kips of concentric axial load (50% dead load and 50% live load). The column has 2% longitudinal grade 60 steel and has tied hoops and has ƒ⬘c 4000-psi-design strength concrete. Design and detail a strengthening system to increase the axial load-carrying capacity of a VSL V-Wrap C-100 strengthening system. Check the strengthening limits (assuming a dead load/live load ratio of 1⬊1 in the original column) and the limiting strains in the FRP and steel in the strengthened column.

11.7

To strengthen a circular reinforced concrete column, it is proposed to use a precured Sika Carbodur 2-in.-wide FRP strip wound spirally around the column at an angle to the horizontal (see Fig. 11.3 for an example). Since the conﬁning effect is due to the hoop reinforcement, the effective modulus, Eƒ(), in the hoop (horizontal) direction is needed to do the design (assuming that the strength of the system is governed by the 0.004 strain limit). Plot the modulus of the Carbodur system in the hoop direction as a function of the wind angle of the strip relative to the horizontal. At what spiral angle does the system start to become ineffective for conﬁnement? (Hint: You need to use the stiffness transformation equations in Chapter 3. To do this you need the four in-plane orthotropic elastic constants of the strip. Since the manufacturer does not supply these, you will need to make assumptions and estimates using micromechanics. Justify all your assumptions.) Also note that to use this type of system for conﬁnement, equations for intermittent strips provided in the literature must be used.

11.8

Consider the 20-in.-diameter circular column in Design Example 11.1. Determine the maximum conﬁned concrete strain that can be obtained when the column is wrapped with six layers of the carbon

356

FRP CONFINING

sheet system (option a) and with six layers of the glass fabric system (option b). 11.9

Construct a schematic P–M interaction diagram for the circular column in Design Example 11.1 (option b, glass ﬁber fabric) in the same manner as that done for the rectangular column in Analysis Example 11.2. Use an appropriate formula to transform the circular column in to an idealized equivalent rectangular column (e.g., Nawy, 2003, p. 331).

11.10 Consider the rectangular column in the P–M interaction diagram in Analysis Example 11.2. Construct nominal and ultimate P–M diagrams for the column wrapped with ﬁve layers of a Sikawrap Hex 107G FRP strengthening system. Compare the P–M diagram with that obtained in Analysis Example 11.2.

SUGGESTED PROJECT ACTIVITY 11.1 Laboratory assignment.8 The objectives of this assignment are (1) to wrap a concrete ‘‘column’’ (actually, a standard 6 12 in. cylinder) with various FRP strengthening systems, (2) to test the wrapped columns and to determine the strengthened axial capacity experimentally, and (3) to use ACI analytical models to predict the axial capacity enhancement of the wrapped columns and to compare the prediction with the test results. Directions: 1. Obtain samples of FRP strengthening systems.9 Wrap and test two strengthened cylinders and two unstrengthened cylinders. 2. Use a single layer of the FRP wrap in the hoop direction only. 3. Overlap one-fourth of the circumference. 4. Leave about –14 in. at the top and bottom of the cylinder uncovered so that the FRP does not contact the compression test machine’s load head.

8

Note to instructor: This is an easy FRP strengthening project to assign to students. It does not take much in the way of materials or resources. It is best to cast a batch of cylinders at the beginning of the semester for both the strengthened and unstrengthened cylinder test. If the class is large, different materials and numbers of layers can be assigned to different groups and the results compared. 9 If samples of proprietary FRP strengthening systems cannot be obtained from manufacturers, purchase glass ﬁber woven fabric (about 9 to 12 oz / yd2) and epoxy resin from any marine supply store. This is for laboratory purposes only and should not be used for actual FRP strengthening projects.

SUGGESTED FRP STRENGTHENING STRUCTURAL DESIGN PROJECTS

357

5. Allow the FRP to cure, then test the cylinders. Test in displacement control (if possible) to a displacement beyond the peak load. Observe the behavior and the failure modes of the strengthened and unstrengthened cylinders. 6. Plot the stress–strain curves for the strengthened and unstrengthened cylinders on the same graph. 7. Determine the experimental maximum axial capacity of each specimen. 8. Use the ACI 440.2R-02 equations to calculated the maximum conﬁned strength, the axial capacity, and the maximum conﬁned axial strain in the concrete. 9. Compare the experimental and theoretical values for strength and strain at failure.

SUGGESTED FRP STRENGTHENING STRUCTURAL DESIGN PROJECTS The following design projects are suggested for students in a composites for construction design class. The types of projects selected are those in which FRP strengthening systems are known to be beneﬁcial. The design project should preferably be done in groups of two or three students. Students should be given 4 to 6 weeks to compete the design project (which therefore needs to be assigned early in the semester). The ﬁnal deliverable should be a design proposal10 that includes the problem statement, scope, codes and speciﬁcations, loads, materials, design calculations, design drawings, and a cost analysis. A presentation of the design proposal should be given in class. A discussion of the current condition of the existing structure and any problems is recommended. Invite owners and designers to form part of the project jury to obtain feedback from industry on the designs presented. 11.1 FRP strengthening of parking garage T-beams. Design an FRP shear strengthening system for the webs of typical double-T precast and prestressed concrete beams. Scout your local area and identify a precast parking garage built in recent years using a system of this type. Use the dimensions of one of the typical double-T beams in the structure. Obtain plans, if possible, or take approximate measurements from the structure. (Typical double-Ts have a top ﬂange 12 ft wide by 4 in. deep, a tapered web 30 in. by approximately 5 in., and spans of 60 to 90 ft.) Assume that the shear capacity of the webs needs to be increased to carry an additional superimposed dead load of 20 lb/ft2 on the simply supported double-Ts.

10

Items listed are at the discretion of the instructor.

358

FRP CONFINING

11.2 Strengthening a reinforced concrete slab. Design an FRP ﬂexural and shear strengthening system to increase the load-carrying capacity of a reinforced concrete pedestrian bridge. Scout your local area and identify a reinforced concrete bridge or elevated walkway (such as a footbridge over a road or an elevated walkway between buildings) that has a concrete slab ﬂoor (or deck). Obtain plans for the structure, if possible. Design a ﬂexural strengthening system to increase the live-load capacity on the slab by 50%. If the slab is supported on concrete beams and stringers, design the strengthening system for these elements as well. If the walkway is supported on columns (without drop panels), consider the punching shear capacity of the slab. 11.3 Strengthening a ﬂoor slab to accommodate a cutout. Design a FRP strengthening system to strengthen a reinforced concrete ﬂoor slab in a university building to accommodate a 3 5 ft cutout (penetration) for new mechanical equipment to be installed. Place the cutout at the center of the slab. Obtain plans for a typical ﬂoor beam and column layout. Consult with local experts on how this would be accomplished with conventional engineering materials and propose an FRP strengthening alternative. 11.4 Increasing the capacity of a concrete column. Design an FRP wrap to increase the axial load capacity of a reinforced concrete column. Scout your local area and identify a free-standing exposed exterior reinforced concrete column (either as part of a building frame or a support for a walkway or small bridge). Design an FRP strengthening system to increase the axial load capacity on the column by 40%. If the column is rectangular, suggest alternatives design guides to ACI 440.2R-02 to achieve this objective.

12 12.1

Design Basis for FRP Proﬁles

OVERVIEW

In this chapter we provide an introduction to the design of structures with ﬁber-reinforced polymer (FRP) proﬁles produced by the pultrusion method. In this and the following chapters we focus on commercially manufactured thin-walled pultruded glass FRP proﬁles of I-, box-, channel-, and angleshaped sections. However, there is no standard for the dimensions or properties of these proﬁles. Guidance is provided on where to obtain these data. There is also no approved code or guide for the design of pultruded structures, and therefore the design basis for pultruded structural design needs to be deﬁned by the designer (as opposed to simply being chosen by the designer of FRP rebars and strengthening systems as in previous chapters). Guidance is provided on how to develop both an allowable stress design (ASD) basis and a load and resistance factor design (LRFD) basis for pultruded structures. Speciﬁc forms of an ASD and an LRFD basis are recommended for use in design. These are used in later chapters to design pultruded structural members, such as tension members, beams, columns, and connections. Thin-walled FRP components can also be produced using other FRP manufacturing processes, such as ﬁlament winding, resin-transfer molding, and centrifugal casting. Such specialty FRP components are generally not intended for use by structural engineers in truss or framed structures, are not identiﬁed as structural sections by their manufacturers, and are therefore not covered by the design guidelines presented in what follows. The reader is assumed to have some familiarly with the properties of orthotropic materials and the mechanics of laminated plates, discussed in Chapter 3. A review of that chapter is highly recommended prior to studying this section of the book. Background and familiarity in the behavior of thin-walled steel sections are required. The reader should know how to design steel truss and frame structures, including the design of chords, ties, struts, beams, columns, and connections and should also have knowledge of the failure modes of thin-walled steel members and structures. The reader is expected to have some familiarity with both allowable stress design (ASD) and load and resistance factor design (LRFD) procedures, for steel structures in particular (AISC, 2005). In addition, reference is made to the European limits states design (LSD) basis. Some knowledge of the design of structures following the European partial factor approach is recommended. Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

359

360

12.2

DESIGN BASIS FOR FRP PROFILES

INTRODUCTION

Truss structures and braced framed structures have been designed and constructed with FRP pultruded members for over 30 years. Pultruded structural proﬁles1 (referred to as pultrusions, or pultruded shapes, or pultruded members) have been used in a signiﬁcant number of structures to date, including pedestrian bridges, vehicular bridges, building frames, stair towers, cooling towers, and walkways and platforms, as described and illustrated in Chapter 1. Pultruded proﬁles are often the structural members of choice where signiﬁcant corrosion and chemical resistance is required (such as in food and chemical processing plants, cooling towers, and offshore platforms), where electromagnetic transparency is required (such as in electronics manufacturing plants), or where accessibility is limited and lightweight skeletal structures are assembled on site (such as for pedestrian bridges in parklands). Pultrusion is a continuous and highly cost-effective manufacturing technology for producing constant-cross-section ﬁber-reinforced-plastic2 (FRP) structural proﬁles.3 Pultruded proﬁles are made of pultruded materials. Pultruded materials consist of ﬁber reinforcements (typically, glass ﬁber or carbon ﬁber) and thermosetting resins (typically, polyester, vinylester, and epoxy polymers). The ﬁber architecture within a thin panel or plate (such as a web or a ﬂange) in a pultruded proﬁle typically consists of longitudinal continuous ﬁber bundles (called rovings or tows) and continuous ﬁlament mats (CFMs).4 In specialized custom pultruded proﬁles, bidirectional stitched fabrics are also used to improve mechanical or physical properties. The volume fraction of the ﬁber reinforcement in a pultruded proﬁle is typically between 30 and 50%. In addition to the base polymer resin, pultruded materials typically contain inorganic ﬁllers, chemical catalysts and promoters, release agents, ultraviolet retardants, ﬁre retardants, pigments, and surfacing veils. Commercially produced pultruded proﬁles made with glass ﬁbers cost $2 to $4 per pound. Custom pultruded proﬁles utilizing high-performance carbon ﬁbers, sophisticated fabrics, and high-performance resin systems may be considerably more expensive. Pultruded proﬁles are produced for use in commercial products (such as ladders and window frames) and for use in building and bridge structures (such as beams, columns, and truss members). The former are often referred to as nonstructural applications; the latter are referred to by civil and structural

1 In what follows, the term pultruded proﬁle is used when referring to the part itself. Pultruded member (or beam or column) is used when referring to the structural design. 2 The term ﬁber-reinforced plastic as opposed to polymer is used most commonly in the industry when referring to these FRP proﬁles. 3 The reader is referred to Chapter 2 for a more in-depth discussion of pultruded materials and pultrusion processing. 4 More commonly known in the United States as continuous strand mats.

12.2

INTRODUCTION

361

engineers as structural applications.5 Most commercial product proﬁles are custom designed and have unique shapes that are compatible with their end markets. Most structural product proﬁles are produced in conventional proﬁle shapes similar in geometry to those of metallic materials (e.g., steel and aluminum) such as the I-, wide ﬂange (WF), angle, tube, and channel proﬁles (Fig. 12.1). Pultruded proﬁles for commercial and structural applications are produced by many pultrusion manufacturers around the world. Most manufacturers produce custom proﬁles for commercial applications. Only the larger manufacturers produce the conventional structural proﬁles discussed in this book. These include Strongwell, Creative Pultrusions, and Bedford Reinforced Plastics in the United States, Fiberline in Denmark, TopGlass in Italy, and Paciﬁc Composites in Australia, Asia, and the UK. A number of industry groups represent and loosely coordinate the activities of pultrusion manufacturers. Leading groups are the Pultrusion Industry Council of the American Composites Manufacturers Association (ACMA) and the European Pultrusion Technology Association (EPTA). There is a similarity in the geometry and properties of the pultruded proﬁles produced by different manufacturers; however, no standard geometries and standard mechanical and physical properties for pultruded proﬁles are used by all (or even some) manufacturers at this time (2006). Nevertheless, these conventional proﬁles are commonly referred to as standard pultruded structural proﬁles. In this book they are referred to as conventional proﬁles. Company-speciﬁc literature provides details of the geometries and mechanical properties of their conventional proﬁles (e.g., Fiberline, 2003; Creative Pultrusions, 2004; Strongwell, 2002; Bedford, 2005). Commonly produced conventional pultruded proﬁles that are usually available from stock inventories include I, wide-ﬂange, square tube, rectangular tube, channel, and angle proﬁles, as well as plate materials. Standard proﬁles range from 2 in. (50 mm)

Figure 12.1 Conventional pultruded proﬁles: I, wide ﬂange, angle, tube, and channel. (Courtesy of Racquel Hagen.) 5 This is not meant to imply that nonstructural pultruded proﬁles may not have a structural purpose—rather, that they are not used in structural engineering as load-carrying structural members in buildings and bridges.

362

DESIGN BASIS FOR FRP PROFILES

in height and width to approximately 12 in. (300 mm) in height and width and have pultruded material thicknesses of –14 to –12 in. (6 to 13 mm). At this time there are no consensus guidelines for the design of framed structures using either conventional or custom pultruded structural proﬁles as there are for concrete structures reinforced with FRP rebars or strengthened with FRP strengthening systems. However, two design manuals that have been developed by consensus procedures are available for structural engineers: the Structural Plastics Design Manual (ASCE, 1984) and the Eurocomp Design Code and Handbook (Eurocomp, 1996). Guidance provided by these two consensus manuals is presented below. Since the early 1980s, many laboratory studies have been conducted to investigate the behavior of pultruded structural members (mostly on wideﬂange and tubular proﬁles used in beams and columns). Based on these studies, there is sufﬁcient evidence to conﬁrm that the analytical equations presented in the consensus manuals and in the technical literature for structural members are suitable for use when designing framed structures with conventional pultruded proﬁles. Analytical equations for designing connections between pultruded members are less well developed or validated, and as discussed below, are still mostly empirically based (which is similar to connections in steel structures). Although the suitability of the speciﬁc analytical equations provided in the manuals to predict the behavior of pultruded members has been demonstrated, there is signiﬁcantly less consensus on what safety factors (for allowable stress design) and resistance factors (for load and resistance factor design) to use in structural design. In addition to the two consensus manuals noted above, a number of companies have produced their own design manuals over the years. The most comprehensive manuals of this type at present are those by Creative Pultrusions (2004), Strongwell (2002), and Fiberline (2003). According to current company literature, the ﬁrst Extren engineering manual was published by Strongwell (then known as Morrison Molded Fiberglass Company) in 1979, and the ﬁrst Pultex design manual was published by Creative Pultrusions in 1973. Fiberline published their ﬁrst design manual in 1995. Recently, Bedford Reinforced Plastics published their ﬁrst manual (Bedford, 2005). Equations and load tables provided for design in these manuals are based on company testing and are intended to be used only with the proﬁles produced by the company whose manual is being consulted. These company design manuals and other useful property and design data are available at the Internet addresses listed in the reference section. There are many excellent classic texts on the mechanics and to some extent the design of composite materials for aerospace and mechanical engineering structures. These include classics by Tsai and Hahn (1980), Daniel and Ishai (1994), and Agarwal and Broutman (1990). Texts by Hollaway (1993), Kim (1995), Barbero (1999), and Kolla´r and Springer (2003) bridge the gap between the mechanics of composite materials and composite structures and

12.3

PROPERTIES OF PULTRUDED PROFILES

363

have more emphasis on applications to civil engineering but do not explicitly cover the design of structures with pultruded proﬁles.

12.3

PROPERTIES OF PULTRUDED PROFILES

Conventional pultruded proﬁles are constructed of ﬂanges and webs of orthotropic thin plates in which the principal axes of orthotropy of the discrete plates (referred to as walls in what follows) in the proﬁle are aligned with global axes of the proﬁle as illustrated in Fig. 12.2. This type of orthotropic plate, known as a specially orthotropic plate, was discussed in Chapter 3. The internal architecture of the plate elements, which may consist of roving bundles, fabrics, and mats, is such that the laminate is assumed to be both balanced and symmetric, in order to prevent extensional-shear coupling and extensional-ﬂexural coupling (Tsai and Hahn, 1980, p. 217) in the plate and in the proﬁle. The in-plane constitutive relation for a specially orthotropic plate made of a laminated material is given as (see Chapter 3)

冦冧

0 1 0 2 0 6

冤

1 E 01 0 ⫽ ⫺ 210 E1 0

0 ⫺ 120

E2 1 E 02

0

0 0 1 E 06

冥

冦冧 1 2 6

(12.1)

where 0i are the in-plane strains in the plate and i are the (average) in-plane stresses in the plate in the longitudinal (1), transverse (2), and shear (6) directions, respectively. The in-plane engineering constants are E 01, longitudinal

y T

x

L T L

z

T L

Figure 12.2 Relationship between local and global coordinates in a pultruded proﬁle.

364

DESIGN BASIS FOR FRP PROFILES

modulus; E 02, transverse modulus; 012, major Poisson ratio; 021, minor Poisson ratio; and E 06, in-plane shear modulus. As noted in Chapter 3, only four of these ﬁve properties are independent. In structural engineering, a different notation is used to identify the directions and hence the constants and the stresses and strains in a plate of a pultruded proﬁle. The in-plane directions are identiﬁed as the longitudinal (L), transverse (T), and shear (LT) directions. The out-of-plane direction is referred to as the through-the-thickness direction (TT). The in-plane stiffness constants are deﬁned as EL, longitudinal modulus; ET, transverse modulus; L, major Poisson ratio6; T, minor Poisson ratio; and GLT, in-plane shear modulus. The in-plane stresses are identiﬁed as L, T, and ; the in-plane strains are identiﬁed as L, T, and ␥. [Note, however, that in manufacturers’ design guides, the longitudinal direction is often referred to as the machine or pultrusion direction and called the lengthwise (LW) direction, and the transverse direction is called the crosswise (CW) direction.] In analysis it is often assumed that the longitudinal and transverse moduli are the same in tension and compression. This is often not the case. Manufacturers generally report tensile and compressive moduli separately. In this case, the superscript t is used for tension, and the superscript c is used for compression. The in-plane strengths of an orthotropic plate in a pultruded proﬁle are characterized with ﬁve independent constants. In Chapter 3 these ﬁve strength constants were identiﬁed as Xt, longitudinal tensile strength; Xc, longitudinal compressive strength; Yt, transverse tensile strength; Yc, transverse compressive strength, and S, in-plane shear strength. In structural engineering these are identiﬁed as, L,t, L,c, T,t, T,c, and LT. The out-of-plane (through-thethickness) properties of an orthotropic plate of pultruded material are generally not measured and are not used in design. The exception to this is the interlaminar shear strength (ILSS), also known as the short beam shear (SBS) strength, which is measured routinely. It is a measure of the through-thethickness (TT) shear strength of the laminate and is identiﬁed as TT. In addition, for design purposes a quasistructural pin-bearing strength in either the longitudinal or transverse direction is also measured and identiﬁed as, L,b or T,b. Since a plate of pultruded material is not homogeneous through its thickness [i.e., it consists of layers or laminae (or plies) of ﬁber-reinforced materials that have different in-plane properties], the in-plane ﬂexural properties are not the same as the in-plane extensional properties. However, as noted in Chapter 3, laminates are typically thin and loaded in-plane in structural proﬁles. Consequently, in design formulas for pultruded proﬁles in structural engineering, the in-plane effective engineering properties of the laminate are

6 A shorthand form is used for Poisson ratios in this book for the sake of brevity and to avoid confusion with the order of the subscripts for the major and minor Poisson ratios, which depends on the mechanics deﬁnition used (i.e., LT or TL).

12.3

PROPERTIES OF PULTRUDED PROFILES

365

used in design calculations. In thin-shell structures where laminates are loaded out of plane, the ﬂexural properties are used. The in-plane stiffness properties may be calculated using classical lamination theory (CLT), in which the pultruded plate is characterized by its in-plane extensional stiffness coefﬁcients, Aij, as discussed in Chapter 3. Alternatively, the in-plane engineering stiffness properties may be obtained from standard tests on coupons extracted from the pultruded proﬁle. In this approach, the laminate is assumed to be homogeneous. Standard ASTM tests that are recommended for determining the properties of pultruded materials are listed in Table 3.1. Since the orthotropic plates in the pultruded proﬁle are assumed to be homogeneous on a macromechanics level, the plate ﬂexural properties can be calculated from their in-plane extensional engineering properties (obtained either from test data or from the in-plane extensional matrix). This assumption is made routinely in the analysis of pultruded structures and is appropriate given the geometrical properties of pultruded proﬁles. The orthotropic plate ﬂexural rigidities (the equivalents of EI per unit width for a beam) are given as DL ⫽

ELtp3 12(1 ⫺ LT)

(12.2a)

DT ⫽

ET tp3 12(1 ⫺ LT)

(12.2b)

T ELtp3 LET tp3 ⫽ 12(1 ⫺ LT) 12(1 ⫺ LT)

(12.2c)

GLT tp3 12

(12.2d)

DLT ⫽

DS ⫽

where DL, DT, DLT, and DS are the longitudinal, transverse, coupling, and shear ﬂexural rigidities and tp is the plate thickness. The ﬂexural rigidities relate the plate bending moments (per unit length) to the plate curvatures and are measured in units of force ⫻ length. In classical texts on plate behavior, the equations of state are written in terms of plate ﬂexural rigidities (e.g., Timoshenko and Woinowsky-Krieger, 1959), and this notation is often used in analytical equations for pultruded proﬁles. The in-plane strength properties may be obtained from theoretical calculations or from testing of coupons taken from the laminate. Where theoretical predictions are used, the ﬁrst ply failure (FPF) is assumed to represent the strength of the laminate. Coupon testing is recommended for obtaining the strength properties for structural design, as discussed in Chapter 3.

366

DESIGN BASIS FOR FRP PROFILES

The European Standard EN 13706 (CEN 2002b) is currently the only published standards document that speciﬁes minimum properties for various grades of pultruded materials. The two grades speciﬁed for pultruded proﬁles by EN 13706 are E23 grade and E17 grade. The grade number is taken from the minimum longitudinal tensile modulus of the grade in GPa. The minimum properties for the two grades and the tests required for obtaining them are listed in Table 12.1.7 Also listed in Table 12.1 are additional mechanical and physical properties that EN 13706 deﬁnes as being optionally reported properties; no limits are speciﬁed for these. Property data provided in pultrusion manufacturer design guides are obtained from tests on coupons of pultruded materials taken from pultruded proﬁles. Data reported are typically applicable to a broad range of proﬁle sizes and types. The speciﬁc ﬁber architectures (volume fractions of roving, mats, and fabrics) in the different proﬁle sizes and types varies. Fiber architecture may also vary within the proﬁle (e.g., web reinforcement architecture may be different from ﬂange reinforcement architecture). The properties given by manufacturers can be assumed to be lower bounds for the class of proﬁles indicated in the manuals. No data are provided to determine the statistics of these properties for use in probability-based design. In addition, the property data are not related to the capacity of members subjected to speciﬁc loading conditions (e.g., axial load, ﬂexure). Published data are based on coupon testing. Representative mechanical property data for pultruded materials used in commercially available pultruded proﬁles, ﬂat sheets, and rods are given in Table 1.4. The properties of a pultruded carbon–epoxy precured strip for FRP strengthening is shown for comparison purposes. Selected physical and electrical property data for pultruded materials reported by manufacturers is shown in Table 1.5. For design purposes, it is generally assumed that pultruded materials behave in a linear elastic manner in tension, compression, and shear in both the longitudinal and transverse directions and that failure is brittle. These assumptions are reasonable in the service range (⬃20% ultimate) but are not reasonable, especially in the shear and transverse directions, at higher strains, where the stress–strain behavior is found to be highly nonlinear and the failure may be progressive. Since the current design of the majority of pultruded proﬁles is controlled by serviceability criteria (e.g., deﬂections) and large factors of safety8 are currently used in the ultimate limit state, service stress levels around 20% are reasonable. Conventional pultruded proﬁles are often assumed to be homogeneous on the proﬁle level (i.e., the proﬁle consists of plates all having the same prop-

7

These test methods are discussed in greater detail in Chapter 3. Currently, the factors of safety used in design are larger than for conventional materials. However, they are expected to decrease as our understanding of the properties and design methods for pultruded structures increases. 8

12.3

TABLE 12.1

PROPERTIES OF PULTRUDED PROFILES

367

Properties of Pultruded Materials Minimum Properties

Property

Test Method

a

Units

E23 Grade

E17 Grade

Minimum Properties That Are Required for Each Grade Full-section bending modulus Tensile modulus Longitudinalb

Annex D, EN 13706-2

GPa (Msi)

23 (3.3)

17 (2.5)

EN ISO 527-4

GPa (Msi) GPa (Msi)

23 (3.3) 7 (1.0)

17 (2.5) 5 (0.7)

MPa (ksi) MPa (ksi)

240 (34.8) 50 (7.3)

170 (24.7) 30 (4.4)

Annex E, EN 13706-2 Annex E, EN 13706-2

MPa (ksi) MPa (ksi)

150 (21.8) 70 (10.2)

90 (12.1) 50 (7.3)

Flexural strength Longitudinal

EN ISO 14125

Transverse

EN ISO 14125

MPa (ksi) MPa (ksi) MPa (ksi)

240 (34.8) 100 (14.5) 25 (3.6)

170 (24.7) 70 (10.2) 15 (2.2)

Transverse

EN ISO 527-4

Tensile strength Longitudinal

EN ISO 527-4

Transverse

EN ISO 527-4

Pin-bearing strength Longitudinal Transverse

Interlaminar shear strength, longitudinal

EN ISO 14130

Material Properties That May Be Reportedc Compression strength Longitudinal Transverse Fiber content by weight Density Poisson ratio Longitudinal Transverse Thermal expansion Longitudinal Transverse In-plane shear modulus

EN ISO 14126 EN ISO 14126 ISO 1183 ISO 1183

MPa MPa % kg / m3

EN ISO 527-4 EN ISO 527-4 ISO 11359-2 ISO 11359-2 ISO 15310

10⫺6 ⬚C⫺1 10⫺6 ⬚C⫺1 GPa

Source: EN 13706. a Original minimum values are in SI units. U.S. Customary values are converted and are rounded off. b EN 13706 refers to the longitudinal direction as the axial direction. c No minimum (or maximum) properties are stipulated for either grade material in EN 13706.

368

DESIGN BASIS FOR FRP PROFILES

erties). However, it should be noted that some manufacturers (e.g., Creative Pultrusions) have modiﬁed their proﬁles and provide properties separately for the webs and the ﬂanges of many of their proﬁles. For the purposes of analysis, it is assumed that the properties of the junctions between the plates (e.g., the web–ﬂange junctions in an I-proﬁle) are the same as those of the plates themselves. Testing, shows this not to be the case, however. Determination of these very local properties is exceedingly difﬁcult (Turvey and Zhang, 2005). The ratio of the longitudinal modulus to the shear modulus, EL /GLT, for pultruded orthotropic plates can be larger than that for isotropic plates. For typical glass-reinforced pultruded proﬁles it is approximately 6 (as opposed to 2.6 for isotropic materials). Because of this fact and the fact that pultruded proﬁles are generally more stocky9 than metal proﬁles, shear deformation can play a signiﬁcant role in the analysis of thin-walled pultruded proﬁles. The effects of shear deformation should be accounted for in deﬂection calculations and may need to be considered in stability calculations, as discussed below. The properties of pultruded proﬁles are affected by the environment in which the proﬁles are used. These environmental-use effects can include time, temperature, radiation, solvents, ﬁre, impact, abrasion, and fatigue. The way in which these effects are accounted for in design is not yet clear. For some conditions (e.g., temperature and creep) some guidance is available. The safety factors recommended by pultrusion companies for use in design are intended to account for some of these effects. In the case of elevated-temperature service, pultrusion companies speciﬁcally recommend reductions in strength and stiffness properties as a function of temperature for various resin systems (usually, isophthalic polyester or vinylester). Table 12.2 gives retention data for strength and stiffness properties of pultruded proﬁles recommended by Strongwell for their proprietary pultruded materials. Long-term changes in stiffness and strength can be accounted for using analytical methods and test data. For creep deﬂections the models due to Findley proposed by the Structural Plastics Design Manual (ASCE, 1984) can be used to determine effective viscoelastic full-section moduli for use in predicting long-term deﬂections of pultruded structures. Protection against long-term degradation of pultruded proﬁles due to corrosive environments is typically determined by use of corrosion-resistance guides, which provide recommendations for use of pultruded materials having speciﬁc resins in a variety of chemical environments and temperatures. These guides are based on in-house coupon testing according to the standard practice in ASTM C 581 (see the list of standards in Chapter 3). Research studies to develop models to predict the long-term degradation of FRP composites in various service environments are ongoing but cannot yet be used for reliable lifetime prediction.

9

That is, they are deeper than metal proﬁles when they span the same length.

12.4

DESIGN BASIS FOR FRP PULTRUDED STRUCTURES

369

TABLE 12.2 Property Retention of Conventional Pultruded Proﬁles as a Function of Ambient Temperature Property Retained (%) Property

Temperature [⬚F (⬚C)]

Glass Polyester Pultruded Material

Glass Vinylester Pultruded Material

Strength

100 125 150 175 200

(37.8) (51.7) (65.6) (79.4) (93.3)

85 70 50 do not use do not use

90 80 80 75 50

Modulus

100 125 150 175 200

(37.8) (51.7) (65.6) (79.4) (93.3)

100 90 85 do not use do not use

100 95 90 88 85

Source: Strongwell, 2002.

12.4

DESIGN BASIS FOR FRP PULTRUDED STRUCTURES

In the two previous topics covered in this book—FRP rebars (Chapters 4 to 7) and FRP strengthening systems (Chapters 8 to 11)—the limit states design basis of the American Concrete Institute design guides, ACI 440.1R-06 and ACI 440.2R-02, were adopted. As such, a design basis did not need to be developed for the design of structures using FRP composites for these applications. In the case of design with FRP pultruded proﬁles, a consensus-based design basis on the same level as those developed by the ACI (or other code bodies related to FRP rebars and strengthening systems) does not yet exist. Design bases are provided in the Structural Plastics Design Manual (ASCE, 1984) and the Eurocomp Design Code and Handbook (Eurocomp, 1996), but these two documents do not have the model code–like status of the ACI (or other national model code–like) documents developed for FRP rebars and strengthening systems. It is a professional requirement for a structural engineer to declare the basis for design of a structure clearly and unambiguously. The basis for design is so well established for conventional materials that structural engineers routinely note in construction documents and plans the appropriate building codes used for the design. [For example, in the United States this includes building codes IBC (2003) or NFPA (2003) and the model design codes and speciﬁcations ASCE 7-02 (ASCE, 2002), ANSI/AISC 360-5 (AISC, 2005) and ACI 318-05 (ACI, 2005) for steel and concrete structures.10] For the case 10 Or applicable national building codes and speciﬁcations, depending on the location of the structure being built and the governing codes in that location.

370

DESIGN BASIS FOR FRP PROFILES

of design of structures with FRP proﬁles, this step in the design process is not routine, and the designer must take care to provide details of the design basis used and provide additional written special provisions in the construction documents to deﬁne aspects of the design basis that may be ambiguous in referenced documents. It is also important that the client (or owner) be aware of and accept the design basis proposed before developing the detailed design of an FRP structure. In what follows two different design bases are suggested for use in design of structures using FRP pultruded proﬁles: (1) allowable stress design (ASD) and (2) load and resistance factor design (LRFD). A performance-based design (PBD) basis is mentioned brieﬂy, but at this time a procedure for its use is not suggested for use with FRP proﬁles. Performance-based design is currently (2005) being developed for materials and structures in structural engineering and may have advantages in the future for structural design with FRP composites (Inokuma, 2002). 12.4.1

Allowable Stress Design

Allowable stress design (ASD) is based on the philosophy that the safety of a structure is obtained by ensuring that no structural member reaches its ultimate strength under nominal service loads. This is accomplished by ensuring that the design stress11 in every member, or the required stress, reqd, obtained from calculations using elastic theory and using the nominal service loads on the structure, be less than the ultimate strength, ult, of the material used in the structural member, divided by a factor of safety, SF. The ultimate strength divided by the safety factor is termed the allowable stress, allow, and the fundamental ASD equations are given as reqd ⱕ allow allow ⫽

ult SF

reqd ⫽ ƒ(loads, geometry, elastic analysis)

(12.3) (12.4) (12.5)

With respect to serviceability, ASD philosophy is to assign different factors (analogous to strength safety factors) to the material moduli to determine deﬂections and displacements under the nominal service loads. The nominal service loads used in design are obtained from building codes or model load codes (such as ASCE 7-02). Allowable stress design is recommended by most U.S. pultrusion companies in their design manuals. The safety factors recommended by U.S. pul is used symbolically to represent any design stress (e.g., shear stress, tensile stress, bearing stress).

11

12.4

DESIGN BASIS FOR FRP PULTRUDED STRUCTURES

371

trusion companies, and generally accepted by the structural engineering community in the United States at this time, are given in Table 12.3. These factors are applied to the material properties provided in manufacturers’ design guides and are intended for use with analytical equations provided in these design guides. Many of these are empirical design equations that differ from manufacturer to manufacturer. Material properties for use in design (ultimate strengths and moduli) that are obtained using designated tests (either ASTM standard test methods or in-house test methods) are provided in the design guides for a variety of pultruded materials (according to different resin systems) and proﬁles (according to shape). Allowable stress design is also recommended by AASHTO (2001) for designing FRP luminaire and sign support structures. The analytical equations provided in the AASHTO speciﬁcations are based on theoretical and empirical equations for orthotropic plates, beams, and columns of linear elastic materials made of glass-reinforced polyester (the only ﬁber and resin types permitted) and apply to members manufactured by pultrusion, centrifugal casting, or ﬁlament winding. The AASHTO speciﬁcation recommends the minimum safety factors shown in Table 12.4 that are to be used with material properties obtained from speciﬁed ASTM tests (stipulated in AASHTO, 2001). Designs are based on loads provided in the AASHTO (2001) speciﬁcation, according to which, when the analytical allowable stress design method is used, ‘‘design calculations provided shall be veriﬁed by documented test results on similar structures’’ (AASHTO, 2001, p. 8-5). As an alternative to the analytical design approach based on the allowable stress design basis, fullscale testing according to ASTM 4923 (Standard Speciﬁcation for Reinforced Plastic Thermosetting Poles) can be used in a performance-based design philosophy to design an FRP luminaire. Allowable stress design is also commonly used by structural designers in conjunction with design equations based on theoretical equations for orthoTABLE 12.3 Safety Factors for Allowable Stress Design Provided by Pultrusion Manufacturers Strength or Modulus

Typical Member

Design Objective

Safety Factor

Flexural strength Flexural modulus Shear strength Shear modulus Compressive strength Compression modulus Tensile strength Tensile modulus Bearing strength Bearing modulus

Beam Beam Beam Beam Column or truss member Column or truss member Tie or truss member Tie or truss member Joint or connection Joint or connection

Strength Serviceability Strength Serviceability Strength Serviceability Strength Serviceability Strength Serviceability

2.5 1.0 3.0 1.0 3.0 1.0 not provided not provided 4.0a not applicable

a The SF for connections should be applied to all stresses in a connection; however, this assumes that connections in pultruded structures will be dimensioned to fail in bearing (see Chapter 15).

372

DESIGN BASIS FOR FRP PROFILES

TABLE 12.4

Safety Factors for Allowable Stress Design

Strength or Modulus

Typical Member

Flexural strength Flexural modulus Shear strength Shear modulus Compressive strength Compression modulus Tensile strength Tensile modulus Bearing strength Bearing modulus

Beam Beam Beam Beam Column or truss member Column or truss member Tie or truss member Tie or truss member Joint or connection Joint or connection

Design Objective Safety Factor a Strength Serviceability Strength Serviceability Strength Serviceability Strength Serviceability Strength Serviceability

2.5 not provided 3.0 not provided 3.0 not provided 2.0 not provided not provided not applicable

Source: AASHTO (2001). a The SF for connections should be applied to all stresses in a connection; however, most connections in pultruded structures are dimensioned to fail in bearing (see Chapter 15).

tropic plates, beams, and columns provided in the Structural Plastics Design Manual (ASCE, 1984) or the Eurocomp Design Code and Handbook (Eurocomp, 1996). Material properties are often obtained from independent testing using standard ASTM tests or are taken from manufacturers’ speciﬁcations. Safety factors recommended by pultrusion companies or by AASHTO (2001) are generally used in this approach. Designs are based on nominal service loads taken from building codes or model load codes (e.g., ASCE 7-02). The allowable stress design basis is not considered to provide a known degree of structural reliability. That is, even with a known safety factor, it is not known with a quantiﬁable degree of conﬁdence what the probability is that the structure will be able to carry the design loads in the various limit states. This is due to the fact that (1) the safety factors that are used in the ASD basis have been developed by pultrusion manufacturers from simple tests on pultruded members and accepted conventions for safety factors in civil engineering structures that range from 2 to 3; (2) the material property data provided by manufacturers that are used in the ASD basis are provided without statistical data (mean, variation, number of tests, etc.) and therefore the variability in the properties and the conﬁdence limits on the values cannot be established in a quantiﬁable manner; and (3) the stresses determined in developing the safety factors from test data depend on the complexity (or naivety) of the analytical and empirical equations used in their determination. However, although no statistical data are provided for the pultruded material properties given in manufacturers’ design guides, it is well known that the values provided are conservative and represent the lower ranges of the properties measured. In addition, the ASD basis is generally used with loads obtained from probabilistically based load codes such as ASCE 7 (even though probabilistically based load factors are not used). This implies that there is some statistically and probabilistically based element to the way in

12.4

DESIGN BASIS FOR FRP PULTRUDED STRUCTURES

373

which the ASD basis is used today. Nevertheless, since the material data and the safety factors are not statistically and probabilistically derived to yield a deﬁned structural reliability, the ASD basis is regarded as providing an ad hoc level of safety and is not regarded as a modern scientiﬁc design basis (Ellingwood, 2003). However, as discussed in Section 12.4.2, a probabilitybased design basis for FRP pultruded structures is not yet fully developed, and therefore the ASD basis is still used in the design of the vast majority of pultruded structures in the United States. In what follows a version of the ASD basis is presented as a basis for the design of FRP structures. The elements of the ASD basis used in this book are: 1. Analytical equations presented in the Structural Plastics Design Manual (ASCE, 1984) and the Eurocomp Design Code and Handbook (Eurocomp, 1996) and supplemented with equations from the technical literature (detailed in what follows) 2. Design properties of pultruded materials taken from manufacturers’ design guides 3. Safety factors taken from AASHTO (2001) 4. Nominal service loads and service load combinations taken from ASCE 7-02 12.4.2

Load and Resistance Factor Design

The load and resistance factor design (LRFD) basis used in the United States and the closely related limit states design (LSD) basis used in Europe have at their heart the fundamental philosophy that the level of safety or serviceability provided by a design must produce a quantiﬁable level of structural reliability. In the LRFD basis, (1) the nominal loads, P, are factored by probabilistically derived load factors, ␥, which depend on load type (dead load, live load, etc.) and load combinations, and (2) the material or structural nominal resistances (e.g., the material strengths or member load-carrying capacities), Rn, are factored by resistance factors, , that depend on the material variability, the type of failure mode predicted (brittle or ductile), and the type of resistance required (e.g., shear, ﬂexural). The required member resistance, Rreqd, is determined using elastic or inelastic analytical methods as a function of the factored loads. This is represented in a general form as Rreqd ⱕ Rn

(12.6)

Rreqd ⫽ ƒ(␥iPi)

(12.7)

A reliability index, , is used to quantify the structural reliability in probability-based design (Nowak and Collins, 2000). For conventional struc-

374

DESIGN BASIS FOR FRP PROFILES

tural materials such as steel and concrete, reliability indices between  ⫽ 2.0 and 4.0 are common (Ellingwood, 2003). A reliability index of  ⫽ 2.5 corresponds to a probability of failure of Pƒ ⫽ 0.005. When ASCE 7 load factors are used, target reliability indices of  ⫽ 2.5 to 4.5 are generally accepted for structural engineering design with conventional materials (Ellingwood, 2003; Szerszen and Nowak, 2003). For members (beams, columns, etc.) where analytical methods are well established to predict deformation and failure, the lower values of  in the range noted above are generally accepted, whereas for connections and joints, where analytical methods to predict deformation and failure are less developed, higher values of  are generally accepted. For materials that fail in a brittle fashion and whose long-term behavior is not well known, higher values of  are also used. For this reason target reliability indexes for FRP pultruded structures are expected to be in the  range 3.0 to 4.5 until more data become available. The reliability index is not used explicitly by structural engineers to design a structure. It is used by code-writing bodies and researchers to determine the appropriate resistance factors, , for use in the LRFD procedure. Structural engineers then use the probability-based LRFD procedure in a conventional deterministic manner. In the LRFD basis (as in the ASD basis), two primary limit states are considered in design: the ultimate limit state and the serviceability limit state. The ultimate limit state is associated with life safety and is controlled by collapse, instability, and failure of the structure or structural members. The serviceability limit state is associated with short- and long-term serviceability of the structure and is controlled by deﬂection, vibration, and degradation of the materials, the members, and the connections in the structure (Eurocomp, 1996). A probability-based LRFD speciﬁcation or design procedure for FRP pultruded structures does not exist at this time. However, use of the LRFD approach for the design of pultruded FRP structures is quite possible, and a prestandard outline has been prepared by ASCE (Chambers, 1997). Fundamental issues associated with developing an LRFD design procedure for pultruded FRP structural proﬁles, with measurable reliability indexes, are discussed in Ellingwood (2003). The difﬁculties associated with developing an LRFD basis for FRP pultruded structures are associated primarily with the determination of the statistical material design properties for common pultruded proﬁles and the appropriate analytical models to use for predicting the member resistances. Since a standard material speciﬁcation is not followed by pultrusion manufacturers at this time, the statistical properties of pultruded materials are not available. In the future it is anticipated that manufacturers will follow a standard material speciﬁcation such as European Standard EN 13706 (2002) or will develop one based on proposed model speciﬁcations such as that of Bank et al. (2003). An LRFD procedure for the design of doubly symmetric and singly symmetric pultruded columns that accounts for global ﬂexural buckling, global torsional buckling, ﬂexural–torsional buckling, and material compression has

12.4

375

DESIGN BASIS FOR FRP PULTRUDED STRUCTURES

been presented by Zureick and Scott (1997), Zureick (1998), and Zureick and Steffen (2000). In these studies, resistance factors were determined based on detailed tests of glass–vinylester pultruded materials (from a single manufacturer) and on full-scale buckling experiments conducted on pultruded columns having wide-ﬂange, square-tube (box), and equal-leg-angle proﬁles. Analytical equations based on orthotropic plate theory were used to predict the buckling loads. The resistance factors to be used with ASCE 7 load factors, determined in these studies, are given in Table 12.5. Unfortunately, these resistance factors are only applicable to the types of proﬁles and pultruded materials tested in these studies. For doubly symmetric proﬁles, Zureick and Scott (1997) did not conduct a rigorous reliability analysis, and the resistance factors were obtained from lower bounds of comparisons between experimental data and theoretical predictions. Reliability indices are therefore not provided for these resistance factors. For the singly symmetric angles, Zureick and Steffen (2000) chose target reliability indices of  ⫽ 3, 3, and 4 for the ﬂexural buckling, ﬂexural– torsional buckling, and material compressive failure limit states. Design property values for the pultruded materials in this study were based on the 95% lower conﬁdence limit on the 5th percentile of the test data. A three-parameter Weibull distribution was used to characterize the test data statistically. Based on further work Zureick and co-workers (Alqam et al., 2002) have recommended a two-parameter Weibull distribution to characterize pultruded materials statistically. European Limits States Design Basis In the LSD basis used predominantly in Europe, instead of using resistance factors to account for the variability in the material, safety factors or material partial factors (coefﬁcients) are used (Hollaway and Head, 2001). The characteristic material property value,12 Xk, TABLE 12.5 LRFD Resistance Factors for Glass–Vinylester Pultruded Columns Proﬁle WF or tube

Single-angle

12

Failure Mode Flexural (Euler) buckling Axial shortening Flexural (Euler) buckling Flexural–torsional buckling Material compression

Resistance Factor,

Reliability Index, 

Ultimate

0.85

not available

Serviceability

0.80

not available

Ultimate

0.65

3.0

Ultimate

0.85

4.0

Ultimate

0.50

4.0

Limit State

Typically deﬁned as the 5th percentile of the test data.

376

DESIGN BASIS FOR FRP PROFILES

is divided by the material partial coefﬁcient as opposed to being multiplied by the resistance factor in the LRFD approach in the following general form: Rreqd ⱕ Rd

(12.8)

冉 冊

Rd ⫽ ƒ

Xk ,a ␥m 0

(12.9)

where Rd is the design resistance and a0 is the effect on resistance of geometric variation of the section. The LSD safety factor approach is somewhat different from the LRFD approach in that the resistance factor in the LRFD approach is selected based on the member type (ﬂexural, compression, shear) and failure mode, whereas in the LSD method the safety factors are selected primarily based on material properties. However, analytical factors similar to the geometric factors can be introduced to account for failure modes. The development of limit states design procedures for FRP structures for structural applications was initiated in Europe by Head and Templeman (1986). As noted previously, the Structural Plastic Design Manual, developed in the United States in the late 1970s, also follows a limit states design procedure, but explicit factors for design use are not provided in this document (ASCE, 1984). A difﬁculty exists with the use of the LSD basis for FRP pultruded structures similar to that with the LRFD basis (Hollaway and Head, 2001): that is, determination of the material partial factors with known probability so that a structural reliability analysis can be conducted. In Europe, the load factors and load combinations are those prescribed by Eurocode 1 (CEN, 2002b). An approach to obtaining the material partial factors for member design13 is provided in the Eurocomp Design Code and Handbook (Eurocomp, 1996), following the Eurocode approach, in which the material partial factor, ␥m, is obtained as the product of coefﬁcients that are intended to account for separate and quantiﬁable inﬂuences on the material properties as follows: ␥m ⫽ ␥m,1␥m,2␥m,3

(12.10)

where, ␥m,1 accounts for the method in which the material property data were obtained, ␥m,2 accounts for the material manufacturing process,14 and ␥m,3 accounts for the effects of environment and the duration of loading on the material properties. According to the Eurocomp design code, the material

13 For connection and joint design a similar approach is followed, however, additional safety factors are used to account for local connection effects and for the method of analysis used (Eurocomp, 1996, Sec. 5). 14 The Eurocomp design code permits any manufacturing process and is not applicable only to pultruded proﬁles.

12.4

DESIGN BASIS FOR FRP PULTRUDED STRUCTURES

377

partial factor may not be less than 1.5 for ultimate limit states (nor need be greater than 10) and not less than 1.3 for serviceability limit states. However, in the opinion of many designers, the 1.3 material partial factor for the serviceability limit state is regarded as too conservative if the material characteristic properties (see Table 12.7) are obtained from manufacturer-published data. A material partial factor of 1.0 for the serviceability limit state is recommended if manufacturer material data are used in design. Table 12.6 lists key values of the material partial factors for the ultimate limit state (ULS) for commercially produced pultruded materials, as listed in the Eurocomp Design Code and Handbook.15 According to the Eurocomp design code, the material manufacturer is required to provide proof that the material is fully cured in order for the designer to use the fully cured partial safety coefﬁcients. Although the Eurocomp design code is written from an LSD or LRFD basis, detailed data are not provided as to how the material partial safety coefﬁcients were determined, and therefore the structural reliability of a structure designed with these coefﬁcients cannot be ascertained with certainty at this time (Hollaway and Head, 2001). However, the Eurocomp design code does provide tables of characteristic values for pultruded materials as a function of the ﬁber volume fraction and ratio of the longitudinal ﬁber to a continuous strand mat. The characteristic properties that are stated have been determined from the mean of test data minus 1.64 standard deviations; however, the number of tests and a detailed description of the materials are not provided to verify this claim. Characteristic property data for three typical types of glass–FRP pultruded materials speciﬁed by the Eurocomp design code are listed in Table 12.7. The data provided for pultruded material 2 are very similar to those presented TABLE 12.6

ULS Material Partial Factors

Source of Factor Properties of the pultruded plate are derived from test Properties of the pultruded plate are derived from laminate theory Fully cured pultruded material Non-fully cured pultruded material Short-term loading for 25 ⬍ T ⬍ 50⬚C and Tg a ⬎ 90⬚C Short-term loading for 0 ⬍ T ⬍ 25⬚C and Tg ⬎ 80⬚C Long-term loading for 25 ⬍ T ⬍ 50⬚C and Tg ⬎ 90⬚C Long-term loading for 0 ⬍ T ⬍ 25⬚C and Tg ⬎ 80⬚C

Material Partial Factor ␥m,1 ␥m,1 ␥m,2 ␥m,2 ␥m,3 ␥m,3 ␥m,3 ␥m,3

⫽ ⫽ ⫽ ⫽ ⫽ ⫽ ⫽ ⫽

1.15 1.5 1.1 1.7 1.0 1.0 2.5 2.5

Source: Eurocomp Design Code and Handbook (1996). a Tg is the glass transition temperature of the FRP pultruded material. For commercially manufactured, fully cured pultruded proﬁles, it should not be less than 80⬚C.

15

Consult the Eurocomp design code for a full list of safety factors.

378 30.0 7.0 30.0 14.9 4.5 not provided 30.0 10.0 not provided not provided

39.2 not provided 2.2 not provided 58.0 16.7 not provided not provided

38% Roving and CFM (ratio 1⬊1) Polyester Conventional structural pultruded proﬁle (I, WF, L, 䡺, [)

Pultruded Material 2

59.5 6.4

Polyester, vinylester Special nonstructural pultruded proﬁle (e.g., grating I-bar, ladder rail)

Resin system Typical part

Strength properties (⫻103 psi) Tensile Longitudinal Transverse Compressive Longitudinal Transverse Shear In-plane Out-of-plane Flexural Longitudinal Transverse Bearing Longitudinal Transverse

48% Roving and CFM (ratio 4⬊1)

Pultruded Material 1

Characteristic Properties of Pultruded Materials for Design (Eurocomp)

Fiber volume (typical) Fiber architecture

TABLE 12.7

not provided not provided

100.1 not provided

5.5 not provided

60.0 not provided

100.1 not provided

Polyester Round solid pultruded rod

65% Roving only

Pultruded Material 3

379

Stiffness properties (⫻106 psi) Tensile Longitudinal Transverse Compressive Longitudinal Transverse Shear, in-plane Flexural Longitudinal Transverse Poisson Ratio Longitudinal Transverse 2.5 0.8 2.5 1.0 0.4 2.0 0.8 0.33 0.11

3.9 0.5 3.5 0.7 0.6 2.0 1.2 0.2 0.1

not provided not provided

5.9 not provided

not provided not provided not provided

5.9 not provided

380

DESIGN BASIS FOR FRP PROFILES

historically in U.S. manufacturers’ design manuals for conventional glass– FRP pultruded shapes and (e.g., Strongwell, 2002) and would appear to have ‘‘embedded’’ knock-down factors included. It is unlikely that they are truly characteristic values for conventional pultruded materials obtained (as can be seen by comparison with test data in Zureick and Scott, 1997, for example). In what follows a version of the LRFD basis is presented as an acceptable design basis for FRP structures. The elements of the LRFD basis used in this book are: 1. Analytical equations presented in the Structural Plastics Design Manual (ASCE, 1984) and Eurocomp Design Code and Handbook (Eurocomp, 1996), supplemented with equations from the technical literature 2. Characteristic design properties of pultruded materials taken from European Standard EN 13706 (CEN, 2002a) or from U.S. manufacturers’ design guides 3. Resistance factors taken as the inverse of the material partial factors given in the Eurocomp Design Code and Handbook (Eurocomp, 1996) 4. Nominal loads, load factors, and factored load combinations taken from ASCE 7-02 However, it must be noted that the LRFD basis as described above and presented in what follows in the design examples does not have a fundamental probability-based foundation and does not yield known reliability indices. Nevertheless, based on comparisons with the ASD procedure, it is expected that this approach will yield reliability indexes in the range  ⫽ 2.5 to 3.0 (Ellingwood, 2003).

12.5

PERFORMANCE-BASED DESIGN

The structural design of an FRP pultruded structure or a portion of the structure can be based on a performance speciﬁcation (ICC, 2003). In this approach, the entire structure or a portion of the structure is required to meet speciﬁc structural performance objectives, which are evaluated in a predetermined manner according to predetermined performance criteria. The performance objectives are typically applied to both local and global deformations and capacities. Full-scale testing of the structure or a portion of the structure is usually required to meet the performance speciﬁcation. Both proof testing of the actual structure and failure testing of a full-sized mock-up of the structure (or parts thereof) may be used. A factor of safety or a structural reliability index must be deﬁned and agreed upon by designer and client as part of the performance speciﬁcation. The performance speciﬁcation is usually appended to the construction documents and plans and is part of the construction contract. Performance speciﬁcations are typically developed on a case-by-case

PROBLEMS

381

basis. They are not uncommon in the FRP industry. In highway construction documents in the United States, they are often appended to the construction documents as ‘‘special provisions.’’ In some situations, a combined prescriptive and performance approach is used. A prescriptive set of material speciﬁcations is mandated along with a number of structural-level performance speciﬁcations. The material speciﬁcation may stipulate the manufacturing method, the limiting mechanical and physical properties of the materials produced, and the requirements for quality assurance testing. PROBLEMS 12.1 Visit the following pultrusion manufacturers’ Web sites16 and request or download copies of their most recent pultrusion design guides and their pultruded proﬁle geometry and property speciﬁcations (typically, included in the design guides). These will be needed for solving design problems in the chapters to follow. Strongwell: www.strongwell.com Creative Pultrusions: www.pultrude.com Bedford Reinforced Plastics: www.bedfordplastics.com Fiberline: www.ﬁberline.com TopGlass: www.topglass.it 12.2 From U.S. manufacturers’ speciﬁcation sheets (Strongwell, Creative Pultrusions, and Bedford Reinforced Plastics), extract and list the manufacturer-reported geometric and mechanical properties (in-plane stiffness and strength properties for the web and the ﬂange) for the following pultruded sections17 commonly used in truss and light-frame pultruded structures: Glass–polyester 3 ⫻ –14 (b ⫻ t) in. square tube Glass–polyester 2 ⫻ –14 (b ⫻ t) in. square tube Glass–polyester 6 ⫻ –14 ⫻ 1–58 ⫻ –14 (d ⫻ tw ⫻ bƒ ⫻ tƒ) in. channel Glass–polyester 3 ⫻ –14 (b ⫻ t) in. equal leg angle 12.3 From U.S. manufacturers’ speciﬁcation sheets (Strongwell, Creative Pultrusions, and Bedford Reinforced Plastics) extract and list the manufacturers’ reported geometric and mechanical properties (in-plane stiffness and strength properties for the web and the ﬂange) for the 16 No endorsement of the manufacturers listed is implied. The reader is free to choose any manufacturer’s products to use in the examples that follow, and is encouraged to collect similar data for locally available FRP pultruded shapes. 17 Not all manufacturers may produce all shapes listed in Problems 12.2 to 12.4.

382

DESIGN BASIS FOR FRP PROFILES

following pultruded sections commonly used in heavy-frame pultruded structures: Glass–polyester 8 ⫻ 8 ⫻ –38 (d ⫻ b ⫻ t) in. wide-ﬂange I-shaped section Glass–polyester 10 ⫻ 5 ⫻ –12 (d ⫻ b ⫻ t) in. narrow-ﬂange I-shaped section Glass–vinylester 6 ⫻ 6 ⫻ –14 (d ⫻ b ⫻ t) in. wide-ﬂange I-shaped section Glass–vinylester 6 ⫻ –38 (b ⫻ t) in. square tube Glass–vinylester 6 ⫻ –12 (b ⫻ t) in. equal leg angle Glass–polyester 10 ⫻ –12 ⫻ 2–34 ⫻ –12 (d ⫻ tw ⫻ bƒ ⫻ tƒ) in. channel 12.4 From European manufacturers’ speciﬁcation sheets (Fiberline or TopGlass), extract and list the manufacturer-reported geometric and mechanical properties (in-plane stiffness and strength properties for the web and the ﬂange) for the following pultruded sections18 commonly used in heavy-frame pultruded structures. Provide your answers in both metric and U.S. units to allow for comparison with properties of U.S.produced proﬁles. Glass–vinylester/polyester19 240 ⫻ 120 ⫻ 12 (d ⫻ b ⫻ t) mm narrowﬂange I-shaped section Glass–vinylester/polyester 300 ⫻ 8 ⫻ 150 ⫻ 12 (d ⫻ tw ⫻ bƒ ⫻ tƒ) mm narrow-ﬂange I-shaped section Glass–vinylester/polyester 200 ⫻ 10 (b ⫻ t) mm square tube Glass–vinylester/polyester 150 ⫻ 8 (b ⫻ t) inch equal leg angle Glass–vinylester/polyester 240 ⫻ 7 ⫻ 72 ⫻ 10 (d ⫻ tw ⫻ bƒ ⫻ tƒ) mm channel 12.5 Contact pultrusion companies or local distributors of pultruded proﬁles and obtain current pricing (per unit length, ft or m) of the pultruded beams listed in Problems 12.2 to 12.4. 12.6 Read and write a one-page report on the following technical papers that discuss design bases for pultruded structures: Head, P., and Templeman, R. B. (1986), The application of limit states design principles to ﬁbre reinforced plastics, Proceedings of the British Plastics Federation Congress ’86, Nottingham, England, September 17–19, pp. 69–77. Chambers, R. E. (1997), ASCE design standard for pultruded ﬁber-reinforced plastic (FRP) structures, Journal of Composites for Construction, Vol. 1, pp. 26–38.

18

If the exact size is not manufactured by the manufacturer, choose one close to the size listed. European manufacturers generally do not provide different properties for polyester and vinylester proﬁles. 19

SUGGESTED ACTIVITY

383

Ellingwood, B. R. (2003), Toward load and resistance factor design for ﬁber-reinforced polymer composite structures, Journal of Structural Engineering, Vol. 129, pp. 449– 458.

SUGGESTED ACTIVITY 12.1 Contact a pultrusion manufacturer20 and ask them to send you some samples of pultruded proﬁles (1-ft-long lengths of an I-shape and a tube are good). The simple qualitative experiments listed below will enable you to understand more about the properties of the material and its workability. Write short (e.g., two-page) reports on the materials, methods, and results of your examinations. Consider the following: (a) Weigh and measure the sample and determine the mass density of the pultruded material. Compare measured densities to the manufacturers’ reported densities. (b) Mark and drill holes of –14 - and 1-in. diameter in the pultruded material. Experiment with various ways of marking the material (pencil, pen, scoring, etc.) and various drill bits (solid, hole, etc.) (c) If possible, cut a coupon 1 in. wide ⫻ 3 in. long from the material in both the longitudinal and transverse directions. Use a masonry blade or diamond-tipped blade and a power saw (table, circular, or radial arm saw) or a hand hacksaw or box saw (cross-cut saw). (d) Expose the coupon to a constant ﬂame in a Bunsen burner (in a fully ventilated hood with an exterior exhaust system). Observe what happens. Examine the residue and record your observations. (e) Sand and polish (to 200 grit, if possible) the cut ends of the coupon and examine the cut ends in the longitudinal and transverse directions under an optical microscope. Try to distinguish between roving and mat layers. Look for voids in the material.

20 It is preferable for the instructor to contact the manufacturer on behalf of the class early in the semester to ensure that the materials are available when needed.

13 13.1

Pultruded Flexural Members

OVERVIEW

In this chapter, design procedures are presented for ﬂexural members made of pultruded FRP proﬁles. Axially loaded members in tension and compression or combined axial and ﬂexural members are discussed in Chapter 14. Connections and joints for pultruded proﬁles are discussed in Chapter 15. Theoretical mechanics-based equations are presented here for analyzing strength, stability, and deformation limit states of ﬂexurally loaded pultruded structural members. Design procedures for the allowable stress design (ASD) and the load and resistance factor design (LRFD) bases described in Chapter 12 are presented. Since pultruded proﬁles behave essentially as linear elastic (or linear viscoelastic) structural members, the analytical equations developed for predicting stresses and deformations in these members for the ultimate and the serviceability limit states are valid for either of the design bases selected. Therefore, it is only the safety factors for ASD or the load and resistance factors for the LRFD that differentiate the design procedures for the two design bases. 13.2

INTRODUCTION

The design of pultruded proﬁles that are symmetric with respect to the plane of loading and consist of horizontal plates (ﬂanges) and vertical plates (webs) is discussed in this section. This includes conventionally manufactured Ishaped,1 square tube, rectangular tube, round tube, and multicelled tubular proﬁles. It also includes unsymmetric or singly symmetric sections, such as equal or unequal leg angles, or channel sections, or built-up sections, if they are loaded in their plane of symmetry through the shear center or are used back to back to create a symmetric composite proﬁle. Typical member cross sections and orientations for loading in the vertical plane (i.e., the plane of the web) are shown in Fig. 13.1. In vertical braced frame or horizontal unbraced grid structures, wide-ﬂange and tubular sections are most frequently used as beams and girders since they are readily connected using clip angles or gusset plates and traditional me-

1

The term I-shaped proﬁles is used to describe both narrow- and wide-ﬂange I-shaped proﬁles.

384

Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

13.3

STRESSES IN FLEXURAL MEMBERS

385

Figure 13.1 Cross sections and orientations of typical ﬂexural members.

chanical connectors, such as nuts and bolts (e.g., see Figs. 1.15 and 1.18). In vertical braced frames the beams may need to be designed as combined load members (beam-columns or tension-bending members), which are discussed in Chapter 14. The choice of proﬁle used as a beam often depends on the connection detailing required, as discussed further in Chapter 15. In trusses or stick-built frames, back-to-back angles and small channels, as well as small square tubular elements, are most commonly used (see e.g., Figs. 1.17 and 1.19) as the primary structural elements. In this case, the elements are usually treated as continuous beams (such as chords, girts, purlins, or rafters) or as axially loaded members (such as columns, struts, or ties) or combined load members (beam-columns or tension-bending members). Axially loaded and combined load members are discussed in Chapter 14.

13.3

STRESSES IN FLEXURAL MEMBERS

The ﬂexural member discussed in this chapter is designed to resist stress resultants (or internal forces) in the global x,y,z coordinate system that are caused by the applied transverse distributed loads, w(z), or concentrated loads, P, in the y–z plane, as shown in Fig. 13.2. These stress resultants are the

P w(z)

y x

Mx

Vy

z

Figure 13.2 Transversely loaded beam.

Vy

Mx

386

PULTRUDED FLEXURAL MEMBERS

bending moment, Mx, and the transverse shear force, Vy. According to onedimensional beam theory for beams of homogeneous material,2 the bending moment, Mx, causes the member to develop a linearly varying axial (ﬂexural) stress, x, through the depth of the cross section and along its length that is given by the ﬂexural stress equation My z ⫽ ⫺ x Ix

(13.1)

where Ix is the second moment of area of the cross section about the x-axis and y is the vertical distance from the neutral axis. For the (positive) moment shown in Fig. 13.2, a compressive (negative) stress is obtained in the top part of the cross section above the neutral axis, and a tensile (positive) stress is obtained in the bottom part of the cross section below the neutral axis. For a beam with nonhomogeneous properties through the depth of the cross section, such as a pultruded proﬁle with different longitudinal elastic moduli in its webs and ﬂanges, as may be the case in some pultruded proﬁles, the relationship between the bending moment and the axial (ﬂexural) stress is not closed formed but is written in general form as

冕 y dA

Mx ⫽ ⫺

A

z

(13.2)

where the integral is taken over the cross-sectional area of the beam. Since the pultruded material is assumed to be linear elastic in this one-dimensional beam theory, the strain through the depth of the ﬂexural member, z, varies linearly, and the stress at any height of the section, z, can be found directly using the longitudinal modulus, EL, at the position of interest. Beams of this type have traditionally been known as composite beams since they are composed of different materials3 and are treated extensively in many texts (e.g., Gere and Timoshenko, 1997). Stress analysis of beams of this type is commonly performed using the transformed section method or the composite mechanics method. These methods were used extensively in previous chapters dealing with FRP-reinforced and FRP-strengthened concrete ﬂexural members (Chapters 5 and 9). The shear force resultant, Vy, causes a homogeneous material beam to develop a nonuniformly varying transverse shear stress,4 , along its length 2 This implies that the longitudinal stiffness does not vary through the depth in the cross section. This assumption will be revisited when pultruded proﬁles having differing properties in their webs and ﬂanges are discussed. 3 Although the historically used term composite used to describe these beams may cause some initial confusion, it is actually perfectly appropriate for the FRP beams being considered. 4 No subscript is used for the shear stress in one-dimensional thin-walled beam theory, since it is used to represent either yz (in the web) or xz (in the ﬂange).

13.3

STRESSES IN FLEXURAL MEMBERS

387

and throughout its cross section that is given by the familiar thin-walled section shear stress equation as ⫽

VyQx Ix t

(13.3)

where Qx is the ﬁrst moment of area of the cross section calculated at the point of interest, Ix the second moment of area of the cross section, and t the thickness wall (perpendicular to the contour) at the point of interest. In a nonhomogeneous beam, the properties Qx and Ix of the transformed section must be used in equation (13.3). Equation (13.3) can only be used to determine the in-plane shear stress in the direction of the shear ﬂow in the thinwalled section. It cannot be used to determine the interlaminar shear stress through the thickness of the ﬂange. Since the shear stress causes shear distortion (as opposed to extension or contraction in the case of the normal stress due to the bending moment) in the individual orthotropic plates (or walls) of the thin-walled section, the sign of the shear stress is not signiﬁcant.5 Therefore, the stress given by equation (13.3) is always taken as positive regardless of the sign of Vy. In addition to the stresses described above, which are developed as a result of the global bending moment and transverse shear force and are obtained using one-dimensional beam theory, additional local stresses at points of concentrated loads must be accounted for in the design of pultruded members. These local, primarily bearing-type stresses are not obtained from beam theory but are obtained using commonly employed engineering approximations for the ‘‘length of bearing’’ similar to those used for steel proﬁles. Due to concentrated loads along the beam and reactions at the supports, the proﬁle is assumed to develop a uniform compressive bearing stress in the vertical plates (web or webs) of the section at the points of load application or at the support given by y ⫽

F Aeff

(13.4)

where F is the transverse force and Aeff is the effective area over which the force is applied. For a web with outstanding ﬂanges on both sides (e.g., an I-shaped proﬁle) the effective area is given as

5 It should be noted that the strength of a highly orthotropic unidirectional laminate can depend on the sign of the shear stress when certain multiaxial failure criteria are used to predict failure (Agarwal and Broutman, 1990, p. 181). However, no distinction is made between positive and negative shear stress for the purpose of design of pultruded proﬁles where only uniaxial failure criteria are used in design.

388

PULTRUDED FLEXURAL MEMBERS

Aeff ⫽ (tw ⫹ 2tƒ ⫹ 2tbp)Leff

(13.5)

For a web with an outstanding ﬂange on one side only (e.g., a corner of a square tube proﬁle) the effective area is given as Aeff ⫽ (tw ⫹ tƒ ⫹ tbp)Leff

(13.6)

where Leff is the effective bearing length along the beam in the z-direction (taken as the width of the support or the length over which the concentrated load is applied) and tw, tƒ, and tbp are the web thickness, the ﬂange thickness, and the thickness of a bearing plate under the ﬂange (if applicable), respectively, as shown in Fig. 13.3. For a section with multiple webs, the contributions to the effective area from the webs having two outstanding ﬂanges and a single outstanding ﬂange are added as appropriate. For example, for a single-cell tube section (also known as a box section) having two webs, each with one outstanding ﬂange, the effective area is given as twice the area obtained from equation (13.6) (assuming that both webs have a thickness of tw). The stresses (or force resultants) calculated must be less than the material strengths and critical buckling stresses (or the critical resistances or buckling capacities) according to the design basis selected. 13.4

DEFORMATIONS IN FLEXURAL MEMBERS

Due to the stress resultants, Mx and Vy, the member will deﬂect in its plane of loading. The elastic curve that describes the deﬂected shape of the beam is a function of the ﬂexural rigidity, EI, and the transverse shear rigidity, KAG, of the member. The deﬂection can be obtained using Timoshenko beam theory (also known as shear deformation beam theory) (Timoshenko, 1921). In Timoshenko beam theory, the elastic curve is deﬁned by two independent var-

tw

tw tf tbp tw+ tf + tbp

tw+ tf + tbp

Figure 13.3 Effective bearing width for beam webs (shown as a thick dark line).

13.4

DEFORMATIONS IN FLEXURAL MEMBERS

389

iables, the transverse deﬂection, ␦(z), due to bending and shearing, and the slope of the elastic curve, (z), due to bending only.6 They are obtained by simultaneous solution of the differential equations d Mx ⫽ dz EI

(13.7)

Vy dy ⫺⫽⫺ dz KAG

(13.8)

and boundary conditions for the deﬂection and bending slope at ﬁxed, pinned, and free ends as in Euler–Bernoulli beam theory. The solution to equations (13.7) and (13.8) with appropriate boundary conditions leads to the general expression for the total beam deﬂection as a sum of the deﬂection due to bending deformation and the deﬂection due to shear deformation: y(z) ⫽ yb(z) ⫹ ys(z) ⫽

ƒ1(z) ƒ2(z) ⫹ EI KAG

(13.9)

where ƒ1(z) and ƒ2(z) are functions that depend on loading and boundary conditions. For determinate beams with common loads and support conditions, the functions are given in Table 13.1. It can be seen that the deﬂection function, ƒ1(z), that represents the bending contribution to the deﬂection is the same as that obtained by traditional Euler–Bernoulli beam theory. In addition, it is important to recognize that for statically indeterminate beams (and frames) the member internal forces, Mx and Vy (and Nz in frames), will also be a function of the shear rigidity of the beam and will not be the same as those for the same indeterminate beam when Euler–Bernoulli beam theory is used.7 For determinate beams the internal forces are not functions of the deﬂections; therefore, the internal forces will be the same regardless of the beam theory used. For the serviceability limit state, the calculated maximum deﬂections must be less than the building code–stipulated deﬂections. The Structural Plastics Design Manual (ASCE, 1984) gives typical deﬂection limits as L/180 for visual appearance to L/400 for vibration sensitivity. The Eurocomp Design Code and Handbook (Eurocomp, 1996) recommends limiting instantaneous deﬂections to L/300 and long-term deﬂection to L/250 for frame structures. In Timoshenko beam theory the bending slope, (z), is an independent variable and is not equal to dy / dz as in Euler–Bernoulli beam theory. In Timoshenko beam theory the total slope is the sum of the bending slope and the shear slope (i.e., dy / dz ⫽ ⫹ ␥). 7 Indeterminate beams can by solved by hand using Timoshenko beam theory and the force method. In computerized analysis of building frames, a shear-deformable beam element should always be used for frames of pultruded members. These elements are available in most commercial structural analysis codes. 6

390

a

Loads are deﬁned as positive as shown in Fig. 13.2.

Concentrated load (P) at tip

⫺P(z)

w (ᐉz ⫺ z2) 2 P ⫺ (z) 2 w ⫺ (2ᐉz ⫺ z2) 2 ⫺

w 4 (z ⫺ 2ᐉz3 ⫹ ᐉ3z) 24 P ⫺ (3ᐉz2 ⫺ 4z3) 48 w ⫺ (z4 ⫺ 4ᐉz3 ⫹ 6ᐉ2z2) 24 P ⫺ (3ᐉz2 ⫺ z3) 6 ⫺

ƒ2(z)

ƒ1(z)

Deﬂection Functions for Common Determinate Beamsa

Simply supported beam Uniformly distributed load (w) Concentrated load (P) at midspan (0 ⬍ z ⬍ ᐉ / 2) Cantilever beam Uniformly distributed load (w)

Beam

TABLE 13.1

⫺

4

5wᐉ 384 Pᐉ3 ⫺ 48 wᐉ4 ⫺ 8 Pᐉ3 ⫺ 3

ƒ1 (␦max)

ᐉ

⫺Pᐉ

ᐉ

ᐉ

2

ᐉ

2

wᐉ 8 Pᐉ ⫺ 4 wᐉ2 ⫺ 2 ⫺

z (␦max) 2

ƒ2 (␦max)

13.4

DEFORMATIONS IN FLEXURAL MEMBERS

391

Ultimately, local building code regulations should be followed regarding allowable service load deﬂections. It is generally accepted that deﬂections should not exceed L/240 when brittle nonstructural elements such as ﬂoors, partition walls, ducts, and piping are attached to the structure. Analysis Example 13.1: Timoshenko Beam Theory Obtain the equation of the elastic curve for the uniformly loaded cantilever beam shown in the Fig. 13.4 using Timoshenko beam theory. SOLUTION The free-body diagram of a portion of the beam at the ﬁxed end is shown in Fig. 13.5. The bending moment and shear force along the length of the beam are expressed as Mx(z) ⫽ wᐉz ⫺

wᐉ2 wz2 ⫺ 2 2

and Vy(z) ⫽ wᐉ ⫺ wz The mathematical boundary conditions for the physical conditions of no transverse deﬂection and no bending slope at the ﬁxed end are y(0) ⫽ 0

(0) ⫽ 0

The ﬁrst differential equation of Timoshenko beam theory is written as

冉

d 1 wᐉ2 wz2 ⫽ wᐉz ⫺ ⫺ dz EI 2 2

冊

Integrating gives

y

w z l

Figure 13.4 Uniformly loaded cantilever beam.

392

PULTRUDED FLEXURAL MEMBERS

w

wl 2 2

M x (z ) z

Vy

wl

Figure 13.5 Free-body diagram of the ﬁxed end of a cantilever beam.

(z) ⫽

冉

冊

1 wᐉz2 wᐉ2z wz3 ⫺ ⫺ ⫹ C1 EI 2 2 6

Substituting the boundary condition (0) ⫽ 0 gives C1 ⫽ 0. The second differential equation of the Timoshenko beam theory is then written as

冉

冊

dy 1 1 wᐉz2 wᐉ2z wz3 ⫽⫺ (wᐉ ⫺ wz) ⫹ ⫺ ⫺ dz KAG EI 2 2 6 and integrating gives y⫽

冉

冊 冉

冊

1 wz2 1 wᐉz3 wᐉ2z2 wz4 ⫺wᐉz ⫹ ⫹ ⫺ ⫺ ⫹ C2 KAG 2 EI 6 4 24

Substituting the boundary condition y(0) ⫽ 0 gives C2 ⫽ 0. Finally, the solution is rearranged and written in its usual form, y(z) ⫽ ƒ1(z)/EI ⫹ ƒ2(z)/ KAG, as y(z) ⫽ ⫽

冉

冊

冉

1 wᐉz3 wᐉ2z2 wz4 1 wz2 ⫺ ⫺ ⫹ ⫺wᐉz ⫹ EI 6 4 24 KAG 2

冊

⫺w 4 w (z ⫹ 4ᐉz3 ⫺ 6ᐉ2z2) ⫺ (⫺z2 ⫹ 2ᐉz) 24EI 2KAG

which can be found in the third row of Table 13.1.

13.5 DETERMINATION OF DEFLECTIONS AND STRESSES FOR SERVICEABILITY AND ULTIMATE LIMIT STATES For ﬂexural members the deﬂections are determined for the serviceability limit state (SLS) and stresses (or stress resultants) are determined for the ultimate limit state (ULS). Since pultruded proﬁles have low stiffness-tostrength ratios relative to conventional structural materials, the serviceability limit states of ﬂexural members are checked ﬁrst (i.e., the deﬂection calculation is the ﬁrst step in the design procedure). Thereafter, the ultimate

13.6

SERVICEABILITY LIMITS STATES

393

strength limit states are checked. These are usually governed by critical buckling stresses. The axial and shear material strengths very seldom control the design of ﬂexural members. The order of the limit states presented follows this order. Notice that this is typically not the order in which limit states are considered for design with proﬁles of metallic materials that are braced against global lateral–torsional buckling. In such cases the material strength criteria are checked ﬁrst and thereafter, shear stresses and transverse deﬂections are checked. This is because most standard I-shaped steel sections (proﬁles) used as ﬂexural members are classiﬁed as compact sections, which means that they will reach their full plastic moment capacity prior to local buckling of their ﬂanges. If pultruded proﬁles are produced with the same cross-sectional geometries as steel compact sections, they will not be compact, due to their different mechanical properties. In such steel-like geometry pultruded proﬁles, local buckling of ﬂanges (and occasionally, webs) becomes a critical limit state.8 13.6 13.6.1

SERVICEABILITY LIMITS STATES Deformation Limit State: Transverse Deﬂection

Timoshenko shear deformation beam theory is used to determine the deﬂection of a pultruded beam. This is the procedure recommended by the Structural Plastic Design Manual (1984) and the Eurocomp Design Code and Handbook (1996). The use of shear deformation beam theory is especially important in pultruded beams because of the relatively low longitudinal modulus (leading to beams with short spans) and the relatively high EL /GLT ratios, due to the low shear modulus of pultruded materials (Bank, 1989a,b). To calculate the deﬂection, appropriate choices of the ﬂexural rigidity, EI, and the transverse shear rigidity, KAG, are required. For homogeneous pultruded beams having the same properties in the ﬂanges and webs of the proﬁle, the ﬂexural rigidity is obtained as EI ⫽ ELIx

(13.10)

where Ix is the second moment of the cross section and EL is the longitudinal modulus of the pultruded material in the proﬁle. For nonhomogeneous pultruded proﬁles having different longitudinal moduli in the parts of the cross section, the ﬂexural rigidity can be found using the composite section method9 or the transformed-section method. The longitudinal modulus, especially that

8 Due to the high longitudinal strength and low longitudinal stiffness of glass-reinforced pultruded proﬁles, it is difﬁcult to design a compact type of section in which compressive failure would occur before local ﬂange buckling, as we discuss further below. 9 As discussed previously.

394

PULTRUDED FLEXURAL MEMBERS

of the ﬂanges, is the dominant material property in the ﬂexural rigidity. It has been shown that ﬂexural rigidity is insensitive to the transverse modulus of the pultruded material. For homogeneous pultruded beams, having the same properties in the ﬂanges and webs of the proﬁle, the transverse shear rigidity is obtained from KAG ⫽ ktim AGLT ⬇ AwebGLT(web)

(13.11)

where, ktim is the Timoshenko shear coefﬁcient, A the area of the entire cross section, GLT the in-plane shear modulus of the webs and the ﬂanges (assumed to be equal), Aweb the total area of the web or webs of the section, and GLT(web) the in-plane shear modulus of the web or webs. The transverse shear rigidity is a function of the shear ﬂow in the ﬂanges and the webs of open, singlecell, and multicell thin-walled sections (Cowper, 1966; Bank, 1987; Bank and Melehan, 1989). Equations for ktim for I- and single-cell box-shaped sections are given in Table 13.2 following the procedure described in Bank (1987) for proﬁles for which the in-plane properties of the pultruded material are the same in the webs and the ﬂanges. For proﬁles in which the properties of the pultruded material in the webs and the ﬂanges are not the same, a modiﬁed form of the Timoshenko beam theory is required (Bank, 1987). For conventionally manufactured glass-reinforced pultruded I- and boxshaped proﬁles it has been shown that the transverse shear rigidity can be approximated by either the full-section shear rigidity deﬁned as AGb or by the area of the web multiplied by the in-plane shear modulus of the web, AwebGLT(web) (Bank 1989a; Nagaraj and GangaRao, 1997). The full-section shear modulus is obtained from tests on full-section pultruded beams (Bank, 1989b; Roberts and Al-Ubaidi, 2002; Giroux and Shao, 2003). Analysis Example 13.2: Determination of the Flexural and Shear Rigidities for Pultruded Proﬁles Determine the value of the ﬂexural rigidity, EI, and the shear rigidity, KAG, for the homogeneous FRP beams shown in Table 13.3. Compare the predictions of the exact theory (i.e., KAG ⫽ Ktim AGLT) with those of the approximate theory (i.e., KAG ⫽ AwebGLT(web)). SOLUTION The values calculated for the proﬁles considered are displayed in Table 13.4. It can be seen from the table that the difference between the exact and approximate methods of determining the transverse shear rigidity for I-shaped proﬁles is between 10 and 20%, with the approximate method giving a lower value. (For box-shaped sections, the approximate method will generally give a higher value than that of the exact method.) A lower value of transverse shear stiffness translates into a higher value of predicted shear deﬂection, which is conservative from a design perspective. The effect of shear deformation increases as the ratio of the ﬂexural stiffness to the transverse shear stiffness increases. It can be seen from the last column in Table 13.4 that the effect of shear deformation will be larger in sections with wider

395

20(1 ⫹ 3m)2 (180m ⫹ 300m ⫹ 144m ⫹ 60m2n2 ⫹ 60mn2 ⫹ 24) ⫹ (LGLT / EL)(30m2 ⫺ 50mn2 ⫺ 30m2n2 ⫹ 6m ⫺ 4)

80 192 ⫹ (LGLT / EL)(⫺12)

I-shaped section

Box-shaped section

Source: Bank (1987).

3

2

2

20(1 ⫹ 3m)2 (180m ⫹ 300m ⫹ 144m ⫹ 60m2n2 ⫹ 60mn2 ⫹ 24) ⫹ (LGLT / EL)(30m2 ⫹ 40mn2 ⫹ 60m2n2 ⫹ 6m ⫺ 4) 3

80 192 ⫹ (LGLT / EL)(33)

Proﬁle

Unsymmetric Geometry (EL, GLT, L constant, n ⫽ b / h and m ⫽ tƒb / twh)

Homogeneous Proﬁle

Timoshenko Shear Coefﬁcient for Homogeneous I and Box Proﬁles

Symmetric Geometry (EL, GLT, L constant and tw ⫽ tƒ, b ⫽ h)

TABLE 13.2

396

8

8

8

8

4

4

4

4

0.375

0.500

0.500

0.375

0.375

tƒ (in.)

0.375

0.375

0.375

0.375

0.375

tw (in.)

55.45

77.80

67.05

55.45

99.18

Ix (in4)

5.72

9.26

6.63

5.72

8.72

A (in2)

3.0

6.0

3.0

3.0

3.0

Aweb (in2)

13.7

2.6

2.6

2.6

2.6

EL (Msi)

0.450

0.425

0.425

0.425

0.425

GLT ⫽ GLT(web) (Msi)

0.31

0.33

0.33

0.33

0.33

LT

GFRP, properties reported by manufacturers of glass–vinylester conventional pultruded proﬁles; CFRP, calculated properties of custom pultrusion: three-ply glass CFM (3 ⫻ 0.025 in.) ⫹ two-ply 50% unidirectional carbon–vinylester (2 ⫻ 0.15 in.). Only the ﬁrst two proﬁles are conventional off-the-shelf proﬁles.

a

8

h (in.)

8

b (in.)

Geometric and Mechanical Properties of Pultruded Proﬁles for Example 13.2

GFRP WF section 8 ⫻ 8 ⫻ –38 GFRP I section 4 ⫻ 8 ⫻ –38 GFRP I section 4 ⫻ –12 ⫻ 8 ⫻ –38 GFRP box section 4 ⫻ –12 ⫻ 8 ⫻ –38 CFRP I section 4 ⫻ 8 ⫻ –38

Proﬁlea

TABLE 13.3

13.6

SERVICEABILITY LIMITS STATES

397

TABLE 13.4 Flexural and Transverse Shear Rigidities of Pultruded Beams in Example 13.2 Proﬁle GFRP WF 8⫻8⫻ GFRP I 4⫻8⫻ GFRP I 4 ⫻ –12 ⫻ GFRP box 4 ⫻ –12 ⫻ CFRP 4⫻8⫻

ELIx ktim AGLT AwebGLT(web) (Mlb) (Mlb) Percent diff. ktim AGLT

ELIx (Mlb-in2)

ktim

257.9

0.413

1.530

1.257

⫺17.8

169

144.2

0.608

1.478

1.257

⫺14.9

98

174.3

0.554

1.561

1.257

⫺19.5

112

200.4

0.558

2.196

2.514

⫹14.5

91

759.7

0.610

1.570

1.350

⫺14.0

484

–38 –38

8 ⫻ –38 8 ⫻ –38 –38

ﬂanges and in proﬁles made from pultruded materials having higher in-plane anisotropy ratios (i.e., EL /GLT ratios), such as a carbon ﬁber–reinforced beam. However, the total deﬂection in the beam will be signiﬁcantly less, due to its signiﬁcantly larger ﬂexural rigidity, EI. 13.6.2

Long-Term Deﬂection in Pultruded Beams

The moduli of a pultruded proﬁle will decrease over time if the proﬁle is subjected to sustained loads. This is because ﬁber-reinforced polymeric materials are viscoelastic and creep under sustained loads. Although reinforced polymers do not creep as much as unreinforced polymers, they are nevertheless susceptible to increases in deﬂection over time without a commensurate increase in load. Reinforced polymers with oriented continuous ﬁbers creep less than those with random reinforcement, as do those with higher volume fractions of ﬁbers (Scott et al., 1995). As shown in Table 1.5, most conventional pultruded proﬁles have approximately 40% ﬁber reinforcement by volume, of which about 60 to 70% consists of continuous longitudinal reinforcement. Therefore, pultruded proﬁles are considered ‘‘reasonably’’ creep resistant, particularly when the sustained loads are small, such as in walkways, platforms, and short bridges. However, where pultruded structures are subjected to a signiﬁcant amount of sustained load, long-term creep deformation must be considered in design. To predict the long-term deﬂection, time-dependent versions of longitudinal modulus and in-plane shear modulus are used in deﬂection equations. They are referred to as viscoelastic moduli and are used instead of the conventional instantaneous moduli to predict long-term deﬂection using the Timoshenko beam theory described previously. The viscoeleastic moduli are identiﬁed with a superscript v to distinguish them from the instantaneous

398

PULTRUDED FLEXURAL MEMBERS

moduli that are typically reported for pultruded materials and measured using standard coupon tests. The longitudinal viscoelastic modulus, E vL (t), and the in-plane viscoelastic shear modulus, G vLT (t), are deﬁned as ELE tL EL ⫽ E tL ⫹ ELt ne 1 ⫹ (EL /E Lt ) t ne

(13.12)

GLTG tLT GLT ⫽ G ⫹ GLT t ng 1 ⫹ (GLT /G tLT) t ng

(13.13)

E vL(t) ⫽ and G vLT (t) ⫽

t LT

where t is time in hours and EL and GLT are the instantaneous (i.e., the usual) moduli. E tL and G tLT are known as creep moduli and ne and ng are the creep rate exponents. The creep moduli and creep rate exponents are constants for a given material type and are obtained from long-term creep tests using the linearized version of Findley’s theory (ASCE, 1984). The theory has been applied to determine the creep constants for conventional pultruded sections by a number of authors (Bank and Mosallam, 1992; Mottram, 1993; Scott and Zureick, 1998; Shao and Shanmugam, 2003). The values of the creep moduli and creep rate exponents recommended for design are given in Table 13.5. They were obtained by Mosallam and Bank (1991) for ﬂexural members, and by Scott and Zureick (1998) for compression members (discussed later). In typical pultruded structures, the long-term sustained stress is usually between 10 and 20% of the ultimate strength of the material. The constants above are intended to be used at these load levels. At higher sustained stress levels the creep moduli show a time dependency and the constant reported in Table 13.5 cannot be used. The creep rate constants appear to be relatively insensitive to stress level (Scott and Zureick, 1998; Shao and Shanmugam, 2003). The reason for the difference in the creep constants for pultruded members in ﬂexure and in pure compression has not been fully explained but is felt to be due to structural effects in ﬂexural members, such as complex stress states at load and support points and the nonuniformity of the stress along the member length, which inﬂuences long-term tests. Greater creep

TABLE 13.5 Creep Constants for Use in Design of Pultruded Structural Members Sustained Loading Type Flexure Compression

EtL (psi) 180 ⫻ 10 216 ⫻ 106 6

ne

GtLT (psi)

ng

0.30 0.25

27 ⫻ 10 NA

0.30 NA

6

13.6

SERVICEABILITY LIMITS STATES

399

deformation is obtained in a pultruded structural member as both the creep rate exponent and the ratio of the instantaneous modulus to the creep modulus increase. 0 ⫽ Using instantaneous longitudinal moduli E 0L ⫽ 2.6 ⫻ 106 psi and G LT 6 0.425 ⫻ 10 psi for glass–vinylester pultruded proﬁles, the following expressions are obtained for viscoelastic moduli for ﬂexural members for use in design calculations: E vL ⫽ G vLT ⫽

468 ⫻ 106 180 ⫹ 2.6t 0.3

psi

(13.14)

11.475 ⫻ 106 .27 ⫹ 0.425t 0.3

psi

(13.15)

Using these expressions, Table 13.6 shows the values calculated for the viscoleastic longitudinal and shear moduli for these pultruded members under sustained loading durations of 1, 10, 30, and 50 years. Analysis Example 13.3: Instantaneous and Long-Term Deﬂection of a Pultruded Beam Under Sustained Load A simply supported WF 8 ⫻ 8 ⫻ 3/ 8 glass–vinylester pultruded beam spans 12 ft. Its properties are given in the ﬁrst row of Table 13.3. The beam has a nominal self-weight of 6.97 lb/ft. It is loaded with a uniformly distributed sustained dead load of 150 lb/ft and a live load of 200 lb/ft. Determine the instantaneous midspan deﬂection and the midspan deﬂection after 30 years of sustained load on the beam under self-weight, sustained dead load, and live load. Assume that none of the live load is sustained. SOLUTION Using the data from Tables 13.4 and 13.5 the following stiffness properties are obtained for the beam for the instantaneous and 30-year long-term deﬂection calculations. ELIx ⫽ 257.9 ⫻ 106 lb-in2 ktim AGLT ⫽ 1.530 ⫻ 106 lb

TABLE 13.6 Longitudinal and Shear Moduli of Glass–Vinylester Pultruded Proﬁles for Various Sustained Load Durations E (⫻10 psi) G (⫻106 psi) v L v LT

6

Initial

1 Year

10 Years

30 Years

50 Years

2.60 0.425

2.13 0.343

1.81 0.287

1.62 0.255

1.52 0.239

400

PULTRUDED FLEXURAL MEMBERS

E vLIx ⫽ (1.62 ⫻ 106)(99.18) ⫽ 160.67 ⫻ 106 lb-in2 ktim AG vLT ⫽ 0.413(8.72)(0.255 ⫻ 106) ⫽ 0.918 ⫻ 106 lb The maximum midspan deﬂection is given as 5wᐉ4 wᐉ2 ␦max ⫽ ⫺ ⫺ 384(EI) 8(KAG) The deﬂections due to the sustained loads and live loads are calculated separately and added. For the live load deﬂection, the instantaneous moduli are used at all times (according to the Boltzmann superposition principle; ASCE, 1984). Substituting in the deﬂection equation, the instantaneous deﬂection is 5(156.97/12)(144)4 (156.97/12)(144)2 ␦max(sw⫹DL) ⫽ ⫺ ⫺ 384(257.9 ⫻ 106) 8(1.530 ⫻ 106) ⫽ ⫺0.284 ⫺ 0.0222 ⫽ ⫺0.3060 in.

5(200/12)(144)4 (200/12)(144)2 ␦max(LL) ⫽ ⫺ ⫺ 384(257.9 ⫻ 106) 8(1.530 ⫻ 106) ⫽ ⫺0.3618 ⫺ 0.0282 ⫽ ⫺0.3900 in.

The total instantaneous midspan deﬂection is therefore ␦max(instantaneous) ⫽ ⫺0.3060 ⫺ 0.3900 ⫽ ⫺0.6962 in.

which is ᐉ /206

The 30-year (long-term) deﬂection is 5(156.97/12)(144)4 (156.97/12)(144)2 ␦max(sw⫹DL) ⫽ ⫺ ⫺ 384(160.67 ⫻ 106) 8(0.918 ⫻ 106) ⫽ ⫺0.4558 ⫺ 0.0369 ⫽ ⫺0.4927 in.

The live load deﬂection calculation is unchanged: 5(200/12)(144)4 (200/12)(144)2 ␦max(LL) ⫽ ⫺ ⫺ 384(257.9 ⫻ 106) 8(1.530 ⫻ 106) ⫽ ⫺0.3618 ⫺ 0.0282 ⫽ ⫺0.3900 in.

The total long-term (30-year) midspan deﬂection is therefore

13.7

ULTIMATE LIMIT STATES

␦max(30 year) ⫽ ⫺0.4927 ⫺ 0.3900 ⫽ ⫺0.8827 in.

401

which is ᐉ /163

This is a 26.8% increase in the total deﬂection and a 61.0% increase in the sustained load deﬂection over the 30-year period chosen. It can also be observed that the shear deﬂection for both instantaneous and long-term deﬂection is approximately 8% of the total deﬂection in a beam that has the mechanical and geometric properties stipulated.

13.7 13.7.1

ULTIMATE LIMIT STATES Lateral–Torsional Buckling

The term lateral–torsional buckling is used to describe a speciﬁc type of physical instability that commonly occurs in open-section (typically, I-shaped) ﬂexural members loaded by transverse loads. When the critical lateral– torsional buckling load is reached, the ﬂanges displace laterally (or sideways) relative to the transverse load direction, and the web twists, causing the entire beam to move out of its vertical plane. Figure 13.6 shows lateral–torsional buckling of a pultruded wide-ﬂange I-shaped proﬁle. Lateral–torsional buckling of doubly symmetric pultruded proﬁles has been studied experimentally by a number of researchers (Mottram, 1992; Turvey, 1996; Davalos and Qiao, 1997). It is generally accepted that the well-known equation that is used for isotropic beam sections (see, e.g., Salmon and Johnson, 1996) can be used for conventional pultruded I-shaped proﬁles provided that the appropriate values of E and G are used in the equations. Inclusion of the effects of shear deformation on lateral–torsional buckling of conven-

Figure 13.6 Lateral–torsional buckling of an I-shaped pultruded proﬁle. (Copyright G. J. Turvey and Y.-S. Zhang, published with permission.)

402

PULTRUDED FLEXURAL MEMBERS

tional pultruded proﬁles is small and can generally be neglected, as shown by Roberts (2002). The critical lateral–torsional buckling stress for homogeneous doubly symmetric open proﬁles is given as lat cr ⫽

Cb Sx

冪

2ELIyGLT J 4E 2LIyC ⫹ (kƒ Lb)2 (kƒ Lb)2(k Lb)2

(13.16)

and the critical lateral–torsional bending moment (for a homogeneous section10) is given as lat M lat cr ⫽ cr Sx

(13.17)

where Cb is a coefﬁcient that accounts for moment variation along the length of the beam, Sx ⫽ Ix /c is the section modulus about the strong axis, J is the torsional constant, Iy the second moment about the weak (i.e., vertical) axis, C the warping constant, kƒ the effective length coefﬁcient for ﬂexural buckling about the weak axis (i.e., kƒ ⫽ 1.0 for simple supports that permit rotation about the y-axis at the beam ends), k an effective length coefﬁcient for torsional buckling of the section (i.e., k ⫽ 1.0 for supports that prevent twisting about the neutral axis but permit the ﬂanges to warp and move in the z-direction at the beam ends), and Lb the unbraced length of the member (or a portion thereof). The lateral–torsional buckling load depends on the height of the load relative to the neutral axis of the beam (Timoshenko and Gere, 1961; Mottram, 1992). Equation (13.16) assumes that the transverse load acts at the neutral axis of the section in its undeformed conﬁguration. When the load acts on the top ﬂange (above the neutral axis), the beam is more susceptible to lateral– torsional buckling; when the load acts on the bottom ﬂange (below the neutral axis), the beam is less susceptible to lateral–torsional buckling. For I-shaped proﬁles, C ⫽ Iy(d 2 /4), where d is the depth of the proﬁle. For other common thin-walled sections, values of the warping constant, identiﬁed as C, can be found in texts such as Timoshenko and Gere (1961) and Salmon and Johnson (1996). The coefﬁcient Cb can also be found in the aforementioned texts. For the common case of a simply supported uniformly loaded beam with kƒ ⫽ k ⫽ 1.0, Cb ⫽ 1.13. The values of kƒ and k depend on the connection detailing. kƒ is usually assumed to be equal to k in pultruded structures as it is in metallic structures. In typical shear-plate (clip-angle) connections in pultruded structures, little warping restraint of the ﬂanges can be expected and k ⫽ 1.0 for simply supported (z-axis) beams. Some degree of rotational restraint may be possible 10 For a nonhomogeneous beam composite section, properties in the buckling equation and the critical bending moment are found by integrating the axial stress as described previously.

13.7

ULTIMATE LIMIT STATES

403

about the y-axis; however, this is also likely to be small in pultruded connections, and kƒ ⫽ 1.0 is recommended for simply supported (z-axis) beams unless rotational restraint can be demonstrated by testing. A ﬂexural member in a pultruded structure will typically be designed to be braced along its length to prevent lateral–torsional buckling. Often, this bracing is provided continuously along the length of the compression ﬂange of the member by a continuous diaphragm (e.g., a ﬂoor plate attached to the top ﬂange). Where continuous support in not provided to the top ﬂange, equation (13.16), should be used to calculate the distance required between lateral braces, Lb, to prevent lateral–torsional buckling. The torsional resistance of a closed cross section such as a square tube is much larger than that of an open section, and lateral–torsional buckling is not likely to be a critical limit state. To determine the critical lateral–torsional buckling stress for a closed section, the ﬁrst term only in equation (13.16) can be used (ASCE, 1984). For singly symmetric sections such as channels and angles few experimental data are available for pultruded proﬁles. Use of appropriate equations for isotropic metallic members is recommended at this time, with substitution of the orthotropic material properties in the isotropic equations (Razzaq et al., 1996). If the ﬂexural member is subjected to long-term sustained loading, the instantaneous longitudinal and shear moduli in the lateral buckling equation should be replaced by the appropriate viscoelastic moduli. This will reduce the lateral–torsional buckling load for the member and will decrease the design unbraced length. Although such an approach is recommended, no test data exist that have documented the occurrence of creep buckling of pultruded proﬁles under sustained load. 13.7.2

Local Buckling of Walls Due to In-Plane Compression

Conventional pultruded GFRP proﬁles are especially susceptible to local buckling under transverse loads due to the low in-plane moduli and the slenderness (width-to-thickness ratio) of the plate elements (known as walls) that make up the thin-walled proﬁle. Local buckling in compression ﬂanges of beams has been demonstrated in numerous tests (e.g., Barbero et al., 1991; Bank et al., 1994b; 1996a). Figure 13.7 shows local compression ﬂange buckling in the constant moment region of a transversely loaded wide-ﬂange pultruded proﬁle. If the load is increased beyond the elastic buckling load, the proﬁle will typically fail as a result of separation of the ﬂange from the web due to high transverse tensile stresses (Bank and Yin, 1999), which is followed immediately by in-plane buckling of the then-unsupported web, as shown in Fig. 13.8. The critical buckling load (or stress) in a wall (or panel) of a proﬁle is a function of the boundary conditions on the longitudinal edges of the wall. In wide-ﬂange I-shaped proﬁles the ﬂange is particularly susceptible to buckling since the one edge is free while the other edge is elastically restrained at the

404

PULTRUDED FLEXURAL MEMBERS

Figure 13.7 Local compression ﬂange buckling in a wide-ﬂange pultruded proﬁle.

web–ﬂange junction. There is no exact closed-form solution for the case of a free and rotationally restrained orthotropic plate. The characteristic transcendental equations required to obtain the buckling load for the plate in terms of the coefﬁcient of edge restraint of the plate are given in Bank and Yin (1996). For I-shaped proﬁles, both the Structural Plastics Design Manual (ASCE, 1984) and the Eurocomp Design Code and Handbook (Eurocomp, 1996) recommend that the elastically restrained edge be assumed to be simply supported. This is known to be an overly conservative assumption. Experimental tests on both pultruded beams and short columns (where local ﬂange buckling also is critical) clearly show that the local buckling stress is signiﬁcantly higher than that predicted by the free/simply supported plate assumption (Bank et al., 1995a; Qiao et al., 2001; Mottram, 2004). However, it is also well known that the ﬂange buckling load is lower than that predicted by assuming that the restraining web provides a ﬁxed edge condition (Bank et al., 1995a). An approximate method to obtain closed-form equations for the buckling load for free and rotationally restrained orthotropic plates has been proposed by Kolla´r (2002). Kolla´r subsequently extended this work to give closed-form equations for buckling of many different thin-walled sections with orthotropic walls (Kolla´r, 2003), using his equations together with existing equations in the literature for other boundary conditions. Kolla´r’s results show very good

Figure 13.8 Ultimate failure following local ﬂange buckling.

13.7

ULTIMATE LIMIT STATES

405

agreement with ﬁnite element analyses and tests of conventional pultruded proﬁles and reduce to well-known solutions in the literature for plates with special properties. Kolla´r’s equations are presented below for the design of pultruded proﬁles. Kolla´r’s method has the ability to distinguish between ﬂange buckling in beams subjected to transverse loads (ﬂexure) and ﬂange buckling in columns subjected to axial loads (pure compression) since the web restraint is given as a function of the end conditions of the restraining plate following the procedure presented by Bleich (1952). None of the other existing empirical equations have this ability (Mottram, 2004). Kolla´r’s method also allows the user to determine a priori whether ﬂange buckling or web buckling will control the design based on the slenderness ratios of the ﬂange and web of the section. Kolla´r has presented results for I-, box-, singleleg-angle-, channel-, and Z-shaped sections. Only the design equations for doubly symmetric I- and box-shaped proﬁles are presented in this book, due to the fact that at present these proﬁles are most commonly used as beams and columns in pultruded structures. This includes built-up sections that are I- and box-shaped. The reader is referred to Kolla´r’s work for singly symmetric sections. The cross-sectional notation for I- and box-shaped proﬁles is shown in Fig. 13.9. Note that the wall widths and depths are measured from the centerline of the walls (shown by the dashed lines in Fig. 13.9). Since local buckling of the ﬂange and web of a section due to normal loads are interrelated, ﬂange and web buckling are treated together in this section. Local buckling due to shear (tangential) loads is treated separately. It should be noted, however, that only local ﬂange buckling has been observed experimentally in I-shaped proﬁles since conventional pultruded proﬁles have aspect ratios that lead to ﬂange buckling occurring before web buckling. Neither has in-plane shear buckling been observed experimentally in beam tests. To use Kolla´r’s method, ﬁrst the buckling stresses (or loads) of the walls are found, assuming that they are simply supported at their restrained edges. These buckling stresses are then used to determine which wall buckles ﬁrst and the coefﬁcient of edge restraint for the critical wall. The ﬁnal solution

b bf = b

d

bf

dw

dw tw

tf

tf

tw

Figure 13.9 Cross-sectional notation for I- and box-shaped proﬁles.

406

PULTRUDED FLEXURAL MEMBERS

for the buckling stress for the restrained wall is then given by a closed-form equation that includes the coefﬁcient of edge restraint, , of the critical wall. Three types of simply supported walls11 are needed for the ﬁrst part of the solution. 1. A wall that is free and simply supported on its edges under uniform compressive stress. This solution is used to determine the critical stress in the ﬂange of an I-shaped proﬁle.12 It is given in terms of the ﬂexural rigidities13 of the ﬂange as ss ( free )ƒ ⫽

冋冉 冊

bƒ /2 2 DL 2 tƒ(bƒ /2) a

2

⫹

12 D 2 S

册

(13.18)

where, tƒ the ﬂange thickness, bƒ the proﬁle width (twice the nominal width of the ﬂange), and a the length of the ﬂange.14 For long ﬂanges, as is typically the case, the ﬁrst term in brackets is negligible and the critical stress can be found from ss ( free )ƒ ⫽

4t 2ƒ G b2ƒ LT

(13.19)

In this mode the plate buckles with one buckle half-wavelength, a, equal to the plate length (like a simply supported Euler column). 2. A wall that is simply supported along both edges under uniform compressive stress. This solution is used to determine the critical stress in the ﬂange of a box section. It is given in terms of the ﬂexural rigidities of the ﬂange as ( ss ss)ƒ ⫽

2 2 (兹DLDT ⫹ DLT ⫹ 2DS) tƒb2ƒ

(13.20)

The length of the buckle half-wavelength for this mode is given by

11 For all cases it is assumed that the loaded edges are simply supported. The super- and subscripts are used to identify the longitudinal unloaded edges of the wall. 12 A different notation from that used in Kolla´r (2003) is used in what follows, to make the equations more familiar to structural engineers unfamiliar with laminated plate and composite material notation. Equations are given for plate buckling stresses and not plate buckling loads, for the same reason. 13 See Chapter 12 for a deﬁnition of plate ﬂexural rigidities. 14 Note that in many texts the parameter b is used to denote the width of the ﬂange only and is equal to one-half of bƒ.

13.7

ULTIMATE LIMIT STATES

407

冪EE

(13.21)

2 (13.9兹DLDT ⫹ 11.1DLT ⫹ 22.2DS) twd w2

(13.22)

(ass ss)ƒ ⫽ bƒ

4

L T

3. A wall that is simply supported along both edges under linearly varying compressive stress. This solution is used to determine the critical stress in the web of an I or box section. It is given in terms of the ﬂexural rigidities of the web as ( ss ss)w ⫽

where tw is the thickness of the web and dw is the depth of the web. The length of the buckle half-wavelength for this mode is given by

冪

ss (ass )w ⫽ 0.707dw 4

EL ET

(13.23)

Coefﬁcient of Restraint A nondimensional coefﬁcient known as the coefﬁcient of restraint (Bleich, 1952), , is deﬁned to account for the combined effect of the rotational stiffness of the junction itself and the plate geometric and mechanical properties on the critical buckling stress.15 It is deﬁned as ⫽

DT kLT

(13.24)

where k is the rotational spring constant of the junction between the walls and LT and DT are the width and ﬂexural rigidity of the plate perpendicular to the edge being restrained (i.e., in the transverse direction of the orthotropic plate, hence the subscript T). Local Buckling Equations for an I-Shaped Proﬁle in Bending About Its Major ss Axis If ( ss free)ƒ /(EL)ƒ ⬍ ( ss)w /(EL)w, the ﬂange will buckle before the web. The ﬂange will therefore be ‘‘restrained’’ by the web. Except in very unusual circumstances, this will be the local buckling mode for conventional pultruded GFRP proﬁles. The spring constant is given as

15 That is, even if the junction has a relatively high rotational spring stiffness but the plate is very ﬂexible and wide (small DT and large LT), the restraining effect of the junction on the buckling load will not be very signiﬁcant.

408

PULTRUDED FLEXURAL MEMBERS

kI-flange ⫽

冋

册

( ss 2(DT)w free)ƒ(EL)w 1⫺ ss dw ( ss )w(EL)ƒ

(13.25)

and the local buckling stress for the rotationally restrained ﬂange is given in terms of the properties of the ﬂange as16

冉冪

冊

1 DLDT 7 ⫹ 12DS 2 (bƒ /2) tƒ 1 ⫹ 4.12I-flange

(13.26)

(DT)ƒ (ET)ƒt ƒ3 ⫽ kI-flange(bƒ /2) 6kI-flangebƒ[1 ⫺ (T)ƒ(L)ƒ]

(13.27)

local,I-flange cr ⫽

where I-flange ⫽

The critical bending moment for local ﬂange buckling for a homogeneous I-shaped section for bending about the major axis is given as local,I-flange M local,I-flange ⫽ cr Sx cr

(13.28)

The buckle half-wavelength, a, for this case is given in terms of the properties of the ﬂange as (Kollar and Springer, 2003, Table 4.10)

冪

bƒ D aI-flange ⫽ 1.675 4 L(1 ⫹ 4.12I-flange) 2 DT

(13.29)

The length of the buckle half-wavelength may be used to determine the required spacing of bracing members to prevent local ﬂange buckling in Ishaped members. The length of buckle half-wavelength is typically between 1.0 to 2.0 times the ﬂange width, bƒ, for conventional FRP pultruded proﬁles. This implies that to brace the section against local buckling, the compression ﬂange needs to be supported (or restrained) continuously by a ﬂooring or wall system. The spacing of the fasteners used to attach the ﬂooring system to the compression ﬂange must be less than the buckle half-wavelength, and the ﬂooring system must be stiff enough, and attached ﬁrmly enough, to prevent the local instability of the ﬂange. ss If ( ss free)ƒ /(EL)ƒ ⬎ ( ss)w /(EL)w, the web will buckle before the ﬂange. A closed-form expression to predict the buckling stress of the web when re-

16

Kolla´r (2003) provides an alternative, more detailed equation for greater accuracy for highly orthotropic walls. The equations presented in this book are suitable for the design of conventional pultruded proﬁles.

13.7

ULTIMATE LIMIT STATES

409

strained by the ﬂanges and loaded with a linearly varying axial stress is not currently available. Equation (13.22), for a wall simply supported on its two edges and loaded with a linearly varying axial stress, can be used as a realocal,I-web ) as the ﬂanges will not prosonable approximation, (i.e., ( ss ss)w ⫽ cr vide signiﬁcant rotational restraint to the web. The critical bending moment for local web buckling for a homogeneous Ishaped section for bending about the major axis is given as local,I-web M local,I-web ⫽ cr cr

2Ix d ⫺ 2tƒ

(13.30)

Bending of an I-shaped proﬁle about its minor axis is not treated in this book since a conventional pultruded I-shaped proﬁle will generally be used in bending about its major axis because of serviceability deﬂection requirements. When used as a beam-column (discussed in Chapter 14), it will be assumed that the beam is also bent about its major axis and braced about its minor axis. Local buckling of the ﬂanges of an I-shaped proﬁle in bending about its minor axis can be treated in a fashion similar to local buckling of the leg of a single-angle section (presented in Kolla´r, 2003). Local Buckling Equations for a Rectangular Box Proﬁle in Bending If ss ( ss ss)ƒ /(EL)ƒ ⬍ ( ss)w /(EL)w, the compression ﬂange will buckle before one of the webs. The ﬂange will therefore be restrained by both webs, one on either longitudinal edge of the ﬂange. The spring constant is then given as kbox-flange ⫽

冋

册

( ss 4(DT)w ss)ƒ(EL)w 1 ⫺ ss dw ( ss)w(EL)ƒ

(13.31)

and the local buckling stress for the rotationally restrained ﬂange is given in terms of the properties of the ﬂange as local,box-flange ⫽ cr

2 [2兹(DLDT)(1 ⫹ 4.139) b2ƒtƒ ⫹ (DLT ⫹ 2DS)(2 ⫹ 0.62box-flange2)]

(13.32)

where box-flange ⫽

1 1 ⫽ 1 ⫹ 10box-flange 1 ⫹ 10 [(DT)ƒ /kbox-flangebƒ]

(13.33)

The critical bending moment for local ﬂange buckling for a homogeneous box-shaped section for bending about the major axis is given as

410

PULTRUDED FLEXURAL MEMBERS

M local,box-flange ⫽ local,box-flange cr cr

2Ix d

(13.34)

The buckle half-wavelength, a, for this case is given in terms of the properties of the ﬂange as (Kolla´r and Springer, 2003, Table 4.10) abox-flange ⫽ bƒ

冪DD 冉1 4

L T

冊

1 ⫹ 4.139box-flange

(13.35)

ss If ( ss ss)ƒ /(EL)ƒ ⬎ ( ss)w /(EL)w, the webs will buckle before the ﬂange. A closed-form expression to predict the buckling stress of the web when restrained by the top and bottom ﬂanges and loaded with a linearly varying axial stress is not currently available. Equation (13.22), for a web simply supported on its two edges, can be used as a conservative approximation (i.e. ). For conventional pultruded GFRP square-box beams, (ss)w ⫽ local,box-web cr the ﬂange will buckle before the web. Only in the case of rectangular box proﬁles with large depth-to-width ratios (⬎2) will the web possibly buckle before the ﬂange. The critical bending moment for local web buckling for a homogeneous box-shaped section for bending about the major axis is given as

local,box-web local,box-web M cr ⫽ cr

2Ix d ⫺ 2tƒ

(13.36)

Approximate Procedure for Local Buckling of I-Shaped Proﬁles To use the equations due to Kolla´r (2003) presented previously, all of the in-plane properties of the orthotropic walls of the section are required to predict the buckling stress. However, the in-plane shear modulus is often not reported by manufacturers and is not required to be reported by the European Standard EN 13706 (CEN, 2002a). In this situation, the simpliﬁed form suggested in the Structural Plastics Design Manual (ASCE, 1984, p. 676) for obtaining the critical ﬂange buckling stress for the free and rotationally restrained ﬂange in an I-proﬁle can be used as an approximation (Mottram, 2004): local,I-flange ⫽ cr,approx

2t ƒ2 (bƒ /2)2

冋冉

0.45 ⫹

冊

册

兹ELET bƒ2 4a2 12(1 ⫺ LT)

(13.37)

where the mechanical properties are those of the ﬂange. This expression requires the length of the buckle half-wavelength, a, which is not known a priori. To use this equation, the buckle half-wavelength can be taken conservatively as 2bƒ for wide-ﬂange and 3bƒ for narrow-ﬂange conventional pultruded I-shaped proﬁles. Alternatively, the ﬁrst term in brackets can be taken even more conservatively as 0.45.

13.7

ULTIMATE LIMIT STATES

411

The approximate critical bending moment for the local ﬂange buckling of a homogeneous I-shaped proﬁle loaded in ﬂexure is therefore local,I-flange local,I-flange M cr,approx ⫽ cr,approx

2Ix d

(13.38)

Further Discussion of Flange Buckling in I-Sections In many designs of Ishaped proﬁles, particularly those with wide ﬂanges, the local buckling stress in the ﬂange will control the design and the ultimate compressive or tensile strength of the material will not be realized such that the pultruded material will be underutilized (from a strength and therefore economic perspective). In standard steel proﬁles, ﬂange width-to-thickness slenderness ratios are used to ensure that local ﬂange buckling does not occur prior to the material in the ﬂange reaching its yield strength (or its fully plastic moment capacity, known as compact sections in steel ASD terminology) (Salmon and Johnson, 1996). This convenient method is not used in the design of conventional pultruded proﬁles for the following primary reason: Conventional pultruded proﬁles are manufactured in far, far fewer (by two orders of magnitude) sizes than are steel proﬁles. The typical dimensions of these proﬁles in the United States were established in the late 1970s and early 1980s and were controlled by the ﬂexural stiffness, EI, of the section and the need to prevent excessive deﬂections. For this reason, wide-ﬂange proﬁles with thin walls were designed. The designs were also a function of the pultrusion processing technology of that time, which made pultruding shapes with variable crosssectional thickness difﬁcult. For this reason, large-radius ﬁllets at the web and ﬂange junctions were not produced. Although many of these processing obstacles have been overcome in recent years, the manufacturers have a large inventory of pultrusion dies and continue to produce shapes with these existing dies. Some manufactures have attempted to improve the properties of their shapes by using different layups in the ﬂanges and webs of their sections (e.g., SuperStructural sections from Creative Pultrusions). However, in the United States the geometric shapes have not changed much since the 1980s. I-shaped proﬁles currently produced by Fiberline Composites (Denmark) have narrow ﬂanges which in some cases are thicker than the webs, in order to increase the local buckling resistance of the proﬁles. Nevertheless, designers should check all I-shaped sections for local buckling. For this reason, designers of pultruded structures must contend with local buckling and cannot simply choose compact shapes from conventional sections. In addition to the above, it is not really desirable to develop a proﬁle that fails before local buckling of the walls, for the following reasons: 1. Pultruded materials are linear elastic in the roving direction and neither a yield (plastic) moment or a fully plastic moment exist for pultruded proﬁles. This means that postbuckling capacity cannot be developed. It

412

PULTRUDED FLEXURAL MEMBERS

has been demonstrated that when elastic local instability occurs, the proﬁle is very close to its ultimate capacity (Bank et al., 1994b). Therefore, a compact section designation is not applicable. A partially compact designation may be possible (Salmon and Johnson, 1996). 2. The material strength (yield for steel, ultimate for pultruded materials)to-stiffness ratio for typical GFRP pultruded materials is much higher than for steel proﬁles (30/2,600 versus 50/29,000), meaning that the ﬂanges would have to be either very thick or very narrow to prevent local buckling prior to ultimate material failure. This would make the proﬁles difﬁcult to manufacture. To increase the local ﬂange buckling capacity of an I-shaped proﬁle, several details can be used: 1. The ﬂange stiffness can be increased by bonding a higher stiffness plate to the proﬁle. This is the same philosophy as welding a steel cover plate to a steel section (or FRP strengthening of a concrete beam). Care must be taken to ensure that the cover plate does not delaminate from the ﬂange of the proﬁle when subjected to compressive stress (leading to delamination buckling, as it is known). Composite section mechanics can be used to obtain the properties of the built-up section (and builtup web) in this case. 2. The rotational stiffness of the junction can be increased by bonding a small single-leg angle into the ﬁllet region of the proﬁle, as shown in Fig. 13.10. In this case, the mechanics analysis is more complicated and testing is recommended.

Figure 13.10 Details to increase the rotational stiffness of a web–ﬂange junction.

13.7

13.7.3

413

ULTIMATE LIMIT STATES

Local Buckling of Walls Due to In-Plane Shear

The vertical web of an I- or box-shaped proﬁle can buckle in shear at locations of high shear forces that typically occur at concentrated load points or near support locations. The equation for the buckling of an orthotropic plate in pure shear is a function of the restraint provided by the ﬂanges, the aspect ratio, and the orthotropy ratio (EL /ET). Experimental evidence of this buckling mode in conventional pultruded GFRP beams has not been reported in the literature. The critical shear stress for local shear buckling of an orthotropic web is given as 4

local cr ⫽

4 kLT兹DLD3T twd w2

(13.39)

The critical shear force for local web buckling of a homogeneous beam, local V local ⫽ cr cr

Ix tw Qmax

(13.40)

may be approximated for an I-shaped proﬁle as V local ⬇ local Aweb ⫽ local twd cr cr cr

(13.41)

where dw is the depth of the web, d the nominal depth of the proﬁle, tw the thickness of the web, and kLT a shear buckling coefﬁcient given in charts in the Structural Plastics Design Manual (ASCE, 1984, p. 682) or in an approximate closed-form by Kolla´r (2003) as kLT ⫽ 8.125 ⫹ 5.045K

for K ⱕ 1

(13.42)

where K⫽

2DS ⫹ DLT 2GLT (1 ⫺ LT) ⫹ T EL ⫽ 兹DLDT 兹ELET

(13.43)

Kolla´r also presents equations for K ⬎ 1; however, for the orthotropic materials in conventional GFRP pultruded proﬁles, K ⬍ 1, and these equations are not presented here. For isotropic materials, K ⫽ 1. When the beam is subjected simultaneously to high shear forces and high bending moments,17 the web is subjected to combined in-plane shear stress, , and in-plane axial compressive (ﬂexural) stress, z, the critical web buck17

Such as near the interior support of a continuous beam.

414

PULTRUDED FLEXURAL MEMBERS

ling stress may be reduced. The Structural Plastics Design Manual (ASCE, 1984, p. 667) recommends using a second-order interaction equation taken from isotropic plate theory to determine the critical transverse load on the beam, given in terms of stresses as

冉 冊 冉 冊 2

z local cr

⫹

2

local cr

ⱕ 1.0

(13.44)

ⱕ 1.0

(13.45)

or in terms of forces as

冉 冊 冉 冊 Mx M local cr

13.7.4

2

⫹

Vy V local cr

2

Web Crushing and Web Buckling in the Transverse Direction

Webs of pultruded beams are particularly susceptible to local failure at concentrated loads or reactions, due to the relatively low transverse compressive strength and stiffness of the web. This is often referred to as web resistance to transverse forces. Bearing plates at load and reaction points should always be placed directly over (or under) the web of a section and not on outstanding cantilevered ﬂanges. Due to processing, pultruded sections tend to have slightly concave ﬂanges (i.e., ‘‘curled’’ inward) such that load is transferred directly to the web or webs in a concentrated fashion (Mottram, 1991). Local failure and deformation at a roller support of a wide-ﬂange I-section is shown in Fig. 13.11. To design for web crushing18 failure, the critical crushing stress is assumed to be equal to the transverse compressive strength of the material in the web, crush (y)cr ⫽ T,c

(13.46)

and the critical crushing force is Fcrush ⫽ (y)crush Aeff cr cr

(13.47)

In addition to the web being susceptible to crushing at locations of local concentrated forces, the web may also buckle in the vertical plane as if it were a wide but slender column. In this case it is assumed that the web acts as a plate simply supported on its unloaded edges (parallel to the load direction) in the transverse direction with the load applied over an effective width, beff. The equation to predict the critical local buckling stress is the same as 18 This is sometimes referred to as crippling failure. Since the web does not yield prior to the failure in local compression, the term crushing is preferred.

13.7

ULTIMATE LIMIT STATES

415

Figure 13.11 Local bearing failure at a simple support.

that used for the wall simply supported on its two longitudinal edges presented in Eq. (13.20); however, in this case the plate is oriented in the transverse direction of the web. In terms of the effective width (along the beam length), it is written as (y)local ⫽ cr

2 2 (兹DLDT ⫹ DLT ⫹ 2DS) twb2eff

(13.48)

and the critical transverse buckling load is local F local ⫽ (y)cr Aeff cr

(13.49)

In the equations above, beff is taken as the web depth, dw, or the distance between the vertical web stiffeners, for point loads. At simply supported beam ends, beff is taken as equal to the length of bearing plus half the web depth, Leff ⫹ dw /2 (ASCE, 1984, p. 724). 13.7.5 Additional Factors Affecting Local Buckling in Pultruded Proﬁles Since the pultruded material is viscoelastic and will creep, local buckling of the slender walls of a pultruded proﬁle can be affected by reduction in the moduli of the thin walls due to sustained axial (ﬂexural) and shear stresses.

416

PULTRUDED FLEXURAL MEMBERS

Since the ﬂanges are the most highly stressed portions of the proﬁle under ﬂexural loads, where high levels of sustained stresses occur, viscoelastic moduli can be used to determine the critical buckling loads under sustained stresses as a function of time. Since the sustained stress is primarily in the longitudinal direction of the ﬂange, the Structural Plastics Design Manual (ASCE, 1984), following Bleich (1952, p. 343), suggests19 multiplying by 兹E L /EL the critical buckling stress obtained using the instantaneous elastic constants. For example, considering the properties in Table 13.6, after 30 years of sustained load on the ﬂange the critical buckling stress would be 79% of the instantaneous buckling stress calculated (i.e., 兹1.62/2.6 ⫽ 0.79). Local buckling may also be inﬂuenced by shear deformation effects in the same manner as shear deformation affects global deformation. A higher-order shear-deformable plate theory is required to evaluate such phenomena; however, they are expected to be small in conventional GFRP pultruded proﬁles since the effect of shear deformation on global buckling of pultruded proﬁles has been shown to be small (less than 5% in most cases) (Roberts, 2002). Shear lag in very wide ﬂanges of I-shaped and rectangular box proﬁles may reduce the axial stress and increase the in-plane shear stress carried by the ﬂanges of the proﬁle in bending. This is not expected to be a signiﬁcant source of error in the design of conventional pultruded GFRP proﬁles. In experiments on beams, very little change in the axial strain across the width of the ﬂanges has been observed. In some situations, coupling between local wall buckling and global lateral–torsional buckling of I-shaped proﬁles, referred to as distortional buckling, may occur (Davalos and Qiao, 1999) in a similar fashion to that of steel I-shaped sections (Hancock, 1978). Design guidance is not provided for this coupled buckling mode, as most conventional pultruded beams will be braced against lateral–torsional buckling, and therefore local buckling criteria will govern. Web Stiffeners Vertical web stiffeners can be used to increase the critical buckling stress in a web for in-plane shear stresses, in-plane ﬂexural (compressive) stresses, and transverse compression stresses at supports and load points. Based on isotropic material assumptions, the Structural Plastics Design Manual (ASCE, 1984) recommends that the minimum ﬂexural rigidity, (EI)stiffener of a vertical web stiffener about the plane of the web be taken as (EI)stiffener ⫽ 0.34

(EL)sdw4 t w3 b3s

(13.50)

19 Note that Eq. 6.73 in the SPDM is not correct, as it will lead not to smaller buckling loads, as would be expected, but to larger loads, due to viscoelastic effects.

13.7

ULTIMATE LIMIT STATES

417

where bs is the spacing of the stiffeners along the length of the beam and (EL)s is the longitudinal modulus of the stiffener in the vertical direction, which must be equal to or larger than the longitudinal modulus of the pultruded material in the web, (EL)w. Single-leg angles and small square tubes are commonly used as web stiffeners. They should be bonded or bolted to the web and extended to the compression ﬂange of the section wherever possible (see Chapter 15 for a detailed discussion of connection issues). Bearing Stiffeners At the location of concentrated loads and vertical supports, bearing stiffeners should be used to stabilize the section and distribute the loads into the proﬁle at the location of the loads. Without such stiffeners, severe local deformation can occur at locations of concentrated loads (see the support point in Fig. 13.6). These stiffeners should bear on the inside surface of the loaded ﬂange and on the inside surface of the opposite ﬂange. If possible, they should also be attached to the web of the section. In I-shaped proﬁles, bearing stiffeners should be placed symmetrically on both sides of the web. Figure 13.12 shows vertical bearing stiffeners of this type at a simple support. Vertical bearing stiffeners can be designed as pinned–pinned columns with height dw, subjected to one-half the applied load at the point, according to the procedures detailed in Chapter 14. 13.7.6

Flange and Web Longitudinal Material Failure

For pultruded proﬁles where the slenderness ratio of the ﬂange, 0.5bƒ /tƒ, and the slenderness ratio of the web, dw /tw, are small and local buckling does not

Figure 13.12 Vertical bearing stiffeners at a simple support.

418

PULTRUDED FLEXURAL MEMBERS

occur (or is prevented by multiple longitudinal and transverse stiffeners), the ﬂexural member may fail due to compressive crushing or tensile rupture of the pultruded material due to ﬂexural stresses. To design for ﬂange or web material compressive failure, the critical compressive stress is taken as the longitudinal ultimate compressive strength of the pultruded material in the web or the ﬂange, comp ⫽ L,c cr

(13.51)

The critical bending moment for a homogeneous proﬁle due to compressive material failure is M comp ⫽ comp cr cr

Ix y

(13.52)

where y is the distance to the point of interest from the neutral axis. To design for ﬂange or web material tensile failure, the critical tensile stress is taken as the longitudinal ultimate tensile strength of the pultruded material in the web or the ﬂange, ten cr ⫽ L,t

(13.53)

The critical bending moment for a homogeneous proﬁle due tensile material failure is ten M ten cr ⫽ cr

Ix y

(13.54)

where y is the distance to the point of interest from the neutral axis. 13.7.7

Flange and Web Material Shear Failure

To design for ﬂange or web material in-plane shear failure, the critical shear stress in the ﬂanges and webs of a pultruded proﬁle is taken as the ultimate in-plane shear strength of the pultruded material: shear ⫽ LT cr

(13.55)

The critical shear force for a homogeneous proﬁle due to web material failure is

13.8

DESIGN PROCEDURE FOR FLEXURAL MEMBERS

local local V cr ⫽ cr

Ix t ⬇ local Aweb cr Q

419

(13.56)

where t is the thickness of the ﬂange or web at the point of interest and Q is the ﬁrst moment of area at the point of interest. Manufacturers often do not report the in-plane shear strength of pultruded proﬁles. However, they usually report the out-of-plane (or interlaminar) shear strength, TT. If necessary, the out-of-plane shear strength can be used in place of the in-plane shear strength, although this will lead to overly conservative designs for conventional pultruded proﬁles. Unlike in the case of buckling stresses, interaction between in-plane normal stresses and shear stresses is not generally considered for pultruded proﬁles. Since the maximum stress failure criterion20 is typically used to determine material failure in pultruded materials, no interaction is assumed between the effects of normal and shear stress on material failure, and each condition is considered separately. More sophisticated interactive failure criteria, such as the Tsai-Wu and Tsai-Halpin criteria, are seldom, if ever, used in the design of pultruded proﬁles. In addition, the principal stresses are not calculated. Since the material is orthotropic, the value of the principal normal and maximum shear stresses at a point are not particularly relevant. In orthotropic materials, the stresses parallel and perpendicular to the major axes of orthotropy are those that control in design. 13.8

DESIGN PROCEDURE FOR FLEXURAL MEMBERS

The design procedure presented here for ﬂexural members permits design by the allowable stress design (ASD) basis or the load and resistance factor design (LRFD) basis, as discussed in Chapter 12. Both of these bases use the analytical, mechanics-based equations presented in preceding sections. They do not use the empirical equations presented in the U.S. pultrusion manufacturers’ design guides mentioned in Chapter 12. Consequently, the load tables presented in manufacturers’ design guides are not used in this book to size conventional pultruded proﬁles. However, the empirical equations presented in the guides, and hence the load tables, can be used to estimate the size or the proﬁle, or its load-carrying capacity, if necessary for the purposes of a preliminary design. Step 1. Determine the design loads, choose the design basis, and determine the basis factors. The distributed and concentrated loads on ﬂexural members and their types are determined from the structural geometry and load20

Discussed in Chapter 3.

420

PULTRUDED FLEXURAL MEMBERS

ing requirements. The support conditions for the beam are established. The design basis for the ﬂexural member is chosen and the appropriate safety factors (ASD) and resistance factors (LRFD) are determined. Load factors for the LRFD method are listed. Maximum short- and long-term deﬂection criteria are taken from codes or established by the project speciﬁcations. Step 2. Select a proﬁle type and select a trial size for serviceability. Using the maximum allowable deﬂection criteria, select a proﬁle and size to meet this criterion (for the short and long terms). Neglect shear deformation for the ﬁrst trial. Check the chosen trial proﬁle and size with the shear deformation included. Service loads are used for both the ASD and LRFD procedures. Step 3. Determine the maximum design stresses or forces. The maximum ﬂexural, shear, and bearing stresses on a member subjected to the nominal loads are calculated for the ASD procedure. The maximum bending moment, shear force, and reactions on the member subjected to the factored loads are calculated for the LRFD procedure. Step 4. Determine the critical stresses or forces. For the proﬁle chosen, determine (or calculate) the lateral–torsional buckling, local buckling (normal and shear), web buckling, web crippling, compressive strength, tensile strength, and shear strength critical stresses (ASD) or forces (LRFD). Step 5. Determine the factored critical stresses or forces. For ASD, divide the critical stresses determined in step 4 by the appropriate safety factors for ﬂexural, compressive, or tensile stresses. For LRFD, multiply the critical forces by the appropriate resistance factors for ﬂexural members. Step 6. Check the ultimate strength or capacity of the proﬁle selected. For ASD, check that the design stresses are less than the allowable stresses. For LRFD, check that the factored design forces are less than the factored resistances. Return to step 3 if the trail size does not work. Step 7. Dimension the ancillary bracing, stiffeners, and bearing plates. Dimension (or design if quantitative procedures are available) braces, stiffeners, and bearing plates for the ﬂexural member. Provide a sketch of the beam showing all ancillary elements, dimensions, and important construction notes. (If the beam is connected to other framing members, the connection should be dimensioned and detailed following the design procedure described in Chapter 15.) Design Example 13.4: Pultruded Beam Design A conventional commercially produced pultruded E-glass/vinylester wide-ﬂange I-shaped proﬁle is to be used as a simply supported interior ﬂoor beam of a building structure with a typical repeating ﬂoor plan as shown in Fig. 13.13. Pultruded gratings attached with grating clips are to be used as the ﬂooring system. Assume that the ﬂooring system does not provide any restraint against global lateral– torsional buckling or local compression ﬂange buckling. The ﬂoor dead load is 20 psf and the ﬂoor live load is 40 psf. Live load reduction is not permitted.

13.8

DESIGN PROCEDURE FOR FLEXURAL MEMBERS

421

15 ft

6 ft

6 ft

Figure 13.13 Typical repeating ﬂoor plan.

TABLE 13.7

Pultruded Material Properties in Flange and Web

Symbol EcL EtL EcT EtT GLT L L,c L,t T,c T,t TT LT Eb Gb a

NR, not reported.

Description

Valuea

Longitudinal compressive modulus Longitudinal tensile modulus Transverse compressive modulus Transverse tensile modulus In-plane shear modulus Major (longitudinal) Poisson ratio Longitudinal compressive strength Longitudinal tensile strength Transverse compressive strength Transverse tensile strength Interlaminar shear strength In-plane shear strength Full-section ﬂexural modulus Full-section shear modulus

2.6 ⫻106 psi 2.6 ⫻106 psi 1.0 ⫻106 psi 0.8 ⫻106 psi NR 0.33 30,000 psi 30,000 psi 16,000 psi 7,000 psi 4,500 psi NR 2.5 ⫻106 psi 0.425 ⫻106 psi

422

PULTRUDED FLEXURAL MEMBERS

The beams are to be designed for a maximum short-term deﬂection of L/240. The beams are loaded on their top ﬂanges and are connected to the columns with web clip angles21 (simple shear connections). The material properties for a conventional pultruded glass FRP proﬁle taken from a manufacturer design guide (e.g., Strongwell, Bedford) are listed in Table 13.7. SOLUTION Step 1. Determine the design loads, choose the design basis, and determine the basis factors. Design loads and internal forces For the given tributary width of a typical beam of 6 ft, the beam loads are calculated as follows. For ASD and LRFD serviceability limit state calculations: Dead load:

wDL ⫽ (20 psf ⫻ 6 ft) ⫹ 10 lb/ft ⫽ 130 lb/ft (assuming a beam self-weight of 10 lb/ft)

Live load: Total service load:

wLL ⫽ (40 psf ⫻ 6 ft) ⫽ 240 lb/ft 130 ⫹ 240 ⫽ 370 lb/ft

For LRFD design the ASCE 7 load factors for dead and live loads are 1.2 and 1.6, respectively, and the factored loads are Dead load:

WD ⫽ 1.2(130) ⫽ 156 lb/ft

Live load:

WL ⫽ 1.6(240) ⫽ 384 lb/ft

Total factored load:

Wu ⫽ 156 ⫹ 384 ⫽ 540 lb/ft

ASD and LRFD factors The ASD safety factors to be used are taken from Chapter 12: flexure ⫽ 2.5 compression ⫽ 3.0 shear ⫽ 3.0 The LRFD resistance factors are determined using the Eurocomp material factors (Chapter 12), as follows:

21 The design of the columns and clip angle connections are treated in Chapters 14 and 15, respectively.

13.8

DESIGN PROCEDURE FOR FLEXURAL MEMBERS

423

␥m,1 ⫽ 1.15 (material properties obtained from test data) ␥m,2 ⫽ 1.1 (fully cured pultruded material) ␥m,3 ⫽ 1.0 (Tg ⬎ 80⬚ and room-temperature service conditions)

No other environmental or long-term reduction factors are assumed for this problem. Therefore, ␥m ⫽ ␥m,1␥m,s␥m,3 ⫽ 1.15(1.1)(1.0) ⫽ 1.265 ⱕ 1.5

Therefore, ␥m ⫽ 1.5 (minimum value permitted by Eurocomp for ultimate limit state). The LRFD resistance factor is taken as the inverse of the Eurocomp material factor:

⫽

1 1 ⫽ ⫽ 0.67 ␥m 1.5

For the serviceability limit state, the material factor is taken as 1.0 and the resistance factor is therefore also 1.0. Step 2. Select a proﬁle type and select a trial size for serviceability. The maximum allowable midspan deﬂection of the beam is

␦max ⫽

L 15 ⫻ 12 ⫽ ⫽ 0.75 in. 240 240

The minimum required second moment of the section to limit the deﬂection to this is

Ireqd ⫽

5 wL4 5 (370/12)(15 ⫻ 12)4 ⫽ ⫽ 216.13 in4 384 E␦max 384 (2.6 ⫻ 106)(0.75)

Using U.S. manufacturers’ conventional wide-ﬂange proﬁles, choose a W 10 ⫻ 10 ⫻ –12 proﬁle with the geometric properties given in Table 13.8.

424

PULTRUDED FLEXURAL MEMBERS

TABLE 13.8 Geometric Properties of Conventional Glass FRP W 10 ⴛ 10 ⴛ –12 Proﬁle Symbol Ix Iy Sx Az J tw tƒ d dw b bƒ w

Description

Value

Second moment about major axis Second moment about minor axis Major axis section modulus Area Torsional constant Web thickness Flange thickness Nominal section depth Web depth Nominal section width (breadth) Flange width (breadth) Nominal weight

256.20 in4 83.42 in4 51.20 in3 14.55 in2 1.208 in4 0.5 in 0.5 in 10 in 9.5 in 10 in 10 in 11.64 lb / ft

Recalculate design loads with actual beam weight. For ASD and LRFD serviceability limit state calculations, Dead load:

wDL ⫽ (20 psf ⫻ 6 ft) ⫹ 11.64 lb/ft ⫽ 131.64 lb/ft 艑 132 lb/ft

Live load: Total service load:

wLL ⫽ (40 psf ⫻ 6 ft) ⫽ 240 lb/ft 140 ⫹ 240 ⫽ 372 lb/ft

For LRFD design the ASCE 7 load factors for dead and live loads are 1.2 and 1.6, respectively, and the factored loads are Dead load:

WD ⫽ 1.2(131.64) ⫽ 157.97 lb/ft ⯝ 158 lb/ft

Live load:

WL ⫽ 1.6(240) ⫽ 384 lb/ft

Total factored load:

Wu ⫽ 158 ⫹ 384 ⫽ 542 lb/ft

Determine the actual deﬂection for the proﬁle chosen using shear deformation beam theory. KAG ⫽ ktim AGLT ⫽ 0.413(14.55)(0.425 ⫻ 106) ⫽ 2.55 ⫻ 106 lb Note that the value of GLT is taken as the full-section shear modulus Gb since the in-plane shear modulus is not reported by the manufacturer.

13.8

DESIGN PROCEDURE FOR FLEXURAL MEMBERS

425

EI ⫽ ELIx ⫽ (2.6 ⫻ 106)(256.2) ⫽ 666.12 ⫻ 106 lb–in2 Note that the longitudinal modulus of the ﬂange, EL, is used in this calculation. If the full-section ﬂexural modulus, Eb, is used, a more conservative (i.e., larger deﬂection) prediction is obtained. The full-section ﬂexural modulus is a value that may already include the effects of shear deformation, depending on how the test was conducted (not reported by the manufacturer). ␦max ⫽

5wL4 wL2 5(372/12)(15 ⫻ 12)4 (372/12)(15 ⫻ 12)2 ⫹ ⫽ ⫹ 384EI 8KAG 384(666.12 ⫻ 106) 8(2.55 ⫻ 106)

⫽ 0.64 ⫹ 0.05 ⫽ 0.69 in. ⬍ 0.75 in.

OK

(Note that the shear deﬂection is only 7% of the total deﬂection for this relatively long pultruded beam. For shorter beams, the shear deﬂection will be a higher percentage of the total deﬂection.) Step 3. Determine the maximum design stresses or forces. The maximum design service load moment, shear force, and stresses are mmax ⫽

wL2 372(15)2 ⫽ ⫽ 10,462.5 ft-lb 8 8

max ⫽

mmax 10,462.5(12) ⫽ ⫽ 2452 psi Sx 51.20

y ⫽

w 372/12 ⫽ tw 0.5

⫽ 62.0 psi (transverse stress in the web due to the distributed load)

vmax ⫽

wL 372(15) ⫽ ⫽ 2790 lb 2 2

max ⫽

vmax

Aw

⫽

2790 ⫽ 558 psi (10)(0.5)

The maximum design ultimate bending moment, shear force, and transverse force are

426

PULTRUDED FLEXURAL MEMBERS

Mmax ⫽

WuL2 542(15)2 ⫽ ⫽ 15,243.8 ft-lb 8 8

Vmax ⫽

WuL 542(15) ⫽ ⫽ 4065 lb 2 2

Fy,max ⫽ Wud ⫽ 542(10/12) ⫽ 451.7 lb (transverse force on web acting over Leff ⫽ d)

Step 4. Determine the critical stresses and forces. Global lateral–torsional buckling For the simply supported uniformly loaded beam the moment coefﬁcient Cb ⫽ 1.13 and the end-restraint coefﬁcients kƒ and k ⫽ 1.0. The warping constant is C ⫽

Iyd 2 83.4(10)2 ⫽ ⫽ 2086 in6 4 4

and the critical lateral torsional buckling stress is lat cr ⫽

⫽

Cb Sx

冪

1.13 51.2

2ELIyGLT J 4E L2 IyC ⫹ (kƒ Lb)2 (kƒ Lb)2(k Lb)2

冪

2(2.6 ⫻ 106)(83.42)(0.425 ⫻ 106)(1.208) (1.0 ⫻ 15 ⫻ 12)2 ⫹

4(2.6 ⫻ 106)2(83.42)(2,085) (1.0 ⫻ 15⫻12)2(1.0 ⫻ 15 ⫻ 12)2

⫽ 8348 psi

The critical lateral–torsional bending moment is lat M lat cr ⫽ cr Sx ⫽ 8348(51.2) ⫽ 427,418 lb-in. ⫽ 35,618 lb-ft

Local buckling Calculate the plate minor (transverse) Poisson ratio: T ⫽

E cT 1.0 L ⫽ (0.33) ⫽ 0.13 c EL 2.6

Calculate the plate ﬂexural rigidities:

13.8

DESIGN PROCEDURE FOR FLEXURAL MEMBERS

DL ⫽

E cLt 3p (2.6 ⫻ 106)(0.5)3 ⫽ ⫽ 28,297 lb-in. 12(1 ⫺ LT) 12(1 ⫺ (0.33)(0.13))

DT ⫽

E cT 1.0 DL ⫽ (28,297) ⫽ 10,883 lb-in. c EL 2.6

427

DLT ⫽ T DL ⫽ 0.13(28,297) ⫽ 3679 lb-in. DS ⫽

GLT t 3p (0.425 ⫻ 106)(0.5)3 ⫽ ⫽ 4227 lb-in. 12 12

Calculate the buckling stresses for the simply supported ﬂange and web to determine which wall buckles ﬁrst: ( ss free)ƒ ⫽

( ss ss)w ⫽ ⫽

4t 2ƒ 4(0.5)2(0.425 ⫻ 106) GLT ⫽ ⫽ 4250 psi 2 bƒ (10)2

2 (13.9兹DLDT ⫹ 11.1DLT ⫹ 22.2DS) twd 2w 2 [13.9兹(28,297)(10,883) ⫹ 1.11(3679) ⫹ 22.2(4427)] 0.5(9.5)2

⫽ 83,778 psi

Since the longitudinal compressive modulus in the ﬂange and the web are the ss same, the ﬂange buckles ﬁrst, since ( ss free)ƒ /(EL)ƒ ⬍ ( ss)w /(EL)w, or 4250 ⬍ 83,655 psi. Now calculate the local buckling stress for the ﬂange. First calculate the junction stiffness, k, and then the coefﬁcient of restraint, . kI-flange ⫽

冋

册

冉

⫽ 2174.9 lb

I-flange ⫽

DT kI-flangeLT

⫽

10,883 2174.9(10/2)

⫽ 1.001 (nondimensional coefficient of restraint)

and

冊

( ss 2(DT)w 2(10,883) 4250 free)ƒ(EL)w 1⫺ ⫽ 1⫺ ss dw ( ss )w(EL)ƒ 9.5 83,655

428

PULTRUDED FLEXURAL MEMBERS

local,I-flange ⫽ cr

⫽

冉冪 冋冪

冊

1 DLDT 7 ⫹ 12DS (bƒ /2)2tƒ 1 ⫹ 4.12I-flange

册

1 28,297(10,883) 7 ⫹ 12(4427) (10/2)2(0.5) 1 ⫹ 4.12(1.001)

⫽ 8591.3 psi

The length of the buckle half-wavelength (for information purposes) is

冪

bƒ D aI-flange ⫽ 1.675 4 L(1 ⫹ 4.12I-flange) 2 DT

冉 冊冪

⫽ 1.675

10 2

4

28,297 [1 ⫹ 4.12(1.001)] ⫽ 16.0 in. 10,883

The critical bending moment at which local ﬂange buckling occurs is local,I-flange M local,I-flange ⫽ cr Sx ⫽ cr

8591.3(51.2) ⫽ 36,656.2 lb-ft 12

Local web shear buckling. To calculate the critical shear stress for local in-plane shear buckling of the web, the shear buckling coefﬁcient, kLT, is ﬁrst found as a function of the shear anisotropy ratio, K. K⫽

2(4427) ⫹ 3679 2DS ⫹ DLT ⫽ ⫽ 0.714 ⬍ 1.0 兹DLDT 兹(28,297)(10,883)

OK

kLT ⫽ 8.125 ⫹ 5.045K ⫽ 8.125 ⫹ 5.045(0.714) ⫽ 11.727 4

local ⫽ cr

4

4 kLT 兹DLDT3 4(11.728)兹28,297(10,883)3 ⫽ ⫽ 14,365.7 psi twd w2 0.5(9.5)2

The critical in-plane web shear force is local V local ⬇ local Aweb ⫽ cr tw d ⫽ 14,365.7(0.5)(10) ⫽ 71,829 lb cr cr

Local transverse web buckling The effective web width, beff, that resists the distributed load as a ‘‘column’’ is equal to the depth of the web, dw, for a distributed load applied to the top ﬂange of the section. The critical transverse buckling stress is

13.8

(y)local ⫽ cr ⫽

DESIGN PROCEDURE FOR FLEXURAL MEMBERS

429

2 2 (兹DLDT ⫹ DLT ⫹ 2DS) twb2eff 2 2 [兹28,297(10,883) ⫹ 3679 ⫹ 2(4427)] ⫽ 13,159 psi 0.5(9.5)2

The critical transverse buckling load is local F local ⫽ (y)cr Aeff ⫽ 13,159(9.5)(0.5) ⫽ 62,505 lb cr

Tensile, compressive, and shear material failure Using the material tensile, compressive, and shear strengths, the critical bending, shear, and transverse resistances are obtained as M comp ⫽ comp cr cr tens M tens cr ⫽ cr

Ix 256.2 ⫽ (30,000) ⫽ 1,537,200 in.-lb ⫽ 128,100 ft-lb y 5

Ix 256.2 ⫽ (30,000) ⫽ 1,537,200 in.-lb ⫽ 128,100 ft-lb y 5

V local ⫽ local Aweb ⫽ 4500(0.5)(10) ⫽ 22,500 lb cr cr F crush ⫽ (y)crush Aeff ⫽ 16000(0.5)(9.5) ⫽ 76,000 lb cr cr Step 5. Determine the factored critical stresses or forces. The critical stresses and loads are summarized in Table 13.9. Using the ASD safety factors and the LRFD resistance determined in step 1, the allowable stresses for ASD and the member resistances for LRFD are tabulated in Table 13.9. Step 6. Check the ultimate strength or capacity of the proﬁle selected. For the ultimate limit state, the design stress and forces are compared to the allowable stresses and member resistances in Table 13.10. For the serviceability limit state, the maximum midspan deﬂection is compared with the prescribed allowable deﬂection limit of L/240 for both the ASD and LRFD bases. Based on the comparisons shown, it is seen that the W 10 ⫻ 10 ⫻ –12 conventional pultruded proﬁle meets the design demands. The controlling critical ultimate limit state is lateral-torsional buckling for this beam. However, the design is actually controlled by the serviceability limit state. This can be seen by comparing the ratio of design deﬂection to the allowable deﬂection limit (0.684/0.75 ⫽ 91%) to that of the ﬂexural stress to the critical buckling stresses ratio (2452/3339 ⫽ 73%). However, it is also observed that these two efﬁciency ratios are reasonable high (⬃75% or more) and that the section is reasonably well optimized for both the ULS and the SLS.

430

PULTRUDED FLEXURAL MEMBERS

TABLE 13.9 Critical Stress, ASD Design Stresses and Loads, and LRFD Design Resistances Mode Lateral– torsional buckling Local buckling (ﬂange controls) Flange tensile failure Flange compressive failure Web transverse buckling Web transverse crushing Web shear buckling Web shear failure

cr

SF

allow

Rcr

a

Rcr

8,348 psi

2.5

3,339 psi

35,618 ft-lb

0.67

23,864 ft-lb

8,591 psi

2.5

3,436 psi

36,656 ft-lb

0.67

24,560 ft-lb

30,000 psi

2.5

12,000 psi

128,100 ft-lb

0.67

85,827 ft-lb

30,000 psi

2.5

12,000 psi

128,100 ft-lb

0.67

85,827 ft-lb

13,159 psi

3.0b

4,380 psi

62,505 lb

0.67

41,878 lb

16,000 psi

3.0b

5,333 psi

76,000 lb

0.67

50,920 lb

14,366 psi

3.0

4,772 psi

71,829 lb

0.67

48,125 lb

4,500 psi

3.0

1,500 psi

22,500 lb

0.67

15,075 lb

a According to the Eurocomp partial factor method, different ultimate modes of failure (e.g., ﬂexure, compression) are not treated independently as in a traditional LRFD or ASD approach. b The web is considered to be a slender column and the SF for compressive stress is used.

PROBLEMS 13.1

Using the Timoshenko beam theory, derive the expressions for the bending and shear deﬂections [ƒ1(z) and ƒ2(z)] for a simply supported beam with a span, ᐉ, having a concentrated load, P, at its midspan. Provide the expression for the midspan deﬂection. Check your result with the expressions in Table 13.1, line 2.

13.2

Using the Timoshenko beam theory, derive the expressions for the bending and shear deﬂections [ƒ1(z) and ƒ2(z)] for a simply supported beam with a span, ᐉ, and having concentrated loads, P, at its quarter points. Provide the expression for the midspan deﬂection and for the deﬂection under one of the load points. Compare your result with those published in the literature for this case.

13.3

Using the Timoshenko beam theory, determine the reactions and draw the shear force and bending moment diagrams for a uniformly loaded,

PROBLEMS

TABLE 13.10 and LRFD Mode

431

Comparison of Design Demands with Permitted Values for ASD design

Ultimate limit state Lateral torsional 2,452 buckling Local buckling 2,452 (ﬂange) Flange tensile 2,452 failure 2,452 Flange compressive failure Web transverse 62 buckling Web transverse 62 crushing Web shear 558 buckling Web shear failure 558

vs.

allow

Rdesign

vs.

Rcr

psi

⬍

3,339 psi

15,244 ft-lb

⬍ 23,864 ft-lb

psi

⬍

3,436 psi

15,244 ft-lb

⬍ 24,560 ft-lb

psi

⬍ 12,000 psi

15,244 ft-lb

⬍ 85,827 ft-lb

psi

⬍ 12,000 psi

15,244 ft-lb

⬍ 85,827 ft-lb

psi

⬍

4,380 psi

452 lb

⬍ 41,878 lb

psi

⬍

5,333 psi

452 lb

⬍ 50,920 lb

psi

⬍

4,772 psi

4,065 lb

⬍ 48,125 lb

psi

⬍

1,500 psi

4,065 lb

⬍ 15,075 lb

⬍

0.75 in.

Serviceability limit state Midspan 0.684 in. deﬂection

0.684 in.

⬍

0.75 in.

w, continuous beam on three simple (pinned) supports having two equal spans of length, ᐉ. Determine an expression for the maximum deﬂection of the beam. (To aid you in your solution, you can assume that the maximum deﬂection occurs at approximately the same location in the span as in an Euler–Bernoulli beam.) Compare the maximum negative moment obtained at the middle support with that of an Euler–Bernoulli beam for E/G ratios of 2.6 (isotropic material), 5, 10, 15, and 20. Assume that K ⫽ 1 and A ⫽ 0.1I. [Hint: Use the force method (method of consistent deformations).] 13.4

Analyze the two-span continuous Timoshenko beam in Problem 13.3 using a commercial structural analysis computer program using beam elements that permit the inclusion of shear deformation effects. Choose appropriate values of I, A, w, ᐉ, E and G for your numerical computations in order to compare your results with your closed-form solutions developed in Problem 13.3.

13.5

For proﬁles a to e from U.S. manufacturers (Strongwell, Creative Pultrusions, and Bedford Reinforced Plastics) and proﬁles ƒ to h from

432

PULTRUDED FLEXURAL MEMBERS

European manufacturers (Fiberline or TopGlass) listed in Table P13.5,22 determine the Timosheko shear coefﬁcient, ktim, using the equations listed in Table 13.2. For nonhomogeneous proﬁles from Creative Pultrusions, use average values of the mechanical properties in the webs and ﬂanges of the sections. For I sections, assume bending about the major axis. 13.6

For proﬁles a to e from U.S. manufacturers (Strongwell, Creative Pultrusions, and Bedford Reinforced Plastics) and proﬁles ƒ to h from European manufacturers (Fiberline or TopGlass) listed in Table P13.5, determine the ﬂexural rigidity, EI, and the shear rigidity, KAG, for bending about the major axis. Calculate the shear rigidity using the ktim AGLT and the AwebGLT(web) methods and compare the results. For nonhomogeneous proﬁles, use the transformed section method or the composite mechanics method to determine EI. For nonhomogeneous proﬁles, use average values of the properties in the webs and ﬂanges of the sections to calculate the shear rigidity KAG when using the Timoshenko shear coefﬁcient. [For a more rigorous treatment of the problem of shear deﬂection in nonhomogeneous proﬁles using the Timosheko beam theory, see Bank (1987).]

13.7

A 10 ⫻ 5 ⫻ –12 glass–polyester narrow-ﬂange I section (proﬁle b in Table P13.5) produced by Strongwell is used as a simply supported beam and spans 9 ft. The beam has a nominal self-weight of 4.61 lb/ ft. It is loaded with a uniformly distributed sustained dead load of 100 lb/ft and a live load of 200 lb/ft. Determine the instantaneous midspan deﬂection and the midspan deﬂection after 25 years of sustained load on the beam under the self-weight, sustained dead load, and the live load.

TABLE P13.5 a b c d e ƒ g h

Pultruded Proﬁles

Glass–polyester 8 ⫻ 8 ⫻ –38 (d ⫻ b ⫻ t) in. wide-ﬂange I-shaped section Glass–polyester 10 ⫻ 5 ⫻ –12 (d ⫻ b ⫻ t) in. narrow-ﬂange I-shaped section Glass–vinylester 6 ⫻ 6 ⫻ –14 (d ⫻ b ⫻ t) in. wide-ﬂange I-shaped section Glass–vinylester 6 ⫻ –38 (b ⫻ t) in. square tube Glass-polyester 3 ⫻ –38 (b ⫻ t) in. square tube Glass–vinylester 200 ⫻ 100 ⫻ 10 (d ⫻ b ⫻ t) mm narrow-ﬂange I-shaped section Glass–vinylester 300 ⫻ 8 ⫻ 150 ⫻ 12 (d ⫻ tw ⫻ bƒ ⫻ tƒ) mm narrow-ﬂange I-shaped section Glass–vinylester 120 ⫻ 8 (b ⫻ t) mm square tube

22 Instructors may assign only selected beams or may choose other singly symmetric sections from manufacturer design guides.

PROBLEMS

433

13.8

Solve Problem 13.7 using the Creative Pultrusions 10 ⫻ 5 ⫻ –12 nonhomogeneous section. Compare the results with those obtained in Problem 13.7.

13.9

Determine the critical lateral torsional buckling stress for the I-shaped pultruded proﬁles a, b, and c (U.S. manufacturers’ properties23) and proﬁles ƒ and g (European manufacturers’ properties24) in Table P13.5 when loaded by a uniformly distributed load over a 12-ft unbraced simply supported span. What is the maximum nominal (no ASD or LRFD factors) uniformly distributed load that can be placed on the beam based on the critical lateral torsional buckling stress of the chosen beam?

13.10 Determine the critical local buckling stress, critical bending moment, and length of the buckle half-wavelength, a, for the I-shaped pultruded proﬁles a, b, and c (U.S. manufacturers’ properties25) and proﬁles ƒ and g (European manufacturers’ properties) in Table P13.5 when loaded in ﬂexure. 13.11 Calculate the critical local buckling stress for the I-shaped beams in Problem 13.10 using the approximate equations [equation (13.37)] suggested by the Structural Plastics Design Manual. Compare these predictions with those obtained in Problem 13.10 using the exact method. 13.12 Determine the critical local buckling stress, critical bending moment, and length of the buckle half-wavelength, a, for square-tube proﬁles d and e (U.S. manufacturer properties) and proﬁle h (European manufacturers’ properties) in Table P13.5 when loaded in ﬂexure. 13.13 Determine the critical local buckling stress, critical bending moment, and length of the buckle half-wavelength, a, for a Strongwell 9 ⫻ 6 5 ⫻ –– 16 (d ⫻ b ⫻ t) in. rectangular-tube beam when loaded in bending about (a) its major axis and (b) its minor axis. 13.14 Determine the critical web in-plane shear buckling stress and the critical shear force for proﬁles a and c (U.S. manufacturers) and proﬁles g and h (European manufacturers) in Table P13.5. 13.15 Consider a 24 ⫻ 3 ⫻ 0.25 (d ⫻ bƒ ⫻ t) in. glass–vinylester channel section with material properties given in Table 13.7. Determine (a) the critical web in-plane shear buckling stress and (b) the critical local in-plane buckling load when the beam is bent about its major axis and loaded through its shear center. To determine the local ﬂange 23

Use nonhomogeneous materials properties for Creative Pultrusions’ beams when appropriate. If available. 25 Use nonhomogeneous materials properties for Creative Pultrusions’ beams when appropriate. 24

434

PULTRUDED FLEXURAL MEMBERS

buckling stress for the channel, the formula for an I-shaped section is used with two modiﬁcations: (1) the channel ﬂange width, bƒ (3 in. for this case), is used in place of bƒ /2 in the buckling stress equation for the I-shaped section [equation (13.26)], and (2) the expression for k [equation (13.25)] is multiplied by 2 since the web restrains only one ﬂange (Kolla´r, 2003). 13.16 Consider a built-up section of two of the channels in Problem 13.15 used back to back to form a deep I-section with dimensions of 12 ⫻ –12 ⫻ 6 ⫻ –14 (d ⫻ tw ⫻ b ⫻ tƒ) inches. (Assume that the channel webs are fully bonded to each other back to back and act as a single –12 -in.thick wall.) The beam is to be used as a simply supported beam loaded by a concentrated load at midspan (applied at the beam centroidal axis) over a 14-ft-long span. Determine the (a) critical lateral torsional buckling stress, (b) critical in-plane buckling stress, and (c) critical web shear buckling stress for this built-up section. Assume that the section behaves as an I-shaped section for the purposes of calculating in-plane buckling of the web and ﬂanges and shear buckling of the web. 13.17 Determine the maximum concentrated load, P, that can be applied to the top ﬂange (directly above the web) of a 12 ⫻ 6 ⫻ –12 Strongwell glass–vinylester pultruded I-shaped section when the load is controlled by (a) local web compression buckling or (b) local web compression crushing. The concentrated load is applied over a bearing length (lengthwise along the beam axis) of 3 in. Vertical web plate stiffeners are placed 6 in. apart on either side of the load point on both sides of the web. 13.18 Determine the maximum reaction (or shear force at the beam end), R, that can be carried by a creative pultrusions 6 ⫻ –38 glass–vinylester square tube when used as a simply supported beam. The beam is seated on a support having a 4-in. width. A pultruded material bearing plate –38 in. thick is placed between the support and the beam. 13.19 Redesign the beam in Design Example 13.4 using a vinylester wideﬂange I-shaped proﬁle from the Creative Pultrusions SuperStructural series. Design the beam using (a) the ASD basis and (b) the LRFD basis. Compare the section selected to that published in Creative Pultrusions’ design guide, ‘‘Allowable Uniform Load Tables,’’ for the loading given. 13.20 Consider a 12 ⫻ 6 ⫻ –12 in. Strongwell glass–vinylester narrow-ﬂange I-shaped section for the beam in Design Example 13.4 and determine if it will be an adequate section to carry the design loads. 13.21 Consider the ﬂoor plan shown in Fig. 13.13 and assume that this represents the plan for a single-story structure. To decrease deﬂec-

PROBLEMS

435

tions, 30-ft-long pultruded beams that are continuous over the columns spaced at 15 ft on center are suggested in place of the 15-ft-long beams considered in Design Example 13.4. Design the 30-ft-long continuous pultruded beams using the material properties given in Table 13.7. Design using (a) the ASD basis and (b) the LRFD basis. [Note: Include effects of shear deformation in the calculation of the beam deﬂection (see Problem 13.3), use appropriate values of Cb in the lateral torsional buckling equations that account for the moment gradient, and examine local buckling at both positive and negative moment locations. Justify all design assumptions in writing.] 13.22 Design a laterally braced simply supported wide–ﬂange glassvinylester pultruded section to carry a uniformly distributed load of 95 lb/ft (not including beam self-weight) on a 15-ft span. Assume that a maximum short-term deﬂection of L/180 is permitted. Do not consider long-term deﬂection. Determine the spacing of the lateral braces to prevent lateral torsional buckling of the beam selected. Consider pultruded materials from three different U.S. manufacturers and use the ASD and LRFD design bases. Compare your ﬁnal design to that given in the allowable load tables of the manufacturer selected. 13.23 Design (a) a conventional steel I-beam, (b) a cold-formed steel Ibeam, (c) an aluminum I-beam, and (d) a structural grade lumber beam to meet the requirements of Design Example 13.4. Use appropriate design bases and design speciﬁcations for the conventional material beams. Choose the lowest-possible strength and stiffness grades of the conventional materials for the sizes chosen. Compare the crosssectional sizes, unit weights, and costs of these conventional material beams to that of the pultruded beam designed in Design Example 13.4.

14 14.1

Pultruded Axial Members

OVERVIEW

In this chapter, design procedures are presented for axial members made of pultruded FRP proﬁles. This includes axially loaded compression members called columns, axially loaded tension members, and combined axial and ﬂexural members (called beam-columns when the axial load is compressive). Flexural members are discussed in Chapter 13. Connections and joints for pultruded proﬁles are discussed in Chapter 15. Theoretical mechanics-based equations are presented here for determining strength, stability, and deformation limit states of axially loaded pultruded structural members. Design procedures for the allowable stress design (ASD) and the load and resistance factor design (LRFD) bases described in Chapter 12 are presented. Since pultruded proﬁles behave essentially as linear elastic (or linear viscoelastic) structural members, the analytical equations developed for predicting stresses and deformations in these members for the ultimate and serviceability limit states are valid for either of the design bases selected. Therefore, it is only the safety factors for ASD or the load and resistance factors for the LRFD that differentiate the design procedures for the two design bases.

14.2

INTRODUCTION

The design of pultruded proﬁles that are doubly symmetric with respect to their principal coordinate axes and consist of horizontal plates (ﬂanges) and vertical plates (webs) are discussed in this section. This includes the conventionally manufactured I-shaped,1 square tube, rectangular tube, round tube, and multicelled tubular proﬁles. Typical member cross sections and orientations are shown in Fig. 14.1. In braced frame structures, wide-ﬂange I-sections and tubular sections are most frequently used as columns and bracing members, since they are readily connected using proﬁles or gusset plates and traditional mechanical connectors such as nuts and bolts (see, e.g., Figs. 1.15 and 1.18). The choice of

1

The term I-shaped proﬁles is used to describe both narrow- and wide-ﬂange I-shaped proﬁles.

436

Composites for Construction: Structural Design with FRP Materials. Lawrence C. Bank © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-68126-7

14.3

CONCENTRICALLY LOADED COMPRESSION MEMBERS

437

Figure 14.1 Cross sections and orientations of typical axial members.

proﬁle used as a column or brace often depends on the connection detailing required, as discussed further in Chapter 15. In trusses or stick-built frames, back-to-back angles and small channels, as well as small square tubular elements, are most commonly used (see, e.g., Figs. 1.17 and 1.19) as the primary structural elements. In this case, the elements are usually treated as continuous beams (such as chords, girts, purlins, or rafters), as axially loaded members (such as columns, struts, or ties), or as combined load members (beam-columns or tension-bending members). Flexural members are discussed in Chapter 13. The design of axially loaded members is divided here into three subsections: (1) concentrically loaded compression members, (2) concentrically loaded tension members, and (3) combined load members. 14.3

CONCENTRICALLY LOADED COMPRESSION MEMBERS

The compression member discussed in this section is designed to resist stress resultants (or internal forces) in the global x,y,z coordinate system that are caused by the concentric axial load, Pz, applied at the centroid of the cross section in the y–z plane, as shown in Fig. 14.2. The single stress resultant

y x

Pz

z

Pz

Figure 14.2 Concentrically loaded compression member.

438

PULTRUDED AXIAL MEMBERS

that the concentrically loaded compression member is designed for is the axial force, Pz. According to one-dimensional bar theory, if the member is homogeneous, this concentric axial force causes the member to develop a uniform axial (compressive) stress, z, throughout its cross section along its length, given by the normal stress equation z ⫽

Pz Az

(14.1)

where Az is the cross-sectional area of the member. For a beam with nonhomogeneous properties through the depth of the cross section, such as a pultruded proﬁle with different longitudinal elastic moduli in its webs and ﬂanges, the relationship between the axial force and the axial stress is not closed form but is written in general form as Pz ⫽

冕 dA A

z

(14.2)

where the integral is taken over the cross-sectional area of the beam. Since the pultruded material is assumed to be linear elastic in this one-dimensional bar theory, the strain through the depth of the axial member, z, is constant and the stress at point on the cross section, z, can be found directly using the longitudinal modulus, EL, at the point of interest. One-dimensional bar theories for bars having material of different moduli in the axial direction are covered in all elementary texts on mechanics of materials texts (e.g., Gere and Timoshenko, 1997). In what follows the properties of the inhomogeneous section are referred to as composite section properties, as noted in Chapter 13. In a typical pultruded proﬁle consisting of webs and ﬂanges having different longitudinal moduli, the axial force is found by summation as Pz ⫽

冘

z(flanges)

Az(flanges) ⫹ z(webs) Az(webs)

(14.3)

A

As shown in Fig. 14.2, the axial force will have a negative sign, and therefore compressive stresses will have a negative sign; however, for concentrically loaded members, the negative sign will be dropped here, and all equations for compression members will be written with a positive sign, as is customary in structural engineering. The axial stress (or axial force) calculated must be less than the material strength and critical buckling stress (or the critical resistance or buckling capacity) according to the design basis selected.

14.6

439

SERVICEABILITY LIMIT STATES: AXIAL SHORTENING

14.4 DEFORMATIONS IN CONCENTRICALLY LOADED COMPRESSION MEMBERS Due to the concentric axial force, Pz, a homogeneous member will shorten by the amount ␦z ⫽

Pz L Az E

(14.4)

where AzE is the axial rigidity of the member in compression (deﬁned below.) If the member is inhomogeneous, its axial rigidity is found using composite section mechanics. 14.5 DETERMINATION OF DEFLECTIONS AND STRESSES FOR SERVICEABILITY AND ULTIMATE LIMIT STATES For compression members the deﬂections are determined for the serviceability limit state and stresses (or stress-resultants) are determined for the ultimate limit state. As in the case of pultruded beam design discussed in Chapter 13, the low longitudinal modulus of conventional pultruded proﬁles will lead to appreciable axial deﬂections in column and truss members that should not be ignored in design. However, these deﬂections are nevertheless not usually the controlling limit state for compression members as they are for beams, due to the shorter lengths of compression members in most pultruded structures and the larger cross sections needed for axial members to resist global and local buckling. Consequently, the design procedure for compression members is slightly different from that for beams. Nevertheless, the serviceability limit states are ﬁrst discussed. 14.6

SERVICEABILITY LIMIT STATES: AXIAL SHORTENING

Uniaxial bar theory is used to determine the deﬂection of pultruded compression members. This is the procedure recommended by the Structural Plastic Design Manual (1984) and the Eurocomp Design Code and Handbook (Eurocomp, 1996). For the calculation of axial deformation, the axial rigidity is taken as Az E ⫽ Az EL

(14.5)

where EL is the longitudinal modulus of the pultruded material in compression. It is generally assumed that the tensile and compressive longitudinal moduli of the FRP material are the same, and most manufacturers report the

440

PULTRUDED AXIAL MEMBERS

same value for the tensile and compressive moduli or do not differentiate between the two. Some manufacturers report different values for the tensile and compressive moduli. If compressive moduli are reported, they should be used in deformation and buckling calculations for compression members. In the case of a nonhomogenous proﬁle having different moduli in different walls of the proﬁle, the composite axial rigidity, 兺i Ei Ai, is used (provided that the property variation is symmetric with respect to the centroidal axes). To determine long-term axial shortening, the viscoelastic longitudinal modulus, EL, with the creep parameters for compression given in Table 13.5 should be used. The axial shortening of compression members must be less than codestipulated maxima for axially loaded members. A limit of L/1500 is suggested for design of pultruded compression members; however, in a typical section, local buckling will probably occur well before this limit is reached. Often, these deformation requirements will be enforced via global deﬂection or lateral displacement limits on the entire structure.

14.7 14.7.1

ULTIMATE LIMIT STATES Global Flexural Buckling

The term global ﬂexural buckling is used to describe the commonly observed overall physical instability that can occur in compression members loaded by axial loads. It is commonly referred to as Euler buckling. When the critical global load is reached, the entire proﬁle displaces laterally about one of the centroidal axis planes (usually, the one with the larger slenderness ratio, kL/ r), causing the entire beam to move out of its vertical plane. Figure 14.3 shows global buckling of an I-shaped proﬁle about its weak (minor) axis. Global ﬂexural buckling of conventional pultruded proﬁles has been studied in a number of experimental investigations (Barbero and Tomlin, 1993; Zureick and Scott, 1997; Zureick and Steffen, 2000; Mottram et al., 2003a). It has been shown that the classical Euler equation can be used to describe the global ﬂexural buckling of conventional pultruded proﬁles. However, since pultruded proﬁles can be used as columns with low story heights (8 to 10 ft) and due to a higher EL /GLT ratio than the E/G ratio for isotropic columns, the effects of shear deformation should be considered, although in many cases the inﬂuence will be small (⬍ 5%) (Zureick and Scott, 1997; Roberts, 2002). The critical ﬂexural buckling load for a homogeneous member, including the effects of shear deformation, is given as (Zureick, 1998), Pflex cr ⫽ where

Peuler 1 ⫹ Peuler /ktim AzGLT

(14.6)

14.7

ULTIMATE LIMIT STATES

441

Figure 14.3 Global buckling of an I-shaped proﬁle. (Courtesy of Pizhong Qiao and Julio Davalos.)

Peuler ⫽

2ELI (kL)2

(14.7)

As discussed in Chapter 13, the transverse shear rigidity, KAG, can be approximated by ktim AzGLT ⬇ AwebGLT(web) The critical ﬂexural buckling stress, including the effects of shear deformation, is given as

442

PULTRUDED AXIAL MEMBERS

flex cr ⫽

冋

册

2EL 1 2 2 (kL/r)max 1 ⫹ (1/ktimGLT)( 2EL /(kL/r)max )

(14.8)

where (kL/r)max is the maximum slenderness ratio of the proﬁle, k the end restraint coefﬁcient, L the unbraced length (often called the height, h, in the case of a column), and r the radius of gyration for the axis under consideration. ktim is the Timoshenko shear coefﬁcient (deﬁned in Chapter 13) and Az is the cross-sectional area of the section. To neglect the effects of shear deformation, the term in brackets in equation (14.8) is set to unity. For nonhomogeneous members, composite section properties are used in the equations above. The Timoshenko shear coefﬁcient and the transverse shear rigidity, KAG, for a nonhomogeneous member can be found following procedures described in Bank (1987).

14.7.2

Global Torsional Buckling

Open-section compression members can buckle in a pure torsional mode. For doubly symmetric sections such as I-shaped proﬁles and tubular box sections, the torsional rigidity is high and torsional buckling is seldom a limiting state. However, for open sections in which the walls all meet at the centroid (such as a cruciform section), torsional buckling can be critical. Neglecting the inﬂuence of shear deformation, the critical torsional buckling stress in a homogeneous member is tor cr ⫽

冋

1 2ELC ⫹ GLT J Ip (k L)2

册

(14.9)

where Az is the cross-sectional area, Ip the polar second moment of area, J the torsional constant, C the warping constant, k an end restraint coefﬁcient for torsional buckling, and L the unbraced length of the member. GLT is the previously deﬁned in-plane shear modulus of the pultruded material. The GLTJ term is a conservative approximation for the Saint-Venant torsional rigidity, GJ, of a pultruded proﬁle. Its value can be obtained from full-section uniform torsion tests (Roberts and Al-Ubaidi, 2002). The critical torsional buckling load for homogeneous members is tor Ptor cr ⫽ cr Az

(14.10)

An approximate equation for the critical torsional buckling load that includes the effect of shear deformation (Roberts, 2002) for proﬁles with J/Ip ⬍⬍ 1 is

14.7

Ptor⫹sd ⫽ cr

ULTIMATE LIMIT STATES

Ptor cr 1 ⫹ Ptor cr /KAG

443

(14.11)

The torsional shear rigidity, KAG, can be approximated conservatively as the transverse shear stiffness, ktim AzGLT, or can be obtained by full-section torsional tests (Roberts and Ul-Ubaidi, 2002). For a nonhomogeneous member, the composite section properties need to be used in the equations above. The Timoshenko shear coefﬁcient and the transverse shear rigidity, KAG, for a nonhomogeneous member can be found following procedures described in Bank (1987). The composite warping stiffness, ELC, and the composite SaintVenant/torsional stiffness, GLT J, are not easily obtained, and approximate values of these values may need to be used for design. Guidance can be found in texts dealing with Vlasov thin-walled bar theory (Gjelsvik, 1981). Alternatively, full-section torsion tests can be performed to obtain the values for a speciﬁc section as described by Roberts and Ul-Ubaidi (2002). Singly symmetric sections such as angle proﬁles are not covered in this book; however, the reader should note that they are susceptible to global buckling in a ﬂexural–torsional mode consisting of Euler buckling about the major axis of the cross section and torsional buckling about the longitudinal axis of the member. Equations for this special case are presented by Zureick and Steffen (2000). 14.7.3

Local Buckling Due to Axial Loads

Conventional pultruded GRFP proﬁles are especially susceptible to local buckling when subjected to axial loads, due to the low in-plane moduli and the slenderness (width-to-thickness ratio) of the plate elements (known as walls) that make up the thin-walled proﬁle. Local buckling in compression ﬂanges of columns has been demonstrated in numerous tests (e.g., Yoon et al., 1992; Tomblin and Barbero, 1994; Pecce and Cosenza, 2000; Mottram, 2004). Figure 14.4 shows local compression ﬂange buckling in a concentrically loaded wide-ﬂange pultruded proﬁle. The local buckling seen in concentrially loaded columns is physically very similar in appearance to that in the compression ﬂanges of the ﬂexurally loaded beams discussed in Chapter 13 and shown in Fig. 13.7. However, in axially loaded columns, both ﬂanges buckle at the same time, whereas in a beam, only the compression ﬂange buckles. Therefore, the restraint provided by the web on the buckling of the ﬂange in the column is less than that provided by the web of a beam, and the local buckling equations are different from those for a beam. As discussed for beams in Chapter 13, the critical buckling load (or stress) in a wall (or panel) of a proﬁle is a function of the boundary conditions on the longitudinal edges of the wall. In I-shaped proﬁles2 the ﬂange is partic2

The term I-shaped proﬁles is used to describe both narrow- and wide-ﬂange I-shaped proﬁles.

444

PULTRUDED AXIAL MEMBERS

Figure 14.4 Local compression ﬂange buckling in both ﬂanges of a wide-ﬂange pultruded proﬁle subjected to axial load. (Courtesy of J. T. Mottram.)

ularly susceptible to buckling, since one edge is free while the other edge is elastically restrained at the web–ﬂange junction. As in the case of the transversely loaded beam, the method due to Kolla´r (2003) is presented for local buckling of the walls of a concentrically loaded column. The reader is referred to the discussion in Chapter 13 related to the choice of Kolla´r’s method. Only the design equations for doubly symmetric I- and box-shaped proﬁles are presented in this book, due to the fact that at this time, these proﬁles are most commonly used as beams and columns in pultruded structures. This includes built-up sections that are of I or box shape. The reader is referred to Kolla´r’s work for singly symmetric sections. The cross-sectional notation for I- and box-shaped proﬁles are shown in Fig. 13.9. Since local buckling of the ﬂange and the web of a section due to in-plane normal loads are interrelated, ﬂange and web buckling are treated together in this section. To use Kolla´r’s method, ﬁrst the buckling stresses (or loads) of the walls, assuming they are simply supported at their restrained edges, are found. These stresses are then used to determine which wall buckles ﬁrst and the coefﬁcient of edge restraint for the critical wall. The ﬁnal solution for the buckling stress for a restrained wall is then given by a closed-form equation that includes the coefﬁcient of edge restraint, , of the critical wall. Two types of simply supported walls3 are needed for the ﬁrst part of the solution4: 1. A wall that is free and simply supported on its edges under uniform axial stress. This solution is used to determine the critical stress in the

3 For all cases it is assumed that the loaded edges are simply supported. The descriptors are used to identify the longitudinal unloaded edges of the wall. 4 Many of the equations presented in this section are identical to those presented for local buckling in Chapter 13. They are repeated in this chapter to aid the reader and to make the section on axial members self-contained.

14.7

ULTIMATE LIMIT STATES

445

ﬂange of an I-shaped proﬁle.5 It is given in terms of the ﬂexural rigidities6 of the ﬂange as ss ( free )ƒ ⫽

冋冉 冊

bƒ /2 2 DL 2 tƒ(bƒ /2) a

2

⫹

12 D 2 S

册

(14.12)

where tƒ is the ﬂange thickness, bƒ the proﬁle width (twice the nominal width of the ﬂange), and a the buckle half-wavelength, which is equal to the length of the ﬂange in this special case.7 For long ﬂanges, as is typically the case, the ﬁrst term in brackets in equation (14.12) is negligible and the critical stress can be found from ( ss free)ƒ ⫽

4t2ƒ G bƒ2 LT

(14.13)

In this mode the plate buckles with one buckle half-wavelength, equal to the plate length (like a simply supported Euler column). 2. A wall that is simply supported along both edges under uniform axial stress. This solution is used to determine the critical stress in the web of an I-shape and the web and ﬂange of a box section. It is given in terms of the ﬂexural rigidities of the wall, i, as ( ss ss)i ⫽

2 2 (兹DLDT ⫹ DLT ⫹ 2DS) tt bi2

(14.14)

where the subscript i implies w for the web and ƒ for the ﬂange and the symbol b implies b for the ﬂange and d for the web. The length of the buckle half-wavelength for this mode is given by

冪EE

4 (ass ss)i ⫽ bi

L

(14.15)

T

Local Buckling Equations for an I-Shaped Proﬁle in Axial Compression ss If ( ss free)ƒ / (EL)ƒ ⬍ ( ss)w / (EL)w, the ﬂange will buckle before the web. The ﬂange will therefore be restrained by the web. Except in very unusual cir-

5 A different notation from that used in Kolla´r (2003) is used in what follows to make the equations more familiar to structural engineers unfamiliar with laminated plate and composite material notation. For the same reason, equations are given for plate buckling stresses but not for plate buckling loads. 6 See Chapter 12 for a deﬁnition of plate ﬂexural rigidities. 7 Note that in many texts the parameter b is used to denote the width of the ﬂange only and is equal to one-half of bƒ.

446

PULTRUDED AXIAL MEMBERS

cumstances, this will be the buckling mode that will control for conventional pultruded GFRP proﬁles. The spring constant is then given as kl-flange ⫽

冋

册

( ss (DT)w free)ƒ(EL)w 1⫺ dw ( ss ss)w(EL)ƒ

(14.16)

and the buckling stress for the rotationally restrained ﬂange is given in terms of the properties of the ﬂange as8

冊

(14.17)

(DT)ƒ (ET)ƒt3ƒ ⫽ kI-flange (bƒ /2) 6kI-flange bƒ [1 ⫺ (T)ƒ(L)ƒ]

(14.18)

local,I-flange cr ⫽

冉冪

1 7 (bƒ /2)2tƒ

DLDT ⫹ 12DS 1 ⫹ 4.12I-flange

where I-flange ⫽

The buckle half-wavelength, a, for this case is given in terms of the properties of the ﬂange as (Kolla´r and Springer, 2003, Table 4.10)

aI-flange ⫽ 1.675

bƒ 2

冪DD (1 4

L

⫹ 4.12I-flange)

(14.19)

T

The critical axial load for the local ﬂange buckling of a homogeneous Ishaped proﬁle loaded in axial compression is therefore local,I-flange Plocal,I-flange ⫽ cr Az cr

(14.20)

In the case of a nonhomogeneous section, the critical axial load is found by integration of the axial stresses over the various property walls in the section. The strain corresponding to the critical stress in the ﬂange is ﬁrst found and then the stresses in all the walls of the section are determined. ss If ( ss free)ƒ / (EL)ƒ ⬎ ( ss)w / (EL)w, the web will buckle before the ﬂange. The spring constant is then obtained by assuming that the outstanding ﬂanges act as longitudinal stiffeners at the web edges (Kolla´r, 2003), and the equivalent spring constant is given as

8

Kolla´r (2003) provides an alternative equation for this case that provides greater accuracy if needed.

14.7

kI-web ⫽

ULTIMATE LIMIT STATES

冋

册

4(DT)ƒ ( ss ss)w(EL)ƒ 1 ⫺ ss bƒ ( free)ƒ(EL)w

447

(14.21)

and the buckling stress for the rotationally restrained web is given in terms of the properties of the web as local,I-web ⫽ cr

2 [2兹(DLDT)(1 ⫹ 4.139) d 2wtw

(14.22)

⫹ (DLT ⫹ 2DS)(2 ⫹ 0.62 2I-web)]

where I-web ⫽

1 1 ⫽ 1 ⫹ 10I-web 1 ⫹ 10 [(DT)w /kI-webdw]

(14.23)

The buckle half-wavelength, a, for this case is given in terms of the properties of the web as (Kolla´r and Springer, 2003, Table 4.10) aI-web ⫽ bƒ

冪DD 冉1 4

L T

1 ⫹ 4.139 I-web

冊

(14.24)

The critical axial load for the local web buckling of a homogeneous Ishaped proﬁle loaded in axial compression is therefore local,I-web Plocal,I-web ⫽ cr Az cr

(14.25)

For a nonhomogeneous section, the critical axial load is found by integration of the axial stresses over the various property walls in the section. The strain corresponding to the critical stress in the web is ﬁrst found, and then the stresses in all the walls of the section are determined. Local Buckling Equations for a Rectangular Box Proﬁle in Axial ss Compression If ( ss ss)ƒ / (EL)ƒ ⬍ ( ss)w / (EL)w, the ﬂanges will buckle before the webs. The ﬂanges will therefore be restrained by both of the webs, one on either longitudinal edge of the ﬂange. The spring constant is then given as kbox-flange ⫽

冋

册

( ss 2(DT)w ss)ƒ(EL)w 1 ⫺ ss dw ( ss)w(EL)ƒ

(14.26)

and the buckling stress for the rotationally restrained ﬂange is given in terms of the properties of the ﬂange as

448

PULTRUDED AXIAL MEMBERS

local,box-flange ⫽ cr

2 [2兹(DLDT)(1 ⫹ 4.139) b2ƒtƒ ⫹ (DLT ⫹ 2DS)(2 ⫹ 0.62 2box-flange)]

(14.27)

where box-flange ⫽

1 1 ⫽ 1 ⫹ 10box-flange 1 ⫹ 10 [(DT)ƒ /kbox-flangebƒ]

(14.28)

The buckle half-wavelength, a, for this case is given in terms of the properties of the ﬂange as (Kolla´r and Springer, 2003, Table 4.10)

abox-flange ⫽ bƒ

冪DD 冉1 4

L T

1 ⫹ 4.139 box-flange

冊

(14.29)

The critical axial load for the local ﬂange buckling of a homogeneous boxshaped proﬁle loaded in axial compression is therefore, Plocal,box-flange ⫽ local,box-flange Az cr cr

(14.30)

For a nonhomogeneous section, the critical axial load is found by integration of the axial stresses over the different property walls in the section. The strain corresponding to the critical stress in the ﬂange is found ﬁrst, and then the stresses in all the walls of the section are determined. ss If ( ss ss)ƒ / (EL)ƒ ⬎ ( ss)w / (EL)w, the webs will buckle before the ﬂanges. The webs will therefore be restrained by both of the ﬂanges, one on either longitudinal edge of each web. The spring constant is then given as kbox-web ⫽

冋

册

ss 2(DT)ƒ ( ss )w(EL)ƒ 1 ⫺ ss bƒ ( ss)ƒ(EL)w

(14.31)

and the buckling stress for the rotationally restrained web is given in terms of the properties of the web as local,box-web ⫽ cr

2 [2兹(DLDT)(1 ⫹ 4.139) d 2wtw ⫹ (DLT ⫹ 2DS)(2 ⫹ 0.62

where

(14.32)

2 box-web

)]

14.7

box-web ⫽

ULTIMATE LIMIT STATES

1 1 ⫽ 1 ⫹ 10box-web 1 ⫹ 10 [(DT)w /kbox-webdw]

449

(14.33)

The buckle half-wavelength, a, for this case is given in terms of the properties of the web as (Kolla´r and Springer, 2003, Table 4.10) abox-web ⫽ dw

冪 冉 4

冊

DL 1 DT 1 ⫹ 4.139 box-web

(14.34)

The critical axial load for the local web buckling of a homogeneous boxshaped proﬁle loaded in axial compression is therefore local,box-web Plocal,box-web ⫽ cr Az cr

(14.35)

For a nonhomogeneous section, the critical axial load is found by integration of the axial stresses over the various property walls in the section. The strain corresponding to the critical stress in the web is ﬁrst found and then the stresses in all the walls of the section are determined. It can be observed that the buckling equations for the webs and ﬂanges of the rectangular box beams are of the same form but have the web and ﬂange properties interchanged. Approximate Procedure for I-Proﬁles To use the equations presented previously due to Kolla´r (2003), all of the in-plane properties of the orthotropic walls of the section are required to predict the buckling stress. However, the in-plane shear modulus is often not reported by manufacturers and is not required to be reported by the European Standard EN 13706 (CEN, 2002a). In this situation a simpliﬁed form suggested in the Structural Plastics Design Manual (ASCE, 1984, p. 676) for obtaining the critical ﬂange buckling stress for the free and rotationally restrained ﬂange in an I-shaped proﬁle can be used (Mottram, 2004): local,I-flange cr,approx ⫽

2t2ƒ (bƒ /2)2

冋冉

0.45 ⫹

冊

册

兹ELET b2ƒ 4a2 12(1 ⫺ LT)

(14.36)

where the mechanical properties are those of the ﬂange. This expression requires the length of the buckle half-wavelength, a, which is not known a priori. To use this equation the buckle half-wavelength can be taken conservatively as 2bƒ for wide-ﬂange and 3bƒ for narrow-ﬂange conventional pultruded I-shaped proﬁles. Alternatively, the ﬁrst term in brackets can be taken even more conservatively as 0.45. Note that Equation (14.36) is identical to Equation (13.37) as the simpliﬁed method does not distinguish between ﬂange buckling in a beam and a column. The approximate critical axial load for the

450

PULTRUDED AXIAL MEMBERS

local ﬂange buckling of a homogeneous I-shaped proﬁle loaded in axial compression is therefore Plocal,I-flange ⫽ local,I-flange Az cr,approx cr,approx

(14.37)

Additional Issues Related to Buckling of Pultruded Proﬁles A comparison between the equations presented in this chapter for predicting local buckling of webs and ﬂanges in axially loaded compression members with those presented in Chapter 13 for predicting similar phenomena reveals that it is only the coefﬁcients of restraint at the web ﬂange junction that leads to different, and expected, results for these members. For further discussion on local buckling-related phenomena in pultruded proﬁles, the reader should refer to the discussions in Section 13.7.2 under the heading ‘‘Further Discussion of Flange Buckling in I-Sections’’ related to slenderness ratios of thin walls in pultruded proﬁles, and in Section 13.7.5 related to the inﬂuence of sustained load and creep deformation on buckling of pultruded proﬁles. These discussions are also applicable to pultruded compression members. 14.7.4 Interaction Between Local and Global Buckling Modes in Intermediate-Length Compression Members Whether a pultruded compression member fails due to global ﬂexural buckling, local buckling, or material compressive failure depends on the slendern